*176*
*58*
*3MB*

*English*
*Pages 502
[501]*
*Year 2014*

Table of contents :

Cover

Preface to the ninth edition

Contents

Data on specific materials in text

Introduction

The electron as a particle

1.1 Introduction

1.2 The effect of an electric field—conductivity and Ohm’s law

1.3 The hydrodynamicmodel of electron flow

1.4 The Hall effect

1.5 Electromagnetic waves in solids

1.6 Waves in the presence of an appliedmagnetic field: cyclotron resonance

1.7 Plasma waves

1.8 Johnson noise

1.9 Heat

Exercises

The electron as a wave

2.1 Introduction

2.2 The electron microscope

2.3 Some properties of waves

2.4 Applications to electrons

2.5 Two analogies

Exercises

The electron

3.1 Introduction

3.2 Schrödinger’s equation

3.3 Solutions of Schrödinger’s equation

3.4 The electron as a wave

3.5 The electron as a particle

3.6 The electron meeting a potential barrier

3.7 Two analogies

3.8 The electron in a potential well

3.9 The potential well with a rigid wall

3.10 The uncertainty relationship

3.11 Philosophical implications

Exercises

The hydrogen atom and the periodic table

4.1 The hydrogen atom

4.2 Quantum numbers

4.3 Electron spin and Pauli’s exclusion principle

4.4 The periodic table

Exercises

Bonds

5.1 Introduction

5.2 General mechanical properties of bonds

5.3 Bond types

5.3.1 Ionic bonds

5.3.2 Metallic bonds

5.3.3 The covalent bond

5.3.4 The van der Waals bond

5.3.5 Mixed bonds

5.3.6 Carbon again

5.4 Feynman’s coupledmode approach

5.5 Nuclear forces

5.6 The hydrogen molecule

5.7 An analogy

Exercises

The free electron theory of metals

6.1 Free electrons

6.2 The density of states and the Fermi–Dirac distribution

6.3 The specific heat of electrons

6.4 The work function

6.5 Thermionic emission

6.6 The Schottky effect

6.7 Field emission

6.8 The field-emissionmicroscope

6.9 The photoelectric effect

6.10 Quartz–halogen lamps

6.11 The junction between two metals

Exercises

The band theory of solids

7.1 Introduction

7.2 The Kronig–Penneymodel

7.3 The Ziman model

7.4 The Feynmanmodel

7.5 The effectivemass

7.6 The effective number of free electrons

7.7 The number of possible states per band

7.8 Metals and insulators

7.9 Holes

7.10 Divalent metals

7.11 Finite temperatures

7.12 Concluding remarks

Exercises

Semiconductors

8.1 Introduction

8.2 Intrinsic semiconductors

8.3 Extrinsic semiconductors

8.4 Scattering

8.5 A relationship between electron and hole densities

8.6 III–V and II–VI compounds

8.7 Non-equilibrium processes

8.8 Real semiconductors

8.9 Amorphous semiconductors

8.10 Measurement of semiconductor properties

8.10.1 Mobility

8.10.2 Hall coefficient

8.10.3 Effective mass

8.10.4 Energy gap

8.10.5 Carrier lifetime

8.11 Preparation of pure and controlled-impurity single-crystal semiconductors

8.11.1 Crystal growth from the melt

8.11.2 Zone refining

8.11.3 Modern methods of silicon purification

8.11.4 Epitaxial growth

8.11.5 Molecular beam epitaxy

8.11.6 Metal–organic chemical vapour deposition

8.11.7 Hydride vapour phase epitaxy (HVPE) for nitride devices

Exercises

Principles of semiconductor devices

9.1 Introduction

9.2 The p–n junction in equilibrium

9.3 Rectification

9.4 Injection

9.5 Junction capacity

9.6 The transistor

9.7 Metal–semiconductor junctions

9.8 The role of surface states; real metal–semiconductor junctions

9.9 Metal–insulator–semiconductor junctions

9.10 The tunnel diode

9.11 The backward diode

9.12 The Zener diode and the avalanche diode

9.12.1 Zener breakdown

9.12.2 Avalanche breakdown

9.13 Varactor diodes

9.14 Field-effect transistors

9.15 Heterostructures

9.16 Charge-coupled devices

9.17 Silicon controlled rectifier

9.18 The Gunn effect

9.19 Strain gauges

9.20 Measurement ofmagnetic field by the Hall effect

9.21 Gas sensors

9.22 Microelectronic circuits

9.23 Plasma etching

9.24 Recent techniques for overcoming limitations

9.25 Building in the third dimension

9.26 Microelectro-mechanical systems (MEMS)

9.26.1 A movable mirror

9.26.2 A mass spectrometer on a chip

9.27 Nanoelectronics

9.28 Social implications

Exercises

Dielectric materials

10.1 Introduction

10.2 Macroscopic approach

10.3 Microscopic approach

10.4 Types of polarization

10.5 The complex dielectric constant and the refractive index

10.6 Frequency response

10.7 Anomalous dispersion

10.8 Polar and non-polar materials

10.9 The Debye equation

10.10 The effective field

10.11 Acoustic waves

10.12 Dielectric breakdown

10.12.1 Intrinsic breakdown

10.12.2 Thermal breakdown

10.12.3 Discharge breakdown

10.13 Piezoelectricity, pyroelectricity, and ferroelectricity

10.13.1 Piezoelectricity

10.13.2 Pyroelectricity

10.13.3 Ferroelectrics

10.14 Interaction of optical phonons with drifting electrons

10.15 Optical fibres

10.16 The Xerox process

10.17 Liquid crystals

10.18 Dielectrophoresis

Exercises

Magneticmaterials

11.1 Introduction

11.2 Macroscopic approach

11.3 Microscopic theory (phenomenological)

11.4 Domains and the hysteresis curve

11.5 Softmagneticmaterials

11.6 Hardmagnetic materials (permanentmagnets)

11.7 Microscopic theory (quantum-mechanical)

11.7.1 The Stern–Gerlach experiment

11.7.2 Paramagnetism

11.7.3 Paramagnetic solids

11.7.4 Antiferromagnetism

11.7.5 Ferromagnetism

11.7.6 Ferrimagnetism

11.7.7 Garnets

11.7.8 Helimagnetism

11.8 Magnetic resonance

11.8.1 Paramagnetic resonance

11.8.2 Electron spin resonance

11.8.3 Ferromagnetic, antiferromagnetic, and ferrimagnetic resonance

11.8.4 Nuclear magnetic resonance

11.8.5 Cyclotron resonance

11.9 The quantum Hall effect

11.10 Magnetoresistance

11.11 Spintronics

11.11.1 Spin current

11.11.2 Spin tunnelling

11.11.3 Spin waves and magnons

11.11.4 Spin Hall effect and its inverse

11.11.5 Spin and light

11.11.6 Spin transfer torque

11.12 Some applications

11.12.1 Isolators

11.12.2 Sensors

11.12.3 Magnetic read-heads

11.12.4 Electric motors

Exercises

Lasers

12.1 Equilibrium

12.2 Two-state systems

12.3 Lineshape function

12.4 Absorption and amplification

12.5 Resonators and conditions of oscillation

12.6 Some practical laser systems

12.6.1 Solid state lasers

12.6.2 The gaseous discharge laser

12.6.3 Dye lasers

12.6.4 Gas-dynamic lasers

12.6.5 Excimer lasers

12.6.6 Chemical lasers

12.7 Semiconductor lasers

12.7.1 Fundamentals

12.7.2 Wells, wires, and dots

12.7.3 Bandgap engineering

12.7.4 Quantum cascade lasers

12.8 Laser modes and control techniques

12.8.1 Transverse modes

12.8.2 Axial modes

12.8.3 Q switching

12.8.4 Cavity dumping

12.8.5 Mode locking

12.9 Parametric oscillators

12.10 Optical fibre amplifiers

12.11 Masers

12.12 Noise

12.13 Applications

12.13.1 Nonlinear optics

12.13.2 Spectroscopy

12.13.3 Photochemistry

12.13.4 Study of rapid events

12.13.5 Plasma diagnostics

12.13.6 Plasma heating

12.13.7 Acoustics

12.13.8 Genetics

12.13.9 Metrology

12.13.10 Manipulation of atoms by light

12.13.11 Optical radar

12.13.12 Optical discs

12.13.13 Medical applications

12.13.14 Machining

12.13.15 Sensors

12.13.16 Communications

12.13.17 Nuclear applications

12.13.18 Holography

12.13.19 Raman scattering

12.14 The atom laser

Exercises

Optoelectronics

13.1 Introduction

13.2 Light detectors

13.3 Light emitting diodes (LEDs)

13.4 Electro-optic, photorefractive, and nonlinear materials

13.5 Volume holography and phase conjugation

13.6 Acousto-optic interaction

13.7 Integrated optics

13.7.1 Waveguides

13.7.2 Phase shifter

13.7.3 Directional coupler

13.7.4 Filters

13.8 Spatial light modulators

13.9 Nonlinear Fabry–Perot cavities

13.10 Optical switching

13.11 Electro-absorption in quantum well structures

13.11.1 Excitons

13.11.2 Excitons in quantum wells

13.11.3 Electro-absorption

13.11.4 Applications

Exercises

Superconductivity

14.1 Introduction

14.2 The effect of amagnetic field

14.2.1 The critical magnetic field

14.2.2 The Meissner effect

14.3 Microscopic theory

14.4 Thermodynamical treatment

14.5 Surface energy

14.6 The Landau–Ginzburg theory

14.7 The energy gap

14.8 Some applications

14.8.1 High-field magnets

14.8.2 Switches and memory elements

14.8.3 Magnetometers

14.8.4 Metrology

14.8.5 Suspension systems and motors

14.8.6 Radiation detectors

14.8.7 Heat valves

14.9 High-Tc superconductors

14.10 New superconductors

Exercises

Artificial materialsor metamaterials

15.1 Introduction

15.2 Natural and artificialmaterials

15.3 Photonic bandgap materials

15.4 Equivalent plasma frequency of a wire medium

15.5 Resonant elements for metamaterials

15.6 Polarizability of a current-carrying resonant loop

15.7 Effective permeability

15.8 Effect of negative material constants

15.9 The ‘perfect’ lens

15.10 Detectors for magnetic resonance imaging

Epilogue

Appendix I: Organic semiconductors

Appendix II: Nobel laureates

Appendix III: Physical constants

Appendix IV: Variational calculus. Derivation of Euler’s equation

Appendix V: Thermoelectricity

Appendix VI: Principles of the operation of computer memories

Appendix VII:Medical imaging

Appendix VIII: Suggestions for further reading

Answers to exercises

Index

Cover

Preface to the ninth edition

Contents

Data on specific materials in text

Introduction

The electron as a particle

1.1 Introduction

1.2 The effect of an electric field—conductivity and Ohm’s law

1.3 The hydrodynamicmodel of electron flow

1.4 The Hall effect

1.5 Electromagnetic waves in solids

1.6 Waves in the presence of an appliedmagnetic field: cyclotron resonance

1.7 Plasma waves

1.8 Johnson noise

1.9 Heat

Exercises

The electron as a wave

2.1 Introduction

2.2 The electron microscope

2.3 Some properties of waves

2.4 Applications to electrons

2.5 Two analogies

Exercises

The electron

3.1 Introduction

3.2 Schrödinger’s equation

3.3 Solutions of Schrödinger’s equation

3.4 The electron as a wave

3.5 The electron as a particle

3.6 The electron meeting a potential barrier

3.7 Two analogies

3.8 The electron in a potential well

3.9 The potential well with a rigid wall

3.10 The uncertainty relationship

3.11 Philosophical implications

Exercises

The hydrogen atom and the periodic table

4.1 The hydrogen atom

4.2 Quantum numbers

4.3 Electron spin and Pauli’s exclusion principle

4.4 The periodic table

Exercises

Bonds

5.1 Introduction

5.2 General mechanical properties of bonds

5.3 Bond types

5.3.1 Ionic bonds

5.3.2 Metallic bonds

5.3.3 The covalent bond

5.3.4 The van der Waals bond

5.3.5 Mixed bonds

5.3.6 Carbon again

5.4 Feynman’s coupledmode approach

5.5 Nuclear forces

5.6 The hydrogen molecule

5.7 An analogy

Exercises

The free electron theory of metals

6.1 Free electrons

6.2 The density of states and the Fermi–Dirac distribution

6.3 The specific heat of electrons

6.4 The work function

6.5 Thermionic emission

6.6 The Schottky effect

6.7 Field emission

6.8 The field-emissionmicroscope

6.9 The photoelectric effect

6.10 Quartz–halogen lamps

6.11 The junction between two metals

Exercises

The band theory of solids

7.1 Introduction

7.2 The Kronig–Penneymodel

7.3 The Ziman model

7.4 The Feynmanmodel

7.5 The effectivemass

7.6 The effective number of free electrons

7.7 The number of possible states per band

7.8 Metals and insulators

7.9 Holes

7.10 Divalent metals

7.11 Finite temperatures

7.12 Concluding remarks

Exercises

Semiconductors

8.1 Introduction

8.2 Intrinsic semiconductors

8.3 Extrinsic semiconductors

8.4 Scattering

8.5 A relationship between electron and hole densities

8.6 III–V and II–VI compounds

8.7 Non-equilibrium processes

8.8 Real semiconductors

8.9 Amorphous semiconductors

8.10 Measurement of semiconductor properties

8.10.1 Mobility

8.10.2 Hall coefficient

8.10.3 Effective mass

8.10.4 Energy gap

8.10.5 Carrier lifetime

8.11 Preparation of pure and controlled-impurity single-crystal semiconductors

8.11.1 Crystal growth from the melt

8.11.2 Zone refining

8.11.3 Modern methods of silicon purification

8.11.4 Epitaxial growth

8.11.5 Molecular beam epitaxy

8.11.6 Metal–organic chemical vapour deposition

8.11.7 Hydride vapour phase epitaxy (HVPE) for nitride devices

Exercises

Principles of semiconductor devices

9.1 Introduction

9.2 The p–n junction in equilibrium

9.3 Rectification

9.4 Injection

9.5 Junction capacity

9.6 The transistor

9.7 Metal–semiconductor junctions

9.8 The role of surface states; real metal–semiconductor junctions

9.9 Metal–insulator–semiconductor junctions

9.10 The tunnel diode

9.11 The backward diode

9.12 The Zener diode and the avalanche diode

9.12.1 Zener breakdown

9.12.2 Avalanche breakdown

9.13 Varactor diodes

9.14 Field-effect transistors

9.15 Heterostructures

9.16 Charge-coupled devices

9.17 Silicon controlled rectifier

9.18 The Gunn effect

9.19 Strain gauges

9.20 Measurement ofmagnetic field by the Hall effect

9.21 Gas sensors

9.22 Microelectronic circuits

9.23 Plasma etching

9.24 Recent techniques for overcoming limitations

9.25 Building in the third dimension

9.26 Microelectro-mechanical systems (MEMS)

9.26.1 A movable mirror

9.26.2 A mass spectrometer on a chip

9.27 Nanoelectronics

9.28 Social implications

Exercises

Dielectric materials

10.1 Introduction

10.2 Macroscopic approach

10.3 Microscopic approach

10.4 Types of polarization

10.5 The complex dielectric constant and the refractive index

10.6 Frequency response

10.7 Anomalous dispersion

10.8 Polar and non-polar materials

10.9 The Debye equation

10.10 The effective field

10.11 Acoustic waves

10.12 Dielectric breakdown

10.12.1 Intrinsic breakdown

10.12.2 Thermal breakdown

10.12.3 Discharge breakdown

10.13 Piezoelectricity, pyroelectricity, and ferroelectricity

10.13.1 Piezoelectricity

10.13.2 Pyroelectricity

10.13.3 Ferroelectrics

10.14 Interaction of optical phonons with drifting electrons

10.15 Optical fibres

10.16 The Xerox process

10.17 Liquid crystals

10.18 Dielectrophoresis

Exercises

Magneticmaterials

11.1 Introduction

11.2 Macroscopic approach

11.3 Microscopic theory (phenomenological)

11.4 Domains and the hysteresis curve

11.5 Softmagneticmaterials

11.6 Hardmagnetic materials (permanentmagnets)

11.7 Microscopic theory (quantum-mechanical)

11.7.1 The Stern–Gerlach experiment

11.7.2 Paramagnetism

11.7.3 Paramagnetic solids

11.7.4 Antiferromagnetism

11.7.5 Ferromagnetism

11.7.6 Ferrimagnetism

11.7.7 Garnets

11.7.8 Helimagnetism

11.8 Magnetic resonance

11.8.1 Paramagnetic resonance

11.8.2 Electron spin resonance

11.8.3 Ferromagnetic, antiferromagnetic, and ferrimagnetic resonance

11.8.4 Nuclear magnetic resonance

11.8.5 Cyclotron resonance

11.9 The quantum Hall effect

11.10 Magnetoresistance

11.11 Spintronics

11.11.1 Spin current

11.11.2 Spin tunnelling

11.11.3 Spin waves and magnons

11.11.4 Spin Hall effect and its inverse

11.11.5 Spin and light

11.11.6 Spin transfer torque

11.12 Some applications

11.12.1 Isolators

11.12.2 Sensors

11.12.3 Magnetic read-heads

11.12.4 Electric motors

Exercises

Lasers

12.1 Equilibrium

12.2 Two-state systems

12.3 Lineshape function

12.4 Absorption and amplification

12.5 Resonators and conditions of oscillation

12.6 Some practical laser systems

12.6.1 Solid state lasers

12.6.2 The gaseous discharge laser

12.6.3 Dye lasers

12.6.4 Gas-dynamic lasers

12.6.5 Excimer lasers

12.6.6 Chemical lasers

12.7 Semiconductor lasers

12.7.1 Fundamentals

12.7.2 Wells, wires, and dots

12.7.3 Bandgap engineering

12.7.4 Quantum cascade lasers

12.8 Laser modes and control techniques

12.8.1 Transverse modes

12.8.2 Axial modes

12.8.3 Q switching

12.8.4 Cavity dumping

12.8.5 Mode locking

12.9 Parametric oscillators

12.10 Optical fibre amplifiers

12.11 Masers

12.12 Noise

12.13 Applications

12.13.1 Nonlinear optics

12.13.2 Spectroscopy

12.13.3 Photochemistry

12.13.4 Study of rapid events

12.13.5 Plasma diagnostics

12.13.6 Plasma heating

12.13.7 Acoustics

12.13.8 Genetics

12.13.9 Metrology

12.13.10 Manipulation of atoms by light

12.13.11 Optical radar

12.13.12 Optical discs

12.13.13 Medical applications

12.13.14 Machining

12.13.15 Sensors

12.13.16 Communications

12.13.17 Nuclear applications

12.13.18 Holography

12.13.19 Raman scattering

12.14 The atom laser

Exercises

Optoelectronics

13.1 Introduction

13.2 Light detectors

13.3 Light emitting diodes (LEDs)

13.4 Electro-optic, photorefractive, and nonlinear materials

13.5 Volume holography and phase conjugation

13.6 Acousto-optic interaction

13.7 Integrated optics

13.7.1 Waveguides

13.7.2 Phase shifter

13.7.3 Directional coupler

13.7.4 Filters

13.8 Spatial light modulators

13.9 Nonlinear Fabry–Perot cavities

13.10 Optical switching

13.11 Electro-absorption in quantum well structures

13.11.1 Excitons

13.11.2 Excitons in quantum wells

13.11.3 Electro-absorption

13.11.4 Applications

Exercises

Superconductivity

14.1 Introduction

14.2 The effect of amagnetic field

14.2.1 The critical magnetic field

14.2.2 The Meissner effect

14.3 Microscopic theory

14.4 Thermodynamical treatment

14.5 Surface energy

14.6 The Landau–Ginzburg theory

14.7 The energy gap

14.8 Some applications

14.8.1 High-field magnets

14.8.2 Switches and memory elements

14.8.3 Magnetometers

14.8.4 Metrology

14.8.5 Suspension systems and motors

14.8.6 Radiation detectors

14.8.7 Heat valves

14.9 High-Tc superconductors

14.10 New superconductors

Exercises

Artificial materialsor metamaterials

15.1 Introduction

15.2 Natural and artificialmaterials

15.3 Photonic bandgap materials

15.4 Equivalent plasma frequency of a wire medium

15.5 Resonant elements for metamaterials

15.6 Polarizability of a current-carrying resonant loop

15.7 Effective permeability

15.8 Effect of negative material constants

15.9 The ‘perfect’ lens

15.10 Detectors for magnetic resonance imaging

Epilogue

Appendix I: Organic semiconductors

Appendix II: Nobel laureates

Appendix III: Physical constants

Appendix IV: Variational calculus. Derivation of Euler’s equation

Appendix V: Thermoelectricity

Appendix VI: Principles of the operation of computer memories

Appendix VII:Medical imaging

Appendix VIII: Suggestions for further reading

Answers to exercises

Index

- Author / Uploaded
- Laszlo Solymar
- Donald Walsh
- Richard R. A. Syms

Electrical properties of materials NINTH EDITION

L. Solymar Department of Electrical and Electronic Engineering Imperial College, London

D. Walsh Department of Engineering Science University of Oxford

R. R. A. Syms Department of Electrical and Electronic Engineering Imperial College, London

3

3 Great Clarendon Street, Oxford, OX2 6DP, United Kingdom Oxford University Press is a department of the University of Oxford. It furthers the University’s objective of excellence in research, scholarship, and education by publishing worldwide. Oxford is a registered trade mark of Oxford University Press in the UK and in certain other countries © Oxford University Press, 1970, 1979, 1984, 1988, 1993, 1998, 2004, 2010, 2014 The moral rights of the authors have been asserted First edition 1970 Second edition 1979 Third edition 1984 Fourth edition 1988 Fifth edition 1993 Sixth edition 1998 Seventh edition 2004 Eighth edition 2010 Ninth edition 2014 Impression: 1 All rights reserved. No part of this publication may be reproduced, stored in a retrieval system, or transmitted, in any form or by any means, without the prior permission in writing of Oxford University Press, or as expressly permitted by law, by licence or under terms agreed with the appropriate reprographics rights organization. Enquiries concerning reproduction outside the scope of the above should be sent to the Rights Department, Oxford University Press, at the address above You must not circulate this work in any other form and you must impose this same condition on any acquirer Published in the United States of America by Oxford University Press 198 Madison Avenue, New York, NY 10016, United States of America British Library Cataloguing in Publication Data Data available Library of Congress Control Number: 2013952760 ISBN 978–0–19–870277–1 (hbk.) ISBN 978–0–19–870278–8 (pbk.) Printed and bound by CPI Group (UK) Ltd, Croydon, CR0 4YY Links to third party websites are provided by Oxford in good faith and for information only. Oxford disclaims any responsibility for the materials contained in any third party website referenced in this work.

Preface to the ninth edition The major change relative to all of the previous editions is that Professor Richard Syms of Imperial College has joined us as an author. There are new topics added and old topics updated, but the style remains as light as ever. Topics that needed considerable updating are semiconductor technology, semiconductor devices, nanoelectronics, plasma etching, ferroelectric materials, and spintronics. We have been aware of many physical phenomena of interest, which we have failed to include in the past because, in our opinion at the time, their application prospects were not strong enough. Some of these have now come to the fore and we have included them; they are dielectrophoresis, Raman spectroscopy, thermoelectricity, and pyroelectricity. We believe that one of the most important applications of the electrical properties of materials is in the ﬁeld of memory elements. We have previously described these in the respective chapters, e.g. semiconductor memories in the chapter on semiconductor devices and magnetic memories in the chapter on magnetism. We felt that this time, in order to emphasise their similarities and differences, we needed to collect them into a separate chapter, which has turned out to be an appendix. We have also added another appendix describing the two major directions in medical imaging: computed tomography (CT) and magnetic resonance imaging (MRI). We have to express here our gratitude to our wives who were willing to put up with the long hours we spent bringing this edition up to date.

Contents

Data on specific materials in text Introduction

1

The electron as a particle

1.1 Introduction 1.2 The effect of an electric ﬁeld—conductivity and Ohm’s law 1.3 The hydrodynamic model of electron ﬂow 1.4 The Hall effect 1.5 Electromagnetic waves in solids 1.6 Waves in the presence of an applied magnetic ﬁeld: cyclotron resonance 1.7 Plasma waves 1.8 Johnson noise 1.9 Heat Exercises

2

1 2 4 5 6 13 16 19 21 23

The electron as a wave

2.1 Introduction 2.2 The electron microscope 2.3 Some properties of waves 2.4 Applications to electrons 2.5 Two analogies Exercises

3

xiii xv

25 28 29 31 33 34

The electron

3.1 Introduction 3.2 Schrödinger’s equation 3.3 Solutions of Schrödinger’s equation 3.4 The electron as a wave 3.5 The electron as a particle 3.6 The electron meeting a potential barrier 3.7 Two analogies 3.8 The electron in a potential well 3.9 The potential well with a rigid wall 3.10 The uncertainty relationship 3.11 Philosophical implications Exercises

36 38 39 40 41 41 44 45 47 47 48 50

vi

Contents

4

The hydrogen atom and the periodic table

4.1 The hydrogen atom 4.2 Quantum numbers 4.3 Electron spin and Pauli’s exclusion principle 4.4 The periodic table Exercises

5 5.1 5.2 5.3

Bonds Introduction General mechanical properties of bonds Bond types 5.3.1 5.3.2 5.3.3 5.3.4 5.3.5 5.3.6

Ionic bonds Metallic bonds The covalent bond The van der Waals bond Mixed bonds Carbon again

5.4 Feynman’s coupled mode approach 5.5 Nuclear forces 5.6 The hydrogen molecule 5.7 An analogy Exercises

6

7.1 7.2 7.3 7.4

66 67 69 69 70 70 73 74 74 75 80 81 82 82

The free electron theory of metals

6.1 Free electrons 6.2 The density of states and the Fermi–Dirac distribution 6.3 The speciﬁc heat of electrons 6.4 The work function 6.5 Thermionic emission 6.6 The Schottky effect 6.7 Field emission 6.8 The ﬁeld-emission microscope 6.9 The photoelectric effect 6.10 Quartz–halogen lamps 6.11 The junction between two metals Exercises

7

53 58 59 59 64

84 85 88 89 89 92 95 95 97 97 98 99

The band theory of solids Introduction The Kronig–Penney model The Ziman model The Feynman model

101 102 106 109

Contents 7.5 The effective mass 7.6 The effective number of free electrons 7.7 The number of possible states per band 7.8 Metals and insulators 7.9 Holes 7.10 Divalent metals 7.11 Finite temperatures 7.12 Concluding remarks Exercises

8 8.1 8.2 8.3 8.4 8.5 8.6 8.7 8.8 8.9 8.10

Introduction Intrinsic semiconductors Extrinsic semiconductors Scattering A relationship between electron and hole densities III–V and II–VI compounds Non-equilibrium processes Real semiconductors Amorphous semiconductors Measurement of semiconductor properties Mobility Hall coefﬁcient Effective mass Energy gap Carrier lifetime

Preparation of pure and controlled-impurity single-crystal semiconductors 8.11.1 8.11.2 8.11.3 8.11.4 8.11.5 8.11.6 8.11.7

Crystal growth from the melt Zone reﬁning Modern methods of silicon puriﬁcation Epitaxial growth Molecular beam epitaxy Metal–organic chemical vapour deposition Hydride vapour phase epitaxy (HVPE) for nitride devices

Exercises

9 9.1 9.2 9.3 9.4 9.5 9.6 9.7 9.8 9.9 9.10 9.11

112 114 115 117 117 119 120 121 122

Semiconductors

8.10.1 8.10.2 8.10.3 8.10.4 8.10.5

8.11

vii

123 123 128 132 134 136 140 141 143 143 143 146 146 147 151 151 151 152 154 154 156 156 157 158

Principles of semiconductor devices Introduction The p–n junction in equilibrium Rectiﬁcation Injection Junction capacity The transistor Metal–semiconductor junctions The role of surface states; real metal–semiconductor junctions Metal–insulator–semiconductor junctions The tunnel diode The backward diode

161 161 166 168 170 171 176 178 180 183 186

viii

Contents 9.12

The Zener diode and the avalanche diode 9.12.1 9.12.2

9.13 9.14 9.15 9.16 9.17 9.18 9.19 9.20 9.21 9.22 9.23 9.24 9.25 9.26

Zener breakdown Avalanche breakdown

Varactor diodes Field-effect transistors Heterostructures Charge-coupled devices Silicon controlled rectiﬁer The Gunn effect Strain gauges Measurement of magnetic ﬁeld by the Hall effect Gas sensors Microelectronic circuits Plasma etching Recent techniques for overcoming limitations Building in the third dimension Microelectro-mechanical systems (MEMS) 9.26.1 9.26.2

A movable mirror A mass spectrometer on a chip

9.27 Nanoelectronics 9.28 Social implications Exercises

186 187 187 188 189 194 198 200 201 204 205 205 206 210 212 213 215 215 216 218 222 223

10 Dielectric materials 10.1 10.2 10.3 10.4 10.5 10.6 10.7 10.8 10.9 10.10 10.11 10.12

Introduction Macroscopic approach Microscopic approach Types of polarization The complex dielectric constant and the refractive index Frequency response Anomalous dispersion Polar and non-polar materials The Debye equation The effective ﬁeld Acoustic waves Dielectric breakdown 10.12.1 10.12.2 10.12.3

10.13

Intrinsic breakdown Thermal breakdown Discharge breakdown

Piezoelectricity, pyroelectricity, and ferroelectricity 10.13.1 10.13.2 10.13.3

Piezoelectricity Pyroelectricity Ferroelectrics

10.14 Interaction of optical phonons with drifting electrons 10.15 Optical ﬁbres 10.16 The Xerox process 10.17 Liquid crystals 10.18 Dielectrophoresis Exercises

225 225 226 227 228 229 230 231 233 234 236 240 240 240 241 241 241 247 248 249 250 252 252 254 256

Contents

ix

11 Magnetic materials 11.1 11.2 11.3 11.4 11.5 11.6 11.7

Introduction Macroscopic approach Microscopic theory (phenomenological) Domains and the hysteresis curve Soft magnetic materials Hard magnetic materials (permanent magnets) Microscopic theory (quantum-mechanical) 11.7.1 11.7.2 11.7.3 11.7.4 11.7.5 11.7.6 11.7.7 11.7.8

11.8

Magnetic resonance 11.8.1 11.8.2 11.8.3 11.8.4 11.8.5

11.9 11.10 11.11

Paramagnetic resonance Electron spin resonance Ferromagnetic, antiferromagnetic, and ferrimagnetic resonance Nuclear magnetic resonance Cyclotron resonance

The quantum Hall effect Magnetoresistance Spintronics 11.11.1 11.11.2 11.11.3 11.11.4 11.11.5 11.11.6

11.12

The Stern–Gerlach experiment Paramagnetism Paramagnetic solids Antiferromagnetism Ferromagnetism Ferrimagnetism Garnets Helimagnetism

Spin current Spin tunnelling Spin waves and magnons Spin Hall effect and its inverse Spin and light Spin transfer torque

Some applications 11.12.1 11.12.2 11.12.3 11.12.4

Isolators Sensors Magnetic read-heads Electric motors

Exercises

259 260 260 264 268 270 273 278 278 280 281 281 282 282 282 282 282 283 283 283 284 284 286 287 287 289 290 290 290 291 291 291 292 292 293 293

12 Lasers 12.1 12.2 12.3 12.4 12.5 12.6

Equilibrium Two-state systems Lineshape function Absorption and ampliﬁcation Resonators and conditions of oscillation Some practical laser systems 12.6.1 12.6.2 12.6.3 12.6.4 12.6.5 12.6.6

Solid state lasers The gaseous discharge laser Dye lasers Gas-dynamic lasers Excimer lasers Chemical lasers

295 295 299 301 301 302 303 304 305 306 307 307

x

Contents 12.7

Semiconductor lasers 12.7.1 12.7.2 12.7.3 12.7.4

12.8

Laser modes and control techniques 12.8.1 12.8.2 12.8.3 12.8.4 12.8.5

12.9 12.10 12.11 12.12 12.13

Fundamentals Wells, wires, and dots Bandgap engineering Quantum cascade lasers Transverse modes Axial modes Q switching Cavity dumping Mode locking

Parametric oscillators Optical ﬁbre ampliﬁers Masers Noise Applications 12.13.1 12.13.2 12.13.3 12.13.4 12.13.5 12.13.6 12.13.7 12.13.8 12.13.9 12.13.10 12.13.11 12.13.12 12.13.13 12.13.14 12.13.15 12.13.16 12.13.17 12.13.18 12.13.19

Nonlinear optics Spectroscopy Photochemistry Study of rapid events Plasma diagnostics Plasma heating Acoustics Genetics Metrology Manipulation of atoms by light Optical radar Optical discs Medical applications Machining Sensors Communications Nuclear applications Holography Raman scattering

12.14 The atom laser Exercises

307 307 312 316 318 319 319 320 321 321 321 322 323 324 326 326 327 327 327 328 328 328 328 328 328 328 329 329 329 330 330 331 331 332 334 335 336

13 Optoelectronics 13.1 13.2 13.3 13.4 13.5 13.6 13.7

Introduction Light detectors Light emitting diodes (LEDs) Electro-optic, photorefractive, and nonlinear materials Volume holography and phase conjugation Acousto-optic interaction Integrated optics 13.7.1 13.7.2 13.7.3 13.7.4

13.8 13.9 13.10

Waveguides Phase shifter Directional coupler Filters

Spatial light modulators Nonlinear Fabry–Perot cavities Optical switching

338 339 341 345 346 351 353 354 354 355 357 357 359 362

Contents 13.11

Electro-absorption in quantum well structures 13.11.1 13.11.2 13.11.3 13.11.4

Excitons Excitons in quantum wells Electro-absorption Applications

Exercises

xi 364 364 365 365 367 369

14 Superconductivity 14.1 14.2

Introduction The effect of a magnetic ﬁeld 14.2.1 14.2.2

14.3 14.4 14.5 14.6 14.7 14.8

The critical magnetic ﬁeld The Meissner effect

Microscopic theory Thermodynamical treatment Surface energy The Landau–Ginzburg theory The energy gap Some applications 14.8.1 14.8.2 14.8.3 14.8.4 14.8.5 14.8.6 14.8.7

High-ﬁeld magnets Switches and memory elements Magnetometers Metrology Suspension systems and motors Radiation detectors Heat valves

14.9 High-Tc superconductors 14.10 New superconductors Exercises

371 373 373 374 375 376 381 382 389 393 393 394 394 395 395 395 396 396 401 403

15 Artiﬁcial materials or metamaterials 15.1 15.2 15.3 15.4 15.5 15.6 15.7 15.8 15.9 15.10

Introduction Natural and artiﬁcial materials Photonic bandgap materials Equivalent plasma frequency of a wire medium Resonant elements for metamaterials Polarizability of a current-carrying resonant loop Effective permeability Effect of negative material constants The ‘perfect’ lens Detectors for magnetic resonance imaging

404 405 407 408 410 411 412 414 417 422

Epilogue

424

Appendix I: Organic semiconductors Appendix II: Nobel laureates Appendix III: Physical constants Appendix IV: Variational calculus. Derivation of Euler’s equation Appendix V: Thermoelectricity

427 434 436 438 440

xii

Contents Appendix VI: Principles of the operation of computer memories Appendix VII: Medical imaging Appendix VIII: Suggestions for further reading Answers to exercises

444 463 471 474

Index

477

Data on specific materials in text Errors using inadequate data are much less than using no data at all Charles Babbage

Threshold wavelengths for alkali metals Electrical and thermal conductivities measured at 293 K Figure 4.5 The periodic table of the elements Table 4.1 The electronic conﬁgurations of the elements Table 5.1 Mohs hardness scale (modiﬁed) Table 6.1 Fermi levels of metals Table 6.2 Work functions of metals Figure 6.10 Field-ion micrograph of a tungsten tip Table 8.1 Energy levels of donor (group V) and acceptor (group III) impurities in Ge and Si Figure 8.7 Electron and hole mobilities in Ge and Si as a function of impurity concentration Figure 8.8 Electron and hole mobilities in GaAs as a function of impurity concentration Table 8.2 Size of atoms in tetrahedral bonds Table 8.3 Semiconductor properties I. Energy gap and structure Table 8.4 Semiconductor properties II. Current carriers Figure 8.18 (a) General arrangement of an optical transmission measurement and the result for (b) GaAs and (c) Si Exercise 9.6 Speciﬁc doping data in Ge and Si Table 10.1 Dielectric constant and refractive index of some non-polar, weakly polar, polar, and semiconducting materials Table 10.2 Frequencies of maximum reﬂection ( fr ) and minimum transmission ( ft ) for a number of alkali halides Table 10.3 Piezoelectric ceramics Table 10.4 Pyroelectric coefﬁcients for various materials

Table Table

1.1 1.2

11 22 64 63 72 87 91 96 129 135 137 138 140 145 149

223 232

238

243 247

xiv

Data on speciﬁc materials in text Exercise Figure

10.5 11.9

Table

11.1

Figure

11.12

Table Exercise

11.2 11.6

Figure

12.15

Table Table Table Table

12.1 13.1 13.2 13.3

Table

14.1

Figure

14.9

Figure

14.13

Table

14.2

Figure

14.21

Table

14.3

Figure

14.24

Figure

A1.4

Appendix III

Dielectric loss in thoria Hysteresis loops of (a) Supermalloy and (b) Alnico 5 and 9 Major families of soft magnetic materials with typical properties Hysteresis curves of some rare-earth magnets in the second quadrant Hard magnetic materials Magnetic susceptibility of Ni at varying temperature Relationship between energy gap and lattice spacing for some mixed III–V semiconductors Compounds for laser diodes Electronegativities of elements Properties of electro-optic materials Properties of some materials used for acousto-optic interaction The critical temperature and critical magnetic ﬁeld of a number of superconducting elements Temperature dependence of the speciﬁc heat of tin near the critical temperature (after Keesom and Kok, 1932) The temperature variation of the energy gap (related to the energy gap at T = 0) as a function of T/Tc The critical temperature and critical magnetic ﬁeld (at T = 4.2 K) of the more important hard superconductors The maximum critical temperature against time for traditional and oxide superconductors Approximate critical temperatures (K) of a selection of high-Tc superconductors Critical current densities as a function of magnetic ﬁeld at 77 K (- - -) and at 4.2 K (—) for BSCCO, Nb–Ti, and Nb3 Sn The benzene series, showing optical absorption progressing from the uv to the visible Physical constants

256 269 271 273 273 294 316 316 342 345 352 374 380

389

393

396 397 400

429 436

Introduction Till now man has been up against Nature; from now on he will be up against his own nature. Dennis Gabor Inventing the future It is a good thing for an uneducated man to read books of quotations. W.S. Churchill Roving commission in my early life (1930)

Engineering used to be a down-to-earth profession. The Roman engineers, who provided civilized Europe with bridges and roads, did a job comprehensible to all. And this is still true in most branches of engineering today. Bridge-building has become a sophisticated science, the mathematics of optimum structures is formidable; nevertheless, the basic relationships are not far removed from common sense. A heavier load is more likely to cause a bridge to collapse, and the use of steel instead of wood will improve the load-carrying capacity. Solid state electronic devices are in a different category. In order to understand their behaviour, you need to delve into quantum mechanics. Is quantum mechanics far removed from common sense? Yes, for the time being, it is. We live in a classical world. The phenomena we meet every day are classical phenomena. The ﬁne details represented by quantum mechanics are averaged out; we have no ﬁrst-hand experience of the laws of quantum mechanics; we can only infer the existence of certain relationships from the ﬁnal outcome. Will it always be this way? Not necessarily. There are quantum phenomena known to exist on a macroscopic scale as, for example, superconductivity, and it is quite likely that certain biological processes will be found to represent macroscopic quantum phenomena. So, a ten-year-old might be able to give a summary of the laws of quantum mechanics—half a century hence. For the time being there is no easy way to quantum mechanics; no short cuts and no broad highways. We just have to struggle through. I believe it will be worth the effort. It will be your ﬁrst opportunity to glance behind the scenes, to pierce the surface and ﬁnd the grandiose logic of a hidden world. Should engineers be interested at all in hidden mysteries? Isn’t that the duty and privilege of the physicists? I do not think so. If you want to invent new electronic devices, you must be able to understand the operation of the existing ones. And perhaps you need to more than merely understand the physical mechanism. You need to grow familiar with the world of atoms and electrons, to feel at home among them, to appreciate their habits and characters. We shall not be able to go very deeply into the subject. Time is short, and few of you will have the mathematical apparatus for the frontal assault. So we shall approach the subject in carefully planned steps. First, we shall try to deduce as much information as possible on the basis of the classical picture. Then, we shall talk about a number of phenomena that are clearly in contrast with classical ideas and introduce quantum mechanics, starting with Schrödinger’s equation. You will become acquainted with the properties of individual atoms and what happens when they conglomerate and take the form of

xvi

Introduction a solid. You will hear about conductors, insulators, semiconductors, p–n junctions, transistors, lasers, superconductors, and a number of related solid state devices. Sometimes the statement will be purely qualitative but in most cases we shall try to give the essential quantitative relationships. These lectures will not make you an expert in quantum mechanics nor will they enable you to design a computer the size of a matchbox. They will give you no more than a general idea. If you elect to specialize in solid state devices you will, no doubt, delve more deeply into the intricacies of the theory and into the details of the technology. If you should work in a related subject then, presumably, you will keep alive your interest, and you may occasionally ﬁnd it useful to be able to think in quantum-mechanical terms. If your branch of engineering has nothing to do with quantum mechanics, would you be able to claim in ten years’ time that you proﬁted from this course? I hope the answer to this question is yes. I believe that once you have been exposed (however superﬁcially) to quantum-mechanical reasoning, it will leave permanent marks on you. It will inﬂuence your ideas on the nature of physical laws, on the ultimate accuracy of measurements, and, in general, will sharpen your critical faculties.

The electron as a particle

1

And I laugh to see them whirl and ﬂee, Like a swarm of golden bees. Shelley The Cloud

1.1 Introduction In the popular mind the electron lives as something very small that has something to do with electricity. Studying electromagnetism does not change the picture appreciably. You learn that the electron can be regarded as a negative point charge and it duly obeys the laws of mechanics and electromagnetism. It is a particle that can be accelerated or decelerated but cannot be taken to bits. Is this picture likely to beneﬁt an engineer? Yes, if it helps him to produce a device. Is it a correct picture? Well, an engineer is not concerned with the truth, that is left to philosophers and theologians; the prime concern of an engineer is the utility of the ﬁnal product. If this physical picture makes possible the birth of the vacuum tube, we must deem it useful; but if it fails to account for the properties of the transistor then we must regard its appeal as less alluring. There is no doubt, however, that we can go quite far by regarding the electron as a particle even in a solid—the subject of our study. What does a solid look like? It consists of atoms. This idea originated a few thousand years ago in Greece,∗ and has had some ups and downs in history, but today its truth is universally accepted. Now if matter consists of atoms, they must be somehow piled upon each other. The science that is concerned with the spatial arrangement of atoms is called crystallography. It is a science greatly revered by crystallographers; engineers are respectful, but lack enthusiasm. This is because the need to visualize structures in three dimensions adds to the hard enough task of thinking about what the electron will do next. For this chapter, let us assume that all materials crystallize in the simple cubic structure of Fig. 1.1, with the lattice ions ﬁxed (it is a solid) and some electrons are free to wander between them. This will shortly enable us to explain Ohm’s law, the Hall effect, and several other important events. But if you are sceptical about over simpliﬁcation, look forward to Fig. 5.3 to see how the elemental semiconductors crystallize in the diamond structure, or get a greater shock with Fig. 5.4 which shows a form of carbon that was discovered in meteorites but has only recently been fabricated in laboratories. Let us specify our model a little more closely. If we postulate the existence of a certain number of electrons capable of conducting electricity, we must also say that a corresponding amount of positive charge exists in the solid. It must look electrically neutral to the outside world. Second, in analogy with our picture of gases, we may assume that the electrons bounce around in the

∗ From

‘ατoµoδ’ = indivisible.

Fig. 1.1 Atoms crystallizing in a cubical lattice.

2

The electron as a particle

∗ We

interatomic spaces, colliding occasionally with lattice atoms. We may even go further with this analogy and claim that in equilibrium the electrons follow the same statistical distribution as gas molecules (that is, the Maxwell–Boltzmann distribution) which depends strongly on the temperature of the system. The average kinetic energy of each degree of freedom is then 21 kB T where T is absolute temperature and kB is Boltzmann’s constant. So we may say that the mean thermal velocity of electrons is given by the formula∗

shall see later that this is not so for metals but it is nearly true for conduction electrons in semiconductors.

vth is the thermal velocity, and m is the mass of the electron.

2 1 2 mvth

= 23 kB T

(1.1)

because particles moving in three dimensions have three degrees of freedom. We shall now calculate some observable quantities on the basis of this simplest model and see how the results compare with experiment. The success of this simple model is somewhat surprising, but we shall see as we proceed that viewing a solid, or at least a metal, as a ﬁxed lattice of positive ions held together by a jelly-like mass of electrons approximates well to the modern view of the electronic structure of solids. Some books discuss mechanical properties in terms of dislocations that can move and spread; the solid is then pictured as a ﬁxed distribution of negative charge in which the lattice ions can move. These views are almost identical; only the external stimuli are different.

1.2

The effect of an electric ﬁeld—conductivity and Ohm’s law

Suppose a potential difference U is applied between the two ends of a solid length L. Then an electric ﬁeld E =

U L

(1.2)

is present at every point in the solid, causing an acceleration a=

e E. m

(1.3)

Thus, the electrons, in addition to their random velocities, will acquire a velocity in the direction of the electric ﬁeld. We may assume that this directed velocity is completely lost after each collision, because an electron is much lighter than a lattice atom. Thus, only the part of this velocity that is picked up in between collisions counts. If we write τ for the average time between two collisions, the ﬁnal velocity of the electron will be aτ and the average velocity vaverage = 12 aτ .

† See, for example, W. Shockley, Electrons and holes in semiconductors, D. van Nostrand, New York, 1950, pp. 191–5.

(1.4)

This is simple enough but not quite correct. We should not use the average time between collisions to calculate the average velocity but the actual times and then the average. The correct derivation is fairly lengthy, but all it gives is a factor of 2.† Numerical factors like 2 or 3 or π are generally not worth worrying about in simple models, but just to agree with the formulae generally quoted in the literature, we shall incorporate that factor 2, and use vaverage = aτ .

(1.5)

The effect of an electric ﬁeld—conductivity and Ohm’s law

3

The average time between collisions, τ , has many other names; for example, mean free time, relaxation time, and collision time. Similarly, the average velocity is often referred to as the mean velocity or drift velocity. We shall call them ‘collision time’ and ‘drift velocity’, denoting the latter by vD . The relationship between drift velocity and electric ﬁeld may be obtained from eqns (1.3) and (1.5), yielding e τ E, (1.6) vD = m

where the proportionality constant in parentheses is called the ‘mobility’. This is the only name it has, and it is quite a logical one. Assuming now that all electrons drift with their drift velocity, the total number of electrons crossing a plane of unit area per second may be obtained by multiplying the drift velocity by the density of electrons, Ne . Multiplying further by the charge on the electron we obtain the electric current density J = Ne evD .

(1.7)

Notice that it is only the drift velocity, created by the electric ﬁeld, that comes into the expression. The random velocities do not contribute to the electric current because they average out to zero.∗ We can derive similarly the relationship between current density and electric ﬁeld from eqns (1.6) and (1.7) in the form J=

Ne e2 τ E. m

The higher the mobility, the more mobile the electrons.

(1.8)

∗ They give rise, however, to electrical noise in a conductor. Its value is usually much smaller than the signals we are concerned with so we shall not worry about it, although some of the most interesting engineering problems arise just when signal and noise are comparable. see Section 1.8 on noise.

This is a linear relationship which you may recognize as Ohm’s law J = σE ,

(1.9)

where σ is the electrical conductivity. When ﬁrst learning about electricity you looked upon σ as a bulk constant; now you can see what it comprises of. We can write it in the form e τ (Ne e) m = μe (Ne e).

σ =

(1.10)

That is, we may regard conductivity as the product of two factors, charge density (Ne e) and mobility (μe ). Thus, we may have high conductivities because there are lots of electrons around or because they can acquire high drift velocities, by having high mobilities. Ohm’s law further implies that σ is a constant, which means that τ must be independent of electric ﬁeld.† From our model so far it is more reasonable to assume that l, the distance between collisions (usually called the mean free path) in the regularly spaced lattice, rather than τ , is independent of electric ﬁeld. But l must be related to τ by the relationship, l = τ (vth + vD ).

(1.11)

In metals, incidentally, the mobilities are quite low, about two orders of magnitude below those of semiconductors; so their high conductivity is due to the high density of electrons.

† It

seems reasonable at this stage to assume that the charge and mass of the electron and the number of electrons present will be independent of the electric ﬁeld.

4

The electron as a particle Since vD varies with electric ﬁeld, τ must also vary with the ﬁeld unless vth ≫ vD .

In a typical metal μe = 5 × 10–3 m2 V–1 s–1 , which gives a drift velocity vD of 5 × 10–3 m s–1 for an electric ﬁeld of 1 V m–1 .

∗ This

is less true for semiconductors as they violate Ohm’s law at high electric ﬁelds.

vx

vth

vx vy

Fig. 1.2 Distributions of electrons in velocity space.

As Ohm’s law is accurately true for most metals, this inequality should hold. The thermal velocity at room temperature according to eqn (1.1) (which actually gives too low a value for metals) is 3kB T 1/2 ~ 5 vth = (1.13) = 10 m s–1 . m Thus, there will be a constant relationship between current and electric ﬁeld accurate to about 1 part in 108 .∗ This important consideration can be emphasized in another way. Let us draw the graph (Fig. 1.2) of the distribution of particles in velocity space, that is with rectilinear axes representing velocities in three dimensions, vx , vy , vz . With no electric ﬁeld present, the distribution is spherically symmetric about the origin. The surface of a sphere of radius vth represents all electrons moving in all possible directions with that r.m.s. speed. When a ﬁeld is applied along the x-axis (say), the distribution is minutely perturbed (the electrons acquire some additional velocity in the direction of the x-axis) so that its centre shifts from (0, 0, 0) to about (vth /108 , 0, 0). Taking copper, a ﬁeld of 1 V m–1 causes a current density of 108 A m–2 . It is quite remarkable that a current density of this magnitude can be achieved with an almost negligible perturbation of the electron velocity distribution.

1.3

The hydrodynamic model of electron ﬂow

By considering the ﬂow of a charged ﬂuid, a sophisticated model may be developed. We shall use it only in its crudest form, which does not give much of a physical picture but leads quickly to the desired result. The equation of motion for an electron is m

ζ may be regarded here as a measure of the viscosity of the medium.

(1.12)

dv = eE . dt

(1.14)

If we now assume that the electron moves in a viscous medium, then the forces trying to change the momentum will be resisted. We may account for this by adding a ‘momentum-destroying’ term, proportional to v. Taking the proportionality constant as ζ eqn (1.14) modiﬁes to dv + ζ v = eE . (1.15) m dt In the limit, when viscosity dominates, the term dv/dt becomes negligible, resulting in the equation mvζ = eE ,

(1.16)

which gives for the velocity of the electron v=

e 1 E. mζ

(1.17)

The Hall effect

5

It may be clearly seen that by taking ζ = 1/τ eqn (1.17) agrees with eqn (1.6); hence we may regard the two models as equivalent and, in any given case, use whichever is more convenient.

1.4 The Hall effect Let us now investigate the current ﬂow in a rectangular piece of material, as shown in Fig. 1.3. We apply a voltage so that the right-hand side is positive. Current, by convention, ﬂows from the positive side to the negative side, that is in the direction of the negative z-axis. But electrons, remember, ﬂow in a direction opposite to conventional current, that is from left to right. Having sorted this out let us now apply a magnetic ﬁeld in the positive y-direction. The force on an electron due to this magnetic ﬁeld is (1.18)

e(v × B).

To get the resultant vector, we rotate vector v into vector B. This is a clockwise rotation, giving a vector in the negative x-direction. But the charge of the electron, e, is negative; so the force will point in the positive x-direction; the electrons are deﬂected upwards. They cannot move farther than the top end of the slab, and they will accumulate there. But if the material was electrically neutral before, and some electrons have moved upwards, then some positive ions at the bottom will be deprived of their compensating negative charge. Hence an electric ﬁeld will develop between the positive bottom layer and the negative top layer. Thus, after a while, the upward motion of the electrons will be prevented by this internal electric ﬁeld. This happens when EH = vB.

Equilibrium is established when the force due to the transverse electric ﬁeld just cancels the force due to the magnetic ﬁeld.

(1.19)

Expressed in terms of current density,

RH is called the Hall coefﬁcient.

EH = RH JB,

RH =

1 . Ne e

(1.20)

Voltmeter

In this experiment EH , J , and B are measurable; thus RH , and with it the density of electrons, may be determined.

Electrons

•

B

I

x

z

+ + + + + + + + + + + J y +

Fig. 1.3 Schematic representation of the measurement of the Hall effect.

B

6

The corresponding electric ﬁeld in a semiconductor is considerably higher because of the higher mobilities.

The electron as a particle What can we say about the direction of EH ? Well, we have taken meticulous care to ﬁnd the correct direction. Once the polarity of the applied voltage and the direction of the magnetic ﬁeld are chosen, the electric ﬁeld is well and truly deﬁned. So if we put into our measuring apparatus one conductor after the other, the measured transverse voltage should always have the same polarity. Yes . . . the logic seems unassailable. Unfortunately, the experimental facts do not conform. For some conductors and semiconductors the measured transverse voltage is in the other direction. How could we account for the different sign? One possible way of explaining the phenomenon is to say that in certain conductors (and semiconductors) electricity is carried by positively charged particles. Where do they come from? We shall discuss this problem in more detail some time later; for the moment just accept that mobile positive particles may exist in a solid. They bear the unpretentious name ‘holes’. To incorporate holes in our model is not at all difﬁcult. There are now two species of charge carriers bouncing around, which you may imagine as a mixture of two gases. Take good care that the net charge density is zero, and the new model is ready. It is actually quite a good model. Whenever you come across a new phenomenon, try this model ﬁrst. It might work. Returning to the Hall effect, you may now appreciate that the experimental determination of RH is of considerable importance. If only one type of carrier is present, the measurement will give us immediately the sign and the density of the carrier. If both carriers are simultaneously present it still gives useful information but the physics is a little more complicated (see Exercises 1.7 and 1.8). In our previous example we took a typical metal where conduction takes place by electrons only, and we got a drift velocity of 5 × 10–3 m s–1 . For a magnetic ﬁeld of 1 T the transverse electric ﬁeld is EH = Bv = 5 × 10–3 V m–1 .

1.5

(1.21)

Electromagnetic waves in solids

So far as the propagation of electromagnetic waves is concerned, our model works very well indeed. All we need to assume is that our holes and electrons obey the equations of motion, and when they move, they give rise to ﬁelds in accordance with Maxwell’s theory of electrodynamics. It is perfectly simple to take holes into account, but the equations, with holes included, would be considerably longer, so we shall conﬁne our attention to electrons. We could start immediately with the equation of motion for electrons, but let us ﬁrst review what you already know about wave propagation in a medium characterized by the constants permeability, μ, dielectric constant, ǫ, and conductivity, σ (it will not be a waste of time). First of all we shall need Maxwell’s equations: E ∂E 1 ∇×B=J+ǫ , μ ∂t ∂B ∇ ×E = – . ∂t

(1.22) (1.23)

Electromagnetic waves in solids

7

Second, we shall express the current density in terms of the electric ﬁeld as E. J = σE

(1.24)

It would now be a little more elegant to perform all the calculations in vector form, but then you would need to know a few vector identities, and tensors (quite simple ones, actually) would also appear. If we use coordinates instead, it will make the treatment a little lengthier, but not too clumsy if we consider only the one-dimensional case, when ∂ = 0, ∂x

∂ = 0. ∂y

(1.25)

Assuming that the electric ﬁeld has only a component in the x-direction (see the coordinate system in Fig. 1.3), then ex ey ez ∂ ∂Ex = ∇ ×E = 0 0 ey , ∂z ∂z Ex 0 0

(1.26)

where ex , ey , ez are the unit vectors. It may be seen from this equation that the magnetic ﬁeld can have only a y-component. Thus, eqn (1.23) takes the simple form ∂By ∂Ex =– . ∂z ∂t

(1.27)

We need further ex ey ez ∂ ∂By = ∇ × B = 0 0 ex , ∂z ∂z 0 By 0

∗ We

(1.28)

which, combined with eqn (1.24), brings eqn (1.22) to the scalar form –

∂By ∂Ex = μσ Ex + μǫ . ∂z ∂t

(1.29)

Thus, we have two fairly simple differential equations to solve. We shall attempt the solution in the form∗ Ex = Ex0 exp {–i(ωt – kz)}

(1.30)

By = By0 exp {–i(ωt – kz)} .

(1.31)

and

have here come face to face with a dispute that has raged between physicists and engineers for ages. For some odd reason the physicists (aided and abetted by√mathematicians) use the symbol i for –1 and the exponent –i(ωt – kz) to describe a wave travelling in the zdirection. The engineers’ notation is j for √ –1 and j(ωt – kz) for the exponent. In this course we have, rather reluctantly, accepted the physicists’ notations so as not to confuse you further when reading books on quantum mechanics.

ω represents frequency, and k is the wavenumber.

8

The electron as a particle Then, ∂ ≡ ik, ∂z

∂ ≡ –iω, ∂t

(1.32)

which reduces our differential equations to the algebraic equations ikEx = iωBy

(1.33)

–ikBy = (μσ – iωμǫ)Ex .

(1.34)

and

This is a homogeneous equation system. By the rules of algebra, there is a solution, apart from the trivial Ex = By = 0, only if the determinant of the coefﬁcients vanishes, that is –ik iω μσ – iωμǫ ik = 0.

(1.35)

Expanding the determinant we get Different people call this equation by different names. Characteristic, determinantal, and dispersion equation are among the names more frequently used. We shall call it the dispersion equation because that name describes best what is happening physically. cm c is the velocity of the electromagnetic wave in the medium.

k 2 – iω(μσ – iωμǫ) = 0.

(1.36)

Essentially, the equation gives a relationship between the frequency, ω, and the wavenumber, k, which is related to phase velocity by vP = ω/k. Thus, unless ω and k are linearly related, the various frequencies propagate with different velocities and at the boundary of two media are refracted at different angles. Hence the name dispersion. A medium for which σ = 0 and μ and ǫ are independent of frequency is nondispersive. The relationship between k and ω is simply ω √ k = ω μǫ = . cm

(1.37)

Solving eqn (1.36) formally, we get ∗ The

negative sign is also permissible though it does not give rise to an exponentially increasing wave as would follow from eqn (1.39). It would be very nice to make an ampliﬁer by putting a piece of lossy material in the way of the electromagnetic wave. Unfortunately, it violates the principle of conservation of energy. Without some source of energy at its disposal no wave can grow. So the wave which seems to be exponentially growing is in effect a decaying wave which travels in the direction of the negative z-axis.

k = (ω2 μǫ + iωμσ )1/2 .

(1.38)

Thus, whenever σ = 0, the wavenumber is complex. What is meant by a complex wavenumber? We can ﬁnd this out easily by looking at the exponent of eqn (1.30). The spatially varying part is exp(ikz) = exp i(kreal + ikimag )z

= exp(ikreal z) exp(–kimag z).

(1.39)

Hence, if the imaginary part of k is positive, the amplitude of the electromagnetic wave declines exponentially.∗

Electromagnetic waves in solids

9

If the conductivity is large enough, the second term is the dominant one in eqn (1.38) and we may write ~ (iωμσ )1/2 = ±(i√+ 1) (ωμσ )1/2 . k= 2

(1.40)

So if we wish to know how rapidly an electromagnetic wave decays in a good conductor, we may ﬁnd out from this expression. Since kimag =

ωμσ 1/2 2

the amplitude of the electric ﬁeld varies as

ωμσ 1/2 z . |Ex | = Ex0 exp – 2

(1.41)

(1.42)

The distance δ at which the amplitude decays to 1/e of its value at the surface is called the skin depth and may be obtained from the equation 1=

ωμσ 1/2

δ=

yielding

2

2 ωμσ

δ,

1/2

.

(1.43)

(1.44)

You have seen this formula before. You need it often to work out the resistance of wires at high frequencies. I derived it solely to emphasize the major steps that are common to all these calculations. We can now go further, and instead of taking the constant σ , we shall look a little more critically at the mechanism of conduction. We express the current density in terms of velocity by the equation J = Ne ev.

(1.45)

This is really the same thing as eqn (1.7). The velocity of the electron is related to the electric and magnetic ﬁelds by the equation of motion dv v E + v × B). m = e(E (1.46) + dt τ We are looking for linearized solutions leading to waves. In that approximation the quadratic term v × B can clearly be neglected and the total derivative can be replaced by the partial derivative to yield ∂v v E. = eE (1.47) + m ∂t τ Assuming again that the electric ﬁeld is in the x-direction, eqn (1.47) tells us that the electron velocity must be in the same direction. Using the rules set

The symbol v still means the average velocity of electrons, but now it may be a function of space and time, whereas the notation vD is generally restricted to d.c. phenomena. 1/τ is introduced again as a ‘viscous’ or ‘damping’ term.

10

The electron as a particle out in eqn (1.32) we get the following algebraic equation 1 mvx –iω + = eEx . τ

(1.48)

The current density is then also in the x-direction: Jx = Ne evx 1 Ne e2 τ Ex m 1 – iωτ σ Ex , = 1 – iωτ =

(1.49)

where σ is deﬁned as before. You may notice now that the only difference from our previous (J – E ) relationship is a factor (1 – iωτ ) in the denominator. Accordingly, the whole derivation leading to the expression of k in eqn (1.38) remains valid if σ is replaced by σ/(1 – iωτ ). We get σ 1/2 k = ω2 μǫ + iωμ 1 – iωτ 1/2 iσ . = ω(μǫ)1/2 1 + ωǫ(1 – iωτ

(1.50)

If ωτ ≪ 1, we are back where we started from, but what happens when ωτ ≫ 1? Could that happen at all? Yes, it can happen if the signal frequency is high enough or the collision time is long enough. Then, unity is negligible in comparison with iωτ in eqn (1.50), leading to k = ω(μǫ)1/2 1 –

σ 1/2

.

(1.51)

σ Ne e2 (Ne e2 /m)τ = = mǫ ǫτ ǫτ

(1.52)

ω2 ǫτ

Introducing the new notation ωp2 ≡ Equation (1.53) suggests a generalization of the concept of the dielectric constant. We may introduce an effective relative dielectric constant by the relationship εeff = 1 –

ωp2 ω

. 2

It may now be seen that, depending on frequency, εeff may be positive or negative.

we get

k = ω(μǫ)

1/2

1–

ωp2 ω2

1/2

.

(1.53)

Hence, as long as ω > ωp , the wavenumber is real. If it is real, it has (by the rules of the game) no imaginary component; so the wave is not attenuated. This is quite unexpected. By introducing a slight modiﬁcation into our model, we may come to radically different conclusions. Assuming previously J = σ E , we worked out that if any electrons are present at all, the wave is bound to decay. Now we are saying that for sufﬁciently large ωτ an electromagnetic wave may travel across our conductor without attenuation. Is this possible? It seems to contradict the empirical fact that radio waves cannot penetrate metals. True;

Electromagnetic waves in solids but that is because radio waves have not got high enough frequencies; let us try light waves. Can they penetrate a metal? No, they can not. It is another empirical fact that metals are not transparent. So we should try even higher frequencies. How high? Well, there is no need to go on guessing, we can work out the threshold frequency from eqn (1.52). Taking the electron density in a typical metal as 6 × 1028 per m3 , we then get 1/2 Ne e2 mǫ0

1/2 6 × 1028 (1.6 × 10–19 )2 1 = 2π 9.11 × 10–31 × 8.85 × 10–12

fp =

1 π

= 2.2 × 1015 Hz,

(1.54)

where ε0 is the free-space permittivity. At this frequency range you are probably more familiar with the wavelengths of electromagnetic waves. Converting the above calculated frequency into wavelength, we get λ=

3 × 108 c = = 136 nm, fp 2.2 × 1015

(1.55)

where c is the velocity of light. Thus, the threshold wavelength is well below the edge of the visible region (400 nm). It is gratifying to note that our theory is in agreement with our everyday experience; metals are not transparent. There is one more thing we need to check. Is the condition ωτ ≫ 1 satisﬁed? For a typical metal at room temperature, the value of τ is usually above 10–14 s, making ωτ of the order of hundreds at the threshold frequency. By making transmission experiments through a thin sheet of metal, the critical wavelength can be determined. The measured and calculated values are compared in Table 1.1. The agreement is not too bad, considering how simple our model is. Before going further I would like to say a little about the relationship of transmission, reﬂection, and absorption to each other. The concepts are simple and one can always invoke the principle of conservation of energy if in trouble. Table 1.1 Threshold wavelengths for alkali metals Metal

Observed wavelength (nm)

Calculated wavelength (nm)

Cs Rb K Na Li

440 360 315 210 205

360 320 290 210 150

11

12

The electron as a particle Medium 1

Medium 2

Vacuum

Conductor

Incident wave Transmitted wave

Incident electromagnetic wave partly reﬂected and partly transmitted.

ωτ

ωp

Medium 1

Medium 2

Vacuum

Conductor

Incident wave No transmitted wave

ωτ

Fig. 1.5

ωp

Let us take the case when ω τ ≫ 1; k is given by eqn (1.53), and our conductor ﬁlls half the space, as shown in Fig. 1.4. What happens when an electromagnetic wave is incident from the left? 1. ω > ωp . The electromagnetic wave propagates in the conductor. There is also some reﬂection, depending on the amount of mismatch. Energy conservation says energy in the incident wave = energy in the transmitted wave + energy in the reﬂected wave. Is there any absorption? No, because ωτ ≫ 1.

If there is a smaller amplitude transmitted, there will be a larger amplitude reﬂected.

2. ω < ωp . In this case k is purely imaginary; the electromagnetic wave decays exponentially. Is there any absorption? No. Can the electromagnetic wave decay then? Yes, it can. Is this not in contradiction with something or other? The correct answer may be obtained by writing out the energy balance. Since the wave decays and the conductor is inﬁnitely long, no energy goes out at the right-hand side. So everything must go back. The electromagnetic wave is reﬂected, as shown in Fig. 1.5. The energy balance is energy in the incident wave = energy in the reﬂected wave. 3. Let us take now the case shown in Fig. 1.6 when our conductor is of ﬁnite dimension in the z-direction. What happens if ω < ωp ? The wave has a chance to get out at the other side, so there is a ﬂow of energy, forwards and backwards, in the conductor. The wider the slab, the smaller is the amplitude of the wave that appears at the other side because the amplitude decays exponentially in the conductor. There is decay, but no absorption. The amplitudes of the reﬂected and transmitted waves rearrange themselves in such a way as to conserve energy. If we choose a frequency such that ωτ ≪ 1, then, of course, dissipative processes do occur and some of the energy of the electromagnetic wave is

Waves in the presence of an applied magnetic ﬁeld: cyclotron resonance Medium 1

Medium 2

Medium 3

Vacuum

Conductor

Vacuum

Incident wave

Forward travelling wave

Transmitted wave

Fig. 1.6 Incident electromagnetic wave transmitted to medium 3. The amplitude of the wave decays in medium 2 but without any energy absorption taking place.

Backward

Reflected wave

travelling wave 1

ω

>

1 condition necessary? Well, τ is the collision time; τ = 1/ωc means that the electron collides with a lattice atom after going round one radian. Clearly, if the electron is exposed to the electric ﬁeld for a considerably shorter time than a cycle, not much absorption can take place. The limit might be ωc τ = 1. Now we may again ask the question: what is cyclotron resonance good for? There have been suggestions for making ampliﬁers and oscillators with the

Notice that any increase in speed must come from the electric ﬁeld; the acceleration produced by a magnetic ﬁeld changes direction, not speed, since the force is always at right angles to the direction of motion. This is the basis of Fourier transform ion cyclotron mass spectrometry (FT–ICR–MS).

16

The electron as a particle aid of cyclotron resonance, where by clever means the sign of attenuation is reversed, turning it into gain. As far as I know none of these devices reached the ultimate glory of commercial exploitation. If cyclotron resonance is no good for devices, is it good for something else? Yes, it is an excellent measurement tool. It is used as follows: we take a sample, put it in a waveguide and launch an electromagnetic wave of frequency, ω. Then we apply a magnetic ﬁeld and measure the amplitude of the output electromagnetic wave while the strength of magnetic ﬁeld is varied. When the output is a minimum, the condition of cyclotron resonance is satisﬁed. We know ω so we know ωc ; we know the value of the magnetic ﬁeld, B0 so we can work out the mass of the electron from the formula m=

∗ The actual value is called, quite reason-

ably, the effective mass.

The charge of the electron is a fundamental constant in a solid; the mass of an electron is not.

eB0 . ω

(1.64)

But, you would say, what is the point in working out the mass of the electron? That’s a fundamental constant, isn’t it? Well, it is, but not in the present context. When we put our electron in a crystal lattice, its mass will appear to be different. The actual∗ value can be measured directly with the aid of cyclotron resonance. So once more, under the pressure of experimental results we have to modify our model. The bouncing billiard balls have variable mass. Luckily, the charge of the electron does remain a fundamental constant. We must be grateful for small favours.

1.7

Plasma waves

Electromagnetic waves are not the only type of waves that can propagate in a solid. The most prominent ones are sound waves and plasma waves. We know about sound waves; but what are plasma waves? In their simplest form they are density waves of charged particles in an electrically neutral medium. So they exist in a solid that has some mobile carriers. The main difference between this case and the previously considered electromagnetic case is that now we permit the accumulation of space charge. At a certain point in space, the local density of electrons may exceed the local density of positive carriers. Then an electric ﬁeld arises, owing to the repulsive forces between these ‘unneutralized’ electrons. The electric ﬁeld tries to restore the equilibrium of positive and negative charges. It drives the electrons away from the regions where they accumulated. The result is, of course, that the electrons overshoot the mark, and some time later, there will be a deﬁciency of electrons in the same region. An opposite electric ﬁeld is then created which tries to draw back the electrons, etc. This is the usual case of harmonic oscillation. Thus, as far as an individual electron is concerned, it performs simple harmonic motion. If we consider a one-dimensional model again, where everything is the same in the transverse plane, then the resulting electric ﬁeld has a longitudinal comE is worked out, will convince ponent only. A glance at eqn (1.26), where ∇×E E = 0, that is you that if the electric ﬁeld has a z-component, only then ∇×E B = 0. There is no magnetic ﬁeld present; the interplay is solely between the charges and the electric ﬁeld. For this reason these density waves are often referred to as electrostatic waves.

Plasma waves

17

If B = 0, then eqn (1.22) takes the simple form J+ǫ

E ∂E = 0. ∂t

(1.65)

We need the equation of motion, which for longitudinal motion will have exactly the same form as for transverse motion, namely m

∂v E, = eE ∂t

(1.66) ∗ Ignoring

losses will considerably restrict the applicability of the formulae derived, but our aim here is to show no more than the simplest possible case.

mv/τ .∗

where we have neglected the damping term Current density and velocity are related again by J = Ne0 ev.

(1.67)

Ne0 is the equilibrium density of electrons.

We have changed over to scalar quantities. Substituting E from eqn (1.66) and J from eqn (1.67) into (1.65), we obtain Ne0 ev +

ǫm ∂ 2 v = 0. e ∂t2

(1.68)

Following again our favourite method of replacing ∂/∂t by –iω, eqn (1.69) reduces to ǫm (–ω2 ) = 0. (1.69) v Ne0 e + e Since v must be ﬁnite, this means Ne0 e –

ǫm 2 ω = 0, e

(1.70)

v

(b) Light line

or, rearranging, ω2 =

Ne0 e2 . mǫ

(1.71)

vp

This is our dispersion equation. It is a rather odd one because k does not appear in it. A relationship between k and ω gives the allowed values of k for a given ω. If k does not appear in the dispersion equation, all values of k are allowed. On the other hand, there is only a single value of ω allowed. Looking at it more carefully, we may recognize that it is nothing else but ωp , the frequency we met previously as the critical frequency of transparency for electromagnetic waves. Historically, it was ﬁrst discovered in plasma oscillations (in gas discharges by Langmuir); so it is more usual to call it the ‘plasma frequency’, and that is where the subscript p comes from. The dispersion curve given by eqn (1.71) is just a straight horizontal line, as shown in Fig. 1.8. The dispersion curve of the electromagnetic wave corresponding to eqn (1.53) may also be seen in the same ﬁgure. As explained before, in the latter case there is no propagation unless the frequency is above the plasma frequency. For high enough frequencies the dispersion curve tends

vp √2

(a)

(c)

k

Fig. 1.8 Dispersion curves of plasma waves. (a) Plasma density wave, (b) bulk plasma wave or bulk plasmon polariton, (c) surface plasma wave or surface plasmon polariton. The equation of the light line is ω = kc.

18

The electron as a particle

Metal

Air

Amplitude

Fig. 1.9 A surface wave may exist at a metal–air boundary. The amplitude of the wave is highest at the surface, from where it declines exponentially in both directions.

to the light line, i.e. its velocity tends to the velocity of light. The wave is of course not a pure electromagnetic wave, which would always propagate with the velocity of light. It is a combination of a plasma wave and an electromagnetic wave. One might call it a hybrid wave. In fact the modern term is much more pompous. It is called a bulk plasma wave or, even worse, a bulk plasmon polariton. The word ‘polariton’ is attached to it to signify that it is a hybrid wave. But why a bulk plasmon polariton? Because there is another variety as well, called a surface plasma wave or surface plasmon polariton. Such a wave, needless to say, is called a surface wave because it sticks to a surface. What kind of surface? The best example of such a wave, and the one relevant here, is a wave at the interface of a metal and a dielectric, say air. If the wave sticks to the surface, its amplitude must decline in both directions, both in the metal and in air, as shown schematically in Fig. 1.9. One could say that it is the electric ﬁeld that acts as the glue, sticking to charges in the metal as illustrated in Fig. 1.10. We shall not derive the dispersion equation here. It is a fairly long derivation. We just give here the equation itself, which is quite simple:

k = ω(ε0 μ0 )1/2

εeff 1 + εeff

1/2

,

(1.72)

where μ0 = 4π × 10–7 H m–1 is the free-space permeability and (ε0 μ0 )–1/2 = c.

(1.73)

For propagation, k must be real. This occurs when εeff < –1.

(1.74)

Conveniently, as discussed in the previous section, the effective dielectric constant of a metal is negative below the plasma frequency. The limit is when εeff = –1. Below this frequency (see eqn (1.53)), εeff declines further so that eqn (1.72) always yields a real value and, consequently, a surface wave can always exist. Substituting eqn (1.53) into (1.72), we ﬁnd the dispersion equation. The corresponding dispersion curve is shown in Fig. 1.8. The wave is what one calls a slow wave since it is to the right of the light line, having a phase velocity always below that of light.

Metal

.H

Fig. 1.10 Electric ﬁeld lines for a surface plasma wave in the vicinity of a metal–air boundary.

E

Dielectric

Johnson noise This is for one boundary. If there are two boundaries, each one of them will have a surface wave. For a thick metal slab, the two surface waves do not know about each other. However, for a thin∗ slab the two surface waves interact. Curve (c) in Fig. 1.8 splits into two branches, as may be seen in Fig. 1.11. It may be shown that for the upper mode, less power is carried in the metal than in the air. Since electron motion in the metal is responsible for losses, the mode which propagates more in the air is less lossy. This mode is called a long-range surface plasmon. How long is ‘long-range’? Not very long. At optical frequencies, ‘long-range’ may mean 20 mm at best. On the other hand, with modern techniques, one can have a large number of various devices within 20 mm.

19

∗ ‘Thin’

really means thin. At a wavelength of 360 nm the slab must be thinner than 50 nm.

v Light line vp

1.8 Johnson noise

(b)

The electrons have so far behaved very reasonably. When no force acted upon them they stayed put. Under the effect of a force they moved. They obeyed Newton’s law without qualm or hesitation. Unfortunately, this is not the whole truth. I may quote a very sophisticated and most profound theorem of physics the so-called ﬂuctuation–dissipation theorem, which tells us that whenever there is dissipation there will be ﬂuctuation as well. As we have already discussed there is bound to be dissipation. It occurs when an electron bumps into a lattice atom. So there must also be ﬂuctuation. There is no such thing as an electron waiting patiently for some force to turn up and then it moves; they are moving all the time. It makes good sense that when the temperature is ﬁnite the electrons will jiggle. They will move a little bit to the left, a little bit to the right, in fact a little bit in any conceivable direction. Is that good or bad? Deﬁnitely bad. For our communications we rely on electronic signals. If the jiggling of the electrons interferes with that it’s bad. The situation is the same as in direct verbal communications. If there is nearby some source of unrequited sound waves (say a workshop where they repair motorcycles) then the clarity of those verbal communications may suffer considerably. When we rely on sound waves then we refer to the undesirable sound waves as noise. As a generalization of this concept we may always refer to an undesirable interfering agent as noise whatever the useful signal is. For example if we gaze at the stars, then the random motion of the constituents of air can be regarded as the source of noise that will make our star twinkle. When it comes to electronic signals, then the noise is due to the random motion of electrons. Resistors contain electrons hence they are a source of noise. The ﬁrst to investigate this effect was John B. Johnson, at Bell Labs in 1928. Johnson carried out a careful set of experiments using resistors of different values held at different temperatures, and a measurement system containing a band-pass ﬁlter. His results showed that any resistor generates a random series voltage whose power spectral density is ﬂat, at least at low frequencies, and proportional to both the resistance and the absolute temperature. Almost immediately, his colleague Harry Nyquist provided a theoretical explanation. We will avoid a detailed derivation and simply state the standard expression for what is now known as Johnson noise. The root mean square (r.m.s.) voltage generated by a resistance R at an absolute temperature T is = 4kB TRdf .

(1.75)

vp √2 (c)

(a) 0

Fig. 1.11 Dispersion curves: (a) for a single metal–air boundary [same as curve (c) in Fig. 1.8]; (b), (c) for a thin metal slab in air.

k

20

The electron as a particle Here df is the measurement bandwidth, sometimes written as B. An analogous expression exists for noise generated √ At room√temperature √ as a shunt current. (300 K) this result implies that = 0.129 R √ nV per Hz. For example, for a 1 M resistor and a 10 kHz bandwidth, = 12.9 µV. That gives you an idea. The main point is that there is no getting away from noise. All electrical sources have an output resistance. Consequently, while they may generate a signal (which we want) they will also generate noise (which we don’t want). As a result, the perfect signal is an idealization, although a convenient one. More realistic signals must be described in terms of a signal-to-noise ratio or SNR, deﬁned as the signal power divided by the noise power. For a sinusoidal signal with r.m.s. voltage VS , the SNR is clearly VS2 /. If the SNR is too low (which occurs at about unity), it will be difﬁcult to distinguish the signal from noise. As a result, SNR will in the end set a limit to the signals that can be measured and the distances over which they can be transmitted. There is not much we can do to improve the situation. There is no way of subtracting away the noise, since it is generated randomly. Additional circuitry will make matters worse, because it will contain some conductive elements. We can illustrate this using the simple circuits shown below. Figure 1.12(a) shows a source with r.m.s. voltage and output impedance RS connected to a load RL . We know from the maximum power theorem that the best way to transfer the signal power to the load resistor is to take RS = RL , so we will assume this directly. The r.m.s. current in the circuit is then IS = VS /2RL , so the signal power dissipated in the load is PS = IS2 RL = VS2 /4RL . For SNR calculations, we should include a noise voltage VnS in the circuit, as shown in Fig. 1.12(b). Similar reasoning suggests that the noise power 2 /4R . However, we already know that delivered to the load is PnS = VnS L 2 the average value of VnS is 4kB TRL df , so the noise power in this optimum case (known as the available noise power) is PnS = kB Tdf . This result is entirely independent of the resistor values, suggesting that temperature and thermal energy are the important factors. The SNR at the load is PS /PnS = VS2 /4kB TRL df . Suppose we now add a series resistor R between the source and the load, as shown in Fig. 1.12(c). We can anticipate two effects: the signal power at the load will reduce, and there will be additional noise. For example, the r.m.s. signal current is now IS = VS /(2RL + R), so the signal power is PS = IS2 RL = VS2 /{4RL (1 + R/2RL )2 }. This value has clearly reduced. A similar expression can be found for the noise power due to the source.

R VnS

RS

Fig. 1.12 Simple circuits for noise calculations: (a) noiseless, (b) assuming source noise, and (c) assuming an additional resistive element.

RL

Vn

VnS

RS

RL

RS

RL

VS VS (a)

VS (b)

(c)

Heat Although this term has reduced as well, we must add to it the noise due to the additional resistor. If this is done, we obtain a total noise power of 2 + V 2 )/{4R (1 + R/2R )2 . Assuming that everything is at the same Pn = (VnS L L n temperature, the average value of Vn2 is 4kB TRdf . As a result, the SNR at the load is now PS /Pn = VS2 /{4kB TRL df (1 + R/RL )}. Clearly, the SNR has got worse, by a factor 1 + R/RL , known as the noise factor F. All intermediate circuits, whether passive or active, have a noise factor. Often this is expressed in decibels, as the noise ﬁgure NF = 10 log10 (F). The better the circuit, the closer F will be to unity, and the closer NF will be to zero. In this case, R should clearly be made as small as possible. The effect of any additive noise should be minimized, by placing ampliﬁers at the front end of the system. Is that the end of the story for noise? Unfortunately no, because there are other physical mechanisms that create it. We will discuss these later.

1.9 Heat When the aim is to unravel the electrical properties of materials, should we take a detour and discuss heat? In general, no, we should not do that but when the two subjects overlap a little digression is permissible. I want to talk here ﬁrst about the relationship between the electrical conductivity and heat conductivity, and then point out some discrepancies suggesting that something is seriously wrong with our model. We have already discussed electrical conductivity. Heat conductivity is the same kind of thing but involves heat. An easy but rather unpleasant way of learning about it is to touch a piece of metal in freezing weather. The heat from your ﬁnger is immediately conducted away and you may get frostbite. Now back to that relationship. Denoting heat conductivity by κ, it was claimed around the middle of the nineteenth century that for metals κ = CWF T, σ

(1.76)

where CWF , the so-called Wiedemann–Franz constant, was empirically derived. It was taken as CWF = 2.31 × 10–8 W S–1 K–2 .

(1.77)

How well is the Wiedemann–Franz law satisﬁed? Very well, as Table 1.2 shows. Can it be derived from our model in which our electrons bounce about in the solid? Yes, that is what Drude did in about 1900. Let us follow what he did. At equilibrium, the average energy of an electron (eqn 1.1) is E = 3/2 kB T. The speciﬁc heat CV is deﬁned as the change in the average energy per unit volume with temperature 3 dE kB . = Ne (1.78) CV = Ne dT 2 Let us now consider heat ﬂow, assuming that all the heat is carried by the electrons. We shall take a one-dimensional model in which the electrons move

21

22

The electron as a particle Table 1.2 Electrical and thermal conductivities measured at 293 K Metal Silver Copper Aluminium Sodium Cadmium Iron

σ (107 –1 m–1 )

κ(W m–1 K –1 )

CWF (10–8 W K –2 )

6.15 5.82 3.55 2.10 1.30 1.00

423 387 210 135 102 67

2.45 2.37 2.02 2.18 2.64 2.31

only in the x direction. If there is a heat ﬂow the average energy may change slightly from point to point. Taking an interval from x – ℓ to x + ℓ (remember ℓ is the mean free path) the average at the two boundaries will be E – (dE/ dx)ℓ and E + (dE/dx)ℓ respectively. Referring now to a result from the kinetic theory of gases that the number of particles ﬂowing in a given direction per unit surface per unit time is 61 Ne vth , the net ﬂow across the plane at x is net energy ﬂow = (1/3)Ne vth

dE ℓ. dx

(1.79)

According to the simple theory of heat, the ﬂow of heat energy is proportional to the gradient of temperature where the proportionality constant is the heat conductivity, κ, yielding net heat energy ﬂow = κ

dT dx

.

(1.80)

Equating now eqn (1.79) with (1.80) we obtain κ=

1 Ne vth ℓkB . 2

(1.81)

We may now relate the heat conductivity to the electrical conductivity as follows: 1 Ne vth ℓkB 3 κ = = 2 2 σ Ne (e τ )/m 2

∗ Valid

at room temperature but fails at low temperatures.

kB e

2

T,

(1.82)

where the relation ℓ = vth τ (neglect vD in eqn (1.11)) has been used. The functional relationship is exactly the same: the ratio of the two conductivities is indeed proportional to T as was stipulated by the empirical formula. But what is the value of the constant? Inserting the values of e and kB into eqn (1.82), we obtain for the Wiedemann–Franz constant a value of 1.22 × 10–8 W S–1 K–2 , about a factor 2 smaller than the experimental value. Up to now we have talked only about the electronic contribution to the speciﬁc heat and quoted it as being 23 Ne kB , but classically the lattice will also contribute a term∗ 3NkB where N is the density of atoms. Thus, we should expect an alkali metal (in which Ne = N) to have a 50% greater speciﬁc heat than

Exercises an insulator having the same number of lattice atoms because of the electronic contribution. These expectations are, however, wrong. It turns out that metals and insulators have about the same speciﬁc heat. Our model fails again to explain the experimentally observed value. What shall we do? Modify our model. But how? Up to now the modiﬁcations have been fairly obvious. The ‘wrong sign’ of the Hall voltage could be explained by introducing positive carriers, and when cyclotron resonance measurements showed that the mass of an electron in a solid was different from the ‘free’ electron mass, we simply said: ‘all right, the electron’s mass is not a constant. How should we modify our model now?’ There seems to be no simple way of doing so. An entirely new start is needed. There is no quick ﬁx for this real dilemma. We have to go quite deeply into wave theory and quantum mechanics. Finally, all is revealed in Section 6.3 when we ﬁnd that electrons do make a quantiﬁable contribution to speciﬁc heat, which turns out to be very small.

23

Metals behave as if the free electrons make practically no contribution to the speciﬁc heat.

Exercises 1.1. A 10 mm cube of germanium passes a current of 6.4 mA when 10 mV is applied between two of its parallel faces. Assuming that the charge carriers are electrons that have a mobility of 0.39 m2 V–1 s–1 , calculate the density of carriers. What is their collision time if the electron’s effective mass in germanium is 0.12 m0 where m0 is the free electron mass? 1.2. An electromagnetic wave of free space wavelength 0.5 mm propagates through a piece of indium antimonide that is placed in an axial magnetic ﬁeld. There is resonant absorption of the electromagnetic wave at a magnetic ﬁeld, B = 0.323 wb m–2 . (i) What is the effective mass of the particle in question? (ii) Assume that the collision time is 15 times longer (true for electrons around liquid nitrogen temperatures) than in germanium in the previous example. Calculate the mobility. (iii) Is the resonance sharp? What is your criterion? 1.3. If both electrons and holes are present the conductivities, add. This is because under the effect of an applied electric ﬁeld the holes and electrons ﬂow in opposite directions, and a negative charge moving in the (say) +z-direction is equivalent to a positive charge moving in the –z-direction. Assume that in a certain semiconductor the ratio of electronic mobility, μe , to hole mobility, μh , is equal to 10, the density of holes is Nh = 1020 m–3 , and the density of electrons is Ne = 1019 m–3 . The measured conductivity is 0.455 ohm–1 m–1 . Calculate the mobilities.

1.4. Measurements on sodium have provided the following data: resistivity 4.7 × 10–8 ohm m, Hall coefﬁcient –2.5 × 10–10 m3 C–1 , critical wavelength of transparency 210 nm, and density 971 kg m–3 . Calculate (i) the density of electrons, (ii) the mobility, (iii) the effective mass, (iv) the collision time, (v) the number of electrons per atom available for conduction. Electric conduction in sodium is caused by electrons. The number of atoms in a kg mole is 6.02 × 1026 and the atomic weight of sodium is 23. 1.5. For an electromagnetic wave propagating in sodium plot the real and imaginary part of the wavenumber k as a function of frequency (use a logarithmic scale) from 106 to 1016 Hz. Determine the penetration depth for 106 , 1015 , and 2 × 1015 Hz. Use the conductivity and the collision time as obtained from Exercise 1.4. 1.6. A cuboid of Ge has contacts over all of its 2 mm × 1 mm ends and point contacts approximately half way along its 5 mm length, at the centre of the 5 mm × 1 mm faces. A magnetic ﬁeld can be applied parallel to this face. A current of 5 mA is passed between the end contacts when a voltage of 310 mV is applied. This generates a voltage across the point contacts of 3.2 mV with no magnetic ﬁeld and 8.0 mV when a ﬁeld of 0.16 T is applied. (i) Suggest why an apparent Hall voltage is observed with no magnetic ﬁeld.

24

The electron as a particle

(ii) Using the corrected Hall voltage ﬁnd the carrier density in the Ge sample. (iii) Estimate the conductivity of the Ge. (iv) What is the mobility of the carriers? (v) Is it a p or n type semiconductor? 1.7. The Hall effect (see Fig. 1.3) is measured in a semiconductor sample in which both electrons and holes are present. Under the effect of the magnetic ﬁeld both carriers are deﬂected in the same transverse direction. Obviously, no electric ﬁeld can stop simultaneously both the electrons and the holes, hence whatever the Hall voltage there will always be carrier motion in the transverse direction. Does this mean that there will be an indeﬁnite accumulation of electrons and holes on the surface of one of the boundaries? If not, why not? 1.8. Derive an expression for the Hall coefﬁcient RH [still deﬁned by eqn (1.20)] when both electrons and holes are present. The experimentally determined Hall coefﬁcient is found to be negative. Can you conclude that electrons are the dominant charge carriers? [Hint: Write down the equation of motion (neglect inertia) for both holes and electrons in vectorial form. Resolve the equations in the longitudinal (z-axis in Fig. 1.3) and in the transverse (x-axis in Fig. 1.3) directions. Neglect the product of transverse velocity with the magnetic ﬁeld. Find the transverse velocities for electrons and holes. Find the transverse

current, and ﬁnally ﬁnd the transverse ﬁeld from the condition that the transverse current is zero.] 1.9. An electromagnetic wave is incident from Medium 1 upon Medium 2 as shown in Figs 1.4 and 1.5. Derive expressions for the reﬂected and transmitted power. Show that the transmitted electromagnetic power is ﬁnite when ω > ωp and zero when ω < ωp . [Hint: Solve Maxwell’s equations separately in both media. Determine the constants by matching the electric and magnetic ﬁelds at the boundary. The power in the wave (per unit surface) is given by the Poynting vector.] 1.10. An electromagnetic wave is incident upon a medium of width d, as shown in Fig. 1.6. Derive expressions for the reﬂected and transmitted power. Calculate the transmitted power for the cases d = 0.25 µm and d = 2.5 µm when ω = 6.28 × 1015 rad s–1 , ωp = 9 × 1015 rad s–1 (take ǫ = ǫ0 and μ = μ0 ). 1.11. In a medium containing free charges the total current E , where J is the density may be written as Jtotal = J – iωǫE particle current density, E electric ﬁeld, ǫ dielectric constant, and ω frequency of excitation. For convenience, the above expression is often written in the form Jtotal = –iωǫ¯¯eqvE , deﬁning thereby an equivalent dielectric tensor ǫ¯¯eqv . Determine ǫ¯¯eqv for a fully ionized electron–ion plasma to which a constant magnetic ﬁeld B0 is applied in the z-direction.

The electron as a wave

2

The old order changeth, yielding place to new. Tennyson The Idylls of the King Vezess uj utakra, Lucifer. Madách Az Ember Tragédiája

2.1 Introduction We have considered the electron as a particle and managed to explain successfully a number of interesting phenomena. Can we explain the rest of the electronics by gentle modiﬁcations of this model? Unfortunately (for students if not lecturers), the answer is no. The experimental results on speciﬁc heat have already warned us that something is wrong with our particles, but the situation is, in fact, a lot worse. We ﬁnd that the electron has wavelike properties too. The chief immigrant in this particular woodpile, the experiment that could not possibly be explained by a particle model, was the electron diffraction experiment of Davisson∗ and Germer in 1927. The electrons behaved as waves. We shall return to the experiment a little later; let us see ﬁrst what the basic difference is between particle and wave behaviour. The difference can best be illustrated by the following ‘thought’ experiment. Suppose we were to ﬁre bullets at a bullet-proof screen with two slits in it (Fig. 2.1). We will suppose that the gun barrel is old and worn, so that the bullets bespatter the screen around the slits uniformly after a fairly large number of shots. If at ﬁrst, slit B is closed by a bullet-proof cover, the bullets going through A make a probability pattern on the target screen, shown graphically in Fig. 2.1 as a plot of probability

Screen with holes

∗ Davisson

received the Nobel Prize in

1937.

Target screen

P1

P12 = P1 + P2

A

Gun

B P2

Fig. 2.1 An experiment with bullets.

26

The electron as a wave Screen with holes

Wave detector

P1 P12 = P1 + P2 A Source of waves

•

B P2

Fig. 2.2 An experiment with waves.

against distance from the gun nozzle–slit A axis. Calling this pattern P1 , we expect (and get) a similar but displaced pattern P2 if slit B is opened and slit A is closed. Now if both slits are open, the combined pattern, P12 , is simply P12 = P1 + P2 .

(2.1)

We will now think of a less dangerous and more familiar experiment, with waves in a ripple tank (Fig. 2.2). The gun is replaced by a vibrator or ripplegenerator, the slits are the same, and in the target plane there is a device to measure the ripple intensity, that is a quantity proportional to the square of the height of the waves produced. Then, with one slit open we ﬁnd P1 = |h1 |2 ,

(2.2)

P2 = |h2 |2 ,

(2.3)

or with the other open

where we have taken h1 and h2 as complex vectors and the constant of proportionality is unity. The probability functions are similar to those obtained with one slit and bullets. So far, waves and bullets show remarkable similarity. But with both slits open we ﬁnd P12 = P1 + P2 .

(2.4)

Instead, as we might intuitively suppose, the instantaneous values of the wave heights from each slit add; and as the wavelength of each set of ripples is the same, they add up in the familiar way δ is the phase difference between the two interfering waves.

∗ Nobel

Prize, 1929.

P12 = |h1 + h2 |2 = |h1 |2 + |h2 |2 + 2|h1 ||h2 | cos δ.

(2.5)

Thus, the crucial difference between waves and particles is that waves interfere, but particles do not. The big question in the 1920s was: are electrons like bullets or do they follow a theoretical prediction by L. de Broglie∗ ? According to de Broglie,

Introduction

27

Detector Electron gun

d

e ect

ele

s

on

ctr

Incident electron beam

Fig. 2.3

ﬂ

Re

d

θ

• •

d

•

•

•

•

•

•

•

•

θ sin

θ d

the electrons should have wavelike properties with a wavelength inversely proportional to particle momentum, namely h . (2.6) mv To test de Broglie’s hypothesis, Davisson and Germer ﬁred a narrow beam of electrons at the surface of a single crystal of nickel (Fig. 2.3). The wavelike nature of the electron was conclusively demonstrated. The reﬂected beam displayed an interference pattern. The arrangement is analogous to a reﬂection grating in optics; the grating is replaced by the regular array of atoms and the light waves are replaced by electron waves. Maximum response is obtained when the reﬂections add in phase, that is when the condition λ=

nλ = d sin θ

(2.7)

is satisﬁed. From eqn (2.7) the difference in angle between two successive maxima is of the order of λ/d. Thus, if the wavelength of the radiation is too small, the maxima lie too close to each other to be resolved. Hence, for good resolution, the wavelength should be about equal to the lattice spacing, which is typically a fraction of a nanometre. The electron velocity corresponding to a wavelength of 0.1 nm is v=

h 6.6 × 10–34 J s kg–1 m–1 = 7.25 × 106 ms–1 . = mλ 9.1 × 10–31 × 10–10

(2.8)

The accelerating voltage may be obtained from the condition of energy conservation 2 1 2 mv

= eV ,

whence V=

mv2 9.1 × 10–31 (7.25 × 106 )2 = kg m2 s–2 C–1 = 150 V. 2e 2 × 1.6 × 10–19

The voltages used by Davisson and Germer were of this order.

(2.9)

Schematic representation of Davisson and Germer’s experiment with low energy electrons. The electrons are effectively reﬂected by the surface layer of the crystal. The detector shows maximum intensity when the individual reﬂections add in phase.

h is Planck’s constant∗ (not the height of the waves in the ripple tank) with a rather small numerical value, namely 6.6 × 10–34 J s, and m and v are the mass and speed of the electron.

n is an integral number, d is the lattice spacing, and λ is the wavelength to be determined as a function of electron-gun accelerating voltage.

∗

Planck (Nobel Prize, 1918) introduced this quantity in 1901 in a theory to account for discrepancies encountered in the classical picture of radiation from hot bodies. He considered a radiator as an assembly of oscillators whose energy could not change continuously, but must always increase or decrease by a quantum of energy, hf. This was the beginning of the twentieth century for science and science has not been the same since. The conﬁdence and assurance of nineteenth-century physicists disappeared, probably forever. The most we can hope nowadays is that our latest models and theories go one step further in describing Nature.

28

The electron as a wave So electrons are waves. Are protons waves? Yes, they are; it can be shown experimentally. Are neutrons waves? Yes, they are; it can be shown experimentally. Are bullets waves? Well, they should be, but there are some experimental difﬁculties in proving it. Take a bullet which has a mass of 10–3 kg and travels at a velocity 103 m s–1 . Then the bullet’s wavelength is 6.6 × 10–34 m. Thus, our reﬂecting agents or slits should be about 10–34 m apart to observe the diffraction of bullets, and that would not be easily realizable. Our bullets are obviously too fast. Perhaps with slower bullets we will get a diffraction pattern with slits a reasonable distance apart. Taking 10 mm for the distance between the slits and requiring the same wavelength for the bullets, their velocity comes to 10–28 m s–1 ; that is, the bullet would travel 1 m in about 1021 years. Best modern estimates give the age of the universe as 1010 years so this way of doing the experiment runs again into practical difﬁculties. The conclusion from this rather eccentric aside is of some importance. It seems to suggest that everything, absolutely everything, that we used to regard as particles may behave like waves if the right conditions are ensured. The essential difference between electrons and particles encountered in some other branches of engineering is merely one of size. Admittedly, the factors involved are rather large. The bullet in our chosen example has a mass 1027 times the electron mass, so it is not entirely unreasonable that they behave differently.

2.2

The electron microscope

Particles are waves, waves are particles. This outcome of a few simple experiments mystiﬁes the layman, delights the physicist, and provides the philosopher with material for a couple of treatises. What about the engineer? The engineer is supposed to ask the consequential (though grammatically slightly incorrect) question: what is this good for? Well, one well-known practical effect of the wave nature of light is that the resolving power of a microscope is fundamentally limited by the wavelength of the light. If we want greater resolution, we need a shorter wavelength. Let me use X-rays then. Yes, but they can not be easily focused. Use electrons then; they have short enough wavelengths. An electron accelerated to a voltage of 150 V has a wavelength of 0.1 nm. This is already four thousand times shorter than the wavelength of violet light, and using higher voltages we can get even shorter wavelengths. Good, but can electrons be focused? Yes, they can. Very conveniently, just about the same time that Davisson and Germer proved the wave properties of electrons, Busch discovered that electric and magnetic ﬁelds of the right conﬁguration can bring a diverging electron beam to a focus. So all we need is a ﬂuorescent screen to make the incident electrons visible, and the electron microscope is ready. You know, of course, about the electron microscope, that it has a resolving power so great that it is possible to see large molecules with it, and using the latest techniques even individual atoms can be made visible. Our aim is mainly to emphasize the mental processes that lead from scientiﬁc discoveries to practical applications. But besides, there is one more interesting aspect of the electron microscope. It provides perhaps the best example for what is known as the ‘duality of the electron’. To explain the operation of the electron microscope, both the ‘wave’ and the ‘particle’ aspects of the electron are

Some properties of waves needed. The focusing is possible because the electron is a charged particle, and the great resolution is possible because it is a wave of extremely short wavelength.

2.3 Some properties of waves You are by now familiar with all sorts of waves, and you know that a wave of frequency, ω, and wave number, k, may be described by the formula u = a exp iϕ;

ϕ = –(ωt – kz),

where the positive z-axis is chosen as the direction of propagation. The phase velocity may be deﬁned as ∂z ω = = f λ. vp = ∂t ϕ=constant k

(2.10)

29

It must be admitted that the resolving power of the electron microscope is not as large as would follow from the available wavelengths of the electrons. The limitation in practice is caused by lens aberrations.

(2.11)

This is the velocity with which any part of the wave moves along. For a single frequency wave this is fairly obvious. One can easily imagine how the crest moves. But what happens when several waves are superimposed? The resultant wave is given by an exp{–i(ωn t – kn z)}, (2.12) u= n

where to each value of kn belongs an an and an ωn . Going over to the continuum case, when the number of components within an interval k tends to inﬁnity, we get ∞ a(k) exp{–i(ωt – kz)} dk, (2.13) u=

a(k)

–∞

where a(k) and ω are functions of k. We shall return to the general case later; let us take for the time being, t = 0, then u(z) =

∞

a(k) exp(ikz) dk

–∞

k k < k < k0 + 2 2

(2.15)

and a(k) = 0 outside this interval. The integral (2.14) reduces then to k0 +k/2 exp (ikz) dk, u(z) = k0 –k/2

k0

(2.14)

and investigate the relationship between a(k) and u(z). We shall be interested in the case when the wavenumber and frequency of the waves do not spread out too far, that is a(k) is zero everywhere with the exception of a narrow interval k. The simplest possible case is shown in Fig. 2.4 where a(k) = 1 for k0 –

Δk 1

(2.16)

k

Fig. 2.4 The amplitude of the waves as a function of wavenumber, described by eqn (2.15).

30

The electron as a wave U(Z) ΔZ

Fig. 2.5

Z

The spatial variation of the amplitude of the wave packet of Fig. 2.4.

−6π

−4π

−2π

2π

4π

6π

which can be easily integrated to give u(z) = k exp (ik0 z)

sin 21 (kz) 1 2 (kz)

.

(2.17)

We have here a wave whose envelope is given by the function sin 21 (kz) 1 2 (kz)

,

(2.18)

plotted in Fig. 2.5. It may be seen that the function is rapidly decreasing outside a certain interval z. We may say that the wave is essentially contained in this ‘packet’, and in future we shall refer to it as a wave packet. We chose the width of the packet, rather arbitrarily, to be determined by the points where the amplitude drops to 0.63 of its maximum value, that is where π kz =± . 2 2

(2.19)

Hence, the relationship between the spread in wavenumber k, and the spread in space z, is as follows k z = 2π . For having a narrow wave packet in space, we need a larger spread in wave number.

(2.20)

An obvious consequence of this relationship is that by making k large, z must be small, and vice versa. Let us return now to the time-varying case, still maintaining that a(k) is essentially zero beyond the interval k. Equation (2.13) then takes the form u=

k0 +k/2

a(k) exp{–i(ωt – kz)}dk.

(2.21)

k0 –k/2

Let us now rewrite the above formula in the following form ω0 is the frequency at k = k0 .

u(z, t) = A(z, t) exp{–i(ω0 t – k0 z)},

(2.22)

where A(z, t) =

k0 +k/2

k0 –k/2

a(k) exp[–i{(ω – ω0 )t – (k – k0 )z}]dk.

(2.23)

Applications to electrons

31

We may now deﬁne two velocities. One is ω0 /k0 , which corresponds to the previously deﬁned phase velocity, and is the velocity with which the central components propagate. The other velocity may be deﬁned by looking at the expression for A. Since A represents the envelope of the wave, we may say that the envelope has the same shape whenever (ω – ω0 )t – (k – k0 )z = constant.

(2.24)

Hence, we may deﬁne a velocity, vg =

∂z ω – ω0 = , ∂t k – k0

which, for sufﬁciently small δk, reduces to ∂ω . vg = ∂k k=k0

(2.25)

(2.26)

2.4 Applications to electrons We have discussed some properties of waves. It has been an exercise in mathematics. Now we take a deep plunge and will try to apply these properties to the particular case of the electrons. The ﬁrst step is to identify the wave packet with an electron in your mental picture. This is not unreasonable. We are saying, in fact, that where the ripples are, there must be the electron. If the ripples are uniformly distributed in space, as is the case for a single frequency wave, the electron can be anywhere. If the ripples are concentrated in space in the form of a wave packet, the presence of an electron is indicated. Having identiﬁed the wave packet with an electron, we may identify the velocity of the wave packet with the electron velocity. What can we say about the energy of the electron? We know that a photon of frequency ω has an energy E = hf = ℏω,

(2.27)

where f is the frequency of the electromagnetic wave and ℏ = h/2π . Analogously, it may be suggested that the energy of an electron in a wave packet centred at the frequency ω is given by the same formula. Hence, we may write down the energy of the electron, taking the potential energy as zero, in the form ℏω = 12 mv2g .

(2.28)

We can differentiate this partially with respect to k to get ℏ

∂vg ∂ω = mvg ∂k ∂k

(2.29)

which, with the aid of eqn (2.26), reduces to ℏ=m

∂vg . ∂k

(2.30)

Integrating, and taking the integration constant as zero, we get ℏk = mvg ,

(2.31)

vg is called the group velocity because it gives the velocity of the wave packet.

32

The electron as a wave which can be expressed in terms of wavelength as λ=

If we know the position of the electron with great precision, that is if z is very small, then the uncertainty in the velocity of the electron must be large.

h , mvg

(2.32)

and this is nothing else but de Broglie’s relationship. Thus, if we assume the validity of the wave picture, identify the group velocity of a wave packet with the velocity of an electron, and assume that the centre frequency of the wave packet is related to the energy of the electron by Planck’s constant, de Broglie’s relationship automatically drops out. This proves, of course, nothing. There are too many assumptions, too many identiﬁcations, representations, and interpretations; but, undeniably, the different pieces of the jigsaw puzzle do show some tendency to ﬁt together. We have now established some connection between the wave and particle aspects, which seemed to be entirely distinct not long ago. What can we say about the electron’s position? Well, we identiﬁed the position of the electron with the position of the wave packet. So, wherever the wave packet is, there is the electron. But remember, the wave packet is not inﬁnitely narrow; it has a width z, and there will thus be some uncertainty about the position of the electron. Let us look again at eqn (2.20). Taking note of the relationship expressed in eqn (2.31) between wavenumber and momentum, eqn (2.20) may be written as p z = h.

(2.33)

This is known as Heisenberg’s (Nobel Prize, 1932) uncertainty relationship. It means that the uncertainty in the position of the electron is related to the uncertainty in the momentum of the electron. Let us put in a few ﬁgures to see the orders of magnitude involved. If we know the position of the electron with an accuracy of 10–9 m then the uncertainty in momentum is p = 6.6 × 10–25 kg m s–1 ,

(2.34)

~ 7 × 105 m s–1 , v =

(2.35)

corresponding to

that is, the uncertainty in velocity is quite appreciable. Taking macroscopic dimensions, say 10–3 m for the uncertainty in position, and a bullet with a mass 10–3 kg, the uncertainty in velocity decreases to v = 6.6 × 10–28 m s–1 ,

(2.36)

which is something we can easily put up with in practice. Thus, whenever we come to very small distances and very light particles, the uncertainty in velocity becomes appreciable, but with macroscopic objects and macroscopic distances the uncertainty in velocity is negligible. You can see that everything here depends on the value of h, which happens to be rather small in our universe. If it were larger by a factor of, say 1040 , the police would have considerable difﬁculty in enforcing the speed limit. The uncertainty relationship has some fundamental importance. It did away (probably for ever) with the notion that distance and velocity can be simultaneously measured with arbitrary accuracy. It is applicable not only to position

Two analogies and velocity, but to a number of other related pairs of physical quantities.∗ It may also help to explain qualitatively some complicated phenomena. We may, for example, ask the question why there is such a thing as a hydrogen atom consisting of a negatively charged electron and a positively charged proton. Why doesn’t the electron eventually fall into the proton? Armed with our knowledge of the uncertainty relationship, we can now say that this event is energetically unfavourable. If the electron is too near to the proton then the uncertainty in its velocity is high; so it may have quite a high velocity, which means high kinetic energy. Thus the electron’s search for low potential energy (by moving near to the proton) is frustrated by the uncertainty principle, which assigns a large kinetic energy to it. The electron must compromise and stay at a certain distance from the proton (see Exercise 4.4).

2.5 Two analogies The uncertainty relationship is characteristic of quantum physics. We would search in vain for anything similar in classical physics. The derivation is, however, based on certain mathematical formulae that also appear in some other problems. Thus, even if the phenomena are entirely different, the common mathematical formulation permits us to draw analogies. Analogies may or may not be helpful. It depends to a certain extent on the person’s imagination or lack of imagination and, of course, on familiarity or lack of familiarity with the analogue. We believe in the use of analogies. We think they can help, both in memorizing a certain train of thought, and in arriving at new conclusions and new combinations. Even such a high-powered mathematician as Archimedes resorted to mechanical analogies when he wanted to convince himself of the truth of certain mathematical theorems. So this is quite a respectable method, and as we happen to know two closely related analogies, we shall describe them. Notice ﬁrst of all that u(z) and a(k) are related to each other by a Fourier integral in eqn (2.14). In deriving eqn (2.20), we made the sweeping assumption that a(k) was constant within a certain interval, but this is not necessary. We would get the same sort of ﬁnal formula, with slightly different numerical constants, for any reasonable a(k). The uncertainty relationship, as derived from the wave concept, is a consequence of the Fourier transform connection between a(k) and u(z). Thus, whenever two functions are related in the same way, they can readily serve as analogues. Do such functions appear in engineering practice? They do. The time variation of a signal and its frequency spectrum are connected by Fourier transform. A pulse of length τ has a spectrum (Fig. 2.6) exactly like the envelope we encountered before. The width of the frequency spectrum, referred to as bandwidth in common language, is related to the length of the pulse. All communication engineers know that the shorter the pulse the larger is the bandwidth to be transmitted. For television, for example, we need to transmit lots of pulses (the light intensity for some several hundred thousand spots twenty-ﬁve times per second), so the pulses must be short and the bandwidth large. This is why television works at much higher frequencies than radio broadcasting.

33 ∗ You

might ﬁnd it interesting to learn that electric and magnetic intensities are also subject to this law. They cannot be simultaneously measured to arbitrary accuracy.

34

The electron as a wave Amplitude

Fig. 2.6

(a)

τ

A rectangular pulse and its frequency spectrum.

Amplitude

(b)

l/τ

t

ω

In the mathematical formulation, k and z of eqn (2.20) are to be replaced by the frequency ω and time t. Hence, the relationship for communication engineering takes the form, ω t = 2π .

∗ Incidentally

there is another reason why radio telescopes must be bigger than, say, radar aerials. They do a lot of work at a wavelength of 210 mm, which is seven times longer than the wavelength used by most radars. Hence for the same resolution an aerial seven times bigger is needed.

θ is the beamwidth, z is the linear dimension of the aerial, and λ is the wavelength of the electromagnetic radiation (transmitted or received).

(2.37)

The analogy is close indeed. In the second analogue the size of an aerial and the sharpness of the radiation pattern are related. It is the same story. In order to obtain a sharp beam one needs a big aerial. So if you have ever wondered why radio astronomers use such giant aerials, here is the answer. They need narrow beams to be able to distinguish between the various radio stars, and they must pay for them by erecting (or excavating) big antennas.∗ The mathematical relationship comes out as follows: θ z = λ.

(2.38)

Exercises 2.1. Find the de Broglie wavelength of the following particles: (i) an electron in a semiconductor having average thermal velocity at T = 300 K and an effective mass of m∗e = am0 , where a is a constant, (ii) a helium atom having thermal energy at T = 300 K, (iii) an α-particle (He4 nucleus) of kinetic energy 10 MeV. 2.2. A ﬁnite wave train moves with constant velocity v. Its proﬁle as a function of space and time is given as f (a) =

exp iu 0

if

|u| < u0 |u| > u0

where u = t – kx and k = /v. At t = 0 the wave packet extends from x = –u0 v –1 to x = u0 v –1 , that is, it has a length of l = 2u0 v –1 .

Find the spectral composition of the wave train at x = 0 and ﬁnd from that the spectral width ω (range within which the amplitude drops to 63% of its maximum value). Prove the uncertainty relationship p l = h. 2.3. A typical operating voltage of an electron microscope is 50 kV. (i) What is the smallest distance that it could possibly resolve? (ii) What energy of neutrons could achieve the same resolution? (iii) What are the main factors determining the actual resolution of an electron microscope? 2.4. Electrons accelerated by a potential of 70 V are incident perpendicularly on the surface of a single crystal metal. The

Exercises crystal planes are parallel to the metal surface and have a (cubic) lattice spacing of 0.352 nm. Sketch how the intensity of the scattered electron beam would vary with angle. 2.5. A beam of electrons of 10 keV energy passes perpendicularly through a very thin (of the order of a few nanometres) foil of our previous single crystal metal. Determine the diffraction pattern obtained on a photographic plate placed 0.1 m behind the specimen. How will the diffraction pattern be modiﬁed for a polycrystalline specimen? [Hint: Treat the lattice as a two-dimensional array.] 2.6. Consider again an electron beam incident upon a thin metal foil but look upon the electrons as particles having a certain kinetic energy. In experiments with aluminium foils (J. Geiger and K. Wittmaack, Zeitschrift für Physik, 195, 44,

35

1966) it was found that a certain fraction of the electrons passing through the metal had a loss of energy of 14.97 eV. We could explain this loss as being the creation of a particle of that much energy. But what particle? It cannot be a photon (a transverse electromagnetic wave in the wave picture) because an electron in motion sets up no transverse waves. It must be a particle that responds to a longitudinal electric ﬁeld. So it might be a plasma wave of frequency ωp which we could call a ‘plasmon’ in the particle picture. The energy of this particle would be ℏωp . Calculate the value of ℏωp for aluminium assuming three free electrons per atom. Compare it with the characteristic energy loss found. The density of aluminium is 2700 kg m–3 and its atomic weight is 27.

The electron

3

That’s how it is, says Pooh. A.A. Milne Now we are six

3.1

Introduction

We have seen that some experimental results can be explained if we regard the electron as a particle, whereas the explanation of some other experiments is possible only if we look upon our electron as a wave. Now which is it? Is it a particle or is it a wave? It is neither, it is an electron. An electron is an electron; this seems a somewhat tautological deﬁnition. What does it mean? I want to say by this that we don’t have to regard the electron as something else, something we are already familiar with. It helps, of course, to know that the electron sometimes behaves as a particle because we have some intuitive idea of what particles are supposed to do. It is helpful to know that the electron may behave as a wave because we know a lot about waves. But we do not have to look at the electron as something else. It is sufﬁcient to say that an electron is an electron as long as we have some means of predicting its properties. How can we predict what an electron will do? Well, how can we predict any physical phenomenon? We need some mathematical relationship between the variables. Prediction and mathematics are intimately connected in science—or are they? Can we make predictions without any mathematics at all? We can. Seeing, for example, dark heavy clouds gathering in the sky we may say that ‘it is going to rain’ and on a large number of occasions we will be right. But this is not really a very profound and accurate prediction. We are unable to specify how dark the clouds should be for a certain amount of rain, and we would ﬁnd it hard to guess the temporal variation of the positions of the clouds. So, as you know very well, meteorology is not yet an exact science. In physics fairly good predictions are needed because otherwise it is difﬁcult to get further money for research. In engineering the importance of predictions can hardly be overestimated. If the designer of a bridge or of a telephone exchange makes some wrong predictions, this mistake may bring upon him the full legal apparatus of the state or the frequent curses of the subscribers. Thus, for engineers, prediction is not a triﬂing matter. Now what about the electron? Can we predict its properties? Yes, we can because we have an equation which describes the behaviour of the electron in mathematical terms. It is called Schrödinger’s (Nobel Prize, 1933) equation. Now I suppose you would like to know where Schrödinger’s equation came from? It came from nowhere; or more correctly it came straight from Schrödinger’s head, not unlike Pallas Athene who is reputed to have sprung out

Introduction

37

of Zeus’ head (and in full armour too!). Schrödinger’s equation is a product of Schrödinger’s imagination; it cannot be derived from any set of physical assumptions. Schrödinger’s equation is, of course, not unique in this respect. You have met similar cases before. In the sixth form you learned Newton’s equation. At the time you had just gained your ﬁrst glances into the hidden mysteries of physics. You would not have dared to question your schoolmaster about the origin of Newton’s equation. You were probably more reverent at the time, more willing to accept the word of authorities, and besides, Newton’s equation looks so simple that one’s credulity is not seriously tested. Force equals mass times acceleration; anyone is prepared to believe that much. And it seems to work in practice. At the university you are naturally more inquisitive than in your schooldays; so you may have been a bit more reluctant to accept Maxwell’s equations when you ﬁrst met them. It must have been very disturbing to be asked to accept the equation, ∇ ×E = –

∂B , ∂t

(3.1)

as the truth and nothing but the truth. But then you were shown that this equation is really identical with the familiar induction law, V =–

∂φ , ∂t

(3.2)

and the latter merely expresses the result of a simple experiment. Similarly ∇×H=J

(3.3)

is only a rewriting of Ampère’s law. So all is well again or rather all would be well if there was not another term on the right-hand side, the displacement current ∂D/∂t. Now what is this term? Not many lecturers admit that it came into existence as a pure artiﬁce. Maxwell felt there should be one more term there, and that was it. True, Maxwell himself made an attempt to justify the introduction of displacement current by referring to the a.c. current in a capacitor, but very probably that was just a concession to the audience he had to communicate with. He must have been more concerned with refuting the theory of instantaneous action at a distance, and with deriving a velocity with which disturbances can travel. The extra term had no experimental basis, whatsoever. It was a brilliant hypothesis which enabled Maxwell to predict the existence of electromagnetic waves. When some years later Hertz managed to ﬁnd these waves, the hypothesis became a law. It was a momentous time in history, though most history books keep silent about the event.∗ I am telling you all this just to show that an equation which comes from nowhere in particular may represent physical reality. Of course, Schrödinger had good reasons for setting up his equation. He had immediate success in several directions. Whilst Maxwell’s displacement current term explained no experimental observation, Schrödinger’s equation could immediately account for the atomic spectrum of hydrogen, for the energy levels of the Planck oscillator, for the non-radiation of electronic currents in atoms, and for the shift

∗ According

to most historians’ deﬁnition, an event is important if it affects a large number of people to a considerable extent for a long time. If historians were faithful to this deﬁnition they should write a lot about Maxwell and Hertz because by predicting and proving the existence of electromagnetic waves, Maxwell and Hertz had more inﬂuence on the life of ordinary people nowadays than any nineteenth-century general, statesman, or philosopher.

38

∗ In

the above discussion the role of Schrödinger in setting up modern quantum physics was very much exaggerated. There were a number of others who made comparable contributions, but since this is not a course in the history of science, and the Schrödinger formulation is adequate for our purpose, we shall not discuss these contributions.

The electron of energy levels in strong transverse ﬁelds. He produced four papers in quick succession and noted at the end with quiet optimism: ‘I hope and believe that the above attempt will turn out to be useful for explaining the magnetic properties of atoms and molecules, and also the electric current in the solid state.’ Schrödinger was right.∗ His equation turned out to be useful indeed. He was not exactly right, though. In order to explain all the properties of the solid state (including magnetism) two further requisites are needed: Pauli’s principle and ‘spin’. Fortunately, both of them can be stated in simple terms, so if we make ourselves familiar with Schrödinger’s equation, the rest is relatively easy.

3.2

Schrödinger’s equation

After such a lengthy introduction, let us have now the celebrated equation itself. In the usual notation, m is the mass of the electron, and V is the potential in which the electron moves.

–

∂ ℏ2 2 ∇ + V = iℏ . 2m ∂t

(3.4)

We have a partial differential equation in . But what is ? It is called the wave function, and |(x, y, z; t)|2 dx dy dz

This interpretation was proposed by Max Born, Nobel Prize, 1954.

(3.5)

gives the probability that the electron can be found at time, t, in the volume element, dx dy dz, in the immediate vicinity of the point, x, y, z. To show the signiﬁcance of this function better ||2 is plotted in Fig. 3.1 for a hypothetical case where ||2 is independent of time and varies only in one dimension. If we make many measurements on this system, we shall ﬁnd that the electron is always between z0 and z4 (the probability of being outside this region is zero), that it is most likely to be found in the interval dz around z3 , and it is three times as probable to ﬁnd the electron at z2 than at z1 . Since the electron must be somewhere, the probability of ﬁnding it between z0 and z4 must be unity, that is, z4 |(z)|2 dz = 1. (3.6) z0

The above example does not claim to represent any physical situation. It is shown only to illustrate the meaning of ||2 .

0.5

|Ψ(z)|2

0.4

Fig. 3.1 Introducing the concept of the wave function. |ψ(z)|2 dz proportional to the probability that the electron may be found in the interval dz at the point z.

0.3 0.2 0.1 0.0

z0

z1

z2

z3

z4

z

Solutions of Schrödinger’s equation

39

The physical content of eqn (3.4) will be clearer when we shall treat more practical problems, but there is one thing we can say immediately. Schrödinger’s equation does not tell us the position of the electron, only the probability that it will be found in the vicinity of a certain point. The description of the electron’s behaviour is statistical, but there is nothing particularly new in this. After all, you have met statistical descriptions before, in gas dynamics for example, and there was considerably less fuss about it. The main difference is that in classical mechanics, we use statistical methods in order to simplify the calculations. We are too lazy to write up 1027 differential equations to describe the motion of all the gas molecules in a vessel, so we rely instead on a few macroscopic quantities like pressure, temperature, average velocity, etc. We use statistical methods because we elect to do so. It is merely a question of convenience. This is not so in quantum mechanics. The statistical description of the electron is inherent in quantum theory. That is the best we can do. We cannot say much about an electron at a given time. We can only say what happens on the average when we make many observations on one system, or we can predict the statistical outcome of simultaneous measurements on identical systems. It may be sufﬁcient to make one single measurement (speciﬁc heat or electrical conductivity) when the phenomenon is caused by the collective interaction of a large number of electrons. We cannot even say how an electron moves as a function of time. We cannot say this because the position and the momentum of an electron cannot be simultaneously determined. The limiting accuracy is given by the uncertainty relationship, eqn (2.33).

3.3 Solutions of Schrödinger’s equation Let us separate the variables and attempt a solution in the following form (r, t) = ψ(r)w(t).

(3.7) Now r represents all the spatial variables.

Substituting eqn (3.7) into eqn (3.4), and dividing by ψw we get –

1 ∂w ℏ2 ∇ 2 ψ + V = iℏ . 2m ψ w ∂t

(3.8)

Since the left-hand side is a function of r and the right-hand side is a function of t, they can be equal only if they are both separately equal to a constant which we shall call E, that is we obtain two differential equations as follows: iℏ

∂w = Ew ∂t

(3.9)

and ℏ2 2 (3.10) ∇ ψ + V ψ = Eψ. 2m The solution of eqn (3.9) is simple enough. We can immediately integrate and get E (3.11) w = exp –i t , ℏ –

40

The electron and this is nothing else but our good old wave solution, at least as a function of time, if we equate E = ℏω.

(3.12)

This is actually something we have suggested before [eqn (2.27)] by recourse to Planck’s formula. So we may call E the energy of the electron. However, before making such an important decision let us investigate eqn (3.10) which also contains E. We could rewrite eqn (3.10) in the form: 2 ℏ – ∇ 2 + V ψ = Eψ. (3.13) 2m The second term in the bracket is potential energy, so we are at least in good company. The ﬁrst term contains ∇ 2 , the differential operator you will have met many times in electrodynamics. Writing it symbolically in the form: –

ℏ2 2 1 ∇ = (–iℏ∇)2 , 2m 2m

(3.14)

we can immediately see that by introducing the new notation, p = –iℏ∇,

(3.15)

and calling it the ‘momentum operator’ we may arrive at an old familiar relationship: p2 = kinetic energy. 2m

(3.16)

Thus, on the left-hand side of eqn (3.13) we have the sum of kinetic and potential energies in operator form and on the right-hand side we have a constant E having the dimensions of energy. Hence, we may, with good conscience, interpret E as the total energy of the electron. You might be a little bewildered by these deﬁnitions and interpretations, but you must be patient. You cannot expect to unravel the mysteries of quantum mechanics at the ﬁrst attempt. The fundamental difﬁculty is that ﬁrst steps in quantum mechanics are not guided by intuition. You cannot have any intuitive feelings because the laws of quantum mechanics are not directly experienced in everyday life. The most satisfactory way, at least for the few who are mathematically inclined, is to plunge into the full mathematical treatment and leave the physical interpretation to a later stage. Unfortunately, this method is lengthy and far too abstract for an engineer. So the best we can do is to digest alternately a little physics and a little mathematics and hope that the two will meet.

3.4

The electron as a wave

Let us look at the simplest case when V = 0 and the electron can move only in one dimension. Then eqn (3.13), which is often called the time-independent Schrödinger equation, reduces to ℏ2 ∂ 2 ψ + Eψ = 0. 2m ∂z2

(3.17)

The electron meeting a potential barrier

41

The solution of this differential equation is a wave in space. Hence the general solution of Schrödinger’s equation for the present problem is E = exp –i t {A exp(ikz) + B exp(–ikz)}. ℏ

(3.18)

In this example we have chosen the potential energy of the electron as zero, thus eqn (3.19) must represent the kinetic energy. Hence, we may conclude that ℏk must be equal to the momentum of the electron. We have come to this conclusion before, heuristically, on the basis of the wave picture, but now we have the full authority of Schrödinger’s equation behind us. You may notice too that p = ℏk is an alternative expression of de Broglie’s relationship, thus we have obtained from Schrödinger’s equation both the wave behaviour and the correct wavelength. What can we say about the position of the electron? Take B = 0 for simplicity, then we have a forward travelling wave with a deﬁnite value for k. The probability of ﬁnding the electron at any particular point is given by |ψ(z)|2 which according to eqn (3.18) is unity, independently of z. This means physically that there is an equal probability of the electron being at any point on the z-axis. The electron can be anywhere; that is, the uncertainty of the electron’s position is inﬁnite. This is only to be expected. If the value of k is given then the momentum is known, so the uncertainty in the momentum of the electron is zero; hence the uncertainty in position must be inﬁnitely great.

A and B are constants representing the amplitudes of the forward and backward travelling waves, and k is related to E by E=

ℏ2 k 2 . 2m

(3.19)

3.5 The electron as a particle Equation (3.17) is a linear differential equation, hence the sum of the solutions is still a solution. We are therefore permitted to add up as many waves as we like; that is, a wave packet (as constructed in Chapter 2) is also a solution of Schrödinger’s equation. We can now be a little more rigorous than before. A wave packet represents an electron because |(z)|2 is appreciably different from zero only within the packet. With the choice a(k) = 1 in the interval k and zero elsewhere, it follows from eqns (2.16) and (2.17) that the probability of ﬁnding the electron is given by∗ 2

|ψ(z)| = K

sin 21 (kz) 1 2 (kz)

2

.

(3.20)

3.6 The electron meeting a potential barrier Consider again a problem where the motion of the electron is constrained in one dimension, and the potential energy is assumed to take the form shown in Fig. 3.2. You are familiar with the classical problem, where the electron starts somewhere on the negative z-axis (say at –z0 ) in the positive direction with a deﬁnite velocity. The solution may be obtained purely from energetic considerations. If the kinetic energy of the electron E is smaller than V2 , the electron is turned

∗ The constant K may be determined by the normalization condition ∞ |ψ(z)|2 dz = 1. –∞

1

2 V

Electron V2

V1 = 0 0

z

Fig. 3.2 An electron incident upon a potential barrier.

42

∗ So

that the interaction between the electrons can be neglected.

The charge of the electron is not smoothed out. When the electron is found, the whole electron is there.

The electron back by the potential barrier at z = 0. If E > V2 , the electron slows down but carries on regardless. How should we formulate the equivalent quantum mechanical problem? We should represent our electron by a wave packet centred in space on –z0 and should describe its momentum with an uncertainty p. We should use the wave function obtained as initial condition at t = 0 and should solve the timedependent Schrödinger equation. This would be a very illuminating exercise, alas much too difﬁcult mathematically. We have to be satisﬁed by solving a related problem. We shall give our electron a deﬁnite energy, that is a deﬁnite momentum, and we shall put up with the concomitant uncertainty in position. We shall not be able to say anything about the electron’s progress towards the potential barrier, but we shall have a statistical solution which will give the probability of ﬁnding the electron on either side of this potential barrier. Specifying the momentum and not caring about the position of the electron is not so unphysical as you might think. The conditions stated may be approximated in practice by shooting a sufﬁciently sparse∗ electron beam towards the potential barrier with a well-deﬁned velocity. We are not concerned then with the positions of individual electrons, only with their spatial distribution on the average, which we call the macroscopic charge density. Hence we may identify e|ψ|2 with the charge density. This is not true in general. What is always true is that |ψ|2 gives the probability of an electron being found at z. Be careful, |ψ(z)|2 does not give the fraction of the electron’s charge residing at z. If, however, a large number of electrons behave identically, then |ψ|2 may be justiﬁably regarded to be proportional to the charge density. Let us proceed now to the mathematical solution. In region 1 where V1 = 0 the solution is already available in eqns (3.18) and (3.19), E 1 = exp –i t {A exp(ik1 z) + B exp(–ik1 z)}, (3.21) ℏ and k12 =

2mE . ℏ2

(3.22)

In region 2 the equation to be solved is as follows (the time-dependent part of the solution remains the same because E is speciﬁed) ℏ2 ∂ 2 ψ + (E – V2 )ψ = 0, 2m ∂z2

(3.23)

E 2 = exp –i t {C exp(ik2 z) + D exp(–ik2 z)}, ℏ

(3.24)

with the general solution

where k22 =

2m (E – V2 ). ℏ2

(3.25)

The electron meeting a potential barrier

43

Now we shall ask the question, depending on the relative magnitudes of E and V2 , what is the probability that the electron can be found in regions 1 and 2, respectively. It is actually easier to speak about this problem in wave language because then the form of the solution is automatically suggested. Whenever a wave is incident on some sort of discontinuity, there is a reﬂected wave, and there is a transmitted wave. Since no wave is incident from region 2, we can immediately decide that D must be zero. In order to determine the remaining constants, we have to match the two solutions at z = 0, requiring that both ψ and ∂ψ/∂z should be continuous. From eqns (3.21) and (3.24), the above conditions lead to the algebraic equations, A+B=C

(3.26)

ik1 (A – B) = ik2 C,

(3.27)

and

whence B k1 – k2 = , A k1 + k2

2k1 C = . A k1 + k2

(3.28)

Let us distinguish now two cases: (i) E > V2 . In this case k22 > 0, k2 is real, which means an oscillatory solution in region 2. The values of k2 and k1 are, however, different. Thus, B/A is ﬁnite, that is, there is a ﬁnite amount of reﬂection. In contrast to the classical solution, there is some probability that the electron is turned back by the potential discontinuity. (ii) E < V2 . In this case k22 < 0, k2 is imaginary; that is, the solution declines exponentially in region 2.∗ Since |C/A| > 0, there is a ﬁnite, though declining, probability of ﬁnding the electron at z > 0. Classically, an electron has no chance of getting inside region 2. Under the laws of quantum mechanics the electron may penetrate the potential barrier. A third case of interest is when the potential proﬁle is as shown in Fig. 3.3, and E < V2 . Then k2 is imaginary and k3 is real. Hence one may expect that |ψ|2 declines in region 2 and is constant in region 3. The interesting thing is that |ψ|2 in region 3 is not zero. Thus, there is a ﬁnite probability that the electron crosses the potential barrier and appears at the other side with energy unchanged. Since there is an exponential decline in region 2, it is necessary that that region should be narrow to obtain any appreciable probability in region 3. If we are thinking in terms of the incident electron beam, we may say that a certain fraction of the electrons will get across the potential barrier. This tendency for electrons to escape across the potential barrier is called the tunnel effect, or simply tunnelling. As you will see later, it is an important effect which we shall often invoke to explain phenomena as different as the bonding of the hydrogen molecule or the operation of the tunnel diode.†

∗ The

exponentially increasing solution cannot be present for physical reasons.

1

3

2 V

Electron V2

V1 = 0 0

V3 = 0 d

z

Fig. 3.3 An electron incident upon a narrow potential barrier. †A

more mundane example of tunnelling occurs every time we switch on an electric light. The contacts are always covered with an oxide ﬁlm, that in bulk would be an insulator. But it is rubbed down to a few molecules’ thickness by the mechanical action of the switch, and the tunnelling is so efﬁcient that we do not notice it.

44

The electron

3.7

Two analogies

Without the help of Schrödinger’s equation, we could not have guessed how electrons behaved when meeting a potential barrier. But having found the solutions in the form of propagating and exponentially decaying waves, a physical picture, I hope, is emerging. There is always a physical picture if you are willing to think in terms of waves. Then it is quite natural that discontinuities cause reﬂections and only a part of the wave is transmitted. The concepts are not appreciably more difﬁcult than those needed to describe the motion of classical electrons, but you need time to make yourself familiar with them. ‘Familiarity breeds contempt’ may very well apply to arts subjects, but in most branches of science the saying should be reformulated as ‘familiarity breeds understanding’ or, more poignantly, as ‘lack of familiarity breeds bewilderment’. Assuming that you have already developed some familiarity with waves, it may help to stress the analogy further. If we went a little more deeply into the mathematical relationships, we would ﬁnd that the problem of an electron meeting a potential barrier is entirely analogous to an electromagnetic wave meeting a new medium. Recalling the situations depicted in Figs. 1.4 to 1.6, the analogies are as follows. 1. There are two semi-inﬁnite media (Fig. 1.4); electromagnetic waves propagate in both of them. Because of the discontinuity, a certain part of the wave is reﬂected. This is analogous to the electron meeting a potential barrier (Fig. 3.2) with an energy E > V2 . Some electrons are reﬂected because of the presence of a discontinuity in potential energy. 2. There are two semi-inﬁnite media (Fig. 1.5); electromagnetic waves may propagate in the ﬁrst one but not in the second one. The ﬁeld intensities are, however, ﬁnite in medium 2 because the electromagnetic wave penetrates to a certain extent. This is analogous to the electron meeting a potential barrier (Fig. 3.2) with an energy E < V2 . In spite of not having sufﬁcient energy, some electrons may penetrate into region 2. 3. There are two semi-inﬁnite media separated from each other by a third medium (Fig. 1.6); electromagnetic waves may propagate in media 1 and 3 but not in the middle one. The wave incident from medium 1 declines in medium 2 but a ﬁnite amount arrives and can propagate in medium 3. This is analogous to the electron meeting a potential barrier shown in Fig. 3.3, with an energy E < V2 . In spite of not having sufﬁcient energy some electrons may cross region 2 and may appear and continue their journey in region 3. Instead of taking plane waves propagating in inﬁnite media, one might make the analogy physically more realizable though mathematically less perfect, by employing hollow metal waveguides. Discontinuities can then be represented by joining two waveguides of different cross-sections, and the exponentially decaying wave may be obtained by using a cut-off waveguide (of dimension smaller than half free-space wavelength). Then all the above phenomena can be easily demonstrated in the laboratory.

The electron in a potential well

45

3.8 The electron in a potential well In our previous examples, the electron was free to roam in the one-dimensional space. Now we shall make an attempt to trap it by presenting it with a region of low potential energy which is commonly called a potential well. The potential proﬁle assumed is shown in Fig. 3.4. If E > V1 , the solutions are very similar to those discussed before, but when E < V1 , a new situation arises. We have by now sufﬁcient experience in solving Schrödinger’s equation for a constant potential, so we shall write down the solutions without further discussions. In region 3 there is only an exponentially decaying solution ψ3 = C exp(–γ z),

L is the width of the well.

(3.29)

where 2m (V1 – E). (3.30) ℏ2 In region 2 the potential is zero. The solution is either symmetric or antisymmetric.∗ Accordingly, γ2 =

ψ2s = A cos kz

(3.31)

ψ2a = A sin kz

(3.32)

or

∗ This

is something we have not proved. It is true (the proof can be obtained fairly easily from Schrödinger’s equation) in general that if the potential function is symmetric the solution must be either symmetric or antisymmetric.

where 2m E. (3.33) ℏ2 In region 1 the solution must decay again, this time towards negative inﬁnity. If we wish to satisfy the symmetry requirement as well, the wave function must look like k2 =

ψ1 = ± C exp γ z.

(3.34)

Let us investigate the symmetric solution ﬁrst. We have then eqns (3.29) and (3.31), and eqn (3.34) with the positive sign. The conditions to be satisﬁed are the continuity of ψ and ∂ψ/∂z at L/2 and –L/2,† but owing to the symmetry it is sufﬁcient to do the matching at (say) L/2. From the continuity of the wave function L L = 0. (3.35) A cos k – C exp –γ 2 2

V

V1

are a number of different proofs that these conditions are physically reasonable. For example, direct integration of Schrödinger’s equation over an interval involving a boundary can yield the condition that ∂ψ/∂z must generally be continuous. One exception is when the potential step at the boundary becomes inﬁnite, for example when an electron is conﬁned in an inﬁnite potential well. In this case, ∂ψ/∂z is not continuous.

3

2

1

† There

V3 = V1

V2 = 0 –L 2

0

L 2

z

Fig. 3.4 An electron in a potential well.

46

The electron From the continuity of the derivative of the wave function L L Ak sin k – Cγ exp –γ = 0. 2 2

(3.36)

We have now two linear homogeneous equations in A and C which are soluble only if the determinant vanishes, that is cos k L – exp –γ L 2 2 (3.37) = 0, k sin k L –γ exp –γ L 2 2 leading to

L k tan k = γ. 2

(3.38)

Thus, k and γ are related by eqn (3.38). Substituting their values from eqns (3.30) and (3.33) respectively, we get E

1/2

2m L2 tan E ℏ2 4

1/2

= (V1 – E)1/2 ,

(3.39)

which is a transcendental equation to be solved for E. Nowadays one feeds this sort of equation into a computer and has the results printed in a few seconds. But let us be old-fashioned and solve the equation graphically by plotting the left-hand side and the right-hand side separately. Putting in the numerical values, we know m = 9.1 × 10–31 kg,

ℏ = 1.05 × 10–34 J s,

and we shall take L = 5 × 10–10 m, 2 If E > V1 the electron can have any energy it likes, but if E < V1 there are only three possible energy levels.

V1 = 1.6 × 10–18 J.

As may be seen in Fig. 3.5, the curves intersect each other in three points; so there are three solutions and that is the lot. To be correct, there are three energy levels for the symmetric solution and a few more for the antisymmetric solution. We have at last arrived at the solution of the ﬁrst quantum-mechanical problem which deserves literally the name quantum mechanical. Energy is no longer continuous, it cannot take arbitrary values. Only certain discrete energy levels are permitted. In the usual jargon of quantum mechanics, it is said: energy is quantized. We may generalize further from the above example. The discrete energy levels obtained are not a coincidence. It is true in general that whenever we try to conﬁne the electron, the solution consists of a discrete set of wave functions and energy levels.

The uncertainty relationship

47

1

V 12 r.h.s. 1

0.75V 12

1

0.50V 12 l.h.s. 1

0.25V 12

Fig. 3.5 0.25V

0.00

A plot of the two sides of eqn (3.39) against E for L/2 = 5 × 10–10 m and V1 = 1.6 × 10–18 J.

l.h.s.

l.h.s.

0.75V

0.50V

E

V

3.9 The potential well with a rigid wall We call the potential wall rigid when the electron cannot escape from the well, not even quantum-mechanically. This happens when V1 = ∞. We shall brieﬂy investigate this case because we shall need the solution later. Equations (3.31) and (3.32) are still valid in the zero potential region, but now (since the electron cannot penetrate the potential barrier) the continuity condition is L ψ ± = 0. (3.40) 2 The solutions are given again by eqns (3.31) and (3.32) for the symmetric and antisymmetric cases, respectively. The boundary conditions given by eqn (3.40) will be satisﬁed when π kL = (2r + 1) 2 2

and

kL = sπ , 2

(3.41)

for the symmetric and antisymmetric wave functions, respectively, where r and s are integers. This is equivalent to saying that kL is an integral multiple of π . Hence, the expression for the energy is E=

h2 n2 ℏ2 k 2 = , 2m 8mL2

n = 1, 2, 3, . . .

(3.42)

3.10 The uncertainty relationship The uncertainty relationship may be looked upon in a number of ways. We have introduced it on the basis of the wave picture where electrons were identiﬁed with wave packets.

48

The electron Can we now make a more precise statement about the uncertainty relationship? We could, if we introduced a few more concepts. If you are interested in the details, you can consult any textbook on quantum mechanics. Here, I shall merely outline one of the possible ways of deriving the uncertainty relationship. First, the average value of a physically measurable quantity, called an observable, is deﬁned in quantum mechanics as ψ ∗ Aψ d(volume) , (3.43) A = V 2 V |ψ| d(volume) where the integration is over the volume of interest, wherever ψ is deﬁned. A is in general an operator; it is –iℏ∇ for the momentum and simply r, the radius vector, for the position. Assuming that Schrödinger’s equation is solved for a particular case, we know the wave function ψ, and hence, with the aid of eqn (3.43), we can work out the average and r.m.s. values of both the electron’s position and of its momentum. Identifying z and p with {(z – z )2 }1/2

and

{( p – p )2 }1/2

respectively, we get z p h.

(3.44)

There is actually another often-used form of the uncertainty relationship E t h,

The emitted radiation is not monochromatic; it covers a ﬁnite range of frequencies.

(3.45)

which may be derived from relativistic quantum theory (where time is on equal footing with the spatial coordinates) and interpreted in the following way. Assume that an electron sits in a higher energy state of a system, for example in a potential well. It may fall to the lowest energy state by emitting a photon of energy ℏω. So if we know the energy of the lowest state, we could work out the energy of that particular higher state by measuring the frequency of the emitted photon. But if the electron spends only a time t in the higher state, then the energy of the state can be determined with an accuracy not greater than E = h/t. This is borne out by the measurements.

3.11

Philosophical implications

The advent of quantum mechanics brought problems to the physicist which previously belonged to the sacred domain of philosophy. The engineer can still afford to ignore the philosophical implications but by a narrow margin only. In another decade or two philosophical considerations might be relevant in the discussion of devices, so I will try to give you a foretaste of the things which might come. To illustrate the sort of questions philosophers are asking, take the following one: We see a tree in the quad, so the tree must be there. We have the evidence of our senses (the eye in this particular case) that the tree exists. But what happens when we don’t look at the tree, when no one looks at the tree at all; does the tree still exist? It is a good question.

Philosophical implications Had philosophers been content asking this and similar questions, the history of philosophy would be an easier subject to study. Unfortunately, driven by usual human passions (curiosity, vivid imagination, vanity, ambition, the desire to be cleverer than the next man, craving for fame, etc.), philosophers did try to answer the questions. To the modern scientist, most of their answers and debates don’t seem to be terribly edifying. I just want to mention Berkeley who maintained that matter would cease to exist if unobserved, but luckily there is God who perceives everything, so matter may exist after all. This view was attacked by Ronald Knox in the following limerick: There was a young man who said, ‘God Must think it exceedingly odd If he ﬁnds that this tree Continues to be When there’s no one about in the Quad.’ Berkeley replied in kind: Dear Sir: Your astonishment’s odd: I am always about in the Quad. And that’s why the tree Will continue to be, Since observed by Yours faithfully, God. You do, I hope, realize that only a minority of philosophical arguments were ever conducted in the form of limericks, and the above examples are not typical. I mention them partly for entertainment and partly to emphasize the problem of the tree in the quad a little more. In the light of quantum mechanics we should look at the problem from a slightly different angle. The question is not so much what happens while the tree is unobserved, but rather what happens while the tree is unobservable. The tree can leave the quad because for a brief enough time it can have a high enough energy at its disposal, and no experimenter has any means of knowing ~ h) from about it. We are prevented by the uncertainty relationship (Et = ever learning whether the tree did leave the quad or not. You may say that this is against common sense. It is, but the essential point is whether or not it violates the Laws of Nature, as we know them today. Apparently it does not. You may maintain that for that critical t interval the tree stays where it always has stood. Yes, it is a possible view. You may also maintain that the tree went over for a friendly visit to the quad of another college and came back. Yes, that’s another possible view. Is there any advantage in imagining that the tree did make that brief excursion? I cannot see any, so I would opt for regarding the tree as being in the quad at all times. But the problem remains, and becomes of more practical interest when considering particles of small size. A free electron travelling with a velocity 106 m s–1 has an energy of 2.84 eV. Assume that it wants to ‘borrow’ the same amount of energy again. It may borrow that much energy for an interval

49

50

The electron ~ 1.5 × 10–15 s. Now, you may ask, what can an electron do t = h/2.84 eV = in a time interval as short as 1.5 × 10–15 s? Quite a lot; it can get comfortably from one atom to the next. And remember all this on borrowed energy. So if there was a barrier of (say) ﬁve electron volts, our electron could easily move over it, and having scaled the barrier it could return the borrowed energy, and no one would be able to ﬁnd out how the electron made the journey. Thus, from a purely philosophical argument we could make up an alternative picture of tunnelling. We may say that tunnelling across potential barriers comes about because the electron can borrow energy for a limited time. Is this a correct description of what happens? I do not know, but it is a possible description. Is it useful? I suppose it is always useful to have various ways of describing the same event; that always improves understanding. But the crucial test is whether this way of thinking will help in arriving at new conclusions which can be experimentally tested. For an engineer the criterion is even clearer; if an engineer can think up a new device, using these sorts of arguments (e.g. violating energy conservation for a limited time) and the device works (or even better it can be sold for ready money) then the method is vindicated. The end justiﬁes the means, as Machiavelli said. Theoretical physicists, I believe, do use these methods. In a purely particle description of Nature, for example, the Coulomb force between two electrons is attributed to the following cause. One of the electrons borrows some energy to create a photon that goes dutifully to the other electron, where it is absorbed, returning thereby the energy borrowed. The farther the two electrons are from each other, the lesser the energy that can be borrowed, and therefore lower frequency photons are emitted and absorbed. Carrying on these arguments (if you are interested in more details ask a theoretical physicist) they do manage to get correctly the forces between electrons. So there are already some people who ﬁnd it useful to play around with these concepts. This is about as much as I want to say about the philosophical role of the electron. There are, incidentally, a number of other points where philosophy and quantum mechanics meet (e.g. the assertion of quantum mechanics that no event can be predicted with certainty, merely with a certain probability), but I think we may have already gone beyond what is absolutely necessary for the education of an engineer.

Exercises 3.1. An electron, conﬁned by a rigid one-dimensional potential well (Fig. 3.4 with V1 = ∞) may be anywhere within the interval 2a. So the uncertainty in its position is x = 2a. There must be a corresponding uncertainty in the momentum of the electron and hence it must have a certain kinetic energy. Calculate this energy from the uncertainty relationship and compare it with the value obtained from eqn (3.42) for the ground state.

[Hint: Use eqn (3.43). The momentum operator in this onedimensional case is –iℏ∂/∂z.]

3.2. The wave function for a rigid potential well is given by eqns (3.31) and (3.32) and the permissible values of k by

(i) Calculate the classical average values of the quantities enumerated in the previous example.

eqn (3.42). Calculate the average values of z,

(z – z )2 ,

p,

( p – p )2 .

3.3. The classical equivalent of the potential well is a particle bouncing between two perfectly elastic walls with uniform velocity.

Exercises (ii) Show that, for high-enough energies, the quantummechanical solution tends to the classical solution. 3.4. In electromagnetic theory the conservation of charge is represented by the continuity equation ∇ · J = –e

3.8. An electron beam is incident from the x < 0 region upon the one-dimensional potential shown in Fig. 3.6 with an energy E = 1 eV. Without detailed calculations what can you say about the reﬂection coefﬁcient at x = 0?

∂N , ∂t

V V3 = 3 eV

where J = current density and N = density of electrons. Assume that (x, t) is a solution of Schrödinger’s equation in a one-dimensional problem. Show that, by deﬁning the current density as ∂ ∗ ∂ iℏe ∗ , – J (x) = – 2m ∂x ∂x the continuity equation is satisﬁed. 3.5. The time-independent Schrödinger equation for the onedimensional potential shown in Fig. 3.2 is solved in Section 3.6. Using the deﬁnition of current density given in the example above, derive expressions for the reﬂected and transmitted currents. Show that the transmitted current is ﬁnite when E > V2 and zero when E < V2 . Comment on the analogy with Exercise 1.9. 3.6. Solve the time-independent Schrödinger equation for the one-dimensional potential shown in Fig. 3.2; V (z) = 0, V (z) = V2 , V (z) = 0,

z < 0, 0 < z < d, z > d.

Assume that an electron beam is incident from the z < 0 region with an energy E. Derive expressions for the reﬂected and transmitted current. Calculate the transmitted current when V2 = 2.5 eV, E = 0.5 eV, d = 2 Å, and d = 20 Å. 3.7. Exercise 3.6 may be solved approximately by assuming that the wave function in region 2 is of the form

51

x

V2 = –2 e V

Fig. 3.6 A one-dimensional potential variation. 3.9. Solve the time-independent Schrödinger equation for a two-dimensional rigid potential well having dimensions Lx and Ly in the x and y directions respectively. Determine the energy of the Five lowest lying states when Ly = (3/2)Lx . 3.10. The antisymmetric solution of the time-independent Schrödinger equation for the potential well of Fig. 3.4 is given by eqns (3.32) and (3.34). Estimate the energy (a rough estimate will do) of the lowest antisymmetric state for L = 10–9 m and V1 = 1.6 × 10–18 J. 3.11. Solve the time-independent Schrödinger equation for the one-dimensional potential well shown in Fig. 3.7, restricting the analysis to even functions of x only. The solution may be expressed in determinant form. Without expanding the determinant explain what its roots represent.

∞

∞

–k2i x

ψ2 = Ce

V (x)

(where k2i = Imk2 ) and then coming to the conclusion (note that the potential in region 3 is the same as that in region 1 and therefore k3 = k1 ) that

V0 E (electron energy)

J3 = e–2k2i d . J1 How accurate is this approximation? If the wave function in region 2 is real, as it is assumed in this exercise, then the quantum mechanical current, as deﬁned in Exercise 3.4, yields zero. How is it possible that the equation given above still gives good approximation for the ratio of the currents whereas the direct use of the proper formula leads to no current at all?

x 2b 2a

Fig. 3.7 A one-dimensional potential well.

52

The electron

3.12. Show that the differential equation for the electric ﬁeld of a plane electromagnetic wave, assuming exp(–iωt) time dependence has the same form as the time-independent Schrödinger equation for constant potential. Show further that the expression for the Poynting vector of the electromagnetic wave is of the same functional form as that for the quantum-mechanical current. 3.13. The potential energy of a classical harmonic oscillator is given as V (x) =

2 2 1 2 mω0 x .

We get the ‘quantum’ harmonic oscillator by putting the above potential function into Schrödinger’s equation.

The solutions for the four lowest states are as follows:∗ ψ(ζ ) = Hn (ζ ) exp(– 12 ζ 2 ), where ζ = αx, H0 = 1,

mω0 , ℏ 2 H2 = 4ζ – 2,

α2 =

H1 = 2ζ ,

and

3

H3 = 8ζ – 12ζ . Find the corresponding energies. Compare them with the energies Planck postulated for photons. *Here Hn is the Hermite polynomial of order n, named after Charles Hermite (who studied them in 1864).

The hydrogen atom and the periodic table I see the atoms, free and ﬁne, That bubble like a sparkling wine; I hear the songs electrons sing, Jumping from ring to outer ring; Lister The Physicist

4.1 The hydrogen atom Up to now we have been concerned with rather artiﬁcial problems. We said: let us assume that the potential energy of our electron varies as a function of distance this way or that way without specifying the actual physical mechanism responsible for it. It was not a waste of time. It gave an opportunity of becoming acquainted with Schrödinger’s equation, and of developing the ﬁrst traces of a physical picture based, perhaps paradoxically, on the mathematical solution. It would, however, be nice to try our newly acquired technique on a more physical situation where the potential is caused by the presence of some other physical ‘object’. The simplest ‘object’ would be a proton, which, as we know, becomes a hydrogen atom if joined by an electron. We are going to ask the following questions: (i) What is the probability that the electron is found at a distance r from the proton? (ii) What are the allowed energy levels? The answers are again provided by Schrödinger’s equation. All we have to do is to put in the potential energy due to the presence of a proton and solve the equation. The wave function is a function of time, and one might want to solve problems, where the conditions are given at t = 0, and one is interested in the temporal variation of the system. These problems are complicated and of little general interest. What we should like to know is how a hydrogen atom behaves on the average, and for that purpose the solution given in eqn (3.7) combined with (3.11) is adequate. We may then forget about the temporal variation, because |w(t)|2 = 1,

(4.1)

and solve eqn (3.13), the time-independent Schrödinger equation. The proton, we know, is much heavier than the electron; so let us regard it as inﬁnitely heavy (that is immobile) and place it at the origin of our coordinate system. The potential energy of the electron at a distance, r, from the proton is known from electrostatics: e2 . (4.2) V (r) = – 4π ǫ0 r

4

54

The hydrogen atom and the periodic table Thus, the differential equation to be solved is 2 e ℏ2 2 ∇ ψ+ + E ψ = 0. 2m 4π ǫ0 r

(4.3)

It would be hard to imagine a physical conﬁguration much simpler than that of a proton and an electron, and yet it is difﬁcult to solve the corresponding differential equation. It is difﬁcult because the 1/r term does not lend itself readily to analytical solutions. Thanks to the arduous efforts of nineteenthcentury mathematicians, the general solution is known, but it would probably mean very little to you. Unless you have a certain familiarity with the properties of associated Legendre functions, it will not make you much happier if you learn that associated Legendre functions happen to be involved. So I will not quote the general solution because that would be meaningless, nor shall I derive it because that would be boring. But just to give an idea of the mathematical operations needed, I shall show the derivation for the simplest possible case, when the solution is spherically symmetric, and even then only for the lowest energy. The potential energy of the electron depends only on the distance, r; it therefore seems advantageous to solve eqn (4.3) in the spherical coordinates r, θ , φ (Fig. 4.1). If we restrict our attention to the spherically symmetrical case, when ψ depends neither on φ nor on θ but only on r, then we can transform eqn (4.3) without too much trouble. We shall need the following partial derivatives

z

r θ y φ

∂ψ ∂r ∂ψ = ∂x ∂x ∂r

x

Fig. 4.1

(4.4)

and

Coordinate system used to transform eqn (4.3) to spherical coordinates.

∂ 2ψ ∂ = 2 ∂x ∂x

∂ψ ∂r . ∂r ∂x

(4.5)

When we differentiate eqn (4.5), we have to remember that ∂ψ/∂r is a function of r and ∂r/∂x is still a function of x; therefore, ∂ ∂ψ ∂r ∂r ∂ ∂ψ ∂r ∂ψ ∂ 2 r = + ∂x ∂r ∂x ∂x ∂r ∂r ∂x ∂r ∂x2 ∂ 2 ψ ∂r 2 ∂ψ ∂ 2 r = + . (4.6) ∂r ∂x2 ∂r2 ∂x Obtaining the derivatives with respect to y and z in an analogous manner, we ﬁnally get ∂ 2ψ ∂ 2ψ ∂ 2ψ + 2 + 2 ∂x2 ∂y ∂z 2 2 ∂r ∂r 2 ∂r 2 ∂ ψ + + = 2 ∂x ∂y ∂z ∂r 2 2 2 ∂ψ ∂ r ∂ r ∂ r + . + + ∂r ∂x2 ∂y2 ∂z2

∇ 2ψ =

(4.7)

The hydrogen atom We now have to work out the partial derivatives of r. Since r = (x2 + y2 + z2 )1/2 ,

(4.8)

x ∂r = 2 2 ∂x (x + y + z2 )1/2

(4.9)

∂ 2r 1 x2 = 2 – 2 , 2 2 2 1/2 2 ∂x (x + y + z ) (x + y + z2 )3/2

(4.10)

we get

and

and similar results for the derivatives by y and z. Substituting all of them in eqn (4.7), we get x2 ∂ 2ψ y2 z2 2 ∇ ψ= 2 + + ∂r x2 + y2 + z2 x2 + y2 + z2 x2 + y2 + z2 3 ∂ψ x2 + – (4.11) ∂r (x2 + y2 + z2 )1/2 (x2 + y2 + z2 )3/2

∂ 2 ψ 2 ∂ψ z2 y2 . = – + – 2 r ∂r (x + y2 + z2 )3/2 (x2 + y2 + z2 )3/2 ∂r2 Thus, for the spherically symmetrical case of the hydrogen atom the Schrödinger equation takes the form, ℏ2 ∂ 2 ψ 2 ∂ψ e2 + + E+ ψ = 0. (4.12) 2m ∂r2 r ∂r 4π ǫ0 r It may be seen by inspection that a solution of this differential equation is ψ = e–c0 r .

(4.13)

The constant, c0 , can be determined by substituting eqn (4.13) in eqn (4.12)

ℏ2 2 e2 c20 e–c0 r + (–c0 e–c0 r ) + E + e–c0 r = 0. (4.14) 2m r 4π ǫ0 r The above equation must be valid for every value of r, that is the coefﬁcient of exp(–c0 r) and that of (1/r) exp(–c0 r) must vanish. This condition is satisﬁed if E=–

ℏ2 c20 2m

(4.15)

and ℏ2 c0 e2 . = m 4π ǫ0

(4.16)

e2 m , 4π ℏ2 ǫ0

(4.17)

From eqn (4.16), c0 =

55

56

The hydrogen atom and the periodic table

The negative sign of the energy means only that the energy of this state is below our chosen zero point. [By writing the Coulomb potential in the form of eqn (4.2) we tacitly took the potential energy as zero when the electron is at inﬁnity.]

which substituted in eqn (4.15) gives E=–

me4 . 8ǫ02 h2

(4.18)

Thus, the wave function assumed in eqn (4.13) is a solution of the differential equation (4.12), provided that c0 takes the value prescribed by eqn (4.17). Once we have obtained the value of c0 , the energy is determined as well. It can take only one single value satisfying eqn (4.18). Let us work out now the energy obtained above numerically. Putting in the constants, we get E=–

kg C4 (9.1 × 10–31 )(1.6 × 10–19 )4 8(8.85 × 10–12 )2 (6.63 × 10–34 )2 F2 m–2 J2 s2

= –2.18 × 10–18 J.

(4.19)

Expressed in joules, this number is rather small. Since in most of the subsequent investigations this is the order of energy we shall be concerned with, and since there is a strong human temptation to use numbers only between 0.01 and 100, we abandon with regret the SI unit of energy and use instead the electron volt, which is the energy of an electron when accelerated to 1 volt. Since 1 eV = 1.6 × 10–19 J, From experimental studies of the spectrum of hydrogen it was known, well before the development of quantum mechanics, that the lowest energy level of hydrogen must be –13.6 eV, and it was a great success of Schrödinger’s theory that the same ﬁgure could be deduced from a respectablelooking differential equation.

(4.20)

the above energy in the new unit comes to the more reasonable-looking numerical value E = –13.6 eV.

(4.21)

What can we say about the electron’s position? As we have discussed many times before, the probability that an electron can be found in an elementary volume (at the point r, θ , φ) is proportional to |ψ|2 —in the present case it is proportional to exp(–2c0 r). The highest probability is at the origin, and it decreases exponentially to zero as r tends to inﬁnity. We could, however, ask a slightly different question: what is the probability that the electron can be found in the spherical shell between r and r + dr? Then, the probability distribution is proportional to r2 |ψ|2 = r2 e–2c0 r ,

(4.22)

which has now a maximum, as can be seen in Fig. 4.2. The numerical value of the maximum can be determined by differentiating eqn (4.22) d 2 –2c0 r (r e ) = 0 = e–2c0 r (2r – 2c0 r2 ), dr

(4.23)

whence r=

Niels Bohr, Nobel Prize, 1922.

1 4π ℏ2 ǫ0 = = 0.0528 nm. c0 e2 m

(4.24)

This radius was again known in pre-quantum-mechanical times and was called the radius of the ﬁrst Bohr orbit, where electrons can orbit without radiating. Thus, in quantum theory, the Bohr orbit appears as the most probable position of the electron.

The hydrogen atom

57

|ψ|2r2

Fig. 4.2

0.0

0.8

1.6

2.4

rc0

Plot of eqn (4.22) showing the probability that an electron (occupying the lowest energy state) may be found in the spherical shell between r and r + dr.

We have squeezed out about as much information from our one meagre solution as is possible; we should look now at the other solutions which I shall give without any proof. Sticking for the moment to the spherically symmetrical case, the wave function is ψn (r) = e–cn r Ln (r),

(4.25)

where Ln is a polynomial, and the corresponding energies are (in electron volts), En = –13.6

1 , n2

n = 1, 2, 3. . . .

(4.26)

The solution we obtained before was for n = 1. It gives the lowest energy, and it is therefore usually referred to as the ground state. If we have a large number of hydrogen atoms, most of them are in their ground state but some of them will be in excited states, which are given by n > 1. The probability distributions for the higher excited states have maxima farther from the origin as shown in Fig. 4.3 for n = 1, 2, 3. This is fair enough; for n > 1 the energy of the electron is nearer to zero, which is the energy of |ψ|2r 2 n=1

Fig. 4.3 n=2 n=3

0

2

4

6

8

10

12

14

16

18

20 rc0

Plots of ψn2 r2 for the three lowest energy (n = 1, 2, 3) spherically symmetrical solutions. The curves are normalized so that the total probabilities (the area under curves) are equal.

58

The hydrogen atom and the periodic table a free electron; so it is less strongly bound to the proton. If it is less strongly bound, it can wander farther away; so the radius corresponding to maximum probability increases.

4.2

Quantum numbers

So much about spherically symmetrical solutions. The general solution includes, of course, our previously obtained solutions, denoted by R(r) from here on but shows variations in θ and φ as well. It can be written as We have met n before; l and ml represent two more discrete sets of constants which ensure that the solutions have physical meaning. These discrete sets of constants always appear in the solutions of partial differential equations; you may remember them from the problems of the vibrating string or of the vibrating membrane. They are generally called eigenvalues; in quantum mechanics they are referred to as quantum numbers.

m

ψn,l,ml (r, θ , φ) = Rnl (r)Yl l (θ , φ).

(4.27)

It may be shown (alas, not by simple means) from the original differential equation (eqn (4.12)) that the quantum numbers must satisfy the following relationships n = 1, 2, 3 . . . l = 0, 1, 2, . . . n – 1

(4.28)

ml = 0, ±1, ±2 . . . ± l. For n = 1 there is only one possibility: l = 0 and ml = 0, and the corresponding wave function is the one we guessed in eqn (4.13). For the spherically symmetrical case the wave functions have already been plotted for n = 1, 2, 3; now let us see a wave function which is dependent on direction. Choosing n = 2, l = 1, ml = 0, the corresponding wave function is ψ210 = R21 (r)Y10 (θ , φ) = re–c0 r/2 cos θ .

5 c0 z 3

1 |ψ | 2 = 0.9, 0.5, 0.2 –1

–3

–5 –4

–2

0

2 c0 x 4

Fig. 4.4 Plots of constant |ψ210 |2 in the xz-plane.

(4.29)

This equation tells us how the probability of ﬁnding the electron varies as a function of r and θ . Thus, the equal-probability surfaces may be determined. The spherical symmetry has gone, but there is still cylindrical symmetry (no dependence on φ). It is therefore sufﬁcient to plot the curves in, say, the xz-plane. This is done in Fig. 4.4, where the unit of distance is taken as one Bohr radius, and the maximum probability (at x = 0 and z = ±2/c0 ) is normalized to unity. It can be clearly seen that the θ = 0 and θ = π directions are preferred (which of course follows from eqn (4.29) directly); there is a higher probability of ﬁnding the electron in those directions. With n = 2 and l = 1 there are two more states, but they give nothing new. The preferential directions in those cases are in the direction of the ±x and ±y-axes, respectively. For higher values of n and l the equal-probability curves look more and more complicated. Since at this level of treatment they will not add much to our picture of the hydrogen atom, we can safely omit them. I have to add a few words about notations. However convenient the parameters n and l might appear, they are never (or at least very rarely) used in that form. The usual notation is a number, equal to the value of n, followed by a letter, which is related to l by the following rule

The periodic table l=0 s

1 p

2 d

3 f

4 g

5 h

6 i

59

7 k

Thus, if you wish to refer to the states with n = 3 and l = 1, you call them the 3p states or the 3p conﬁguration. The reason for this rather illogical notation is of course historical. In the old days when only spectroscopic information was available about these energy levels they were called s for sharp, p for principal, d for diffuse, and f for fundamental. When more energy levels were found, it was decided to introduce some semblance of order and denote them by subsequent letters of the alphabet. That is how the next levels came to bear the letters g, h, i, k, etc.

4.3 Electron spin and Pauli’s exclusion principle The quantum numbers n, l, and ml have been obtained from the solution of Schrödinger’s equation. Unfortunately, as I mentioned before, they do not represent the whole truth; there is one more quantum number to be taken into account. It is called the spin quantum number, denoted by s, and it takes the values ± 21 . Historically, spin had to be introduced to account for certain spectroscopic measurements, where two closely spaced energy levels were observed when only one was expected. These were explained in 1925 by Uhlenbeck and Goudsmit by assuming that the electron can spin about its own axis. This classical description is very much out of fashion nowadays, but the name spin stuck and has been universally used ever since. Today the spin is looked upon just as another quantum number obtainable from a more complicated theory which includes relativistic effects as well. So we have now four quantum numbers: n, l, ml , and s. Any permissible combination of these quantum numbers [eqn (4.28) shows what is permissible] gives a state; the wave function is determined, the electron’s energy is determined, everything is determined. But what happens when we have more than one electron? How many of them can occupy the same state? One, said Pauli. There can be no more than one electron in any given state. This is Pauli’s exclusion principle. We shall use it as a separate assumption, though it can be derived from a relativistic quantum theory, due to Dirac. Although both the spin and the exclusion principle are products of rather involved theories, both of them can be explained in simple terms. So even if you do not learn where they come from, you can easily remember them.

4.4 The periodic table We have so far tackled the simplest conﬁguration when there are only two particles: one electron and one proton. How should we attempt the solution for a more complicated case; for helium, for example, which has two protons and two electrons? (Helium has two neutrons as well, but since they are neutral they have no effect on the electrons; thus when discussing the energy levels of electrons neutrons can be disregarded.) The answer is still contained in Schrödinger’s equation, but the form of the equation is more complicated. The differential operator ∇ operated on the

Wolfgang Pauli, Nobel Prize, 1945. Paul Adrien Maurice Dirac, Nobel Prize, 1933.

60

The hydrogen atom and the periodic table coordinate of the electron. If we have two electrons, we need two differential operators. Thus, ∇ 2ψ is replaced by ∇12 ψ + ∇22 ψ,

∗ It

is a separate story how positively charged protons and neutrons can peacefully coexist in the nucleus.

Note that the wave function ψ now depends on six variables, namely on the three spatial coordinates of each electron.

where the indices 1 and 2 refer to electrons 1 and 2, respectively. We may take the protons∗ as if they are inﬁnitely heavy again and put them at the origin of the coordinate system. Thus, the potential energy of electron 1 at a distance r1 from the protons is –2e2 /4π ǫ0 r1 , and similarly for electron 2. There is, however, one more term in the expression for potential energy: the potential energy due to the two electrons. If the distance between them is r12 , then this potential energy is e2 /4π ǫ0 r12 . It is of positive sign because the two electrons repel each other. We can now write down Schrödinger’s equation for two protons and two electrons: 1 ℏ2 – (∇12 ψ + ∇22 ψ) + 2m 4π ǫ0

2e2 2e2 e2 – ψ = Eψ. – + r1 r2 r12

(4.30)

Can this differential equation be solved? The answer, unfortunately, is no. No analytical solutions have been found. So we are up against mathematical difﬁculties even with helium. Imagine then the trouble we should have with tin. A tin atom has 50 protons and 50 electrons; the corresponding differential equation has 150 independent variables and 1275 terms in the expression for potential energy. This is annoying. We have the correct equation, but we cannot solve it because our mathematical apparatus is inadequate. What shall we do? Well, if we can’t get exact solutions, we can try to ﬁnd approximate solutions. This is fortunately possible. Several techniques have been developed for solving the problem of individual atoms by successive approximations. The mathematical techniques are not particularly interesting, and so I shall mention only the simplest physical model that leads to the simplest mathematical solution. In this model we assume that there are Z positively charged protons in the nucleus, and the Z electrons ﬂoating around the nucleus are unaware of each other. If the electrons are independent of each other, then the solution for each of them is the same as for the hydrogen atom provided that the charge at the centre is taken as Ze. This means putting Ze2 instead of e2 into eqn (4.2) and Z 2 e4 instead of e4 into eqn (4.18). Thus, we can rewrite all the formulae used for the hydrogen atom, and in particular the formula for energy, which now stands as En = –13.6

Z2 . n2

(4.31)

That is, the energy of the electrons decreases with increasing Z. In other words, the energy is below zero by a large amount; that is, more energy is needed to liberate an electron. This is fairly easy to understand; a large positive charge in the nucleus will bind the electron more strongly. The model of entirely independent electrons is rather crude, but it can go a long way towards a qualitative explanation of the chemical properties of the

The periodic table

61

elements. We shall see how Mendeleev’s periodic table can be built up with the aid of the quantum-mechanical solution of the hydrogen atom. We shall start by taking the lowest energy level, count the number of states, ﬁll them up one by one with electrons, and then proceed to the next energy level; and so on. According to eqn (4.31) the lowest energy level is obtained with n = 1. Then l = 0, ml = 0, and there are two possible states of spin s = ± 12 . Thus, the lowest energy level may be occupied by two electrons. Putting in one electron we get hydrogen, putting in two electrons we get helium, putting in three electrons . . . No, we cannot do that; if we want an element with three electrons, then the third electron must go into a higher energy level. With helium the n = 1 ‘shell’ is closed, and this fact determines the chemical properties of helium. If the helium atom happens to meet other electrons (in events ofﬁcially termed collisions), it can offer only high-energy states. Since all electrons look for low-energy states, they generally decline the invitation. They manifest no desire to become attached to a helium atom. If the probability of attracting an electron is small, can the helium atom give away one of its electrons? This is not very likely either. It can offer to its own electrons comfortable low-energy states. The electrons are quite satisﬁed and stay. Thus, the helium atom neither takes up nor gives away electrons. Helium is chemically inert. We now have to start the next energy shell with n = 2. The ﬁrst element there is lithium, containing two electrons with n = 1, l = 0 and one electron with n = 2, l = 0. Adopting the usual notations, we may say that lithium has two 1s electrons and one 2s electron. Since the 2s electron has higher energy, it can easily be tempted away. Lithium is chemically active. The next element is beryllium with two 1s and two 2s electrons; then comes boron with two 1s, two 2s, and one 2p electrons, which, incidentally, can be denoted in an even more condensed manner as 1s2 , 2s2 , 2p1 . Employing this new notation, the six electrons of carbon appear as 1s2 , 2s2 , 2p2 , the seven electrons of nitrogen as 1s2 , 2s2 , 2p3 , the eight electrons of oxygen as 1s2 , 2s2 , 2p4 , and the nine electrons of ﬂuorine as 1s2 , 2s2 , 2p5 . Let us pause here for a moment. Recall that a 2p state means n = 2 and l = 1, which according to eqn (4.28) can have three states (ml = 0 and ml = ±1) or, taking account of spin as well, six states altogether. In the case of ﬂuorine ﬁve of them are occupied, leaving one empty low-energy state to be offered to outside electrons. The offer is often taken up, and so ﬂuorine is chemically active. Lithium and ﬂuorine are at the opposite ends, the former having one extra electron, the latter needing one more electron to complete the shell. So it seems quite reasonable that when they are together, the extra electron of lithium will occupy the empty state of the ﬂuorine atom, making up the compound LiF. A chemical bond is born, a chemist would say. We shall discuss bonds later in more detail. Let us return meanwhile to the rather protracted list of the elements. After ﬂuorine comes neon. The n = 2 shell is completed: no propensity to take up or give away electrons. Neon is chemically inert like helium. The n = 3 shell starts with sodium, which has just one 3s electron and should therefore behave chemically like lithium. A second electron ﬁlls the 3s

There are two important points to realize: 1. We have our set of quantum numbers n, l, ml , and s, each one specifying a state with a deﬁnite energy. The energy depends on n only, but several states exist for every value of n. 2. Pauli’s exclusion principle must be obeyed. Each state can be occupied by one electron only.

62

∗ In

the hydrogen-type solutions the energy depends only on n, whereas taking account of electron interactions the energy increases with increasing values of l. It just happens that in potassium the energy of the 3d level (n = 3, l = 2) is higher than that of the 4s level (n = 4, l = 0).

Whenever a new shell is initiated, there is one electron with considerably higher energy than the rest. Since all electrons strive for lower energy, this electron can easily be lost to another element.

The hydrogen atom and the periodic table shell in magnesium. Then come aluminium, silicon, phosphorus, sulphur, and chlorine with one, two, three, four, and ﬁve 3p electrons, respectively. Chlorine is again short of one electron to ﬁll the 3p shell, and so behaves like ﬂuorine. The 3p shell is completed in argon, which is again inert. So far everything has gone regularly, and by the rules of the game the next electron should go into the 3d shell. It does not. Why? Well, why should it? The electrons in potassium are under no obligation to follow the energy hierarchy of the hydrogen atom like sheep. They arrange themselves in such a way as to have the lowest energy. If there were no interaction between the electrons, the energy levels of the element would differ only by the factor Z 2 , conforming otherwise to that of the hydrogen atom. If the interaction between the electrons mattered a lot, we should completely abandon the classiﬁcation based on the energy levels of the hydrogen atom. As it happens, the electron interactions are responsible for small quantitative∗ changes that cause qualitative change in potassium—and in the next few elements, called the transition elements. First the 4s shell is ﬁlled, and only after that are the 3d states occupied. The balance between the two shells remains, however, delicate. After vanadium (with three 3d and two 4s electrons) one electron is withdrawn from the 4s shell; hence chromium has ﬁve 3d electrons but only one 4s electron. The same thing happens later with copper, but apart from that everything goes smoothly up to krypton, where the 4p shell is ﬁnally completed. The regularity is somewhat marred after krypton. There are numerous deviations from the hydrogen-like structure but nothing very dramatic. It might be worthwhile mentioning the rare earth elements in which the 4f shell is being ﬁlled while eleven electrons occupy levels in the outer shells. Since chemical properties are mainly determined by the outer shells, all these elements are hardly distinguishable chemically. A list of all these elements with their electron conﬁgurations is given in Table 4.1. The periodic table (in one of its more modern forms) is given in Fig. 4.5. You may now look at the periodic table with more knowing eyes. If you were asked, for example, why the alkali elements lithium, sodium, potassium, rubidium, caesium, and francium have a valency of one, you could answer in the following way. The properties of electrons are determined by Schrödinger’s equation. The solution of this equation for one electron and one proton tells us that the electron may be in one of a set of discrete states, each having a deﬁnite energy level. When there are many electrons and many protons, the order in which these states follow each other remains roughly unchanged. We may then derive the various elements by ﬁlling up the available states one by one with electrons. We cannot put more than one electron in a state because the exclusion principle forbids this. The energy of the states varies in steps. Within a ‘shell’ there is a slow variation in energy but a larger energy difference between shells. All the alkali elements start new shells. Therefore each of them may lose an electron; each of them may contribute one unit to a new chemical conﬁguration; and each of them has a valency of one. We may pause here for a moment. You have had the ﬁrst taste of the power of Schrödinger’s equation. You can see now that the solution of all the basic problems that have haunted the chemists for centuries is provided by

Table 4.1 The electronic conﬁgurations of the elements Atomic Element number symbol

Number of electrons 1s 2s 2p 3s 3p 3d

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36

H He Li Be B C N O F Ne Na Mg Al Si P S Cl A K Ca Sc Ti V Cr Mn Fe Co Ni Cu Zn Ga Ge As Se Br Kr

1 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2

1 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2

1 2 3 4 5 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6

1 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2

1 2 3 4 5 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6

– – 1 2 3 5 5 6 7 8 10 10 10 10 10 10 10 10

Atomic Element number symbol

4s 4p 4d 4f

1 2 2 2 2 1 2 2 2 2 1 2 2 2 2 2 2 2

1 2 3 4 5 6

–

–

37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60 61 62 63 64 65 66 67 68 69 70 71 72

Rb Sr Y Zr Nb Mo Tc Ru Rh Pd Ag Cd In Sn Sb Te I Xe Cs Ba La Ce Pr Nd Pm Sm Eu Gd Tb Dy Ho Er Tm Yb Lu Hf

Number of electrons

Atomic Element number symbol

4s 4p 4d

4f

5s 5p 5d 5f 5g 6s

2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2

– – – – – – – – – – – – – – – – – – – – –

1 2 2 2 1 1 1 1 1 – 1 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2

6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6

– – 1 2 4 5 6 7 8 10 10 10 10 10 10 10 10 10 10 10 10 10 10 10 10 10 10 10 10 10 10 10 10 10 10 10

2 3 4 5 6 7 7 8 9 10 11 12 13 14 14

– –

1 2 3 4 5 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6

– –

1 – – – – – – 1 1 1 1 1 1 1 1 2

– –

–

– –

–

– –

1 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2

Number of electrons 5p 5d 5f 5g 6s 6p 6d 6f 7s 7p

73 74 75 76 77 78 79 80 81 82 83 84 85 86 87 88 89 90 91 92 93 94 95 96 97 98 99 100

Ta W Re Os Ir Pt Au Hg Tl Pb Bi Po At Rn Fr Ra Ac Th Pa U Np Pu Am Cm Bk Cf – –

6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6

3 – – 4 5 6 9 9 10 10 10 10 10 10 10 10 10 10 10 10 10 10 10 5 10 5 10 6 10 7 10 8 10 9 10 10 10 11

2 2 2 2 0 1 1 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2 2

–

1 2 3 4 5 6 6 6 6 6 6 6 6 6 6 6 6 6 2 2

–

1 2 3 4 – 1 1 1 1 1 1 1

–

–

1 2 2 2 2 2 2 2 2 2 2 2 2 2

–

64

The hydrogen atom and the periodic table 1

2

H

He

IIIB IVB VB VIB VIIB

IA

IIA

3

4

5

6

7

8

9

10

Li

Be

B

C

N

O

F

Ne

11

12

Na Mg

IIIA

IVA

VA VIA VIIA

16

17

18

Si

P

S

Cl

Ar

29

30

31

32

33

34

35

36

Ga Ge As

Se

Br

Kr

53

54

22

23

24

K

Ca

Sc

Ti

V

Cr Mn Fe Co Ni Cu Zn

37

38

39

40

41

42

Rb

Sr

Y

Zr Nb Mo Tc

55

56

57

72

73

74

75

76

77

78

Cs Ba

La

Hf

Ta

W

Re Os

Ir

Pt

60

61

63

64

87

88

89

Ra

Ti 58

59

Ce

Pr

90

91

92

Th

Pa

U

45

28

15

Al

21

44

27

14

IIB

20

43

26

13

IB

19

Fr

25

VIII

46

47

48

Ru Rh Pd Ag Cd

62

79

80

Au Hg

65

66

67

49

50

51

52

In

Sn

Sb

Te

I

Xe

81

82

83

84

85

86

Tl

Pb

Bi

Po

At Rn

68

69

70

71

Nd Pm Sm Eu Gd Tb Dy Ho Er Tm Yb Lu 93

94

95

96

97

98

Np Pu Am Cm Bk Cf

99

100

101

102

103

Es Fm Md No

}

IIIA

Fig. 4.5 The periodic table of the elements.

a modest-looking differential equation. The chaos prevailing before has been cleared, and a sturdy monument has been erected in its stead. If you look at it carefully, you will ﬁnd that it possesses all the requisites of artistic creation. It is like a Greek temple. You can see in the background the stern regularity of the columns, but the statues placed between them are all different.

Exercises 4.1. Calculate the wavelength of electromagnetic waves needed to excite a hydrogen atom from the 1s into the 2s state. 4.2. Electromagnetic radiation of wavelength 20 nm is incident on atomic hydrogen. Assuming that an electron in its ground state is ionized, what is the maximum velocity at which it may be emitted? 4.3. An excited argon ion in a gas discharge radiates a spectral line of wavelength 450 nm. The transition from the excited to the ground state that produces this radiation takes an average time of 10–8 s. What is the inherent width of the spectral line? 4.4. Determine the most probable orbiting radius of the electron in a hydrogen atom from the following very crude considerations. The electron tries to move as near as possible

to the nucleus in order to lower its potential energy. But if the electron is somewhere within the region 0 to rm (i.e. we know its position with an uncertainty, rm ), the uncertainty in its mo~ ℏ/rm . So the kinetic energy of the mentum must be p = 2 . electron is roughly ℏ2 /2mrm Determine rm from the condition of minimum energy. Compare the radius obtained with that of the ﬁrst Bohr orbit. 4.5. Determine the average radius of an electron in the ground state of the hydrogen atom. 4.6. The spherically symmetric solution for the 2s electron (n = 2) of the hydrogen atom may be written in the form ψ(r) = A(1 + c1 r) exp(–rc0 /2),

(4.32)

Exercises where c0 is the reciprocal of the Bohr radius [see eqn (4.24)]. (i) The function given by the above equation may be referred to as the ψ200 wave function. Why? (ii) Determine c1 from the condition that eqn (4.32) satisﬁes Schrödinger’s equation. (iii) Find the corresponding energy. (iv) Determine A from the condition that the total probability of ﬁnding the electron somewhere must be unity. (v) Find the most probable orbit of the electron for the wave function of eqn (4.32) and compare your result with that given by the curve in Fig. 4.3 for n = 2.

65

4.7. Show that ψ210 as given by eqn (4.29) satisﬁes Schrödinger’s equation. Find the corresponding energy. Compare this energy with that obtained for the wave function in the previous example. Can you draw any conclusions from these results concerning the whole n = 2 shell? 4.8. Solve Schrödinger’s equation for the ground state of helium neglecting the potential term between the two electrons. What is the energy of the ground state calculated this way? The measured value is –24.6 eV. What do you think the difference is caused by? Give an explanation in physical terms. 4.9. Write down the time-independent Schrödinger equation for lithium.

Bonds

5

Striking the electric chain wherewith we are darkly bound Byron Childe Harold’s Pilgrimage Those whom God has joined together, Let no man put asunder. Marriage service

5.1

Introduction

As we have seen, an electron and a proton may strike up a companionship, the result being a hydrogen atom. We have found that the energy of the electron is a negative number, that is, the electron in the vicinity of the proton has a lower energy than it would have if it were an inﬁnite distance away, which corresponds to zero energy. The minimum comes about as some sort of compromise between the kinetic and potential energy, but the important thing is that a minimum exists. The electron comes closer to ﬁnd lower energy. Can we say the same thing about two hydrogen atoms? Would they too come close to each other in order to reduce the total energy? Yes, they come close; they combine and make up a hydrogen molecule. This combination between atoms is called a chemical bond, and the discipline that is concerned with these combinations is chemistry. You may justiﬁably ask why we talk of chemistry in a course on electrical properties of materials. Well, in a sense, chemistry is just a branch of the electrical properties of materials. The only way to explain chemical bonds is to use electrical and some speciﬁc quantum-mechanical properties. And not only is chemistry relegated to this position: metallurgy, is too. When a large number of atoms conglomerate and make up a solid, the reason is again to be sought in the behaviour of electrons. Thus, all the mechanical properties of solids, including their very solidity, spring from the nature of their electrical components. This is true in principle but not quite true in practice. We know the fundamental laws, and so we could work out everything (the outcome of all chemical reactions, the strength of all materials) if only the mathematical problems could be overcome. Bigger computers and improved techniques of numerical analysis might one day make such calculations feasible, but for the moment it is not practicable to go back to ﬁrst principles. So we are not going to solve the problems of chemistry and metallurgy here. Nevertheless, we need to understand the nature of the chemical bond to proceed further. The bond between hydrogen atoms leads to the bond between the atoms of heavier elements. We shall encounter among others germanium and silicon, their band structure, how they can be doped, and how they can serve as the basis upon which most of our electronic devices are built. Is it worth starting with the fundamentals? It is far

General mechanical properties of bonds

67

from obvious. Unless you ﬁnd these glimpses behind the scenes fascinating in themselves you might come to the conclusion that the labour to be expended is just too much. But try not to think in too narrow terms. Learning something about the foundations may help you later when confronting wider problems.

5.2 General mechanical properties of bonds Before classifying and discussing particular bond types, we can make a few common-sense deductions about what sort of forces must be involved in a bond. First, there must be an attractive force. An obvious candidate for this role is the Coulomb attraction between unlike charges, which we have all met many times, giving a force proportional to r–2 , where r is the separation. We know that sodium easily mislays its outer-ring (often called valence) electron, becoming Na+ , and that chlorine is an avid collector of a spare electron. So, just as we mentioned earlier with lithium and ﬂuorine, the excess electron of sodium will ﬁll up the energy shell of chlorine, creating a positively charged sodium ion with a negatively charged chlorine ion. These two ions will attract each other; that is obvious. What is less obvious, however, is that NaCl crystallizes into a very deﬁnite structure with the Na and Cl ions 0.28 nm apart. What stops them getting closer? Surely the Coulomb forces are great at 0.28 nm. Yes, they are great, but they are not the only forces acting. When the ions are very close to each other and start becoming distorted, new forces arise that tend to re-establish the original undistorted separate state of the ions. These repulsive forces are of short range. They come into play only when the interatomic distance becomes comparable with the atomic radius. Thus, we have two opposing forces that balance each other at the equilibrium separation, r0 . It is possible to put this argument into graphical and mathematical form. If we plot the total energy of two atoms against their separation, the graph must look something like Fig. 5.1. The ‘common-sense’ points about this diagram are as follows: 1. The energy tends to zero at large distances—in other words, we deﬁne zero energy as the energy in the absence of interaction. 2. At large distances the energy is negative and increases with increasing distance. This means that from inﬁnity down to the point r0 the atoms attract each other. 3. At very small distances the energy is rising rapidly, that is, the atoms repel each other up to the point r0 . 4. The curve has a minimum value at r0 corresponding to an equilibrium position. Here the attractive and repulsive forces just balance each other. In the above discussion we have regarded r as the distance between two atoms, and r0 as the equilibrium distance. The same argument applies, however, if we think of a solid that crystallizes in a cubic structure. We may then interpret r as the interatomic distance in the solid. Let us now see what happens when we compress the crystal, that is, when we change the interatomic distance by brute force. According to our model, illustrated in Fig. 5.1, the energy will increase, but when the external inﬂuence is removed, the crystal will return to its equilibrium position. In some other

E(r)

r0 Ec

r

Fig. 5.1 The essential general appearance of the energy versus separation curve if two atoms are to bond together. The equilibrium separation is r0 and the bond energy is Ec .

68

Bonds T

T

T a

Fig. 5.2 A cube of material, side a, is isotropically compressed.

branches of engineering this phenomenon is known as elasticity. So if we manage to obtain the E(r) curve, we can calculate all the elastic properties of the solid. Let us work out as an example the bulk elastic constant. We shall take a cubical piece of material of side a (Fig. 5.2) and calculate the energy changes under isotropic compression. If we regard E(r) as the energy per atom, the total energy of the material is Na a3 E(r0 ) in equilibrium, where Na is the number of atoms per unit volume. If the cube is uniformly compressed, the interatomic distance will decrease by r, and the total energy will increase to Na a3 E(r0 – r). Expanding E(r0 – r) into a Taylor series and noting that (∂E/∂r)r = r0 = 0, we get 1 ∂ 2E E(r0 – r) = E(r0 ) + (r)2 + · · · (5.1) 2 ∂r2 r = r0 Hence, the net increase in energy is equal to 2 1 3 ∂ E (r)2 . Na a 2 ∂r2 r = r0

(5.2)

This increase in energy is due to the work done by moving the six faces of the cube. The total change in linear dimensions is (a/r0 )r; thus we may say that each face has moved by a distance (a/2r0 )r. Hence, while the stress is increasing from 0 to T, the total work done on the piece of material is ar 1 . 6 × Ta2 2 2r0

(5.3)

From the equality of eqns (5.2) and (5.3) we get 3 a3 1 a3 ∂ 2 E T r = (r)2 , 2 r0 2 r03 ∂r2 r = r0

(5.4)

whence T=

1 3r0

∂ 2E ∂r2

r = r0

r . r0

(5.5)

Deﬁning the bulk elastic modulus by the relationship of stress to the volume change caused, that is T =c

It is worth noting that most materials do obey this Hooke’s law for small deformations, but not for large ones. This is in line with the assumptions we have made in the derivation.

3r a3 ~ 3a =c , =c 3 a r0 a

we can obtain c with the aid of eqn (5.5) in the form 1 ∂ 2E c= . 9r0 ∂r2 r = r0

(5.6)

(5.7)

So we have managed to obtain both Hooke’s law and an expression for the bulk elastic modulus by considering the interaction of atoms. If terms higher than second order are not negligible, we have a material that does not obey Hooke’s law.

Bond types

69

For the purpose of making some rough calculations, the characteristic curve of Fig. 5.1 may be approximated by the following simple mathematical expression, A B – , (5.8) rn rm where the ﬁrst term on the right-hand side represents repulsion and the second term attraction. By differentiating eqn (5.8) we can get Ec the minimum of the E(r) curve at the equilibrium distance r = r0 , in the form B m –1 . (5.9) Ec = m r0 n E(r) =

For a stable bond, Ec < 0, which can be satisﬁed only if m < n.

(5.10)

The repulsive force has a higher index than the attractive one.

5.3 Bond types There is no sharp distinction between the different types of bonds. For most bonds, however, we may say that one or the other mechanism dominates. Thus, a classiﬁcation is possible; the four main types are: (i) ionic, (ii) metallic, (iii) covalent, and (iv) van der Waals.∗

5.3.1

Ionic bonds

A typical representative of an ionic crystal is NaCl, which we have already discussed in some detail. The crystal structure is regular and looks exactly like the one shown in Fig. 1.1. We have negatively charged Cl ions and positively charged Na ions. We may now ask the question, what is the cohesive energy of this crystal? Cohesive energy is what we have denoted by Ec in Fig. 5.1, that is the energy needed to take the crystal apart. How could we calculate this? If the binding is due mainly to electrostatic forces, then all we need to do is to sum the electrostatic energy due to pairs of ions. Let us start with an arbitrary Na ion. It will have six Cl ions at a distance, a, giving the energy, e2 6 . (5.11) 4π ǫ0 a √ There are then 12 Na ions at a distance a 2 contributing to the energy by the amount –

e2 12 √ . 4π ǫ0 a 2

(5.12)

√ Next come eight chlorine atoms at a distance a 3, and so on. Adding up the contributions from all other ions, we have an inﬁnite sum (well, practically inﬁnite) of the form e2 6 12 8 – – √ + √ ··· . (5.13) 4π ǫ0 a a 2 a 3 We have to add together sums such as eqn (5.13) for every Na and Cl ion to get the cohesive energy. It would actually be twice the cohesive energy, because

∗ Johannes

Diderik Van der Waals, Nobel Prize, 1910.

70

Bonds we counted each pair twice, or we may say that it is the cohesive energy per NaCl unit. The inﬁnite summations look a bit awkward, but fortunately there are mathematicians who are fond of problems of this sort; they have somehow managed to sum up all these series, not only for the cubical structure of NaCl, but for the more complicated structures of some other ionic crystals as well. Their labour brought forth the formula

M is called the Madelung constant. For a simple cubic structure its value is 1.748.

e2 . (5.14) 4π ǫ0 a Taking a = 0.28 nm and putting the constants into eqn (5.14) we get for the cohesive energy, Electrostatic energy = –M

E = 8.94 eV,

(5.15)

which is about ten per cent above the experimentally observed value. There are other types of energies involved as well (as, e.g. the energy due to the slight deformation of the atoms) but, as the numerical results show, they must be of lesser signiﬁcance. We have thus conﬁrmed our starting point that NaCl may be regarded as an ionic bond.

5.3.2 Metallic bonds Having studied the construction of atoms, we are now in a somewhat better position to talk about metals. Conceptually, the simplest metal is a monovalent alkali metal, where each atom contributes one valence electron to the common pool of electrons. So we are, in fact, back to our very ﬁrst model, when we regarded a conductor as made up of lattice ions and charged billiard balls bouncing around. We may now ask the question: how is a piece of metal kept together? ‘By electrostatic forces’, is the simplest, though not quite accurate, answer. Thus, the metallic bond is similar to the ionic bond in the sense that the main role is played by electrostatic forces, but there is a difference as far as the positions of the charges are concerned. In metals the carriers of the negative charge are highly mobile; thus we may expect a bond of somewhat different properties. Since electrons whizz around and visit every little part of the metal, the electrostatic forces are ubiquitous and come from all directions. So we may regard the electrons as a glue that holds the lattice together. It is quite natural, then, that a small deformation does not cause fracture. Whether we compress or try to pull apart a piece of metal the cohesive forces are still there and acting vigorously. This is why metals are so outstandingly ductile and malleable.

5.3.3 The covalent bond So far we have discussed two bonds, which depend on the fact that unlike charges attract—a familiar, old but nevertheless true, idea. But why should atoms like carbon or silicon hang together? It is possible to purify silicon, so that its resistivity is several ohm metres—there can be no question of a lot of free electrons swarming around, nor is there an ionic bond. Carbon in its diamond form is the hardest material known. Not only must it form strong bonds, but they must also be exceptionally precise and directional to achieve this hardness.

Bond types The properties of the covalent bond, also called the valence or homopolar bond on occasions, is the most important single topic in chemistry, yet its mechanism was completely inexplicable before the rise of quantum mechanics. The exact mathematical description is immensely difﬁcult, even for people with degrees, so in an undergraduate course we must be modest. The most we can hope for is to get a good physical picture of the bond mechanism, and perhaps an inkling of how a theoretical physicist would start solving the problem. The simplest example of the covalent bond is the hydrogen molecule, where two protons are kept together by two electrons. The bond comes about because both electrons orbit around both atoms. Another way of describing the bond is to appeal to the atoms’ desire to have ﬁlled shells. A hydrogen atom needs two electrons (of opposite spin) to ﬁll the 1s shell, and lacking any better source of electrons, it will consider snatching that extra electron from a fellow hydrogen atom. Naturally the other hydrogen atom will resist, and at the end they come to a compromise and share both their electrons. It is as if two men, each anxious to secure two wives for himself, were to agree to share wives.∗ Another example is chlorine, which has ﬁve 3p electrons and is eagerly awaiting one more electron to ﬁll the shell. The problem is again solved by sharing an electron pair with another chlorine atom. Thus, each chlorine atom for some time has the illusion that it has managed to ﬁll its outer shell. Good examples of covalent bonds in solids are carbon, silicon, and germanium. Their electron conﬁgurations may be obtained from Table 4.1. They are as follows:

71

∗ The

analogy also works, as a feminist friend has pointed out, if two women, each anxious to secure two husbands for herself, were to agree to share husbands.

C: 1s2 , 2s2 , 2p2 Si: 1s2 , 2s2 , 2p6 , 3s2 , 3p2 Ge: 1s2 , 2s2 , 2p6 , 3s2 , 3p6 , 3d10 , 4s2 , 4p2 . It can be easily seen that the common feature is two s and two p electrons in the outer ring. The s shells (2s, 3s, 4s, respectively) are ﬁlled; so one may expect all three substances to be divalent, since they have two extra electrons in the p shells. Alas, all of them are tetravalent. The reason is that because of interaction (which occurs when several atoms are brought close together), the spherical symmetry of the outer s electrons is broken up, and they are persuaded to join the p electrons in forming the bonds. Hence, for the purpose of bonding, the atoms of carbon, silicon, and germanium may be visualized with four dangling electrons at the outside. When the atoms are brought close to each other, these electrons establish the bonds by pairing up. The four electrons are arranged symmetrically in space, and the bonds must therefore be tetrahedral, as shown in Fig. 5.3. In covalent bonds all the available electrons pair up and orbit around a pair of atoms; none of them can wander away to conduct electricity. This is why carbon in the form of diamond is an insulator.† The covalent bonds are weaker in silicon and germanium, and some of the electrons might be ‘shaken off ’ by the thermal vibrations of the crystal. This makes them able to conduct electricity to a certain extent. They are not conductors; we call them semiconductors.

† Incidentally,

carbon can have another type of bond as well. In its graphite form, consisting of layers on top of each other, it is a fairly good conductor.

72

Bonds

a

Fig. 5.3 The diamond structure. Notice that each atom is symmetrically surrounded in an imaginary cube by its four nearest neighbours. These are covalently bonded, indicated by tubular connections in the ﬁgure.

Table 5.1 Mohs hardness scale (modiﬁed) Hardness number

Material

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15

Talc Mg3 Si4 O10 (OH)2 Gypsum CaSO4 · 2H2 O Calcite CaCO3 Fluorite CaF2 Apatite Ca5 (PO4 )3 (OH, F, Cl) Orthoclase KAlSi3 O8 Vitreous Silica SiO2 Quartz, Stellite SiO2 Topaz Al2 SiO3 (OH, F)2 Garnet ZnAl2 O4 Fused Zirconia ZrO2 Fused Alumina Al2 O3 Silicon Carbide SiC Boron Carbide BC Diamond C

We have already remarked on the hardness of diamond, which is a measure of its resistance to deformation, whether it will crush, scratch, stretch, or dent. It is difﬁcult to quantify precisely—the engineers’ rule of thumb is called the Mohs scale, measured by the dent caused by a standard probe. On this scale diamond was initially given the top rating of 10, but to include more hard materials, the scale was uprated to 15, as is shown in Table 5.1. The softest material, rated 1, is the familiarly soft talcum powder. Common

Bond types abrasive materials include silicon carbide, a group IV compound with a similar diamond type covalent bond, but less symmetry; and tungsten carbide, whose bonds are partly ionic. The diamond structure also gives a high value of bulk elastic modulus [eqn (5.7)]. Diamond has two other superlatives. It has a much greater thermal conductivity than metals at room temperature, conducting energy by lattice vibrations rather than free electrons. It is thus a good heat sink for electronic devices where heat can be removed without prejudicing the electrical behaviour. As well as using ‘industrial’ rather than gem grade diamonds for this purpose, it is possible to grow suitable plane layers of diamond by molecular beam epitaxy and related techniques described in a little more detail in Section 8.11. The second superlative that takes us out of science and into high ﬁnance is the ‘sparkle’ of diamond in jewellery. But see Table 10.1; it is the high refractive index which makes sparklers. The sale of diamonds of jewel quality is controlled by the Central Selling Organisation (CSO) of de Beers who in 1948 hired a New York advertising agency to create a slogan to stimulate their industry. The young lady assigned to this task thought long and hard, weeks passed with no idea. She thought she would work on this forever, so said “diamonds are forever”. It was a great success. Carbon dating is an important impact of science on ancient history and archaeology, removing some of the luxury of literary speculation from its practitioners. Atmospheric CO2 , which is the source of carbon in living organisms, contains 1 atom of C14 in 7.8 × 1011 atoms of stable C12 . C14 , decays with a half-life of 5700 years emitting an electron. These extreme numbers result in appreciable radioactivity, giving 15 disintegrations per gram per minute. When the organism dies the intake of atmospheric CO2 stops and the C14 within it decays exponentially. Thus, a count of radioactivity in dead bones or wood etc. will give a dating for the time of death. In the two decades after 1950, scientiﬁc archaeology matured rapidly with the advent of the nuclear physics-based methods of carbon and thermoluminescent dating. Samples of diamonds from ancient jewels and numerous samples mined in the past two centuries were dated. They were all found to have been formed within an order of magnitude of 109 years ago. On a human scale, 109 years is pretty close to ‘forever’. So the slogan is more accurate than the average advertisement. Diamonds are not always forever. Their one vice is that at 700 ◦ C in air they burn to carbon dioxide. This rules out diamond for large-scale cutting of steels and other hard metals. It has stimulated research for hard compounds with better temperature stability and hardness perhaps even greater than 15 on the Mohs scale. Compounds of C with N, B, and Si have shown promise, the possible winner is C3 N4 ; but not yet.

5.3.4 The van der Waals bond If the outer shell is not ﬁlled, atoms will exert themselves to gain some extra electrons, and they become bonded in the process. But what happens when the shell is already ﬁlled, and there are no electrostatic forces either, as for example in argon? How will argon solidify? For an explanation some quantum-mechanical arguments are needed again.

73

74

The forces in van der Waals bonds are fairly weak (and may be shown to vary with the inverse seventh power of distance); consequently these materials have low melting and boiling points.

Bonds We have described the atoms as consisting of a positive nucleus and the electrons around the nucleus, with the electrons having certain probabilities of being in certain places. Since the electrons are sometimes here and sometimes there, there is no reason why the centres of positive and negative charge should always be coincident. Thus, we could regard atoms as ﬂuctuating dipoles. If atom A has a dipole moment, then it will induce an opposite dipole moment on atom B. On average there will be an attractive force, since the tendency described leads always to attraction, never to repulsion. This attraction is called a van der Waals bond. Such bonds are responsible for the formation of organic crystals. Searching for an anthropomorphic analogy once more (it’s good because it aids the memory) we could look at a dipole as a permanent bond between a man and a woman established by mutual attraction. Now would two such dipoles attract each other? To facilitate the discussion let us introduce the notation m1 and m2 , and w1 and w2 for the two men and two women in dipoles 1 and 2 respectively. For an attractive force to develop between two dipoles all we need is that the attraction between m1 and w2 , and m2 and w1 should be stronger than the repulsions between m1 and m2 and w1 and w2 . In a modern society this is indeed the likely thing to happen. The attraction can be there without the need to break the bond.

5.3.5

Mixed bonds

In most practical cases the bonds are of course not any of these pure types. An example of a mixed bond is that in carbon steel in which the presence of both metallic and ionic bonds leads to a material with considerably more strength than that of iron on its own. Mixed bonds of particular signiﬁcance to the semiconductor industry are some III–V and II–VI compounds (where the Roman numbers refer to the respective columns in the periodic table of Fig. 4.5) as for example GaAs or ZnSe. They have a combination of ionic and covalent bonds. We shall discuss their properties in more detail in Section 8.6.

5.3.6

Fig. 5.4 A view of C60 containing pentagonal and hexagonal structure.

Carbon again

It may be worth noting that the diamond structure is not the only one in which carbon can crystallize. Another form is graphite, which consists of arrays of hexagons stuck together in ﬂat sheets. Interestingly, and rather unexpectedly, lots of further crystalline forms of carbon have been discovered in the last two decades. Their signiﬁcance in engineering is not obvious as yet, but they are certainly fun to look at. We shall show here only the one discovered earliest, which gave the name of fullerenes to the family after Buckminster Fuller, a US architect who originated the geodesic dome of similar shape. It comes about by removing an atom from some of the hexagons. The sheet may then fold up into a conﬁguration of 60 atoms containing 12 pentagons and 20 hexagons as shown in Fig. 5.4. It resembles a football, which would be a better name for it. Alas, the architects got there ﬁrst. A further allotrope of carbon, graphene, exists in the form of ﬂat sheets one atom thick. The Nobel Prize in Physics was awarded to its discoverers, Andre Geim and Konstantin Novoselov of the University of

Feynman’s coupled mode approach Manchester, in 2010. It can be isolated very simply in a process known as exfoliation, by using adhesive tape to peel off very thin graphitic ﬂakes from a lump of graphite. However, a wide variety of other more conventional deposition methods exist, including chemical vapour deposition on metal catalyst substrates such as nickel. The atoms are arranged in a hexagonal or honeycomb lattice. Graphene is extremely strong, with an ultimate tensile strength over 100 times greater than steel. It also has extremely high electron mobility at room temperature, above 15,000 cm2 V–1 S–1 . As a result, it is currently being extensively investigated for applications as the conducting channel in a ﬁeld effect transistor. Progress has been rapid and the ﬁrst graphene based integrated circuit was announced in 2011 (by IBM). Graphene is both recyclable and sustainable. However the difﬁculties of processing such a material, which may literally vanish in a puff of smoke (or CO2 ) if heated, are formidable. Another interesting conﬁguration is the tube which has a thin wall that usually consists of a single layer and may be a hundred atoms long. The family, called nanotubes, may lead to a new type of transistor as discussed brieﬂy later in Section 9.27 concerned with nanoelectronics. Talking about carbon we should mention the existence of double and triple bonds, which play a crucial role in organic and polymer chemistry. The single covalent bond, which can be expressed in terms of molecular orbitals, occurs when two dangling bonds pair up so that their electron orbitals merge to form a cylindrical two-electron cloud shared between the two atoms. Since this looks similar to a pair of s orbitals (quantum number l = 0, Section 4.2) it is called a σ bond. When two carbon atoms are so paired, they can each have three spare bonds. These can be combined with other elements (e.g. H), or a pair perpendicular to the plane of the σ bond can form a weaker bond by sharing electrons with a similar structure of two p orbitals (l = 1, see Fig. 4.4) called a π bond. Going even further, a gas such as acetylene (C2 H2 ) has the carbons joined to each other and to hydrogen by σ bonds, leaving two pairs of 2p electrons perpendicular to the plane of the carbon σ bond, which form two π bonds. These three bond types contribute hugely to the complexity and versatility of organic chemistry.∗

5.4 Feynman’s coupled mode approach We are now going to discuss a more mathematical theory of the covalent bond, or rather of its simplest case, the bonding of the hydrogen molecule. We shall do this with the aid of Feynman’s (Nobel Prize, 1965) coupled modes. This approach proved amazingly powerful in Feynman’s hands, enabling him to explain, besides the hydrogen molecule, such diverse phenomena as the nuclear potential between a proton and a neutron, and the change of the K◦ particle into its own antiparticle. There is in fact hardly a problem in quantum mechanics that Feynman could not treat by the technique of coupled modes. Of necessity, we shall be much less ambitious and discuss only a few relatively simple phenomena. I should really start by deﬁning the term ‘coupled mode’. But to deﬁne is to restrict, to put a phenomenon or a method into a neat little box in contradistinction to other neat little boxes. I am a little reluctant to do so in the present

75

∗ For

more about organic bonds and crystals see Appendix I.

76

Bonds instance because I am sure I would then exclude many actual or potential applications. Not being certain of the limitations of the approach, I would rather give you a vague description, just a general idea of the concepts involved. The coupled mode approach is concerned with the properties of coupled oscillating systems like mechanical oscillators (e.g. pendulums), electric circuits, acoustic systems, molecular vibrations, and a number of other things you might not immediately recognize as oscillating systems. The approach was quite probably familiar to the better physicists of the nineteenth century but has become fashionable only recently. Its essence is to divide the system up into its components, investigate the properties of the individual components in isolation, and then reach conclusions about the whole system by assuming that the components are weakly coupled to each other. Mathematicians would call it a perturbation solution because the system is perturbed by introducing the coupling between the elements. First of all we should derive the equations. These, not unexpectedly, turn out to be coupled linear differential equations. Let us start again with Schrödinger’s equation [eqn (3.4)], but put it in the operator form, that is

The operator in parentheses is usually called the Hamiltonian operator and denoted by H.

2 ∂ ℏ 2 . – ∇ + V = iℏ 2m ∂t

(5.16)

We may also write Schrödinger’s equation in the simple and elegant form H = iℏ

∂ . ∂t

(5.17)

We have attempted [eqn (3.7)] the solution of this partial differential equation before by separating the variables, = w(t)ψ(r).

(5.18)

Let us try to do the same thing again but in the more general form, = wj (t)ψj (r), (5.19) j

where a number of solutions (not necessarily ﬁnite) are superimposed. Up to now we have given all our attention to the spatial variation of the wave function. We have said that if an electron is in a certain state, it turns up in various places with certain probabilities. Now we are going to change the emphasis. We shall not enquire into the spatial variation of the probability at all. We shall be satisﬁed with asking the much more limited question: what is the probability that the electron (or more generally a set of particles) is in state j at time t? We do not care what happens to the electron in state j as long as it is in state j. We are interested only in the temporal variation, that is, we shall conﬁne our attention to the function w(t). We shall get rid of the spatial variation in the following way. Let us substitute eqn (5.19) into eqn (5.17) j

wj Hψj = iℏ

j

ψj

dwj , dt

(5.20)

Feynman’s coupled mode approach

77

then multiply both sides by ψk and integrate over the volume. We then obtain dwj (5.21) wj ψk Hψj dv = iℏ ψj ψk dv, dt j

j

where dv is the volume element. Now ψj and ψk are two solutions of the time-independent Schrödinger equation, and they have the remarkable property (I have to ask you to believe this) of being orthogonal to each other. You may have met simple examples of orthogonality of functions before, if at no other place than in the derivation of the coefﬁcients of a Fourier series. The condition can be simply stated in the following form, Ckj if k = j, ψk ψj dv = (5.22) 0 if k = j. Multiplying the wave function with judiciously chosen constants, Ckj can be made unity, and then the wave functions are called orthonormal. Assuming that this is the case and introducing the notation, Hkj = ψk Hψj dv, (5.23) we get the following differential equations:∗ iℏ

dwk = Hkj wj dt

∗ The

(5.24)

j

for each value of k. This is the equation we sought. It is independent of the spatial variables and depends only on time. It is therefore eminently suitable for telling us how the probability of being in a certain state varies with time. You may quite justiﬁably worry at this point about how you can ﬁnd the wave functions, how you can make them orthonormal, and how you can evaluate integrals looking as complex as eqn (5.23). The beauty of Feynman’s approach is that neither the wave function nor Hkj need be calculated. It will sufﬁce to guess Hkj on purely physical grounds. We have not so far said anything about the summation. How many wave functions (i.e. states) are we going to have? We may have an inﬁnite number, as for the electron in a rigid potential well, or it may be ﬁnite. If, for example, only the spin of the electron matters, then we have two states and no more. The summation should run through j = 1 and j = 2. Two is of course the minimum number. In order to have coupling, one needs at least two components, and it turns out that two components are enough to reach some quite general conclusions about the properties of coupled systems. So the differential equations we are going to investigate appear as follows: dw1 = H11 w1 + H12 w2 , dt dw2 iℏ = H21 w1 + H22 w2 . dt

iℏ

(5.25) (5.26)

derivation would be analogous if, instead of one electron, a set of particles were involved. Schrödinger’s equation would then be written in terms of a set of spatial variables and there would be multiple integrals instead of the single integral here. The integrations would be more difﬁcult to perform, but the ﬁnal form would still be that of eqn (5.24).

78

Bonds If H12 = H21 = 0 the two states are not coupled. Then the differential equation for state (1) is iℏ

dw1 = H11 w1 , dt

(5.27)

which has a solution H11 w1 = K1 exp –i t . ℏ

(5.28)

The probability of being in state (1) is thus |w1 (t)|2 = |K1 |2 .

(1)

⊗

⊗

(2)

⊗

⊗

Electron Protons

Fig. 5.5 The two basic states of the hydrogen molecular ion. The shaded area represents the electron in its ground state. It is attached either to proton 1 or to proton 2.

When the electron jumps from one proton to the other proton, it introduces coupling between the two states.

(5.29)

This is not a very exciting solution, but it is at least consistent. If there is no coupling between the states, then the probability of being in state (1) does not vary with time—once in state (1), always in state (1). The same is true, of course, for state (2). In the absence of coupling nothing changes. Before solving the coupled differential equations, let us brieﬂy discuss the physical concepts of uncoupled states and the meaning of coupling. What do we mean exactly by coupling? We can explain this with our chosen example, the hydrogen molecule, or better still the even simpler case, the hydrogen molecular ion. The hydrogen molecular ion consists of a hydrogen atom to which a proton is attached. We may then imagine our uncoupled states as shown in Fig. 5.5. We choose for state (1) the state when the electron is in the vicinity of proton 1 and occupying the lowest energy (ground) level, and proton 2 is just alone with no electron of its own. State (2) represents the alternative arrangement when the electron is attached to proton 2 and proton 1 is bare. When we say that we consider only these two states, we are not denying the existence of other possible states. The electron could be in any of its excited states around the proton, and the whole conﬁguration of three particles may vibrate, rotate, or move in some direction. We are going to ignore all these complications. We say that as far as our problem is concerned, only the two states mentioned above are of any signiﬁcance. What do we mean when we say that these two states are uncoupled? We mean that if the electron is at proton 1 in the beginning, it will always stay there. Similarly, if the electron is at proton 2 in the beginning, it will always stay at proton 2. Is this complete separation likely? Yes, if the protons are far from each other, this is the only thing that can happen. What can we expect when the protons are brought closer to each other? Classically, the electron that is in the vicinity of proton 1 should still remain with proton 1 because this is energetically more favourable. The electron cannot leave proton 1 because it faces an adverse potential barrier. According to the laws of quantum mechanics, this is no obstacle, however. The electron may tunnel through the potential barrier and arrive at proton 2 with energy unchanged. Thus, as the two protons approach each other, there is an increasing probability that the electron jumps over from proton 1 to proton 2 and vice versa. And this is what we mean by coupling. The two states are not entirely separate.

Feynman’s coupled mode approach What do we mean by weak coupling? It means that even in the presence of coupling, it is still meaningful to talk about one or the other state. The states inﬂuence each other but may preserve their separate entities. Let us return now to the solution of equations (5.25) and (5.26). As we are going to investigate symmetric cases only, we may introduce the simpliﬁcations H11 = H22 = E0 ,

H12 = H21 = –A,

(5.30)

leading to dw1 = E0 w1 – Aw2 , dt dw2 = –Aw1 + E0 w2 . iℏ dt iℏ

(5.31) (5.32)

Following the usual recipe, the solution may be attempted in the form E w1 = K1 exp –i t , ℏ

E w2 = K2 exp –i t . ℏ

(5.33)

Substituting eqn (5.33) into equations (5.31) and (5.32) we get K1 E = E0 K1 – AK2

(5.34)

K2 E = –AK1 + E0 K2 ,

(5.35)

and

which have a solution only if E0 – E –A –A E0 – E = 0.

(5.36)

Expanding the determinant we get

(E0 – E)2 = A2 ,

(5.37)

E = E0 ± A.

(5.38)

whence

If there is no coupling between the two states, then E = E0 ; that is, both states have the same energy. If there is coupling, the energy level is split. There are two new energy levels E0 + A and E0 – A. This is a very important phenomenon that you will meet again and again. Whenever there is coupling, the energy splits. The energies E0 ± A may be deﬁned as the energies of so-called stationary states obtainable from linear combinations of the original states. For our purpose it will sufﬁce to know that we can have states with energies E0 + A and E0 – A.

79

Energy E

80

Bonds

A Eo d

Fig. 5.6

Energy

The variation of E0 and A with the interproton separation, d. E0 is the energy when the states shown in Fig. 5.5 are uncoupled. A is the coupling term.

E0 + A d E0 – A

Fig. 5.7 Summing the quantities in Fig. 5.6 to get E0 + A and E0 – A. The latter function displays all the characteristics of a bonding curve.

∗ If

you permit us a digression in a digression, I should like to point out that Yukawa, a Japanese, was the ﬁrst nonEuropean ever to make a signiﬁcant contribution to theoretical physics. Many civilizations have struck independently upon the same ideas, as for example the virgin births of gods or the commandments of social conduct, invented independently useful instruments like the arrow or the wheel, and developed independently similar judicial procedures and constitutions, but, interestingly, no civilization other than the European one bothered about theoretical physics.

How will these energies vary with d, the distance between the protons? What is A anyway? A has come into our equations as a coupling term. The larger A, the larger the coupling, and the larger the split in energy. Hence A must be related to the tunnelling probability that the electron may get through the potential barrier between the protons. Since tunnelling probabilities vary exponentially with distance—we have talked about this before when solving Schrödinger’s equation for a tunnelling problem—A must vary roughly in the way shown in Fig. 5.6. Now what is E0 ? It is the energy of the states shown in Fig. 5.5. It consists of the potential and kinetic energies of the electron and of the potential energies of the protons (assumed immobile again). When the two protons are far away, their potential energies are practically zero, and the electron’s energy, since it is bound to a proton, is a negative quantity. Thus, E0 is negative for large interproton distances but rises rapidly when the separation of the two protons is less than the average distance of the ﬂuctuating electron from the protons. A plot of E0 against d is also shown in Fig. 5.6. We may now obtain the energy of our states by forming the combinations E0 ± A. Plotting these in Fig. 5.7, we see that E0 – A has a minimum, that is, at that particular value of d a stable conﬁguration exists. We may also argue in terms of forces. Decreasing energy means an attractive force. Thus, when the protons are far away, and we consider the state with the energy E0 – A, there is an attractive force between the protons. This will be eventually balanced by the Coulomb repulsion between the protons, and an equilibrium will be reached. Thus, in order to explain semi-quantitatively the hydrogen molecular ion, we have had to introduce a number of new or fairly new quantum-mechanical ideas.

5.5

Nuclear forces

Feynman in his Lectures on Physics goes on from here and discusses a large number of phenomena in terms of coupled modes. Most of the phenomena are beyond what an engineering undergraduate needs to know; so with regret we omit them. (If you are interested you can always read Feynman’s book.) But I cannot resist the temptation to follow Feynman in saying a few words about nuclear forces. With the treatment of the hydrogen molecular ion behind us, we can really acquire some understanding of how forces between protons and neutrons arise. It is essentially the same idea that we encountered before. A hydrogen atom and a proton are held together owing to the good services of an electron. The electron jumps from the hydrogen atom to the proton converting the latter into a hydrogen atom. Thus, when a reaction H, p → p, H

(5.39)

takes place, a bond is formed. Yukawa∗ proposed in the middle of the 1930s that the forces between nucleons may have the same origin. Let us take the combination of a proton and a neutron. We may say again that a reaction p, n → n, p

(5.40)

The hydrogen molecule

81

takes place, and a bond is formed. ‘Something’ goes over from the proton to the neutron which causes the change, and this ‘something’ is called a positively charged π -meson. Thus, just as an electron holds together two protons in a hydrogen molecular ion, in the same way a positively charged π -meson holds together a proton and a neutron in the nucleus.

5.6 The hydrogen molecule The hydrogen molecule differs from the hydrogen molecular ion by having one more electron. So we may choose our states as shown in Fig. 5.8. State (1) is when electron a is with proton 1 and electron b with proton 2, and state (2) is obtained when the electrons change places. How do we know which electron is which? Are they not indistinguishable? Yes, they are, but we may distinguish them by assigning opposite spins to them. We may now explain the bond of the hydrogen molecule in a manner analogous to that of the hydrogen molecular ion, but instead of a single electron jumping to and fro, we now have two electrons changing places. Thus, we may argue again that owing to symmetry, the energies of the two states are identical. The coupling between the states—due to the exchange of electrons—splits the energy levels, one becoming somewhat higher, the other somewhat lower. Having the chance to lower the energy results in an attractive force which is eventually balanced by the repulsive force between the protons. And that is the reason why the hydrogen molecule exists. It is interesting to compare this picture with the purely intuitive one described earlier, based on the atoms’ ‘desire’ to ﬁll the energy shells. In the present explanation we are saying that the bond is due to the exchange of electrons; previously we said the bond was due to sharing of the electrons. Which is it; is it sharing or swapping? It is neither. Both explanations are no more than physical pictures to help the imagination. We could equally well have said that the hydrogen molecule exists because it comes out mathematically from our basic premises, that is the spin and Pauli’s principle added to Schrödinger’s equation. The problem is a purely mathematical one, which can be solved by numerical methods. There is no need, whatsoever, for a physical picture. This argument would hold its ground if numerical solutions were always available. But they are not available. Computers are not powerful enough, not as yet and will not be for a long time to come. So we need mathematical approximations based on a simpliﬁed physical picture and then we must strive to build up a new, more sophisticated physical picture from the mathematical solution obtained, and then attempt a better mathematical approximation based on the new physical picture, and so on, and so on. It seems a tortuous way of doing things, but that is how it is. It is a lot easier in classical physics. Our physical picture is readily acquired in conjunction with our other faculties. We do not need to be taught that two bricks cannot occupy the same place: we know they cannot. In studying phenomena concerned with extremely small things beyond the powers of direct observation, the situation is different. The picture of an atom with ﬁlled and unﬁlled energy shells is not a picture acquired through personal experience. It has come about by solving a differential equation. But once the solution is obtained, a physical picture starts emerging. We may visualize little

b

a (1)

+

(2)

+

+

b

a +

Fig. 5.8 The two basic states of the hydrogen molecule. Each electron can be attached to either proton leading to a coupling between the states.

82

Bonds boxes, or concentric spheres, or rows of seats in the House of Commons ﬁlling up slowly with MPs. The essential thing is that we do form some kind of picture of the energy shells. And once the shell picture is accepted, it helps us ﬁnd an explanation for the next problem, the bond between the atoms. So you should not be unduly surprised that many alternative explanations are possible. They reﬂect attempts to develop intuition in a discipline where intuition does not come in a natural way. Whenever confronted with new problems, one selects from this store of physical pictures the ones likely to be applicable. If one of the physical pictures does turn out to be applicable, it is a triumph both for the picture and for the person who applied it. If all attempts fail, then either a new physical picture or a brighter person is needed to tackle the problem.

5.7

An analogy

One of the most important conclusions of the foregoing discussion was that ‘whenever there is coupling, the energy levels split’. This is a very important relationship in quantum mechanics, but it could also be regarded as a simple mathematical consequence of the mathematical formulation. If we have coupled differential equations, something will always get split somewhere. The example we are all familiar with is that of coupled electric resonant circuits shown in Fig. 5.9. If the two circuits are far away from each other, that is they are uncoupled, both of them have resonant frequencies ω0 . When the circuits are coupled, there are two resonant frequencies ω0 ± a, that is, we may say the resonant frequencies are split. Response

Fig. 5.9

M

The coupled circuit analogy. Two resonant circuits tuned to ω0 when far apart (no coupling between them), have their resonant frequency split to ω0 ± a (cf. E0 ± A) when coupled.

ω 0 – a ω0

ω0 + a

Frequency

Exercises 5.1. Discuss qualitatively the various mechanisms of bonding. Give examples of materials for each type of bond and also materials that do not have a clear single bond type. 5.2. Show that the force between two aligned permanent dipoles, a distance r apart, is attractive and varies as r–4 . r

————– +≺ – +≻ – d˙ d˙ ↔

↔

5.3. The interaction energy between two atoms may be phenomenologically described by eqn (5.8). Show that the molecule will break up when the atoms are pulled apart to a distance rb =

n+1 m+1

1/(n–m)

r0 ,

Exercises where r0 is the equilibrium distance between the atoms. Discuss the criterion of breaking used to get the above result. 5.4. For the KCl crystal the variation of energy may also be described by eqn (5.8), but now r means the interatomic distance in the cubic crystal, and the energy is for an ion pair. Take m = 1, n = 9, B = 1.75e2 /4π ǫ0 . The bulk modulus of elasticity is 1.88 × 1010 N m–2 . Calculate the separation of the K+ – Cl– ions in the ionic solid. 5.5. Show with the aid of eqns (5.7)–(5.9) that the bulk modulus may be obtained in the form

83 c=–

mn Ec . 9r03

5.6. Calculate the energy of a negative ion in a linear chain of equally spaced ions, which carry alternative positive and negative charges. 5.7. For a symmetrical coupled system, the decrease in energy (with respect to the uncoupled case) is A, as shown by eqn (5.38). Show that, for an unsymmetrical system (H11 = H22 ) with the same coupling (H12 H21 = A2 ), the decrease in energy is less than A.

6

The free electron theory of metals Struggling to be free, art more engaged Hamlet Much have I travelled in the realms of gold, And many goodly states and kingdoms seen. Keats On First Looking in Chapman’s Homer

6.1

The electrons inside the metal (more correctly, the valence electrons, which occupy the outer ring) are entirely free to roam around, but they are not allowed to leave the metal.

Free electrons

The electrical and magnetic properties of solids are mainly determined by the properties of electrons in them. Protons can usually be relegated to subordinate roles, like ensuring charge neutrality. Neutrons may sometimes need to be considered, as for example in some superconducting materials, in which the critical temperature depends on the total mass of the nucleus, but on the whole, the energy levels of electrons hold the key to the properties of solids. The mathematical problem is not unlike the one we met in the case of individual atoms. How can we determine the energy levels of electrons in a solid? Take a wave function depending on the coordinates of 1025 electrons; write down the Coulomb potential between each pair of electrons, between electrons and protons; and solve Schrödinger’s equation. This is an approach which, as you have probably guessed, we are not going to try. But what can we do instead? We can take a much simpler model, which is mathematically soluble, and hope that the solution will make sense. Let us start our search for a simple model by taking a piece of metal and noting the empirical fact (true at room temperature) that there are no electrons beyond the boundaries of the metal. So there is some mechanism keeping the electrons inside. What is it? It might be an inﬁnite potential barrier at the boundaries. And what about inside? How will the potential energy of an electron vary in the presence of that enormous number of nuclei and other electrons? Let us say it will be uniform. You may regard this as a sweeping assumption (and, of course, you are absolutely right), but it works. It was introduced by Sommerfeld in 1928, and has been known as the ‘free electron’ model of a metal. You may recognize that the model is nothing else but the potential well we met before. There we obtained the solution for the one-dimensional case in the following form, E=

h2 n2 ℏ2 k 2 = . 2m 8 m L2

(6.1)

The density of states and the Fermi–Dirac distribution

85

If we imagine a cube of side L containing the electrons, then we get for the energy in the same manner E=

ℏ2 2 h2 2 2 2 n . kx + ky2 + kz2 = + n + n x y z 2m 8 mL2

(6.2)

nx , ny , nz are integers.

6.2 The density of states and the Fermi–Dirac distribution The allowed energy, according to eqn (6.2), is an integral multiple of h2 /8 mL2 . For a volume of 10–6 m3 this unit of energy is Eunit =

(6.62 × 10–34 )2 = 0.6 × 10–33 J = 3.74 × 10–15 eV. 8 × 9.1 × 10–31 × 10–4

(6.3)

~ 1.22 × 10–7 eV, E =

(6.4)

This is the energy difference between the ﬁrst and second levels, but since the squares of the integers are involved, the difference between neighbouring energy levels increases at higher energies. Let us anticipate the result obtained in the next section and take for the maximum energy E = 3 eV, which is a typical ﬁgure. Taking n2x = n2y = n2z , this maximum energy corresponds to a ~ 1.64 × 107 . Now an energy level just below the maximum energy value of nx = can be obtained by taking the integers nx – 1, nx , nx . We get for the energy difference

We can therefore say that, in a macroscopically small energy interval d E, there are still many discrete energy levels. So we can introduce the concept of density of states, which will simplify our calculations considerably. The next question we ask is how many states are there between the energy levels E and E + d E? It is convenient to introduce for this purpose the new variable n with the relationship n2 = n2x + n2y + n2z .

(6.5)

Thus n represents a vector to a point nx , ny , nz in three-dimensional space. In this space every point with integer coordinates speciﬁes a state; that is, a unit cube contains exactly one state. Hence, the number of states in any volume is just equal to the numerical value of the volume. Thus, in a sphere of radius n, the number of states is 4n3 π . 3

(6.6)

Since n and E are related, this is equivalent to saying that the number of states having energies less than E is 4n3 π 4π 3/2 3/2 = K E 3 3

with K =

8 mL2 . h2

(6.7)

Similarly, the number of states having energies less than E + d E is 4π 3/2 K (E + d E)3/2 . 3

(6.8)

Even at the highest energy, the difference between neighbouring energy levels is as small as 10–7 eV.

86

The free electron theory of metals So the number of states having energies between E and E + d E is equal to 4π 3/2 Z(E)d E = K (E + d E)3/2 – E3/2 3 ~ 2π K 3/2 E1/2 d E. (6.9) = This is not the end yet. We have to note that only positive values of nx , ny , nz are permissible; therefore we have to divide by a factor 8. Allowing further for the two values of spin, we have to divide by 4 only. We get ﬁnally Z(E)d E = C E1/2 d E

Enrico Fermi (Nobel Prize, 1938) and Paul Dirac (Nobel Prize, 1933) both made fundamental contributions to quantum mechanics. ∗ If

we use the assumption that a state may contain any number of particles, the so-called Bose–Einstein distribution is obtained. It turns out that all particles belong to one or the other of these distributions and are correspondingly called fermions or bosons. For this book, it is of great importance that electrons are fermions and they obey the Fermi–Dirac distribution. The properties of bosons (e.g. quantized electromagnetic waves and lattice waves) are of somewhat less signiﬁcance. We occasionally need to refer to them as photons and phonons but their statistics is usually irrelevant for our purpose. The Bose–Einstein distribution, and the so-called boson condensation do come into the argument in Section 12.14, where we talk brieﬂy about atom lasers and in Chapter 14 concerned with superconductivity, but we shall not need any mathematical formulation of the distribution function.

with C =

4π L3 (2 m)3/2 . h3

(6.10)

Equation (6.10) gives us the number of states, but we would also like to know the number of occupied states, that is, the number of states that contain electrons. For that we need to know the probability of occupation, F(E). This function can be obtained by a not-too-laborious exercise in statistical mechanics. One starts with the Pauli principle (that no state can be occupied by more than one electron) and works out the most probable distribution on the condition that the total energy and the total number of particles are given. The result is the so-called Fermi–Dirac distribution∗ F(E) =

1 , exp{(E – EF )/kB T} + 1

(6.11)

where EF is a parameter called the Fermi level. It has the easily memorized property that at E = EF ,

F(E) =

1 , 2

(6.12)

that is, at the Fermi level the probability of occupation is 12 . As may be seen in Fig. 6.1, F(E) looks very different from the classical distribution exp(–E/kT). Let us analyse its properties in the following cases: 1. At T = 0. F(E) = 1 F(E) = 0

for

E < EF E > EF .

(6.13)

Thus, at absolute zero temperature, all the available states are occupied up to EF , and all the states above EF are empty. But remember, Z(E) d E is the number of states between E and E + d E. Thus, the total number of states is EF Z(E) d E, (6.14) 0

which must equal the total number of electrons NL3 , where N is the number of electrons per unit volume. Thus, substituting eqn (6.10) into eqn (6.14), the following equation must be satisﬁed: EF 4π L3 (2 m)3/2 /h3 E1/2 d E = NL3 . (6.15) 0

The density of states and the Fermi–Dirac distribution 1

F(E) = 1 + exp

( ( E–EF

exp (–E/kBT)

kBT

1.0

87

1.0

T= 0 K

Maxwell–Boltzmann

600 K 0.5

6000 K

T= 0 K 600 K

Fermi–Dirac

6000 K (a)

EF = 2.5 eV

E

2.5 eV

(b)

E

Fig. 6.1 (a) The Fermi–Dirac distribution function for a Fermi energy of 2.5 eV and for temperatures of 0 K, 600 K, and 6000 K. (b) The classical Maxwell–Boltzmann distribution function of energies for the same temperatures.

Integrating and solving for EF , we get EF =

h2 2m

3N 8π

2/3

.

(6.16)

EF , calculated from the number of free electrons, is shown in Table 6.1. Thus, even at absolute zero temperature, the electrons’ energies cover a wide range. This is strongly in contrast with classical statistics, where at T = 0, all electrons have zero energy. 2. For electron energies above the Fermi level, so that E – EF ≫ kB T, the term unity in eqn (6.11) may be neglected, leading to

~ exp – (E – EF ) , F(E) = kB T

(6.17)

(6.18)

Table 6.1 Fermi levels of metals calculated from eqn (6.16) Li Na K Rb Cs Cu Ag Al

4.72 eV 3.12 eV 2.14 eV 1.82 eV 1.53 eV 7.04 eV 5.51 eV 11.70 eV

which you may recognize as the classical Maxwell–Boltzmann distribution. That is, for sufﬁciently large energies the Fermi–Dirac distribution is reduced to the Maxwell–Boltzmann distribution, generally referred to as the ‘Boltzmann tail’. 3. For electron energies below the Fermi level, so that EF – E ≫ kB T,

(6.19)

eqn (6.11) may be approximated by ~ 1 – exp F(E) =

(E – EF ) . kB T

(6.20)

It is sometimes useful to talk about the probability of a state not being occupied and use the function 1 – F(E). We may say then, for the present case, that the probability of non-occupation varies exponentially.

The probability of a state being occupied is very close to unity.

88

The free electron theory of metals 4. In the range E ≈ EF the distribution function changes rather abruptly from nearly unity to nearly zero. The rate of change depends on kB T. For absolute zero temperature the change is inﬁnitely fast, for higher temperatures (as can be seen in Fig. 6.1) it is more gradual. We may take this central region (quite arbitrarily) as between F(E) = 0.9 and F(E) = 0.1. The width of the region comes out then [by solving eqn (6.11)] to about 4.4 kB T. Summarizing, we may distinguish three regions for ﬁnite temperatures: from E = 0 to E = EF – 2.2 kB T, where the probability of occupation is close to unity, and the probability of non-occupation varies exponentially; from E = EF – 2.2 kB T to E = EF + 2.2 kB T, where the distribution function changes over from nearly unity to nearly zero; and from E = EF + 2.2 kB T to E = ∞, where the probability of occupation varies exponentially.

6.3

The speciﬁc heat of electrons

Classical theory, as we have mentioned before (Section 1.8), failed to predict the speciﬁc heat of electrons. Now we can see the reason. The real culprit is not the wave nature of the electron nor Schrödinger’s equation but Pauli’s principle. Since only one electron can occupy a state, electrons of lower energy are not in a position to accept the small amount of energy offered to them occasionally. The states above them are occupied, so they stay where they are. Only the electrons in the vicinity of the Fermi level have any reasonable chance of getting into states of higher energy; so they are the only ones capable of contributing to the speciﬁc heat. The speciﬁc heat at constant volume per electron is deﬁned as dE , (6.21) dT where E is the average energy of electrons. A classical electron would have an average energy 3/2 kB T, which tends to zero as T → 0. Quantum-mechanically, if an electron satisﬁes the Fermi–Dirac statistics, then the average energy of the electrons is ﬁnite and can quite easily be determined (see Exercise 6.6). For the purpose of estimating the speciﬁc heat, we may make up a simple argument and claim that only the electrons in the region E = EF – 2.2 kB T to E = EF need to be considered as being able to respond to heat, and they can be regarded as if they were classical electrons possessing an energy (3/2) kB T. Hence the average energy of these electrons is 3 2.2 kB T E = kB T , (6.22) 2 EF cv =

which gives for the speciﬁc heat, cv = 6.6

kB 2 T. EF

(6.23)

A proper derivation of the speciﬁc heat would run into mathematical difﬁculties, but it is very simple in principle. The average energy of an electron following a distribution F(E) is given by 1 ∞ F(E)Z(E)E d E, (6.24) E = N 0

Thermionic emission which should be evaluated as a function of temperature∗ and differentiated. The result is cv =

π 2 kB 2 T, 2 EF

89 ∗ See,

for example. F. Seitz. Modern theory of solids. McGraw-Hill, New York, 1940, p. 146.

(6.25)

which agrees reasonably well with eqn (6.23) obtained by heuristic arguments. This electronic speciﬁc heat is vastly lower than the classical value (3/2)kB for any temperature at which a material can remain solid.

6.4 The work function If the metal is heated, or light waves are incident upon it, then electrons may leave the metal. A more detailed experimental study would reveal that there is a certain threshold energy the electrons should possess in order to be able to escape. We call this energy (for historical reasons) the work function and denote it by φ. Thus, our model is as shown in Fig. 6.2. At absolute zero temperature all the states are ﬁlled up to EF , and there is an external potential barrier φ. It must be admitted that our new model is somewhat at variance with the old one. Not long ago, we calculated the energy levels of the electrons on the assumption that the external potential barrier is inﬁnitely large, and now I go back on my word and say that the potential barrier is ﬁnite after all. Is this permissible? Strictly speaking, no. To be consistent, we should solve Schrödinger’s equation subject to the boundary conditions for a ﬁnite potential well. But since the potential well is deep enough, and the number of electrons escaping is relatively small, there is no need to recalculate the energy levels. So I am cheating, but not excessively.

6.5 Thermionic emission In this section we shall be concerned with the emission of electrons at high temperatures (hence the adjective thermionic). As we agreed before, the electron needs at least EF + φ energy in order to escape from the metal, and all this, of course, should be available in the form of kinetic energy. Luckily, in the free-electron model, all energy is kinetic energy, since the potential energy is zero and the electrons do not interact; so the relationship between energy and momentum is simply E=

1 2 px + p2y + p2z . 2m

(6.26)

A further condition is that the electron, besides having the right amount of energy, must go in the right direction. Taking x as the coordinate perpendicular to the surface of the metal, the electron momentum must satisfy the inequality p2 p2x > x0 = EF + φ. 2m 2m

(6.27)

However, this is still not enough. An electron may not be able to scale the barrier even if it has the right energy in the right direction. According to the

Metal

Vacuum φ

EF

Energy

Distance

Fig. 6.2 Model for thermionic emission calculation. The potential barrier that keeps the electrons in the metal is above the Fermi energy level by an energy φ.

90

The free electron theory of metals rules of quantum mechanics, it may still suffer reﬂection. Thus, the probability of escape is 1 – r(px ), where r(px ) is the reﬂection coefﬁcient. If the number of electrons having a momentum between px and px + d px is N(px )d px , then the number of electrons arriving at the surface per second per unit area is px (6.28) N(px ) d px , m and the number of those escaping is {1 – r(px )}

px N(px ) d px . m

(6.29)

Adding the contributions from all electrons that have momenta in excess of px0 , we can write for the emission current density, e ∞ {1 – r(px )}px N(px )d px . (6.30) J= m p x0 We may obtain the number of electrons in an inﬁnitesimal momentum range in the same way as for the inﬁnitesimal energy range. First, it consists of two factors, the density of states and the probability of occupation. The density of states, Z(px ), can be easily obtained by noting from eqns (6.2) and (6.26) that px =

h nx , 2

py =

h ny , 2

pz =

h nz . 2

(6.31)

The number of states in a cube of side one is exactly one. Therefore, the number of states in a volume of sides dnx , dny , dnz is equal to dnx dny dnz , which with the aid of eqn (6.31) can be expressed as 3 2 d px d py d pz . (6.32) h Dividing again by 8 (because only positive integers matter) and multiplying by two (because of spin) we get Z(px , py , pz ) =

2 . h3

(6.33)

Hence, the number of electrons in the momentum range px , px + d px ; py , py + d py ; pz , pz + d pz is N(px , py , pz ) d px d py d pz d px d py d pz 2 . = 3 h exp[{(1/(2 m))(p2x + p2y + p2z ) – EF }/kB T] + 1

(6.34)

To get the number of electrons in the momentum range px , px + d px , the above equation needs to be integrated for all values of py and pz , N(px ) d px ∞ ∞ d py d pz 2 . (6.35) = 3 dpx 2 + p2 + p2 ) – E }/k T] + 1 h exp[{(1/(2 m))(p F B –∞ –∞ x y z This integral looks rather complicated, but since we are interested only in those electrons exceeding the threshold (ϕ ≫ kB T), we may neglect the unity

Thermionic emission

91

term in the denominator. We are left then with some Gaussian functions, whose integrals between ±∞ can be found in the better integral tables (you can derive them for yourself if you are fond of doing integrals). This leads us to N(px )d px =

4π mkB T EF /kB T –p2x /2 mkB T e e d px . h3

(6.36)

Substituting eqn (6.36) into (6.30) and assuming that r(px ) = r is independent of px , which is not true but gives a good enough approximation, the integration can be easily performed, leading to J = A0 (1 – r)T 2 e–φ/kB T ,

(6.37)

where A0 =

4π emkB 2 = 1.2 × 106 A m–2 K–2 . h3

(6.38)

This is known as the Richardson (Nobel Prize, 1928) equation. The most important factor in eqn (6.37) is exp(–φ/kB T), which is strongly dependent both on temperature and on the actual value of the work function. Take, for example, tungsten (the work functions for a number of metals are ~ 4.5 eV and take T = 2500 K. Then, a given in Table 6.2), for which φ = 10% change in the work function or temperature changes the emission by a factor of 8. The main merit of eqn (6.37) is to show the exponential dependence on temperature, which is well borne out by experimental results. The actual numerical values are usually below those predicted by the equation, but this is not very surprising in view of the many simpliﬁcations we had to introduce. In a real crystal, φ is a function of temperature, of the surface conditions, and of the directions of the crystallographic axes, which our simple model did not take into account. There is one more thing I would like to discuss, which is really so trivial that most textbooks do not even bother to mention it. Our analysis was one for a piece of metal in isolation. The electron current obtained in eqn (6.37) is the current that would start to ﬂow if the sample were suddenly heated to a temperature T. But this current would not ﬂow for long because, as electrons leave the metal, it becomes positively charged, making it more difﬁcult for further electrons to leave. Thus, our formulae are valid only if we have some means of replenishing the electrons lost by emission. That is, we need an electric circuit like the one in Fig. 6.3(a). As soon as an electron is emitted from our piece of metal, another electron will enter from the circuit. The current ﬂowing can be measured by an ammeter. A disadvantage of this scheme is that the electrons travelling to the electrode will be scattered by air; we should really evacuate the place between the emitter and the receiving electrode, making up the usual cathode–anode conﬁguration of a vacuum tube. This is denoted in Fig. 6.3(b) by the envelope shown. The electrons are now free to reach the anode but also free to accumulate in the vicinity of the cathode. This is bad again, because by their negative charge they will compel many of their fellow electrons to interrupt their planned journey to the anode and return instead to the emitter. So again we do not measure the ‘natural’ current.

Table 6.2 Work functions of metals Metal

Work function (eV)

Li Na K Cs

2.48 2.3 2.2 1.9

Cu Ag Au

4.45 4.46 4.9

Mg Ca Ba

3.6 3.2 2.5

Al

4.2

Cr Mo Ta W

4.6 4.2 4.2 4.5

Co Ni Pt

4.4 4.9 5.3

92

The free electron theory of metals Electron collector

Ammeter

Metal

Fig. 6.3 Stages in measuring thermionic emission. (a) A current ﬂows but it is impeded by air molecules. (b) A current ﬂows in a vacuum until it builds up a charge cloud that repels further electrons. The steady-state ammeter reading is much less than the total emission current. (c) By employing a battery all the emission current is measured.

Vacuum envelope

A

(a)

A

(b)

+

Battery

(c) A

In order to prevent the accumulation of electrons in front of the cathode, a d.c. voltage may be applied to the anode [Fig. 6.3(c)]; this will sweep out most of the unwanted electrons from the cathode–anode region. This is the arrangement used for measuring thermionic current. The requirements to be fulﬁlled by cathode materials vary considerably according to the particular application. The cathodes must have a large emission current for high-power applications, low temperature for low-noise ampliﬁcation, and long life when the tubes are used at not easily accessible places. All these various requirements have been admirably met by industry, though the feat should not be attributed to the powers of science. To make a good cathode is still an art, and a black art at that.

6.6

The Schottky effect

We are now going to reﬁne our model for thermionic emission further by including (a) image force and (b) electric ﬁeld. It is a simple and rather picturesque consequence of the laws of electrostatics that the forces on an electron in front of an inﬁnitely conducting sheet are correctly given by replacing the sheet by the ‘mirror’ charge (a positively charged particle the same distance behind the sheet as shown in Fig. 6.4). The force between these two charges is F=

1 e2 , 4π ǫ0 (2x)2

(6.39)

and the potential energy is the integral of this force from the point x to inﬁnity: ∞ e2 . (6.40) F(y)dy = – V (x) = 16π ǫ0 x x

The Schottky effect

93

Fig. 6.4 x

x

Conducting plane

The ‘image charge’ theorem. The effect of a plane conductor on the static ﬁeld due to a charged particle is equivalent to a second, oppositely charged, particle in the mirror image position.

x

x

Remove plane add + charge

x0

Energy

B

Metal–vacuum interface

Image ﬁeld

x

A

A

(a)

(b)

Fig. 6.5 The Schottky effect. (a) Potential at metal–vacuum interface. A denotes the bottom of the potential well. (b) Potential changed by image charge ﬁeld. (c) Potential due to applied anode voltage in vacuum region. (d) Total potential ﬁeld showing reduction in height of the potential barrier compared with (a).

Summarization

(c)

(d)

In the above calculation, we took the potential energy as zero at x = ∞ to agree with the usual conventions of electrostatics, but remember that our zero a short while ago was that of a valence electron at rest. Hence, to be consistent, we must redraw the energy diagram inside and outside the metal as shown in Fig. 6.5(a). If we include now the effect of the mirror charges,∗ then the potential barrier modiﬁes to that shown in Fig. 6.5(b). In the absence of an electric ﬁeld this change in the shape of the potential barrier has practically no effect at all. But if we do have electric ﬁelds, the small correction due to mirror charges becomes signiﬁcant. For simplicity, let us investigate the case when the electric ﬁeld is constant. Then, V (x) = –eE x,

(6.41)

as shown in Fig. 6.5(c). If both an electric ﬁeld is present and the mirror charges are taken into account, then the potentials should be added, leading to the potential barrier shown in Fig. 6.5(d). Clearly, there is a maximum that can be

∗ Note

that the curve between A and B does not satisfy eqn (6.40). This is because the concept of a homogeneous sheet is no longer applicable when x is comparable with the interatomic distance. The energy is, however, given for x = 0 (an electron resting on the surface must have the same energy as an electron at rest inside the metal); so we simply assume that eqn (6.40) is valid for x > x0 and connect the points A and B by a smooth line.

94

The free electron theory of metals calculated from the condition, d e2 – – eE x = 0, dx 16π ǫ0 x

(6.42)

leading to The energy needed to escape from the metal is reduced by –Vmax .

Vmax

eE = –e 4π ǫ0

1/2

.

(6.43)

The effective work function is thus reduced from φ to φeff = φ – e

eE 4π ǫ0

1/2

.

(6.44)

Substituting this into eqn (6.37) we get the new formula for thermionic emission √ {φ – e (eE /4π ǫ0 )} 2 J = A0 (1 – r)T exp – . (6.45) kB T The reduction in the effective value of the work function is known as the Schottky effect, and plotting log J against E 1/2 , we get the so-called Schottky line. A comparison with experimental results in Fig. 6.6 shows that above a certain value of the electric ﬁeld the relationship is quite accurate. Do not be too impressed, though; in graphs of this sort the constants are generally ﬁddled to get the theoretical and experimental curves on top of each other. But it certainly follows from Fig. 6.6 that the functional relationship between J and E 1/2 is correct.

log J

T=1566 K

T=1437 K

Theoretical curve

Fig. 6.6 Experimental veriﬁcation of the Schottky formula [eqn (6.45)].

Experimental points 1 2

The ﬁeld-emission microscope

95

6.7 Field emission As we have seen in the previous section, the presence of an electric ﬁeld increases the emission current because more electrons can escape over the reduced barrier. If we increase the electric ﬁeld further, towards 109 V m–1 , then a new escape route opens up. Instead of going over the potential barrier, the electrons tunnel across it. It may be seen in Fig. 6.7 that for high-enough electric ﬁelds the barrier is thin, and thus electrons may sneak through. This is called ﬁeld emission, and it is practically independent of temperature. To derive a theoretical formula for this case, we should consider all the electrons that move towards the surface and calculate their tunnelling probability. It follows from the shape of the potential barrier that electrons with higher energy can more easily slip through, but (at ordinary temperatures) there are few of them; so the main contribution to the tunnelling current comes from electrons situated around the Fermi level. For them the width of the barrier is calculable from the equation (see Fig. 6.7) –φ = –eE xF ,

(6.46)

and the height of the potential barrier they face is φeff . Hence, very approximately, we may represent the situation by the potential proﬁle of Fig. 6.8. It may be shown (see Exercise 3.7) that the tunnelling current varies approximately exponentially with barrier width, (2 φeff )1/2 xF , J ∼ exp – ℏ

φ eff EF V = –e x

Fig. 6.7 With very high applied electric ﬁelds the potential barrier is thin, thus, instead of moving over the barrier, electrons at the Fermi level may tunnel across the barrier.

(6.47) xF

which, with the aid of eqn (6.46) reduces to

J ∼ exp –

(2 m)1/2

1/2 φeff φ

ℏe

E

φ eff

.

(6.48)

The exponential factor in eqn (6.48) represents quite a good approximation to the exact formula, which is unfortunately too long to quote. It may be noted that the role of temperature in equations (6.37) and (6.45) is taken over here by the electric ﬁeld. The theory has been fairly well conﬁrmed by experiments. The major difﬁculty in the comparison is to take account of surface irregularities. The presence of any protuberances considerably alters the situation because the electric ﬁeld is higher at those places. This is a disadvantage as far as the interpretation of the measurements is concerned, but the existence of the effect made possible the invention by Erwin Müller in 1936 of an ingenious device called the ﬁeld-emission microscope.

6.8 The ﬁeld-emission microscope The essential part of a ﬁeld-emission microscope is a very sharp tip (≈ 100 nm in diameter), which is placed in an evacuated chamber (Fig. 6.9). A potential of a few thousand volts is applied between the tip (made usually of tungsten) and

Equivalent barrier for tunnelling

Fig. 6.8 Equivalent barrier, for simplifying the calculation of tunnelling current in Fig. 6.7.

96

The free electron theory of metals Fluorescent screen

Fine point

+ 0 –104V Power supply

Vacuum envelope –

Fig. 6.9 Sketch showing the principle of the ﬁeld-emission microscope.

the anode, which creates at the tip an electric ﬁeld high enough to draw out electrons. The emitted electrons follow the lines of force and produce a magniﬁed picture (magniﬁcation = r2 /r1 , where r2 = radius of the screen and r1 = radius of the tip) on the ﬂuorescent screen. Since the magniﬁcation may be as large as 106 , we could expect to see a periodic variation in the electron emission caused by the atomic structure. The failure to observe this is explained by two reasons: quantum-mechanical diffraction, and deviation from the ‘theoretical’ course owing to a random transverse component in the electron velocity when leaving the metal. The limitations we have just mentioned can be overcome by introducing helium into the chamber and reversing the polarity of the applied potential. The helium atoms that happen to be in the immediate vicinity of the tungsten tip become ionized owing to the large electric ﬁeld, thus acquiring a positive charge, and move to the screen. Both the quantum-mechanical diffraction (remember, the de Broglie wavelength is inversely proportional to mass) and the random thermal velocities are now smaller, so that the resolution is higher and individual atoms can indeed be distinguished as shown in Fig. 6.10. This

Fig. 6.10 Field-ion micrograph of a tungsten tip. The atoms on the surface can be clearly distinguished (Courtesy of E. W. Muller).

Quartz–halogen lamps

97

device, called the ﬁeld-ion microscope, was the ﬁrst in the history of science to make individual atoms visible. Thus, just about two and a half millennia after introducing the concept of atoms, it proved possible to see them.

6.9 The photoelectric effect Emission of electrons owing to the incidence of electromagnetic waves is called the photoelectric effect. The word photo (light in Greek) came into the description because the effect was ﬁrst found in the visible range. Interestingly, it is one of the earliest phenomena that cast serious doubts on the validity of classical physics and was instrumental in the birth of quantum physics. A schematic representation of the basic experimental set-up may be seen in Fig. 6.11. When an electromagnetic wave is incident, an electric current starts to ﬂow between the electrodes. The magnitude of the current is proportional to the input electromagnetic power, but there is no current unless the frequency is high enough to make ℏω > φ.

Albert Einstein received the Nobel Prize in 1921 for ‘his discovery of the law of the photoelectric effect’. It is interesting to note that although the main tenets of the Special Theory of Relativity were already proven experimentally by that time, the Nobel citation made no mention of relativity.

(6.49)

Light input

This is probably the best place to introduce photons which are the particle equivalents of electromagnetic waves. Each photon carries an energy of E = ℏω.

A

(6.50)

Electrons will be emitted when this energy is larger than the work function. In an electromagnetic wave of power P and frequency ω the number of photons incident per unit time is Nphot = P/ℏω. A detailed calculation of the current is not easy because a photon is under no obligation to give its energy to an electron. One must calculate transition probabilities, which are different at the surface and in the bulk of the material. The problem is rather complex; we shall not go more deeply into the theory. It might be some consolation for you that the ﬁrst engineers who used and designed photocells (the commercially available device based on the photoelectric effect) knew much less about its functioning than you do.

6.10 Quartz–halogen lamps Filaments of tungsten have been used not only as sources of electrons but also as radiating elements in light bulbs. The basic design has changed little during the last hundred years until quite recently when quartz–halogen lamps were developed. The advantage of the quartz envelope (aided by the judicious use of molybdenum in the sealing process) is that the possible running temperature is higher than with ordinary glass envelopes, and so we can get much better luminous efﬁciency (light output is proportional to T 4 ). However, this alone is not much good because the tungsten ﬁlament has long been a prime example of the universal law of cussedness (things will go wrong if they can) called Sod’s or Murphy’s law, depending on which side of the Atlantic (and how far from Ireland) you live. What happens is that the ﬁlament has a region of cracks or thinning that has higher resistance and thus gets hotter than the rest. Thus,

+

Fig. 6.11 An experiment showing the photoelectric effect. If the frequency of the light is above a certain threshold value, the incident photons knock out electrons from the cathode. These cause a current in the external circuit by moving to the anode.

98

The free electron theory of metals

φ1

Fig. 6.12

φ2

EF

1

The Fermi levels and work functions of two metals to be brought into contact.

EF

2

the local rate of evaporation is increased, it gets still thinner, and by a rapidly accelerating process of positive feedback, burnout occurs. Incidentally, the fact that a light seems much brighter for a few seconds before it burns out, even although the electrical power consumed is less, is a qualitative conﬁrmation of the T 4 law. This effect can be overcome by adding some halogen gas, such as chlorine, to the lamp during processing. The tungsten vapour is now converted into chloride, which is sufﬁciently volatile to leave the hot silica envelope transparent. When chloride molecules strike the much hotter ﬁlament, they decompose, depositing tungsten and liberating chlorine to take part in further reactions. The rate of depositing goes up with temperature, so that a ‘hot spot’ is thickened, and hence cooled. This negative feedback process stabilizes the lamp. So next time you are dazzled by a quartz–halogen headlight, remember that it is an example of the very rare anti-Sod’s law.

6.11

φ2 _ φ1 φ2 φ1 EF

Fig. 6.13 When the two metals are brought into contact there is potential difference φ2 – φ1 , between them.

The junction between two metals

If two metals of different work functions are brought into contact (Fig. 6.12), the situation is clearly unstable. Electrons will cross from left to right to occupy the lower energy states available. However, as electrons cross over there will be an excess of positive charge on the left-hand side and an excess of negative charge on the right-hand side. Consequently, an electric ﬁeld is set up with a polarity that hinders the ﬂow of electrons from left to right and encourages the ﬂow of electrons from right to left. A dynamic equilibrium is established when equal numbers of electrons cross in both directions. At what potential difference will this occur? An exact solution of this problem belongs to the domain of statistical thermodynamics. The solution is fairly lengthy, but the answer, as is so often the case in thermodynamics, could hardly be simpler. The potential difference between the two metals, called the contact potential, is equal to the difference between the two work functions; or, in more general terms, the potential difference may be obtained by equating the Fermi levels of the two media in contact. This is a general law valid for any number of materials in equilibrium at any temperature. The resulting energy diagram is shown in Fig. 6.13. The potential difference appearing between the two metals is a real one. If we could put an extra electron in the contact region, it would feel a force towards the left. The potential difference is real but, alas, it cannot perform the function of a battery. Why? Because in real life you never get something for nothing and, anyway, extracting power from an equilibrium state is against the second law of thermodynamics.

Exercises

99

Exercises 6.1. Evaluate the Fermi function for an energy kB T above the Fermi energy. Find the temperature at which there is a 1% probability that a state, with an energy 0.5 eV above the Fermi energy, will be occupied by an electron.

(ii) Find a mean value for the temperature coefﬁcient of resistance. (iii) Find how the heater power varies with temperature, and estimate the Stefan–Boltzmann coefﬁcient. (iv) If the anode voltage is increased to 2.3 kV by how much will the emission current rise?

6.2. Indicate the main steps in the derivation of the Fermi level and calculate its value for sodium from the data given in Exercise 1.4.

Filament temperature (K) Filament current (A) Filament voltage (V) Emission current (mA)

6.3. Ultraviolet light of 0.2 µm wavelength is incident upon a metal. Which of the metals listed in Table 6.2 will emit electrons in response to the input light?

6.5. Use free-electron theory to determine the Fermi level in a two-dimensional metal. Take N as the number of electrons per unit area.

6.7. A tungsten ﬁlament is 0.125 mm diameter and has an effective emitting length of 15 mm. Its temperature is measured with an optical pyrometer at three points, at which also the voltage, current, and saturated emission current to a 5 mm diameter anode are measured as given in the table below.

6.10. Figure 6.14(a) shows the energy diagram for a metal–insulator–metal sandwich at thermodynamic equilibrium. Take the insulator as representing a high potential barrier. The temperature is sufﬁciently low for all states above

(i) Check that the data obey the Richardson law, and estimate the work function and value of A0 in eqn (6.37).

(b)

Energy

E0+EF +eU

E0+EF

eU

1

EF

1

2

EF

2

E0+eU

E0 E=0 Zl(E)

2600 2.30 7.40 91.2

6.9. Work out the Fermi level for conduction electrons in copper. Estimate its speciﬁc heat at room temperature; what fraction of it is contributed by the electrons? Check whether your simple calculation agrees with data on speciﬁc heat given in a reference book. Assume one conduction electron per atom. The atomic weight of copper is 63.5 and its density 9.4 × 103 kg m–3 .

6.6. Show that the average kinetic energy of free electrons, following Fermi–Dirac statistics, is (3/5)EF at T = 0 K.

Energy

2300 1.96 5.12 5.20

6.8. Light from a He–Ne laser (wavelength 632.8 nm) falls on a photo-emissive cell with a quantum efﬁciency of 10–4 (the number of electrons emitted per incident photon). If the laser power is 2 mW, and all liberated electrons reach the anode, how large is the current? Could you estimate the work function of the cathode material by varying the anode voltage of the photocell?

6.4. Determine the density of occupied states at an energy kB T above the Fermi level. Find the energy below the Fermi level which will yield the same density of occupied states.

(a)

2000 1.60 3.37 0.131

Zr(E)

Fig. 6.14 Energy against density of states for a metal–insulator–metal tunnel junction.

E=0 Zl(E)

Zr(E)

100

The free electron theory of metals

the Fermi level to be regarded as unoccupied. When a voltage U is applied [Fig. 6.14(b)] electrons may tunnel through the insulator from left to right. Assume that the tunnelling current in each energy range d E is proportional to the number of ﬁlled states from which tunnelling is possible and to the number of empty states on the other side into which electrons can tunnel. In the coordinate system of Fig. 6.14(a) the density of states as a function of energy may be written as Z1 (E) = C1 (E – E0 )1/2

for E > E0

and Zr (E) = Cr E1/2

for E > 0,

where C1 , Cr , and E0 are constants.

Show (i) that the tunnelling current takes the form EF +eU 2 I∼ (E – eU – E0 )1/2 E1/2 d E EF2

and (ii) that Ohm’s law is satisﬁed for small voltages. 6.11. Assume that the energy levels in a certain system are integral multiples of a basic unit (zero energy being permitted), and each energy level is doubly degenerate, which means that two different states can have the same energies. Assume further that there are only ﬁve fermions (particles which obey the rule that only one of them can occupy a state) in the system with a total energy of 12 units. Find 10 allowed distributions of the particles into the energy levels mentioned.

The band theory of solids Band of all evils, cradle of causeless care. Sir Philip Sidney

7

7.1 Introduction Most properties of metals can be well explained with the aid of the free-electron model, but when we come to insulators and semiconductors the theory fails. This is not very surprising because the term ‘free electron’, by deﬁnition, means an electron free to roam around and conduct electricity; and we know that the main job of an insulator is to insulate; that is, not to conduct electricity. It is not particularly difﬁcult to ﬁnd a model explaining the absence of electrical conductivity. We only need to imagine that the valence electrons cling desperately to their respective lattice ions and are unwilling to move away. So we are all right at the two extremes; free electrons mean high conductivity, tightly bound electrons mean no conductivity. Now what about semiconductors? They are neither good conductors nor insulators; so neither model is applicable. What can we do? Well, we have touched upon this problem before. Silicon and germanium are semiconductors in spite of the covalent bonds between the atoms. The bonding process uses up all the available electrons, so at absolute zero temperature there are no electrons available for conduction. At ﬁnite temperatures, however, some of the electrons may escape. The lattice atoms vibrate randomly, having occasionally much more than the average thermal energy. Thus, at certain instants at certain atoms there is enough energy to break the covalent bond and liberate an electron. This is a possible description of the electrical properties of semiconductors and, physically, it seems quite plausible. It involves no more than developing our physical picture of the covalent bond a little further by taking account of thermal vibrations as well. All we need to do is to put these arguments into some quantitative form, and we shall have a theory of semiconductors. It can be done, but somehow the ensuing theory never caught the engineers’ imagination. The theory that did gain wide popularity is the one based on the concept of energy bands. This theory is more difﬁcult to comprehend initially, but once digested and understood it can provide a solid foundation for the engineers’ ﬂights of fancy. The job of engineers is to invent. Physicists discover the laws of nature, and engineers exploit the phenomena for some useful (sometimes not so useful) end. But in order to exploit them, the engineer needs to combine the phenomena, to regroup them, to modify them, to interfere with them; that is, to create something new from existing components. Invention has never been an easy task, but at least in the good old days the basic mechanism was simple to understand. It was not very difﬁcult to be wise after the event. It was,

The higher the temperature the more likely it is that some electrons escape.

102

The band theory of solids for example, an early triumph of engineering to turn the energy of steam into a steam engine but, having accomplished the feat, most people could comprehend that the expanding steam moved a piston, which was connected to a wheel, etc. It needed perhaps a little more abstract thought to appreciate Watt’s invention of the separate condenser, but even then any intelligent man willing to devote half an hour of his time to the problem of heat exchange could realize the advantages. Alas, these times have gone. No longer can a layman hope to understand the working principles of complex mechanisms, and this is particularly true in electronics. And most unfortunately, it is true not only for the layman. Even electronic engineers ﬁnd it hard nowadays to follow the phenomena in an electronic device. Engineers may nowadays be expected to reach for the keyboard of a computer at the slightest provocation, but the fundamental equations are still far too complicated for a direct numerical attack. We need models. The models need not be simple ones, but they should be comprehensive and valid under a wide range of conditions. They have to serve as a basis for intuition. Such a model and the concurrent physical picture are provided by the band theory of solids. It may be said without undue exaggeration that the spectacular advance in solid-state electronic devices in the second half of the twentieth century owed its existence to the power and simplicity of the band theory of solids. Well, after this rather lengthy introduction, let us see what this theory is about. There are several elementary derivations, each one giving a slightly different physical picture. Since our aim is a thorough understanding of the basic ideas involved it is probably best to show you the three approaches I know.

7.2

The ions are located at x = 0, a, 2a, . . . etc. The potential wells are separated from each other by potential barriers of height V0 , and width w.

The Kronig–Penney model

This model is historically the ﬁrst (1930) and is concerned with the solution of Schrödinger’s equation, assuming a certain potential distribution inside the solid. According to the free-electron model, the potential inside the solid is uniform; the Kronig–Penney model, goes one step further by taking into account the variation of potential due to the presence of immobile lattice ions. If we consider a one-dimensional case for simplicity, the potential energy of an electron is shown in Fig. 7.1. The highest potential is halfway between the ions, and the potential tends to minus inﬁnity as the position of the ions is approached. This potential distribution is still very complicated for a straightforward mathematical solution. We shall, therefore, replace it by a simpler one, which still displays the essential features of the function, namely (i) it has the same period as the lattice; (ii) the potential is lower in the vicinity of the lattice ion and higher between the ions. The potential distribution chosen is shown in Fig. 7.2. The solution of the time-independent Schrödinger equation ℏ2 d2 ψ + {E – V (x)}ψ = 0 2m dx2

(7.1)

for the above chosen potential distribution is not too difﬁcult. We can solve it for the V (x) = V0 /2 and V (x) = –V0 /2 regions separately, match the solutions at the boundaries, and take good care that the solution is periodic. It is all

The Kronig–Penney model

103

V

Fig. 7.1 The variation of the electron’s potential energy in a one-dimensional crystal.

x a

V V0 2

w

x

0

V0 2

Fig. 7.2 An approximation to the potential energy of Fig. 7.1, suitable for analytical calculations.

a

fairly simple in principle; one needs to prove a new theorem followed by a derivation, which takes the best part of an hour, and then one gets the ﬁnal result. It is a rather laborious exercise. I shall give here only some indications how the energy structure is obtained. As was shown by Felix Bloch (Nobel Prize, 1952) we can solve eqn (7.1) by assuming the wave function in the form ψ(x) = uk (x)eikx ,

(7.2)

where k is related to the quantum-mechanical momentum and uk (x) is a periodic function, called the Bloch function, having the same period as V (x). A solution exists if k is related to the energy E by the following equation∗ cos ka = P

sin αa + cos αa, αa

(7.3)

∗ There

is actually one more mathematical simpliﬁcation introduced in arriving at eqn (7.3), namely w and V0 are assumed to tend to zero and inﬁnity respectively, with their product V0 w kept constant.

104

The band theory of solids P sin αa + cos α a αa

+1 αa

Fig. 7.3 The right-hand side of eqn (7.3) for P = 3π/2 as a function of αa.

–1 –3π

–2π

–π

0

π

2π

3π

where P=

ma V0 w, ℏ2

(7.4)

and α=

1 (2mE). ℏ

(7.5)

Remember, for a free electron we had the relationship E=

There are allowed and forbidden bands of energy.

ℏ2 k 2 . 2m

(7.6)

The relationship is now different, implying that the electron is no longer free. In order to ﬁnd the E – k curve, we plot the right-hand side of eqn (7.3) in Fig. 7.3 as a function of αa. Since the left-hand side of eqn (7.3) must always be between +1 and –1, a solution exists only at those values of E for which the right-hand side is between the same limits; that is, there is a solution for the shaded region and no solution outside the shaded region. Since α is related to E, this means that the electron may possess energies within certain bands but not outside them. This is our basic conclusion, but we can draw some other interesting conclusions from eqn (7.3). 1. If V0 w is large, that is, if P is large, the function described by the righthand side of eqn (7.3) crosses the +1, –1 region at a steeper angle, as shown in Fig. 7.4. Thus, the allowed bands are narrower and the forbidden bands wider. In the limit P → ∞ the allowed band reduces to one single energy level; that is, we are back to the case of the discrete energy spectrum existing in isolated atoms. For P → ∞ it follows from eqn (7.3) that sin αa = 0;

(7.7)

that is, the permissible values of energy are En =

π 2 ℏ2 2 n , 2ma2

(7.8)

The Kronig–Penney model

105

P sin α a + cos α a αa

+1 αa –1

π

3π

Fig. 7.4 The right-hand side of eqn (7.3) for P = 6π as a function of αa.

which may be recognized as the energy levels for a potential well of width a. Accordingly, all electrons are independent of each other, and each one is conﬁned to one atom by an inﬁnite potential barrier. 2. In the limit P → 0, we get cos αa = cos ka;

(7.9)

that is, E=

ℏ2 k 2 , 2m

(7.10)

as for the free electron. Thus, by varying P from zero to inﬁnity, we cover the whole range from the completely free electron to the completely bound electron. E

Fig. 7.5 π a

2π a

3π a

k

The energy as a function of k. The discontinuities occur at k = nπ/a, n = 1, 2, 3 . . .

106

The band theory of solids 3. At the boundary of an allowed band cos ka = ±1; that is, k=

nπ , a

n = 1, 2, 3 . . .

(7.11)

Looking at a typical energy versus k plot (Fig. 7.5), we can see that the discontinuities in energy occur at the values of k speciﬁed above. We shall say more about this curve, mainly about the discontinuities in energy, but let us see ﬁrst what the other models can tell us.

7.3

The Ziman model

This derivation relies somewhat less on mathematics and more on physical intuition. We may start again with the assertion that the presence of lattice ions will make the free-electron model untenable—at least under certain circumstances. Let us concentrate now on the wave aspect of the electron and look upon a free electron as a propagating plane wave. Its wave function is then ψk = eikx .

(7.12)

We know that waves (whether X-rays or electron waves) can easily move across a crystal lattice, but not always. There are exceptions. When individual reﬂections add up in phase (see Fig. 7.6), i.e. when nλ = 2a sin θ , William Henry Bragg and William Lawrence Bragg, father and son, received the Nobel Prize in 1915.

n = 1, 2, 3,

(7.13)

the simple plane wave picture is no longer valid. Eqn (7.13) is a well-known relationship (called Bragg reﬂection) for X-rays and, of course, it is equally applicable to electron waves. So we

a

θ

Fig. 7.6 Geometry of reﬂection from atomic planes.

The Ziman model

107

may argue that the propagation of electrons is strongly disturbed whenever eqn (7.13) is satisﬁed. In one dimension the condition reduces to nλ = 2a.

(7.14)

Using the relationship between wavelength and wavenumber, the above equation may be rewritten as k=

nπ . a

(7.15)

Thus, we may conclude that our free-electron model is not valid when eqn (7.15) applies. The wave is reﬂected, so the wave function should also contain a term representing a wave in the opposite direction, ψ–k = e–ikx .

(7.16)

Since waves of that particular wavelength are reﬂected to and fro, we may expect the forward- and backward-travelling waves to be present in the same proportion; that is, we shall assume wave functions in the form √ cos kx 1 ikx –ikx , (7.17) ψ± = √ (e ± e ) = 2 i sin kx 2 where the constant is chosen for correct normalization. Let us now calculate the potential energies of the electrons in both cases. Be careful; we are not here considering potential energy in general but the potential energy of the electrons that happen to have the wave functions ψ± . These electrons have deﬁnite probabilities of turning up at various places, so their potential energy∗ may be obtained by averaging the actual potential V (x) weighted by the probability function |ψ± |2 . Hence, 1 V± = |ψ± |2 V (x) dx L 1 2 cos2 kx = V (x) dx. (7.18) 2 sin2 kx L Since k = nπ/a, the function V (x) contains an integral number of periods of |ψ± |2 ; it is therefore sufﬁcient to average over one period. Hence, 1 a 2 cos2 kx V (x) dx V± = a 0 2 sin2 kx 1 a 1 + cos 2kx = V (x) dx a 0 1 – cos 2kx a 1 =± cos 2kx V (x) dx, a 0

(7.19)

since V (x) integrates to zero. Therefore, V± = ±Vn .

(7.20)

∗ You

may also look upon eqn (7.18) as an application of the general formula given by eqn (3.43).

L is the length of the onedimensional ‘crystal’ and V (x) is the same function that we met before in the Kronig–Penney model but now, for simplicity, we take 2w = a.

108

The band theory of solids The integration in eqn (7.19) can be easily performed, but we are not really interested in the actual numerical values. The important thing is that Vn = 0 and has opposite signs for the wave functions ψ± . Let us go through the argument again. If the electron waves have certain wave numbers [satisfying eqn (7.15)], they are reﬂected by the lattice. For each value of k two distinct wave functions ψ+ and ψ– can be constructed, and the corresponding potential energies turn out to be +Vn and –Vn . The kinetic energies are the same for both wave functions, namely

E

E= E+

ℏ2 k 2 . 2m

(7.21)

Thus, the total energies are E– π/a

E± =

k

Fig. 7.7

Ziman, Electrons in metals, a short guide to the Fermi surface, Taylor and Francis, 1962.

(7.22)

This is shown in Fig. 7.7 for k = π/a. The energy of the electron may be

The two possible values of the electron’s total energy at k = π/a.

∗ J.M.

ℏ2 k 2 ± Vn . 2m

ℏ2 k 2 – V1 2m

or

ℏ2 k 2 + V1 , 2m

(7.23)

but cannot be any value in between. There is an energy gap. What will happen when k = nπ/a? The same argument can be developed further, and a general form may be obtained for the energy.∗ It is, however, not unreasonable to assume that apart from the discontinuities already mentioned, the E–k curve will proceed smoothly; so we could construct it in the following manner. Draw the free electron parabola (dotted lines in Fig. 7.8) add and subtract Vn at the points k = nπ/a, and connect the end points with a smooth curve, keeping close to the parabola. Not unexpectedly, Fig. 7.8 looks like Fig. 7.5, obtained from the Kronig–Penney model.

E 2V3

2V2

2V1

Fig. 7.8 Construction of the E–k curve from the free-electron parabola.

π a

2π a

3π a

k

The Feynman model

109

7.4 The Feynman model This is the one I like best, because it combines mathematical simplicity with an eloquent physical picture. It is essentially a generalization of the model we used before to understand the covalent bond—another use of the coupled mode approach. Remember, the energy levels of two interacting atoms are split; one is slightly above, the other slightly below the original (uncoupled) energy. What happens when n atoms are brought close together? It is not unreasonable to expect that there will be an n-fold split in energy. So if the n atoms are far away from each other, each one has its original energy levels denoted by E1 and E2 in Fig. 7.9(a), but when there is interaction they split into n separate energy levels. Now looking at this cluster of energy levels displayed in Fig. 7.9(b), we are perfectly entitled to refer to allowed energy bands and to forbidden gaps between them. To make the relationship a little more quantitative, let us consider the onedimensional array of atoms shown in Fig. 7.10. We shall now put a single electron on atom j into an energy level E1 and deﬁne by this the state ( j). Just as we discussed before in connection with the hydrogen molecular ion, there is a ﬁnite probability that the electron will jump from atom j to atom j + 1, that is from state ( j) into state ( j + 1). There is of course no reason why the electron should jump only in one direction; it has a chance of jumping the other way too. So the transition from state ( j) into state ( j–1) must have equal probability. It is quite obvious that a direct jump to an atom farther away is also possible but much less likely; we shall therefore disregard that possibility.

(a)

(b) n n –1 n/2+2 n/2+1 n/2 n/2–1

E2

Allowed

1 0 Forbidden n n –1 n/2+2 n/2+1 n/2 n/2–1

E1

Allowed

There is an n-fold split in energy when n atoms are brought close to each other, resulting in a band of allowed energies, when n is large.

2 1

j–2

j–1

j

j+1 a

Fig. 7.9

j+2

Fig. 7.10 A one-dimensional array of atoms.

110

The band theory of solids We have now a large number of states so we should turn to eqn (5.24), which looks formidable with j running through all the atoms of the one-dimensional crystal. Luckily only nearest neighbours are coupled (or so we claim), so the differential equation for atom j takes the rather simple form iℏ

dwj = E1 wj – Awj–1 – Awj+1 , dt

(7.24)

where, as we mentioned before, E1 is the energy level of the electron in the absence of coupling, and the coupling coefﬁcient is taken again as –A. We could write down analogous differential equations for each atom, but fortunately there is no need for it. We can obtain the general solution for the whole array of atoms from eqn (7.24). Let us assume the solution in the form E is the energy to be found.

wj = Kj e–iEt/ℏ .

(7.25)

Substituting eqn (7.25) into eqn (7.24) we get EKj = E1 Kj – A(Kj–1 + Kj+1 ).

(7.26)

Note now that atom j is located at xj , and its neighbours at xj ± a, respectively. We may therefore look upon the amplitudes Kj , Kj+1 , and Kj–1 as functions of the x-coordinate. Rewriting eqn (7.26) in this new form we get EK(xj ) = E1 K(xj ) – A{K(xj + a) + K(xj – a)}.

(7.27)

This is called a difference equation and may be solved by the same method as a differential equation. We can assume the trial solution K(xj ) = eikxj ,

(7.28)

which, substituted into eqn (7.27) gives Eeik xj = E1 eik xj – A{eik(xj +a) + eik(xj –a) }.

(7.29)

Dividing by exp(ikxj ) eqn (7.29) reduces to the ﬁnal form E = E1 – 2A cos ka,

The coupling coefﬁcient between nearest neighbours is now taken as –B.

(7.30)

which is plotted in Fig. 7.11. Thus, once more, we get the result that energies within a band, between E1 – 2A and E1 + 2A, are allowed and outside that range are forbidden. It is a great merit of the Feynman model that we have obtained a very simple mathematical relationship for the E – k curve within a given energy band. But what about other energy bands that have automatically come out from the other models? We could obtain the next energy band from the Feynman model by planting our electron into the next higher energy level of the isolated atom, E2 , and following the same procedure as before. We could then obtain for the next band E = E2 – 2B cos ka,

(7.31)

The Feynman model

111

E E1+2A

E1

E1–2A

Fig. 7.11 –π/a

0

π/a

Energy as a function of k obtained from the Feynman model.

k

Another great advantage of the Feynman model is that it is by no means restricted to electrons. It could apply to any other particles. But, you may ask, what other particles can there be? Well, we have talked about positively charged particles called holes. They may be represented as deﬁciency of electrons, and so they too can jump from atom to atom. But there are even more interesting possibilities. Consider, for example, an atom that somehow gets into an excited state, meaning that one of its electrons is in a state of higher energy, and can with a certain probability transfer its energy to the next atom down the line. The concepts are all familiar, and so we may describe this process in terms of a particle moving across the lattice. Yet another advantage of this model is its easy applicability to threedimensional problems. Whereas the three-dimensional solution of the Kronig– Penney model would send shudders down the spines of trained numerical analysts, the solution of the same problem, using the Feynman approach, is well within the power of engineering undergraduates, as you will presently see. In a three-dimensional lattice, assuming a rectangular structure, the distances between lattice points are a, b, and c in the directions of the coordinate axes x, y, and z, respectively. Denoting the probability that an electron is attached to the atom at the point x, y, z by |w(x, y, z, t)|2 , we may write down a differential equation analogous to eqn (7.24): iℏ

∂w(x, y, z, t) = E1 w(x, y, z, t) ∂t – Ax w(x + a, y, z, t) – Ax w(x – a, y, z, t) – Ay w(x, y + b, z, t) – Ay w(x, y – b, z, t) – Az w(x, y, z + c, t) – Az w(x, y, z – c, t).

(7.32)

The solution of the above differential equation can be easily guessed by analogy with the one-dimensional solution in the form w(x, y, z, t) = exp(–iEt/ℏ) exp{i(kx x + ky y + kz z)},

(7.33)

which, substituted in eqn (7.32), gives in a few easy steps E = E1 – 2Ax cos kx a – 2Ay cos ky b – 2Az cos kz c.

(7.34)

Ax , Ay , Az are the coupling coefﬁcients between nearest neighbours in the x, y, z directions respectively.

112

The band theory of solids Thus, in the three-dimensional case, the energy band extends from the minimum energy Emin = E1 – 2(Ax + Ay + Az )

(7.35)

Emax = E1 + 2(Ax + Ay + Az ).

(7.36)

to the maximum energy

7.5 The mass of an electron in a crystal appears, in general, different from the free-electron mass, and is usually referred to as the effective mass.

The effective mass

It has been known for a long time that an electron has a well-deﬁned mass, and when accelerated by an electric ﬁeld it obeys Newtonian mechanics. What happens when the electron to be accelerated happens to be inside a crystal? How will it react to an electric ﬁeld? We have already given away the secret when talking about cyclotron resonance. We shall obtain the answer by using a semi-classical picture, which, as the name implies, is 50% classical and 50% quantum-mechanical. The quantummechanical part describes the velocity of the electron in a one-dimensional lattice by its group velocity, vg =

1 ∂E , ℏ ∂k

(7.37)

which depends on the actual E–k curve. The classical part expresses dE as the work done by a classical particle travelling a distance, vg dt, under the inﬂuence of a force eE yielding dE = eE vg dt 1 ∂E dt. = eE ℏ ∂k

(7.38)

We may obtain the acceleration by differentiating eqn (7.37) as follows: dvg 1 d ∂E 1 ∂ 2 E dk = = . dt ℏ dt ∂k ℏ ∂k 2 dt

(7.39)

Expressing now dk/dt from eqn (7.38) and substituting it into eqn (7.39) we get dvg 1 ∂ 2E = 2 2 eE . dt ℏ ∂k

(7.40)

Comparing this formula with that for a free, classical particle m

dv = eE , dt

(7.41)

we may deﬁne ∗

m =ℏ

2

∂ 2E ∂k 2

–1

(7.42)

The effective mass

113

as the effective mass of an electron. Thus, the answer to the original question is that an electron in a crystal lattice does react to an electric ﬁeld, but its mass is given by eqn (7.42) in contrast to the mass of a free electron. Let us just check whether we run into any contradiction with our E–k curve for a free electron. Then E=

ℏ2 k 2 , 2m

and thus ∂ 2 E ℏ2 = , m ∂k 2 which substituted into eqn (7.42) gives m∗ = m. E

So everything is all right. For an electron in a one-dimensional lattice we may take E in the form of eqn (7.30), giving m∗ =

ℏ2 sec ka. 2Aa2

(7.43)

The graphs of energy, group velocity, and effective mass are plotted for this case in Fig. 7.12 as a function of k between –π/a and π/a. Oddly enough, m∗ may go to inﬁnity and may take on negative values as well. If an electron, initially at rest at k = 0, is accelerated by an electric ﬁeld, it will move to higher values of k and will become heavier and heavier, reaching inﬁnity at k = π/2a. For even higher values of k the effective mass becomes negative, heralding the advent of a new particle, the hole, which we have casually met from time to time and shall often meet in the rest of this course. The deﬁnition of effective mass as given in eqn (7.42) is for a onedimensional crystal, but it can be easily generalized for three dimensions. If the energy is given in terms of kx , ky , and kz , as for example in eqn (7.34), then the effective mass in the x-direction is m∗x

=ℏ =

2

∂ 2E ∂kx2

(a)

υg (b)

m* (c)

–1

ℏ2 sec kx a. 2Ax a2

(7.44)

In the y-direction it is

–π/a

m∗y = ℏ2 =

∂ 2E ∂ky2

–1

ℏ2 sec ky b. 2Ay b2

0

k

π/a

Fig. 7.12 Energy, group velocity, and effective mass as a function of k.

(7.45)

114

The band theory of solids

If you are fond of mathematics you may think of the effective mass (or rather of its reciprocal) as a tensor quantity, but if you dislike tensors just regard the electron in a crystal as an extremely whimsical particle which, in response to an electric ﬁeld in the (say) z-direction, may move in a different direction.

A similar formula applies in the z-direction. So, oddly enough, the effective mass may be quite different in different directions. Physically, this means that the same electric ﬁeld applied in different directions will cause varying amounts of acceleration. This is bad enough, but something even worse may happen. There can be a term like m∗xy = ℏ2

not mistake this for the rate of change of electric current under stationary conditions. For the steady state to apply one must take collisions into account as well.

† We

have already done it twice before, but since the density of states is a rather difﬁcult concept (making something continuous having previously stressed that it must be discrete), and since this is a slightly different situation, we shall do the derivation again. Remember, we are in one dimension, and we are interested in the number of states in momentum space in an interval dpx . According to eqn (6.31), px =

h nx , 2

where nx is an integer. So for unit length there is exactly one state and for a length dpx the number of states, dnx , is (2/h) dpx , which is equal to (1/π ) dkx . We have to divide by 2 because only positive values of n are permitted and have to multiply by 2 because of the two possible values of spin. Thus, the number of states in a dkx interval remains 1 dkx . π

∂ 2E ∂kx ∂ky

–1

.

(7.46)

With our simple model, m∗xy turns out to be inﬁnitely large, but it is worth noting that in general an electric ﬁeld applied in the x-direction may accelerate an electron in the y-direction. As far as I know there are no electronic devices making use of this effect; if you want to invent something quickly, bear this possibility in mind.

7.6 ∗ Do

The effective number of free electrons

Let us now leave the fanciful world of three dimensions and return to the mathematically simpler one-dimensional case. In a manner rather similar to the derivation of effective mass we can derive a formula for the number of electrons available for conduction. According to eqn (7.40), dvg 1 ∂ 2E = 2 2 eE . dt ℏ ∂k

(7.47)

We have here the formula for the acceleration of an electron. But we have not only one electron, we have lots of electrons. Every available state may be ﬁlled by an electron; so the total effect of accelerating all the electrons may be obtained by a summation over all the occupied states. We wish to sum dvg /dt for all electrons. Multiplying by the electron charge, d (evg ) dt is nothing else but the rate of change of electric current that ﬂows initially when an electric ﬁeld is applied.∗ Thus, dI d = (evg ) dt dt ∂ 2E 1 = 2 e2 E , ℏ ∂k 2

(7.48)

or, going over to integration, 1 1 dI = e2 E dt ℏ2 π

d2 E dk, dk 2

where the density of states in the range dk is dk/π .†

(7.49)

The number of possible states per band

115

E

States empty

Ea

States occupied –π/a

–ka

Fig. 7.13 One-dimensional energy band ﬁlled up to ka at T = 0 K.

π/a

ka

If there were N non-interacting free electrons, we should obtain dI e2 E = N. dt m

(7.50)

For free electrons eqn (7.50) applies; for electrons in a crystal eqn (7.49) is true. Hence, if we wish to create a mental picture in which the electrons in the crystal are replaced by ‘effective’ electrons, we may deﬁne the number of effective electrons by equating eqn (7.49) with eqn (7.50). Hence Neff =

1 m π ℏ2

d2 E dk. dk 2

(7.51)

This, as you may have already guessed, applies only at absolute zero because we did not include the probability of occupation. In this case all the states are occupied up to an energy E = Ea , and all the states above Ea are empty. If Ea happens to be somewhere inside an energy band (as shown in Fig. 7.13) then the integration goes from k = –ka to k = k a . Performing the integration: Neff

dE dE – dk k=ka dk k=–ka 2 m dE . = π ℏ2 dk k=ka

1 m = π ℏ2

(7.52)

This is a very important result. It says that the effective number of electrons capable of contributing to electrical conduction depends on the slope of the E–k curve at the highest occupied energy level. At the highest energy in the band dE/dk vanishes. We thus come to the conclusion that the number of effective electrons for a full band is zero.

If the energy band is ﬁlled there is no electrical conduction.

7.7 The number of possible states per band

∗ It would be more logical to demand that

In order to ﬁnd the number of states, we must introduce boundary conditions. The simplest one (though physically the least defensible) is the so-called ‘periodic boundary condition’.∗ It is based on the argument that a macroscopic crystal is so large in comparison with atomic dimensions that the detailed

the wave function should disappear at the boundary, but that would involve us only in more mathematics without changing any of the conclusions. So I must ask you to accept the rather artiﬁcial boundary condition expressed by eqn (7.53).

116

The band theory of solids x

Na

1

2

3

Na–1

4

5

L

Fig. 7.14 Illustration of periodic boundary condition for a one-dimensional crystal.

nature of the boundary conditions does not matter, and we should choose them for mathematical convenience. In the case of the periodic boundary condition, we may simply imagine the one-dimensional crystal biting its own tail. This is shown in Fig. 7.14, where the last atom is brought into contact with the ﬁrst atom. For this particular conﬁguration, it must be valid that ψ(x + L) = ψ(x).

(7.53)

Then, with the aid of eqn (7.2), it follows that eik(x+L) uk (x + L) = eikx uk (x).

(7.54)

Since uk is a periodic function repeating itself from atom to atom, uk (x + L) = uk (x)

(7.55)

and, therefore, to satisfy eqn (7.54), we must have r is a positive or negative integer.

∗ The Feynman model gives only one en-

ergy band at a time, but it shows clearly that the energy is a periodic function of ka, that is the same energy may be described by many values of k. Hence it would have been equally justiﬁed (as some people prefer) to choose the interval from k = 0 to k = π/a.

kL = 2π r.

(7.56)

It follows from the Kronig–Penney and from the Ziman models that in an energy band (that is in a region without discontinuity in energy) k varies from nπ/a to (n + 1)π/a.∗ Hence kmax ≡ (n + 1)

π 2π rmax = a L

(7.57)

2π rmin . L

(7.58)

and kmin ≡ n(π/a) = Rearranging, we have rmax – rmin =

L 2a

L = Na , 2

(7.59)

Holes where Na is the number of atoms per unit length. Since r may have negative values as well, the total number of permissible values of k is

2(rmax – rmin ) = Na L.

(7.60)

Now to each value of k belongs a wave function; so the total number of wave functions is Na L, and thus, including spin, the total number of available states is 2Na L.

7.8 Metals and insulators At absolute zero some materials conduct well, some others are insulators. Why? The answer can be obtained from the formulae we have derived. If each atom in our one-dimensional crystal contains one electron, then the total number of electrons is Na L, and the band is half-ﬁlled. Since dE/dk is large in the middle of the band, this means that there is a high effective number of electrons; that is, high conductivity. If each atom contains two electrons, the total number of electrons is 2Na L; that is, each available state is ﬁlled. There is no conductivity: the solid is an insulator. If each atom contains three electrons, the total number of electrons is 3Na L; that is, the ﬁrst band is ﬁlled and the second band is half-ﬁlled. The value of dE/dk is large in the middle of the second band; therefore a solid containing atoms with three electrons each (it happens to be lithium) is a good conductor. It is not difﬁcult to see the general trend. Atoms with even numbers of electrons make up the insulators, whereas atoms with odd numbers of electrons turn out to be metals. This is true in general, but it is not true in every case. All we need to know is the number of electrons, even or odd, and the electric behaviour of the solid is determined. Diamond, with six electrons, must be an insulator and aluminium, with thirteen electrons, must be a metal. Simple, isn’t it? It is a genuine triumph of the one-dimensional model that the electric properties of a large number of elements may be promptly predicted. Unfortunately, it does not work always. Beryllium with four electrons and magnesium with twelve electrons should be insulators. They are not. They are metals; though metals of an unusual type in which electric conduction, evidenced by Halleffect measurements, takes place both by holes and electrons. What is the mechanism responsible? For that we need a more rigorous deﬁnition of holes.

7.9 Holes We ﬁrst met holes as positively charged particles that enjoy a carefree existence quite separately from electrons. The truth is that they are not separate entities but merely by-products of the electrons’ motion in a periodic potential. There is no such thing as a free hole that can be ﬁred from a hole gun. Holes are artiﬁces but quite lively ones. The justiﬁcation for their existence is as follows.

117

118

The band theory of solids Using our deﬁnition of effective mass [eqn (7.42)] we may rewrite eqn (7.48) in the following manner: 1 dI = e2 E , dt m∗i

(7.61)

i

where the summation is over the occupied states. If there is only one electron in the band, then dIe e2 E = ∗. dt m

(7.62)

If the band is full, then according to eqn (7.52) the effective number of electrons is zero; that is, 1 dI = e2 E = 0. dt m∗i

(7.63)

i

Assume now that somewhere towards the top of the band an electron, denoted as j, is missing. Then, the summation in eqn (7.61) must omit the state j, which we may write as 1 dIh = e2 E . dt m∗i

(7.64)

i

i =j

But from eqn (7.63) ⎞

⎛

⎜ 1 1 ⎟ ⎟ = 0. e2 E ⎜ ⎝ m∗ + m∗ ⎠ j

i

(7.65)

i

i =j

Equation (7.64) therefore reduces to

dIh 1 = –e2 E ∗ . dt mj

(7.66)

In the upper part of the band, however, the effective mass is negative; therefore Hence, an electron missing from the top of the band leads to exactly the same formula as an electron present at the bottom of the band.

dIh e2 E = ∗. dt |mj |

(7.67)

Now there is no reason why we should not always refer to this phenomenon as a current due to a missing electron that has a negative mass. But it is a lot shorter, and a lot more convenient, to say that the current is caused by a positive particle, called a hole. We can also explain the reason why the signs of eqn (7.62) and of eqn (7.67) are the same. In response to an electric ﬁeld, holes move in an opposite direction carrying an opposite charge; their contribution to electric current is therefore the same as that of electrons.

Divalent metals

119

We may now return to the case of beryllium and magnesium and to their colleagues, generally referred to as divalent metals. One-dimensional theory is unable to explain their electric properties; let us try two dimensions. The E – kx , ky surface may be obtained from eqn (7.34) as follows:

The divalent metals, having two valency electrons, are found in groups IIA and IIB of the periodic table (Fig. 4.5).

7.10 Divalent metals

E = E1 – 2Ax cos kx a – 2Ay cos ky b.

(7.68)

Let us plot now the constant energy curves in the kx – ky plane for the simple case when E1 = 1,

Ax = Ay = 14 ,

a = b.

(7.69)

It may be seen in Fig. 7.15 that the minimum energy E = 0 is at the origin and for higher values of kx and ky the energy increases. Note well that the boundaries kx = ±π/a and ky = ±π/a represent a discontinuity in energy. (This is something we have proved only for the one-dimensional case, but the generalization to two dimensions is fairly obvious.) There is an energy gap there. If the wave vector changes from point B just inside the rectangle, to point C, just outside the rectangle, the corresponding energy may jump from one unit to (say) 1.5 units. Let us now follow what happens at T = 0 as we ﬁll up the available states with electrons. There is nothing particularly interesting until all the states up to E = 1 are ﬁlled, as shown in Fig. 7.16(a). The next electron coming has an itch to leave the rectangle; it looks out, sees that the energy outside is 1.5 units, and therefore stays inside. This will go on until all the states are ﬁlled up to an energy E = 1.5, as shown in Fig. 7.16(b). The remaining states inside our rectangle have energies in excess of 1.5, and so the next electron in its search for lowest energy will go outside. It will go into a higher band because there are lower energy states in that higher band (in spite of the energy gap) than inside the rectangle. π/a

The usual notation is to call the rectangle the ‘ﬁrst Brillouin zone’, and as we step out of it (say at point C) we reach the ‘second Brillouin zone’. The shape of the higher Brillouin zones can be determined with not too much effort but it is beyond the scope of the present book.

C B 1.85 1.5

ky 1.0 0.5 0

E=0.15

Fig. 7.15 –π/a –π/a

0

kx

π/a

Constant energy contours for a two-dimensional crystal in the kx – ky plane on the basis of the Feynman model.

120 (a)

The band theory of solids π/a

ky 0

–π/a –π a

0

kx

π a

The detailed continuation of the story depends on the variation of energy with k in the higher band, but one thing is certain: the higher band will not be empty. For an atom with two electrons, the number of available states is equal to the number of electrons. If the energy gap is large (say, two units instead of half a unit), then all the states in the rectangle would be ﬁlled, and the material would be an insulator. If the energy gap is small (half a unit in our example), then some states will remain unﬁlled in the rectangle, and some states will be ﬁlled in the higher band. This means that both bands will contribute to electrical conduction. There will be holes coming from the rectangle and electrons from the higher band. This is how it happens that in some metals holes are the dominant charge-carriers.

7.11

(b)

ky

–π a

0

kx

π a

Fig. 7.16 (a) All energy levels ﬁlled up to E = 1. (b) All energy levels ﬁlled up to E = 1.5.

At ﬁnite temperatures a metal is a metal, but an insulator is no longer an insulator.

As you can see, there is no profound difference in principle; insulators and semiconductors are distinguished only by the magnitudes of their respective energy gaps.

Finite temperatures

All we said so far applies to zero temperature. What happens at ﬁnite temperatures? And what is particularly important, what happens at about room temperature, at which most electronic devices are supposed to work? For ﬁnite temperatures it is no longer valid to assume that all states up to the Fermi energy are ﬁlled and all states above that are empty. The demarcation line between ﬁlled and unﬁlled states will become less sharp. Let us see ﬁrst what happens to a metal. Its highest energy band is about half-ﬁlled at absolute zero; at higher temperatures some of the electrons will acquire somewhat higher energies in the band, but that is all. There will be very little change in the effective number of electrons. A metal will stay a metal at higher temperatures. What will happen to an insulator? If there are many electrons per atom, then there are a number of completely ﬁlled bands that are of no interest. Let us concentrate our attention on the two highest bands, called valence and conduction bands, and take the zero of energy at the top of the valence band. Since at absolute zero the valence band is completely ﬁlled, the Fermi level must be somewhere above the top of the valence band. Assuming that it is about halfway between the bands (I shall prove this later), the situation is depicted in Fig. 7.17(a) for zero temperature and in Fig. 7.17(b) for ﬁnite temperature. Remember, when the Fermi function is less than 1, it means that the probability of occupation is less than 1; thus, some states in the valence band must remain empty. Similarly, when the Fermi function is larger than 0, it means that the probability of occupation is ﬁnite; that is, some electrons will occupy states in the conduction band. We have come to the conclusion that at ﬁnite temperatures, an insulator is no longer an insulator. There is conduction by electrons in the conduction band, and conduction by holes in the valence band. The actual amount of conduction depends on the energy gap. This can be appreciated if you remember that well away from the Fermi level the Fermi function varies exponentially; its value at the bottom of the conduction band and at the top of the valence band therefore depends critically on the width of the energy gap. For all practical purposes diamond with an energy gap of 5.4 eV is an insulator, but silicon and germanium with energy gaps of 1.11 and 0.67 eV show noticeable conduction at room temperature. They are called semi-conductors.

Concluding remarks

121

E Conduction band T=0

Energy gap

Valence band (a) F(E)

E

Conduction band

T>>0

Energy gap

Valence band

(b) F(E)

Fig. 7.17 (a) The two highest bands at T = 0 K. (b) The two highest bands at T ≫ 0 K. There are electrons at the bottom of the conduction band, and holes at the top of the valence band.

7.12 Concluding remarks The band theory of solids is not an easy subject. The concepts are a little bewildering at ﬁrst and their practical utility is not immediately obvious. You could quite well pass examinations without knowing much about band theory, and you could easily become the head of a big electrical company without having any notion of bands at all. But if you ever want to create something new in solid-state electronic devices, which will be more and more numerous in your professional life, a thorough understanding of band theory is imperative. So my advice would be to go over it again and again until familiarity breeds comprehension. I would like to add a few more words about the one-dimensional models we use so often. The reason for using one-dimensional models is mathematical simplicity, and you must appreciate that the results obtained are only qualitatively true. The real world is three-dimensional, thus our models must also be three-dimensional if we want to have good agreement between theory and experiment. Having said that I must admit that this is not quite true. When we look at some of the recently invented devices, we ﬁnd that some are two-dimensional, some are one-dimensional, and some have zero dimension.∗

∗I

know it is rather hard to swallow that there can be such things as zero-dimensional devices but all will be clear when we discuss them (they are known as low-dimensional devices) in Section 12.7.2 among semiconductor lasers.

122

The band theory of solids

Exercises 7.1. Classify metals, semiconductors, and insulators on the basis of their band structure. Find out what you can about materials on the border lines of these classiﬁcations. 7.2. X-ray measurements show that electrons in the conduction band of lithium have energies up to 4.2 eV. Take this as the highest ﬁlled energy level in the band. If you further identiﬁed this energy level with the Fermi level, what average effective mass will give you the same result from free-electron theory? Assume one free electron per atom. The atomic weight of lithium is 6.94, and its density is 530 kg m3 . 7.3. Show, using the Feynman model, that the effective mass at the bottom of the band is inversely proportional to the width of the band. 7.4. Show from eqns (7.3) and (7.5) that the group velocity of the electron is zero at k = nπ/a. 7.5. In general, the reciprocal of the effective mass is a tensor whose components are given by the mixed derivatives. How would the classical equation of motion m be modiﬁed?

dν =F dt

7.6. The reciprocal mass tensor for Bi close to the bottom of the conduction band is of the form ⎞ ⎛ axx 0 0 ⎝ 0 ayy ayz ⎠ . 0 ayz azz (i) Find the components of the effective mass tensor. (ii) Find the function E(kx , ky , kz ). (iii) Show that the constant energy surfaces are ellipsoids. 7.7. Using the potential energy distribution of Fig. 7.2, determine, with the aid of the Ziman model, the width of the ﬁrst forbidden band. Take w = a/2. 7.8. Assume, as in the Kronig–Penney model of Section 7.2, that w and V0 in Fig. 7.2 tend to zero and inﬁnity, respectively, but their product V0 w is kept constant. Determine with the aid of the Ziman model the widths of the nth allowed band and the nth forbidden band. Can you conclude that the higher the band the wider it is? 7.9. The lowest energy bands in a solid are very narrow because there is hardly any overlap of the wave functions. In general, the higher up the band is, the wider it becomes. Assuming that the collision time is about the same for the valence and conduction bands, which would you expect to have higher mobility, an electron or a hole?

Semiconductors Whatsoever things are true . . . whatsoever things are pure . . . think on these things. Philippians iv 8

8.1 Introduction With the aid of band theory we have succeeded in classifying solids into metals, insulators, and semiconductors. We are now going to consider semiconductors (technologically the newest class) in more detail. Metals and insulators have been used for at least as long as we have been civilized, but semiconductors have found application only in the last century, and their more widespread application dates from the 1950s. Over this period the electronics industry has been (to use a hackneyed word justiﬁably) revolutionized, ﬁrst by the transistor, then by microelectronic circuitry. Each of these in succession, by making circuitry much cheaper and more compact, has led to the wider use of electronic aids, such as computers, in a way that is revolutionary in the social sense too. Perhaps the key reason for this sudden change has been the preparation of extremely pure semiconductors, and hence the possibility of controlling impurity; this was a development of the 1940s and 1950s. By crystal pulling, zone-reﬁning, and epitaxial methods it is possible to prepare silicon and germanium with an impurity of only 1 part in 1010 . Compare this with long-established engineering materials, such as steel, brass, or copper where impurities of a few parts per million are still virtually unattainable (and for most purposes, it must be admitted, not required). Probably the only other material that has ever been prepared with purity comparable to that of silicon and germanium is uranium, and we know what that led to. I shall now try to show why the important electrical properties of semiconductors occur and how they are inﬂuenced and controlled by small impurity concentrations. Next, we shall consider what really came ﬁrst, the preparation of pure material. We shall be ready then to discuss junction devices and integrated circuit technology.

8.2 Intrinsic semiconductors The aim in semiconductor technology is to purify the material as much as possible and then to introduce impurities in a controlled manner. We shall call the pure semiconductor ‘intrinsic’ because its behaviour is determined by its intrinsic properties alone, and we shall call the semiconductor ‘extrinsic’ after external interference has changed its inherent properties. In devices it is mostly extrinsic semiconductors that are used, but it is better to approach our subject gradually and discuss intrinsic semiconductors ﬁrst.

8

124

Semiconductors To be speciﬁc, let us think about silicon, although most of our remarks will be qualitatively true of germanium and other semiconductors. Silicon has the diamond crystalline structure; the four covalent bonds are symmetrically arranged. All four valence electrons of each atom participate in the covalent bonds, as we discussed before. But now, having learned band theory, we may express the same fact in a different way. We may say that all the electrons are in the valence band at 0 K. There is an energy gap of 1.1 eV above this before the conduction band starts. Thus, to get an electron in a state in which it can take up kinetic energy from an electric ﬁeld and can contribute to an electric current, we ﬁrst have to give it a package of at least 1.1 eV of energy. This can come from thermal excitation, or by photon excitation quite independently of temperature. Let us try to work out now the number of electrons likely to be free to take part in conduction at a temperature T. How can we do this? We have already solved this problem for the one-dimensional case: eqn (7.51) gives us the effective number of electrons in a partly ﬁlled band; so all we need to do is to include the Fermi function to take account of ﬁnite temperature and to generalize the whole thing to three dimensions. It can be done, but it is a bit too complicated. We shall do something else, which is less justiﬁable on strictly theoretical grounds, but is physically much more attractive. It is really cheating because we use only those concepts of band theory that suit us, and instead of solving the problem honestly, we shall appeal to approximations and analogies. It is a compromise solution that will lead us to easily manageable formulae. First of all we shall say that the only electrons and holes that matter are those near the bottom of the conduction band and the top of the valence band, respectively. Thus, we may assume that kx a,

ky b,

kz c ≪ 1,

(8.1)

and we may expand the cosine term in eqn (7.34) to get the energy in the form, E = E1 – 2Ax 1 – 21 kx2 a2 – 2Ay 1 – 12 ky2 b2 – 2Az 1 – 21 kz2 c2 . (8.2) Using our deﬁnition of effective mass, we can easily show from the above equation that m∗x =

ℏ2 , 2Az a2

m∗y =

ℏ2 , 2Ay b2

m∗z =

ℏ2 . 2Az c2

(8.3)

Substituting the values of Ax a2 , Ay b2 , and Az c2 from eqn (8.3) back into eqn (8.2) and condensing the constant terms into a single symbol, E0 , we may now express the energy as ky2 kz2 ℏ2 kx2 + + E = E0 + . (8.4) 2 m∗x m∗y m∗z Taking further E0 = 0, and assuming that everything is symmetric, that is m∗x = m∗y = m∗z = m∗ ,

(8.5)

Intrinsic semiconductors

125

(8.6)

This formula is identical to eqn (6.2) obtained from the free-electron model—well, nearly identical.

we get ℏ2 2 2 2 k + k + k E= z . y 2m∗ x

The mass in the denominator is not the real mass of an electron but the effective mass. But that is the only difference between eqn (8.6) and the free-electron model. Thus, we are going to claim that electrons in the conduction band have a different mass but apart from that behave in the same way as free electrons. Hence the formula derived for the density of states [eqn (6.10)] is also valid, and we can use the same method to determine the Fermi level. So we shall have the total number of electrons by integrating . . . Wait, we forgot about holes. How do we include them? Well, if holes are the same sort of things as electrons apart from having a positive charge, then everything we said about electrons in the conduction band should be true for holes in the valence band. The only difference is that the density of states must increase downwards for holes. Choosing now the zero of energy at the top of the valence band, we may write the density of states in the form Z(E) = Ce (E – Eg )1/2 ,

Ce = 4π (2m∗e )3/2 /h3

(8.7)

for electrons, and Z(E) = Ch (–E)1/2 ,

Ch = 4π (2m∗h )3/2 /h3

(8.8)

for holes, both of them per unit volume. This is shown in Fig. 8.1, where E is plotted against Z(E). You realize of course that the density of states has meaning only in the allowed energy band and must be identically zero in the gap between the two bands. Let us return now to the total number of electrons. To obtain that we must take the density of states, multiply by the probability of occupation (getting thereby the total number of occupied states), and integrate from the bottom to the top of the conduction band. So, formally, we have to solve the following integral: top of conduction band (density of states)(Fermi function) dE. (8.9) Ne =

E

Eg Range of forbidden energies 0 Z(E)

bottom of conduction band

There are several difﬁculties with this integral: 1. Our solution for the density of states is valid only at the bottom of the band, 2. The Fermi function

E – EF –1 (8.10) F(E) = 1 + exp kB T is not particularly suitable for analytical integration. 3. We would need one more parameter in order to include the width of the conduction band. We are saved from all these difﬁculties by the fact that the Fermi level lies in the forbidden band, and in practically all cases of interest its distance from

Fig. 8.1 Density of states plotted as a function of energy for the bottom of the conduction (electrons) and top of the valence (holes) bands. See eqns (8.7) and (8.8).

126

Semiconductors E

(a)

E

Z(E)

(b)

E

F(E)

F(E) Z(E)

(c)

Fig. 8.2 (a) The density of states as a function of energy for the bottom of the conduction band. (b) The Fermi function for the same range of energies. (c) A plot of F(E)Z(E) showing that the ﬁlled electron states are clustered together close to the bottom of the conduction band.

the band edge is large in comparison with kB T (0.025 eV at room temperature). Hence, E – EF ≫ kB T

(8.11)

and the Fermi function may be approximated by

–(E – EF ) , F(E) = exp kB T

(8.12)

as shown already in eqn (6.18). If the Fermi function declines exponentially, then the F(E)Z(E) product will be appreciable only near the bottom of the conduction band as shown in Fig. 8.2. Thus, we do not need to know the density of states for higher energies (nor the width of the band) because the fast decline of F(E) will make the integrand practically zero above a certain energy. But if the integrand is zero anyway, why not extend the upper limit to inﬁnity? We may then come to an integral that is known to mathematicians. Substituting now eqns (8.7) and (8.12) into eqn (8.9), we get

∞ –(E – EF ) 1/2 dE. (8.13) (E – Eg ) exp Ne = Ce kB T Eg Introducing now the new variable x=

(E – Eg ) , kB T

(8.14)

the integral takes the form Ne = Ce (kB T)3/2 exp ∗ Even

better, you could work it out for yourself; it’s not too difﬁcult.

–(Eg – EF ) kB T

∞

x1/2 e–x dx.

(8.15)

0

According to mathematical tables of high reputation,∗

0

∞

x1/2 e–x dx =

1√ π, 2

(8.16)

Intrinsic semiconductors

127

leading to the ﬁnal result Ne = Nc exp

–(Eg – EF ) , kB T

(8.17)

where 2π m∗e kB T Nc = 2 h2

3/2

.

(8.18)

Thus, we have obtained the number of electrons in the conduction band as a function of some fundamental constants, of temperature, of the effective mass of the electron at the bottom of the band, and of the amount of energy by which the bottom of the band is above the Fermi level. We can deal with holes in an entirely analogous manner. The probability of a hole being present (that is of an electron being absent) is given by the function 1 – F(E),

(8.19)

which also declines exponentially along the negative E-axis. So we can choose the lower limit of integration as –∞, leading to the result for the number of holes in the valence band, Nh = Nv exp(–EF /kB T),

(8.20)

Nv = 2(2π m∗h kB T/h2 )3/2 .

(8.21)

where

For an intrinsic semiconductor each electron excited into the conduction band leaves a hole behind in the valence band. Therefore, the number of electrons should be equal to the number of holes (this would actually follow from the condition of charge neutrality too); that is Ne = Nh .

(8.22)

Substituting now eqns (8.17) and (8.20) into eqn (8.22), we get Nc exp{–(Eg – EF )/kB T} = Nv exp(–EF /kB T),

(8.23)

from which the Fermi level can be determined. With a little algebra we get EF =

m∗ Eg 3 + kB T loge h∗ . 2 4 me

(8.24)

We may now ask how carrier concentration varies with temperature. Strictly speaking, the energy gap is also a function of temperature for the reason that it depends on the lattice constant, which does vary with temperature. That is, however, a small effect on the normally used temperature range, so we are nearly always entitled to disregard it. Substituting eqn (8.24) into eqns (8.17) and (8.20), we ﬁnd that both Ne and Nh are proportional to exp(–Eg /2kB T), an important relationship. We know now everything we need to about intrinsic semiconductors. Let us now look at the effect of impurities.

Since kB T is small, and the effective masses of electrons and holes are not very much different, we can say that the Fermi level is roughly halfway between the valence and conduction bands.

128

Semiconductors

8.3

If the impurity is less than, say, 1 in 106 silicon atoms, the lattice will be hardly different from that of a pure silicon crystal.

∗ The impurity atom donates an electron.

Extrinsic semiconductors

We shall continue to consider silicon as our speciﬁc example, but now with controlled addition of a group V impurity (this refers to column ﬁve in the periodic table of elements) such as, for example, antimony (Sb), arsenic (As), or phosphorus (P). Each group V atom will replace a silicon atom and use up four of its valence electrons for covalent bonding [Fig. 8.3(a)]. There will, however, be a spare electron. It will no longer be so tightly bound to its nucleus as in a free group V atom, since the outer shell is now occupied (we might look at it this way) by eight electrons, the number of electrons in an inert gas; so the dangling spare electron cannot be very tightly bound. However, the impurity nucleus still has a net positive charge to distinguish it from its neighbouring silicon atoms. Hence, we must suppose that the electron still has some afﬁnity for its parent atom. Let us rephrase this somewhat anthropomorphic picture in terms of band theory. We have said the energy gap represents the minimum energy required to ionize a silicon atom by taking one of its valence electrons. The electron belonging to the impurity atom clearly needs far less energy than this to become available for conduction. Let us call this energy Eimp . If an electron loosely bound to the impurity atom receives an energy Eimp it will be available for conduction, or in other words will be promoted into the conduction band. If an energy Eimp is needed for the promotion then the energy level of an impurity atom must be below the conduction band by that much, i.e. it will be at ED = Eg – Eimp . This energy level is called the donor∗ level. See Table 8.1 for measured values of Eimp . Interestingly, a very rough model serves to give a quantitative estimate of the donor levels. Remember, the energy of an electron in a hydrogen atom [given by eqn (4.18)] is E = –me4 /8ǫ02 h2 .

(8.25)

We may now argue that the excess electron of the impurity atom is held by the excess charge of the impurity nucleus; that is, the situation is like that in the hydrogen atom, with two minor differences. 1. The dielectric constant of free space should be replaced by the dielectric constant of the material. 2. The free-electron mass should be replaced by the effective mass of the electron at the bottom of the conduction band.

4

4

(a) The extra electron ‘belonging’ to the group V impurity is much more weakly bound to its parent atom than the electrons taking part in the covalent bond. (b) This is equivalent to a donor level close to the conduction band in the band representation.

4 Extra electron

Fig. 8.3

(a)

Eg ED

4

5

4

4

4

4

0

( b)

Extrinsic semiconductors

129

Table 8.1 Energy levels of donor (group V ) and acceptor (group III) impurities in Ge and Si. The energies given are the ionization energies, that is, the distance of the impurity level from the band edge (in electron volts) Impurity

Ge

Si

Donors

Antimony (Sb) Phosphorus (P) Arsenic (As)

0.0096 0.0120 0.0127

0.039 0.045 0.049

Acceptors

Indium (In) Gallium (Ga) Boron (B) Aluminium (Al)

0.0112 0.0108 0.0104 0.0102

0.160 0.065 0.045 0.057

Thus, this model leads to the following estimate: Eg – ED = m∗ e4 /8ǫ 2 h2 .

(8.26)

Taking silicon as an example, for which m∗ = 0.58m (see Table 8.4) and εr = 12 (see Table 10.1), this energy level is smaller by a factor of 248 than the value of –13.6 eV given by eqn (4.21) for the hydrogen atom. That comes to 0.0548 eV, not very far from the experimental ﬁgures in Table 8.1. Note, however, that the parameters in eqn (8.26) depend only on the properties of the host material, so this model cannot possibly say anything on how Eg – ED varies with the type of dopant. If instead of a group V impurity we had some group III atoms, for example, indium (In), aluminium (Al), or boron (B), there would be an electron missing from one of the covalent bonds (see Fig. 8.4). If one electron is missing, there must be a hole present. Before going further, let me say a few words about holes. You might have been slightly confused by our rather inconsistent references to them. To clear this point—there are three equivalent representations of holes, and you can always (or nearly always) look at them in the manner most convenient under the circumstances. You may think of a hole as a full-blooded positive particle moving around in the crystal, or as an electron missing from the top of the valence band, or as the actual physical absence of an electron from a place where it would be desirable to have one. Eg

4

4

3

4 EA

4 (a)

0 (b)

Fig. 8.4 (a) In the case of a group III impurity one bonding electron is missing— there is a ‘hole’ which any valence electron with a little surplus energy can fall into. (b) This shows in the band representation as an acceptor level just above the valence band edge.

130

NA– is the number of ionized acceptor atoms, which accepted an electron from the valence band, and ND+ is the number of ionized donor atoms, which donated an electron to the conduction band.

Semiconductors In the present case, the third interpretation is the most convenient one—to start with. A group III atom has three valence electrons. So when it replaces a silicon atom at a certain atomic site, it will try to contribute to bonding as much as it can. However, it possesses only three electrons for four bonds. Any electron wandering around would thus be welcomed to help out. More aggressive impurity nuclei might even consider stealing an electron from the next site. The essential point is that a low energy state is available for electrons—not as low an energy as at the host atom but low enough to come into consideration when an electron has acquired some extra energy and feels an urge to jump somewhere. Therefore (changing now to band theory parlance), the energy levels due to group III impurities must be just above the valence band. Since these atoms accept electrons so willingly, they are called acceptors and the corresponding energy levels are referred to as acceptor levels. A real material will usually have both electron donors and acceptors present (not necessarily group V and group III elements; these were chosen for simplicity of discussion and because they are most often used in practice). However, usually one type of impurity exceeds the other, and we can talk of impurity semiconductors as n- (negative carrier) or p- (positive carrier) types according to whether the dominant charge carriers are electrons or holes. If we had some silicon with 1020 atoms per cubic metre of trivalent indium, it would be a p-type semiconductor. If we were somehow to mix in 1021 atoms per cubic metre of pentavalent phosphorus, the spare phosphorus electrons would not only get to the conduction band but would also populate the acceptor levels, thus obliterating the p characteristics of the silicon and turning it into an n-type semiconductor. Let us calculate now the number of electrons and holes for an extrinsic semiconductor. We have in fact already derived formulae for them, as witnessed by eqns (8.17) and (8.20); but they were for intrinsic semiconductors. Did we make any speciﬁc use of the fact that we were considering intrinsic semiconductors? Perhaps not. We said that only electrons at the bottom of the band matter, and we also said that the bottom of the band is many times kB T away from the Fermi level in energy but this could all be equally valid for extrinsic semiconductors. It turns out that these approximations are valid, apart from certain exceptional cases (we shall meet one exception when we consider devices). But how can we determine the Fermi level? It is certainly more difﬁcult for an extrinsic semiconductor. We have to consider now all the donors and acceptors. The condition is that the crystal must be electrically neutral, that is, the net charge density must be zero. Let us consider what sort of charges we may meet in an extrinsic semiconductor. There are our old friends, electrons and holes; then there are the impurity atoms that donated an electron to the conduction band, and are left with a positive charge; and ﬁnally there are the acceptor atoms that accepted an electron from the valence band and thus have a negative charge. Hence the formula for overall charge neutrality is Ne + NA– ⇌ Nh + ND+ .

(8.27)

We have written eqn (8.27) with the ⇌ sign used by chemists to show that it is a dynamic equilibrium, rather than a once and for all equation. How can we ﬁnd the number of ionized impurities, NA– and ND+ , from the actual number of impurity atoms NA and ND ? Looking at Fig. 8.3(b) you may

Extrinsic semiconductors recollect that the ND donor electrons live at the level ED (at 0 K) all ready and willing to become conduction electrons if somehow they can acquire (Eg – ED ) joules of energy. ND+ is hence a measure of how many of them have gone. Therefore, ND+

= ND {1 – F(ED )}.

(8.28)

131

If we multiply ND by the probability of an electron not being at ED we should get ND+ .

For acceptor atoms the argument is very similar. The probability of an electron occupying a state at the energy level EA is F(EA ). Therefore the number of ionized acceptor levels is NA– = NA F(EA ).

(8.29)

We are now ready to calculate the position of the Fermi level in any semiconductor whose basic properties are known; that is, if we know NA and ND , the energy gap, Eg , and the effective masses of electrons and holes. Substituting for Ne , Nh , NA– , ND+ from eqns (8.17), (8.20), (8.28), and (8.29) into eqn (8.27) we get an equation that can be solved for EF . It is a rather cumbersome equation but can always be solved with the aid of a computer. Fortunately, we seldom need to use all the terms, since, as mentioned above, the dominant impurity usually swamps the others. For example, in an n-type semiconductor, usually Ne ≫ Nh and ND+ ≫ NA– and eqn (8.27) reduces to ~ N+. Ne = (8.30) D

This, of course, implies that all conduction electrons come from the donor levels rather than from host lattice bonds. Substituting eqns (8.17) and (8.28) into eqn (8.30) we get∗ Eg – EF ~ EF – ED –1 Nc exp – . (8.31) = N D 1 + exp kB T kB T For a particular semiconductor eqn (8.31) is easily solvable, and we may plot EF as a function of ND or of temperature. Let us ﬁrst derive a formula for the simple case when (EF –ED )/kB T is a large negative number. Equation (8.31) then reduces to (constant) exp

EF ~ = ND . kB T

(8.32)

So we have already learned that the position of the Fermi level moves upwards, and varies rather slowly with impurity concentration. Let us consider now a slightly more complicated situation where the above approximation does not apply. Take silicon at room temperature and arsenic as the dopant with the data Eg = 1.15 eV,

Eg – ED = 0.049 eV,

ND = 1022 m–3 .

(8.33)

We may get the solution easily by introducing the notation EF , kB T

(8.34)

ND , 1 + Bx

(8.35)

x = exp reducing thereby eqn (8.31) to the form Ax =

∗ Equation

(8.31) is not, however, valid at the limit of no impurity, because holes cannot then be neglected; nor is it valid when ND is very large, because some of the approximations [e.g. eqn (8.11)] are then incorrect, and in any case many impurity atoms getting close enough to each other will create their own impurity band.

EF increases with the logarithm of ND .

132

Semiconductors

EF Eg ED 1

2

3

Eg

EFi

2

0

0

T

Fig. 8.5 The variation of the Fermi level as a function of temperature for an n-type semiconductor. The curves 1, 2, and 3 correspond to increasing impurity concentrations. EFi is the intrinsic Fermi level (plotted from eqn (8.24)) for mh > me to which all curves tend at higher temperatures. EF Eg

EFi Eg 2 1 EA 0 0

2

3

T

Fig. 8.6 The variation of the Fermi level as a function of temperature for a p-type semiconductor. The curves 1, 2, and 3 correspond to increasing impurity concentrations. EFi is the intrinsic Fermi level to which all curves tend at higher temperatures.

which leads to a quadratic equation in x, giving ﬁnally for the Fermi level, EF = 0.97 eV. Thus, in the practical case of an extrinsic semiconductor the Fermi level is considerably above the middle of the energy gap. Let us consider now the variation of Fermi level with temperature. This is somewhat complicated by the fact that Eg and ED are dependent on lattice dimensions, and hence both change with temperature, but we shall ignore this effect for the moment. At very low temperatures (a few degrees absolute), the chance of excitation across the gap is fantastically remote compared with the probability of ionization from a donor level (which is only remote). Try calculating this for a 1 eV value of Eg and a 0.05 eV value of Eg – ED . You should ﬁnd that with 1028 lattice atoms per cubic metre, of which only 1021 are donors, practically all the conduction electrons are from the latter. Thus, at low temperature the material will act like an intrinsic semiconductor whose energy gap is only Eg – ED . So we can argue that the Fermi level must be about halfway within this ‘gap’, that is ~ 1 (Eg + ED ). EF = 2

(8.36)

Is this analogy so close that we can generalize the relationship obtained before for the temperature variation of intrinsic carriers? Can we claim that it will now be exp[–(Eg – ED )/2kB T] instead of exp(–Eg /2kB T)? Yes, this is true under certain conditions. It can be derived from eqn (8.31) (see Exercise 8.14). At the other extreme, at very high temperatures, practically all the electrons from the impurity atoms will be ionized, but because of the larger reservoir of valency electrons, the number of carriers in the conduction band will be much greater than ND . In other words, the material (now a fairly good conductor) will behave like an intrinsic semiconductor with the Fermi level at about Eg /2. For larger impurity concentration the intrinsic behaviour naturally comes at a higher temperature. Thus, a sketch of EF against temperature will resemble Fig. 8.5 for an n-type semiconductor. The relationship for a p-type semiconductor is entirely analogous and is shown in Fig. 8.6. There is just one further point to note about the variation of energy gap with temperature. We have seen in the Ziman model of the band structure that the interband gap is caused by the interaction energy when the electrons’ de Broglie half-wavelength is equal to the lattice spacing. It is reasonable to suppose that this energy would be greater at low temperatures for the following reason. At higher temperatures the thermal motion of the lattice atoms is more vigorous; the lattice spacing is thus less well deﬁned and the interaction is weaker. This, qualitatively, is the case; for example, in germanium the energy gap decreases from about 0.75 eV at 4 K to 0.67 eV at 300 K.

8.4

Scattering

Having learned how to make n-type and p-type semiconductors and how to determine the densities of electrons and holes, we now know quite a lot about semiconductors. But we should not forget that so far we have made no statement about the electrical conductivity, more correctly nothing beyond that at the beginning of the course [eqn (1.10)], where we produced the formula

Scattering σ =

e2 τ Ne . m

(8.37)

An obvious modiﬁcation is to put the effective mass in place of the actual mass of the electron. But there is still τ , the mean free time between collisions. What will τ depend on and how? We have now asked one of the most difﬁcult questions in the theory of solids. As far as I know no one has managed to derive an expression for τ starting from ﬁrst principles (i.e. without the help of experimental results). Let us ﬁrst see what happens at absolute zero temperature. Then all the atoms are at rest;∗ so the problem seems to be: how long can an electron travel in a straight line without colliding with a stationary atom? Well, why would it collide with an atom at all? Classically a lattice looks to an electron like a dense forest through which there is no chance of passing without bumping into a tree here and there. But the quantum-mechanical picture is quite different. As we know from the Feynman model, the electron does something quite different. It sits in an energy level of a certain atom, then tunnels through the adverse potential barrier and takes a seat at the next atom, and again at the next atom—so it just walks across the crystal without any collision whatsoever. The mean free path is the length of the crystal—so it is not the presence of the atoms that causes the collisions. What then? The imperfections? If the crystal were perfect, we should have nice periodic solutions [as in eqn (7.33)] for the wave function, and there would be equal probability for an electron being at any atom. It could thus start at any atom and could wriggle through the crystal to appear at any other atom. But the crystal is not perfect. The ideal periodic structure of the atoms is upset, partly by the thermal motion of the atoms, and partly by the presence of impurities, to mention only the two most important effects. So, strictly speaking, the concept of collisions, as visualized for gas molecules, makes little sense for electrons. Strictly speaking, there is no justiﬁcation at all for clinging to the classical picture. Nevertheless, as so often before, we shall be able to advance some rough classical arguments, which lead us into the right ballpark. First notice [eqns (1.11) and (1.13)] that the mean free path may be written with good approximation as proportional to l ∼ τ T 1/2 .

(8.38)

Arguing now that the mean free path is inversely proportional to the scattering probability, and the scattering probability may be taken to be proportional to the energy of the lattice wave (i.e. to T), we obtain for the collision time τthermal ∼ lT –1/2 ∼ T –3/2 .

(8.39)

The argument for ionized impurities is a little more involved. We could say that no scattering will occur unless the electron is so close to the ion that the electrostatic energy [given by eqn (4.2) if e2 is replaced by Ze2 ] is comparable with the thermal energy 3 Ze2 = kB T, 4π ǫrs 2

133

(8.40)

∗ For

the purpose of the above discussion we can assume that the atoms are at rest, but that can never happen in an actual crystal. If the atoms were at rest then we would know both their positions and velocities at the same time, which contradicts the uncertainty principle. Therefore, even at absolute zero temperature, the atoms must be in some motion.

134

Semiconductors leading to a radius, rs =

Ze2 . 6π ǫkB T

(8.41)

Next, we argue that the scattering power of the ion may be represented at the radius by a scattering cross-section, Ss = rs2 π =

1 π

Ze2 6ǫkB T

2

.

(8.42)

Finally, assuming that the mean free path is inversely proportional to the scattering cross-section, we obtain the relationship τionized impurity = lT –1/2 ∼ Ss–1 T –1/2 ∼ T 3/2 .

(8.43)

When both types of scattering are present the resultant collision time may be obtained from the equation If a high value of τ is required, then one should use a very pure material and work at low temperatures.

∗ Two

present applications are the Gunn effect and very high frequency transistors, both to be discussed in Chapter 9.

Note that electron mobilities are higher than hole mobilities due to the fact that in both materials the effective mass of electrons is smaller than that of holes.

1 1 1 = + . τ τthermal τionized impurity

(8.44)

A high value of τ means high mobility and hence high average velocity for the electrons. We do not know yet whether high electron velocities in crystals will have many useful applications,∗ but since fast electrons in vacuum give rise to interesting phenomena, it might be worthwhile making an effort to obtain high carrier velocities in semiconductors. How would mobility vary as a function of impurity density? It is bound to decline. Instead of a mathematical model that is quite complicated, we are going to give here actual measured curves for electron and hole mobilities at T = 300 K for Ge and Si (see Fig. 8.7). When both electrons and holes are present the conductivities add σ =

8.5

e2 τe Ne e2 τh Nh + . m∗e m∗h

(8.45)

A relationship between electron and hole densities

Let us now return to eqns (8.17) and (8.20). These were derived originally for intrinsic semiconductors, but they are valid for extrinsic semiconductors as well. Multiplying them together, we get Ne Nh = 4

2π kB T h2

3

Eg . (m∗e m∗h )3/2 exp – kB T

(8.46)

It is interesting to note that the Fermi level has dropped out, and only the ‘constants’ of the semiconductor are contained in this equation. Thus, for a given semiconductor (i.e. for known values of m∗e , m∗h , and Eg ) and temperature

A relationship between electron and hole densities 1

T = 300 K μe

10–1 Mobility (m2 V–1 s–1)

135

Ge

μh

10–2 1

μe 10–1

Si

μh 10–2

1020

1021

1022 1023 Impurity concentration (m–3)

Fig. 8.7 1024

1025

Electron and hole mobilities in Ge and Si as a function of impurity concentration.

we can deﬁne the product Ne Nh exactly, whatever the Fermi energy and hence whatever the impurity density. In particular, for an intrinsic material, where Ne = Nh = Ni , we get Ne Nh = Ni2 .

(8.47)

Let us think over the implications. We start with an intrinsic semiconductor; so we have equal numbers of electrons and holes. Now add some donor atoms. The number of electrons must then increase, but according to eqn (8.47) the product must remain constant. At ﬁrst this seems rather odd. One would think that the number of electrons excited thermally from the valence band into the conduction band (and thus the number of holes left behind) would depend on temperature only, and be unaffected by the presence of donor atoms. This is not so. By increasing the concentration of donors, the total number of electrons in the conduction band is increased, but the number of electrons excited across the gap is decreased (not only in their relative proportion but in their absolute number too). Why? We can obtain a qualitative answer to this question by considering the ‘dynamic equilibrium’ mentioned brieﬂy before. It means that electron–hole pairs are constantly created and annihilated and there is equilibrium when the rate of creation equals the rate of annihilation (the latter event is more usually referred to as ‘recombination’). Now it is not unreasonable to assume that electrons and holes can ﬁnd each other more easily if there are more of them present. For an intrinsic material we may write rintrinsic = aNi2 ,

gintrinsic = aNi2 ,

(8.48)

where a is a proportionality constant, and r and g are the rates of recombination and creation, respectively.

If the number of electrons increases, the number of holes must decrease.

The rate of recombination must be proportional to the densities of holes and electrons.

136

Semiconductors Now we may argue that by adding a small amount of impurity, neither the rate of creation nor the proportionality constant should change. So for an extrinsic semiconductor gextrinsic = aNi2

(8.49)

is still valid. The rate of recombination should, however, depend on the actual densities of electrons and holes, that is rextrinsic = aNe Nh .

(8.50)

From the equality of eqns (8.49) and (8.50) we get the required relationship, Ni2 = Ne Nh .

(8.51)

So we may say that as the density of electrons is increased above the intrinsic value, the density of holes must decrease below the intrinsic value in order that the rate of recombination of electron–hole pairs may remain at a constant value equal to the rate of thermal creation of pairs. Those of you who have studied chemistry may recognize this relationship as a particular case of the law of mass action. This can be illustrated by a chemical reaction between A and B, giving rise to a compound AB, A+B AB.

(8.52)

If we represent the molecular concentration of each component by writing its symbol in square brackets, the quantity [A][B][AB]–1

(8.53)

is a constant at a given temperature. Now our ‘reaction’ is electron + hole bound electron.

(8.54)

As the number of bound electrons (cf. [AB]) is constant, this means that [electron][hole] = Ne Nh

(8.55)

will also be constant.

8.6

III–V and II–VI compounds

In our examples up to now we have referred to germanium and silicon as typical semiconductors, and indeed they are typical, their technology was certainly the earliest mastered. They are both tetravalent, so they can be found in column IVB of our periodic table shown in Fig. 4.5. There are, of course, many other semiconductors. In this section we shall be concerned with two further types which are compounds of elements from columns IIIB, VB, IIB, and VIB, respectively. Let us talk ﬁrst about the III–V compounds. Why are they semiconductors? We can say the same thing about them as about germanium and silicon. They are insulators at low temperatures because all the electrons participate in the bonding process; none of them is available for conduction. At higher temperatures, however, the electronic bond can be broken by thermal

III–V and II–VI compounds excitations, that is electrons can be excited into the conduction band. The only difference relative to Ge and Si is that III–V compounds have an ionic contribution to the bonding as well. This is not particularly surprising. We mentioned in Chapter 5 that the ionic bond of NaCl comes about because the one outer electron of sodium is happy to join the seven outer electrons of chlorine to make up a completed ring—so it is easy to see that, with Ga having three outer electrons and As having ﬁve outer electrons, they will also strike up a companionship in order to complete the ring. Which are the most important III–V materials? The oldest one, and technologically the best developed, is GaAs, to which serious attention has been paid since the middle of the 1950s and which has been the preferred material for a host of devices. Why? One might expect that arsenic was the last thing anyone in any laboratory would have wanted to work on. However, some of the rivals, for example AlSb, fell by the wayside because of a tendency to decompose quickly, and, most importantly, GaAs was the material that offered high mobility relative to Ge and Si. For measured curves of electron and hole mobilities against impurity concentration, see Fig. 8.8. What can we say about the energy gap of GaAs? It is, 1.42 eV, a lot higher than that of Ge, the element between them in the periodic table. The energy gap is higher which means that it is more difﬁcult to break a bond in GaAs than in Ge. Why? Because of the presence of ionic bonding. We can also say something deﬁnite about the energy gaps of some other compounds relative to that of GaAs. If we combine with Ga the element in the periodic table above As, we obtain GaP with an energy gap of 2.24 eV. If we choose for the other element in the compound Sb, which is below As in the periodic table, then we obtain GaSb with an energy gap of 0.67 eV. The same is true if we combine various elements from column III with As. The energy gap of AlAs is 2.2 eV, whereas the energy gap declines to 0.36 eV for InAs. The general rule is easy to remember: the lower you go in the periodic table in your choice of the elements the smaller is the gap. What is the reason? The farther down the columns of the periodic table (Table 4.1) the higher are both the nuclear charge (Ze) and the number of ﬁlled electronic inner shells. Hence, the valency electrons are farther from the nucleus and so more loosely bound. Thus, the bonding force between atoms is weaker (lower melting point) and the energy to promote electrons into the conduction band is less (lower energy gap). This is shown in Table 8.2 where also we have omitted the heaviest group III–V elements thallium (atomic number 81) and bismuth (83) as their compounds have a very narrow gap and so are almost metallic.

137

Note, however, that a III–V ionic bond is weaker than a I–VII ionic bond.

Mobility (m2V–1s–1)

1 e

10–1 h

10–2

1020

1021

1022 1023 Impurity concentration (m–3)

Fig. 8.8 1024

1025

Electron and hole mobilities in GaAs as a function of impurity concentration.

138

Semiconductors Table 8.2 Size of atoms in tetrahedral bonds Element

Atomic number

Atomic weight (AMU)

Atomic radius in tetrahedral covalent bonds Å

IIB Zn Cd Hg

30 48 80

68.38 112.4 200.59

1.31 1.48 1.48

IIIB B Al Ga In

5 13 31 49

10.81 26.98 69.72 114.82

0.88 1.26 1.26 1.44

IVB C Si Ge Sn

6 14 32 50

12.01 28.09 72.59 118.69

0.77 1.17 1.22 1.40

VB N P As Sb

7 15 33 51

14.007 30.97 74.92 121.7

0.70 1.10 1.18 1.36

VIB O S Se Te

8 16 34 52

16.0 32.06 78.96 127.60

0.66 1.04 1.14 1.32

How can we make a III–V material, say GaAs n-type or p-type? The answer is easy in principle. If there is excess Ga it will be p-type, if there is excess As it will be n-type. Or we can try as a dopant a column IV material, for example silicon. It acts as a donor if it replaces a Ga atom, and as an acceptor if it replaces an As atom. In practice, of course, it is not so easy to produce any of these materials to a given speciﬁcation. Most of the semiconductors we consider in this section crystallize like GaAs in the zinc blende structure. This is very like our diamond picture (Fig. 5.3) with the C atoms replaced alternately with a III and V or II and VI. So all bonds are between unlike atoms. We can also visualize this structure as each sub-set of atoms arranged in a face centred cubic (FCC) structure. The two sub-sets are displaced from each other in three dimensions by a half lattice spacing, that is one fourth of the FCC sub-lattice cubic separation. This results (back to Fig. 5.3) in a tetragonal arrangement, each atom being bonded symmetrically to four unlike atoms. In Table 8.2 we list the basic size of atoms, including the atomic radius that they have in tetragonal bonding. One can calculate the bond length of atomic separation in, say, GaP by adding the Ga and P radii. Then by fairly simple geometry we can obtain the lattice parameter by multiplying by 2.31.

III–V and II–VI compounds All the compounds mentioned so far have been binary compounds, that is they consist of two elements. In principle there are no difﬁculties in growing ternary crystals consisting of three elements. However, if the growth is carried out from a melt, variations in vapour pressure between the elements make it almost impossible to maintain their relative concentrations (or stoichiometry) without additional precautions such as a pressurized, impermeable blanket. As a result, binary compounds are often the practical limit for crystals (and hence for substrates). However, the same difﬁculties are not encountered during epitaxy, and it is simple to grow ternary and quaternary compounds on binary substrates. Al for example is quite happy to occupy a Ga site, so there are no difﬁculties in producing a GaAlAs crystal. What will be the effect of adding Al to GaAs? According to the argument given above, the energy gap should increase. The more Al is added the larger will be the energy gap. Is that good for something? Yes. The sources for optical communications depend crucially on our ability to tailor the energy gap. Let me give you an example. The preferred material for blue-green semiconductor lasers is GaN, but its energy gap puts it into the ultraviolet region. This can be adjusted by replacing some of the gallium with indium, the heavier element reducing the gap. We shall say a lot more about this in Section 12.7. There are a few obvious things we can say about II–VI materials. They have more ionic bonding than III–V materials and less ionic bonding than I–VII materials. For more accurate ﬁgures of the contribution of ionic forces to bonding see Table 8.3. What about the energy gaps? Just as GaAs has a higher energy gap than Ge, we would also expect ZnSe (look it up in the periodic table: Zn is to the left of Ga, and Se is to the right of As) to have a higher energy gap than GaAs. It is actually 2.58 eV. The same rule, as for III–V materials, applies again for going up and down in the periodic table. ZnS (S is above Se) has an energy gap of 3.54 eV, whereas that of ZnTe (Te is below Se) is 2.26 eV. Zinc blende is of course the name of the ore from which ZnS is obtained. It is a little unfortunate that ZnS is one of the II–VI compounds which also crystallizes in another form called wurtzite. Here the crystals have similar bond lengths, the formal difference is that alternate (111) plane layers are rotated 180◦ about the 111 axis. This gives a hexagonal atomic arrangement. It is reminiscent of the deviations of diamond to hexagonal planes in graphite and C60 . It is not too serious a problem having two versions of ZnS, as well as ZnO, ZnSe, and CdS. The bond length and density are the same, and electrical properties practically identical. The bonding is only slightly different because of different distances of third nearest atoms. This is characterized by the Madelung constant (Section 5.3.1) which is 1.638 for zinc blende and 1.641 for wurtzite. So we do not have to record different bandgaps and melting points for the two crystal types. Most of the III–V compounds crystallize in the zinc blende structure but the nitrides have the wurtzite form. A clue as to why this happens is that the third nearest atoms are unlike hence attractive. The nitrogen atom with its small size and high electronegativity is prone to take a more ionic form of crystal. The main problems with II–VI materials used to arise from the fact that some compounds could be made p-type, some others n-type, but no compound could be made both types. The change for the better came with the advent

139

140

Semiconductors Table 8.3 Semiconductor properties I. Energy gap and structure Semiconductor

Conduction band (i)

(ii)

Energy gap eV

Melting point K

Ionic % of bond

Lattice spacing Å

Group IV C Si Ge SiC

5.4 1.11 0.67 2.9

382 1680 1210

0 0 0 18

3.56 5.43 5.66 3.08, 5.05

Group III–V Al N Al P Al As Al Sb Ga N Ga P Ga As Ga Sb In N In P In As In Sb

6.02 3.34 2.2 1.6 3.34 2.24 1.42 0.67 2.0 1.27 0.36 0.17

3070 1770 1870 1330 2770 1730 1520 980 2475 1330 1215 798

42 36 32

Group II–VI Zn O Zn S Zn Se Zn Te Cd O Cd S Cd Se Cd Te

3.20 3.54 2.58 2.26 2.5 2.42 1.74 1.44

2248 1925 1790 1658 2020 1750 1512 1368

62 62 63 61 79 69 70 67

Valence band

Fig. 8.9 Three models for obtaining free carriers by illumination: (i) band-toband transitions yielding an electron–hole pair, (ii) ionization of donor atoms, (iii) ionization of acceptor atoms.

4.63 5.41 5.67 6.10 5.58 6.05 6.48

of molecular beam epitaxy (see Section 8.11.5) which makes it possible to produce junctions from II–VI materials.

8.7 (iii)

31 26

3.11, 4.98 5.45 5.66 6.15 3.19, 5.18 5.45 5.65 6.10 3.54, 5.70 5.80 6.06 6.48

Non-equilibrium processes

In our investigations so far, the semiconductor was always considered to be in thermal equilibrium. Let us look brieﬂy at a few cases where the equilibrium is disturbed. The simplest way of disturbing the equilibrium is to shine electromagnetic waves (in practice these are mostly in the visible range) upon the semiconductor. As a result photoemission may occur, as in metals, but more interestingly, the number of carriers available for conduction may signiﬁcantly increase. This case is called photoconduction. The three possible processes of producing carriers for conduction are shown in Fig. 8.9; (i) creating an electron–hole pair, that is exciting an electron from the valence band into the conduction band; (ii) exciting an electron from an impurity level into the conduction band; (iii) exciting an electron from the top of the valence band into an impurity level, and thus leaving a hole behind.

Real semiconductors The extra carriers are available for conduction as long as the semiconductor is illuminated. What happens when the light is switched off? The number of carriers must fall gradually to the equilibrium value. The time in which the extra density is reduced by a factor e = 2.718 is called the lifetime of the carrier and is generally denoted by τ (and is thus quite often confused with the collision time). It is an important parameter in the design of many semiconductor devices. Assume now that only part of the semiconductor is illuminated; we shall then have a region of high concentration in connection with regions of lower concentration. This is clearly an unstable situation, and by analogy with gases, we may expect the carriers to move away from places of high concentration towards places of lower concentration. The analogy is incidentally correct; this motion of the carriers has been observed, and can be described mathematically by the usual diffusion equation J = eD∇N.

(8.56)

Equation (8.56) is equally valid for holes and electrons, though in a practical case, the signs should be chosen with care.

141

D is the diffusion coefﬁcient. This equation is quite plausible physically; it means that if there is a density gradient, a current must ﬂow.

8.8 Real semiconductors All our relationships obtained so far have been based on some idealized model. Perhaps the greatest distortion of reality came from our assumption of a simple cubical lattice for the calculation of the band structure. As we know, silicon and germanium crystallize in the diamond structure, and that makes a signiﬁcant difference. Plotting the E vs kx curve (Fig. 8.10) for the conduction band of silicon, for example, it becomes fairly obvious that it bears no close resemblance to our simple E = E0 – 2Ax cos kx a curve, which had its minimum at kx = 0. Even

E

Eg

Fig. 8.10

kx

0 h

l

s

E–k curve for silicon in a particular direction. Note that the minimum of the conduction band is not at k = 0 and there are three different types of holes. The situation is similar in germanium, which is also an indirect-gap (minimum of conduction band not opposite to maximum of valence band) semiconductor.

142

∗ This

is not true of graphite, for example, which has very different conductivities in different directions, but fortunately single-crystal graphite is not widely used in semiconductor devices. Polycrystalline graphite has, of course, been used ever since the birth of the electrical and electronics industries (for brushes and microphones) but the operational principles of these devices are so embarrassingly simple that we cannot possibly discuss them among the more sophisticated semiconductor devices.

Semiconductors worse, the E vs ky curve would be very different from the one plotted. The surfaces of constant energy in k-space are not spheres. The situation is not much better in the valence band, where the constant energy surfaces are nearly spheres but—I regret to say—there are three different types of holes present. This is shown in Fig. 8.10, where the letters h, l, and s stand for heavy, light, and split-off bands respectively. What does it mean to have three different types of holes? Well, just think of them as holes painted red, blue, and green. They coexist peacefully, though occasionally, owing to collisions, a hole may change its complexion. Does this mean that all we have said so far is wrong? Deﬁnitely not. Does it mean that considerable modiﬁcations are needed? No, for most purposes not even that. We can get away with our simple model because, in general, only average values are needed. It is nice to know that there are three different types of holes in the valence band of silicon but for device operation only the average effective mass and some sort of average collision time are needed. The picture is not as black as it seems. In spite of the anisotropy in the E(k) curves the grand total is isotropic. I mean that by performing all the relevant averaging processes in silicon (still for a single-crystal material), the ﬁnal result is an isotropic effective mass and isotropic collision time. Measuring the conductivity in different directions will thus always give the same result.∗ Another important deviation from the idealized band structure occurs in a number of III–V compounds, where a subsidiary valley appears in the conduction band (shown for GaAs in Fig. 8.11). For most purposes (making a gallium arsenide transistor, for example) the existence of this additional valley can be

E

m* = 0.35 m0

0.36 eV

m* = 0.067 m0 Eg

1.4 eV

Fig. 8.11 Energy band diagram for gallium arsenide showing subsidiary valley in conduction band.

k

0 m* = 0.67 m0 (holes)

Measurement of semiconductor properties

143

ignored but it acquires special signiﬁcance at high electric ﬁelds. It constitutes the basis for the operation of a new type of device, which we shall discuss later among semiconductor devices. You must realize, however, that this is the exception rather than the rule. The details of the band structure generally do not matter. For the description and design of the large majority of semiconductor devices our model is quite adequate.

8.9 Amorphous semiconductors In this chapter we have considered very pure and regular crystal forms of Ge, Si, and other semiconductors, and have used simple models based on this symmetry to derive basic properties like energy gap and conductivity. What happens if the material is not a single crystal—suppose one evaporates a ﬁlm of Si on to a suitable substrate? The ﬁlm consists of randomly oriented clusters of crystallites (small crystals). The structure within the crystallites leads to an energy gap. Remember, in all our three models of band structure (Chapter 7) band edges form when the electrons’ de Broglie wave interferes with the lattice spacing. A small array of lattice points gives a less sharp interference pattern, so the band edges are not so well deﬁned. We still get optical absorption and photoconduction, but with a less sharp spectral variation than shown later in Fig. 8.18(b). Another effect of small crystallites is that the covalent bonds break off where the orientation changes, so that there are ‘dangling bonds’, where the unpaired electrons can act as traps for both itinerant electrons and holes. Mobility is greatly reduced; and also doping is much less effective, as the carriers from the dopant are trapped. This effect ties the Fermi level near the middle of the energy gap, as it is in intrinsic materials and insulators. If the amorphous layer is formed in a gas discharge containing hydrogen, the ‘dangling bond’ is dramatically reduced. The H atoms neutralize the unpaired electrons, and the atomic nucleus has a minimal effect on lattice behaviour. In these circumstances amorphous Si can be doped into both p- and n-type. Why should we use amorphous semiconductors when we can have them in superior single crystal form? The reason is purely economical. When we need them in large areas, as in solar cells (Section 13.2) or in xerographic applications (Section 10.17), we use the amorphous variety.

8.10 Measurement of semiconductor properties The main properties to be measured are (i) mobility, (ii) Hall coefﬁcient, (iii) effective mass, (iv) energy gaps (including the distance of any impurity layer from the band edge), and (v) carrier lifetime.

8.10.1

Mobility

This quantity was deﬁned as the carrier drift velocity for unit ﬁeld, μ = vD /E .

(8.57)

Since the electric ﬁeld is constant in a conductor (and in a semiconductor too), it can be deduced from measurements of voltage and distance. How can we measure the drift velocity? Well, in the same way we always measure velocity; by measuring the time needed to get from point A to C. But can we follow

The most direct way of measuring mobility is to measure the drift velocity caused by a known d.c. electric ﬁeld.

144

Semiconductors

μ = σ/Ne A

C n

Semiconductor +

Switch

Fig. 8.12 Current ﬂow in an n-type semiconductor.

the passage of carriers? Not normally. When, in the circuit of Fig. 8.12, we close the switch the electrons acquire an ordered motion everywhere. Those that happen to be at point C when the switch is closed will arrive at point A some time later, but we have no means of learning when. From the moment the switch is closed, the ﬂow of electrons is uniform at both points, C and A. What we need is a circuit in which carriers can be launched at one point and detected at another point. A circuit that can do this was ﬁrst described by Haynes and Shockley and is shown in Fig. 8.13(a). When S is open, there is a certain current ﬂowing across the resistor R. At t1 the switch is closed and according to the well-known laws of Kirchhoff there is a sudden increase of current [and voltage, as shown in Fig. 8.13(b)] through R. But that is not all. The contact between the metal wire and the n-type semiconductor is a rather special one. It has the curious property of being able to inject holes. We shall say more about injection later, but for the time being please accept that holes appear at point A, when S is closed. Under the inﬂuence of the battery B1 the holes injected at A will move towards C. When they arrive at C (say at time t2 ), there is a new component of current that must ﬂow across R. The rise in current (and in voltage) will be gradual because some holes have a velocity higher than the average, but after a while a steady state develops. Now we know the distance between points A and C, and we know fairly accurately the time needed by the holes to get from A to C; the drift velocity can thus be determined. The electric ﬁeld can easily be obtained, so we have managed to measure, the mobility (Table 8.4). A more modern version of the Haynes–Shockley experiment is to use a narrow light beam for exciting the extra carriers. The physics is then a lot more +

S

+

A

R

C n

+

B1

(a)

V

Fig. 8.13 (a) The Haynes–Shockley experiment. (b) The voltage across R as a function of time. The switch S is closed at t = t1 . The holes drift from A to C in a time t2 – t1 .

(b) t1 Switch closes

t2

Oscilloscope

Time

V

Measurement of semiconductor properties

145

Table 8.4 Semiconductor properties II. Current carriers Semiconductor

m∗e /m

m∗h /m

Group IV C Si Ge SiC

0.2 0.58 0.35

0.25 1.06 0.56

Group III–V Al N Al P Al As Al Sb Ga N Ga P Ga As Ga Sb In N In P In As In Sb Group II–VI Zn O Zn S Zn Se Zn Te Cd O Cd S Cd Se Cd Te

Mobility (cm2 V–1 s–1 ) μe μh 1800 1450 3800 300

1400 500 1820 50

80 1200 200 1350 300 8800 4000

420 550 13 150 400 400 150 460 750

0.33

0.09 0.22 0.35 0.068 0.050 0.11 0.067 0.022 0.014

2.0 1.2 0.4

4600 33 000 78 000

0.38

1.5

180 180 540 340 120 400 450 1200

0.10 0.165 0.13 0.14

0.4 0.5 0.5 0.23

0.8 1.0 0.35

5 28 100 50 50

complicated. As many as three separate phenomena take place simultaneously: drift in the applied ﬁeld, diffusion due to the nonuniform distribution of the created carriers, and recombination as the excess carriers relax back to equilibrium. It is then a little more difﬁcult to work out the mobility, but the basic principles are the same. A less direct way of determining the mobility is to measure the conductivity and use the relationship μ = σ/Ne.

(8.58)

A method often used in practice is the so-called ‘four-point probe’ arrangement shown in Fig. 8.14. The current is passed from contact 1 to 4, and the voltage drop is measured with a voltmeter of very high impedance between points 2 and 3. Since the current ﬂow between the probes is not laminar, some further calculations must be performed. For equally spaced probes, d apart, on a semiconductor of much greater thickness than d, the relationship obtained is σ = I/2π Vd.

(8.59)

Mobility can be calculated from this equation if we know the carrier concentration.

146

Semiconductors Voltmeter leads

Fig. 8.14 The four-point probe. The probes are sharply pointed and held rigidly in a holder which can be pressed with a known force on to the semiconductor. A typical spacing is 1 mm between probes.

Current leads Probe holder 1

2

3

4

Semiconductor sample

Table

It is important to realize that in some applications mobility is a function of ﬁeld. Since practically everything obeys Ohm’s law at low enough ﬁelds we may deﬁne the low ﬁeld mobility as a constant. For high ﬁelds the differential mobility μdiff =

dvD dE

(8.60)

is usually the important quantity in device applications.

8.10.2

The Hall coefﬁcient [eqn (1.20)] is a measure of the charge density, and hence it can be used to relate conductivity to mobility.

For this measurement four contacts have to be made so as to measure the voltage at right angles to the current ﬂow. The basic measurement was described in Chapter 1. However, geometrical factors also come into this. If the distance between voltage probes is greater than that between the current probes the Hall voltage is reduced. Again, this reduction factor is calculable by detailed consideration of the patterns of current ﬂow.

8.10.3 These measurements are commonly made in the microwave region (1010 Hz) at liquid helium temperature (about 4 K) or in the infrared (about 1013 Hz) at liquid nitrogen temperature (77 K).

∗ The

circulator has the following magical properties: a signal fed into arm (1) goes out entirely by arm (2) and a signal fed into arm (2) leaves the circulator by arm (3).

B is the magnetic ﬁeld corresponding to an absorption of signal.

Hall coefﬁcient

Effective mass

The standard method of measuring effective mass uses the phenomenon of cyclotron resonance absorption discussed in Chapter 1. It is essentially an interaction of an electromagnetic wave with charge carriers, which leads to an absorption of the wave when the magnetic ﬁeld causes the electron to vibrate at the same frequency as that of the applied electric ﬁeld. For the resonant absorption to be noticeable the electron must travel an appreciable part of the period without collisions; thus a high-frequency electric ﬁeld, a high-intensity magnetic ﬁeld, and low temperatures are used. In the apparatus for a microwave measurement, shown diagrammatically in Fig. 8.15, the sample is enclosed in a waveguide in a Dewar ﬂask ﬁlled with liquid helium, which is placed between the poles of a large electromagnet. The microwave signal is fed in through a circulator.∗ Thus the signal entering arm (2) is reﬂected by the reﬂecting plate at the end of the waveguide having passed through the semiconductor in each direction and ends up in the receiver connected to arm (3). Employing a wave of ﬁxed frequency and a variable magnetic ﬁeld; the effective mass is given [eqn (1.64)] by m∗ = eB/ωc .

(8.61)

Measurement of semiconductor properties Microwave oscillator

Circulator 1

147

Receiver 3

Waveguide 2 Liquid helium Dewar ﬂask Sample N

S Reﬂecting plate

Fig. 8.15 Schematic representation of the cyclotron resonance experiment.

Electrons

Electromagnet poles

Holes

Holes

Electrons

Absorption

Fig. 8.16 0.0

0.1

0.2

0.3 B Wb m–2

0.4

0.5

0.6

There will generally be several absorption peaks, corresponding to the various holes and electrons present. The experimentally obtained absorption curve for germanium is shown in Fig. 8.16 for a certain orientation between the magnetic ﬁeld and the crystal axes. As may be seen, there are two types of holes, light and heavy. A third resonance peak for the holes in the split-off band is missing because there are hardly any holes so much below the band edge. The two resonance peaks for electrons indicate that something sinister is going on in the conduction band as well. As a matter of fact, these measurements, repeated in various directions, are just the tools for unravelling what the real E–k curve looks like. In addition, from the amplitude and width of the peaks, information about the density and collision times of the various carriers can be obtained (see Exercise 8.19).

8.10.4

Energy gap

A simple way to measure the energy gap between the valence and conduction bands is to see how the conductivity varies with temperature. For any semiconductor the conductivity is given by

Result of a cyclotron resonance experiment for germanium.

148

Semiconductors logeσ Intrinsic region Extrinsic region

Fig. 8.17 Typical log conductivity–reciprocal temperature curve for an extrinsic semiconductor.

l/T

σ = (Ne μe + Nh μh )e,

(8.62)

which is the same as eqn (8.45). For an intrinsic material, we have from eqn (8.46) Ne = Nh = Ni = constant × T 3/2 exp We shall ignore the T 3/2 variation, which will almost always be negligible compared with the exponential temperature variation. Hence a plot of loge σ versus 1/T will have a slope of –Eg /2k, which gives us Eg . Also in eqn (8.64) we have ignored the variation of Eg with temperature.

–Eg 2kT

.

(8.63)

Combining eqn (8.62) with eqn (8.63) we get σ = constant × e(μe + μ h )T Eg . = σ0 exp – 2kT

3/2

Eg exp – 2kT

(8.64)

Let us now consider what happens with an impurity semiconductor. We have discussed the variation of the Fermi level with temperature and concluded that at high temperatures semiconductors are intrinsic in behaviour, and at low temperatures they are pseudo-intrinsic with an energy gap equal to the gap between the impurity level and the band edge. Thus, we would expect two deﬁnite straight-line regions with greatly differing slopes on the plot of loge σ against 1/T, as illustrated in Fig. 8.17. In the region between these slopes the temperature is high enough to ionize the donors fully but not high enough to ionize an appreciable number of electrons from the host lattice. Hence, in this middle temperature range the carrier density will not be greatly inﬂuenced by temperature, and the variations in mobility and the T 3/2 factor that we neglected will determine the shape of the curve. An even simpler method of measuring the energy gap is to study optical transmission. The light is shone through a thin slice of semiconductor [Fig. 8.18(a)] and the amount of transmission is plotted as a function of wavelength. If the wavelength is sufﬁciently small (i.e. the frequency is sufﬁciently large), the incident photons have enough energy to promote electrons

Measurement of semiconductor properties (a)

149

Detector

Light from monochromator

Thin semiconductor sample

(c)

Transmission

Transmission

(b)

Fig. 8.18 0.8

0.9

1.0 1.1 Wavelength, (μm)

1.3

1.2 1.1 Wavelength, (μm)

(a) General arrangement of an optical transmission measurement and the result for (b) GaAs and (c) Si.

1.0

from the valence into the conduction band. Most of the photons are then absorbed, and the transmission is close to zero. As the wavelength increases, there will be a particular value (λ = c/f = hc/Eg ) when band-to-band transitions are no longer possible. The absorption then suddenly declines, and correspondingly, transmission sharply increases as shown in Fig. 8.18(b) for a thin GaAs sample. The point where the sudden rise starts may be estimated from the ﬁgure as about 880 nm, which corresponds to an energy gap of 1.41 eV, which is just about right. Figure 8.18(b) is typical for the so-called direct-gap semiconductors which have an E–k energy band structure [illustrated in Fig. 8.11 and again in Fig. 8.19(a)] where the maximum of the valence band is at the same k value as the minimum of the conduction band. Silicon and germanium are indirect-gap semiconductors as shown in Fig. 8.10 and also in Fig. 8.19(b). The measured transmission as a function

(a)

Light

(b)

E

There are quite a number of directgap semiconductors. In fact, most of the III–V and II–VI compounds belong to that family.

E

hfv

Electron

Light

Eg k

Electron

k

Fig. 8.19 Photon absorption by (a) a direct- and (b) an indirect-gap semiconductor.

150

It may be seen that the energy of the photon is comparable with the gap energies of semiconductors, but its k value is relatively small.

Semiconductors of wavelength for a thin Si sample is plotted in Fig. 8.18(c). The transmission may be seen to vary much more gradually with the wavelength. How does an electron make a transition when excited by a photon? We have not yet studied this problem in any detail. All I have said so far is that if an electron receives the appropriate amount of energy, it can be excited to a state of higher energy. This is not true in general because, as in macroscopic collision processes, not only energy but momentum, as well, should be conserved. There is no way out now. If we wish to explain the excitation of electrons by light in an indirect-gap semiconductor, as shown in Fig. 8.19(b), we have to introduce phonons and we have to consider the momentum of our quantized particles. Phonons are the quantum-mechanical equivalents of lattice vibrations. For a wave of frequency ω the energy of the phonon is ℏω, analogous to the energy of a photon. What can we say about momentum? In Chapter 3 we talked about the momentum operator, and subsequently we showed that the energy of a free electron is equal to E = ℏ2 k 2 /2m, where k comes from the solution of the wave equation. It is the equivalent of the wavenumber of classical waves. The momentum of a free electron is ℏk. When an electron is in a lattice, its energy and momentum are no longer related to each other by the simple quadratic expression. The relationship is then given by the E–k curve, but the momentum is still ℏk. The momenta of photons and phonons are given again by ℏk, but now k = ω/v, where v is the velocity of the wave. For an electromagnetic wave it is v = c = 3 × 108 m s–1 . The velocity of a lattice wave, which may also be called an acoustic wave or, more commonly, a sound wave, is smaller by four or ﬁve orders of magnitude. Hence, for the same frequency the momentum of a phonon is much higher than that of a photon. Let us next do a simple calculation for the momentum of an optical wave. With a wavelength of λ = 1 µm, the corresponding frequency is 3 × 1014 Hz, the energy is 1.24 eV, and kphoton = 6.28 × 106 m–1 . In our simple models of Chapter 7 the zone boundary came to π/a. With a = 0.3 nm, this means that the range of the electronic value of k extends from k = 0 to k = 1010 m–1 . On this scale kphoton is at the origin to a very good approximation. Hence, when we talk about electron excitation in a direct-gap semiconductor, we can regard the transition as practically vertical. The picture of a two-particle interaction is permissible: a photon gives all its energy to an electron. In order to excite an electron in an indirect-gap semiconductor, the photon still has enough energy, but its momentum is insufﬁcient. It needs the good services of a third type of particle, which can provide the missing momentum. These particles are phonons, which are always present owing to the ﬁnite temperature of the solid. They can provide high enough momentum to satisfy momentum conservation. Nevertheless, this is a three-particle interaction between an electron, a photon, and a phonon, which is much less likely than a two-particle interaction. Hence, as the wavelength decreases, the transmission will not suddenly increase as in Fig. 8.18(b). It will instead gently rise and reach saturation when the frequency is large enough [fv in Fig. 8.19(b)] to affect direct transitions between the valence and conduction bands. Whether or not a material is a direct-gap material is of increasing importance in the development of optical semiconductor devices—semiconductor lasers are all direct-gap materials.

Preparation of pure and controlled-impurity single-crystal semiconductors

151

Light input i i1 R +

Voltage measured

– (a)

8.10.5

Fig. 8.20 Dark

Current t1

(b)

Time

(a) Photoconduction experiment in a semiconductor. (b) When the light is switched off the current decays to its dark current value.

Carrier lifetime

We are usually interested in minority carrier lifetime. The reason is simply that, owing to injection or optical generation, the minority carrier density may be considerably above the thermal equilibrium value, whereas the change in the density of majority carriers is generally insigniﬁcant. Consider, for example, silicon with 1022 fully ionized impurities per cubic metre. Then, as Ni for silicon is about 1016 m–3 at room temperature [eqn (8.63)], Nh will be about 1010 m–3 . Now suppose that in addition 1015 electron–hole pairs per cubic metre are created by input light. The hole density in the silicon will then increase by a huge factor, 105 , but the change in electron density will be an imperceptible 10–5 %. Thus, to ‘see’ the change of hole current is relatively simple; the only trick is to make a junction that lets through the holes but restricts the electron ﬂow to a low value. (This again is something we shall discuss later.) Thus, the current ﬂowing in the circuit of Fig. 8.20(a) consists mainly of holes created by the input light. If the light is switched off at t = t1 , the current (and so the voltage) across the resistance R declines exponentially as exp{–(t – t1 )/τh }, where τh is the hole lifetime. By measuring the decay of the current [Fig. 8.20(b)] τh can be determined. How does the exponential decay come about? The differential equation can be easily derived (see Exercise 8.17) on the basis of the physical picture developed in Section 8.5. The rate of change of carriers may always be written as the rate of creation minus the rate of recombination.

8.11 Preparation of pure and controlled-impurity single-crystal semiconductors 8.11.1

Crystal growth from the melt

This is the simplest way of preparing a single crystal. The material is puriﬁed by chemical means, perhaps to an impurity concentration of a few parts per million, then melted in a crucible of the shape shown in Fig. 8.21. The crucible is slowly cooled down. As the pointed end tends to cool slightly faster than the bulk of the material, the crystal ‘seeds’ at the bottom, then grows through the melt. If conditions are well controlled, a single crystal growth is obtained. It is found that the impurity concentration is no longer constant throughout the crystal, but there is a deﬁnite concentration gradient, usually with the purest material at the bottom. To understand the reason for this we have to consider the metallurgical phase diagram for the semiconductor and the impurity. You have probably come across the phase diagram for copper and zinc, stretching from

Molten semiconductor Furnace walls

Fig. 8.21 A form of crucible for melt-grown single crystals.

152

Semiconductors T Liquid A

Ta Tc

Liquidus

Solid

Solidus

Fig. 8.22 Illustration of change of composition on freezing.

The impurity concentration of the solid, still starting at Cb smoothly increases up the crystal.

If it is assumed that k does not change during solidiﬁcation, it is a simple matter to ﬁnd the impurity concentration gradient of the crystal.

Cb

Cd

Ca

Cc

Concentration

100% copper, 0% zinc to 0% copper, 100% zinc, with brasses in the middle, and curves representing liquidus and solidus lines, with temperature as the ordinate. We do not need to consider such a range of composition, since we are considering only a minute amount of impurity in silicon. We need only look at the region close to pure Si, where there will be no complications of eutectics, but only the liquidus and solidus lines, shown diagrammatically in Fig. 8.22. The temperature separations of these lines will be only a few degrees. Suppose there is initially an impurity content Ca (Fig. 8.22). As the melt cools down it stays liquid until it reaches the temperature Ta . At this temperature there can exist liquid of composition Ca and solid of composition Cb . Solid of the latter composition is the ﬁrst to crystallize out. As this is purer material and becomes lost to the rest of the melt once it solidiﬁes, the remainder has a higher impurity concentration, say Cc . Thus, no more solidiﬁcation occurs until the temperature Tc is reached, when more solid impurity concentration Cd comes out. And so it goes on. Of course, if the cooling is slow, this is a continuous process. It is usual to describe this process in terms of the distribution coefﬁcient k, deﬁned as the concentration of impurity in the solid phase divided by the concentration in the liquid phase, both measured close to the phase boundary. For the case of Fig. 8.22, k = Cb /Ca .

(8.65)

In the early days of microelectronics the crystal rods had a diameter of 1–2 cm, as shown in Fig. 8.21. Typical Si chips were 6 mm square. This size persisted for several years but gradually increased so that by the twenty-ﬁrst century the rods were several centimetres in diameter. Now, in 2013, the diameter of a production Si wafer has gone up to about 300 mm (although pre-production experiments have been carried out using 450 mm wafers), so that the melt furnace and crucible are formidable and expensive capital items in the production process.

8.11.2

Zone reﬁning

The different concentrations of impurity in the solid and liquid phase can be exploited in a slightly different way. We start with a fairly uniform crystal,

Preparation of pure and controlled-impurity single-crystal semiconductors (a)

153

Heating coil Furnace wall

Travel

Boat

Molten zone

Temperature Melting point

Fig. 8.23 (b)

Zone reﬁning. The molten zone moving through the crystal sweeps the impurities to the far end.

Distance

melt a slice of it, and arrange for the molten zone to travel along the crystal length. This can be done by putting it in a refractory boat and dragging it slowly through a furnace, as shown in Fig. 8.23. At any point, the solid separating out at the back of the zone will be k times as impure as the melted material which, as k < 1, is an improvement. By a fairly simple piece of algebra it can be shown that the impurity concentration in the solid, Cs (x), after the zone has passed down the crystal (of length l ) once is Cs (x) = C0 {1 – (1 – k) exp(–kx/z)},

(8.66)

where C0 is the initial concentration and z is the length of the molten zone. Clearly, at the end of the crystal that is melted ﬁrst, the value of impurity concentration will be Cs (0) = k n C0

Since k is typically 0.1, it is possible to drive most of the impurity to a small volume at the far end with relatively few passes.

(8.67)

if this process is repeated n times. This very simple idea is the basis of the great success of semiconductor engineering. As we have said before impurities can be reduced to a few parts in 1010 , and then they are usually limited by impurities picked up from reactions with the boat. This latter problem showed up rather strongly when the semiconductor industry went over from germanium (melting point 937 ◦ C) to silicon (melting point 1958 ◦ C). The solution was the ﬂoating zone method, which dispensed with the boat altogether. In this method the crystal is held vertically in a rotating chuck (Fig. 8.24). It is surrounded at a reasonable distance by a cool silica envelope, so that it can be kept in an inert atmosphere, then outside this is a single-turn coil of water-cooled copper tubing. A large high-frequency current (several MHz) is passed through the coil, and the silicon crystal is heated to melting point by the eddy currents induced in it. The coil is slowly moved up

Rotating chuck Floating zone

Heating coil

Silica envelope containing inert atmosphere Crystal

Fig. 8.24 Floating zone reﬁning.

154

Semiconductors the crystal so that the molten zone passes along its length. This technique can be used only for fairly small crystals because the weight has to be supported by the surface tension of the molten zone.

8.11.3

Modern methods of silicon puriﬁcation

Nowadays an entirely different approach is taken to silicon puriﬁcation. Silica (SiO2 ) is ﬁrst reduced to metallurgical grade silicon (98% purity) by reacting it with carbon in an electric arc furnace at 1900 ◦ C–2000 ◦ C. The solid is then converted into a liquid, for example, by reaction with hydrochloric acid (HCl), to form trichlorosilane (SiHCl3 ) in a ﬂuid bed reactor. This liquid is cooled and condensed, and then puriﬁed by fractional distillation, a relatively simple process. Finally, solid silicon with 99.999% purity is created by chemical vapour deposition onto high purity silicon rods or substrates, using a gas source obtained by bubbling hydrogen through the trichlorosilane.

8.11.4

∗ My

friends who speak ancient Greek tell me that epitactic should be the correct adjective. Unfortunately, epitaxial has gained such a wide acceptance among technologists having no Greekspeaking friends that we have no alternative but to follow suit.

Epitaxial growth

The process of growing and reﬁning single crystals made possible the advent of the transistor in the 1950s. The next stage has been the planar technique, starting in about 1960, that has led to the development of integrated circuits, to be discussed in the next chapter. I shall just describe here the epitaxial growth method of material preparation, which is eminently compatible with the manufacture of integrated circuits. ‘Epitaxial’ is derived from a Greek word meaning ‘arranged upon’.∗ There are several ways in which such growth can be carried out. To deposit silicon epitaxially from the vapour phase, the arrangement of Fig. 8.25 can be used. Wafers of single-crystal silicon are contained in a tube furnace at (typically) 1250 ◦ C. Silicon tetrachloride vapour in a stream of hydrogen is passed through the furnace and the chemical reaction SiCl4 + 2H2 Si + 4HCl

(8.68)

takes place. The Si is deposited on the silicon wafers as a single crystal layer following the crystal arrangement of the substrate. Sometimes the silane reaction SiH4 Si + 2H2

(8.69)

is preferred, since it gives no corrosive products. However, silane is pyrophoric; it combusts spontaneously in air, and even dilute mixtures may explode Silicon substrates

Fig. 8.25 Vapour phase epitaxy. The Si forms on the single crystal substrates at a temperature of about 1200◦ C in the furnace.

Gas ﬂow SiCl4+H2

HCl

Heating coil

Preparation of pure and controlled-impurity single-crystal semiconductors

155

violently. As a result silane is extremely dangerous, and handling precautions such as the purging of gas handling systems and the use of concentric stainless steel pipework to surround a silane-carrying pipe with an inert N2 blanket are mandatory. Other hydrides, such as arsine (AsH3 ) and phosphine (PH3 ), which may be used as precursors of the dopants As and P, are even more dangerous. Not only are they pyrophoric, they are also toxic in extremely low concentrations and will kill before their smell (something between garlic and rotting ﬁsh) is noticed. After that, they may also explode. The epitaxial layer can be made very pure by controlling the purity of the chemicals; or more usefully it can be deliberately doped to make it n- or p-type by bubbling the hydrogen through a weak solution of (for example) phosphorus trichloride or boron trichloride, respectively, before it enters the epitaxy furnace. In this way epitaxial layers around 2–20 µm thick can be grown to a known dimension and a resistivity that is controllable to within 5% from batch to batch. Liquid Phase Epitaxy (LPE) has also been used, mainly with compound semiconductors. The substrate crystal is held above the melt on a quartz plate and dipped into the molten semiconductor (Fig. 8.26). By accurately controlling the cooling rate a single-crystal layer can be grown epitaxially on the crystal. In recent years liquid phase epitaxy has been the workhorse in growing semiconductors for lasers (semiconductor lasers will be discussed in Section 12.7). It is simple and quite fast, and it has coped heroically with the problem of stacking semiconductors of differing bandgaps when there was no alternative method, but it cannot really produce the sharply deﬁned layers needed for the latest devices. Some new techniques were bound to come. They are represented by Molecular Beam Epitaxy (MBE), Metal–Organic Chemical Vapour Deposition (MOCVD), Metal–Organic Vapour Phase Epitaxy (MOVPE), and Hydride Vapour Phase Epitaxy (HVPE).

Raise or lower

Seed slice

Quartz holder. Semiconductor seed slice is held on to quartz plate by a quartz spring

Fig. 8.26

Crucible containing semiconductor melt

Furnace wall

SiO2 tube containing inert gas ﬂow

Liquid phase epitaxy. The semiconductor slice is held on the plate by a quartz spring clip and lowered into the molten semiconductor alley. By correct cooling procedures the pure semiconductor is encouraged to precipitate onto the surface of the slice.

156

Semiconductors

8.11.5

Molecular beam epitaxy

This is probably the best and most versatile method. Each material (various semiconductors which make up the desired compound plus the dopants) sits in a little box of its own in which it is heated by an oven to a temperature usually above its melting point, all in ultra-high vacuum. The atoms evaporated from the surface of the heated material are ready to move to the substrate, provided they can get out of the box, that is the shutter is open. The duration for which each shutter is open and the temperature of the oven will then determine the ﬂux of each element toward the substrate, and thus the composition of the growth material. The growth can be monitored by electron scattering from the surface. Altogether this is a very precise method capable of excellent composition control, once all the sources have been experimentally calibrated. It was used to explore ternary and quaternary compounds such as GaAlAs but gave way to cheaper liquid or vapour phase epitaxy once these techniques were established. A further use has been for compounds such as many of the II–VIs, for example ZnS, ZnSe, and CdS where it proved difﬁcult to get both n- and ptypes, usually p was the stumbling block. Whilst the p-type impurities could be established in the crystal lattice, the process of chemical equilibrium on the heated substrate, essential for a good crystalline quality caused the hole centres to be neutralized by electrons. MBE can avoid thermodynamic equilibrium and maintain the p centres active, provided temperature and the ambient atmosphere are controlled. Growing InGaN has been proved to be successful too after overcoming the difﬁculty of a nitrogen source. Initially NH3 was used, but decomposition is only moderately efﬁcient at temperatures below 800◦ C, so copious streams of NH3 are needed in what is ideally a high-vacuum system. Nitrogen plasma sources have evolved based on either an RF discharge at 13.56 MHz or an electron cyclotron resonance breakdown at 2.45 GHz. This allows higher quality growth at about 1 µm h–1 . MOCVD is preferred for commercial production, but MBE has produced higher quality with GaN, for example an electron mobility of 1200 cm2 V–1 s–1 has been reported for an epilayer grown by MBE on a MOCVD template. The usually quoted mobility for ‘typical’ GaN is about half this. The combined use of two techniques to produce better material properties is perhaps the way ahead for InGaN.

8.11.6

Metal–organic chemical vapour deposition

This process is more suited to be adopted by manufacturers. As the name implies, it is a chemical process. The required elements are introduced into the growth tube as compounds bound to organic substances, and they are then chemically released to be deposited upon the substrate. One of the advantages of the technique is that the otherwise poisonous gases are relatively harmless in organic compounds. Another advantage is that the reaction can take place over substrates that have a large area and, in addition, the process is quite fast. Its disadvantage is that it is done at about atmospheric pressure which is in general detrimental to accurate deposition and, among others, it prevents the use of an electron beam to monitor thickness.

Preparation of pure and controlled-impurity single-crystal semiconductors What was largely an effort to pacify safety ofﬁcers and stop the use of large quantities of arsine and phosphine, came into its own with the advent of nitrides. The nitrogen source dimethylhydrazine was used, but it was found that using a similar r.f. discharge source to that used in MBE was preferable. In 1992, several laboratories started work on dilute N additions to semiconductors such as GaAs, InAs, and GaP. Initially the fact that N added to GaAs reduced the bandgap, although GaN has a much wider gap, surprised researchers, but soon the large bowing of the conduction band became well known. A large number of long wavelength devices have been made including lasers in the 1.3 µm range (GaInNAs) and solar cells. In 2002 a 10 Gbit s–1 MOVPE grown Vertical Cavity Surface Emitting Laser (see Section 12.7.3) went onto the market. This work has been done in parallel with MBE and MOCVD usually in the same labs, the former is for research and quality, the latter is preferred for production, especially multilayered structures. The great success of this technique in the past decade has been in the difﬁcult area of producing reasonable quality InGaN for LEDs. There are no nitride substrate crystals, so growth has usually been on sapphire (Al2 O3 ). The reactants are trimethyl gallium and trimethyl indium and ammonia (NH3 ) as a source of nitrogen. The two-ﬂow MOCVD method used at Nichia Chemical Industries ﬁrst heats the sapphire substrate to 1050 ◦ C in a stream of H2 . Then the temperature is lowered to 510 ◦ C to grow a buffer layer of GaN approximately 30 nm thick. Then the main growth of GaN ﬁlm of approximately 2 µm at a temperature of 1020 ◦ C takes about 30 min. At a reduced temperature of about 800 ◦ C the InGaN active layer is grown 0.3 µm in about 60 min. The active layer has a pn detailed structure. InGaN is naturally n-type but the conductivity can be controlled by silicon impurity via a stream of silane (SiH4 ) in the reactant gas. Then there is a very thin layer of InGaN with the In content controlled so that band edge recombination gives the required LED colour. Finally, there is the p layer, which took a while to design. It uses Mg impurity, deposited via a metal-organic compound called bis-cyclopentadienyl magnesium, and has to be followed by an anneal in nitrogen to activate the impurity. The resulting semiconductor slice is riddled with threading dislocations originating at the lattice mismatch with sapphire, typically about 1010 cm–2 . However, once it is metal contacted and cleaved or cut into diodes, usually just under 1 mm2 in area, the LEDs work well with a quantum efﬁciency of 10–50%.

8.11.7

Hydride vapour phase epitaxy (HVPE) for nitride devices

The HVPE technique has attracted great interest because it can produce thick layers at high growth rates and comparatively low cost. The basic reactants are obtained from the following chemical reactions, where the bracketed (g), (l), and (s) refer to gas, liquid, and solid phases, respectively. 2Ga(l) + 2HCl(g) = 2Ga Cl(g) + H2 (g) and for the higher chloride, GaCl(l) + 2HCl(g) = GaCl3 (g) + H2 (g).

157

158

Semiconductors Further, there are two reaction pathways for GaN deposition, GaCl(g) + NH3 (g) = GaN(s) + HCl(g) + H2 (g) 3GaCl(g) + 2NH3 (g) = 2GaN( s) + GaCl(g) + 3H2 (g). The snag in this process is that the decomposition of ammonia is only about 3–4% even at a substrate temperature of 950 ◦ C, and the excess H2 and HCl are no help in the reaction and encourage GaN deposition in other parts of the apparatus. There is also the familiar problem of no readily available, GaN substrate, so sapphire ( Al2 O3 ) is usual, but ZnO, SiC, and Si have been used frequently. As well as threading dislocations from the lattice mismatch, there are also stacking dislocations caused by uneven growth. The main results reported so far have been with layers 10–100 µm thick grown in a few hours, which have produced successful LEDs and lasers. Some layers have been grown up to 300 µm. A major interest is getting free-standing GaN ﬁlms by removing the substrate. One way of doing this is by focusing a laser through the layer on to the sapphire substrate, and by heating it at several points inducing it to crack off. Other substrates such as Si can be etched away with HCl. SiC can be removed by ion etching in SF6 . A very direct method for any substrate is mechanical abrasion with diamond impregnated cloths or a slurry. There is a lot of work going on to improve GaN quality and one possible route to success is by chemical or heat treating free-standing slices for further epitaxy by one of these methods.

Exercises 8.1. Indicate the main steps (and justify the approximations) used in deriving the position of the Fermi level in intrinsic semiconductors. How near is it to the middle of the gap in GaAs at room temperature? The energy gap is 1.4 eV and the effective masses of electrons and holes are 0.067m0 and 0.65m0 respectively. 8.2. Show that the most probable electron energy in the conduction band of a semiconductor is 21 kT above the bottom of the band (assume that the Fermi level is several kT below the conduction band). Find the average electron energy. 8.3. In a one-dimensional model of an intrinsic semiconductor the energy measured from the bottom of the valence band is ℏ2 k12 ℏ2 (k – k1 )2 + . E= 3m0 m0 This is an approximate formula accurate only in the vicinity of the minimum of the conduction band, which occurs when k = k1 = π/a, where a the lattice spacing is 0.314 nm. The Fermi energy is at 2.17 eV.

Calculate (i) the energy gap between the valence and conduction bands, and (ii) the effective mass of electrons at the bottom of the conduction band. Assume that the Fermi level is halfway between the valence and conduction bands. 8.4. The variation of the resistivity of intrinsic germanium with temperature is given by the following table: T(K) 385 455 556 714 ρ( m) 0.028 0.0061 0.0013 0.000274 It may be assumed, as a rough approximation, that the hole and electron mobilities both vary as T –3/2 , and that the forbidden energy gap, Eg , is independent of temperature. (i) Determine the value of Eg . (ii) At about what wavelength would you expect the onset of optical absorption? 8.5. What is the qualitative difference between the absorption spectrum of a direct gap and that of an indirect gap semiconductor?

Exercises 8.6. Considering that Ne Nh = Ni2 in a given semiconductor, ﬁnd the ratio Nh /Ne which yields minimum conductivity. Assume that collision times for electrons and holes are equal and that m∗e /m∗h = 0.5. 8.7. In a certain semiconductor the intrinsic carrier density is Ni . When it is doped with a donor impurity N0 , both the electron and hole densities change. Plot the relative electron and hole densities Ne /Ni and Nh /Ni as a function of N0 /Ni in the range 0 N0 /Ni 10. Assume that all donor atoms are ionized. 8.8. Consider a sample of intrinsic silicon. (i) Calculate the room temperature resistivity. (ii) Calculate the resistivity at 350 ◦ C. (iii) If the resistance of this sample of silicon is R ﬁnd the temperature coefﬁcient of resistance at room temperature deﬁned as (1/R)(dR/dT). How can this be used to measure temperature? Take Eg = 1.1 eV,

m∗e = 0.26m0 ;

μe = 0.15 m2 V–1 s–1 ,

m∗h = 0.39m0 ,

μh = 0.05 m2 V–1 s–1 .

8.9. A sample of gallium arsenide was doped with excess arsenic to a level calculated to produce a resistivity of 0.05 m. Owing to the presence of an unknown acceptor impurity the actual resistivity was 0.06 m, the sample remaining n-type. What were the concentrations of donors and acceptors present? Take μe = 0.85 m2 V–1 s–1 and assume that all impurity atoms are ionized. 8.10. Silicon is to be doped with aluminium to produce p-type silicon with resistivity 10 m. By assuming that all aluminium atoms are ionized and taking the mobility of a hole in silicon to be 0.05 m2 V–1 s–1 , ﬁnd the density of aluminium. 8.11. Estimate what proportion of the aluminium is actually ionized in Exercise 8.10 at room temperature. The acceptor level for aluminium is 0.057 eV above the valence band. 8.12. A sample of silicon is doped with indium for which the electron acceptor level is 0.16 eV above the top of the valence band. (i) What impurity density would cause the Fermi level to coincide with the impurity level at 300 K? (ii) What fraction of the acceptor levels is then ﬁlled? (iii) What are the majority and minority carrier concentrations? Use data from Exercise 8.8. 8.13. A certain semiconductor is doped with acceptor type impurities of density NA which have an impurity level at

159

EA = Eg /5. At the temperature of interest Eg = 20kT and EF = 5kT. The effective masses of electrons and holes are m∗e = 0.12m0 and m∗h = m0 . For NA = 1023 m–3 ﬁnd (i) (ii) (iii) (iv) (v) (vi)

the ionized acceptor density, the ratio of electron density to hole density, the hole density, the electron density, the temperature, the gap energy.

8.14. Show that in the low-temperature region the electron density in an n-type material varies as 1/2

Ne = Nc1/2 ND exp[–(Eg – ED )/2kT]. [Hint: Assume that Ne = ND+ and that the donors are only lightly ionized in that temperature range, i.e. EF > ED .] 8.15. The Bohr radius for a hydrogen atom is given by eqn (4.24). On the basis of the model presented in Section 8.3 determine for silicon the radius of an impurity electron’s orbit. 8.16. The conductivity of an n-type semiconductor is σ at an absolute temperature T1 . It turns out that at this temperature the contributions of impurity scattering and lattice scattering are equal. Assuming that in the range T1 to 2T1 the electron density increases quadratically with absolute temperature, determine the ratio σ (2T1 )/σ (T1 ). 8.17. The rate of recombination (equal to the rate of generation) of carriers in an extrinsic semiconductor is given by eqn (8.50). If the minority carrier concentration in an n-type semiconductor is above the equilibrium value by an amount (δNh )0 at t = 0, show that this extra density will reduce to zero according to the relationship, δNh = (δNh )0 exp(–t/τp ), where

1 . αNe [Hint: The rate of recombination is proportional to the actual density of carriers, while the rate of generation remains constant.] τp =

8.18. Derive the continuity equation for minority carriers in an n-type semiconductor. [Hint: Take account of recombination of excess holes by introducing the lifetime, τp .] 8.19. Figure 8.16 shows the result of a cyclotron resonance experiment with Ge. Microwaves of frequency 24 000 MHz were transmitted through a slice of Ge and the absorption was measured as a function of a steady magnetic ﬁeld applied along a particular crystalline axis of the single-crystal specimen. The ordinate is a linear scale of power absorbed in the specimen. The total power absorbed is always a very small fraction of the incident power.

160

Semiconductors

(i) How many distinct types of charge carriers do there appear to be in Ge from this data? (ii) How many types of charge carriers are really there? How would you deﬁne whether they are ‘real’ charge carriers or not? (iii) What are the effective masses for this particular crystal direction? Can this effective mass be directly interpreted for electrons? For holes?

(iv) If the ﬁgure were not labelled would you be able to tell which peaks referred to electrons? (v) Estimate the collision times of the holes [Hint: Use eqn (1.61)]. (vi) Estimate the relative number density of the holes. (vii) In Section 8.8 we talked about three different types of holes. Why are there only two resonance peaks for holes?

Principles of semiconductor devices

9

Les mystères partout coulent comme les sèves, Baudelaire Les Sept Vieillards This thing with knobs and a pretty light. A. Wesker Chips with everything

9.1 Introduction You have bravely endured lengthy discussions on rather abstract and occasionally nebulous concepts in the hope that something more relevant to the practice of engineering will emerge. Well, here we are; at last we are going to discuss various semiconductor devices. It is impossible to include all of them, for there are so many nowadays. But if you follow carefully (and if everything we have discussed so far is at your ﬁngertips) you will stand a good chance of understanding the operation of all existing devices and—I would add—you should be in a very good position to understand the operation of semiconductor devices to come in the near future. This is because human ingenuity has rather narrow limits. Hardly anyone ever produces a new idea. It is always some combination of old ideas that leads to reward. Revolutions are few and far between. It is steady progress that counts.

9.2 The p–n junction in equilibrium Not unexpectedly, when we want to produce a device, we have to put things together. This is how we get the simplest semiconductor device the p–n junction, which consists of a p- and an n-type material in contact [Fig. 9.1(a)]. Let us imagine now that we literally put the two pieces together.∗ What happens when they come into contact? Remember, in the n-type material there are lots of electrons, and holes abound in the p-type material. At the moment of contact the electrons will rush over into the p-type material and the holes into the ntype material. The reason is, of course, diffusion: both carriers make an attempt to occupy uniformly the space available. Some electrons, moving towards the left, collide head-on with the onrushing holes and recombine, but others will be able to penetrate farther into the p-type material. How far? Not very far; or, to put it another way, not many get very far because their efforts are frustrated by the appearance of an electric ﬁeld. The electrons leave positively charged donor atoms behind, and similarly there are negatively charged acceptor atoms

∗ This

is not how junctions are made.

162

Principles of semiconductor devices (a) p

n

(b)

Conduction band donor levels Fermi level

Fermi level Acceptor levels

Valence band

(c)

(d)

Nh Ne

Fig. 9.1 The p–n junction. (a) A p- and an n-type material in contact, (b) the energy diagrams before contact, (c) the energy diagrams after contact, (d) electron and hole densities.

Log N Nh Ne Junction region

left in the p-type material when the holes move out. This charge imbalance will give rise to an electric ﬁeld, which will increase until equilibrium is reached. Having reached equilibrium, we can now apply a theorem mentioned before when discussing metal–metal junctions. We said that whenever two or more materials are in thermal equilibrium, their respective Fermi levels must agree. The Fermi levels before contact are shown in Fig. 9.1(b) and after contact in Fig. 9.1(c). Here we assume that some (as yet unspeciﬁed) distance away from the junction, nothing has changed; that is, the energy diagram is unaffected, apart from a vertical shift needed to make the two Fermi levels coincide. This is not to diminish the signiﬁcance of the vertical shift. It means that electrons sitting at the bottom of the conduction band on the left-hand side have higher energies than their fellow electrons sitting at the bottom of the conduction band at the right-hand side. By how much? By exactly the difference between the energies of the original Fermi levels. You may complain that by equating the Fermi levels, we have applied here a very profound and general theorem of statistical thermodynamics, and we have lost in the process the physical picture. This is unfortunately true, but nothing stops us returning to the physics. We agreed before that an electric ﬁeld would arise in the vicinity of the metallurgical junction. Thus, the lower energy of the

The p–n junction in equilibrium

163

electrons on the right-hand side is simply due to the fact that they need to do some work against the electric ﬁeld before they can reach the conduction band on the left-hand side. What can we say about the transition region? One would expect the electron and hole densities to change gradually from high to low densities as shown in Fig. 9.1(d). But what sort of relationship will determine the density at a given point? And furthermore, what will be the proﬁle of the conduction band in the transition region? They can all be obtained from Poisson’s equation, d2 U 1 = (net charge density), ǫ dx2

(9.1)

where U is the electric potential used in the usual sense.∗ Since the density of mobile carriers depends on the actual variation of potential in the transition region, this is not an easy differential equation to solve. Fortunately, a simple approximation may be employed, which leads quickly to the desired result. As may be seen in Fig. 9.1(d), the density of mobile carriers rapidly decreases in the transition region. We are, therefore, nearly right if we maintain that the transition region is completely depleted of mobile carriers. Hence we may assume the net charge densities are approximately of the form shown in Fig. 9.2(a). Charge conservation is expressed by the condition NA xp = ND xn .

(9.3)

eNA dU =– (x + C), dx ǫ

(9.4)

Integrating once, we get

C is an integration constant. According to our model, the depletion region ends at –xp . There is no charge imbalance to the left of –xp , hence the electric ﬁeld must be equal to zero at x = –xp . With this boundary condition eqn (9.4) modiﬁes to eNA (x + xp ). ǫ

(9.5)

Similar calculation for the n-type region yields E =

eND (x – xn ). ǫ

(9.6)

The electric ﬁeld varies linearly in both regions, as may be seen in Fig. 9.2(b). It takes its maximum value at x = 0 where there is an abrupt change in its slope. The variation of voltage may then be obtained from x E dx, (9.7) U =– –xp

The transition region is often called the ‘depletion’ region. –xp and xn are the widths of the depletion regions in the p- and n-type materials, respectively.

d2 U eNA = . ǫ dx2

E =

are in a slight difﬁculty here because up to now potential meant the potential energy of the electron, denoted by V . The relationship between the two quantities is eU = V , which means that if you confuse the two things you’ll be wrong by a factor of 1019 .

(9.2)

Poisson’s equation for the region –xp to 0 reduces now to the form

E =–

∗ We

164

Principles of semiconductor devices Net charge density p

n ND +

–xp

x xn

– –NA

(a)

–xp

xn

x

eNDxn ε

(b)

U e (N x 2 + N x 2 ) D n 2ε A p

eNAxp2 2ε

Fig. 9.2 (a) Net charge densities, (b) electric ﬁeld, (c) potential in the transition region of a p–n junction.

–xp

x

xn

(c)

leading to the quadratic function plotted in Fig. 9.2(c). The total potential difference is U0 = U(xn ) – U(–xp ) =

e(NA x2p + ND x2n ) 2ǫ

.

(9.8)

This is called the ‘built-in’ voltage between the p and n regions. A typical ﬁgure for it is 0.7 V. The total width of the depletion region may now be worked out with the aid of equations (9.2) and (9.8), yielding the formula w = xp + xn =

2ǫU0 e(NA + ND )

1/2

NA ND

1/2

+

ND NA

1/2

.

(9.9)

The p–n junction in equilibrium

165

If, say, NA ≫ ND , eqn (9.9) reduces to w=

2ǫU0 eND

1/2

,

(9.10)

which shows clearly that if the p-region is more highly doped, practically all of the potential drop is in the n-region. Taking for the donor density ND = 1021 m–3 and the typical ﬁgure of 0.7 V for the built-in voltage, the width of the transition region in silicon (εr = 11.9) comes to about 1 µm. Remember this is the value for an abrupt junction. In practice, the change from acceptor impurities to donor impurities is gradual, and the transition region is therefore much wider. Thus in a practical case we cannot very much rely on the formulae derived above, but if we have an idea how the acceptor and donor concentrations vary, similar equations can be derived. From our simple model (assuming a depletion region) we obtained a quadratic dependence of the potential energy in the transition region. More complicated models give somewhat different dependence, but they all agree that the variation is monotonic. Our energy diagram is thus as shown in Fig. 9.3. We can describe now the equilibrium situation in yet another way. The electrons sitting at the bottom of the conduction band at the p-side will roll down the slope because they lower their energy this way. So there will be a ﬂow of electrons from left to right, proportional to the density of electrons in the p-type material: Ie(left to right) ∼ Nep .

Hence the electron current from right to left is given by

–(Eg + eU0 – EF ) Ie(right to left) ∼ Nc exp . kB T

eU0

(9.11)

The electrons in the n-type material, being the majority carriers, are very numerous. So, although most of them will be sitting at the bottom of the conduction band, there will still be a considerable number with sufﬁcient energies to cross to the p-side. Assuming Boltzmann statistics, this number is given by –eU0 . (9.12) Nen exp kB T Substituting Nen from eqn (8.17) we get

–(Eg + eU0 – EF ) Nc exp . kB T

The energy difference between the bands on the p- and n-sides is eU0 .

(9.13)

(9.14)

In equilibrium the current ﬂowing from left to right should equal the current ﬂowing right to left; that is,

–(Eg + eU0 – EF ) Nep = Nc exp . (9.15) kB T

Eg

–xp

0

xn

Fig. 9.3 The energy diagram for the transition region of a p–n junction.

166

Principles of semiconductor devices Equation (9.15) gives nothing new. If we express the electron density in the p-type material with the aid of the Fermi level, then we could show from eqn (9.15) that eU0 should be equal to the difference between the original Fermi levels, which we already knew. But although eqn (9.15) does not give any new information, we shall see in a moment that by describing the equilibrium in terms of currents ﬂowing in opposite directions, the rectifying properties of the p–n junction can be easily understood. We could go through the same argument for holes without much difﬁculty, provided we can imagine particles rolling uphill, because for holes that is the way to lower their energy. The equations would look much the same, and I shall not bother to derive them.

9.3

Rectiﬁcation

Let us now apply a voltage as shown in Fig. 9.4. Since there are much fewer carriers in the transition region, we may assume that all the applied voltage will drop across the transition region. Then, depending only on the polarity, the potential barrier between the p and n regions will decrease or increase. (a) p

V1 +

n

–

eU1

eU0

(b) p –

n +

V1

eU0 eU1

Fig. 9.4 The energy diagram of a p–n junction for (a) forward bias and (b) reverse bias.

Rectiﬁcation

167

If the p-side is made positive the potential barrier is reduced, and we talk of forward bias. The opposite case is known as reverse bias; the p-side is then negative, and the potential barrier is increased. It is fairly obvious qualitatively that the number of electrons ﬂowing from left to right is not affected in either case. The same number of electrons will still roll down the hill as in equilibrium. But the ﬂow of electrons from right to left is seriously affected. For reverse bias it will be reduced and for forward bias it will signiﬁcantly increase. So we can see qualitatively that the total current ﬂowing for a voltage U1 will differ from the current ﬂowing at a voltage –U1 . This is what is meant by rectiﬁcation. It is not difﬁcult to derive the mathematical relationships; we have practically everything ready. The current from left to right is the same; let us denote it by I0 . The current from right to left may be obtained by putting e(U0 – U1 ) in place of eU0 in eqn (9.14). [This is because we now want the number of electrons having energies in excess of e(U0 – U1 ), etc.] At U1 = 0, this current is equal to I0 and increases exponentially with U1 ; that is Ie(right to left) = I0 exp(eU1 /kB T).

(9.16)

Hence the total current Ie = Ie(right to left) – Ie(left to right) = I0 [exp(eU1 /kB T) – 1],

(9.17)

which is known as the rectiﬁer equation;∗ it is plotted in Fig. 9.5. For negative values of U1 , Ie tends to I0 , and there is an exponential increase of current with forward voltage. It is worth noting that in spite of the simple reasoning this equation is qualitatively true for real diodes. So, if we plot a graph of log Ie versus applied forward bias voltage, we get a pretty good straight line for most rectiﬁers. However there are two snags:

Above about 1 volt bias, the ﬁnal ‘–1’ in the rectiﬁer equation can be neglected. ∗ Adding the hole current would increase

I0 but the form of the equation would not change because the same exponential factor applies to the hole density in the p-type material.

1. the slope of the line is e/mkB T not e/kB T, where m is a number usually lying between 1 and 2; 2. the current intercept, when the graph is extrapolated back to zero voltage, gives log I0 . But this value of I0 is several orders of magnitude less than the value of I0 obtained by measuring the reverse current (Fig. 9.5). Explaining this away is beyond the scope of this course; it is necessary to take into

I

I0

U1

Fig. 9.5 The current as a function of applied voltage for a p–n junction.

168

Principles of semiconductor devices account recombination and generation of carriers in the depletion region. A good account is given in the book by J.P. McKelvey cited in the further reading list.

9.4

∗ I do not think that the paciﬁst interpret-

ation of the recombination of electrons and holes (they get married, and live happily ever after) can bear closer scrutiny. When an electron and a hole recombine, they disappear from the stage and that’s that. I would however, be willing to accept the above interpretation for excitons which are electron–hole pairs bound together by Coulomb forces but even then one cannot claim that they lived happily ever after because the lifetime of excitons is less than a picosecond, even shorter than the expected duration of modern marriages.

Injection

In thermal equilibrium the number of electrons moving towards the left is equal to the number of electrons moving towards the right. However, when a forward bias is applied, the number of electrons poised to move left is increased by a factor, exp eU1 /kB T. This is quite large; for an applied voltage of 0.1 V the exponential factor is about 55 at room temperature. Thus the number of electrons appearing at the boundary of the p-region is 55 times higher than the equilibrium concentration of electrons there. What happens to these electrons? When they move into the p-region they become minority carriers, rather like immigrants travelling to a new country suddenly become foreigners. But, instead of mere political friction, the electrons’ ultimate fate is annihilation. They are slain by heroic holes, who themselves perish in the battle.∗ Naturally, to annihilate all the immigrants, time and space are needed; so some of them get quite far inside foreign territory as shown in Fig. 9.6, where the density of electrons is plotted as a function of distance in a p–n junction under forward bias. The electron density declines, but not very rapidly. A typical distance is about 1 mm, which is about a thousand times larger than the width of the transition region. Let us go back now to the plight of the holes. They are there in the p-type material to neutralize the negative charge of the acceptor atoms. But how will space charge neutrality be ensured when electrons are injected? It can be done in only one way; whenever the electron density is increased, the hole density must increase as well. And this means that new holes must move in from the contacts. Thus, as electrons move in from the right, holes must move in from the left to ensure charge neutrality. Hence the current of electrons and holes will be made up of six constituents, as shown in Fig. 9.7: (i) The electron current ﬂowing in the n-type material and providing the electrons to be injected into the p-type material. It is constant in the n-region.

Junction Log Ne p

n

Fig. 9.6 The electron distribution in a forward biased p–n junction.

x

Injection

169

Total current (iii) (vi) (iv)

p

(v)

(ii)

n

(i)

Fig. 9.7 The current distribution in a forward biased p–n junction.

(ii) A declining current of injected electrons in the p-region. The current declines because the number of electrons becomes less and less as they recombine with the holes. (iii) The current of holes in the p-region to provide the holes to be injected into the n-region. We have not discussed this because the injection of holes is entirely analogous to the injection of electrons. (iv) A declining current of injected holes in the n-region. The current declines because of recombination with electrons. (v) A declining current of holes in the p-region to compensate for the holes lost by recombination. (vi) A declining current of electrons in the n-region to compensate for the electrons lost by recombination. Adding up the currents, you can see that the total current is constant, as it should be. The discussion above includes all the effects of recombination, which occur when the distance between the depletion layer and the contacts is long. Often the distance is much shorter. In this case a simpler model (known, unsurprisingly, as the short diode approximation) may be used. Recombination may be neglected, on the grounds that the injected minority carriers do not have much of an opportunity to recombine before they reach the contacts. Since the individual currents carried by the injected carriers must now be constant, the minority carrier density variations must now be straight lines (remember that diffusion currents depend on the gradients of carrier densities). When is a diode short and when is it long? Generally it is considered to be short if the distance to the contacts is smaller than the diffusion length, and long otherwise. When do we want it to be short? In microelectronics, most of the time. Recombination will often be accompanied by heating, because the energy given up during recombination must go somewhere. If it is used for phonon generation, the device will run hot. At the very least it will waste energy, and it will very probably not last as long as a device running cold. The exception is optoelectronics, which we will cover later on. In light emitting diodes and laser diodes, direct-gap materials are used, and recombination will be accompanied by photon generation. Because light emission is exactly the desired effect, a long diode is exactly what is required. Let me emphasize again that the current in a p–n junction is quite different from the currents you have encountered before. When you apply a voltage to

170

Principles of semiconductor devices a piece of metal, all that happens is that the electrons, which are already there, acquire some ordered motion. When a forward bias is applied to a p–n junction minority carriers get injected into both regions. These minority carriers were not there originally in such a high density; they came as a consequence of the applied voltage. The distinction between ordinary conduction and minority carrier injection is important. It is the latter which makes transistor action possible.

9.5

U0 is the ‘built-in’ voltage.

Junction capacity

I would like to say a few more words about the reverse biased junction. Its most interesting property (besides the high resistance) is that the presence of two layers of space charge in the depletion region makes it look like a capacitor. We may calculate its capacitance in the following way. We ﬁrst derive the relationship between the width of the depletion layer in the n-region and the voltage in the junction, which may be obtained from eqns (9.2) and (9.8). We get

U1 is the applied voltage in the reverse direction.

xn =

2ǫU0 NA eND (ND + NA )

1/2

.

(9.18)

For reverse bias the only difference is that the barrier becomes larger, that is U0 should be replaced by U0 + U1 , yielding xn =

2ǫ(U0 + U1 )NA eND (ND + NA )

1/2

.

(9.19)

The total charge of the donor atoms is

NA ND 1/2 Q = eND xn = 2ǫe(U0 + U1 ) . NA + ND

Now a small increase in voltage will add charges at the boundary—as happens in a real capacitance. We may, therefore, deﬁne the capacitance of the junction (per unit area) as

R1

C= R (U1)

(9.20)

C (U1)

Fig. 9.8 The equivalent circuit of a p–n junction.

∂Q = ∂U1

NA ND ǫe 2(U0 + U1 ) NA + ND

1/2

.

(9.21)

We can now assign an equivalent circuit to the junction and attribute a physical function to the three elements (Fig. 9.8). R1 is simply the ohmic resistance of the ‘normal’, that is not depleted, semiconductor. R(U1 ) is the junction resistance. It is very small in the forward direction (0.1–10 typically) and large in the reverse direction (106 –108 typically). C(U1 ) is the capacitance that varies with applied voltage, given by eqn (9.21). Clearly, this equation loses validity for strong forward bias because the depletion layer is then ﬂooded by carriers. This is actually borne out by our equivalent circuit, which shows that the capacity is shorted-out when R(U1 ) becomes small. With

The transistor

171

a reverse biased diode, C(U1 ) is easily measured, and can be ﬁtted to an equation like (9.21) very well. The characteristic of a commercial diode is plotted in Fig. 9.9. Here C is proportional to (U1 + 0.8)–1/2 , whence the constant 0.8 V may be identiﬁed with the ‘built-in’ voltage.

C (pF)

60

40

9.6 The transistor Here we are. We have arrived at last at the transistor, the most famous electronic device of the century. It was discovered at Bell Telephone Laboratories by Bardeen, Brattain, and Shockley in 1948. Since then it has conquered the world many times over. It made possible both the pocket radio and giant computers, to mention only two applications. The number of transistors manufactured is still growing fast from year to year. The ﬁgure for 1967, when we ﬁrst prepared these lectures, was a few times 109 ; that is about one transistor for every man, woman, and child living on Earth. I do not think anyone knows the number of transistors produced nowadays. We are rapidly approaching the stage when a single chip may contain as many transistors as the number of inhabitants of the Earth. There is a slight difﬁculty here because it is no longer clear what we mean by a transistor. Originally, there was the point-contact transistor, which was not very reliable, followed then by the junction transistor. Our treatment in this section applies to the junction transistor, which after a while became known as the transistor, but sometime later, in view of the appearance of other varieties, it had to be rechristened. It is now known as the bipolar transistor. I am afraid the discussion of the transistor will turn out to be an anticlimax. It will seem to be too simple. If you ﬁnd it too simple, remember that we have trodden a long tortuous path to get there. It might be worthwhile to recapitulate the main hurdles we have scaled: 1. Postulation of Schrödinger’s equation. 2. The solution of Schrödinger’s equation for a rigid, three-dimensional potential well. 3. Postulation of Pauli’s principle and the introduction of spin. 4. Formulation of free electron theory, where electrons ﬁll up the energy levels in a potential well up to the Fermi energy. 5. Derivation of the band structure by a combination of physical insight and Schrödinger’s equation. 6. Introduction of the concept of holes. 7. Demonstration of the fact that electrons at the bottom of the conduction band (and holes at the top of the valence band) may be regarded as free, provided that an effective mass is assigned to them. 8. Determination of the Fermi level and carrier densities in extrinsic semiconductors. 9. The description of a p–n junction in terms of opposing currents. 10. Explanation of minority-carrier injection. So if you want to go through a logical chain of reasoning and want to explain the operation of the transistor from ﬁrst principles, these are the main steps in the argument.

20 U1 (volt) –6

–4

–2

0

0

Fig. 9.9 Capacitance of a commercially available junction diode as a function of applied voltage.

All three of them received the Nobel Prize for their invention in 1956. It is interesting to note that this was one of the few cases when the Prize was given for the invention of a device rather than for a discovery in physics.

A

Signal input

Collector

because the emitter current is not carried solely by holes. There is also an electron ﬂow from the base into the emitter. However, transistors are designed in such a way that the conductivity of the base is well below the conductivity of the emitter (a typical ﬁgure may be a factor of a hundred); thus the minority-carrier ﬂow from the base to the emitter is usually negligible.

Now let us see the transistor itself. It consists of two junctions with one semiconductor region common to both. This is called the base, and the other two regions are the emitter and the collector as shown in Fig. 9.10 for a p–n–p transistor. There are also n–p–n transistors; the ensuing explanation could be made to apply to them also by judicious changing of words. Consider ﬁrst the emitter–base p–n junction. It is forward biased (positive on p-side for those who like mnemonics). This means that large numbers of carriers ﬂow, holes into the base, electrons into the emitter, Now the holes arriving into the base region will immediately start the process of recombination with electrons. But, as explained before, time and space are needed to annihilate the injected minority-carriers. Hence, for a narrow base region (≪ 1 mm), the hole current leaving the base region will be almost identical to the hole current entering from the emitter. Now what happens to the holes when they arrive at the collector region? They see a negative voltage (the base–collector junction is reverse biased) and carry on happily towards the load. Thus, practically the same current that left the emitter ﬁnds its way to the load.∗ So far there is nothing spectacular; the current gain of the device is somewhat below unity. Why is this an ampliﬁer? It is an ampliﬁer because the voltage gets ampliﬁed by a large factor. This is because the input circuit is a low impedance circuit; a low voltage is thus sufﬁcient to cause a certain current. This current reappears in the high impedance output circuit and is made to ﬂow across a large load resistance, resulting in a high output voltage. Hence the transistor in the common base circuit is a voltage ampliﬁer. We should, however, know a little more about this ampliﬁer. Can we express its properties in terms of the usual circuit parameters: impedances, current sources, and voltage sources? How should we attempt the solution of such a problem? Everything is determined in principle. If the bias voltages are ﬁxed and an a.c. voltage is applied to the input of the transistor in Fig. 9.10, then the output current is calculable. Is this enough? Not quite. We have to express the frequency dependence in the form of rational fractions (this is because impedances are either proportional or inversely proportional to frequency) and then an equivalent circuit can be deﬁned. It is a formidable job; it can be done and it has been done, but, of course, the calculation is far too lengthy to include here.

Base

∗ The above argument is not quite correct

Principles of semiconductor devices

Emitter

172

P

n

P

~

RL

RS B

Fig. 9.10 The p–n–p transistor as an ampliﬁer.

+

+

Signal output

The transistor Although we cannot solve the complete problem, it is quite easy to suggest an approximate equivalent circuit on the basis of our present knowledge. Looking in at the terminals A and B of Fig. 9.10, what is the impedance we see? It comprises three components: the resistance of the emitter, the resistance of the junction, and the resistance of the base. The emitter is highly doped in a practical case, and we may therefore neglect its resistance, but the base region is narrow and of lower conductivity and so we must consider its resistance. Hence we are left with re (called misleadingly the emitter resistance) and rb (base resistance), forming the input circuit shown in Fig. 9.11(a). What is the resistance of the output circuit? We must be careful here. The question is how will the a.c. collector current vary as a function of the a.c. collector voltage? According to our model, the collector current is quite independent of the collector voltage. It is equal to αie , where ie is the emitter current, and α is a factor very close to unity. Hence, our ﬁrst equivalent output circuit must simply consist of the current generator shown in Fig. 9.11(b). In practice the impedance turns out to be less than inﬁnite (a few hundred thousand ohms is a typical ﬁgure); so we should modify the equivalent circuit as shown in Fig. 9.11(c). Having got the input and output circuits, we can join them together to get the equivalent circuit of the common base transistor∗ [Fig. 9.11(d)]. We have not included any reactances. Can we say anything about them? Yes, we can. We have already worked out the junction capacity of a reverse biased junction. That capacity should certainly appear in the output circuit in parallel with rc . There are also some other reactances as a consequence of the detailed mechanism of current ﬂow across the transistor. We can get the numerical values of these reactances if we have the complete solution. But luckily the most important of these reactances, the so-called diffusion reactance, can be explained qualitatively without recourse to any mathematics.

173

re is in fact the resistance of the junction.

∗ This

exceedingly simple construction cannot be done in general but is permissible in the present case when rc ≫ rb .

(b)

(a)

αie ie

re Collector rb

Emitter

(c)

Fig. 9.11

(d) αie

αie re rc

rc Collector

Emitter

rb

Collector

The construction of an equivalent circuit of a transistor. (a) The emitter–base junction. (b) In ﬁrst approximation the collector current depends only on the emitter current. (c) In a more accurate representation there is a collector resistance rc as well as the collector circuit. (d) The complete low-frequency equivalent circuit.

The emitter current as a function of time when the emitter voltage is suddenly increased. It looks like the current response of a parallel RC circuit.

∗ Not

to depart from the usual notations, we are using j here as honest engineers do, but had we done the analysis with our chosen exp(–iωt) time dependence, we would have come up with –i instead of j.

† The

full expression for ie should contain a term dependent on the emitter-tocollector voltage. This is usually small. Look it up in a circuitry book if you are interested in the ﬁner details.

Emitter current

Fig. 9.12

Principles of semiconductor devices

Emitter voltage

174

t

t

Let us look again at the p–n junction of the p–n–p transistor. When a step voltage is applied in the forward direction, the number of holes able to cross into the n-region suddenly increases. Thus, in the ﬁrst moment, when the injected holes appear just inside the n-region, there is an inﬁnite gradient of hole density, leading to an inﬁnitely large diffusion current. As the holes diffuse into the n-region, the gradient decreases, and ﬁnally the current settles down to its new stationary value as shown in Fig. 9.12. But this is exactly the behaviour one would expect from a capacitance in parallel with a resistance. Thus, when we wish to represent the variation of emitter current as a function of emitter voltage, we are entitled to put a capacitance there. This is not a real honest-to-god, capacitance; it just looks as if it were a capacitance, but that is all that matters. When drawing the equivalent circuit, we are interested in appearance only! Including now both capacitances, we get the equivalent circuit of Fig. 9.13. We are nearly there. There is one more important effect to consider: the frequency dependence of α. It is clear that the collector current is in phase with the emitter current when the transit time of the carriers across the base region is negligible, but α becomes complex (and its absolute value decreases) when this transit time is comparable with the period of the a.c. signal. We cannot go into the derivation here, but α may be given by the simple formula∗ α=

α0 , 1 + j(ω/ωα )

(9.22)

where ωα is called the alpha cut-off frequency. The corresponding equivalent circuit is obtained by replacing α in Fig. 9.13 by that given in eqn (9.22). And that is the end as far as we are concerned. Our ﬁnal equivalent circuit represents fairly well the frequency dependence of a commercially available transistor. We have seen that the operation of the transistor can be easily understood by considering the current ﬂow through it. The frequency dependence is more complicated, but still we have been able to point out how the various reactances arise. It has been convenient to describe the common base transistor conﬁguration, but of course the most commonly used arrangement is the common emitter, shown in Fig. 9.14(a). Again, most of the current ie from the forward-biased emitter–base junction gets to the collector, so we can write† ic = αie ,

(9.23)

The transistor

175

αie

re

rc

Ce

Cc rb

Fig. 9.13

Emitter

Collector

A good approximation to the high-frequency equivalent circuit of a transistor.

ic RL

~ +

ib Vbe

ic n Collector p Base n Emitter

RL

+

ib

~

ie

(a)

ie (b)

ib Collector

Base

Fig. 9.14

hfe ib

hie

The common emitter transistor. (a) General circuit arrangement, showing current and voltage nomenclature. (b) Circuit diagram. (c) Equivalent circuit of the transistor.

Emitter (c)

as before, and i c = ie – ib =

αib = hfe ib , 1–α

(9.24)

where we have introduced a current gain parameter, hfe , which is usually much greater than unity. This ﬁxes the right-hand side of the equivalent circuit of Fig. 9.14(c) as a current generator hfe times greater than the input current. The input side is a resistance, hie , which again includes the series resistance of the base and emitter contact regions. I have so far talked about the applications of transistors as ampliﬁers, that is, analogue devices. Historically, these applications came ﬁrst because at the time of the invention of the transistor there was already a mass market in existence eager to snap up transistor ampliﬁers—particularly for portable devices. The real impact of the transistor came, however, not in the entertainment business

Note that the major part of transistor ampliﬁer design is based on the simple equivalent circuit of Fig. 9.14(c). At high frequencies, of course, the capacitances discussed have to be added.

176

Principles of semiconductor devices

Ic

UE

R

IB

UCE

Fig. 9.15 A transistor as a logic element.

but in computers. Admittedly, computers did exist before the advent of the transistor, but they were bulky, clumsy, and slow. The computers you know and respect, from giant ones down to pocket calculators, depend on the good services of transistors. One could easily write a thousand pages about the circuits used in various computers—the trouble is that by the time the thousandth page is jotted down, the ﬁrst one is out of date. The rate of technical change in this ﬁeld is simply breathtaking, much higher than ever before in any branch of technology. Fortunately, the principles are not difﬁcult. For building a logic circuit all we need is a device with two stable states, and that can be easily provided by a transistor, for example in a form (Fig. 9.15) quite similar to its use as an ampliﬁer. When the base current, IB = 0 (we use capital letters to describe the d.c. current), no collector current ﬂows, Ic = 0, and consequently UCE = UE . If a base current is impressed upon the circuit, then a collector current ﬂows, and UCE is close to zero. Hence, we have a ‘high’ and a ‘low’ output voltage which may be identiﬁed with a logical ‘1’ or ‘0’ (or the other way round). I shall not go into any more details, but I would just like to mention some of the acronyms in present-day use for which transistors are responsible. They include TTL (transistor–transistor logic), ECL (emitter coupled logic) and I2 L (integrated injection logic).

9.7

∗ In

a metal the charge inequality is conﬁned to the surface. † We

met a very similar case before when discussing p–n junctions. If one of the materials is highly doped, all the potential drop takes place in the other material.

Metal–semiconductor junctions

Junctions between metals and semiconductors had been used in radio engineering for many years before the distinction between p- and n-type semiconductors was appreciated. Your great-great-grandfathers probably played about with ‘cat’s whiskers’ in their early ‘crystal sets’, as radios were then called, stressing the importance of the piece of coal or whatever was used as the semiconductor detector. The behaviour of metal–semiconductor junctions is more varied to describe than that of p–n junctions. We ﬁnd that there is different behaviour on the one hand, with p- and n-type semiconductors, and on the other, when the metal work function is greater or less than that of the semiconductor. We shall ﬁrst consider the case of an n-type semiconductor in contact with a metal, whose work function is greater than that of the semiconductor. The semiconductor work function (φS in Fig. 9.16) is deﬁned as the energy difference between an electron at the Fermi energy and the vacuum level. The fact that there are usually no electrons at the Fermi energy need not bother us—we do not have to explain deﬁnitions. Another measure often used is the electron afﬁnity, φB . The band structure of the two substances is shown in Fig. 9.16(a). When they are joined together, we may apply again our general theorem and make the Fermi levels equal. Thus, we may start the construction of Fig. 9.16(b) by drawing a horizontal line for the Fermi energy, and a vertical one for the junction. We leave the metal side unchanged because we shall assume that ‘band-bending’ cannot occur in a metal.∗ We are really saying here that all the potential drop will take place in the semiconductor, which, in view of the much smaller number of carriers there, is a reasonable assumption.† Away from the junction we draw the valence band edge, the conduction band edge, and the vacuum level in the same position (relative to the Fermi level) as for the bulk

Metal–semiconductor junctions

177

(a) φS

φM

Conduction band

φB

EFS EFM

Valence band

(b) φM EFM

φM–φB

φM–φS

φS Conduction band EFS

Valence band

material, in Fig. 9.16(a). These are shown as solid lines. Now with an inﬁnitely small gap the vacuum levels are equal; thus, we may join them with a dotted line in Fig. 9.16(b); the conduction and valence band edge must also be continued parallel to the vacuum level. What can we say about the charges? We may argue in the same fashion as for a metal–metal junction. In the ﬁrst instance, when the metal and the semiconductor are brought together, the electrons from the conduction band cross over into the metal in search of lower energy. Hence a certain region in the vicinity of the junction will be practically depleted of mobile carriers. So we may talk again about a depletion region and about the accompanying potential variation, which is incidentally, the same thing as the ‘band-bending’ obtained from the band picture. So the two pictures are complementary to a certain extent. In the ﬁrst one the ‘band-bending’ is a consequence of the matching of the Fermi levels and vacuum levels, and the charge imbalance follows from there. In the second picture electrons leave the semiconductor, causing a charge imbalance and hence a variation in the potential energy. Whichever way we look at it, the outcome is a potential barrier between the metal and the semiconductor. Note that the barrier is higher from the metal side. In dynamic equilibrium the number of electrons crossing over the barrier from the metal to the semiconductor is equal to the number crossing over the barrier from the semiconductor side. We may say that the current I0 ﬂows in both directions. Let us apply now a voltage; according to the polarity, the electrons’ potential energy on the semiconductor side will go up or down. For a forward bias it goes up, which means that we have to draw the band edges higher up. But the vacuum level at the junction stays where it was. So the effect of the

Fig. 9.16 Energy diagrams for a junction between a metal and an n-type semiconductor (φM > φS ), (a) before contact, (b) after contact the Fermi levels agree (EFM = EFS ).

178

Principles of semiconductor devices

φM - φS - eU1

φM

Fig. 9.17 The junction of Fig. 9.16 under forward bias. The potential barrier for electrons on the semiconductor side is reduced by eU1 .

higher band edges is smaller curvature in the vicinity of the junction and a reduced potential barrier, as shown in Fig. 9.17. Now all electrons having energies above φM – φS – eU1 may cross into the metal. By analogy with the case of the p–n junction it follows that the number of carriers (capable of crossing from the semiconductor into the metal) has increased by a factor exp eU1 /kB T, and hence the current has increased by the same factor. Since the current from the metal to the semiconductor has not changed, the total current is I = I0 [exp(eU1 /kT) – 1];

(9.25)

that is, a junction of this type is a rectiﬁer. There is one point I want to make concerning the potential barrier in this junction. One of the electrodes is a metal, and there are charged carriers in the vicinity of the metal surface. Does this remind you of any physical conﬁguration we have studied before? Where have we met a potential barrier and charged carriers giving rise to image charges? In the study of electron emission in Chapter 6 we came to the conclusion that the image charges lead to a lowering of the potential barrier, and you may remember that it was called the Schottky effect. According to the formula we derived there, the reduction was proportional to (E /ǫ0 )1/2 . Well, the same thing applies here with the difference that ǫ0 should be replaced by ǫr ǫ0 , where ǫr is the relative dielectric constant of the semiconductor. For silicon, for example, ǫr = 12, the effect is therefore smaller. So the Schottky effect is not very large, but it happened to give its name to these particular junctions. They are usually referred to as Schottky diodes or Schottky barrier diodes. Let us now investigate the case when the work function of the metal is smaller than that of the n-type semiconductor. The situation before and after contact is illustrated in Fig. 9.18. Now, to achieve equilibrium, electrons had to move from the metal to the semiconductor, establishing there an accumulation region. There is no potential barrier now from whichever side we look at the junction. As a consequence the current ﬂow does not appreciably depend on the polarity of the voltage. This junction is not a rectiﬁer.

9.8 The role of surface states; real metal–semiconductor junctions The theory of metal–semiconductor junctions as presented above is a nice, logical, consistent theory that follows from the physical picture we have developed so far. It has, however, one major disadvantage: it is not in agreement with experimental results, which seem to suggest that all metal–semiconductor

The role of surface states; real metal–semiconductor junctions

179

(a) φM

φS

Conduction band

φB

EFM EFS

Valence band

φS

(b)

Conduction band

φM EFM

φS - φM

EFS

Fig. 9.18 Valence band

junctions are rectiﬁers independently of the relative magnitudes of the work functions. This does not necessarily mean that the theory is wrong. The discrepancy may be caused by the physical realization of the junction. Instead of two clean surfaces lining up, there might in practice be some oxide layers, and the crystal structure might be imperfect. This may be one of the reasons why ‘real’ junctions behave differently from ‘theoretical’ junctions. The other reason could be that the theory, as it stands, is inadequate, and to get better agreement with experiments, we must take into account some hitherto neglected circumstance. Have we taken into account anywhere that our solids are of ﬁnite dimensions? Yes, we have; we determine the number of allowed states from the boundary conditions. True, but that is not the only place where the ﬁniteness of the sample comes in. Remember, in all our models leading to the band picture we have taken the crystal as perfectly periodic, and we have taken the potential as perfectly periodic. This is surely violated at the surface. The last step in the potential curve should be different from the others, that is, the potential proﬁle in the solid should rather be chosen in the form displayed in Fig. 9.19. It was shown some years ago that the assumption of such a surface barrier would lead to the appearance of some additional discrete energy levels in the forbidden gap; these are generally referred to as surface states.

Energy diagrams for a junction between a metal and an n-type semiconductor (φM < φS ), (a) before contact, (b) after contact the Fermi levels agree (EFM = EFS ).

Vacuum

V

Surface

Fig. 9.19 The potential energy distribution near the surface of a crystal.

180

Principles of semiconductor devices Conduction band

Occupied surface states

Valence band

Fig. 9.20 In a real semiconductor electrons may occupy surface states. The donor atoms left behind have a positive charge which leads to the ‘bending’ of the band.

Igor Yevgenevich Tamm received the Nobel Prize in 1958.

If we assume a semiconductor is n-type, some of these surface states may be occupied by electrons that would otherwise be free to roam around. Some of the donor atoms will therefore have uncompensated positive charges leading to ‘band-bending’ as shown in Fig. 9.20. Thus, the potential barrier is already there before we even think of making a metal contact. What happens when we do make contact between the semiconductor and the metal? Let us choose the case where the metal has the lower work function, when according to our previous theory the junction is not rectifying. Then, as we have agreed before (and it is still valid) electrons must ﬂow from the metal to the semiconductor until equilibrium is established. But if there is a sufﬁcient number of empty surface states still available, then the electrons will occupy those without much affecting the height of the potential barrier. So the potential barrier stays, and the junction is rectifying. It would be difﬁcult in a practical case to ascertain the share of these ‘theoretical’ surface states, also called Tamm states, in determining the behaviour of the junction because surface imperfections are also there, and those can trap electrons equally well. It seems, however, quite certain that it is the surface effects that make all real metal–semiconductor junctions behave in a similar manner. Finally, I would like to mention ohmic contacts, that is, contacts that do not care which way the voltage is applied. To make such a contact is not easy; it is more an art than a science. It is an important art though, since all semiconductor devices have to be connected to the outside world. The two most often used recipes are: (i) to make the contact with alloys containing metals (e.g. In, Au, Sn) that diffuse into the surface forming a gradual junction; or (ii) to make a heavily doped semiconductor region (usually called n+ or p+ ) with about 1024 carriers per cubic metre in between the metal and semiconductor to be connected.

9.9

Vacuum level Fermi level

Conduction band Valence band

Metal

Insulator Semiconductor

Fig. 9.21 Energy diagram for a metal–insulator–n-type semiconductor junction at thermal equilibrium.

Metal–insulator–semiconductor junctions

Let us now make life a little more complicated by adding one more component and look at metal–insulator–semiconductor junctions. What happens as we join the three materials together? Nothing. If the insulator is thick enough to prevent tunnelling (the situation that occurs in all practical devices of interest), the metal and the semiconductor are just unaware of each other’s existence. What does the energy diagram look like? For simplicity we shall assume that the Fermi levels of all three materials coincide before we join them together. The energy diagram then takes the form shown in Fig. 9.21, where the semiconductor is taken as n-type. Are there any surface states at the semiconductor–insulator interface? In practice there are, but their inﬂuence is less important than for metal– semiconductor junctions, so we shall disregard them for the time being. Let us now apply a positive voltage to the metal as shown in Fig. 9.22(a). Will a current ﬂow? No, there can be no current through the insulator. The electrons will nevertheless respond to the arising electric ﬁeld by moving towards the insulator. That is as far as they can go, so they will accumulate in front of the insulator. Their distribution will be something like that shown in

Metal–insulator–semiconductor junctions (a)

(b)

Vacuum level

(c)

M I S

log Ne

Conduction band EF

Nen +

181

eU0 Valence band

x

0

– U0

Fig. 9.22 A metal–insulator–n-type semiconductor junction under forward bias. (a) Schematic representation. (b) Variation of electron density in the semiconductor as a function of distance. (c) Energy diagram.

Fig. 9.22(b), where Nen is the equilibrium concentration in the bulk semiconductor, and x is the distance away from the insulator. The shape of the curve may be obtained from the same considerations as in a p–n junction. The diffusion current (due to the gradient of the electron distribution) ﬂowing to the right must be equal to the conduction current (due to the applied ﬁeld) ﬂowing to the left. The corresponding energy diagram is shown in Fig. 9.22(c), where the Fermi level in the semiconductor is taken as the reference level. Looking at the energy diagram, we may now argue backwards and say that eqn (8.17) must still be roughly valid so the electron density is approximately an exponential function of the distance of the Fermi level from the bottom of the conduction band. Hence the electron density is increasing towards the insulator. Next, let us apply a negative voltage to the metal [Fig. 9.23(a)]. The electrons will be repelled, creating a depletion region, as in a reverse biased p–n junction. In fact, we could determine the width of the depletion region (see Example 9.4) by a method entirely analogous to that developed in Section 9.2. Alternatively, we can argue that the electron distribution will be of the shape

(a)

(b) M I S

log Ne

Nen –

+

0

x

U0 (c)

(d)

Fig. 9.23 Vacuum level

eU0

eU0

Conduction band EF

Holes

Valence band

A metal–insulator–n-type semiconductor junction under reverse bias. (a) Schematic representation. (b) Variation of electron density in the semiconductor as a function of distance. (c) Energy diagram at moderate voltage. (d) Energy diagram at a voltage high enough for producing holes.

182

The phenomenon of inversion is not restricted of course to n-type semiconductors. Similar inversion occurs in a metal–insulator–p-type semiconductor junction.

Principles of semiconductor devices shown in Fig. 9.23(b), and we may talk again about the balance of diffusion and conduction currents. Finally the band-bending picture is shown in Fig. 9.23(c), from which we can also conclude that the electron density is decreasing towards the insulator. What will happen as we apply higher and higher reverse bias? The obvious answer is that the depletion region will widen. What else could one expect? It is difﬁcult to believe at ﬁrst hearing, but the fact (fortunate as it happens) is that holes will appear. Can we explain this phenomenon by any of our models? If we consider only ionized donor atoms and mobile electrons, as in the model developed in Section 9.2, we have not got the slightest chance of creating holes. On the other hand if we adopt the notion that the density of a carrier at any point is determined by the distance in energy from the Fermi level to the edge of the particular band, then holes have acquired the right to appear. All we need to do is to apply a sufﬁciently large reverse bias [Fig. 9.23(d)] which will bring the Fermi level right down, close to the top of the valence band. Thus, according to this model, holes may become the majority carriers near to the surface of an n-type semiconductor. Odd, is it not? The problem still remains, though, that the holes must come from somewhere. The only process known to produce holes in an n-type semiconductor is thermal generation of electron–hole pairs. But are not the rates of generation and recombination equal? Would not the holes generated thermally immediately disappear by recombination? This is true indeed under thermal equilibrium conditions, but our junction is not necessarily in thermal equilibrium. Let us look again at the whole process, considering time relationships as well. At t = 0 we apply a negative voltage to the junction. Most of the electrons clear out by t1 , leaving a depletion region of the order of 1 µm behind. What happens now to thermally generated electron–hole pairs? The electrons move away from the insulator, and the holes move towards the insulator. Not much recombination will occur because both the electron and hole densities are small, and they are separated in space. What will happen to the holes? They will congregate in the vicinity of the insulator, where they can ﬁnd a nice comfortable potential minimum. The conditions of equilibrium are rather complicated. At the end, say by t2 , the hole diffusion current away from the insulator must be equal to the hole conduction current towards the insulator, and the rates of generation and recombination must balance each other. It is then quite reasonable to conclude that if the applied negative voltage is large enough, that is the potential minimum at the insulator surface is deep enough, then a sufﬁcient number of holes can congregate, and the part of the n-type semiconductor adjacent to the insulator will behave as if it were p-type. This is called inversion. Our conclusion so far is that under equilibrium conditions inversion may occur. Whether equilibrium is reached or not depends on the time constants t1 and t2 . How long is t1 ? As far as we know no one has measured it, but it can not take long for electrons to clear out of a 1 µm part of the material. If we take a snail moving with a velocity of 1 m h–1 it will need about 3 ms to cover 1 µm. Thus electrons, which may be reasonably expected to move faster than snails, would need very little time indeed to rearrange themselves and create a depletion region. On the other hand, in sufﬁciently pure materials the thermal generation time constant might be as long as a few seconds. Thus, if all the operations we perform in a metal–insulator–semiconductor junction are short in comparison with the generation time of electron–hole pairs, then the

The tunnel diode

183

minority carriers will not have the time to appear, a mode of operation called the deep depletion mode. Inversion and deep depletion are some further representations of the multifarious phenomena of semiconductor physics. They are certainly interesting, but are they useful? Can a device through which no current ﬂows be of any use at all in electronics? The secret is that current can ﬂow along the insulator surface. The emerging devices are very important indeed. Under acronyms like MOSFETs and CCDs they are the ﬂagbearers of the microelectronics revolution. I shall talk about them a little later.

9.10 The tunnel diode So far, we have considered impurity semiconductors with very low impurity contents, typically less than one part per million. We have characterized the impurity type and density by working out where the Fermi level is, and have found that in all cases it is well within the energy gap. This has meant, among other things, that the sums are much simpler, for we are able to approximate to the Fermi function. However, when the impurity level becomes very high (typically about 1024 m–3 or about 0.01%), the Fermi level moves right up into the conduction band (or down into the valence band for a p-type impurity). The semiconductor is then said to be ‘degenerate’. What are degenerate semiconductors good for? One can make diode lasers out of them, as will be discussed later in Section 12.7. But well before the appearance of diode lasers, Esaki∗ realized that they were suitable for producing a revolutionary new device, to be shown in this section. For a while, they were called Esaki diodes. They are now known as tunnel diodes because their operation is based on tunnelling. Let us now produce a junction out of two degenerate semiconductors, one p-type and one n-type. The energy diagram at thermal equilibrium is given in Fig. 9.24(a), where, for simplicity, we take the difference between the Fermi level and the band edge as the same on both sides. It is interesting to see that the ‘built-in’ potential is larger than the energy gap (eU0 > Eg ); thus the number of electrons crossing over the potential barrier at thermal equilibrium must be small. Hence, I0 in the rectiﬁer equation is small, and the rectifying characteristic is rather elongated, as shown in Fig. 9.25(a). Looking carefully at the diagram you may realize that another mechanism of electron ﬂow may also be effective. Remember, tunnel diodes are highly doped, and high doping means a narrow transition region. Thus, electrons as well as moving over the potential barrier may also tunnel through the potential barrier, and if one puts in the ﬁgures, it turns out that the tunnelling current is the larger of the two. Hence, we may imagine thermal equilibrium as the state in which the tunnelling currents are equal and in opposite directions. What happens now if we apply a reverse bias? As may be seen in Fig. 9.24(b), the number of electrons tunnelling from left to right is increased because the electrons on the p-side face a large number of empty states on the n-side. We could work out this current by considering a rectangular potential barrier (the one we so skilfully solved when ﬁrst confronted with Schrödinger’s equation) and taking account of the occupancy of states on both sides. It is one of those fairly lengthy and tedious calculations that are usually left as an exercise for the student. The actual value is of little consequence because this diode

∗ Leo

Esaki received a Nobel Prize in 1973. This is another example where the invention of a new device earned for the inventor the Nobel Prize in Physics.

184

Principles of semiconductor devices (a)

Eg

(b)

(c)

eUo

Ef

(d)

eU

(e)

(f)

Fig. 9.24 Energy diagrams of the tunnel diode under various applied voltages. (a) Zero bias. (b) Reverse bias. (c) Small forward bias. (d) Forward bias corresponding to maximum current. (e) Forward bias resulting in a decrease in current. (f) Forward bias at which the tunnelling current is reduced to zero.

∗ In

fact, there is some deviation from this characteristic owing to the inevitable presence of some energy levels in the forbidden gap. There is thus some additional tunnelling, which becomes noticeable in the vicinity of the current minimum. But even including this effect the ratio of current maximum to current minimum may be as high as 15 in a practical case.

is not used under reverse bias conditions. For a forward bias [Fig. 9.24(c)] the situation is essentially the same as before, but now the electrons tunnel from right to left. If the applied voltage is increased, the number of states available on the p-side increases, and so the current increases too. Maximum current ﬂows when electrons on the n-side have access to all the empty states on the p-side, that is, when the Fermi level on the n-side coincides with the valence band edge on the p-side [Fig. 9.24(d)]. If the bias is increased further [Fig. 9.24(e)], there will be an increasing number of electrons ﬁnding themselves opposite the forbidden gap. They cannot tunnel because they have no energy levels to tunnel into. Hence, the tunnelling current must decrease, reaching zero when the top of the valence band on the p-side coincides with the bottom of the conduction band on the n-side [Fig. 9.24(f)]. Therefore, the plot of current against voltage must look like that shown in Fig. 9.25(b). But this is not the total current; it is the current due to tunnelling alone. We can get the total current by simply taking the algebraic sum of the currents plotted in Fig. 9.25(a) and (b), which is a permissible procedure, since the two mechanisms are fairly independent of each other. Performing the addition, we get the I – U characteristics [Fig. 9.25(c)] that we would be able to measure on a real tunnel diode.∗ You know now everything about the tunnel diode with the exception of the reason why it can perform some useful function. The answer follows from the I – U characteristics. There is a region where the slope is negative that is usually referred to as a negative resistance. In case you have not heard this curious phrase before we shall brieﬂy explain it.

The tunnel diode

185

I

(a) Rectifying current

U

I

(b) Tunnelling current

U

I

A

Fig. 9.25 (c) Total current

The current in a tunnel diode is the sum of the tunnelling current and of the usual rectifying current.

U

Consider an ordinary tuned circuit as shown in Fig. 9.26. If we start it oscillating in some way, and then leave it, the oscillations will decay exponentially, their amplitude falling with time according to R exp – t . (9.26) 2L Physically, the resistance R absorbs the oscillating energy and gets a little hotter. If we now put a negative resistance in series with R, odd things happen. In the particular case when the negative resistance (–R1 ) is equal in magnitude to R, the total resistance becomes R – R1 = 0,

(9.27)

and the exponential becomes unity. This means that an oscillation, once started in the circuit, will continue with no decay, the negative resistance replenishing all the energy dissipated as heat in the real resistance.

L

C

Fig. 9.26 A tuned circuit.

R

186

Principles of semiconductor devices If we could get energy like this out of a simple circuit isolated from the rest of the world except for the R, L, and C we have drawn, it would contravene the second law of thermodynamics and make perpetual motion fairly straightforward. As this does not happen, we can conclude that a ‘negative resistance’ has to be an active circuit device that is connected to a power supply other than the oscillating signal with which it interacts. This is very true of the tunnel diode, since to act as a negative resistance, it has to be biased with a battery to the point A in Fig. 9.25(c). The power to overcome the circuit losses comes from this battery. If the magnitude of the negative resistance in Fig. 9.25(c) is greater than the loss resistance R, the initiatory signal will not only persist; it will grow. Its magnitude will, of course, be limited by the fact that the tunnel diode can be a negative resistance for only a ﬁnite voltage swing (about 0.2 V). Thus, given a negative resistance circuit engineers can make oscillators and ampliﬁers. The particular advantage of tunnel diodes is that, as the junctions are thin, the carrier transit times are shorter than in a transistor, and high-frequency operation (up to about 1011 Hz) is possible. Their limitation is that with their inherently low voltage operation, they are very low-power devices.

I

9.11

U

Fig. 9.27 The current voltage characteristics of a backward diode.

I

This is essentially the same thing as the tunnel diode, only the doping is a little lighter. It is called a backward diode because everything is the other way round. It has low impedance in the reverse direction and high impedance in the forward direction, as shown in Fig. 9.27. The secret of the device is that the doping is just that much lighter (than that of the tunnel diode) as to line up the band edges (the top of the valence band on the p-side to coincide with the bottom of the conduction band on the n-side) at zero bias. Hence, for a forward bias there is no tunnelling, just the ‘normal’ ﬂow, which is very small. In the reverse direction, however, a large tunnelling current may ﬂow. The backward diode is a very efﬁcient rectiﬁer (of the order of one to a thousand) for low voltages. For higher voltages, of course, the ‘forward’ current may become signiﬁcant.

9.12

U

Fig. 9.28 The current voltage characteristics of a p–n junction showing the sudden increase in current at a speciﬁc value of reverse voltage.

The backward diode

The Zener diode and the avalanche diode

You should not dwell too heavily on the memory of the backward diode; it is rather exceptional. I am pleased to say that from now on forward means forward and reverse means reverse. We shall now consider what happens at higher voltages. In the forward direction the current goes on increasing, and eventually the diode will be destroyed when more energy is put in than can be conducted away. This is a fascinating topic for those engineers whose job is to make high-power rectiﬁers, but it is of limited scientiﬁc interest for the rest of us. There is considerably more interest in the reverse direction. It is an experimental fact that breakdown occurs very sharply at a certain reverse voltage as shown in Fig. 9.28. Since the ‘knee’ of this breakdown curve is much sharper than the current rise in the forward direction, and since the knee voltage can

The Zener diode and the avalanche diode be controlled by the impurity levels, this effect has applications whenever a sudden increase in current is required at a certain voltage. The diode can therefore be used as a voltage stabilizer or a switch. In the latter application it has the further advantage that the breakdown is not only sharp but occurs very fast as well. The breakdown may occur by two distinct mechanisms: Zener breakdown or avalanche breakdown.

9.12.1

Zener breakdown

187

∗ There

were, of course, no p–n junctions at the time. The mechanism was suggested for bulk breakdown to which, incidentally, it does not apply. The explanation turned out to be applicable to breakdown in p–n junctions. (a)

Conduction band

follows.∗

At The mechanism suggested by Zener (1934) may be explained as low reverse bias there is only the ﬂow of minority electrons from the p-side to the n-side. As the reverse bias is increased, at a certain voltage the bands begin to overlap, and tunnelling current may appear. The tunnelling current does appear if the doping is large enough and the junction is narrow enough. But Zener diodes (in contrast to tunnel diodes and backward diodes) are designed in such a way that practically no tunnelling occurs when the bands just overlap; the potential barrier is too wide [Fig. 9.29(a)]. However, as the reverse bias is increased, the width of the barrier decreases [Fig. 9.29(b)] leading—above a certain voltage—to a very rapid rise in current.

9.12.2

Avalanche breakdown

Avalanche diodes differ from Zener diodes by having somewhat smaller impurity density. The depletion layer is then wider, and the Zener breakdown would occur at a considerably higher voltage. However, before the tunnelling current has a chance to become appreciable another mechanism takes over, which—very aptly—is designated by the word avalanche. You know that electrons in a solid are accelerated by the applied electric ﬁeld. They give up the kinetic energy acquired when they collide with lattice atoms. At a sufﬁciently high electric ﬁeld an electron may take up enough energy to ionize a lattice atom, that is to create an electron–hole pair. The newly created electrons and holes may in turn liberate further electron–hole pairs, initiating an avalanche. Note that the two mechanisms are quite different, as may be clearly seen in Fig. 9.30. In both cases the electron moves from the valence band of the p-type material into the conduction band of the n-type material, but for Zener breakdown it moves horizontally, whereas for avalanche breakdown it must move vertically. But although the mechanisms are different, nevertheless, in a practical case it is difﬁcult to distinguish between them. The diode breaks down, and that is the only experimental result we have. One may attempt to draw the distinction on the basis of the temperature dependence of the two breakdown mechanisms but, in general, it is not worth the effort. For a practical application all that matters is the rapid increase in current, whatever its cause. Avalanche diodes may also be used for generating microwaves. The principles of operation (as for most microwave oscillators) are fairly complicated. The essential thing is that both during the avalanche process and the subsequent drift of the created carriers, the current and the electric ﬁeld are not in phase with each other. By judicious choice of the geometry one may get a 180◦

Valence band

p

n

(b)

Valence band

Conduction band

p

n

Fig. 9.29 A heavily doped p–n junction (a) in thermal equilibrium. (b) at reverse bias. The width of the potential barrier decreases as the bias is increased. Avalanche breakdown

A

p

Zener breakdown n

Fig. 9.30 The mechanism of Zener and avalanche breakdown.

188

Principles of semiconductor devices phase difference between voltage and current, at least for a certain frequency range. But this is nothing more than a frequency-dependent negative resistance. Putting the diode in a cavity, the oscillator is ready.

9.13

Varactor diodes

As I have mentioned above, and shown mathematically in eqn (9.21), the capacitance of a reverse-biased p–n junction is voltage dependent. In other words the capacitance is variable, and that is what the name ‘varactor’ seems to stand for. Varactor diodes are p–n junctions designed for variable capacitance operation. Is a variable capacitance good for anything? Yes, it is the basis of the so-called ‘parametric ampliﬁer’. How does a parametric ampliﬁer work? This is really a circuit problem, but I had better explain its operation brieﬂy. Imagine just an ordinary resonant circuit oscillating at a certain frequency. The charge on the capacitor then varies sinusoidally as shown in Fig. 9.31(a). Suppose the plates of the capacitor are pulled apart when Q reaches its maximum and are pushed back to the initial separation when Q is zero. This is shown in Fig. 9.31(b), where d is the distance between the plates. When Q is ﬁnite and the plates are pulled apart, one is doing work against coulombic attraction. Thus, energy is pumped into the resonant circuit at the times t1 , t3 , t5 , etc. When Q is zero, no energy need be expended to push the plates back. The energy of the resonant circuit is therefore monotonically increasing. To see more clearly what happens, let us try to plot the voltage against time. From t0 to t1 it varies sinusoidally. At t1 the separation between the plates is (a) Q t

d (b)

t0

t1

t2

t3

t4

t5

t6

(c) U

t

(d)

Fig. 9.31 Illustration of the basic principles of parametric ampliﬁcation.

Q

t

Field-effect transistors suddenly increased, that is, the capacitance is decreased. The charge on the plates can not change instantaneously; so the reduced capacitance must lead to increased voltage (Q = CU must stay constant). The voltage across the capacitor therefore jumps abruptly at t1 , t3 , t5 , etc., and it is unaffected at t2 , t4 , t6 , etc., as shown in Fig. 9.31(c). We may argue in a similar manner that the charge must also increase. When the plate is pushed back at t2 , the voltage is not affected, but the capacitance goes back to its original value. Hence, when the capacitor is charged again, Q will come to a higher peak value, as shown in Fig. 9.31(d). Note that the important thing is to vary the capacitance in the resonant circuit at twice the resonant frequency. Ampliﬁcation is achieved then at the expense of the energy available to vary the capacitance. It may be shown (both theoretically and experimentally) that the variation of the capacitance need not be abrupt. Any reasonable variation of the capacitance at twice the rate of the signal frequency would do.∗ It is interesting to note that the possibility of parametric ampliﬁcation had been known for over ﬁfty years, but it has become practical only after the advent of the p–n junction. Now with what sort of properties would we like to endow our p–n junction to make it suitable for this particular application? Well, it will be the integral part of some sort of tuned circuit, where losses are generally unwelcome. Hence, we shall use heavy doping to reduce the resistance. We should not dope too much, however, because that would lead to narrow depletion regions and low Zener breakdown. Since the varactor diode must operate under reverse bias (to get the capacitance) its useful range is between U = 0 and U = UB ; a low breakdown voltage is obviously undesirable. In practice the p-side of the junction is usually doped very heavily, so that it does not contribute at all to the total series resistance. All the depletion layer is then in the n-type material, whose length is limited to the possible minimum. It is equal to the length of the depletion region just below breakdown (when the depletion region is the longest). That is roughly how parametric ampliﬁers work. But is it worth making a complicated ampliﬁer which needs a high-frequency pump oscillator when a ‘simple’ transistor will amplify just as well? The limitation of a transistor is that it will be a source of noise as well as gain. All ampliﬁers introduce additional noise† due to the random part of their electronic motion, so the emitter and collector currents in a transistor are fairly copious noise sources. As there is almost no standing current in a varactor, it introduces very little noise; so parametric ampliﬁers are worth their complications in very sensitive receivers, for example for satellite communication links, radio astronomy, and radar.

9.14 Field-effect transistors Having become acquainted with a number of two-terminal devices, let us now look at another representative of a three-terminal device, the so-called ﬁeldeffect transistor (FET). It is not quite clear why it is regarded as a relative of the bipolar transistor, which we have discussed in quite some detail in Section 9.6. The only common factors are that they are both solid state devices

189

∗ The

magic factor 2 in frequency is not necessary either. Furthermore, it is not even a good thing, because if it were, we would have to know the signal frequency at all times, together with its phase. Clearly this would be impossibly difﬁcult for an arbitrary signal. Instead, a three-frequency scheme is used, in which a strong pump at an unrelated but generally much higher frequency ω3 is used to amplify a weak signal at a frequency ω1 . The process involves two steps. In the ﬁrst, the pump and signal are mixed together in the varactor to create a socalled ‘idler’ at a frequency ω2 = ω3 –ω1 . Because of the relative strength of the pump, the idler is much larger than the signal. In the second, the idler is mixed with the pump to create a new (and even larger) term at the signal frequency, which adds in phase with the signal to give the net effect of ampliﬁcation. To make the device practical, resonant circuits are needed at all three frequencies. These circuits keep the components at each frequency separate, except where they must come together for mixing.

There must be a compromise between reducing the resistivity and ensuring a high breakdown voltage.

† Noise due to electric currents was men-

tioned brieﬂy in a previous footnote (Section 1.2). A fuller discussion is beyond our present scope, but if you wish for further reading in this interesting topic see F.N.H. Robinson, Noise and ﬂuctuations in electronic devices and circuits, O.U.P., 1974.

190

Principles of semiconductor devices –

+

Depletion regions Signal input

n-type semiconductor

Gate

~

Drain Source n+ - contact

Fig. 9.32 Gate

Schematic representation of a ﬁeld-effect transistor (FET). The current between source and drain is controlled by the voltage on the gate electrodes.

Signal output RL

p+ - material –

IDS

+

and both make use of electrons and holes. They work, though, on entirely different principles. The basic idea of the FET originated in the 1920s, although any practical realization had to wait until the 1950s. It consists of a piece of semiconductor—let us suppose n-type—to which two ohmic contacts, called the source and the drain, are made (Fig. 9.32). As may be seen, the drain is positive: thus electrons ﬂow from source to drain. There is also a gate electrode consisting of a heavily doped p-type region (denoted by p+ ). Let us assume for the time being that USG , the voltage between source and gate, is zero. What will be the potential at some point in the n-type material? Since there is an ordinary ohmic potential drop due to the ﬂow of current, the potential grows from zero at the earthed source terminal to UDS at the drain. Hence, the p+ n junction is always reverse biased with the reverse bias increasing towards the drain. As a consequence, the depletion region has an asymmetrical shape as shown in Fig. 9.32. The drain current must ﬂow in the channel between the depletion regions. If we make the gate negative, then the reverse bias, and with it the depletion region, increases, forcing the current to ﬂow through a narrower region, that is through a higher resistance. Consequently, the current decreases. Making the gate more and more negative with respect to the source, there will obviously be a voltage at which the depletion regions join and the drain current decreases to practically zero as shown in Fig. 9.33(a). This ID versus UGS characteristic (b)

(a) ID

ID UGS = 0 UGS decreasing

Fig. 9.33 The characteristics of a junction type ﬁeld-effect transistor.

UGS

0

0

UDS

Field-effect transistors is strongly reminiscent of that of anode current against grid voltage in a good triode, the product of a bygone age when the subject of electronics was nice and simple. The physical picture yielding the ID versus UDS characteristics is a little more complicated. As UDS increases at constant gate voltage, there are two effects occurring simultaneously: (i) the drain current increases because UDS has increased, a simple consequence of Ohm’s law; (ii) the drain current decreases because increased drain voltage means increased reverse bias and thus a smaller channel for the current to ﬂow. Now will the current increase or decrease? You might be able to convince yourself that when the channel is wide, and the increase in U DS means only a relatively small decrease in the width of the channel, the second effect is small, and the current increases. However, as the channel becomes narrower the second effect gradually gains importance, and the increase of ID with UDS slows down, as shown in Fig. 9.33(b). At the so-called pinch-off voltage, the two effects cancel each other, and they keep their balance for voltages beyond that. The current stays constant; it has reached saturation. The actual value of the saturation current would naturally depend on the gate voltage. At lower gate voltages the saturation current is smaller. The physical mechanism of current ﬂow in an FET is entirely different from that in a vacuum tube, but the characteristics are similar, and so is the equivalent circuit. A small change in gate voltage, u gs , results in a large change in drain current. Denoting the proportionality factor by gm , called the mutual conductance, a drain current equal to gm ugs appears. Furthermore, one needs to take into account that the drain current varies with drain voltage as well. Denoting the proportionality constant by rd (called the drain resistance), we may now construct the equivalent circuit of Fig. 9.34, where id , ugs , and uds are the small a.c. components of drain current, gate voltage, and drain voltage, respectively. A modern and more practical variant of this device is the metal–oxide– semiconductor transistor or MOST, also known as metal–oxide–semiconductor ﬁeld-effect transistor or MOSFET. It is essentially a metal–insulator– semiconductor junction provided with a source and a drain as shown in Fig. 9.35(a). To be consistent with our discussion in Section 9.9, we shall assume that the substrate is an n-type semiconductor, and the source and drain are made of p+ material. At zero gate bias, no drain current ﬂows because one of the junctions is bound to be reverse biased. What happens as we make the gate negative? Remembering the physical phenomena described in Section 9.9,

(a)

191

Gate

ugs

Drain gmugs

rd uds Source

Fig. 9.34 Equivalent circuit of a ﬁeld-effect transistor.

(b) Source

Gate Metal

Drain SiO2

p+

Gate

Drain

Fig. 9.35 p+

n-Si substrate

Source

p-channel

Schematic representation of a MOSFET. (a) Zero gate bias. (b) Forward bias inducing a p-channel.

192

Principles of semiconductor devices ID

ID UGS decreasing

Fig. 9.36 The characteristics of a MOSFET.

0

UGS

0

UDS

we may claim that at sufﬁciently large negative gate voltage inversion will occur, that is the material in the vicinity of the insulator will turn into a p-type semiconductor. Holes may then ﬂow unimpeded from source to drain. The rest of the story is the same as for an ordinary FET and the characteristics are fairly similar, as shown in Fig. 9.36, though in the present case there is no proper current saturation, only a knee in the ID versus UDS characteristics. The devices in which conduction occurs by inversion are said to operate in the enhancement mode. There is also a depletion mode device in which one starts with a p-channel [Fig. 9.35(b)] and depletes the holes by applying a positive bias to the gate. This is more similar to the traditional FETs. Naturally, both the enhancement and depletion devices described have their counterparts with n+ drains and sources and p-type substrate. In principle there is no difference between them. In practice there is some difference, because the surface potential at the Si - SiO2 interface tends to be positive, thus it is easier to achieve inversion in an n-type material. Having so many different types of FETs has tested the ingenuity of those whose job it is to think up symbols for new devices. The solutions they came up with are shown in Fig. 9.37. Applications for performing logic functions are obvious. Depending on the gate voltage the FET of Fig. 9.35 is either ON (UDS low) or OFF (UDS high). There are naturally many varieties on the basic theme; I want to mention only one of them, known as CMOS (complementary MOS), which rose to fame

Junction

n-Channel

Fig. 9.37 Symbols for FETs.

p-Channel

Enhancement

Depletion

Field-effect transistors

193

+U0 S M1 D

Uin

Uout

D M2 S

owing to its low power consumption. The simplest CMOS circuit is the inverter shown in Fig. 9.38. The upper device M1 is a p-channel MOS, whereas the lower device M2 is of the n-channel variety. The drains and gates are connected, and the source is connected to the substrate in each device. Let us see what happens when the input voltage Uin is approximately zero. For M2, a positive UGS is required to turn it ON. In the absence of a positive UGS , M2 is OFF. What about M1? It needs a negative UGS to turn it ON. But that is exactly what it has. The source is at a high potential U0 (say 5 V) and the gate is at about zero potential hence M1 is ON, the potential drop across the device is small, and Uout is approximately equal to U0 . Thus when Uin is low, U out is high. This is what an inverter is supposed to do. You may easily convince yourself that when Uin is equal to U0 , M1 is OFF and M2 is ON leading to an output voltage of about zero. Why is this inverter better than other inverters? On account of the low currents ﬂowing. But surely when a device is ON, there will be a lot of current ﬂowing. Is not the best analogy a ﬂoodgate? When the gates are closed there is only a trickle, but when they are open, there is a torrent of water. This analogy does indeed apply to many electronic devices (e.g. to the transistor of Fig. 9.15 or to the FET of Fig. 9.35) but not to the CMOS inverter. The current through M1 cannot be large when it is ON because there is nowhere the current can ﬂow. In fact, the current must be equal to that ﬂowing in M2 when it is OFF, and that is equal to the current through a reverse biased p–n junction, say 50 nA. And of course the situation is similar when M1 is OFF and M2 is ON. With U0 equal to 5 V, the power dissipation is a quarter of a microwatt. There is of course a small gate current, as well, but it will still leave power dissipation well below a microwatt∗ , many orders of magnitude smaller than that of competitive semiconductor devices. Thus CMOS devices are natural candidates for all devices that must either involve extremely low power or very many transistors. Into the former category come battery-powered devices and into the latter all complex digital circuits such as microprocessors, embedded controllers, and semiconductor memory elements. Computers in particular have transformed our lives to such an extent that learning some elegant semiconductor device physics seems a small price to pay.

Fig. 9.38 A CMOS inverter.

∗ It

must be admitted that there is some more appreciable power dissipation during switching due to capacitors being charged up, and there is also a brief interval when both devices are ON.

194

Principles of semiconductor devices

9.15

Heterostructures

All the devices mentioned so far have been made using the same material. Some properties of the material were tampered with, for example doping made one part of the material n-type and another part p-type, but the energy gap always remained the same. We may call such structures homostructures in contrast with heterostructures, which consist of materials of different energy gaps. Is it in any way desirable to change the energy gap? The simple answer is, yes, it gives us a new degree of freedom. In order to appreciate the difference between these two types of junctions, let us ﬁrst redo the construction that leads to the built-in voltage in homojunctions and then repeat the exercise for heterojunctions. The energy diagrams of a p-type and an n-type semiconductor are shown in Fig. 9.39(a) next to each other. Their Fermi levels are at EFp and EFn , respectively. Next [Fig. 9.39(b)], we join them and equate the Fermi levels. The built-in voltage is the same whether we look at it from the valence band or from the conduction band. Assume now that the p-type material has a higher gap than the n-type material (Egp > Egn ) but its Fermi level relative to the top of the valence band is unchanged. The n-type material has the same properties as before, as shown in Fig. 9.39(c). Joining them and equating their Fermi levels leads to Fig. 9.39(d). It may now be seen that the built-in voltage is higher in the conduction band than in the valence band. For the holes, there is no difference between the homojunction and the heterojunction: the amount of hole injection is the same in both cases. But the energy gap of the p-type material being wider in Fig. 9.39(c) means that the electrons see a higher barrier against them and, consequently, electron injection is much smaller in the heterojunction than

(a)

(b) Eg EFn

Eg

Eg EFn – EFp

EFp 0

0

EFp 0 EFn – EFp

(c)

Fig. 9.39 (a) Energy diagrams of a p-type and an n-type material next to each other; energy gaps are the same. (b) Energy diagram when the two materials in (a) are joined together. (c) Energy diagrams of a p-type and an n-type material next to each other; energy gaps are different. (d) Energy diagram when the two materials in (c) are joined together.

Egp

EFp 0

(d) Egn EFn

0

Egp EFn – EFp + Egp – Egn Efp 0 EFn – EFp

Heterostructures

195

in the homojunction. Is this good? If we imagine that this is the emitter–base junction of a p–n–p transistor then this is certainly something desirable. The hole current from emitter to base is the current upon which the operation of the transistor is based. We need that. The electron current from base to emitter, however, does no good. We are better off without it. The conclusion is that by using a heterojunction we can produce a transistor with properties superior to that of a homojunction. The transistor thus obtained has even got a name. It is known as HBT or Heterostructure Bipolar Transistor. The essential thing is that when we turn to heterojunctions, the fates of electrons and holes are no longer tied together. Perhaps an even better illustration of their independence is provided by Fig. 9.40. Figure 9.40(a) shows the energy diagram of a homogeneous bulk semiconductor doped so that the acceptor concentration increases from left to right. Clearly, the electrons will slide down the slope, and the holes have no other option but to slide up the slope. The ﬂow of electrons and holes is in the opposite direction. Take now a piece of undoped semiconductor crystal, grown so that the energy gap gradually shrinks from left to right [Fig. 9.40(b)]. The slopes of the potential energy diagram are now such that electrons and holes move in the same direction. So, there is no doubt, heterojunctions offer more freedom in designing devices. Are the advantages of heterojunctions limited to bipolar devices? One might say, yes, remembering that the separate control of electrons and holes is of no beneﬁt to FETs. In fact, FETs also draw advantages from the availability of heterostructures but in a quite different form. What is it that we are aiming at? We want to have high mobility. But surely that depends on the choice of the material, on the temperature, and on the impurities. Once they are chosen, we no longer have any freedom. Surprisingly, it turns out that we still have some freedom. We can have our cake and eat it. More precisely, we can produce our carriers from impurities without the disadvantage of impurity scattering and the corresponding reduction in mobility. The FET which can incorporate these features is called appropriately the High Electron Mobility Transistor or HEMT (some people call it MODFET an acronym for Modulation-Doped Field Effect Transistor or TEGFET standing for Two-dimensional Electron Gas Field Effect Transistor). What kind of properties should materials A and B, the two semiconductors to be joined in holy matrimony, possess? One should provide the electrons, so it should be doped, and the other one should provide an impurity-free environment, so it should not be doped. The problem is then to persuade the electrons that, once created in the doped material, they should move over into

(a)

(b)

Fig. 9.40 EF

The energy diagram of semiconductor crystals. (a) Variable doping, constant energy gap. (b) Undoped, variable energy gap.

196

Principles of semiconductor devices (a)

A

B

(b)

EF

ΔEc

EFA

EFB

ΔEv (d)

(c) cA

Δ Ec

cB

EF

cA

Fig. 9.41 Energy diagram for a heterojunction. (a) Energy levels before joining the semiconductors. (b) The Fermi levels agree. (c) Energy levels after joining the semiconductors. (d) Details of the conduction band edge in the vicinity of the metallurgical junction.

Note that there are now band offsets, both at the conduction and valence bands, denoted by Ec and Ev , respectively.

EF ΔEv

vB vA Metallurgical junction

cB

Discrete electron energy

the undoped material. This can be achieved by a junction between a doped high-bandgap material (A) and an undoped lower-bandgap material (B). The energy diagrams of the two materials before they are joined are shown in Fig. 9.41(a). The Fermi energy of material A is quite close to the conduction band. The Fermi energy of material B may be seen to be somewhat above the middle of the gap on account of the electron effective mass being smaller than the hole effective mass [see eqn (8.24)]. Next, we need to match the Fermi energies. That can be easily done as shown in Fig. 9.41(b), where we have now dispensed with the vacuum levels. However, the step that follows now is far from being trivial. It is not simply a question of joining together the two band edges. We have to do the construction separately, left and right of the metallurgical junction. First, let us ﬁgure out how the bands bend on the left-hand side. At the moment the two materials are joined, the conduction band of material A is at a higher energy than that of B. We may therefore expect electrons to move initially from A to B. Hence, there is a depletion region in material A and, consequently, the band edges curve upwards reaching the metallurgical junction at points c A and vA as shown in Fig. 9.41(c). At this point the bandgap will suddenly change. So we need to move down from cA by an amount Ec , and move up from vA by an amount Ev to reach the points cB and vB , respectively. Now we can do the construction on the right-hand side. We join cB to the conduction band edge and vB to the valence band edge of material B.

Heterostructures The energy diagram of Fig. 9.41(c) looks quite different from anything we have seen so far. Not surprisingly, this junction has quite striking properties as may be seen in Fig. 9.41(d), where the central part of the diagram is magniﬁed. The remarkable thing is that c B , the deepest point in the potential well, is below the Fermi energy. Thus according to the rules of the game, the electron density there is much higher than in any other parts of the two materials. The second striking property is that the well is very narrow. How narrow? For the materials usually used, the width of the well comes out of the calculations (they are pretty complicated, one needs to solve simultaneously Poisson’s equation in combination with Schrödinger’s equation) as about 8 nm, comparable with atomic dimensions. So the electron is conﬁned in one dimension. We have, in fact, a two-dimensional electron gas, which has discrete energy levels.∗ In the present example we are showing just one such level. Let us return now to our original aim. We wanted to produce a ﬁeld-effect transistor which works faster than those using homojunctions on account of the higher mobility. So what kind of materials are we going to use? For the undoped material we shall choose one which has a high mobility. GaAs with a bandgap of 1.43 eV and a mobility of 0.85 m2 V–1 s–1 at room temperature (up to about 7.5 m2 V–1 s–1 at 77 K) is clearly suitable for the purpose. The doped material should have a considerably higher bandgap and must be suitable for growing on GaAs. All these requirements are satisﬁed by Alx Ga1–x As.† With x = 0.3, the bandgap is 1.85 eV, Ec is 0.28 eV, and Ev is 0.15 eV. The dopant is silicon. A schematic drawing of the device may be seen in Fig. 9.42. There are very few electrons in the AlGaAs, and the few that there are may be eliminated from beneath the gate by operating the metal–semiconductor junction in this region as a Schottky barrier. This region is therefore analogous to the gate oxide in a conventional FET. As a result, the current between the source and the drain ﬂows along the channel, where the electrons congregate in the undoped GaAs. But can we control the current by changing the gate voltage? Yes, we can, by applying a reverse bias, which will lift the whole energy diagram. Not uniformly of course, there will be greater lift where there are fewer carriers, but the essential thing is that with a reasonable voltage (say, 0.5 V), the bottom of the potential well could be lifted above the Fermi energy, which would reduce the current to very close to zero. So this device could work as a fast switch or as an ampliﬁer in analogue circuits. Because of the high speed of the electrons, these ampliﬁers may work up to the mm wavelength region. So much for n-channel devices. Can we have p-channel devices as well? We can. There is no difﬁculty in doping AlGaAs so as to produce a p-type material. But there is a snag. AlGaAs, like most semiconductors, has both heavy and light holes in the valence band. Since the speed of the device will be determined by the sluggishness of the heavy holes, there seems to be no point in producing p-channel HEMTs. This is indeed true for most purposes, but let us remember that complementary logic needs both n-type and p-type devices. So what can be done? By applying a pressure, we can shift the band edge in the energy diagram. In particular, we can effectively suppress the heavy holes in favour of light holes. In fact, there is no need actually to apply a pressure, as it may appear due to the inherent properties of the junction. This is what actually happens when InGaAs

197

∗ The

discrete character of the energy levels does not much affect the argument here. They are, however, of great importance for the Resonant Tunnelling Diode to be discussed in Section 9.27 and for the latest versions of semiconductor lasers which will come up in Section 12.7.

† Remember

our discussion in Section 8.6: Al is higher than both Ga and As in the periodic table, hence adding Al to GaAs leads to a material of higher energy gap.

source

gate

drain

doped Al GaAs channel undoped GaAs

Fig. 9.42 A schematic drawing of a HEMT.

198

Principles of semiconductor devices is grown on GaAs. Since the two materials have different lattice constants, a strain will appear in the InGaAs layer, which will suppress the hole states at the top of the valence band. By good luck the bandgap of InGaAs happens to be smaller than that of GaAs. Hence a fast p-channel HEMT may be constructed by doping an epitaxially grown GaAs layer with acceptors and then growing a layer of undoped InGaAs on top. The p-channel will be made up of lighter holes just inside the InGaAs layer. What can we say about the future? As the new methods of production (MBE and MOCVD) will be more widely used, heterojunctions will hardly cost more than homojunctions. The point is that for economic reasons one wishes to avoid multiple growth (remove the wafer, do some intermediate processing, and then resume the growth) but it does not matter how complicated an individual run is. So heterojunctions are here to stay.

9.16

U1 1

U2 2

(a)

U3 3

SiO2

Surface potential

n- type Si (b) Distance

t = t1 (c) t = t2 (d) t = t3

(e) t = t4

(f) t = t5

Fig. 9.43 A section of a CCD illustrating the basic principles of a charge transfer.

Charge-coupled devices

Charge-coupled devices, abbreviated as CCDs, look very similar to MOSFETs, and in today’s world looking similar is half the battle. Since companies are rather reluctant to invest in new types of manufacturing processes, a new device that can be made by a known process and is compatible with existing devices is an attractive proposition. CCDs were invented in 1969 at AT & T Bell Laboratories, by Willard Boyle and George E. Smith (Nobel Prize, 2009). At the time, they were working on something entirely different, semiconductor bubble memories. However, an analogy between bubbles of charge and magnetic bubbles somehow suggested itself, and their ﬁrst paper crucially listed imaging devices as a possible application, as well as memory. In the end the CCD succeeded beyond all expectations (while the bubble memory is largely conﬁned to history). A charge-coupled device is essentially a metal–insulator–semiconductor junction working in the deep depletion mode. As mentioned in Section 9.9, the carriers are not in thermal equilibrium. There is a potential well for holes as was shown in Fig. 9.23(d), but owing to the long generation–recombination time in a pure material, it is not occupied by holes. The secret of the device is, ﬁrst that the holes are introduced externally and, second, that the charge can be transferred along the insulator surface by applying judiciously chosen voltages to a set of strategically placed electrodes. Let us look ﬁrst at three electrodes only, as shown in Fig. 9.43(a). There is again an n-type semiconductor upon which an oxide layer is grown, and the metal electrodes are on the top, insulated from each other. We can look at each electrode as part of a metal–insulator–semiconductor junction which can be independently biased. In Fig. 9.43(b) there are some holes under electrode 1. They had to get there somehow, for example they could have got there by injection from a forward biased p–n junction. The essential thing is that they got there, and the question is how that positive charge can be transferred from one electrode to the next. At t = t1 (see Fig. 9.44) the three electrodes are biased to voltages –A, 0, 0 respectively. The corresponding surface potential distribution is shown in Fig. 9.43(b). The holes sit in the potential well. At t = t2 we apply a voltage –A to electrode 2, leading to the surface potential distribution of Fig. 9.43(c). The holes are still sitting under electrode 1 but suddenly the potential well has

Charge-coupled devices

199

U1

–A U2

–A U3

Fig. 9.44

–A

t1 t2 t3

t4 t5

t6

The voltages applied to the three electrodes of Fig. 9.43 as a function of time.

become twice as large. Since the holes wish to ﬁll uniformly the space available, some of them will diffuse to electrode 2. At the same time, just to give the holes a gentle nudge, U1 is slowly returning to zero, so that by t3 the potential well is entirely under electrode 2. Thus the transfer of charge from electrode 1 to electrode 2 has been completed [Fig. 9.43(d)]. Let me reiterate the aim. It is to transfer various sizes of charge packet along the insulator. Thus, when we have managed to transfer the charge from electrode 1 to electrode 2, the space under electrode 1 is again available for receiving a new charge packet. How could we create favourable conditions for a new charge packet to reside under electrode 1? We should lower U1 . But if we lower U1 to –A, what will prevent the charge under electrode 2 from rolling back? Nothing. Thus, we cannot as yet introduce a new charge packet. First we should move our original packet of holes further away from electrode 1. Therefore, our next move, at t = t4 , is to apply –A to U3 and increase U2 to zero between t4 and t5 . The surface potential distributions at t4 and t5 are shown in Figs 9.43(e) and (f) respectively. The period ends at t6 . We can now safely lower U1 and receive a new packet of charge under electrode 1. In practice, of course, there is an array of electrodes with each third one joined together as shown in Fig. 9.45. When U1 is lowered at t6 , our original charge packet will start moving to the next electrode, simultaneously with the

U1

U2 U3

Fig. 9.45 The array of electrodes in a CCD.

200

Principles of semiconductor devices

It may be worth mentioning here that CCDs can also be used as detectors for high energy particles, which might simultaneously knock out thousands of electron-hole pairs. (1) (2) (3) p

Ic

n

p

n

Injecting contact

+

new charge packet entering the ﬁrst electrode. With 3000 electrodes in a line, we can have 1000 charge packets stored in the device. How many elements can be in series? It depends on the amount of charge lost at each transfer. And that is actually the limiting factor in speed as well. If we try to transfer the charge too quickly, some of it will get stuck and the information will be gradually corrupted. The troublemakers are the surface states again. They trap and release charge carriers randomly, thereby interfering with the stored information. Thus, the best thing is to keep the charge away from the surface. This can be done by inserting an additional p-channel into the junction in much the same way as in Fig. 9.35(b). The potential minimum is then in the p-channel, which under reverse bias conditions is entirely depleted of its ‘own’ carriers and is ready to accept charge packets from the outside. These are called buried-channel devices. What about other limitations? Well, there is a maximum amount of charge storable above which the potential minimum disappears. There is a minimum frequency, with which the charge can be transferred, below which the information is corrupted by the thermally generated carriers. There is also a minimum size for each cell determined by tunnelling effects (if the cells are too close to each other) and dielectric breakdown (if the insulator is too thin). What can CCDs be used for? The most important application is for optical imaging for which we do of course need a two-dimensional array. If a picture is focused upon the surface of the device (which in this case has transparent electrodes) the incident light creates electron–hole pairs proportional to its intensity. The process now has two steps: the ‘integrate’ period, during which U1 is set to a negative voltage and the holes (in practical devices electron packets are used and everything is the other way round but the principles are the same) are collected in the potential minima, and the ‘readout’ period, during which the information, is read out. Light may still be incident upon the device during readout, but if the readout period is much shorter than the integration period, the resulting distortions of the video signal are negligible. How many elements can we have? CCD sizes have grown rapidly. Arrays containing 16 MP (i.e. 4000 pixels x 4000 pixels) are common nowadays, and there is no reason to suppose there will not be further increases. The development of the CCD and its incorporation into low-cost personal cameras has transformed our view of photography. Once an expensive luxury that required a professional armed with expensive equipment, the classical portrait photograph is a thing of the past. Anyone can take a high quality photograph or video, and more importantly replicate it, enhance it electronically, incorporate it into documents and presentations, and share it with others. These developments have sounded the death-knell for the ﬁlm industry, and the camera industry itself is under attack as mobile phones increasingly combine the simple operation of acquiring the image with the more sophisticated function of communicating it. Surprisingly, photographers have survived, since there is still one day—the wedding day—where only the professional will do.

–

9.17 Fig. 9.46 The silicon controlled rectiﬁer (SCR).

Silicon controlled rectiﬁer

The silicon controlled rectiﬁer (SCR) is a semiconductor device containing four layers of alternating p- and n-type material as shown in Fig. 9.46. It was

The Gunn effect

201

I

Common curve after breakdown of junction (2)

Ic > 0

Ic = 0

Fig. 9.47

Ug (Ic > 0)

Ug (0)

U

ﬁrst proposed by William Shockley in 1950 and developed at GE by a team led by Gordon Hall. Since it replaced an earlier gas-ﬁlled tube device known as a thyratron, where a small control voltage could switch a large current, it is alternatively known as a thyristor (from a combination of thyratron and transistor). Apart from the ohmic contacts at the end, there are three junctions. Suppose that junctions (1) and (3) are forward biased by the external supply, so that (2) must be reverse biased. As the supply voltage increases, the current will be limited by junction (2) to a low value, until it gets to the reverse avalanche breakdown point. Then its resistance falls very rapidly, and the current through the whole device ‘switches’ to follow a curve approximating to the forward bias junction characteristic, starting at this breakdown point, Us (Fig. 9.47). So far we have described a self-switching arrangement: at a certain applied voltage the device resistance might fall from several megohms to a few ohms. The switch is made even more useful by the additional contact shown in Fig. 9.46, which injects holes into the n-region between junctions (1) and (2) by means of an external positive control bias. By injecting extra minority carriers into the junction (2) region the current Ic controls the value of Vs at which the device switches to the on position. For many years, thyristors have been used in variable power supplies (for example, in lighting dimmers). Large units can switch megawatts of power, and are used in high-voltage AC–DC power conversion.

9.18 The Gunn effect In this and the next two sections I am going to discuss devices that for a change, do not depend on a p–n junction but rather on the bulk properties of semiconductors. We have shown how desirable it is to have negative resistance and how it can be achieved with a tunnel junction. But an inherent snag with any p–n junction is that it must behave as if there were a capacitor in parallel with the device—we worked out its value in Section 9.5. So at high frequencies this capacitor lowers the impedance and causes a falling-off of efﬁciency. Can we get round this problem by having a negative resistance characteristic, like

The current voltage characteristics of a SCR. The switching voltage Us may be controlled by the injected current Ic .

202

I

Principles of semiconductor devices

Light electrons A Transition

O

UA

Heavy electrons B

U

Fig. 9.48 Linear current voltage characteristics for GaAs assuming that only light electrons (OA) or only heavy electrons (OB) are present! The actual characteristics follow the OA line for low voltages and the OB line for high voltages. The transition is shown with dotted lines.

that of a tunnel diode, in a bulk semiconductor? This is a long-established El Dorado of semiconductor device engineers. Nearly all semiconductors should behave like this. Look again at an E–k curve that we drew earlier [Fig. 7.12(a)]. If this represents the conduction band, the electrons will be clustered about the lowest energy state: E = 0, k = 0. Now apply a ﬁeld in the x-direction which accelerates the electrons, so their momentum (which, as we have mentioned before, is proportional to k) will increase as well. This means that our electrons are climbing up the E–k curve. At a certain point the effective mass changes sign as shown in Fig. 7.12(c). Now the effective mass is just a concept we introduce to say how electrons are accelerated by a ﬁeld; so this change of sign means that the electrons go the other way. Current opposing voltage is a negative resistance situation. It seems that there should be a good chance of any semiconductor behaving like this, but in fact so far this effect has not been discovered. The reason must be that the electrons move for only a short time without collisions. So to get within this time into the negative mass region, very high ﬁelds are necessary, which causes some other trouble, for example breakdown or thermal disintegration. As a matter of fact, we do not really need to send our electron into the negative mass region to have a negative differential resistance. If the effective mass of the electron increases fast enough as a function of the electric ﬁeld, then the reduced mobility (and conductivity) may lead to a reduction of current— and that is a negative differential resistance, so there seems no reason why our device could not work in the region where m∗ tends rapidly towards inﬁnity. It is a possibility, but experiments have so far stubbornly refused to display the effect. An improvement on the latter idea was put forward by Watkins, Ridley, and Hilsum, who suggested that electrons excited into a subsidiary valley of GaAs (see Fig. 8.10) might do the trick. The curvature at the bottom of this valley is smaller; so the electrons acquire the higher effective mass that is our professed aim. In addition there is a higher density of states (it is proportional to m∗3/2 ); and furthermore, it looks quite plausible that, once an electron is excited into this valley, it would stay there for a reasonable time. The predicted negative differential resistance was indeed found experimentally a few years later by J.B. Gunn, who gave his name to the device. At low ﬁelds most of the conduction-band electrons are in the lower valley. When an electric ﬁeld is applied, the current starts to increase linearly along the line OA in Fig. 9.48. If all electrons had the higher effective mass of the upper valley, then the corresponding Ohm’s law curve would be OB. As the ﬁeld increases, some electrons (as we mentioned before) gain enough energy (0.36 eV) to get into the higher valley, and eventually most of them end up there. So the actual I–U curve will change from something like OA at low ﬁelds to something like OB at high ﬁelds. This transition from one to the other can (and in GaAs does) give a negative differential resistance. Having got the negative resistance, all we should have to do is to plug it into a resonant circuit (usually a cavity resonator at high frequencies) and it will oscillate. Unfortunately it is not as simple as that. A bulk negative resistance in a semiconductor is unstable, and is unstable in the sense that a slight perturbation of the existing conditions will grow.

The Gunn effect

203

U UA

(ii)

(i)

0

d

(ii)

(i) A

Fig. 9.49 0

d

The high-ﬁeld domain fully formed.

Let us apply a voltage UA in the negative-resistance region (Fig. 9.48). The expected electric ﬁeld EA = U A /d (d is the length of the sample), and the expected potential variation, U = EA x, are shown in Fig. 9.49 by curves (i). It turns out that the expectations are wrong because a negative resistance in a bulk material nearly always leads to an instability. In the present case it may be shown that the instability appears in the form of the heavy electrons accumulating in a high-ﬁeld domain, which travels from the cathode to the anode. The potential and ﬁeld distributions at a particular moment in time, when the high-ﬁeld domain is in transit, are shown in Fig. 9.49 by curve (ii). So why is this device an oscillator? Because it provides a periodically varying current. How? When the voltage UA is switched on at t0 , the current is IA , as shown in Fig. 9.50. Between t0 and t1 the high-ﬁeld domain is formed at the cathode. This is equivalent to the insertion of a high resistance material, hence the current must suddenly decline. It remains constant while the high-ﬁeld domain moves along the material. At t = t2 (where t2 – t1 = d/vdomain , and the velocity of the domain is roughly the same as the drift velocity of the carriers) the domain reaches the anode. The high resistance region disappears, and the current climbs back to IA . By the time, t3 , the domain is newly formed at the cathode, and everything repeats itself. We have obtained a periodic current waveform rich in harmonics with a fundamental frequency, ~ vdomain /d. f = 1/(t3 – t1 ) =

(9.28)

204

Principles of semiconductor devices I IA

Fig. 9.50 The current as a function of time in GaAs when high-ﬁeld domains move across the material.

Note that the transit time mode is not the only mode of operation for this GaAs oscillator. By preventing the formation of domains the bulk negative resistance can be directly utilized. Gold wire

n+

n-type active layer

t0t1

Fig. 9.51 Sketch of a typical Gunn diode.

K is a geometrical constant, L is the length, A the cross-sectional area, and ρ the resistivity of the semiconductor.

t

Thus, the Gunn diode has an oscillation frequency governed by the domain transit time. The velocity of the domain is more or less determined by the voltage producing the effect; so in practice the frequency is selected by the length of the device. A typical Gunn diode is made by growing an epitaxial layer of n-type GaAs, with an electron concentration of 1021 –1022 m–3 on to an n+ -substrate (concentration about 1024 m–3 ). The current ﬂow in the device (Fig. 9.51) is through the thickness of the epitaxial layer. For good quality GaAs the domain velocity is about 105 m s–1 ; a 10 µm layer will therefore make an oscillator in the 1010 Hz frequency band (the so-called X-band of radar).

9.19 Heat sink

t2t3

Strain gauges

We have noticed before (in the case of thermal expansion) that a change in lattice dimension causes a change in the energy gap as well as in the value of k at the band edge. These changes will also occur if the expansion or contraction is caused by applied stresses. The changes are slight and with intrinsic semiconductors would cause only a small change in resistance. If, however, we have a p-type semiconductor with impurities only partially ionized, a very small change in the energy bands can cause a large percentage change in the energy difference between the impurity levels and the band edge. Thus, the change in resistance of the material with stress (or strain) is large (Fig. 9.52). Semiconductor strain gauges are pieces of semiconductor with two ohmic contacts that are of a suitable shape to glue on to the component under test. In general, the resistance R can be written R = K(ρL/A).

(9.29)

dR dL dA dρ = – + , R L A ρ

(9.30)

Thus,

Impurity level

Shift due to lattice strain

Fig. 9.52 The shift of the energy diagram with strain; this makes semiconductors suitable materials for strain gauges.

Valence band

Shift due to lattice strain

Gas sensors which can be rearranged as

205 p is Poisson’s ratio.

Fractional resistance change dR/R dρ/ρ = = 1 + 2p + . Strain dL/L dL/L

(9.31)

The last term on the right-hand side is called the gauge factor, G=

dρ/ρ . dL/L

(9.32)

For p-type silicon this factor can be between 100 and 200. Of course, for a metal G ∼ 0 and, since the other two terms on the right-hand side of eqn (9.31) are of the order of unity, the gauge factor gives a measure of the increased sensitivity of strain gauges since semiconductor strain gauges became generally available. Piezoresistive strain gauges convert mechanical strain into a change in resistance. If a piezoresistor is incorporated into one arm of a Wheatstone bridge, this change may in turn be converted into a voltage. Piezoresistors therefore provide a simple method of readout in a variety of silicon-based physical sensors in which the measurand is arranged to generate a mechanical strain in a ﬂexible element such as a beam or a diaphragm. Examples include strain sensors, pressure sensors, and accelerometers fabricated by using microelectromechanical systems technology (see Section 9.26).

9.20 Measurement of magnetic ﬁeld by the Hall effect We can rewrite the Hall-effect equation (1.20) in terms of the mobility and of El , the applied longitudinal electric ﬁeld, as EH = BEl μ.

(9.33)

Hence, B may be obtained by measuring the transverse electric ﬁeld, the sensitivity of the measurement being proportional to mobility. One semiconductor is quite outstanding in this respect, n-type indium antimonide. It has an electron mobility of about 8 m2 V–1 s–1 , an order of magnitude greater than GaAs and about ﬁfty times greater than Si. In general, this is a simpler and more sensitive method of measuring a magnetic ﬁeld than a magnetic coil ﬂuxmeter, and the method is particularly useful for examining the variation of magnetic ﬁeld over short distances, because the semiconductor probe can be made exceedingly small. The disadvantages are that the measurement is not absolute, and that it is sensitive to changes in temperature.

9.21 Gas sensors A quite sophisticated effect is that traces of particular oxidizing, reducing, or other reactive gases will modify device performance, for example by changing the conductivity of a semiconductor, such as doped tin oxide. This is a very versatile ‘Varistor’, which can be doped to sense various gases. For example, in its n-type form it has a lattice deﬁcient in O. Oxygen is chemisorbed and removes conduction band electrons by trapping them on the surface. A reducing

206

Principles of semiconductor devices gas has the opposite effect. These changes can be detected by measuring the conductivity of a thin ﬁlm. For high sensitivity, an extremely large surface area is required and as a result the ﬁlms are generally highly porous or nanostructured. Gas sensors have therefore been major beneﬁciaries of new materials developments in nanotechnology. One problem is to make the response speciﬁc to a single gas species, rather than to many, and to avoid confusing a change in temperature with the presence of the gas. The solution is generally to use several sensors, each having different responses to temperature and to various common gases, and to derive the concentrations of the different species by processing the signals from all the sensors together. Important applications include the detection of combustible and toxic gases, and oxygen depletion. Forms of the varistor can be targetted on the gases associated with explosives or drugs. Hence, these ‘electronic noses’ are replacing the ‘sniffer dogs’ often featured in news items. It is a pity that dogs as well as people are being made redundant by semiconductors, but at least there is now less chance that a cat crossing the road will cause a dog to misbehave and misdiagnose.

9.22

Invented by Jack Kilby in 1959, working at Texas Instruments. He received the Nobel Prize in 2000.

Microelectronic circuits

We shall conclude the discussion of semiconductor devices by saying a few words about the latest techniques for producing them. Since the techniques are suitable for producing very small electronic circuits, they are called microelectronic circuits; and because these circuits can be interconnected, they are often referred to as integrated circuits. The material most often used is silicon; the small piece of material upon which one unit of the manufactured device is presented is known as a chip. Once the exclusive preserve of a few engineers, today even sociologists and politicians know about the silicon chip. They learned to love it or hate it; indifference is no longer possible. The crucial property of silicon that made this technology possible is its ability to acquire a tenacious ‘masking’ layer of silicon dioxide. SiO2 is familiar in an impure state as sand on the beach; it has a ceramic form used for furnace tubes and a crystalline form (quartz) that has good acoustic and optical properties. It is very hard, chemically resistant, an insulator, and has a high melting point (≈1700◦ C). An oxide layer can simply be grown, by heating the silicon to 1200 ◦ C in an oxygen atmosphere. The growth rate is very slow, about 1 µm per hour, and the thickness can thus easily be controlled. To reduce the process temperature (which generally leads to a reduction in the defect density and an increase in device lifetime), oxide layers may alternatively be deposited in a process known as plasma enhanced chemical vapour deposition (PECVD). The sources are gases (silane or dichlorosilane and oxygen), and much thicker layers can be deposited at temperatures of around 350 ◦ C. What else needs to be done besides growing an oxide layer? Quite a lot, there are a number of other operations to be performed. Instead of discussing them separately, we shall give here a brief description of the production of a single n–p–n transistor, and shall introduce the various techniques as we go along. We shall start with a p-type substrate which has an n-type epitaxial layer of about 4–8 µm on the top as shown in Fig. 9.53(a). Next, we grow an oxide layer, then cover it by a thin ﬁlm of a material called a photoresist, place a

Microelectronic circuits mask on top, and illuminate it by ultraviolet light [Fig. 9.53(b)]. The mask has opaque and transparent areas, so it can deﬁne the region of photoresist upon which the ultraviolet light can fall. It is usually a pattern of chrome on glass or quartz, drawn using an electron beam writing system at a size that may be signiﬁcantly larger than the one ﬁnally required. The pattern is reduced using a rather sophisticated ‘enlarger’ operating backwards. The dies are printed in a step-and-repeat mode, so the patterning system is known as a ‘stepper’. Originally, mercury arc lamps (with a deep-UV wavelength of 365 nm at the ‘I’ line) were used as light sources. ArF lasers are now common; since their emission wavelength (193 nm) lies in the vacuum ultraviolet, evacuated light paths are required. Immersion lenses (which have higher numerical aperture and hence can form a smaller focused spot) are used to reduce the feature size still further. Some of these techniques are discussed in more detail in Section 9.24. As a result, equipment for lithography is now extremely expensive. Other techniques are used to make sure the reduced feature size is maintained on the device itself. Plasma etching is used in place of wet chemical etching to ensure that features do not broaden when the pattern is transferred into the layer beneath. Ion implantation and annealing are used in place of diffusion, to reduce the spread of buried features. Self-alignment is used to eliminate the spaces that must normally be allowed between features on different mask layers. Linewidths (0.5 µm in 1990) are now staggeringly small; 22 nm linewidth reached production in 2012 and 14 nm is predicted for 2014 by the International Technology Roadmap for Semiconductors. Photoresists are organic compounds whose solubility is affected by exposure to ultraviolet light. We are using here a positive photoresist in which the exposed areas can be washed away by a suitable developer.∗ After this operation, we are left with two windows in the photoresist, as shown in Fig. 9.53(c). The one chemical that readily attacks SiO2 is hydroﬂuoric acid (HF), but it does not dissolve the photoresist. Hence, the windows in the resist can be turned into windows in the SiO2 by etching with HF [Fig. 9.53(d)] and the remaining photoresist may then be removed [Fig. 9.53(e)]. The purpose of all these operations, starting with oxidation, was to get access to the epitaxial layer at selected places. The next operation that makes use of these windows is diffusion. The silicon is sealed into a clean furnace tube, containing a volatile form of the required doping material. It is then heated for a prescribed time, and the impurity diffuses into the surface. This is a solid state diffusion process, and the important thing is that it is completely inhibited in the oxide covered regions. For the p-type doping we want here we could use boron bromide (BBr3 ) heated to about 1100 ◦ C. The emerging p+ region is shown in Fig. 9.53(f). The oxide layer has now done its duty, so it may be removed, and we are ready to perform the next operation, which is to provide a window for base diffusion. The steps are again oxidation, photoresist coating, masking, illumination by ultraviolet light, removal of the exposed photoresist, and removal of the oxide layer underneath. Then comes the p-type diffusion with which the stage shown in Fig. 9.53(g) is reached. A further repetition of the technique leads to a window for a diffusion of phosphorus, which forms the n+ emitter region [Fig. 9.53(h)]. The n+ –p–n transistor is now ready, though it still needs to be connected to other elements on

207

∗ For

a negative photoresist, as may be expected, the unexposed areas are soluble.

Note that there is lateral diffusion as well, so the p+ region extends somewhat under the oxide layer. The aim of this diffusion is to isolate the present transistor from others made on the same chip.

208

Principles of semiconductor devices (a)

Epitaxially grown n-type p-Type substrate Ultraviolet light

(b)

Mask Photoresist SiO2 Epitaxial layer

n p

Photoresist SiO2 Epitaxial layer

(c) n p

Photoresist SiO2 Epitaxial layer

(d) n p

SiO2

(e)

n

Epitaxial layer

p

(f)

SiO2 n

n

p+

p+

n

Epitaxial layer

p-Type substrate

p (g)

n

p+

p+

n

n p+

n

n p

n+

(h) n

p+ p

p

E (i)

Fig. 9.53 Stages in the production of microelectronic circuits.

n

B

p+ n+

C n p+

p

p

metal n

Microelectronic circuits

209

the same chip; so we need some electrodes. This may be done by forming three more windows and evaporating a metal, usually aluminium, for the emitter, base, and collector contacts. The ﬁnished transistor is shown in Fig. 9.53(i). In practice, the above structure is rarely used because of two major disadvantages, ﬁrst the parasitic p–n–p transistor (formed by the base, collector, and substrate regions) may draw away current to the substrate, and second there is a long path of high resistance from the emitter to the collector. The remedy is to diffuse an n+ buried layer into the p-type substrate prior to the epitaxial growth of the n-layer. Thus, the starting point is as shown in Fig. 9.54(a) instead of that in Fig. 9.53(a). There is also an additional n+ diffusion, following the emitter diffusion, leading to the ﬁnal product shown in Fig. 9.54(b). Note that there is a more modern technique of doping called ion implantation. As the name implies, this involves the implantation (in fact, shooting them in with high energy) of ions to wherever the impurities are needed. Now we know how to make one transistor. The beauty of the technique is that it can make simultaneously millions or billions of transistors. The information where the circuits reside is contained in the corresponding photographic mask. So how many transistors of the type shown in Fig. 9.54(b) can be produced on a chip that is, say, of the size of 1 cm2 ? Let us do a very, very simple calculation which will give us a very rough answer. To make the calculation even simpler let us consider the less elaborate structure of an inversion type MOSFET shown in Fig. 9.55. The crucial quantity that will determine the density of the components is a, the so-called minimum feature size. This would correspond to the minimum distance in Fig. 9.55, which is about half the length of the p+ region or the distance between the metal electrodes. The length of the MOSFET is then about 9a. Taking the width of the device as 4a and the distance between two devices as a, the area required for one MOSFET is 50a2 . Five years ago, this minimum feature size was 120 nm. It has been reduced in subsequent stages to 95 nm, to 65 nm, and then down to the present value (writing in August 2013) of 32 nm. Accepting the above estimate for the size of a transistor, that means that the number of elements on a chip of 1 cm2 has increased from about 140 million to 2 billion, quite a large number.

(a)

n

Epitaxial layer

n+ Buried layer

p

E

(b) n

B

p+

C n+

p

n

p+

Fig. 9.54 n

(a) Buried layer diffusion prior to epitaxial growth. (b) The completed transistor differing from that of Fig. 9.53 by having an additional n+ region.

210

Principles of semiconductor devices Metal p+

p+

SiO2

n

Fig. 9.55 A simple MOST with contacts.

We have to note here that not only is the science difﬁcult, but also that increasing resolution by a factor n, and consequently the component density by n2 , involves formidable problems in costs and man-years, which also go up by n2 . The costs begin to look like the national debt, and the personnel involved lead to management problems of large teams, to reduce (say) 500 man-years to a development period that keeps you ahead of the opposition. This has led to international collaboration involving all the major players. One of the results coming out is a massive document called the International Technology Roadmap for Semiconductors. It sets industry standards and predicts the main trends in the semiconductor industry. The minimum feature size is now supposed to decline to about 10 nm. Is that feasible? Probably it is. Is that the last hooray of the planar process? Probably it is. The same technique cannot go on for ever. So what are the limitations? First, the number of electrons: as dimensions decline, a stage will be reached when the ﬂuctuations will cause unacceptable degradation in performance. Another obvious factor is the increase in capacitance; and remember that capacitors need time to be charged and discharged. Tunnelling across the gate oxide or from source to drain is also a serious limitation. What else? Heat. As the density of components increases, heat dissipation will become a major, maybe insoluble, problem. All the arguments suggest that the planar process will not survive for long, but, as we know from experience, it refuses to die quietly. One of the techniques that has postponed its demise is plasma etching, which we shall discuss in Section 9.23. A number of other approaches that have improved resolution will be presented in Section 9.24. We shall ﬁnish this section with Moore’s famous law that has been quoted in many different forms. Its essence is that the number of components on a chip increases exponentially as a function of time. Figures quoted have been doubling every year, doubling every 18 months, or doubling every two years, depending on the mood of the time, optimistic or pessimistic. Let’s make a simple calculation. Assuming that the process started in 1960 with a single transistor, and that now in 2013 the number of transistors on a chip has increased to 2 billion, we ﬁnd that the rate of increase in those 53 years is equal to p53 = 2 × 109 , which comes to a factor of about 1.5 per year or a doubling of the number about every 18 months. Remarkable. Never in the course of human history has such a steady increase been sustained for such a long time.

9.23

Plasma etching

Plasma etching has become a very important technique, deserving a more detailed description. What can plasma etching do that other etchings can’t? Let’s look at the steps in Fig. 9.53. The etching away of silica or silicon layers,

Plasma etching described there, is an isotropic process—acid reacts sideways as well as downwards, so the sidewalls of channels are eaten away, making a, the minimum feature size, larger. This is worsened if hot hydroﬂuoric acid is used to speed things up or to dissolve silicon nitride layers (which have been used to improve MOST performance). It can damage the edge of the photoresist. There are skilled handling operations involved in the liquid (wet) chemistry, so that operator skills were found to affect device yields. Improvements were needed as a got below 1 μm. Plasma processing was introduced, a dry process, more automated. We ﬁrst mentioned plasma physics∗ in Section 1.7 and it has cropped up several times since then. Usually a gas discharge plasma is about 0.1% ionized and so consists mainly of neutral gas atoms or molecules, outnumbering the ions and electrons. To achieve anisotropic etching we must use a ﬁeld to direct etching ions to the surface, and not to the sidewalls. In the jargon, this is RIE, or reactive ion etching. This ﬁeld can be realized with a d.c. voltage between the input and the earthed electrodes (Fig. 9.56). Or this can be done more cleverly by controlling the gas constituents of the plasma so that the sheath which forms on the surfaces of the electrodes has a built-in ﬁeld which inﬂuences the ions striking the semiconductor slice. The sheath contains positive and negative ions as well as electrons and in practical cases can have a potential difference of several kilovolts. The neutral atoms will slow down the movement of the ions, so to increase their mean free path we need a low gas pressure, but we also need a high ion density for fast processing. The obvious way to satisfy these criteria is to increase the ionization fraction of the gas. One way of doing this is by capacitatively coupling a radio frequency ﬁeld of quite high power into the plasma vessel. This has usually been at a frequency of 13.56 MHz.† The ion density can be increased further by applying a static magnetic ﬁeld to achieve electron cyclotron resonance (Section 1.6) so that the electrons absorb more energy from the r.f. ﬁeld. An outline diagram of an apparatus for this is shown in Fig. 9.56. A well-read textbook, Plasma etching,‡ gives the pressure range of gases used as 0.13 to 133 Pa. The reason for this rather arbitrary choice becomes apparent when we restate it in the previous preferred units of millimetres of mercury, or torr. It then becomes 10–3 Torr to 1 Torr, showing that most plasma engineers were brought up using ‘old money’.

211 ∗ Gas

discharge physics has been a favourite topic for scientists for well over a century. Irving Langmuir, who was a pioneer of diagnosing gas discharges, especially with probes, coined the word ‘plasma’ about 87 years ago at the time of writing (2013). The subject got an immense boost about 60 years ago when the possibility of controlled fusion of hydrogen isotopes was proposed to solve our energy problems with no nasty side products. The science was well established. E = mc2 was believed by everyone, and all the stars used fusion, including our sun, which had enabled life on earth to be established. It could also be man made, as we had the H-bomb, which at some times had threatened to ﬁnish life on earth. So it seemed only a development job to get a controllable fusion energy source. Enormous sums of money and highly skilled man-hours have been spent in failing to do this (so far). A by-product is a lot of skilled plasma physicists who have done good science, but, unfortunately, almost every discovery has revealed new instabilities which make it more difﬁcult to contain the hot plasma in its reaction vessel. It looks as if the right size for a fusion reactor is the size of the sun—much too large to ﬁt into the Los Alamos desert or even the Australian Outback. Thus there is a lot of plasma knowledge which can be separated from fusion plasma physics and instead used to study plasma etching and cleaning of surfaces. †A

frequency allocated by governments for industrial use. We mentioned this frequency, together with 2.45 GHz, in describing molecular beam epitaxy (Section 8.11.5). ‡ M.

Sugawara, Plasma etching, fundamentals and applications, Series on Semiconductor Science and Technology (Oxford University Press, 1998).

Gas inlet

R.F. generator

~ Wafers

Exhaust pump

Field coils

Fig. 9.56 Diagrammatic drawing of plasma etching apparatus. The pressure monitors and controllers to keep the etchant gases at the required levels are not shown.

212

Principles of semiconductor devices A survey of published results on plasma etching shows that r.f.- excited plasmas, usually of argon and various reactive gases, operate at total gas pressures of 9–90 Pa and generate plasma ion densities of between 2.1 × 1012 and 2 × 1016 m–3 . With an applied magnetic ﬂux for electron cyclotron resonance (about 4.8 × 10–4 T for the standard frequency), the operating pressure range is down to 0.01–3 Pa but the ion density is up to 7 × 1016 – 9 × 1017 m–3 . This trend to lower pressure and higher density has been carried on using magnetron-type discharges and helicon waves. All of this is described in the book by Sugawara mentioned above. The basic procedure with the equipment of Fig. 9.56 is to use the diffusion pump to evacuate the chamber to about 10–6 Torr, baking the whole to outgas air, water vapour, and residual chemicals, and then to throttle down the pumping line and open needle valves to admit gases so that the required gas pressure is attained in equilibrium; there is provision to remove volatile products when the r.f. power and the etching process are started. Another method of getting high ionization is to use microwaves fed through a waveguide into the plasma vessel. Frequencies similar to that used for microwave cooking have been used: 2.45 GHz. This corresponds to a wavelength of 12.2 cm so the reaction vessel can be made a resonant cavity, with a highﬁeld region in the vicinity of the Si slice. Again electron cyclotron resonance can be utilized; this requires a magnetic ﬂux density of about 8.7 × 10–2 T, which greatly increases the cost and bulk of the equipment, and so is not very popular. Now we must consider plasma chemistry. The ion must be chemically reactive with the SiO2 surface. By analogy with the wet processes which use HF, a ﬂuorine ion is needed. Carbon tetraﬂuoride (CF4 ), a gas which is chemically a close relation of the well-known degreasing ﬂuid carbon tetrachloride, has been used, as well as other ﬂuorides of carbon. It is usually mixed with one of the inert gases argon or xenon to enhance gas breakdown. A further use of dry processing is to get rid of the photoresist coating. This can be burnt off in an ashing process using a gas mixture including oxygen. The slice can then be taken out of the plasma reactor, recoated, and masked again for the next process, until the ﬁnal contact layer is made.

9.24

Recent techniques for overcoming limitations

The minimum feature size depends on resolution, and the resolution achievable at a particular wavelength λ has been known for well over a century to be equal to λ/(2n sin θ ), where n is the index of refraction and θ is the cone angle of the beam. • Immersion lithography. This technique uses a higher-index material than air. The simplest one that can be used is water, which can improve resolution by about 35%. The disadvantage is the impact of water on the photoresist. This technique has been used to reduce a to 65 nm and then to 45 nm, and it is likely to be used for reaching the next target of 32 nm. • Double patterning. This increases the number of fabrication steps. In double exposure, a photoresist layer is exposed twice with alternating phase-shift masks. The principle can be appreciated by considering a masking pattern

Building in the third dimension consisting of an opaque array of bars interspersed with transparent regions. The shadow of a bar will be made fuzzy by diffraction. Now, if alternate ‘windows’ are ‘glazed’ with a half-wavelength phase shifter, the light through adjacent windows is out of phase, so the light diffracting around the bar will interfere destructively, reducing the fuzziness and making the bar’s shadow sharp, as if it were a larger object, away from the diffraction limit. • High-k gate dielectrics. This is the jargon used. For some reason semiconductor technologists denote the relative dielectric constant by k, instead of the εr that is used by practically everybody else. The problem is with the insulator between the metal electrode and the channel in a MOSFET. As a result of scaling down all the dimensions, this insulating layer went down to 1.2 nm, containing just ﬁve atoms. That led to some leakage current by tunnelling when the transistor was off. Leakage current means more heat and shorter battery life. Thus something had to be done when the next scaling down, to 45 nm, was considered. A thicker insulator was needed but without an increase of the voltage drop across it. The solution was to replace silica (εr = 4.1) by an insulator which had a higher dielectric constant.∗ The two insulators considered by the various companies were hafnium dioxide, with a dielectric constant around 20, and zirconium dioxide, with a slightly higher dielectric constant of 25. It turned out that for technological reasons it was also necessary to return to a metal gate electrode.† The metal used was molybdenum, a high-melting-point material. • Extreme ultraviolet (known also as soft X-ray) lithography. The shorter the wavelength, the higher is the resolution. On that basis, all we need is to ﬁnd some sources at the right wavelength. If we want a minimum feature size of 13 nm (some optimists believe that that is possible) then we need sources at about the same wavelength. As it happens, there are methods to create such radiation. The favourite scheme is to have a powerful pulsed laser, direct it on a piece of metal that has lots of electrons (tin, molybdenum, and silver have been favourite candidates), and turn the metal into a plasma, which will convert the incident radiation with reasonable efﬁciency (a ﬁgure of a few per cent has been quoted) into the desired extreme UV wavelength. This is not easy to do, but if one succeeds, that is only the beginning of the problems. At this wavelength there are no lenses and mirrors of the kind that exist at longer wavelengths. Mirrors have been produced from multilayers (see Section 10.5) but they are very lossy. In fact all materials are lossy at these wavelengths. So no proper projecting optics exist, nor are there appropriate masks or photoresists. Efforts are of course being made in this direction and one day they may succeed, but it is difﬁcult to see when.

213

∗ It follows from the continuity of D, the electric ﬂux density, that the electric ﬁeld is lower in a material with a higher dielectric constant. † In

fact, metal electrodes were replaced by polysilicon ones in the late 1960s but the acronym MOSFET, referring to ‘metal–oxide–semiconductor’, survived. Concerning the principles, it made no difference so there was no reason to mention this in Section 9.22. Lately, however, polysilicon has been abandoned and metals have regained their rightful place.

9.25 Building in the third dimension All the microelectronic circuits we have been talking about were built in two dimensions; that’s why the technique is often called the planar technique. It is invariably a plane surface that is manipulated for producing a host of devices. It is like Flatland,‡ a world of two dimensions. Can we get out of Flatland and start building circuits in the third dimension? A start has already been made. It is believed that the present arrangement of the source, drain, and gate (in spite

‡ Flatland:

A romance of many dimensions is a short novel by Edwin Abbot, published in London in 1884. It is about life that is lived in two dimensions and how the inhabitants can deduce evidence about the existence of a third dimension.

214

Principles of semiconductor devices

FinFET Source Drain

Fig. 9.57 Schematic representation of a FinFET (i.e. a ﬁeld-effect transistor in which the gate is wrapped around a ﬁn-like channel).

Gate

Channel

of the high-dielectric-constant gate oxide) will not survive when the next reduction in size is considered. The basic idea is shown in Fig. 9.57. The channel connecting the source and drain is a thin, ﬁn-like wall jutting out of the silicon substrate. The gate is wrapped around the channel. The device is called a multigate FinFET. There are indeed solutions with more than one gate, but one could also claim that the wrapped-around gate is equivalent to three gates. Having broken the taboo of ﬂatness, one could of course go much further and build genuine three-dimensional circuits. Some optimists believe that they will come some time in the future. How would we attempt to build them? Having completed our circuits in two dimensions we would carefully put an insulating oxide layer on the top and start afresh. Alas, we no longer have our nice, epitaxial layer of silicon: the crystalline regularity has been lost. There is no problem depositing silicon on the top of the insulator but it will be an amorphous layer and everyone knows that amorphous materials are not good for building high quality transistors. This has certainly been the state of the art until recently. What has changed is the ability to produce a ‘good’ amorphous layer by depositing the silicon at the right temperature to be followed by the right heat treatment. Good in this context means that the single crystal grains, of which all amorphous materials are made, can now be quite large, large enough to accommodate a fair number of transistors. One more problem that had to be solved was the presence of irregularities, hills and valleys, after each deposition process. A technique to eliminate them, called chemical-mechanical polishing, has also been perfected. So the road to three-dimension-land is open. What are the advantages? The main advantage, clearly, is higher packing density: to gain a factor of 10 is not to be sniffed at.The devices being closer to each other also means that the signals have shorter paths to travel, and that increases speed. Unfortunately, there are still a number of disadvantages which will exclude them for the moment from ﬂooding the market. The greatest disadvantage is of course a straight consequence of the polycrystalline nature of the layers. Devices that lie on the grain boundaries will not work. Therefore error detection and correction techniques must be an integral part of the system. Speed may also suffer. The advantage of shorter paths is offset by the slower switching speed of amorphous devices. And then comes the problem of heat. It is difﬁcult enough to avoid overheating in a two-dimensional structure. It is much more difﬁcult to do so in three-dimension. The answer is to reduce voltages or simply cool the system. Will it be economic to do so? For some applications, for example, for using them as simple memory cells, the answer may already be yes.

Microelectro-mechanical systems (MEMS)

9.26 Microelectro-mechanical systems (MEMS) Up to now, everything has been immobile. Well, nearly. Electrons had a licence to roam about and the lattice was allowed to vibrate. The difference is that, from now on, part of a structure can mechanically move to perform some useful function. This is a big subject to which we are unable to do justice in the few pages available, but we shall try to convey the essence of the idea by going in some detail through one example (a movable mirror) and discussing the role of a quadrupole ﬁlter in the context of a mass spectrometer.

9.26.1

A movable mirror

In the present section we shall talk about the construction of the mirror (many of the steps in the process are similar to those discussed in relation to microelectronic circuits). The optical aspects will be discussed in Chapter 13. I shall start with a silicon wafer with a SiO2 insulator on the top. We could deposit polysilicon on the insulator, as outlined in the previous section, but if we need a thicker layer and higher quality then another technique, called Bonded Silicon-on-Insulator, is used. It involves the bonding of another silicon wafer to the oxidized silicon substrate. The initial bonding is carried out under ultra-clean conditions, and the assembly is then heated in a furnace to strengthen the bond by inter-diffusion. The bonded layer may then be ground and polished, to leave a high-quality single crystal Si layer which can be of virtually any desired thickness. To fabricate the mirror, the bonded layer is ﬁrst metal-coated, typically with Cr to improve adhesion and then Au to improve reﬂectivity. This is shown in Fig. 9.58(a). We have ﬁve layers on top of each other: silicon, silicon oxide, silicon, chromium, and gold. The next problem is to shape both the mirror and its elastic torsion suspension in the bonded layer. As you may guess, the bonded layer is coated with photoresist which is then patterned with the mechanical shape of the mirror, elastic suspension, and surround. After that come two different kinds of etching, the ﬁrst one to transfer the pattern to the metal and the second to transfer it to the silicon layer. We arrive then at the situation shown in Fig. 9.58(b) (cross-section) and 9.58(c) (top view). The next step is to remove the photoresist after which the whole thing is turned upside down, the substrate side is coated with photoresist and patterned to deﬁne a clearance cavity (we need the cavity for the mirror to be able to move). Two further etchings are needed now, one to remove the silicon and the next one to remove the silicon oxide. At this point the mirror is free to rotate on its suspension [Fig. 9.58(d) and (e)]. The released structure is then turned upside down once more and attached to a second wafer, which carries a pair of patterned metal electrodes on an insulating oxide layer [Fig. 9.58(f)]. The mirror is now complete [Fig. 9.58(g) and (h)], and may be rotated by applying a voltage between the upper electrode and one lower electrode. The mirror will rotate until the attractive electrostatic force between the electrodes is balanced by the restoring force provided by the elastic suspension. The elastic qualities of silicon are surprisingly good, and there are few problems with fatigue and brittle fracture if the assembly is packaged and handled carefully.

215

216

Principles of semiconductor devices (c) Surround

(a)

Cr/Au Si SiO2 Si

Mirror

Resist

(b)

Torsion suspension (e)

Cavity (d)

Mirror (h) Suspension

Cavity

Electrodes (f )

Fig. 9.58 Fabrication sequence for a single-axis electrostatically driven MEMS torsion mirror. After Aksyuk et al. Proc. SPIE, 4178, 320, 2000.

(g) Drive electrode

You will realize that the aim was to show the basic principles by giving an example of practical signiﬁcance. There are better solutions but the present one will also work well for a limited angular range. Turn angles of a few degrees may be achieved with drive voltages of 100–200 V. Two-axis mirrors may be constructed using similar principles, by mounting the mirror in a gymbal with two orthogonal elastic suspensions and two orthogonal sets of drive electrodes.

9.26.2

A mass spectrometer on a chip

Our next example is a mass spectrometer. As the name implies, it measures the range of mass in a particular assembly of molecules. The problem is to ﬁnd out how many molecules are between two limits, say between 150 and 160 atomic units. In principle, we could weigh each molecule on a sensitive balance and, having measured their weight/mass, we could choose the right ones and put them in a box marked ‘150–160’. In practice, this is not a feasible way to proceed. Instead of boxes, we should have detectors and the selection should be done by some sort of ﬁlter. How can we do that? The means at our disposal are electric and magnetic ﬁelds. Unfortunately, they cannot affect neutral molecules.

Microelectro-mechanical systems (MEMS) The solution is to attach, at least to a certain fraction of the molecules, a charge. How? We ionize them. There are actually many ways to do that. We shall mention only one of them: electron impact ionization.∗ Either the electrons are produced by thermionic emission (Section 6.5) or they are ﬁeldinduced (Section 6.7), and then they are accelerated to acquire the right amount of energy. As it happens, the right energy can be found by a very simple argument. The average bond length of the molecules of interest is about 0.15 nm. If we want electrons to break those bonds then it makes good sense to choose an accelerating voltage which leads to a de Broglie wavelength of the same length. Luckily, we have already looked at this calculation when working out the accelerating voltage for the experiments of Davisson and Germer (Section 2.1). We got a de Broglie wavelength of 0.1 nm using a voltage of 150 V. Hence, to obtain 0.15 nm we need about half of that voltage (remember, the de Broglie wavelength is inversely proportional to the square root of the applied voltage), and indeed the voltage usually employed is 70 V. The accelerated electrons are then injected into an ionization region, where they encounter the analyte. Next we need to ﬁlter the ionized molecules according to their mass. The most obvious way of doing that is to introduce the ions into a homogeneous magnetic ﬁeld, where they will be deﬂected (remember eqn (1.46)) by a force perpendicular both to the applied magnetic ﬁeld and to the electron velocity. This type of ﬁltering works very well indeed. Mass spectrometers based on it were developed originally by the fathers of mass spectroscopy, Thomson, Aston, and Bainbridge, some hundred years ago. Nowadays it is less fashionable. The way which is in the ascendancy is quadrupole ﬁltering. It needs four parallel electrodes, which can produce the right electric ﬁeld distribution. Between the electrodes there is a channel, into which the ions are injected. What do we want to achieve? That most of the ions fall by the wayside (bump into electrodes) but those with the right mass sail through unharmed. It turns out that static electric ﬁelds on their own cannot be used for this purpose. On the other hand, if they are aided and abetted by a time-varying voltage in the lower MHz range and, in addition, the electrodes are shaped so as to produce a hyperbolic potential distribution,∗ then the aim can be achieved. For a speciﬁc ratio of the d.c. and a.c. voltages, ions with a particular mass have bounded trajectories and transit without discharging. Tuning of the ﬁlter is done by varying the d.c. and r.f. voltages but keeping their ratio constant. It is an ingenious solution. The inventor, Wolfgang Paul, got a Nobel Prize for it in 1989. Having got the right ions through the channel, we need to detect them. That is relatively easy. Ions may be detected on a separate electrode, where they discharge to become molecules, leaving the charge to be converted into a voltage by a low-noise ampliﬁer. So we have got everything we need: an ion source, a mass ﬁlter, and a detector. But, you may say, what happens if there are two different kinds of molecules with identical mass? Can we distinguish them? Yes, we can, but not on the basis we have described so far. We have not told the full truth. When the molecules are ionized they may fragment into daughter ions. Instead of just one type of ion, each molecule generates a distribution of ions, a kind of signature that can be recognized. Finally, let’s see how a quadrupole can be constructed. A relatively simple way is to etch down crystal planes of silicon in a particular direction. The (111) planes lie at 54◦ to the surface of (100) oriented wafers, and are resistant

217

∗ This is a good method when the analyte

(the substance to be analysed) is a gas.

Francis William Aston, Nobel Prize in Chemistry, 1922.

∗ Ideally,

electrodes of hyperbolic shape are needed but it is not easy to produce them. It turns out, however, that the required potential distribution can be well approximated by electrodes of cylindrical shape.

218

Principles of semiconductor devices

Silicon substrate Electrode Spacer

Fig. 9.59

Oxide

Schematic representation of a quadrupole ﬁlter in a mass spectrometer.

Groove Ion beam

to chemical etches. Hence etching through rectangular mask openings creates V-shaped grooves, which can locate two electrodes. Next the silicon is thermally oxidized to provide a surface oxide layer. This is necessary because the electrodes must be insulated. The whole assembly of the quadrupole ﬁlter (Fig. 9.59) can then be constructed from two dies, each carrying two electrodes and separated by cylindrical spacers in similar grooves. And now we have come to the most interesting question: how large is a mass spectrometer? Those designed by the founding fathers needed a goodsized room to accommodate them. How large is this miniaturized version? The major item is the ﬁlter, which has dimensions of about 6 × 3 × 30 mm3 , considerably below the size of a room. A complete mass spectrometer of course needs an ion source, an ion detector, a vacuum enclosure, vacuum pumps, and drive electronics. There is some way to go before all of these components are miniaturized. However, as unlikely as it seems, desk-top mass spectrometers containing MEMS quadrupole mass ﬁlters, together with other MEMS devices (an electrospray ion source operating at atmospheric pressure and a chip that allows ions to be transported into the vacuum system) are already commercially available.

9.27

Nanoelectronics

We are getting more familiar with devices and techniques in the nanometre region. At the time of writing (August 2013), transistors with a minimum feature size of 32 nm are available commercially. There is, however, still an aura of mystery surrounding the subject. This is partly due to some exaggerated claims made in the past decade by science ﬁction writers aided and abetted by some scientists. It is the dream of nanobots, little robots that will do everything conceivable: producing food from basic elements and, when needed, scrambling up in your veins in order to repair a clot. A further reason might be the awe we all feel when coming to atomic dimensions. Can we really interfere so much with nature? Will nature ﬁght back? The third reason is that, apart from brute force (as manifested in the continual reduction in the size of traditional devices), nobody is sure in what direction to push ahead; or, rather, every participant in the game, which is amply ﬁnanced, is pushing ahead in a different direction. By the nature of the problem there are two basic approaches: top-down and bottom-up. In the former case one proceeds like a sculptor chiselling away unwanted material and adding bits here and there. This is the approach of microelectronics, the familiar approach. The bottom-up approach is the new one. It can be done. It is not impossible, just pretty difﬁcult. Let me

Nanoelectronics give you some indication of how it has been done. The technique is that of Micro-Electro-Mechanical Systems, discussed earlier, but on a much smaller scale so that we can replace the ‘Micro’ by ‘Nano’ arriving at the ﬁeld of NEMS. The bottom-up approach is based on a small cantilever∗ that can actually capture an atom off the surface of some material and deposit it at another place. The principles followed are that of the atomic force microscope. There is no doubt that successful experiments have been done and a lot has been learned but that is still a far cry from building useful devices in a reliable manner. Do we know the laws governing the nanometre scale? Yes, of course, they are the laws of quantum mechanics. We know the basic equations, but computers are just not powerful enough to get even near to solving them for practical situations. So far in this course we have been able to manage by injecting no more than a small amount of quantum mechanics. We needed some basic tenets in order to explain the mechanism of conduction, the role of the periodic structure of atoms, the concept of tunnelling, etc. But having accepted the notion of conduction and valence bands, the presence of two kinds of carriers, energy gaps, impurity levels and so on, we could really use the familiar classical picture. It does not really stretch our magination to the limits to ‘see’ holes diffusing across the base region. We may legitimately boast to have tamed quantum mechanics when dimensions are above about 50 nm. For structures smaller than that the taming has just began. One hopes that it will continue successfully. I shall now discuss in a little more detail one of the devices that needs some structure on the nanoscale. It bears some resemblance to the High-ElectronMobility-Transistor discussed in Section 9.15. The only essential difference, as shown in Fig. 9.60(a), is that the gate electrode is now split. There are now three ﬁnger-gates placed close to each other, where each ﬁnger-gate can be biased independently. Let us have reverse bias on the outer gates, so there is a depletion layer below them. This means that the charge sheet sticking to the AlGaAs/GaAs boundary will have discontinuities. If there are no charges, there is no current. So how will this device work? Let me quickly add that the inner gate is forward biased, so that the potential distribution between source and drain will have the approximate shape shown in Fig. 9.60(b). Well, we have a lower potential in the middle, but will that help? It will if the dimensions are sufﬁciently small—then electrons may tunnel through the barriers. Does this mean that the current will ﬂow as in a tunnel diode? In one sense yes, because tunnelling is necessary for the existence of electron ﬂow. It is different, though, in another sense. In the tunnel diode the energy levels of the electrons were nigh inﬁnitely close to each other. The current depended on the density of states. With gate ﬁngers around 20–50 nm the electrons are conﬁned to such a small range that the individual energy levels can be distinguished. One mode of operation is where the potentials at the outer gates and between the source and the drain are ﬁxed and the inner gate potential is varied, that is the depth of the potential well is controlled. The energy levels are determined by the conﬁnement, so their positions are ﬁxed relative to the bottom of the well. Hence, when the depth of the well is changed, the energy levels move up and down. There will be current ﬂowing whenever a given energy level inside the well matches that of the electrons outside the barrier. The name given to this phenomenon is resonant tunnelling, and the device shown schematically

219

∗ The

small cantilever may also serve as the basis of a new type of memory promising gigabytes of information on a few square centimetres. Several companies, including IBM, made progress in that direction. The information is written by a sharp tip perched at the end of the cantilever dipping into a polymer and creating a pit. The presence of a pit may then be regarded as a one and the absence of a pit as a zero. Reading is also done by a tip relying on a change of electrical resistance when it enters the pit.

(a) source

(b)

split gate

drain

n-type GaAlAs undoped GaAs semi-insulating GaAs

G1 G2 G3

Fig. 9.60 (a) Schematic representation of a Lateral Resonant Tunnelling Transistor; (b) Energy diagram inﬂuenced by the voltages on the split electrodes.

220

Principles of semiconductor devices in Fig. 9.60(a) is known as a Lateral Resonant Tunnelling Transistor. Lateral, because the electrons move in the lateral (horizontal) direction, and resonant because current ﬂows only at certain resonant values of the inner gate voltage. One can see that here is a device which can be switched by very small changes (of the order of millivolts) in voltage. In practice, at least for the present, the energy levels are not so well resolved, mainly due to electron scattering in the well which will spread the electron energies. Cooling the device will help, but we are still very far away from measuring delta functions in current. What we do see are little current maxima at the right voltages. But these are early days. There are a number of other devices too which have been shown to work in the laboratory. Let me mention four of them. Nanotube transistors. In order to make nanotube transistors we ﬁrst need nanotubes. What are they? They are thin-walled cylinders of about 1.5 nm diameter and 25 nm long bearing strong resemblance to the fullerenes discussed in Section 5.3.6. The wall is usually made up of one single atomic layer of carbon atoms. The process of preparing them is relatively easy. An arc needs to be struck between graphite electrodes at the right pressure. They are made up of graphite sheets and have their desirable properties (strong covalent bonds) without the disadvantages (weak bonds between the layers). They are very strong mechanically, they have both metallic and semiconductor varieties. The problem is to get rid of the metallic variety. One of the methods to do this is to burn them out, another is to use chemical compounds to attract metallic and semiconductor tubes to different areas of the surface. What do they look like? They may be tubes hollow all the way or they might be nicely, hemispherically terminated. Their shape also depends on the way the graphite sheet is rolled up. If one of the axes of the hexagonal set coincides with the axis of the nanotube, they take the form shown in Fig. 9.61(a), if it is at an angle we obtain Fig. 9.61(b). They certainly give pretty patterns. A property that is important for applications is that due to van der Waals forces they stick to the surfaces they are deposited on but they do not stick too ﬁrmly, so they can be shifted about, turned around, can be bent and can be cut. When we want to make FETs out of them the substrate can serve as the gate electrode, the tube provides the semiconducting path that is affected by the gate voltage, and the ends of the tube serve as the source and the drain with metal electrodes deposited upon them. The second device or, rather, set of devices we want to talk about is based on graphene, which we previously mentioned in Chapter 5. This is a

Fig. 9.61 Graphite sheets rolled up into nanotubes at different angles.

Nanoelectronics two-dimensional sheet of graphite or can be regarded as a carbon nanotube unfolded. It has a number of remarkable properties, which are being explored at a number of research laboratories around the world. It has odd properties, for example displaying the quantum Hall effect (to be discussed in Section 11.8.6) at room temperature. It is a semiconductor but there is no gap between the valence and conduction bands. The density-of-state functions are two inverted cones meeting at the line separating the two bands. The particles, electrons or holes, resemble in some respects photons. They move with a constant velocity which is independent of their kinetic energy. Even at room temperature they scatter little, so that within a range, comparable with distances in a transistor, they can be regarded as ballistic particles. Can one make ballistic transistors out of graphene? Perhaps. One problem is to have a regime in which no current ﬂows. If there is no energy gap, the current cannot be stopped. This problem has been overcome by introducing constrictions in the material, which turn out to be equivalent to gaps. It is too early to say what kind of devices might emerge. They certainly belong to nanoelectronics since the device sizes might be between 10 and 50 nm. The third device is the Single Electron Transistor which, strictly speaking, does not belong to this chapter since the materials involved are metals and insulators not semiconductors. On the other hand they can only work when the dimensions are in the nanometre region so it is not unreasonable to discuss them here. The effect upon which these devices are built comes from a combination of electrostatics and tunnelling. The basic conﬁguration is a Metal–Insulator–Metal–Insulator–Metal (MIMIM) junction. The metal in the middle is called a Coulomb island. The aim is to show that a single electron can make a difference. This may occur when the electrostatic energy due to a single electron, 12 e2 /C, exceeds the thermal energy 21 kB T, where C is the capacitance. When the dimensions are sufﬁciently small∗ this capacitance is also small allowing a high enough electrostatic energy. When a voltage is applied and an electron tunnels across to the Coulomb island, the resulting change in energy is sufﬁciently large to forbid any further ﬂow until the voltage is raised to such a value as to overcome this barrier. The argument can be made a little more precise by using an energy diagram. At thermal equilibrium [Fig. 9.62(a)], due to the presence of a signiﬁcant electrostatic energy (denoted here by Es ), there are no states available to tunnel into in the vicinity of the Fermi level. The potential barrier Es is partly below and partly above the Fermi level. Clearly, no current can ﬂow in response to a small voltage. This is called a Coulomb blockade. However when the applied voltage is sufﬁciently large to overcome the barrier [Fig. 9.62(b)] there is an opportunity for a single electron, to tunnel across. But only for a single electron because as soon as it tunnels across from right to left a new barrier is erected which can only be overcome by increasing again the voltage above the next threshold. Hence, the current voltage characteristics consist of a series of steps known as a Coulomb staircase. Having discussed the basic phenomena it is now easy to imagine how they can be utilized in a three-terminal device. We need an additional gate electrode to control the ﬂow of electrons as shown schematically in Fig. 9.63(a), or two gates and two islands if we want more sophisticated control [Fig. 9.63(b)]. The latter arrangment, a little similar to that used for CCDs (Section 9.16), permits the transfer of a single electron from source to drain by choosing a suitable sequence of gate voltages. In a practical case one should of course choose

221 (a)

Es

EF

Insulators

(b) eVa = Es

Metal

Fig. 9.62 Energy diagram for a Single Electron Transistor (a) in thermal equilibrium, (b) when a voltage Va is applied. ∗ One

must be a little careful here. One cannot just say that small dimensions lead to small capacitance. In fact, a small intermetallic distance, needed for tunnelling to take place, leads to a high capacitance. It needs to be emphasized then that the metallic areas facing each other must be very small. Taking the insulator as air, the inter-metallic distance as 1.5 nm and the cross-sections facing each other as circles of 10 nm radius we end up with a capacitance of 1.8 × 10–18 F and an electrostatic energy of 7 × 10–21 J. Note that this is about 3.5 times higher than the thermal energy at room temperature.

222

Principles of semiconductor devices

M

(a)

I

M

I

M

gate Vg

(b) M

I

M

Vg2

I

M

I

M

Vg1

Fig. 9.63 Single electron transfer controlled by (a) a gate electrode in the MIMIM, and (b) by two gate electrodes in the MIMIMIM conﬁguration.

a planar conﬁguration. The Coulomb island(s) and the two metal electrodes would be evaporated upon one side of an insulator and the gate electrode(s) upon the other side. If one thinks about it one must acknowledge that this is an amazing feat of science: the control of current down to a single electron. Will these devices ever reach the market place or will they remain a scientiﬁc curiosity? I think they will—in the fullness of time. The idea is so revolutionary, so challenging that sooner or later the necessary effort will be invested into it. What can one hope for? The advent of an entirely new family of logic circuits. The fourth new type of device I wish to mention here but only very brieﬂy is the Molecular Transistor. It is made of Rotoxane—a molecule that can switch from a conducting to a not-so-well-conducting state by the application of a small voltage. Most of the ideas behind devices on the nanometric scale have been around for quite some time and experimental results showing the feasibility of the ideas have also been available. A more detailed investigation of the relevant phenomena is however quite recent for the simple reason that it took time to develop the technology. The main motivation has been to put more devices on a mm2 but many of the experiments conducted have also led to some new physics, as for example to the discovery that in a sufﬁciently narrow bridge both electrical and thermal conductivity are quantized. Nanostructures have been made by a variety of methods. It is obviously beyond the scope of the present course to enumerate them. The one that is worth mentioning is the obvious one, electron beam machining, that can produce the required accuracy due to the very short wavelength of accelerated electrons (see examples in Chapter 2). It can write features on an atomic scale, although that method is not completely free of technical difﬁculties either, for example spurious effects due to the electrons bouncing about in the photoresist. The biggest problem however is cost. In microelectronics one can simultaneously produce the pattern for a million elements. If we use electron beams, the pattern must be written serially, and that takes time and effort.

9.28

Social implications

Do great men change the world? They surely do. History is full of them. But, to use an engineering term, they are randomly distributed in space and time so their effect on the whole cancels out. They can, admittedly, cause signiﬁcant local perturbations, but the associated time constants are invariably small. Technology is in a different class. Whatever is learnt is rarely forgotten. The interactions are cumulative. So it is not unreasonable to assume that when they exceed a critical value society is no longer able to escape their effect. We may roughly say (only a ﬁrst-order approximation, mind you) that present-day society is determined by the invention and by subsequent improvements in the performance of the steam engine. With the same degree of approximation, we may predict that our future society will be determined by the invention and by subsequent improvements in the performance of semiconductor technology. So the scientists and engineers have done their duty. They created wealth. They created a world in which everyone, every inhabitant of the Earth, could have enough to eat, could have clean drinking water, and could have a roof above their head. That has not happened. Many parts of the world

Exercises are plagued by starvation and disease. Corruption is widespread. Unnecessary wars abound. In the developed world, there is the twin problem of unemployment in general and over-employment in administration. People love to create work for each other, as so ably explained by Parkinson.∗ Any chance that the future will bring something better? We should perhaps ﬁnish this section by quoting again Gabor’s aphorism, the motto to the Introduction, page xiv: ‘Till now man has been up against Nature; from now on he will be up against his own nature’.

223

∗ C.

Northcote Parkinson, Parkinson’s law (John Murray, 1958).

Exercises 9.1. Show that the ‘built-in’ voltage in a p–n junction is given by Nhp kT Nen kT loge loge = , U0 = e Nep e Nhn where Nen , Nhn and Nep , and Nhp are the carrier densities beyond the transition region in the n and p-type materials respectively. [Hint: Use eqns (8.17) and (8.20) and the condition that the Fermi levels must agree.] 9.2. If both an electric ﬁeld and concentration gradients are present the resulting current is the sum of the conduction and diffusion currents. In the one-dimensional case it is given in the form dNe , Je = eμe Ne E + eDe dx dNh Jh = eμh Nh E + eDh . dx When the p–n junction is in thermal equilibrium there is no current ﬂowing, i.e. Je = Jh = 0. From this condition show that the ‘built-in’ voltage is U0 =

[Hint: Use the same argument for the conduction and diffusion currents cancelling each other as in the previous example.] 9.4. In a metal–insulator–n-type semiconductor junction the dielectric constants are ǫi and ǫs for the insulator and the semiconductor respectively. Taking the width of the insulator (sufﬁcient to prevent tunnelling) to be equal to di , determine the width of the depletion region as a function of reverse voltage. 9.5. The doping density across a p–n junction is of the form shown in Fig. 9.64. Both the donor and acceptor densities increase linearly in the range |x| < d0 /2 and are constant for |x| > d0 /2. Determine d, the width of the depletion region when the ‘built-in’ voltage is such that (i) d < d0 , (ii) d > d0 . Doping density ND

0

Nen De loge . μe Nep

Distance x

Compare this with the result obtained in Exercise 9.1, and prove the ‘Einstein relationship’

NA = ND

De Dh kT . = = μe μh e

NA d0

Ni2

Prove that Ne Nh = everywhere in the two semiconductors, including the junction region. 9.3. Owing to a density gradient of the donor impurities there is a built-in voltage of 0.125 V at room temperature between the ends of a bar of germanium. The local resistivity at the high impurity density end is 10 m. Find the local resistivity at the other end of the bar. Assume that all donor atoms are ionized.

d

Fig. 9.64 The variation of doping density in a p–n junction. 9.6. Use the expression given in Exercise 9.1 to evaluate the ‘built-in’ voltage for junctions in germanium and silicon. At room temperature the following data may be assumed:

224

Ge Si

Principles of semiconductor devices μh (m2 V–1 s–1 ) 0.17 0.04

μe (m2 V–1 s–1 ) 0.36 0.18

σp ( –1 m–1 ) 104 104

σn ( –1 m–1 ) 100 100

Ni (m–3 ) 2.4 × 1019 1.5 × 1016

where σp and σn are the conductivities of the p- and n-type materials respectively. 9.7. If a forward bias of 0.1 V is applied to the germanium p–n junction given in Exercise 9.6, what will be the density of holes injected into the n-side and the density of electrons injected into the p-side? 9.8. (i) In a certain n-type semiconductor a fraction α of the donor atoms is ionized. Derive an expression for E F – ED , where EF and ED are the Fermi level and donor level respectively. (ii) In a certain p-type semiconductor a fraction β of the acceptor atoms is ionized. Derive an expression for E F – EA , where EA is the acceptor level. (iii) Assume that both of the above materials were prepared by doping the same semiconductor, and that ED = 1.1 eV and EA = 0.1 eV, where energies are measured from the top of the valence band. By various measurements at a certain temperature T we ﬁnd that α = 0.5 and β = 0.05. When a p–n junction is made, the built-in voltage measured at the same temperature is found to be 1.05 eV. Determine T. 9.9. Calculate the reverse breakdown voltage in an abrupt Ge p–n junction for NA = 1023 m–3 , ND = 1022 m–3 , ǫr = 16, and breakdown ﬁeld Ebr = 2 × 107 V m–1 . 9.10. Determine the density distribution of holes injected into an n-type material. Assume that ∂/∂t = 0 (d.c. solution), and neglect the conduction current in comparison with the diffusion current. [Hint: solve the continuity equation subject to the boundary conditions, Nh (x = 0) = injected hole density, N h (x → ∞) = equilibrium hole density in the n-type material. 9.11. Determine from the solution of Exercise 9.10 the distance at which the injected hole density is reduced by a factor e. Calculate this distance numerically for germanium where D h = 0.0044 m2 s–1 and the lifetime of holes is 200 µ sec. 9.12. Determine the spatial variation of the hole current injected into the n-type material. [Hint: Neglect again the conduction current in comparison with the diffusion current.] 9.13. Express the constant I0 in the rectiﬁer equation I = I0 [exp(eU1 /kT) – 1] in terms of the parameters of the p- and n-type materials constituting the junction.

9.14. Owing to the dependence of atomic spacing on pressure, the bandgap Eg of silicon decreases under pressure at the rate of 2 × 10–3 eV per atmosphere from its atmospheric value of 1.1 eV. (i) Show that in an intrinsic semiconductor the conductivity may be expressed with good approximation as σ = σ0 exp(–Eg /2kT) and ﬁnd an expression for σ0 . (ii) Calculate the percentage change in conductivity of intrinsic silicon at room temperature for a pressure change of 10 atmospheres. (iii) Show that I0 , the saturation current of a diode (found in Exercise 9.13), is to a good approximation proportional to exp(–Eg /kT). (iv) Compare the pressure sensitivity of σ with that of I0 . 9.15. Take two identical samples of a semiconductor which are oppositely doped so that the number of electrons in the n-type material (N) is equal to the number of holes in the ptype material. Denoting the lengths of the samples by L and the cross-sections by A, the number of electrons and holes are: p-type

number of holes LAN number of electrons LANi2 /N

n-type

number of holes LANi2 /N number of electrons LAN.

Thus the total number of carriers in the two samples is N2 2LAN 1 + i2 . N Assume now that we join together (disregard the practical difﬁculties of doing so) the two samples. Some holes will cross into the n-type material and some electrons into the p-type material until ﬁnally an equilibrium is established. Show that the total number of mobile carriers is reduced when the two samples are joined together (that is some electrons and holes must have been lost by recombination). 9.16. A pn junction LED made of GaAsP emits red light (approximate wavelength 670 nm). When forward biased it takes 0.015 mA at 1.3 V rising to 17 mA at 1.6 V. When reverse biased its capacity is 83.1 pF at 1 V and 41.7 pF at 10 V. Avalanche breakdown occurs at 20 V. (i) Deduce I0 and the effective device temperature from the rectiﬁer equation. (ii) Assuming that the junction is very heavily doped on the n-side, ﬁnd the carrier density on the p-side. (iii) Deduce the junction area and the built-in voltage. Data for GaAsP: Permittivity = 12ǫ0 ; breakdown ﬁeld = 8 × 107 V m–1 .

Dielectric materials

10

Le ﬂux les apporta, le reﬂux les emporte. Corneille Le Cid

10.1 Introduction In discussing properties of metals and semiconductors we have seen that, with a little quantum mechanics and a modicum of common sense, a reasonable account of experiments involving the transport (the word meaning motion in the ofﬁcial jargon) of electrons emerges. As a dielectric is an insulator, by deﬁnition, no transport occurs. We shall see that we can discuss the effects of dielectric polarization adequately in terms of electromagnetic theory. Thus, all we need from band theory is an idea of what sort of energy gap deﬁnes an insulator. Suppose we consider a material for which the energy gap is 100 times the thermal energy at 300 K, that is 2.5 eV. Remembering that the Fermi level is about halfway across the gap in an intrinsic material, it is easily calculated that the Fermi function is about 10–22 at the band edges. With reasonable density of states, this leads to less than 106 mobile electrons per cubic metre, which is usually regarded as a value for a good insulator. Thus, because we happen to live at room temperature, we can draw the boundary between semiconductors and insulators at an energy gap of about 2.5 eV. Another possible way of distinguishing between semiconductors and insulators is on the basis of optical properties. Since our eyes can detect electromagnetic radiation between the wavelengths of 400 nm and 700 nm, we attribute some special signiﬁcance to this band, so we may deﬁne an insulator as a material in which electron–hole pairs are not created by visible light. Since a photon of 400 nm wavelength has an energy of about 3 eV, we may say that an insulator has an energy gap in excess of that value.

10.2 Macroscopic approach This is really the subject of electromagnetic theory, which most of you already know, so I shall brieﬂy summarize the results. A dielectric is characterized by its dielectric constant ǫ, which relates the electric ﬂux density to the electric ﬁeld by the relationship D = ǫE .

(10.1)

The basic experimental evidence (as discovered by Faraday some time ago) comes from the condenser experiment in which the capacitance increases by a factor, ǫr , when a dielectric is inserted between the condenser plates. The

In the SI system ǫ is the product of ǫ0 ( permittivity of free space) and ǫr (relative dielectric constant).

226

Dielectric materials

V Dielectric

reason is the appearance of charges on the surface of the dielectric (Fig. 10.1) necessitating the arrival of fresh charges from the battery to keep the voltage constant. In vacuum the surface charge density on the condenser plates is Q = ǫ0

Capacitor plates

Fig. 10.1

V , d

(10.2)

where d is the distance between the plates. In the presence of the dielectric the surface charge density increases to

Inserting a dielectric between the plates of a capacitor increases the surface charge.

Q′ = ǫ0 ǫr

V . d

(10.3)

Remember now from electromagnetic theory that the dielectric displacement, D, is equal to the surface charge on a metal plate. Denoting the increase in surface charge density by P, and deﬁning the ‘dielectric susceptibility’ by χ = ǫr – 1,

(10.4)

we may get from eqns (10.2) and (10.3) the relationships P = D – ǫ0 E

10.3

and

P = ǫ0 χ E .

(10.5)

Microscopic approach

We shall now try to explain the effect in terms of atomic behaviour, seeing how individual atoms react to an electric ﬁeld, or even before that recalling what an atom looks like. It has a positively charged nucleus surrounded by an electron cloud. In the absence of an electric ﬁeld the statistical centres of positive and negative charges coincide. (This is actually true for a class of molecules as well.) When an electric ﬁeld is applied, there is a shift in the charge centres, particularly of the electrons. If this separation is δ, and the total charge is q, the molecule has an induced dipole moment, μ = qδ.

(10.6)

Let us now switch back to the macroscopic description and calculate the amount of charge appearing on the surface of the dielectric. If the centre of electron charge moves by an amount δ, then the total volume occupied by these electrons is Aδ, where A is the area. Denoting the number of molecules per unit volume by Nm and taking account of the fact that each molecule has a charge q, the total charge appearing in the volume Aδ is AδNm q, or simply Nm qδ per unit area—this is what we mean by surface charge density. It is interesting to notice that this polarized surface charge density (denoted previously by P, known also as induced polarization or simply polarization) is exactly equal to the amount of dipole moment per unit volume, which from eqn (10.6) is also Nm qδ, so we have obtained our ﬁrst relationship between the microscopic and macroscopic quantities, P = Nm μ.

(10.7)

Types of polarization For low electric ﬁelds, we may assume that the dipole moment is proportional to the local electric ﬁeld, E ′ : μ = αE ′ .

227

α is a constant called the polarizability.

(10.8)

Notice that the presence of dipoles increases the local ﬁeld (Fig. 10.2), which will thus always be larger than the applied electric ﬁeld. _ +

10.4 Types of polarization Electronic All materials consist of ions surrounded by electron clouds. As electrons are very light, they have a rapid response to ﬁeld changes; they may even follow the ﬁeld at optical frequencies. Molecular Bonds between atoms are stretched by applied electric ﬁelds when the lattice ions are charged. This is easily visualized with an alkali halide crystal (Fig. 10.3), where small deformations of the ionic bond will occur when a ﬁeld is applied, increasing the dipole moment of the lattice. Orientational This occurs in liquids or gases when whole molecules, having a permanent or induced dipole moment, move into line with the applied ﬁeld. You might wonder why in a weak static ﬁeld all the molecules do not eventually align just as a weather vane languidly follows the direction of a gentle breeze. If they did, that would be the lowest energy state for the system, but we know from Boltzmann statistics that in thermal equilibrium the number of molecules with an energy E is proportional to exp(–E/kT); so at any ﬁnite temperature other orientations will also be present. Physically, we may consider the dipole moments as trying to line up but, jostled by their thermal motion, not all of them succeed. Since the energy of a dipole in an electric ﬁeld, E is (Fig. 10.4) E = –μE cos θ ,

Fig. 10.2 Presence of an electric dipole increases the local electric ﬁeld. Cl

–

Na +

Fig. 10.3 The inter-atomic bond in NaCl is caused by Coulomb attraction. An external electric ﬁeld will change the separation, thus changing the dipole moment.

(10.9)

the number of dipoles in a solid angle, d , is

A exp

μE cos θ kT

2π sin θ dθ .

(10.10)

A is a constant.

E θ + π

–

–μ

θ

Fig. 10.4 Energy of a dipole in an electric ﬁeld.

228

Dielectric materials Hence, the average dipole moment is given as net moment of the assembly total number of dipoles π μE cos θ (μ cos θ )2π sin θ dθ 0 A exp kT = . π μE cos θ A exp 2π sin θ dθ 0 kT

μ =

(10.11)

Equation (10.11) turns out to be integrable, yielding μ 1 = L(a) = coth a – . μ a

a = (μE /kT), and L(a) is called the Langevin function.

(10.12)

If a is small, which is true under quite wide conditions, eqn (10.12) may be approximated by μ = ∗ The

complex dielectric constant used by electrical engineers is invariably in the form ǫ = ǫ0 (ǫ′ – jǫ ′′ ). We found a different sign because we had adopted the physicists’ time variation, exp(–iωt).

The loss tangent is deﬁned as tan δ ≡ ǫ ′′ /ǫ ′ . (a)

μ2 E . 3kT

(10.13)

That is, the polarizability is inversely proportional to the absolute temperature.

10.5

The complex dielectric constant and the refractive index

In engineering practice the dielectric constant is often divided up into real and imaginary parts. This can be derived from Maxwell’s equations by rewriting the current term in the following manner: J – iωǫE = σ E – iωǫE σ E, = –iω ǫ + i ω

(b)

(10.14)

where the term in the bracket is called the complex dielectric constant. The usual notation is∗ ε = ε′ ε0 ,

σ = ε′′ ε0 , ω

and

tan δ =

ε′′ . ε′

(10.15)

The refractive index is deﬁned as the ratio of the velocity of light in a vacuum to that in the material, n1

n2

n1

n2

n1

n2

Fig. 10.5 Quarter wavelength layers used to make dielectric mirrors. † This is actually not true for a new set of

artiﬁcial materials called metamaterials, which can have effective permeabilities well above unity even in the infrared optical region (see Chapter 15).

c ν √ √ = ǫr μr = ǫ ′ ,

n=

(10.16)

since μr = 1 in all known natural materials that transmit light.† Conventionally, we talk of ‘dielectric constant’ (or permittivity) for the lower frequencies in the electromagnetic spectrum and of refractive index for light. Equation (10.16) shows that they are the same thing—a measure of the polarizability of a material in an alternating electric ﬁeld. A fairly recent and important application of dielectrics to optics has been that of multiply reﬂecting thin ﬁlms. Consider the layered structure represented in Fig. 10.5 with alternate layers of transparent material having refractive

Frequency response

229

indices n1 and n2 respectively. At each interface there will be some light reﬂected and some transmitted. The reﬂection coefﬁcient, from electromagnetic theory, at an interface like (a) in Fig. 10.5 is ra =

n2 – n1 . n2 + n1

(10.17)

By symmetry, the reﬂection coefﬁcient at (b) will be the reverse of this, rb =

n1 – n2 = –ra . n1 + n2

(10.18)

Now suppose that all the layers are a quarter wavelength thick—their actual thickness will be n1 (λ/4) and n2 (λ/4) respectively. Then the wave reﬂected back from (b) will be π radians out of phase with the wave reﬂected back from (a) because of its extra path length, and another π radians because of the phase difference in eqn (10.18). So the two reﬂected waves are 2π radians different; that is, they add up in phase. A large number of these layers, often as many as 17, makes an excellent mirror. In fact, provided good dielectrics (ones with low losses, that is), are used, an overall reﬂection coefﬁcient of 99.5% is possible, whereas the best metallic mirror is about 97–98% reﬂecting. This great reduction in losses with dielectric mirrors has made their use with low-gain gas lasers almost universal. I shall return to this topic when discussing lasers. Another application of this principle occurs when the layer thickness is one half wavelength. Successive reﬂections then cancel, and we have a reﬂectionless or ‘bloomed’ coating, much used for the lenses of microscopes and binoculars. A simpler form of ‘blooming’ uses only one intermediate layer on the glass surface (Fig. 10.6) chosen so that n1 =

√

n2 .

The two reﬂections have a phase difference of π radians. λ/4

Air

(10.19) Glass refractive index n2

The layer of the material of refractive index n1 is this time one quarter wavelength, as can be seen by applying eqn (10.17).

10.6 Frequency response Most materials are polarizable in several different ways. As each type has a different frequency of response, the dielectric constant will vary with frequency in a complicated manner; for example at the highest frequencies (light waves) only the electronic polarization will ‘keep up’ with the applied ﬁeld. Thus, we may measure the electronic contribution to the dielectric constant by measuring the refractive index at optical frequencies. An important dielectric, water has a dielectric constant of about 80 at radio frequencies, but its refractive index is 1.3, not (80)1/2 . Hence we may conclude that the electronic contribution is about 1.7, and the rest is probably due to the orientational polarizability of the H2 O molecule. The general behaviour is shown in Fig. 10.7. At every frequency where ǫ ′ varies rapidly, there tends to be a peak of the ǫ ′′ curve. In some cases this is analogous to the maximum losses that occur at resonance in a tuned circuit: the molecules have a natural resonant frequency because of their binding in

Blooming layer, refractive index

Fig. 10.6 Simple coating for a ‘bloomed’ lens.

230

Dielectric materials

S

Radio

Microwave

Visible

f

Fig. 10.7 Typical variation of ǫ ′ and ǫ ′′ with frequency.

f

the crystal, and they will transfer maximum energy from an electromagnetic wave at this frequency. Another case is the ‘viscous lag’ occurring between the ﬁeld and the polarized charge which is described by the Debye equations, which we shall presently consider. A consequence of all this is that materials that transmit light often absorb strongly in the ultraviolet and infrared regions, for example most forms of glass. Radio reception indoors is comparatively easy because (dry) bricks transmit wireless waves but absorb light; we can listen in privacy. The Earth’s atmosphere is a most interesting dielectric. Of the fairly complete spectrum radiated by the Sun, not many spectral bands reach the Earth. Below 108 Hz the ionosphere absorbs or reﬂects; between 1010 and 1014 Hz there is molecular resonance absorption in H2 O, CO2 , O2 , and N2 ; above 1015 Hz there is a very high scattering rate by molecules and dust particles. The visible light region (about 1014 –1015 Hz) has, of course, been of greatest importance to the evolution of life on Earth. One wonders what we would all be like if there had been just a little more dust around, and we had had to rely on the 108 –1010 Hz atmosphere window for our vision.

10.7

Anomalous dispersion

As shown in Fig. 10.7, there are wide frequency ranges within which ε′ remains constant, but in the vicinity of certain resonances the change is very fast; the dielectric constant declines as a function of frequency. This was already known in the nineteenth century. They called it anomalous dispersion. What is anomalous about it? Well, let’s look at the group velocity. It was deﬁned in eqn (2.26) for electron waves but of course the deﬁnition applies to all kind of waves. It is

vg =

dω , dk

(10.20)

Polar and non-polar materials which is also the velocity with which energy and information travel. Let us relate it to the variation of the refractive index, k c –k dk dn d(c/v) d = , (10.21) = =c + dω dω dω ω ω ω dω whence dω c = . dk n + ω(dn/dω)

(10.22)

What is anomalous is that the group velocity may be negative provided the refractive index varies fast enough with frequency. The phase velocity ω/k is positive, so we have a situation where the phase and group velocities are in opposite directions. The waves in this situation are called backward waves. Phase travels in one direction and energy in the other direction. Is that a very anomalous situation? Not really. One example of a backward wave will appear later in the present chapter when we discuss the optical branch of acoustic waves. Admittedly there are not many types around, but it is mostly a question of getting used to them. Familiarity breeds comprehension.

10.8 Polar and non-polar materials This is a distinction that is often made for semiconductors as well as dielectrics. A non-polar material is one with no permanent dipoles. For example, Si, Ge, and C (diamond) are non-polar. The somewhat analogous III–V compounds, such as GaAs, InSb, and GaP, share their valency electrons, so that the ions forming the lattice tend to be positive (group V) or negative (group III). Hence, the lattice is a mass of permanent dipoles, whose moment changes when a ﬁeld is applied. As well as these ionic bonded materials, there are two other broad classes of polar materials. There are compounds, such as the hydrocarbons (C6 H6 and parafﬁns) that have permanent dipole arrangements but still have a net dipole moment of zero (one can see this very easily for the benzene ring). Then there are molecules such as water and many transformer oils that have permanent dipole moments, and the total dipole moment is determined by their orientational polarizability. A characteristic of non-polar materials is that, as all the polarization is electronic, the refractive index at optical wavelengths is approximately equal to the square root of the relative dielectric constant at low frequencies. This behaviour is illustrated in Table 10.1. From Table 10.1 (more comprehensive optics data would show the same trend) you can see that most transparent dielectrics, polar or not, have a refractive index of around 1.4–1.6; only extreme materials like liquid hydrogen, diamond, and rutile (in our list) show appreciable deviation. Let us look for an explanation of this remarkable coalescence of a physical property; starting with our favourite (simplest) model of a solid, the cubic lattice of Fig. 1.1, with a lattice spacing a. Suppose the atoms are closely packed, each having a radius r, so that a = 2r.

(10.23)

231

232

Dielectric materials Table 10.1 Dielectric constant and refractive index of some non-polar, weakly polor, polar, and semiconducting materials Material

Gaussian sphere of radius d

Envelope perturbed by ﬁeld, centre C –

C– d C

Envelope of electron cloud about centre C

Fig. 10.8 Displacement of electron cloud about an atom centred on C by a distance d, by an applied electric ﬁeld.

Non-polar C (diamond) H2 (liquid) Weakly polar polythene ptfe (poly-tetra ﬂuoro-ethylene) CCl4 (carbontetrachloride) Parafﬁn Polar NaCl (rocksalt) TiO2 (rutile) SiO2 (quartz) Al2 O3 (ceramic) Al2 O3 (ruby) Sodium carbonate Ethanol Methanol Acetone Soda glass Water Semiconductors Si GaAs GaP InSb

Refractive index

(Refractive index)2

Dielectric constant measured at 103 Hz

2.38 1.11

5.66 1.232

5.68 1.23

1.51 1.37

2.28 1.89

2.30 2.10

1.46

2.13

2.24

1.48

2.19

2.20

1.52 2.61 1.46 1.66 1.77 1.53 1.36 1.33 1.357 1.52 1.33

2.25 6.8 2.13 2.77 3.13 2.36 1.85 1.76 1.84 2.30 1.77

5.90 94.0 3.80 6.5 4.31 8.4 24.30 32.63 20.7 7.60 80.4

3.42 3.3 3.2 3.96

11.70 10.89 15.68 15.68

11.9 13.2 17.7 17.7

For an optical property we need to consider only electronic polarizability as ionic, and molecular responses are too slow. Let us suppose that each atomic volume, (4/3)π r3 is uniformly occupied by the total electronic charge, Ze. When an electric ﬁeld, E , is applied, the centre of charge of the electronic cloud shifts a distance d to C – from the nucleus at C (Fig. 10.8). To ﬁnd the restoring force attracting the electrons back towards the nucleus, we can construct a Gaussian surface of radius d about C – , so that C is just excluded. The negative charge inside the Gaussian sphere is, according to the uniform charge approximation, equal to Ze(d/r)3 . So the attractive force, F, towards the nucleus is F=

(Ze)2 d . 4π ǫ0 r3

(10.24)

This must be balanced by the ﬁeld force causing the charge displacement, F = ZeE .

(10.25)

The Debye equation

233

(10.26)

The LHS is the quantity deﬁned as the dipole moment, μ, in eqn (10.6).

So by eqns (10.24) and (10.25), Zed = 4π r3 ǫ0 E . By Ze = q and μ = qd, hence eqn (10.26) may also be written as μ = 4π r3 ǫ0 E

(10.27)

We can now return to eqn (10.7), P = Nm μ, to ﬁnd the induced polarization. The density of atoms per unit volume is Nm =

1 1 = , 3 a (2r)3

(10.28)

leading to P=

π 1 4π r3 ǫ0 E = ǫ0 E . 2 (2r)3

(10.29)

From eqns (10.4) and (10.5) it follows then that χ=

P π = , ǫ0 E 2

(10.30)

whence ~ 2.57, ǫr = 1 + χ =

(10.31)

and n=

√ ~ ǫr = 1.6.

(10.32)

Thus, our very approximate estimate is at the high end of our small sample in Table 10.1. We could reﬁne this model to give a different ﬁt by remarking that less close packing would give N m m2

(2b/m1)1/2

Acoustical branch

Fig. 10.12 / 2a

k

Dispersion curves showing both the acoustical and optical branches of a diatomic lattice.

238

Dielectric materials

∗ Note

that in the presence of absorption the frequency of maximum reﬂection, fr , need not coincide with that of minimum transmission, ft .

Table 10.2 Frequencies of maximum reﬂection (fr ) and minimum transmission (ft ) for a number of alkali halides Crystal

fr (THz)

ft (THz)

NaF TlF NaCl KCl RbCl TlCl KBr KI

7.39 4.44 4.90 4.24 3.54 2.56 3.40 2.94

8.38 6.17 5.76 4.73 4.06 3.26 3.68 3.19

single-element case. There is, however, an upper branch, known as the optical branch. The values of ω at the points k = 0 and π /2a can be obtained from eqn (10.55), and may be seen in Fig. 10.12. The upper branch represents a backward wave. Phase and group velocities are in opposite directions. The highest point in the dispersion curve is at k = 0. The corresponding wavelength is typically tens of micrometres in the middle of the THz region. An interesting effect discovered in the 1920s (known as the Reststrahl effect, or sometimes as residual radiation) is that these lattice vibrations may interact with electromagnetic waves. The effect is manifested in large absorption at one wavelength and in large reﬂection at a slightly different wavelength.∗ The corresponding values are given in Table 10.2 for a few materials. The fact that signiﬁcant reﬂection occurs only within a narrow band has been used to provide monochromatic sources. Another remarkable property of the optical branch is that it can provide, within a certain frequency range, a negative effective dielectric constant. This is quite a rare phenomenon. We have come across it only once before, in Chapter 1, when discussing the critical frequency of transparency of metals, as part of the theory of plasmas. In order to discuss the interaction with electromagnetic waves we shall use a model which is less general in one sense, in that it is valid only in the vicinity of k = 0, but is more general in another sense. We shall assume that the restoring force is electrical. To simplify the mathematics we shall not consider two separate atoms but shall write the equation of motion for a single atom which has a charge e and a reduced mass given by 1 1 1 = + . m∗ m1 m2 The equation of motion may then be written as e d2 xT 2 E, + ω x = – T T m∗ dt2

† Its

physical meaning is that the current ﬂowing out of an element dx can be different from the current ﬂowing in, provided the charge density within that interval has increased or decreased.

(10.56)

(10.57)

where xT is the displacement relative to the centre of gravity of the two atoms, and ω2T is a restoring force. Up to now the two different atoms could be of any kind, provided they make up a solid. A look at Table 10.2 will reveal that all those materials have ionic bonds so we may legitimately assume that one of the atoms has a positive charge and the other one has a negative charge. We are interested in what happens in the infrared region. Whatever happens can be regarded as a small perturbation of the stationary state. We may assume that the density of atoms will have a component, n1 , that varies at a frequency, ω, in the infrared range. Hence the total density may be written as No + n1 exp(–iωt), where No is the unperturbed density and nI ≪ NI . The continuity equation† is then dnI e dt

+

dJI = 0, dx

(10.58)

Acoustic waves

239

where JI is the time-varying ionic current density, equal to JI = eNo νT

with νT =

dxT . dt

(10.59)

One further equation needed is Poisson’s equation, which relates the electric ﬁeld to the net charge density, ε∞

dE = –enI . dx

(10.60)

With our usual wave assumption exp[–i(ωt–kx)] we ﬁnd, after a certain amount of algebra, JI = σ E,

(10.61)

where σ =

iωε∞ ωI2 ωT2

– ω2

and

e2 NI . m∗ ε∞

ωI2 =

(10.62)

The effective permittivity due to lattice wave interaction with electromagnetic waves may be worked out from the relationship JI – iωε∞ E = (σ – iωε∞ )E = –iωεeff E,

(10.63)

whence εeff = ε∞ –

ε∞ (ω2 – ωT2 – ωI2 ) σ . = iω ω2 – ωT2

(10.64)

The usual notation is ωL2 = ωT2 + ωI2 ,

(10.65)

and in the usual terminology ωL is the longitudinal optical phonon frequency and ωT is the transverse optical phonon frequency; these are related to each other by ε∞ ωT2 . ωL2 = (10.66) εs The ﬁnal form for the effective dielectric constant is then εeff =

ε∞ (ω2 – ωL2 ) ω2 – ωT2

.

(10.67)

It may now be seen that the effective dielectric constant is negative in the range ωT < ω < ωL .

(10.68)

Optical phonons∗ have been of only moderate interest in the past. This might change in view of the advent of the new subject of metamaterials. In fact, in Section 15.9 (see Chapter 15) we shall be greatly interested in negative material parameters such as negative permittivity and negative permeability. In that section we shall discuss a device in which a negative dielectric constant due to the mechanism discussed above is used in a novel type of microscope.

∗ This

is a classical phenomenon which should be described as the optical branch of acoustic waves. Alas, the quantummechanical term has now been widely accepted.

240

Dielectric materials

10.12 There are three main mechanisms that are usually blamed for dielectric breakdown: (1) intrinsic, (2) thermal, and (3) discharge breakdown.

I

Electric breakdown is a subject to which it is difﬁcult to apply our usual scientiﬁc rigour. A well-designed insulator (in the laboratory) breaks down in service if the wind changes direction or if a fog descends. An oil-ﬁlled highvoltage condenser will have bad performance, irrespective of the oil used, if there is 0.01% of water present. The presence of grease, dirt, and moisture is the dominant factor in most insulator design. The ﬂowing shapes of highvoltage transmission line insulators are not entirely due to the fact that the ceramic insulator ﬁrms previously made chamberpots; the shapes also reduce the probability of surface tracking. The onset of dielectric breakdown is an important economic as well as technical limit in capacitor design. Generally, one wishes to make capacitors with a maximum amount of stored energy. Since the energy stored per unit volume is 21 ǫE 2 , the capacitor designers value high breakdown strength even more than high dielectric constant. In general, breakdown is manifested by a sudden increase in current when the voltage exceeds a critical value Ub , as shown in Fig. 10.13. Below Ub there is a small current due to the few free electrons that must be in the conduction band at ﬁnite temperature. When breakdown occurs it does so very quickly, typically in 10–8 s in a solid.

10.12.1 Ub

U

Fig. 10.13 Current voltage characteristics for an insulator. The current increases very rapidly at the breakdown voltage, Ub .

Dielectric breakdown

Intrinsic breakdown

When the few electrons present are sufﬁciently accelerated (and lattice collisions are unable to absorb the energy) by the electric ﬁeld, they can ionize lattice atoms. The minimum requirement for this is that they give to the bound (valence) electron enough energy to excite it across the energy gap of the material. This is, in fact, the same effect that we mentioned before in connection with avalanche diodes.

10.12.2

Thermal breakdown

This occurs when the operating or test conditions heat the lattice. For example, an a.c. test on a material in the region of its relaxation frequency, where ǫ ′′ is large would cause heating by the lossy dipole interaction rather than by accelerating free electrons. The heated lattice ions could then be more easily ionized by free electrons, and hence the breakdown ﬁeld could be less than the intrinsic breakdown ﬁeld measured with d.c. voltages. The typical polymer, polyethylene, has a breakdown ﬁeld of 3 to 5 × 108 V m–1 for very low frequencies, but this falls to about 5 × 106 V m–1 around 106 Hz, where a molecular relaxation frequency occurs. Ceramics such as steatite and alumina exhibit similar effects. If it were not for dielectric heating effects, breakdown ﬁelds would be lower at high frequencies simply because the free electrons have only half a period to be accelerated in one direction. I mentioned that a typical breakdown time was 10–8 s; so we might suppose that at frequencies above 108 Hz breakdown would be somewhat inhibited. This is true, but a fast electron striking a lattice ion still has a greater speed after collision than a slow one, and some of these fast electrons will be further accelerated by the ﬁeld. Thus, quite spectacular breakdown may sometimes occur at microwave frequencies (1010 Hz) when

Piezoelectricity, pyroelectricity, and ferroelectricity

241

high power densities are passed through the ceramic windows of klystrons or magnetrons. Recent work with high-power lasers has shown that dielectric breakdown still occurs at optical frequencies. In fact the maximum power available from a solid-state laser is about 1012 W from a series of cascaded neodymium glass ampliﬁer lasers. The reason why further ampliﬁcation is not possible is that the optical ﬁeld strength disrupts the glass laser material.

10.12.3 Discharge breakdown In materials such as mica or porous ceramics, where there is occluded gas, the gas often ionizes before the solid breaks down. The gas ions can cause surface damage, which accelerates breakdown. This shows up as intermittent sparking and then breakdown as the test ﬁeld is increased.

10.13

Piezoelectricity, pyroelectricity, and ferroelectricity

These are three classes of dielectrics, each having some interesting properties arising from their crystal structure. Their names come from Greek and Latin. Piezo means to press, pyr means ﬁre, and ferrum means iron. Unfortunately, ferroelectricity is a misnomer. It has nothing to do with iron. It got its name from the similarity of its properties to ferromagnetism. Piezoeloectricity is the widest class. Next come pyroelectrics and then ferroelectrics. Their interrelationship is shown in Fig. 10.14 in a Venn diagram. All ferroelectrics are pyroelectrics, and all pyroelectrics are piezoelectric. What is the difference between them? Very roughly: ferroelectrics have permanent dipole moments, pyroelectrics are sensitive to heat, and all of them are sensitive to mechanical displacement. The one that has been known about the longest is pyroelectricity; it was found in tourmaline, a natural crystal. Its property to attract bits of straw and wood was noted by Theophrates some 25 centuries ago. Piezoelectricity was discovered by Pierre and Jacques Curie in the 1880s whereas ferroelectricity is hardly a century old, discovered by Valasek in the 1920s.

10.13.1 Piezoelectricity Let us start with the piezoelectric effect. This is easy to describe in a few words: a mechanical strain will produce dielectric polarization and, conversely, an applied electric ﬁeld will cause mechanical strain. Which crystals will exhibit this effect? Experts say that out of the 21 classes of crystals that lack a centre

Piezoelectrics

Pyroelectrics

Ferroelectrics

Fig. 10.14 Relation between the piezoelectric, pyroelectric, and ferroelectric materials.

242

Dielectric materials (a) –

+

–

+

–

+

–

+

–

(b)

+

+

+

+ (c) Applied force +

+

+

+ Applied force

(d) Applied force –

–

–

–

of symmetry 20 are piezoelectric. Obviously we cannot go into the details of all these crystal structures here, but one can produce a simple argument showing that lack of a centre of symmetry is a necessary condition. Take for example the symmetric cubic structure shown in Fig. 10.15(a). The positive atoms are on the corner of a square highlighted on Fig. 10.15(b). When a tensile stress is applied in the vertical direction the lattice is distorted, and the square has turned into a rhombus as shown in Fig. 10.15(c), leaving the centre of charge unchanged for positive charge. The same is true for negative charge, as shown in Fig. 10.15(d). Consequently, the centre of positive charge still coincides with the centre of negative charge. The dimensions have changed but no electric dipole moment has been created. Let us now take a crystal that lacks a centre of symmetry. Both the positive and negative charges occupy the corners of equilateral triangles. In its unstressed form the centre of positive charge coincides with the centre of negative charge as shown in Fig. 10.16(a), and also in Fig. 10.16(b) where the positive charges are highlighted and the construction for ﬁnding the centre of positive charge is shown. There is no electric dipole moment (it is not ferroelectric). Let us next apply a tensile stress in the vertical direction (see Fig. 10.16(c)) similarly to that applied previously to the cubic structure. The centre of positive charge has moved downwards. However, for negative charges (Fig. 10.16(d)) we can see that the centre of negative charge moved upwards. If one moved downwards, and the other one upwards then clearly the centres of positive and negative charges no longer coincide. A dipole moment has been created which points downwards. This is what happens in one unit cell. Summarizing the effect for all unit cells, mobile negative charge will move upwards. The top surface will be negatively charged and there will be positive charge on the bottom surface. If we apply a tensile stress in the horizontal direction we can show by similar argument that the centre of charge of the positive atoms moves upwards and that of the negative charges, downwards. The induced dipole moment points upwards, and now the top surface will be positive and the bottom surface negative. For small deformations and small electric ﬁelds the relationships are linear. The original relationship between dielectric displacement and electric ﬁeld D = εE modiﬁes now to

– Applied force

Fig. 10.15 Schematic representation of a centro-symmetric crystal: (a) and (b) in the absence of applied stress, and (c) and (d) in the presence of applied stress.

D = εE + eS,

(10.69)

where e is the piezoelectric constant. Similarly, Hooke’s law, T = cS (T is stress, c is the elastic constant, and S is strain) modiﬁes to T = cS – εE .

(10.70)

In general the piezoelectric constant is a tensor relating the various mechanical and electrical components to each other. In practical applications, however, one usually relies on a single element in the tensor, which, for a number of piezoelectric materials, is given in Table 10.3. It may be worth noting again that when E = 0, the dielectric displacement, D, may be ﬁnite in spite of the electric ﬁeld being zero and similarly, an electric ﬁeld sets up a strain without a mechanical stress being applied.

Piezoelectricity, pyroelectricity, and ferroelectricity It follows from the properties of piezoelectrics that they are ideally suited to play the role of electromechanical transducers. Common examples are the microphone, where longitudinal sound vibrations in the air are the mechanical driving force, and the gramophone pick-up, which converts into electrical signals the mechanical wobbles in the groove of a record—for these applications Rochelle salt has been used. More recently, ceramics of the barium titanate type, particularly lead titanate, are ﬁnding application. They have greater chemical stability than Rochelle salt but suffer from larger temperature variations. A very important application of piezoelectricity is the quartz (SiO2 ) stabilized oscillator, used to keep radio stations on the right wavelength, with an accuracy of about one part in 108 or even 109 . The principle of operation is very simple. A cuboid of quartz (or any other material for that matter) will have a series of mechanical resonant frequencies of vibration whenever its mechanical length, L, is an odd number of half wavelengths. Thus, the lowest mode will be when L = λ/2. The mechanical disturbance will travel in the crystal with the velocity of sound, which we shall call νs . Hence, the frequency of mechanical oscillation will be f = νs /λ = νs /2L. If the ends of the crystal are metallized, it forms a capacitor that can be put in a resonant electrical circuit, having the same resonant frequency, f . The resonant frequency of a transistor oscillator circuit depends a little on things outside the inductor and capacitor of the resonant circuit. Usually these are small effects that can be ignored, but if you want an oscillator that is stable in frequency to one part in 108 , things like gain variation in the ampliﬁer caused by supply voltage changes or ageing of components become important; on this scale they are virtually uncontrollable. This is where the mechanical oscillation comes in. We have seen it is a function only of the crystal dimension. Provided the electrical frequency is nearly the same, the electrical circuit will set up mechanical as well as electrical oscillations, linked by the piezoelectric behaviour of quartz. The mechanical oscillations will dominate the frequency that the whole system takes up, simply because the ampliﬁer part of the oscillator circuit works over a ﬁnite band of

243

+ –

–

+

+ –

(a)

+

+

+ (b)

Applied force +

+

+

(c) Applied force

Applied force –

–

Table 10.3 Piezoelectric ceramics Material

Quartz, SiO2 Barium titanate, BaTiO3 Lead zirconate titanate, PZT PZT igniter Potassium sodium niobate, KNa(NbO3 )2 Lithium niobate

Density (g cm–3 )

Relative permittivity

2.65 5.7

4.6 1700

7.5

Loss, tan δ (%)

Curie temperature Tc (◦ C)

Piezoelectric constant (pC N–1 )

0.5

115

2.25 190

1750

6

265

292

7.6 4.5

800 400

16 25

285 400

384 100

4.64

78

210

80

(d)

– Applied force

Fig. 10.16 Schematic representation of a non-centro-symmetric crystal: (a) and (b) in the absence of applied stress, and (c) and (d) in the presence of applied stress.

244

Dielectric materials Applied drift ﬁeld voltage V0

CdS Output signal

Input

Fig. 10.17 General arrangement of an acoustic ampliﬁer. The applied electric ﬁeld causes the electrons (photoelectrically generated by the light) to interact with the acoustic wave in the crystal.

Quartz-controlled master oscillators, followed by stages of power ampliﬁcation, are used in all radio and television transmitters, from the most sophisticated, down to the humblest ‘ham’.

Gain (db)

V0

0 B

vs

Fig. 10.18 The gain of an acoustic ampliﬁer as a function of the applied voltage. At the voltage where the electron drift velocity is equal to the sound velocity (νs ) the gain changes from negative to positive.

Transducer Light

frequencies that is greater than the frequency band over which the mechanical oscillations can be driven. A circuit engineer would say that the ‘Q’ of the mechanical circuit is greater than that of the electrical circuit. The only problem in stabilizing the frequency of the quartz crystal-controlled oscillator is to keep its mechanical dimension, L, constant. This of course, changes with temperature, so we just have to put the crystal in a thermostatically controlled box. This also allows for slight adjustment to the controlled frequency by changing the thermostat setting by a few degrees. The reverse effect is used in earphones and in a variety of transducers used to launch vibrations in liquids. These include the ‘echo-sounder’ used in underwater detection and ultrasonic washing and cleaning plants. I should like to discuss in a little more detail another application in which a piezoelectric material, cadmium sulphide (CdS), is used. The basic set-up is shown in Fig. 10.17. An input electric signal is transformed by an electromechanical transducer into acoustic vibrations that are propagated through the crystal and are converted back into electric signals by the second transducer. Assuming for simplicity that the transducers are perfect (convert all the electric energy into acoustic energy) and the acoustic wave suffers no losses, the gain of the device is unity (0 db if measured in decibels). If the crystal is illuminated, that is mobile charge carriers are created, the measured gain is found to decrease to B (Fig. 10.18). If further a variable d.c. voltage is applied across the CdS crystal, the gain varies as shown. These experimental results may be explained in the following way. The input light creates charge carriers that interact with the acoustic waves via the piezoelectric effect. If the carriers move slower than the acoustic wave, there is a transfer of power from the acoustic wave to the charge carriers. If, on the other hand, the charge carriers move faster than the acoustic wave, the power transfer takes place from the carriers to the acoustic wave, or in other words the acoustic wave is ampliﬁed. Hence, there is the possibility of building an electric ampliﬁer relying on the good services of the acoustic waves. Since we can make electric ampliﬁers without using acoustic waves, there is not much point using this acoustic ampliﬁer unless it has some other advantages. The main advantage is compactness. The wavelength of acoustic waves is smaller by ﬁve orders of magnitude

Piezoelectricity, pyroelectricity, and ferroelectricity

245

Load

Input

Surface wave L Piezoelectric substrate

than that of electromagnetic waves, and this makes the acoustic ampliﬁer much shorter than the equivalent electromagnetic travelling wave ampliﬁer (the travelling wave tube). It is unlikely that this advantage will prove very important in practical applications, but one can certainly regard the invention of the acoustic ampliﬁer as a signiﬁcant step for the following two reasons: (i) it is useful when acoustic waves need to be ampliﬁed, and (ii) it has created a feeling (or rather expectation) that whatever electromagnetic waves can do, acoustic waves can do too. So it stimulates the engineers’ brains in he search for new devices, and a host of new devices may one day appear. Other waves we are familiar with are those formed on the surface of disturbed liquids, when for example we throw a pebble into a lake. It was shown a long time ago by Lord Rayleigh that analogous waves rippled across the surface of solids, travelling with a velocity near to the velocity of sound in the bulk material. Devices based on these waves are known as SAW (surface acoustic wave) devices. Why do we want to use surface waves? There are two reasons: (1) they are there on the surface so we can easily interfere with them, and (2) the interfering structures may be produced by the same techniques as those used for integrated circuits. Why do we want to interfere with the waves? Because these devices are used for signal processing which, broadly speaking, requires that the signal which arrives during a certain time interval at the input should be available some time later in some other form at the output. Let us ﬁrst discuss the simplest of these devices which will produce the same waveform at the output with a certain delay. The need for such a device is obvious. We want to compare a signal with another one, which is going to arrive a bit later. A schematic drawing of the device is shown in Fig. 10.19. The electric signal is transformed by the input transducers into an acoustic one, which travels slowly to the output transducer, where it is duly reconverted into an electric signal again. The input and output transducers are so-called interdigital lines. The principles of this transducer’s operations may be explained with the aid of Fig. 10.20. The electric signal appearing simultaneously between ﬁngers 1 and 2, and 2 and 3 excites acoustic waves. These waves will add up in a certain phase depending on the distance d between the ﬁngers. If d is half a wavelength (wavelength and frequency are now related by the acoustic velocity) and considering that the electric signals are in opposite phase (one is plus–minus, the other one is minus–plus) then the effect from each ﬁnger pair adds up, and

Fig. 10.19 Schematic representation of a surface wave device with two interdigital transducers.

1

2

3

+

–

+

d

Fig. 10.20 A section of the interdigital transducer.

l

246

Dielectric materials we have maximum transmission. At twice the frequency, where d is a whole wavelength, the contribution from neighbouring ﬁnger pairs will be opposite, and the transducer will produce no net acoustic wave. This shows that the delay line cannot be a very broad-band device, but it shows in addition that by having a frequency-dependent output, we might be able to build a ﬁlter. The parameters at our disposal are the length of overlap between ﬁngers (l on Fig. 10.20) and the relative position of the ﬁngers, the former controlling the strength of coupling and the latter the relative phase. It turns out that excellent ﬁlters can be produced which are sturdy, cheap, and better than anything else available in the MHz region. In the stone-age days of radio, when we were younger, such a band-pass ﬁlter was accomplished by a series of transformers tuned by capacitors. These would appear ridiculously bulky compared to today’s microelectronic ampliﬁers, so a SAW band-pass ﬁlter on a small chip of piezoelectric ceramic with photoengraved transducers is compatible in bulk and in technology with integrated circuits, and much cheaper than the old hardware. One of the applications is in television sets. What else can one do with SAW devices? One of the applications is quite a fundamental one related to signal processing. The problem to be solved is posed as follows. If a signal with a known waveform and a lot of noise arrives at the input of a receiver, how can one improve the chances of detecting the signal? The answer is that a device exists which will so transform the signal as to make it optimally distinguishable from noise. The device is called, rather inappropriately, a matched ﬁlter. It turns out that SAW devices are particularly suitable for their realization. They are vital parts of certain radar systems. We cannot resist mentioning one more application that will soon appear on the market: a device that monitors the pressure of car tyres while on the road. The heart of the device is a SAW resonator inserted into the tyre. The useful information is contained in its resonant frequency which is pressure dependent. The resonator is interrogated by a pulse from the transmitter attached to the wheel arch. It re-radiates at its resonant frequency providing the pressure information that is then displayed on the instrument panel. I shall ﬁnish this section by mentioning electrostriction, a close relative of piezoelectricity. It is also concerned with mechanical deformation caused by an applied electric ﬁeld, but it is not a linear phenomenon. The mechanical deformation is proportional to the square of the electric ﬁeld, and the relationship applies to all crystals whether symmetric or not. It has no inverse effect. The mechanical strain does not produce an electric ﬁeld via electrostriction. Biased electrostriction is, however, very similar to piezoelectricity. If we apply a large d.c. electric ﬁeld E0 , and a small a.c. electric ﬁeld, E1 , then the relationship is

γ is a proportionality factor.

~ γ E 2 + 2γ E0 E1 , S = γ (E0 + E1 )2 = 0

(10.71)

and we ﬁnd that the a.c. strain is linearly proportional to the amplitude of the a.c. ﬁeld. We would like to conclude this section, following our sophisticated account of signal processing, with a more down-to-earth application of piezoelectrics that most of us use in our homes. This is the gas igniter. The piezoelectric most often used is called PZT, a composite ceramic of lead titanate and zirconate.

Piezoelectricity, pyroelectricity, and ferroelectricity Usually two ceramic cylinders are used to double the charge build-up and hence the voltage across the spark gap. The operating force must be applied quickly as the charge readily leaks away. The great virtue of PZT is a high piezoelectric constant, about 200 times greater than quartz, but it is a lossy dielectric, tan δ is about 10–2 . You press a spring, which is released to impact the ceramic so that a gas ﬂow in air is spark-ignited and your ﬁre or cooker heats up.

10.13.2 Pyroelectricity As mentioned before, pyroelectrics are a subclass of piezoelectrics. Of the 20 piezoelectric classes of crystals 10 are pyroelectric. The distinguishing feature of pyroelectrics is that they have a spontaneous dipole moment, PS . The property that makes them suitable for a variety of applications is the sensitivity of that dipole moment to heat. The pyroelectric coefﬁcient is deﬁned as p = ∂Ps /∂T. Its value is given for a number of materials in Table 10.4. Note the very wide range of values. It is easy to explain why the dipole moment is sensitive to heat. Spontaneous dipole moments are randomly orientated. The resulting electric ﬁelds are compensated by moving charges which charge up the surfaces. This is the situation under steady-state conditions. A voltmeter connected between the top and bottom surfaces of a pyroelectric crystal (Fig. 10.21(a)) would measure a certain voltage. Now change the temperature of the crystal. If it is heated the orientation of the charges will be more random, if it is cooled the randomness

Table 10.4 Pyroelectric coefﬁcients for various materials Material Ferroelectrics Poled ceramic BaTiO3 PbZr0.95 Ti0.05 O3 Crystal LiNbO3 LiTaO3 Pb5 Ge3 O11 Ba2 NaNb5 O15 Sr0.5 Ba0.5 Nb2 O6 (CH2 CF2 )n Trigycine sulphate Nonferroelectrics Crystal CdSe CdS ZnO Tourmaline Li2 SO4 . 2H2 O

Primary coefﬁcient

Secondary coefﬁcient

Total coefﬁcient

–260 –305.7

+60 +37.7

–200 –268

–95.8 –175 –110.5 –141.7 –502 –14 +60

+12.8 –1 +15.5 +41.7 –48 –13 –330

–83 –176 –95 –100 –550 –27 –270

–2.94 –3.0 –6.9 –0.48 +60.2

–0.56 –1.0 –2.5 –3.52 +26.1

–3.5 –4.0 –9.4 –4.0 +86.3

247

248

Dielectric materials (a) Crystal V

(b)

A

Fig. 10.21 (a) Voltmeter and (b) ammeter being used to measure the condition of a crystal. Perovskites

B O A

Fig. 10.22 ABO3 perovskite crystal structure.

declines. If the distribution is more random then there is less resultant surface charge and the voltmeter would show a smaller voltage. And of course conversely: less random distribution would result in a higher voltage. But what happens while the temperature changes? To monitor that let us replace our voltmeter by an ammeter (Fig. 10.21(b)) and measure current. The change of temperature causes a change in the randomness of the dipole moments, the change of randomness causes a change in surface charge, a change in surface charge causes a current to ﬂow, in one direction when the crystal is heated, in the other direction when the crystal is cooled. As the temperature rises, randomness increases until a temperature is reached at which there is a transition to full randomness. This happens at the Curie point and the transition is called a phase transition. The pyroelectric coefﬁcients are higher in the vicinity of the Curie point but are strongly dependent on ambient temperature. Therefore, typically, they are used well below the Curie point. There is a variety of crystal structures that give rise to the pyroelectric effect. The most common one is the perovskite structure, based on crystals with the general chemical formula ABO3 . One example is BaTiO3 , which is ferroelectric as well. The positions of the A, B, and O atoms are shown in Fig. 10.22. We need to mention here that pyroelectrics, being piezoelectrics as well, undergo a secondary effect when heated. Heat may cause thermal expansion and the subsequent change in dimension, due to the piezoelectric effect, will also cause an electric ﬁeld to appear. This changes the effective pyroelectric coefﬁcient (see Table 10.4) and might be responsible for electrical ‘noise’. The application that comes immediately to mind is use of the heat sensitivity of pyroelectrics for infrared detection and imaging. They have many advantages over detectors based on excitation of electrons across a bandgap. In particular: • • • • •

sensitivity over a wide spectral band sensitivity over a wider range of temperatures low power requirement fast response low cost.

Figure 10.23 shows a thermal image taken by a thin ﬁlm array of pyroelectric detectors. The image is clearly of a road. In the distance we can see people, and on the left a house. All are brighter because they are warmer.

10.13.3

Fig. 10.23 Thermal image from a pyroelectric camera from Lang S.B. ‘Pyroelectricity: from ancient curiosity to modern imaging tool’ (Physics Today 58 (8), 31 (2005)).

Ferroelectrics

As mentioned before all ferroelectrics are pyroelectrics; they both have spontaneous polarization. The difference between them is that the polarization of ferroelectrics can be reversed by applying an electric ﬁeld but that of pyroelectrics cannot be reversed. They would break down before the reversal could occur. Why were these new materials, that were discovered to have interesting properties, called ferroelectrics? Just a historical accident. Magnets preceded these new materials by a couple of thousand years. So when the new materials

Interaction of optical phonons with drifting electrons were discovered it was the similarity with ferromagnetics that was ﬁrst noticed. Ferromagnetics have a B–H loop (which will be tackled in much more detail in Sections 11.4–11.6), the new materials have a P–E loop. The former is magnetic, the latter is electric, so at the baptism ceremony, purely on the basis of this analogy, they called the new materials ferroelectric—and once you have a name it is difﬁcult to change it. Ferroelectrics typically have the perovskite structure, like BaTiO3 (shown in Fig. 10.22). The spontaneous polarization comes from the Ti atoms moving up or down. There are also domains (more about domains in Section 11.4 concerned with ferromagnetic materials) in ferroelectrics which have the same direction of spontaneous polarization. When we apply an electric ﬁeld the Ti atoms respond moving out of their position and thereby change the polarization. Above the Curie temperature ferroelectrics become ordinary dielectrics but with the advantage of having very high dielectric constants. That’s a property that can ﬁnd applications in cameras as a way of powering a ﬂash. The ferroelectric is in a capacitor charged up by a battery. High dielectric constant means high stored energy. When the capacitor is connected to a bulb it discharges, the high current creating a ﬂash. Hysteresis, means delay (from the Greek υστερησιζ, meaning delay), and in this context a delay in the appearance of polarization when the magnitude of the electric ﬁeld is varied. Figure 10.24 shows a hysteretic P–E curve. Let us start at a certain point P1 where there is spontaneous polarization in the absence of an electric ﬁeld. As the electric ﬁeld is increased the polarization increases to P2 . If we now reduce the electric ﬁeld the polarization will not retrace the curve at which it rose. It will now decline at a faster rate. It will reach P = 0 at a value of Ec of the electric ﬁeld, that is (another misnomer) called the coercive force. A further decrease in the electric ﬁeld causes the polarization to reverse. When the electric ﬁeld is zero the polarization is P3 . Increasing the electric ﬁeld in the opposite direction will lead to P4 . A decrease in this electric ﬁeld will lead to P = 0 at E = –Ec . A further decrease in the electric ﬁeld to zero where P = P1 will complete the loop. Ferroelectrics have often been considered for applications in the past (e.g. voltage tunable capacitors) but they have never achieved sustained success. This might change in the future due to improved materials. Their potential applications as memory elements will be discussed in Appendix VI.

10.14

Interaction of optical phonons with drifting electrons

In the previous section we discussed the acoustic ampliﬁer, in which acoustic waves could be ampliﬁed by interacting with drifting electrons. The remarkable thing is that there can be transfer of power from the electrons to the acoustic wave in spite of the presence of collisions. The question naturally arises of whether we could transfer power from electrons to the optical branch of the acoustic waves, i.e. produce an ampliﬁer for optical phonons. If we could do that then it would also be possible to build oscillators. Would it be an advantage to have such oscillators? The answer is very much so. Remember the range of the optical phonon resonances. They are all in the THz region—and that is a region of the electromagnetic spectrum that has hardly been explored. A cheap

249

p

p2

p1

−ec

ec −p1

−p2

Fig. 10.24 Ferroelectric hysteresis loop.

e

250

Dielectric materials THz source would lead to numerous applications in security, a consideration not irrelevant today. In order to have transfer of power from electrons to optical phonons, ﬁrst of all, we need electrons. In CdS, used in the acoustic ampliﬁer, they were obtained by optical excitation. That is certainly a possibility but there is no need for it. There are a number of II–VI (e.g. InSb) and III–V (e.g. GaAs) materials which display optical phonon resonances in the THz region (around 5.4 THz for the former and 9 THz for the latter) and happen to be semiconductors with the further advantage of high mobility. Will such oscillators come? There is a chance.

10.15

Optical ﬁbres

I have tried to show that dielectric properties have importance in optics as well as at the more conventional electrical engineering frequencies. That there are no sacred boundaries in the electromagnetic spectrum is shown very clearly by a fairly recent development in communications engineering. This involves the transmission (guiding) of electromagnetic waves. The principle of operation is very simple. The optical power remains inside the ﬁbre because the rays suffer total internal reﬂection at the boundaries. This could be done at any frequency, but dielectric waveguides have distinct advantages only in the region around µm wavelengths. The particular conﬁguration used is a ﬁbre of rather small diameter (say 5–50 µm) made of glass or silica. Whether this transmission line is practical or not will clearly depend on the attenuation. Have we got the formula for the attenuation of a dielectric waveguide? No, we have not performed that speciﬁc calculation, but we do have a formula for the propagation coefﬁcient of a plane wave in a lossy medium, and that gives a sufﬁciently good approximation. Recall eqn (1.38), k = (ω2 μǫ + iωμσ )1/2 ,

(10.72)

ωǫ ≫ σ ,

(10.73)

and assuming this time that

we get the attenuation coefﬁcient kimag

For optical communications to become feasible, A should not exceed 20 db km–1 , ﬁrst pointed out by Kao and Hockham in 1966. Kao received the Nobel Prize in 2009.

√ √ 1 ω ǫ′ σ 1 ω ǫ′ = = tan δ. 2 c ωǫ 2 c

(10.74)

The usual measure is the attenuation in decibels for a length of one kilometre, which may be expressed from eqn (10.74) as follows: A = 20 log10 exp(1000 kimag ) = 8680 kimag √ ω ǫ′ tan δ db km–1 . = 4340 c

(10.75)

Optical ﬁbres

251

Taking an operational frequency of f = 3 × 1014 Hz, a typical dielectric constant ǫ ′ = 2.25, and the best material available at the time with tan δ ≈ 10–7 , we get A ≈ 4 × 103 db km–1 ,

(10.76)

10 000

10 –7

1000

10 –8

100

10 –9

10

10 –10

1.0

0.1 1967

10 –11

Approximate value for tan δ of ﬁbre

Optical ﬁbre attenuation (db km–1)

a far cry from 20. No doubt materials can be improved, but an improvement in tan δ of more than two orders of magnitude looked at the time somewhat beyond the realm of practical possibilities. Nevertheless, the work began, and Fig. 10.25 shows the improvement achieved. The critical 20 db was reached at the end of 1969, and by 1983 the ﬁgure was down to 0.2 db km–1 , an amazing improvement on a difﬁcult enough initial target. The most usual material used for these successful ﬁbres has been puriﬁed silica (SiO2 ) with various dopants to produce the refractive index proﬁle across the diameter to contain the light ray in a small tube along the axis, with total internal reﬂection from the lower refractive index cladding. To get very low attenuations, the wavelength of the light has to be carefully chosen. Even with highly puriﬁed silica, there are some hydroxyl (OH) impurity radicals, which are stimulated into vibrations and hence absorb bands of frequencies. There are ‘windows’ in this absorption spectrum, one of which between 1.5 and 1.7 µm wavelength was used to obtain the 0.2 db km–1 result. A new impetus to the in any case fast-growing optical ﬁbre communications has been given by the invention of a ﬁbre ampliﬁer that makes orthodox repeaters superﬂuous. The principles of operation will be explained in Section 12.10 after some acquaintance with lasers. The lowest attenuation available in 2003 was 0.15 db/km–1 at a wavelength of 1568 nm, not much less than that achieved in 1983. The latest ﬁbres, free of OH absorption, can cover the wavelength range from about 1275–1625 nm. Since the attenuation is now around 1% per km, there is not much scope for improvement. The amount of information one can get through these ﬁbres, using Wavelength Division Multiplex, is enormous, much above present demand. Demultiplexing is usually done by Bragg reﬂection ﬁlters (an example

Fig. 10.25 1969

1971

1973

1975 Year

1977

1979

1981

1983

Improvement in optical ﬁbre attenuation.

252

Dielectric materials of such a ﬁlter has already been given in Section 10.5. Two further realizations in integrated optics form will be discussed in Section 13.7). Up to now about 6×108 km of ﬁbre been laid. The rate of increase halved in 2002 but that was believed to be due to the recession rather than to the coming saturation of the market, and the economic slump continues. In conclusion, it is worth mentioning that the reduction of attenuation by four orders of magnitude in less than two decades is about the same feat as was achieved by strenuous efforts between the ﬁrst attempts of the Phoenicians (around 2000 BC) and the dawn of the ﬁbre age. If you ever encounter a problem that appears to be too daunting, remember the story of optical ﬁbres. It is an excellent illustration of the American maxim (born in the optimism of the post-war years) that the impossible takes a little longer.

10.16

The Xerox process

This great development of the past three decades enables the production of high quality reproductions of documents quickly and easily. This has in turn made decision making more democratic, bureaucrats more powerful, and caused vast forests of trees to disappear to provide the extra paper consumed. Scientiﬁcally, the principles are simple. The heart of the Xerox machine is a plate made of a thin layer of amorphous semiconductor on a metal plate. The semiconductor is a compound of As, Se, and Te. It is almost an insulator, so that it behaves like a dielectric, but it is also photo-conductive; that is, it becomes more conducting in the light (remember Section 8.6). The dielectric plate is highly charged electrostatically by brushing it with wire electrodes charged to about 30 kV. The document to be copied is imaged onto the plate. The regions that are white cause the semiconductor to become conducting, and the surface charge leaks away to the earthed metal backing plate. However, where the dark print is imaged, charge persists. The whole plate is dusted with a ﬁne powder consisting of grains of carbon, silica, and a thermosetting polymer. Surplus powder is shaken off, and it adheres only to the highly charged dark regions. A sheet of paper is then pressed onto the plate by rollers. It picks up the dust particles and is then treated by passing under an infrared lamp. This fuses polymeric particles, which subsequently set, encasing the black C and SiO2 dust to form a permanent image of the printed document. To clear the plate, it is illuminated all over so that it all discharges, the ink is shaken off, and it is ready to copy something else. A very simple process scientiﬁcally, it works so well because of the careful and very clever technological design of the machine.

10.17

Liquid crystals

I suppose we have heard so much about liquid crystal displays (LCD) in the last couple of decades that we tend to ignore the implied contradiction. Is it a liquid, or is it a crystal? Well, it can be both, and the fact has been known for nearly a hundred years. This particular set of viscous liquids happens to have anisotropic properties due to ordering of long rod-like molecules. If you would like to visualize the short-range order of long rods have a look at the photograph shown in Fig. 10.26 taken in Canada by Dr Raynes, an expert on

Liquid crystals

253

Fig. 10.26 Logs drifting in a Canadian river.

liquid crystals. Mind you, the analogy is not exact. In contrast with logs liquid crystals have in addition strong electric dipole moments and easily polarizable chemical groups, so there is a voltage-dependent anisotropy. There are three types of liquid crystal structures, nematic, cholesteric, and smectic. The one most often used for display purposes belongs to the nematic type and is known as the twisted nematic display for reasons which will become obvious in a moment. The liquid crystal is held between two glass plates. If the glass plate is suitably treated, then the molecules next to the surface will align in any desired direction. We can thus achieve that the molecules on the two opposite surfaces will lie at right angles to each other, and those in between change gradually from one orientation to the other [Fig. 10.27(a)]. It is not too difﬁcult to imagine now that light incident with a polarization perpendicular to the direction of the molecules will be able to follow the twist and will emerge with a polarization twisted by 90◦ . Thus, in the conﬁguration of Fig. 10.27(a), with the two polarizers in place, light will be easily transmitted. When a voltage is applied, the molecules line up in parallel with the electric ﬁeld [Fig. 10.27(b)], the incident light no longer twists its polarization, and consequently no light transmission takes place. You may legitimately ask at this stage, why is this a display device? The answer is that this is only a valve, but it can be turned into a display device by placing a mirror behind it. With the voltage off the display is bright because it reﬂects ambient light. With the voltage on there is no light reﬂection. Other types of liquid crystal displays also exist. A colour response can be obtained by the so-called guest–host effect, which relies on an anisotropic dye aligning with the liquid crystal molecules. From a technical point of view, the biggest advantage of liquid crystal displays is that the voltages they need are compatible with those used for semiconductor devices. From the customer’s point of view, they have the major advantage of providing a ﬂat display. In the last ﬁve years they have been

254

Dielectric materials (a)

White light

(b)

White light

Polarizer Glass plates Liquid crystal molecules V

V

Liquid crystal molecules

Glass plates

Fig. 10.27

Polarizer

A schematic representation of the operational principles of a twisted nematic display device.

∗ The way this book is organized, plasma

effects are often discussed but there is no single chapter, not even a single section, devoted entirely to their properties. Hence this point is probably the best for brieﬂy describing the operation of plasma displays. The essential elements are as follows. There are two sets of electrodes perpendicular to each other, to which voltages can be applied by the control circuits. Between each pair of crossed electrodes there is a cell ﬁlled with gas (xenon and neon), in which the gas is ionized by the applied voltage. The ionized gas gives rise to ultraviolet photons, which, on impact, cause red, green, and blue phosphors (just as in a colour cathode ray tube) to emit visible light at the right amplitude, in the right proportion of colours.

very successful in supplanting cathode ray tubes. Their main competitors are plasma displays∗ at present, and organic light-emitting diodes (to be discussed in Appendix I) in the future.

10.18

Dielectrophoresis

A phenomenon related to polarization is dielectrophoresis (or DEP), in which an electric ﬁeld is used to generate a force on a dielectric particle, often when it is suspended in a liquid. Unlike the dielectric effects we have encountered so far, DEP requires a nonuniform ﬁeld. Also unlike most ‘classical’ effects on matter, it was only investigated in detail relatively recently (by Herbert Pohl, in the 1950s). Consider a single dielectric particle, which we assume contains separable charges ±q. In the absence of any ﬁeld, the centres of positive and negative charge coincide. If a uniform electric ﬁeld E is applied in the x-direction, there will be a force ±qE on each charge. These forces cause the charge centres to separate, moving apart by distance dx. This polarization is clearly responsible for any dielectric effects. However, in total the forces cancel, so there is no net force on the particle. Consider now the case when the electric ﬁeld is nonuniform. How could we generate such a ﬁeld? One simple method is to apply a potential between a pair of shaped electrodes. For example, we could apply a voltage V between a cylindrical wire located at the origin and a co-axial cylindrical conducting shell, as shown in Fig. 10.28. At any radius r around the centre, the electric ﬂux and ﬁeld must both act in the radial direction. Symmetry and continuity

Dielectrophoresis of electric ﬂux imply that D must vary only in the radial direction as 1/r, and hence E must also vary in this way. Let us now place the dielectric particle between the wire and the shell, on the x-axis. There may also be a surrounding medium, but the effect will also work in a vacuum. Let us assume that the negative charge centre is at x so the ﬁeld it experiences is E(x). The force it experiences is therefore –qE in the x-direction. The ﬁeld experienced by the positive charge centre has the slightly different value E + dE since the positive and negative charge centres are separated by a distance dx. For small distances, dE = (dE/dx) dx, so the force on the positive charge is +q{E + (dE/dx) dx}. Clearly, the two forces acting on the particle no longer balance, and there is a net force in the x-direction of Fx = q(dE/dx) dx.

(10.77)

For the geometry here, dE/dx is negative, so the particle experiences an attractive force towards the high-ﬁeld region at the origin. Now, qdx is simply the polarization of the particle, which as we have already established depends on the electric ﬁeld and the polarizability α. Consequently, we can write the force as Fx = αE(dE/dx) = (α/2) d(E2 )/dx.

(10.78)

This fundamental result implies that DEP effects are completely different to electrostatic forces. There is no dependence on the sign of the electric ﬁeld, and nothing will happen unless the electric ﬁeld varies in space, so that d(E2 )/dx is non-zero. More generally, the ﬁeld will vary in more than one direction. Consequently, there will be forces in other directions. We can guess that Fy = (α/2) d(E2 )/dy, and hence that the total force in a three-dimensional system can be written as a vector, F = (α/2)∇(E2 ).

(10.79)

Here ∇ is the operator ∂/∂x i + ∂/∂y j + ∂/∂z k. The remaining details are more complicated. Firstly, the polarizability α depends on any surrounding medium (often a liquid in DEP experiments). Secondly, the electric ﬁeld may be time varying rather than static. Clearly the effect must depend on the properties of both the particle and the medium at the frequency involved. For a spherical particle of radius R and complex permittivity εP in a medium of complex permittivity εM , experiencing a RMS ﬁeld Erms at angular frequency ω, the time-averaged DEP force is F = 2π R3 εM Re(fCM ) ∇|Erms |2 .

(10.80)

Here fCM is the Clausius–Mossotti factor, fCM = (εP – εM )/(εP + 2εM )

(10.81)

that we have already met in Section 10.10, in a simpliﬁed form, when we considered a lossless dielectric in free space.

255 y Shell

E (r) Wire

V

E E + dE −q +q x x + dx

Fig. 10.28 Arrangement for generating a nonuniform electric ﬁeld, and its effect on a dielectric particle.

x

256

Dielectric materials The nature of eqn (10.80) now allows us to guess at some applications. Firstly, depending on the relative values of εP and εM , the force may have different signs. In positive DEP, particles are attracted towards ﬁeld concentrations, and in negative DEP they are repelled. In the former case, we can build a particle concentrator. For example, in the geometry above, particles suspended in a liquid between the electrodes will be attracted to the central wire, where they will sediment. More generally, mixtures of particles may experience different forces, and it may then be possible to separate them. Large particles will generally experience larger forces. However, particles of the same size may still be sorted at frequencies where the factors εM Re(fCM ) are signiﬁcantly different. Dielectrophoresis is extensively used to manipulate biological particles such as cells and viruses, where this is the case. Specialized microﬂuidic systems with complex electrode systems have been designed that can transport, sort, trap, rotate, rupture, and even fuse cells. Since the effect works up to optical frequencies—where it is more commonly known as optical trapping—similar results may be obtained using laser beams to generate the electric ﬁelds; a phenomenon ﬁrst investigated by Ashkin. As a result, DEP and optical trapping are workhorse tools for biologists. DEP is also being used by nanotechnologists to sort nanoparticles (for example, to separate metallic and semiconducting carbon nanotubes), and as a basic method of nanoassembly (for example, to place nanotubes between contact electrodes so that their transport properties can be measured).

Exercises 10.1. Sketch qualitatively how you would expect the permittivity and loss tangent to vary with frequency in those parts of the spectrum that illustrate the essential properties, limitations, and applications of the following materials: window glass, water, transformer oil, polythene, and alumina. 10.2. What is the atomic polarizability of argon? Its susceptibility at 273 K and 1 atm is 4.35 × 10–4 . 10.3. A long narrow rod has an atomic density 5 × 1028 m–3 . Each atom has a polarizability of 10–40 farad m2 . Find the internal electric ﬁeld when an axial ﬁeld of 1 V/m is applied. 10.4. The energy of an electric dipole in an electric ﬁeld is given by eqn (10.9). Derive this expression by ﬁnding the work done by the electric ﬁeld when lining up the dipole. 10.5. The tables* show measured values of dielectric loss for thoria (ThO2 ) containing a small quantity of calcium. For this material the static and high-frequency permittivities have been found from other measurements to be ǫs = 19.2ǫ0 ,

ǫ∞ = 16.2ǫ0 .

f = 695 Hz T(K) tan δ

f = 6950 Hz T(K) tan δ

555 543 532 524 516 509 503 494 485 475

631 621 612 604 590 581 568 543 518 498

0.023 0.042 0.070 0.086 0.092 0.086 0.081 0.063 0.042 0.029

0.026 0.036 0.043 0.055 0.073 0.086 0.086 0.055 0.025 0.010

* Data taken from PhD thesis of J. Wachtman, University of Maryland, 1962, quoted in Physics of solids, Wert and Thomson (McGraw–Hill), 1964. Assume that orientational polarization is responsible for the variation of tan δ. Use the Debye equations to show that by expressing the characteristic relaxation time as

Exercises τ = τ0 exp(H/kT) (where τ0 and H are constants) both of the experimental curves can be approximated. Find τ0 and H. If a steady electric ﬁeld is applied to thoria at 500 K, then suddenly removed, indicate how the electric ﬂux density will change with time. 10.6. A more general time-varying relationship between the electric displacement D and the electric ﬁeld E may be assumed to have the form dE dD = bE + c D+a dt dt where a, b, c are constants. Determine the values of these constants in terms of ǫs , the static dielectric constant, ǫ∞ , the high-frequency dielectric constant, and τ , the relaxation time for dipoles under constant electric ﬁeld conditions. 10.7. Figure 10.29 shows two types of breakdown that can occur in the reverse characteristic of a p–n junction diode. The ‘hard’ characteristic is the desired avalanche breakdown discussed in Chapter 9. The ‘soft’ characteristic is a fault that sometimes develops with disastrous effect on the rectiﬁcation efﬁciency. It has been suggested that this is due to precipitates of metals such as copper or iron in the silicon, leading to local breakdown in high-ﬁeld regions. [Goetzberger and Shockley (1960). ‘Metal precipitates in p–n junctions’, J. Appl. Phys., 31, 1821.] Discuss brieﬂy and qualitatively this phenomenon in terms of the simple theories of breakdown given in this chapter.

Reverse current (μA)

100

50 ‘Soft’

0

50 Reverse voltage (V)

‘Hard’

100

Fig. 10.29 10.8. A capacitor is to be made from a dielectric having a breakdown ﬁeld strength Eb and a relative permittivity ǫr . The electrodes are metal plates ﬁxed to the sides of a slab (thickness 0.5 mm) of the dielectric. Owing to a slight distortion

257

of one of the plates, one-third of its area is separated from the dielectric by an air-ﬁlled gap of thickness 1 µm. The remaining two-thirds of the plate and the whole of the second plate are in intimate contact with the dielectric. The breakdown ﬁeld Eb is 2.0 MV m–1 for the dielectric and 3.0 MV m–1 for air, ǫ r is 1000. Discuss the effect of the gap (compared with a gap-free capacitor), on (a) the capacitance and (b) the breakdown voltage. 10.9. Derive an expression for the gain of the piezoelectric ultrasonic ampliﬁer (Hutson, McFee, and White (1961), Phys. Rev. Lett., 7, 237). [Hint: In the one-dimensional case we can work in terms of scalar quantities. Our variables are: ǫ, D, T, S, J , Ne . The equations available are: eqns (10.58) and (10.59) for the relationship between the mechanical and electrical quantities, the equation for the electron current including both a conduction and a diffusion term (given in Exercise 9.2), the continuity equation for electrons, and one of Maxwell’s equations relating D to N e . Altogether there are ﬁve equations and six variables. The missing equation is the one relating strain to stress for an acoustic wave. It is of the form, ∂ 2S ∂ 2T = ρm 2 , 2 ∂z ∂t where ρm is the density of the piezoelectric material. The gain may be derived in a manner analogous to that adopted in Chapter 1 for the derivation of the dispersion relations for electromagnetic and plasma waves. The steps are as follows: (i) Assume that the a.c. quantities are small in comparison with the d.c. quantities (e.g. the a.c. electric ﬁeld is much smaller than the applied d.c. electric ﬁeld) and neglect the products of a.c. quantities. (ii) Assume that the a.c. quantities vary as exp[– i(ωt – kz)] and reduce the linear differential equation system to a set of linear equations. (iii) Derive the dispersion equation from the condition that the linear equation system must have a non-trivial solution. (iv) Substitute k = ω/νs +δ [where ν s = (c/ρm )1/2 is the velocity of sound in the medium] into the dispersion equation and neglect the higher powers of δ. (v) Calculate the imaginary part of δ which will determine (by its sign) the growing or attenuating character of the wave. Show that there is gain for ν0 >νs , where ν0 is the average velocity of the electrons.] 10.10. Find the frequency dependence of the complex permittivity due to electronic polarizability only.

258

Dielectric materials

[Hint: Write down the equation of motion for an electron, taking into account viscous friction (proportional to velocity) and restoring force (proportional to displacement). Solve the equations for a driving force of eE exp(–iωt). Remember that polarization is proportional to displacement and ﬁnally ﬁnd the real and imaginary parts of the dielectric constant as a function of frequency.]

10.11. Using the data for KCl given in Exercise 5.4 estimate a frequency at which the dielectric constant of KCl will relax to a lower value. [Hint: Around the equilibrium value the force is proportional to displacement (to a ﬁrst approximation), whence a characteristic frequency can be derived.]

Magnetic materials Quod superest, agere incipiam quo foedere ﬁat naturae, lapis hic ut ferrum ducere possit, quem Magneta vocant partio de nomine Grai, Magnetum quia ﬁt patriis in ﬁnibus ortus hunc homines lapidem mirantur; . . . Hoc genus in rebus ﬁrmandumst multa prius quam ipsius rei rationem reddere possis, et nimium longis ambagibus est adeundum; Lucretius De Rerum Natura

To pass on, I will begin to discuss by what law of nature it comes about that iron can be attracted by that stone which the Greeks call magnet from the name of its home, because it is found within the national boundaries of the Magnetes. This stone astonishes men . . . In matters of this sort many principles have to be established before you can give a reason for the thing itself, and you must approach by exceedingly long and roundabout ways;

11.1 Introduction There are some curious paradoxes in the story of magnetism that make the topic of considerable interest. On the one hand, the lodestone was one of the earliest known applications of science to industry—the compass for shipping; and ferromagnetism is of even more crucial importance to industrial society today than it was to early navigators. On the other hand, the origin of magnetism eluded explanation for a long time, and the theory is still not able to account for all the experimental observations. It is supposed that the Chinese used the compass around 2500 BC. This may not be true, but it is quite certain that the power of lodestone to attract iron was known to Thales of Miletos in the sixth century BC. The date is put back another two hundred years by William Gilbert (the man of science in the court of Queen Elizabeth the First), who wrote in 1600 that ‘by good luck the smelters of iron or diggers of metal discovered magnetite as early as 800 BC.’ There is little doubt about the technological importance of ferromagnetism today. In the United Kingdom as much as 7 × 1011 W of electricity are generated at times; electrical power in this quantity would be hopelessly impractical without large quantities of expertly controlled ferromagnetic materials. Evidence for the statement that the theory is not fully understood may be obtained from any honest man who has done some work on the theory of magnetism.

11

260

Magnetic materials

11.2

Macroscopic approach

By analogy with our treatment of dielectrics, I shall summarize here brieﬂy the main concepts of magnetism used in electromagnetic theory. As you know, the presence of a magnetic material will enhance the magnetic ﬂux density. Thus the relationship

M is the magnetic dipole moment per unit volume, or simply, magnetization.

B = μ0 H,

(11.1)

B = μ0 (H + M)

(11.2)

valid in a vacuum, is modiﬁed to

in a magnetic material. The magnetization is related to the magnetic ﬁeld by the relationship χm is the magnetic susceptibility.

M = χ m H.

(11.3)

Substituting eqn (11.3) into eqn (11.2) we get μr is called the relative permeability.

B = μ0 (1 + χm ) H = μ0 μr H.

11.3

∗ It

is an unfortunate fact that the usual notation is μ both for the permeability and for the magnetic moment. I hope that, by using the subscripts 0 and r for permeability and m for magnetic moment, the two things will not be confused.

(11.4)

Microscopic theory (phenomenological)

Our aim here is to express the macroscopic quantity, M, in terms of the properties of the material at atomic level. Is there any mechanism at atomic level that could cause magnetism? Reverting for the moment to the classical picture, we can say yes. If we imagine the atoms as systems of electrons orbiting around protons, they can certainly give rise to magnetism. We know this from electromagnetic theory, which maintains that an electric current, I, going round in a plane will produce a magnetic moment,∗ μm = IS,

(11.5)

where S is the area of the current loop. If the current is caused by a single electron rotating with an angular frequency ω0 , then the current is eω0 /2π , and the magnetic moment becomes μm =

eω0 2 r , 2

(11.6)

where r is the radius of the circle. Introducing now the angular momentum = mr2 ω0 , Remember that the charge of the electron is negative; the magnetic moment is thus in a direction opposite to the angular momentum.

(11.7)

we may rewrite eqn (11.6) in the form, μm =

e . 2m

(11.8)

We now ask what happens when an applied magnetic ﬁeld is present. Consider a magnetic dipole that happens to be at an angle θ to the direction of the

Microscopic theory (phenomenological)

261

B

magnetic ﬁeld (Fig. 11.1). The magnetic ﬁeld produces a torque µm × B on the magnetic dipole. Noting that the rate of change of the angular momentum is equal to the torque we may obtain, with the aid of eqn (11.8), the equation dμ/dt = (e/2m)(μ × B).

(11.9a) μm

In a constant magnetic ﬁeld the solution of this equation gives precession around the magnetic ﬁeld at a frequency of ωL = eB/2m,

(11.9b)

which is called the Larmor frequency. If the magnetic dipole precesses, some electric charge must go round. So we could use eqn (11.6) to calculate the magnetic moment due to the precessing charge. Replace ω0 by ωL ; we get (μm )ind

Br2 e2 = , 4m

(11.10)

θ

Fig. 11.1 A magnetic dipole precessing around a static magnetic ﬁeld.

where r is now the radius of the precessing orbit. The sign of this induced magnetic moment can be deduced by remembering Lenz’s law. It must oppose the magnetic ﬁeld responsible for its existence. We are now in a position to obtain M from the preceding microscopic considerations. If there are Na atoms per unit volume and each atom contains Z electrons, the total induced magnetic dipole moment is M = Na Z(μm )ind .

(11.11)

Hence, the magnetic susceptibility is χm =

M Na Ze2 r2 μ0 =– . H 4m

(11.12)

Rarely exceeding 10–5 , χm given by the above equation is a small number, but the remarkable thing is that it is negative. This is in marked contrast with the analogous case of electric dipoles, which invariably give a positive contribution.∗ The reason for this is that the electric dipoles line up, whereas the magnetic dipoles precess in a ﬁeld. Magnetic dipoles can line up as well. The angle of precession will stay constant in the absence of losses but not otherwise. In the presence of some loss mechanism the angle of precession gradually becomes smaller and smaller as the magnetic dipoles lose energy; in other words, the magnetic dipoles do line up. They will not align completely because they occasionally receive some energy from thermal vibrations which frustrates their attempt to line up. This is exactly the same argument we used for dielectrics, and we can therefore use the same mathematical solution. Replacing the electric energy in eqn (10.13) by the magnetic energy, we get the average magnetic moment in the form, μm = μm L(a),

a=

μm μ0 H. kT

(11.13)

Denoting by Nm the number of magnetic dipoles per unit volume, we get for the total magnetic moment, M = Nm μm .

(11.14)

∗ The

electric susceptibility can also be negative, but that is caused by free charges and not by electric dipoles.

262

Magnetic materials At normal temperatures and reasonable magnetic ﬁelds, a ≪ 1 and eqn (11.14) may be expanded to give M=

Nm μ2m μ0 H , 3kB T

(11.15)

Nm μ2m μ0 . 3kB T

(11.16)

leading to Here χm is deﬁnitely positive and varies inversely with temperature.

1.0

χm =

At the other extreme of very low temperatures all the magnetic dipoles line up; this can be seen mathematically from the fact that the function L(a) (plotted in Fig. 11.2) tends to unity for large values of a. The total magnetic moment is then

L(a)

Ms = Nm μm ,

0.5

0.0

0

2

4

6

Fig. 11.2 The Langevin function, L(a).

a

(11.17)

which is called the saturation magnetization, because this is the maximum contribution the material can provide. We have now brieﬂy discussed two distinct cases: (i) when the induced magnetic moment opposes the magnetic ﬁeld, called diamagnetism; and (ii) when the aligned magnetic moments strengthen the magnetic ﬁeld, called paramagnetism. Both phenomena give rise to small magnetic effects that are of little use when the aim is the production of high magnetic ﬂuxes. What about our most important magnetic material, iron? Can we explain its properties with the aid of our model? Not in its present state. We have to modify our model by introducing the concept of the internal ﬁeld. This is really the same sort of thing that we did with dielectrics. We said then that the local electric ﬁeld differs from the applied electric ﬁeld because of the presence of the electric dipoles in the material. We may argue now that in a magnetic material the local magnetic ﬁeld is the sum of the applied magnetic ﬁeld and the internal magnetic ﬁeld, and we may assume (as Pierre Weiss did in 1907) that this internal ﬁeld is proportional to the magnetization, that is

λ is called the Weiss constant.

Hint = λM.

(11.18)

Using this newly introduced concept of the internal ﬁeld, we may replace H in eqn (11.13) by H + λM to obtain for the magnetization,

M μm μ0 (H + λM) . (11.19) =L Nm μm kB T Thus for any given value of H we need to solve eqn (11.19) to get the corresponding magnetization. It is interesting to note that eqn (11.19) still has solutions when H = 0. To prove this, let us introduce the notations, b = μm μ0 λM/kB T,

θ = Nm μ2m μ0 λ/3kB ,

(11.20)

and Tμm μ0 λM/kB T Tb M . = = 2 Nm μm 3Nm μm μ0 λ/3 kB 3θ

(11.21)

Microscopic theory (phenomenological)

263

We can now rewrite eqn (11.19), for the case H = 0, in the form, T b = L(b). 3θ

(11.22)

Plotting both sides of the above equation (Fig. 11.3) it becomes apparent that there is a solution when T < θ but no solution when T > θ . What does it mean if there is a solution? It means that M may be ﬁnite for H = 0; that is, the material can be magnetized in the absence of an external magnetic ﬁeld. This is a remarkable conclusion. We have managed to explain, with a relatively simple model, the properties of permanent magnets. Note that there is a solution only below a certain temperature. Thus, if our theory is correct, permanent magnets should lose their magnetism above this temperature. Is this borne out by experiment? Yes, it is a well-known experimental fact (discovered by Gilbert) that permanent magnets cease to function above a certain temperature. What happens when T > θ ? There is no magnetization for H = 0, but we do get some magnetization for ﬁnite H. The mathematical solution may be obtained from eqn (11.19), noting that the argument of the Langevin function is small, and we may use again the ~ a/3, leading to approximation L(a) = μm μ0 M (H + λM), = Nm μm 3kB T

(11.23)

which may be solved for M to give M=

Nm μ2m μ0 /3kB C H, H= T –θ T – Nm μ2m μ0 λ/3kB

(11.24)

Nm μ2m μ0 3kB

(11.25)

where C=

is called the Curie constant and θ is the Curie temperature. The M–H relationship is linear, and the susceptibility is given by χm =

C . T –θ

(11.26)

Thus, we may conclude that our ferromagnetic material (the name given to materials like iron that exhibit magnetization in the absence of applied magnetic ﬁelds) becomes paramagnetic above the Curie temperature. We have now explained all the major experimental results on magnetic materials. We can get numerical values if we want to. By measuring the temperature where the ferromagnetic properties disappear, we get θ (it is 1043 K for iron), and by plotting χm above the Curie temperature as a function of 1/(T – θ ) we get C (it is about unity for iron). With the aid of eqns (11.20) and (11.25) we can now express the unknowns μm and λ as follows: θ λ= C

and

μm =

3 kB C Nm μ0

1/2

.

(11.27)

M

Nm μ m T

0

θ

T=θ

2

T

4

6

θ

b

Fig. 11.3 Graphical solution of eqn (11.22). There is no solution, that is the curves do not intersect each other, for T > θ.

264

Magnetic materials Taking Nm = 8 × 1028 m–3 and the above-mentioned experimental results, we get for iron, ~ 1000 λ=

and

~ 2 × 10–23 Am2 . μm =

(11.28)

The value for the magnetic dipole moment of an atom seems reasonable. It would be produced by an electron going round a circle of 0.1 nm radius about 1015 times per second. One can imagine that, but it is much harder to swallow a numerical value of 1000 for λ. It means that the internal ﬁeld is 1000 times as large as the magnetization. When all the magnetic dipoles line up, M comes to about 106 A m–1 , leading to a value for the internal ﬂux density Bint = μ0 λM = 103 T, which is about an order of magnitude higher than the highest ﬂux density ever produced. Where does such an enormous ﬁeld come from? It is a mysterious problem, and we shall leave it at that for the time being.

11.4

Domains and the hysteresis curve

We have managed to explain the spontaneous magnetization of iron, but as a matter of fact, freshly smelted iron does not act as a magnet. How is this possible? If, below the Curie temperature, all the magnetic moments line up spontaneously, how can the outcome be a material exhibiting no external magnetic ﬁeld? Weiss, with remarkable foresight, postulated the existence of a domain structure. The magnetic moments do line up within a domain, but the magnetizations of the various domains are randomly oriented relative to each other, leading to zero net magnetism. The three most important questions we need to answer are as follows: 1. Why does a domain structure exist at all? 2. How thick are the domain walls? 3. How will the domain structure disappear as the magnetic ﬁeld increases? It is relatively easy to answer the ﬁrst question. The domain structure comes about because it is energetically unfavourable for all the magnetic moments to line up in one direction. If it were so then, as shown in Fig. 11.4(a), there would be large magnetic ﬁelds and, consequently, a large amount of energy outside the material. This magnetic energy would be reduced if the material would break up into domains as shown in Fig. 11.4(b)–(e). But why would this process ever stop? Should not the material break up into as many domains as it possibly could, down to a single atom? The reason why this would not happen is because domains must have boundaries and, as everyone knows, it is an expensive business to maintain borders of any kind. Customs ofﬁcials must be paid, not mentioning the cost of guard towers and barbed wire, with which some borders are amply decorated. Thus some compromise is necessary. The more domains there are, the smaller will be the magnetic energy outside, but the more energy that will be needed to maintain the boundary walls. When putting up one more wall needs as much energy as the achieved reduction of energy outside, an equilibrium is reached, and the energy of the system is minimized. We have now managed to provide a reasonable answer to question (1). It is much more difﬁcult to describe the detailed properties of domains, and their

Domains and the hysteresis curve

(a)

(b)

265

(c)

Fig. 11.4 (d)

The formation of domains (from C. Kittel, Introduction to solid state physics, John Wiley, New York).

(e)

dependence on applied magnetic ﬁelds. We must approach the problem, as Lucretius said, ‘by exceedingly long and roundabout ways’. However much I dislike talking about crystal structure, there is no escape now because magnetic properties do depend on crystallographic directions. I am not suggesting that magnets are ever made of single-crystal materials, but in order to interpret some of the properties of ordinary polycrystalline magnets, we have to know the magnetic properties of the single crystals. In Fig. 11.5 the magnetization curve (B against H) of iron is plotted for three different directions in the crystal. It may be seen that magnetization is relatively easy in the AB direction and harder in the AC and AG directions, or in other words, it is easier to magnetize iron along a cube edge than along a face or a body diagonal. This does not mean, of course, that all magnetic

AB

2.0 AC

AG

1.5 B (T)

(100) D (110)

K

1.0

A (111

C

B )

G 0.5 E

F

Fig. 11.5 0.0 0.0

1.6

3.2 H (A / m−1)

4.8

Magnetization curve of single-crystal iron in three different crystallographical directions.

266

Magnetic materials materials follow the same pattern. In nickel, another cubic crystal, the directions of easy and difﬁcult magnetization are the other way round. What matters is that in most materials magnetization depends on crystallographic directions. The phenomenon is referred to as anisotropy, and the internal forces which bring about this property are called anisotropy forces. Let us now see what happens at the boundary of two domains, and choose for simplicity two adjacent domains with opposite magnetizations as shown in Fig. 11.6. Note that the magnitude of the magnetic moments is unchanged during the transition, but they rotate from an ‘up’ position into a ‘down’ position. Why is the transition gradual? The forces responsible for lining up the magnetic moments (let us call them for the time being ‘lining up’ forces) try to keep them parallel. If we wanted a sudden change in the direction of the magnetic moments, we should have to do a lot of work against the ‘lining up’ forces, and consequently there would be a lot of ‘lining up’ energy present. The anisotropy forces would act the opposite way. If ‘up’ is an easy direction (the large majority of domains may be expected to line up in an easy direction), then ‘down’ must also be an easy direction. Thus, most of the directions in between must be looked upon unfavourably by the anisotropy forces. If we want to rotate the magnetic moments, a lot of work needs to be done against the anisotropy forces, resulting in large anisotropy energy. According to the foregoing argument, the thickness of the boundary walls will be determined by the relative magnitudes of the ‘lining up’ and the anisotropy forces in the particular ferromagnetic material. If anisotropy is small, the transition will be slow and the boundary wall thick, say 10 µm. Conversely, large anisotropy forces lead to boundary walls which may be as thin as 0.3 µm. We are now ready to explain the magnetization curves of Fig. 11.5. When the piece of single-crystal iron is unmagnetized, we may assume that there are lots of domains, and the magnetization in each domain is in one of the six easy directions. Applying now a magnetic ﬁeld in the AB direction, we ﬁnd that, as the magnetic ﬁeld is increased, the domains which lay originally in the AB direction will increase at the expense of the other domains, until the whole material contains only one single domain. Since the domain walls move easily, the magnetic ﬁeld required to reach saturation is small. What happens if we apply to the same single-crystal iron a magnetic ﬁeld in the AG direction? First, the domain walls will move just as in the previous

Width of wall

Fig. 11.6 Rotation of magnetic moments at a domain wall.

Domains and the hysteresis curve case until only three easy directions are left, namely AB, AD, and AE, that is those with components in the AG direction. This may be achieved with very little magnetic ﬁeld, but from then on (K in Fig. 11.5) the going gets hard. In order to increase the magnetization further, the magnetic moments need to change direction, which can only happen if the internal anisotropy forces are successfully overcome. This requires more effort, hence the slope of the magnetization curve changes, and saturation will only be achieved at greater magnetic ﬁelds. Is this explanation still correct for polycrystalline materials? Well, a polycrystalline material contains lots of single crystal grains, and the above argument applies to each of the single crystals; thus the magnetization curve of a polycrystalline material should look quite similar to that of a single-crystal material in a difﬁcult direction. As you know from secondary school, this is not the case. Figure 11.5 does not tell the whole story. The magnetization curve of a typical ferromagnetic material exhibits hysteresis, as shown in Fig. 11.7. Starting with a completely demagnetized material, we move up the curve along 2, 3, 4, 5 as the magnetic ﬁeld is increased. Reducing then the magnetic ﬁeld, we get back to point 6, which is identical with point 4, but further decrease takes place along a different curve. At 7 there is no applied magnetic ﬁeld, but B is ﬁnite. Its value, B = Br , is the so-called remanent ﬂux density. Reducing further, the magnetic ﬁeld B takes the values along 8, 9, 10. Returning from 10, we ﬁnd that 11 is identical with 9 and then proceed further along 12 and 13 to reach ﬁnally 4. The loop 4, 7, 8, 9, 12, 13, 4 is referred to as the hysteresis loop, already discussed for ferroelectric materials. It clearly indicates that the magnetization of iron is an irreversible phenomenon. The paths 4, 5 and 9, 10 suggest that rotation from easy into difﬁcult directions is reversible, thus the causes of irreversibility should be sought in domain movement. Because of the presence of all sorts of defects in a real material, the domain walls move in little jerks, causing the magnetization to increase in a discontinuous manner (region 2, 3 magniﬁed in Fig. 11.7). The walls get stuck once in a while and then suddenly surge forward, setting up in the process some eddy currents and sound waves, which consume energy. If energy is consumed, the process cannot be reversible, and that is the reason for the existence of the hysteresis loop. B

267

Note that the value of H at 13 is called the coercivity, denoted by Hc . It represents the magnetic ﬁeld needed for the ﬂux density to vanish.

5

6 4

7 3 Br 2

8 1

9 10

11

Hc 13

12

H

Fig. 11.7 The magnetization curve of a typical ferromagnetic material.

268

Magnetic materials

∗ This

boundary

Domain

is, incidentally the cause of the humming noise of transformers.

Fig. 11.8 Non-magnetic impurity surrounded by a domain.

Is it possible to describe more accurately the movement of domains? One can go indeed a little further by taking into account the effect of magnetostriction, which, as you may guess, is the magnetic counterpart of electrostriction. Strictly speaking, one should distinguish between magnetostriction and piezomagnetism, the magnetic counterpart of piezoelectricity. But biased magnetostriction (see discussion on biased electrostriction in Section 10.11) is phenomenologically equivalent to piezomagnetism, and piezomagnetism has not been much investigated anyway; thus most authors just talk about magnetostriction. Disregarding the problem of nomenclature, the relevant fact is that when a magnetic ﬁeld is applied, the dimensions of the material change,∗ and conversely, strain in the material leads to changes in magnetization and may also affect the directions of easy magnetization. Now if the material exhibits a large anisotropy and stresses are present as well, then there will be local easy directions resisting the movement of domain walls everywhere. The stresses may be caused by the usual defects in crystals and particularly by impurities. In addition, a cluster of non-magnetic impurity atoms might be surrounded by domains (see Fig. 11.8). This is a stable conﬁguration which cannot be easily changed. How can we classify magnetic materials? There is a simple division into soft and hard magnetic materials. Why soft and hard? Well, the hard materials are those which are hard to magnetize and demagnetize. So materials which are easy to magnetize and demagnetize should be called easy materials. In fact, they are called soft materials, and there is nothing we can do about that. We have to remember, though, that these are only very tenuously related to mechanical properties, which may also be hard and soft.

11.5

Soft magnetic materials

Their main role is to enhance the magnetic effect produced by a currentcarrying coil. So, obviously, they should have large saturation magnetization and large permeability. If the material is subjected to alternating voltages, then an important consideration is to reduce losses caused by the induced eddy currents, which can be done by increasing resistivity. What else is needed in order to reduce losses? A narrow hysteresis loop is needed as shown below. The energy dissipated in a coil for a period T may be expressed with the aid of the current and voltage as T Ed = V (t)i(t) dt. (11.29) 0

Now, using Faraday’s law (that the voltage is proportional to the derivative of the ﬂux density) and Ampère’s law (that the magnetic ﬁeld is proportional to current) eqn (11.29) may be rewritten as (11.30) Ed = C H d B, where C is a constant. Thus, clearly, the energy loss per cycle is proportional to the area of the hysteresis loop. The most important parameter determining the desirable properties of soft magnetic materials is the frequency at which they are used. For d.c.

Soft magnetic materials applications the best material is the one with the largest saturation magnetization. As the frequency increases, it is still important to have large saturation magnetization, but low coercivity is also a requirement. At high frequencies, considering that eddy current losses are proportional to the square of the frequency, the most important property is high resistivity. Do losses matter? In practical terms this is probably the most important materials science problem that we have touched upon. Something like many millions of megawatts of electricity are being generated around the world, all by generators with hysteresis losses of order 0.5–1.0%. Then a large fraction of this electricity goes into motors and transformers with more iron losses. If all inventors were paid a 1% royalty on what they saved the community, then a good way to become rich would be to make a minute improvement to magnetic materials. Is there any good scientiﬁc way to set about this? Not really. We know that anisotropy, magnetostriction, and local stresses are bad, but we cannot start from ﬁrst principles and suggest alloys which will have the required properties. The considerable advances that have been made in magnetic materials have largely been achieved by extensive and expensive trial and error. To Gilbert’s seventeenth-century crack about ‘good luck’ we must add diligence for the modern smelters of iron. The currently used phrase is actually ‘enlightened empiricism’. Iron containing silicon is used in most electrical machinery. An alloy with about 2% silicon, a pinch of sulfur, and critical cold rolling and annealing processes is used for much rotating machinery. Silicon increases the resistivity, which is a good thing because it reduces eddy-current losses. Iron with a higher silicon content is even better and can be used in transformer laminations, but it is mechanically brittle and therefore no good for rotating machinery. Where small quantities of very low-loss material are required and expense is not important, as for radio-frequency transformers, Permalloy [78.5% Ni, 21.5% Fe] is often used. A further improvement is achieved in the material called ‘Supermalloy’ which contains a little molybdenum and manganese as well. It is very easily magnetizable in small ﬁelds [Fig. 11.9(a)] and has no magnetostriction. We may now mention a fairly new and rather obvious trick. If anisotropy is bad, and anisotropy is due to crystal structure, then we should get rid of the crystal structure. What we obviously need is an amorphous material. How can we produce an amorphous material? We can produce it by cooling the melt rapidly, so that the liquid state disorder is frozen in. The key word is ‘rapidly’. In fact, the whole process is called Rapid Solidiﬁcation Technology, abbreviated as RST. The cooling should proceed at a speed of about a million degrees per second, so the technological problems have not been trivial. In the ﬁrst successful commercial solution a stream of molten metal is squirted on a cooled rotating drum, followed usually by a stress relief anneal at about 300 ◦ C. The resulting magnetic material has the form of long thin ribbons typically about 50 µm thick and a few millimetres wide. New production methods, for example the planar ﬂow casting method, in which a stable rectangular melt ‘puddle’ feeds the material into the drum, have led to further improvements. It is now possible to obtain a uniform ribbon with a thickness of 20–30 µm and up to 20 cm wide. The main advantage of amorphous materials is that they can be produced easily and relatively cheaply, with magnetic properties nearly as good as those of commercial alloys, which require careful

269

B(T) (a) 1.5 1.0 0.5 0.0 –0.5 –1.0 –1.5 –0.5 0 0.5 H(A / m–1) B(T) 1.5

(b) Alnico 9

1.0 0.5

Alnico 5

0.0 –0.5 –1.0 –1.5 –15 –10 –5 0 5 H(A / m–1)

10 15 104

Fig. 11.9 Hysteresis loops of (a) Supermalloy and (b) Alnico 5 and 9. Note the factor 105 between the horizontal scales of (a) and (b).

270

Magnetic materials melting and elaborate sequences of rolling and annealing. The presently available amorphous materials have not quite reached the quality of supermalloy, but they are quite close. The cobalt-based commercially available 2714 A material has a saturation magnetization of 0.5 T with a maximum permeability of a million. Another one, known as 2605S-3 A made of iron and chromium has a saturation magnetization of 1.4 T and a maximum permeability over a quarter of a million. The latest line of soft magnetic materials are the nanocrystalline alloys with grain sizes of the order of 10 nm. They have been around for about 15 years. Typical representatives are Fe–B–Si–Cu–Nb alloys, which may reach relative permeabilities over 100 000. The excellent soft magnetic properties may be explained by the reduction in effective crystal anisotropy expected when grain sizes are reduced below the bulk-domain wall thickness. The situation is somewhat different in power applications, such as transformers. There the traditional materials are cheaper, but amorphous materials may still represent the better choice on account of lower losses; their higher cost may be offset in the long term by lower power consumption (or even possible future legislation in some countries requiring higher efﬁciency in electrical equipment). At higher frequencies, as mentioned before, high resistivities are required for which a family of ferrites with chemical formula MO · Fe2 O3 (where M is a metal, typically Ni, Al, Zn, or Mg) is used. If the metal M is iron, the material is iron ferrite, Fe3 O4 , the earliest-known magnetic material. Ferrites are usually manufactured in four stages. In the ﬁrst stage the material is produced in the form of a powder with the required chemical composition. In the second stage the powder is compressed, and the third stage is sintering to bind the particles together. The fourth stage is machining (grinding, since the material is brittle) to bring the material to its ﬁnal shape. For the properties of a number of soft magnetic materials see Table 11.1.

11.6

Hard magnetic materials (permanent magnets)

What kind of materials are good for permanent magnets? Well, if we want large ﬂux density produced, we need a large value of Br . What else? We need a large Hc . Why? A rough answer is that the high value of Br needs to be protected. If for some reason we are not at the H = 0 point, we do not want to lose much ﬂux, therefore the B–H curve should be as wide as possible. A more rigorous argument in favour of large Hc can be produced by taking account of the so-called demagnetization effect, but in order to explain that, I shall have to make a little digression and go back to electromagnetic theory. First of all, note that in a ring magnet [Fig. 11.10(a)] B = Br = constant everywhere in the material to a very good approximation. Of course, such a permanent magnet is of not much interest because we cannot make any use of the magnetic ﬂux. It may be made available, though, by cutting a narrow gap in the ring, as shown in Fig. 11.10(b). What will be the values of B and H in the gap? One may argue from geometry that the magnetic lines will not spread out (this is why we chose a narrow gap, so as to make the calculations simpler) and the ﬂux density in the gap will be the same as in the magnetic material. But, and this is the question of interest, will the ﬂux density be the same in the

Hard magnetic materials (permanent magnets)

271

Table 11.1 Major families of soft magnetic materials with typical properties Category

Bs (T)

A. Steels lamination (low C) non-oriented (2% Si) convent. grain oriented (CGO M-4) high grain oriented (HGO)

ρ(μ – m) μmax

2.1–2.2 0.4 2.0–2.1 0.35 2.0 0.48

5 000

Typical core loss, W kg–1 measured at f(Hz)

Applications, notes

2.0 (60) 2.7 (60) 0.9 (60)

Inexpensive fractional hp motors High efﬁciency motors 50/60 Hz distribution transformers 50/60 Hz DTs: high design Bmax

2.0

0.45

1.6 1.1 0.8

0.48 0.55 0.58

150 000 110 (50 k) 150 000 40 (50 k) 33 (50 k) 106

2.3

0.35

50 000

2.2 (60)

C. Ferrites MnZn

0.5

2 × 106

6 000

35 (50 k)

NiZn

0.35

1010

4 000

B. Fe–(Ni, Co) alloys 40–50 Ni 77–80 Ni (square permalloy) 79 Ni–4 Mo (4–79 Mo permalloy, supermalloy) 49 Co–2 V (permendur, supermendur)

1.2 (60)

High μ, used as thin ribbon Highest μ/lowest core loss of any metallic material Highest Bs of commercial soft magnetic material Power supply inductors, transformers MHz applications

δ Flux lines

O

O

Fig. 11.10 (a)

(a) Magnetic ﬁeld lines inside a permanent magnet. (b) The same magnet with a narrow gap.

(b)

presence of the gap as in its absence? Without the gap, B = Br (Fig. 11.11). If the value of ﬂux density is denoted by B = Br1 in the presence of the gap, the magnetic ﬁeld in the gap will be Hg = Br1 /μ0 . If you can remember Ampère’s law, which states that the line integral of the magnetic ﬁeld in the absence of a current must vanish for a closed path, it follows that Hg δ + Hm l = 0.

(11.31)

From the above equations we get Br1 = –

μ0 l Hm . δ

(11.32)

Hm is the magnetic ﬁeld in the material, and δ and l are the lengths of the paths in the gap and in the material, respectively.

272

Magnetic materials

B(H) Br Br1

B =–

μ0l H δ

H

Fig. 11.11 Construction for ﬁnding Br1 .

But remember that the relationship between Br1 and Hm is given also by the hysteresis curve. Hence, the value of Br1 may be obtained by intersecting the hysteresis curve by the straight line of eqn (11.32) as shown in Fig. 11.11. The aforegoing construction depends on the particular geometry of the permanent magnet we assume, but similar ‘demagnetization’ will occur for other geometries as well. Hence, we may conclude in general that in order to have a large, useful ﬂux density, the B–H curve must be wide. We may therefore adopt, as a ﬁgure of merit, the product Br Hc or, as is more usual, the product (BH)max in the second quadrant. How can one achieve a large value of Hc ? It is relatively easy to give an answer in principle. All the things which caused the quality of soft materials to deteriorate are good for permanent magnets. In particular, when a domain gets stuck on an impurity, that is bad for a soft magnetic material but good for the hard variety. An obvious way to include impurities is to add some carbon. High-carbon steels were indeed the permanent magnet materials in the nineteenth century until displaced by tungsten steels towards the end of the century. The simplest permanent magnet one could conceive in principle would be a single crystal of a material that has a large anisotropy and has only one axis of easy magnetization. The anisotropy may be characterized by an effective ﬁeld Ha , which attempts to keep the magnetization along the axis. If a single-crystal material is magnetized along this axis, and a magnetic ﬁeld is applied in the opposite direction, nothing should happen in principle until the ﬁeld Ha is reached, and then, suddenly, the magnetization of the whole crystal should reverse. Going one step further in this direction, one could claim that any collection of anisotropic particles that are too small to contain a domain wall (having a diameter of the order of 20 nm) will have large coercivity. This idea, due to Stoner and Wohlfarth, was the inspiration behind many attempts to make better permanent magnets. In particular, the so-called Elongated Single Domain (ESD) magnets owe their existence to the above concept. It is also likely that elongated particles play a signiﬁcant role in the properties of the Alnico series of alloys, which contain aluminium, nickel, and cobalt besides iron. They ﬁrst appeared in the early 1930s but have been steadily improving ever since. A major early advance was the discovery that cooling in a magnetic ﬁeld produced anisotropic magnets with improved properties in the ﬁeld-annealed direction. The hysteresis curves of their best-known representatives (Alnico 5 and 9) are shown in Fig. 11.9(b). Ferrites are also used for hard magnetic materials in the form MO·(Fe2 O3 )6 (M = Ba, Sr, or Pb). They were introduced in the 1950s. They have been steadily growing in tonnage ever since, overtaking the Alnico alloys in the late 1960s and rising in the late 1980s to 97.4% of world production (note that in value they represent only about 60%). Their high coercivity derives from the high anisotropy of the hexagonal phase of the materials. They have many advantages: they are cheap, easily manufactured, chemically stable, and have low densities. Their disadvantages are the relatively low remanence and declining performance for even moderate rises in temperature. One might be forgiven for believing that the late entry of rare-earth magnets into the market place was due to their rarity. In fact, rare-earth elements are not particularly rare, but they occur in mixtures with each other which

Microscopic theory (quantum-mechanical)

273

Table 11.2 Hard magnetic materials Material

Hc (A m–1 )

Br (T)

(BH)max J m–3

Carbon steel 0.9%C, 1% Mn Alnico 5 8% Al, 24% Co, 3% Cu, 14% Ni ‘Ferroxdur’ (BaO)(Fe2 O3 )6 ESD Fe–Co Alnico 9 SmCo5 Nd2 Fe14 B

4.0 × 103

0.9

8 × 102

4.6 × 104 1.6 × 105 8.2 × 104 1.3 × 105 7 × 105 8.8 × 105

1.25 0.35 0.9 1.05 0.8 1.2

2 × 104 1.2 × 104 4 × 104 105 2 × 105 3 × 105

cannot easily be separated owing to their similar chemical properties. However, once the problem of separation was satisfactorily solved (early 1970s) these magnets could be produced at an economic price. Their ﬁrst champion was the samarium–cobalt alloy SmCo5 , produced by powdering and sintering. The next major advance owed its existence to political upheavals in Africa. Uncertainties in the supply of cobalt, not to mention a ﬁve-fold price increase, lent some urgency to the development of a cobalt-free permanent magnet. Experiments involving boron led to new (occasionally serendipitous) discoveries, culminating in the development of the Nd2 Fe14 B, which became known as ‘neo’ magnets, referring not so much to their novelty (although new they were) but to their neodymium content. They hold the current record of (BH)max = 400 kJ m–3 obtained under laboratory conditions. The commercially available value is about 300 kJ m–3 , as may be seen in Table 11.2. They have, though, the major disadvantage of a fairly low Curie temperature. Note that these new materials have radically different looking hysteresis curves as shown in Fig. 11.12 for the second quadrant only. Let us see now two rather revealing indications of progress. As shown in Fig. 11.13, the introduction of new magnetic materials led to quite signiﬁcant shrinking of the magnetic circuit of a moving-coil meter. Our second example is the historical development of the maximum value of (BH)max shown in Fig. 11.14. The points labelled 1–3 are steels, 4–8 are alnicos, and 9–12 are rare-earth magnets. The increase may be seen to be roughly exponential, a factor of 200 in a century—not as spectacular as the improvement in the attenuation of optical ﬁbres, but one certainly gains the impression of steady advance. For the properties of a number of hard magnetic materials, see Table 11.2.

1.4

Sm(Co,Fe,Cu,Zr)

T Nd–Fe–B

Sm Co5 800

400 kA m–1

0 0

Fig. 11.12 Hysteresis curves of some rare-earth magnets in the second quadrant.

11.7 Microscopic theory (quantum-mechanical) Classical theory gives a reasonable physical picture of what is happening in a magnetic material and does give some guidance to people searching for new materials.∗ The question arises whether we should discuss quantum theory as well. I would like to advise against excessive optimism. Do not expect too much; the situation is not as cheerful as for semiconductors, where the injection of a tiny dose of quantum theory sufﬁced to explain all the major phenomena. The same is not true for magnetism. The quantum theory of magnetism is much

∗ The

theory we have discussed so far is not really consistent because classical theory cannot even justify the existence of atoms and so cannot provide any good reasons for the presence of circulating electronic currents in a material.

274

Magnetic materials Cobalt steel Tungsten steel

Iron

Iron

Alnico 2

Alnico 5 SmCo

Fig. 11.13 The evolution of the magnetic circuit of moving-coil meters reﬂects the progress in magnet materials development. Coil size and magnetic ﬁeld are equal in all ﬁve sketches.

Iron

Iron

Iron

1000 12

500 (BH)max(kJ m–3)

11 10

200

9 8

100

7

50

6

20

5

10

3

4

5 2 2

Fig. 11.14 The achieved optimal value of (BH)max against time.

1

1 1880

1900

1920

1940 Year

1960

1980

2000

more complicated and much less useful to an engineer. The most important activity, the search for better magnetic materials, is empirical anyway, and there are not many magnetic devices clamouring for quantum theory to solve the riddle of their operation. I do think, however, that a brief look into the quantum theory of magnetism will yield some dividends. It is worth learning, for example, how quantum numbers come into the picture. We have, after all, come across them when studying the hydrogen atom, so it is not unreasonable to expect them to be able to say something about magnetic properties. It is also worth knowing that there is a very simple experiment showing the quantized nature of magnetic

Microscopic theory (quantum-mechanical) moments, and there are quite a number of devices which need quantum theory for their description. So let me describe the basic concepts. First, we should ask how much of the previously outlined theory remains valid in the quantum-mechanical formulation. Not a word of it! There is no reason whatsoever why a classical argument (as, for example, the precession of magnetic dipoles around the magnetic ﬁeld) should hold water. When the resulting formulae turn out to be identical (as, for example, for the paramagnetic susceptibility at normal temperatures), it is just a lucky coincidence. So we have to start from scratch. Let us ﬁrst talk about the single electron of the hydrogen atom. As we mentioned before, the electron’s properties are determined by the four quantum numbers n, l, ml , and s, which have to obey certain relationships between themselves; as for example, that l must be an integer and may take values between 0 and n – 1. Any set of these four quantum numbers will uniquely determine the properties of the electron. As far as the speciﬁc magnetic properties of the electron are concerned, the following rules are relevant: 1. The total angular momentum is given by = ℏ{ j( j + 1)}1/2 ,

(11.33)

where j = l + 12 , that is a combination of the quantum numbers l and s. 2. The possible components of the angular momentum along any speciﬁed direction∗ are determined by the combination of ml (which may take on any integral value between –l and +l) and s, yielding j, j – 1, . . . , –j + 1, –j. Taking as an example a d-electron, for which l = 2, the total angular momentum is 5 7 · =ℏ 2 2

1/2

ℏ√ 35, = 2

is sheer nonsense classically because, according to classical mechanics, once the angular momentum is known about three axes perpendicular to each other, it is known about any other axes (and it will not therefore take necessarily integral multiples of a certain unit). In quantum mechanics we may know the angular momentum about several axes but not simultaneously. Once the angular momentum is measured about one axis, the measurement will alter the angular momentum about some other axis in an unpredictable way. If it were otherwise, we would get into trouble with the uncertainty relationship. Were we to know the angular momentum in all directions, it would give us the plane of the electron’s orbit. Hence, we would know the electron’s velocity in the direction of the angular momentum vector (it would be zero), and also the position (it would be in the plane perpendicular to the angular momentum in line with the proton). But this is forbidden by the uncertainty principle, which says that it is impossible to know both the velocity and the position coordinate in the same direction as the velocity.

(11.34) 3h/2

5 3 ℏ ℏ 3 5 ℏ, ℏ, , – , – ℏ, – ℏ 2 2 2 2 2 2

h/2

as shown in Fig. 11.15. 3. The quantum-mechanical relationship between magnetic moment and angular momentum is nearly the same as the classical one, represented by eqn (11.8) e . 2m

∗ This

5h/2

and its possible components along (say) the z-axis are

μm = g

275

–h/2

–3h/2

(11.35)

The only difference is the factor g (admirably called the g-factor). For pure orbital motion its value is 1; for pure spin motion its value is 2; otherwise it is between 1 and 2.

–5h/2

Fig. 11.15 The possible directions of the angular momentum vector for a d-electron.

276

∗ Discovered

well before the advent of quantum mechanics. Pieter Zeeman received the Nobel Prize for it in 1902.

The term –eℏ/2m is called a Bohr magneton and denoted by μmB .

Magnetic materials 4. Energy levels split in the presence of a magnetic ﬁeld. The splitting is proportional to the magnetic ﬁeld. This is known as the Zeeman effect.∗ In quantum-mechanical terms this means that the energy of a magnetic dipole in a magnetic ﬁeld H (taken in the z-direction) may be written as Emag = –(μm )z μ0 H = –gez μ0

H . 2m

(11.36)

We may rewrite eqn (11.36) in the form, Emag = gμmB z μ0

H , ℏ

(11.37)

where z /ℏ, as we have seen before, may take the values j, j – 1, etc. down to –j. We now know everything about the magnetic properties of an electron in the various states of the hydrogen atom. In general, of course, the hydrogen atom is in its ground state, for which l = 0 and ml = 0, so that only the spin of the electron counts. The new quantum number j comes to 21 , and the possible values of the angular momentum in any given direction are ℏ/2 and –ℏ/2. Furthermore, g = 2, and the magnetic moment is The magnetic moment of hydrogen happens to be one Bohr magneton.

μm = μmB .

(11.38)

We can get the magnetic properties of more complicated atoms by combining the quantum numbers of the individual electrons. There exists a set of rules (known as Hund’s rules) that tell us how to combine the spin and orbital quantum numbers in order to get the resultant quantum number J . The role of J for an atom is exactly the same as that of j for an electron. Thus, for example, the total angular momentum is given by = ℏ {J (J + 1)}1/2 ,

(11.39)

and the possible components of the angular momentum vector along any axis by ℏ J , ℏ (J – 1), . . . , ℏ (–J + 1), –ℏ J . The general rules are fairly complicated and can be found in textbooks on magnetism. I should just like to note two speciﬁc features of the magnetic properties of atoms: 1. Atoms with ﬁlled shells have no magnetic moments (this is because the various electronic contributions cancel each other); 2. The spins arrange themselves so as to give the maximum possible value consistent with the Pauli principle. It follows from (1) that helium and neon have no magnetic moments; and stretching the imagination a little one may also conclude that hydrogen, lithium, and silver, for example, possess identical magnetic properties (because all of them have one outer electron).

Microscopic theory (quantum-mechanical) (a)

1s

2s

277

2p

B

C

N (b) 1s

2s

2p

3s

3p

3d

4s

Cr Mn

Fe

Co

Ni

Fig. 11.16 The electron conﬁgurations of (a) boron, carbon, and nitrogen and (b) chromium, manganese, iron, cobalt, and nickel.

The consequences of (2) are even more important. It follows from there that states with identical spins are occupied ﬁrst. Thus, boron with a conﬁguration 1s2 2s2 2p1 has one electron with spin ‘up’ in the outer shell [see Fig. 11.16(a)]; carbon has two electrons with spin up, and nitrogen has three. Similarly all ﬁve electrons of chromium and manganese in the 3d shell have spins up, and the states with opposite spins start to ﬁll up only later, when there is no alternative. This is shown in Fig. 11.16(b), where the electronic conﬁgurations are given for chromium, manganese, iron, cobalt, and nickel. We shall return to the spins of the 3d electrons a little later; ﬁrst let me summarize the main points of the argument. The most important thing to realize is that electrons in an atom do not act individually. We have no right to assume (as we did in the classical treatment) that all the tiny electronic currents are randomly oriented. They are not. They must obey Pauli’s principle, and so within an atom they all occupy different states that do bear some strict relationships to each other. The resultant angular momentum of the atom may be obtained by combining the properties of the individual electrons, leading to the quantum number J , which may also be zero. Thus an atom that contains many ‘magnetic’ electrons may end up without any magnetic moment at all. You may ask at this stage what is the evidence for these rather strange tenets of quantum theory? Are the magnetic moments of the atoms really quantized? Yes, they are. The experimental proof actually existed well before the theory was properly formulated.

278

Magnetic materials

11.7.1 Otto Stern received the Nobel Prize in 1943.

The Stern–Gerlach experiment

The proof for the existence of discrete magnetic moments was ﬁrst obtained by Stern and Gerlach in an experiment shown schematically in Fig. 11.17. Atoms of a chosen substance (it was silver in the ﬁrst experiment) are evaporated in the oven. They move then with the average thermal velocity, and those crossing the diaphragms S1 and S2 may be expected to reach the target plane in a straight line—provided they are non-magnetic. If, however, they do possess a magnetic moment, they will experience a force expressed by F = (μm )z μ0

∂H . ∂z

(11.40)

Thus, the deﬂection of the atoms in the vertical plane depends on the magnitude of this force. ∂H/∂z is determined by the design of the magnet [a strong variation in the z-component of the magnetic ﬁeld may be achieved by making the upper pole piece wedge-shaped as shown in Fig. 11.17(b)] and is a constant in the experiment. Hence, the actual amount of deﬂection is a measure of (μm )z . Were the magnetic moments entirely randomly oriented, the trace of the atoms on the target plane would be a uniform smear along a vertical line. But that is not what happens in practice. The atoms in the target plane appear in distinct spots as shown in Fig. 11.17(c). For silver J = 21 , and the beam is duly split into two, corresponding with the angular momenta z = ℏ/2 and –ℏ/2. If the experiment is repeated with other substances, the result is always the same. One gets a discrete number of beams, corresponding with the discrete number of angular momenta the atom may have.

11.7.2

Paramagnetism

We are now in a position to work out, with the aid of quantum theory, the paramagnetic susceptibility of a substance containing atoms with quantum numbers, J = 0. When we apply a magnetic ﬁeld, all the atoms will have some magnetic moments in the direction of the magnetic ﬁeld. The relative numbers of atoms, possessing the same angular momentum, are determined again by Boltzmann statistics. The mathematical procedure for obtaining the

Target plane S1 Oven

S2

Target plane

Magnet N

Atoms deposited

S (a)

Fig. 11.17 Schematic representation of the Stern–Gerlach experiment.

(b)

(c)

Microscopic theory (quantum-mechanical)

279

average magnetic moment is analogous to the one we used for electric dipoles but must now be applied to a discrete distribution. The possible magnetic moments are MJ gμmB ,

where MJ = J , J – 1, . . . , –J + 1, –J .

Hence, their energies are Emag = –MJ gμmB μ0 H,

(11.41)

and the average magnetic moment may be obtained in the form, J MJ gμmB exp(MJ gμmB μ0 H/kB T) μm = –J J . –J exp(MJ gμmB μ0 H/kB T)

(11.42)

The macroscopic magnetic moment may now be calculated by multiplying μm by the number of atoms per unit volume. Equation (11.42) turns out to be a very accurate formula∗ for describing the average magnetic moment as shown in Fig. 11.18, where it is compared with the experimental results of Henry on potassium chromium alum. The vertical scale is in Bohr magnetons per ion. Note that experimental results for paramagnetic properties are often given for ions embedded in some salt. The reason being that in these compounds the ions responsible for magnetism (Cr3+ in the case of potassium chromium alum) are sufﬁciently far from each other for their interaction to be disregarded. If the exponent is small enough, the exponential function may be expanded to give J –J MJ (1 – MJ gμmB μ0 H/kB T) μm = –gμmB J –J (1 – MJ gμmB μ0 H/kB T) =

J g2 μ2mB μ0 H 2 MJ , (2J + 1)kB T

∗ We

need not be too impressed by these close agreements between theory and experiments. The theoretical curve was not calculated from ﬁrst principles, in the sense that the value of J was arrived at by semi-empirical considerations. The problem is far too difﬁcult to solve exactly. The usual approach is to set up a simple model and modify it (e.g. by taking account of the effect of neighbouring atoms) until theory and experiment agree. It is advisable to stop rather abruptly at that point because further reﬁnement of the model might increase the discrepancy.

(11.43)

–J

because J

MJ = 0.

(11.44)

–J

Bohr magnetons/ion

3

2

1

0 0

Fig. 11.18 1

2

3

4 H/T

The magnetic moment as a function of H/T for potassium chromium alum (after Henry).

280

Magnetic materials The summation in eqn (11.43) is one of the simpler ones to perform, yielding 1 3 J (J

+ 1)(2J + 1),

which gives ﬁnally μm = g2 μ2mB J (J + 1)μ0 H/3kB T.

(11.45)

We may now express the above equation in terms of the total angular momentum, = ℏ{J (J + 1)}1/2

(11.46)

and total magnetic momentum μm = ge/2m

(11.47)

μm = μ2m μ0 H/3 kB T,

(11.48)

to get

∗ This

perhaps shows the power of human imagination. If one has a fair idea how the ﬁnal conclusion should look, one can get a reasonable answer in spite of following a false track.

in agreement with the classical result.∗

11.7.3

Paramagnetic solids

As we have seen, the magnetic properties of electrons combine to produce the magnetic properties of atoms. These properties can be measured in a Stern– Gerlach apparatus, where each atom may be regarded as a separate entity. This is because the atoms in the vapour are far enough from each other not to interact. However, when the atoms aggregate in a solid, the individual magnetic properties of atoms combine to produce a resultant magnetic moment. The electrons that are responsible for chemical bonding are usually responsible for the magnetic properties as well. When, for example, sodium atoms and chlorine atoms combine to make up the ionic solid, NaCl, then the valence electron of the sodium atom moves over to the chlorine atom and ﬁlls up the shell. Hence, both the sodium and the chlorine ions have ﬁlled shells, and consequently, solid NaCl is non-magnetic. A similar phenomenon occurs in the covalent bond, where electrons of opposite spin strike up a durable companionship, and as a result, the magnetic moments cancel again. How then can solids have magnetic properties at all? Well, there is ﬁrst the metallic bond, which does not destroy the magnetic properties of its constituents. It is true that the immobile lattice ions have closed shells and hence no magnetic properties, but the pool of electrons does contribute to magnetism, owing to their spin. Some spins will be ‘up’ (in the direction of the magnetic ﬁeld); others will be ‘down’. Since there will be more up than down, the susceptibility of all metals has a paramagnetic component, of the order of 10–5 . This is about the same magnitude as that of the diamagnetic component; hence some metals are diamagnetic. Another possibility is offered by salts of which potassium chromium alum is a typical example. There again, as mentioned above, the atoms responsible for the magnetic properties, being far away from each other, do not interact. In these compounds, however, the atoms lose their valence electrons; they are needed for the chemical bond. Hence, the compound will have magnetic

Microscopic theory (quantum-mechanical)

281

properties only if some of the ions remain magnetic. This may happen in the so-called ‘transition elements’, which have unﬁlled inner shells. The most notable of them is the 3d shell, but Table 4.1 shows that the 4d, 4f, 5d, and 5f shells have similar properties. Taking chromium again as an example, it has a valency of two or three; hence, in a chemical bond it must lose its 4s electron [see Fig. 11.16(b)] and one or two of its 3d electrons. The important thing is that there are a number of 3d electrons left that have identical spins, being thus responsible for the paramagnetic properties of the salt.

11.7.4

Antiferromagnetism

Let us now study the magnetic properties of solid chromium. From what we have said so far, it would follow that chromium is a paramagnetic solid with a susceptibility somewhat larger than that of other metals because free electrons contribute to it, and the lattice ions are magnetic as well. These expectations are not entirely false, and this is what happens above a certain temperature, the Néel temperature (475 K for chromium). Below this temperature, however, a rather odd phenomenon occurs. The spins of the neighbouring atoms suddenly acquire an ordered structure; they become antiparallel as shown in Fig. 11.19. This is an effect of the ‘exchange interaction’, which is essentially just another name for Pauli’s principle. According to Pauli’s principle, two electrons cannot be in the same state unless their spins are opposite. Hence, two electrons close to each other have a tendency to acquire opposite spins. Thus, the electron-pairs participating in covalent bonds have opposite spins, and so have the electrons in neighbouring chromium atoms. Besides chromium, there are a number of compounds like MnO, MnS, FeO, etc. and another element, manganese (Néel temperature 100 K) that have the same antiferromagnetic properties. Antiferromagnetics display an ordered structure of spins; so in a sense, they are highly magnetic. Alas, all the magnetic moments cancel each other (in practice nearly cancel each other) and there are therefore no external magnetic effects.

11.7.5

Louis Néel received the Nobel Prize in 1970.

(a)

Ferromagnetism

Leaving chromium and manganese, we come to iron, cobalt, and nickel, which are ferromagnetic. In a ferromagnetic material the spins of neighbouring atoms are parallel to each other [Fig. 11.19(b)]. Nobody quite knows why. There seems to be general agreement that the exchange interaction is responsible for the lining up of the spins (as suggested ﬁrst by Heisenberg in 1928) but there is no convincing solution yet. The simplest explanation (probably as good as any other) is as follows. Electrons tend to line up with their spins antiparallel. Hence, a conduction electron passing near a 3d electron of a certain iron atom will acquire a tendency to line up antiparallel. When this conduction electron arrives at the next iron ion, it will try to make the 3d electron of that atom antiparallel to itself; that is, parallel to the 3d electron of the previous iron atom. Hence, all the spins tend to line up.

(b)

(c)

Fig. 11.19 The angular momentum vector for (a) antiferromagnetic, (b) ferromagnetic, and (c) ferrimagnetic materials.

282

Magnetic materials

∗ F.

Keffer, Magnetic properties of materials, Scientiﬁc American, September 1967.

In Weiss’s classical picture the magnetic moments are lined up by a longrange internal ﬁeld. In the quantum picture they are lined up owing to nearest-neighbour interaction. ‘One is reminded,’ writes Keffer∗ , ‘of the situation when, as the quiet of evening descends, suddenly all the dogs in a town get to barking together, although each dog responds only to the neighbouring dogs.’

11.7.6

Ferrimagnetism

This type of magnetism occurs in compounds only, where the exchange interaction causes the electrons of each set of atoms to line up parallel, but the two sets are antiparallel to each other. If the magnetic moments are unequal, then we get the situation shown in Fig. 11.19(c), where the resultant magnetic moment may be quite large. For most practical purposes ferrimagnetic materials behave like ferromagnetics but have a somewhat lower saturation magnetization.

11.7.7

Garnets

This is the name for a class of compounds crystallizing in a certain crystal structure. As far as magnetic properties are concerned, their most interesting representative is yttrium-iron garnet (Y3 Fe5 O12 ), which happens to be ferromagnetic for a rather curious reason. The spin of the yttrium atoms is opposite to the spin of the iron atoms, so the magnetic moments would line up alternately—if the orbital magnetic moments were small. But for yttrium the orbital magnetic moment is large, larger actually than the spin, and is in the opposite direction. Hence, the total magnetic moment of the yttrium atom is in the same direction as that of iron, making the compound ferromagnetic.

11.7.8

Helimagnetism

You may wonder why the magnetic moments of neighbouring atoms in an ordered structure are either parallel or antiparallel. One would expect quantum mechanics to produce a larger variety. In actual fact, there are some materials in which the spins in a given atomic layer are all in the same direction, but the spins of adjacent layers lie at an angle (e.g. 129◦ in MnO2 below a certain temperature), producing a kind of helix. For the moment this is a scientiﬁc curiosity with no practical application.

Emag

MJ = 1

11.8 ΔE

11.8.1

MJ = 0 H ΔE MJ = –1

Fig. 11.20 The energy of an atom as a function of magnetic ﬁeld for J = 1.

Magnetic resonance Paramagnetic resonance

The possible energies of an atom in a magnetic ﬁeld are given by eqn (11.41). There are 2 J + 1 energy levels, with separations of E = gμmB μ0 H, as shown in Fig. 11.20 for J = 1. We now put a sample containing magnetic atoms (e.g. a paramagnetic salt) into a waveguide and measure the transmission of the electromagnetic waves as a function of frequency. When f = E/h, the incident photon has just the right energy to excite the atom from a lower energy level into a higher energy level. Thus, some of the photons transfer their energies to the atomic system; this

means loss of photons, or in other words, absorption of electromagnetic energy. Hence, there is a dip in the transmission spectrum as shown in Fig. 11.21. Since the absorption occurs rather sharply in the vicinity of the frequency E/h, it is referred to as resonant absorption, and the whole phenomenon is known as paramagnetic resonance. In practice the energy diagram is not quite like the one shown in Fig. 11.20 (because of the presence of local electric ﬁelds) and a practical measuring apparatus is much more complicated than our simple waveguide (in which the absorption would hardly be noticeable) but the principle is the same.

11.8.2

283

Transmission

Magnetic resonance

1

ΔE h

Electron spin resonance

This is really a special case of paramagnetic resonance, when only the spin of the electron matters. It is mainly used by organic chemists as a tool to analyse chemical reactions. When chemical bonds break up, electrons may be left unpaired, that is the ‘fragments’ may possess a net spin (in which case they are called free radicals). The resonant absorption of electromagnetic waves indicates the presence of free radicals, and the magnitude of the response can serve as a measure of their concentration.

Fig. 11.21 Transmission of electromagnetic waves as a function of frequency through a paramagnetic material. There is resonant absorption where hf = E.

11.8.3 Ferromagnetic, antiferromagnetic, and ferrimagnetic resonance When a crystal with ordered magnetic moments is illuminated by an electromagnetic wave, the mechanism of resonant absorption is quite complicated, owing to the interaction of the magnetic moments. The resonant frequencies cannot be predicted from ﬁrst principles (though semiclassical theories exist) but they have been measured under various conditions for all three types of materials.

11.8.4

Nuclear magnetic resonance

If electrons, by virtue of their spins, can cause resonant absorption of electromagnetic waves, one would expect protons to behave in a similar manner. The main difference between the two particles is in mass and in the sign of the electric charge; so the analogous formula, f =

e 1 g μ0 H, 2π 2mp

(11.49)

should apply. The linear dependence on magnetic ﬁeld is indeed found experimentally, but the value of g is not 2 but 5.58, indicating that the proton is a more complex particle than the electron. Neutrons also possess a spin, so they can also be excited from spin ‘down’ into spin ‘up’ states. Although they are electrically neutral, the resonant frequency can be expressed in the same way, and the measured g-factor is 3.86. The resonance is sharp in liquids but broader, by a few orders of magnitude, in solids. The reason for this is that the nuclear moments are affected by the local ﬁelds, which may vary in a solid from place to place but average to zero in a liquid.

mp is the mass of the proton.

f

284

Magnetic materials Since both the shape of the resonant curve and the exact value of the resonant frequency depend on the environment in which a nucleus ﬁnds itself, nuclear magnetic resonance can be used as a tool to investigate the properties of crystals. An important application in a different direction is the precision measurement of magnetic ﬁelds. The proton resonance of water is generally used for this purpose. The accuracy that can be achieved is about 1 part in 106 . The most important application of Nuclear Magnetic Resonance is of course in imaging, which was not even mentioned in the ﬁrst edition of this book. Maybe it should have been mentioned because the principle was already known but its ﬁrst, rather crude demonstration was still two years away. We shall atone for our past omission by discussing Magnetic Resonance Imaging (MRI) in more detail in Appendix VII devoted to Medical Imaging. The importance of MRI was acknowledged by the award of the Nobel Prize in 2003 to Paul Lauterbur and Peter Mansﬁeld, who made it practical.

11.8.5

Cyclotron resonance

We have already discussed the phenomenon of cyclotron resonance from a classical point of view, and we shall now consider it quantum mechanically. For resonant absorption one needs at least two energy levels or, even better, many energy levels equally spaced from each other. What are the energy levels of an electron in a solid? Remember that in our earlier model we neglected the interaction between electrons and simply assumed that the solid may be regarded as an inﬁnte potential well. The possible energy levels were then given by eqn (6.2), E=

∗ The

effect of the magnetic ﬁeld may be taken into account by replacing p2 by (p – eA)2 in the Hamiltonian of Schrödinger’s equation (where A is the vector potential).

ℏ2 ℏ2 2 (kx + ky2 + kz2 ) = (n2 + n2y + n2z ), 2m 8 m(2a)2 x

where nx , ny , nz are integers. When a magnetic ﬁeld is applied in the z-direction, then the above equation modiﬁes to∗ ℏ2 2 1 ℏωc + k , E = λ+ 2 2m z

(11.50)

where λ is an integer and ωc is the cyclotron frequency. For constant kz , the difference between the energy levels (called Landau levels) is ℏωc . Hence, we may look upon cyclotron resonance as a process in which electrons are excited by the incident electromagnetic wave from one energy level to the next.

11.9

The quantum Hall effect

Strictly speaking this does not belong to magnetic resonance (although Landau levels are involved) and may be a little out of place in an engineering textbook. The argument for including it is that there might be some relationship to high temperature superconductivity (see Section 14.9) which is of great practical signiﬁcance, and it is also true that the effect would have never been discovered had engineers not invented ﬁeld-effect transistors, whose operation depended on a two-dimensional electron gas (see Section 9.14).

You may remember the discussion of the ordinary Hall effect in Chapter 1. The experimental set-up for the quantum Hall effect is exactly the same. The only difference is that the dimension of the current channel perpendicular to the applied magnetic ﬁeld is now comparable with the electron wavelength. ~ 10 T) The requirements for observing the effect are high magnetic ﬁelds (B = and low temperatures, say a few K. The measured value is the so-called Hall resistance, which relates the measured transverse voltage (Hall voltage) to the longitudinal current. Since the Hall voltage is known to be proportional to the applied magnetic ﬁeld [eqn (1.20)] we would expect the Hall resistance versus longitudinal current curve to vary linearly with B. The striking result is that the Hall resistance turns out to be independent of the magnetic ﬂux density within certain intervals as shown in Fig. 11.22. It looks as if the Hall resistance is quantized. How can we explain these results? Surely, if something is quantized, we need quantum theory to explain it. Unfortunately, quantum theories are complicated, so one tries to avoid them. That is what we did in Section 8.4, where relationships for the mobilities of semiconductors were derived. In order to explain the present results there is, however, no reprieve. We have to approach the concept of resistance from an entirely different viewpoint, from that of quantum mechanics. Classically, a piece of resistive material always leads to power absorption. In quantum mechanics we have to ask the question whether an electron is capable of absorbing the energy available. It can only do so if there are empty states at a higher energy into which the electrons can scatter, so we need to ﬁnd out whether there are any empty states available. Let us assume that the temperature is low enough and the magnetic ﬁeld is high enough, so that only the two lowest Landau levels are occupied. The lowest energy level is completely ﬁlled, the second energy level is partially ﬁlled, and the third level is empty. If the magnetic ﬁeld is reduced, then the energy difference between the second and ﬁrst Landau levels is reduced, consequently some electrons must move up from the ﬁrst level to the second level. That means that there are now fewer states at the second level, which an electron can scatter into, hence the probability of transition is smaller, and the resistance (we are talking about longitudinal resistance not Hall resistance) decreases. If the magnetic ﬁeld is further reduced, then at a certain stage the second Landau level will be completely ﬁlled. The only way an electron in the ground state can now absorb energy is by scattering into the third Landau level, but that is too far away. Hence, the probability of scattering into that level is extremely low, which means that the resistance is extremely low. In practice, this resistance would be low indeed, lower than that of copper. Let us now slightly complicate our model and assume that there are some impurity states just below the third Landau level, as shown in Fig. 11.23. The argument for the longitudinal resistance is unaffected: the impurity states are still very far away from the second Landau level. But let us return to the Hall resistance. How will it vary as the magnetic ﬁeld is reduced? The electrons moving into the impurity levels will no longer be available for deﬂection by the magnetic ﬁeld, hence the Hall resistance must remain constant until all the impurity levels are ﬁlled. In the Hall resistance versus magnetic ﬁeld curve this appears as a plateau, whenever a Landau level is ﬁlled. The discrete values

285

Hall resistance

The quantum Hall effect

B

Fig. 11.22 The Hall resistance against magnetic ﬂux density shows distinct plateaus.

Magnetic materials

Energy

286

Fig. 11.23 Discrete energy levels in high magnetic ﬁelds.

3rd Landau level impurity level

2nd Landau level

of the Hall resistance at these plateaus turn out to be dependent only on the fundamental constants h and e and on the number of Landau levels ﬁlled.

11.10

∗ Nobel

† In

Prize in Physics in 2007.

Greek mythology, you may remember, giants challenged the gods but it was not a wise move. The gods, reinforced by Heracles, killed them all off.

Magnetoresistance

The subject has become very popular in the last decade or so but it is not new. It has been around for a century and a half. The effect was ﬁrst observed by Lord Kelvin (William Thomson at the time) in 1857, when he found a few per cent change in electrical resistance depending on the direction of the applied magnetic ﬁeld, whether it was in the same direction or transverse to the ﬂow of the electrons. The effect has become known as anisotropic magnetoresistance. A qualitative description can be based on the Lorenz force. In the presence of a magnetic ﬁeld the electron ﬂow is deﬂected, hence there can be a change in scattering which leads to a changed resistance. In good metals like iron and cobalt the magnetoresistance is indeed a small effect. The change in resistivity is of the order of 0.5 to 3%. It was found in 1988 by Fert and Grunberg∗ (working independently) that magnetoresistance increases signiﬁcantly in multilayer ferromagnetic thin ﬁlms. They called it ‘giant magnetoresistance’, abbreviated as GMR. It is not obvious that ‘giant’ is the right adjective to use because the resistance changed by no more than a factor of two. On the other hand, if we think of giants† we imagine them just about twice the size of homo sapiens. So after all we can use the term with clear conscience. We should also mention here Colossal Magnetoresistance, which can cause changes in current by a factor of several thousand. It has though an entirely different mechanism, related to a magnetically induced metal-to-insulator phase transition. It seems less signiﬁcant at the moment because it has not been harnessed for practical applications. Let us now think of an explanation based on quantum mechanics. We may ﬁrst ask the question of how the band structure of magnetic materials is related to resistance. As we know (see Table 4.1 and Fig. 11.16), magnetic elements from chromium to nickel have partially ﬁlled 3d bands whereas in copper the 3d band is ﬁlled. If we apply a voltage to a specimen of these materials we ﬁnd that the magnetic materials have high resistivity in contrast with copper which is close to having the lowest resistivity of all materials. The number of electrons available in the conduction band is not much different, so what is the reason? It must be low mobility or in other words low relaxation time. In copper when an electron bumps into the lattice or scatters for any other reason, it has nowhere to go; well nowhere relative to an electron in, say, nickel. The scattered electron has then a temporary resting place in the partially ﬁlled 3d band so it does not participate in conduction. Its mobility is reduced. Interestingly this effect also applies inside a ferromagnetic material. Since the ﬁlling of the 3d band is spin

Spintronics

287

dependent, one of the spin species has a higher chance of getting scattered from a 4s state into an empty 3d state. Because of its reduced mobility this spin will contribute less to the total current. The dependence of resistance on spin is the phenomenon that launched the new discipline of spin electronics or brieﬂy, spintronics.

11.11

Spintronics

With the discovery of giant magnetoresistance, spin entered the minds of engineers. Until then conventional electronics always, without exception, ignored spin. But all that changed in 1988. The effect of spin has been the subject of intensive research ever since. Commercial applications are not far away as will be discussed in Section 11.12 and in Appendix VI, devoted entirely to the physical principles on which memory elements have been working or might work in the future.

11.11.1 Spin current We know what current is. The substances may be different but the deﬁnition is always the same. We measure current by counting the number of elements (whatever they are) passing through a cross-section in unit time. The substance could be water (we talk then of a stream, a brook, or a river), it can be oil or gas (which ﬂows in pipes), or electrons (which ﬂow in conductors). Spin current is not analogous to any of these. It arises when the two different kinds of spin, up and down, are not in equilibrium. One kind is more numerous than the other. To ﬁnd out more about spin let us set up the experiment shown in Fig. 11.24(a). There are two materials connected to each other, a ferromagnetic material, F, and a non-magnetic metal, N, and there is a voltage applied between the two materials. We can easily predict what would happen. Both materials are conductors so electrons will ﬂow from the ferromagnetic material into the nonmagnetic metal. That is obvious. There is now a current: an electron current. To emphasize the difference between the ﬂow of electrons and the ﬂow of the electron spin we shall often refer to the former as charge current. What else is there to say? Thirty years ago we would have said: ‘That’s all. There is nothing else we need to think about.’ But ever since the discovery of giant magnetoresistance we have become spin-conscious. We should ask now: ‘What about the spin?’ Let us start by saying that the magnetism in F is polarized. The electrons (say) have spin up. Obeying the electric ﬁeld that has been set up, many of them will move into N. If the spin of the electron that moved over was up in F, then surely its spin will still be up when it crosses the boundary into N. An electron is not so oblivious as to forget its past history. But, the next question is, how long can it keep its spin up while moving in the non-magnetic metal? Clearly, those spin-up electrons ﬁnd themselves in an entirely different environment, one might even say a hostile environment. All the physical phenomena taking place in the non-magnetic material conspire against them. They will be knocked off their privileged position by the various scattering phenomena. What can they do? They cannot vanish. Electrons will remain electrons.∗ Thus all they can do is to turn into spin-down electrons. But if the number

(a)

F

N

(b) M

δM

Position

Fig. 11.24 (a) Voltage applied to an F–N junction (between a ferromagnetic and a non-ferromagnetic material). (b) The resulting spatial distribution of magnetization. ∗ We

are not concerned with particle physics.

288

Magnetic materials of spin-up electrons declines and the number of spin-down electrons increases then it is not unreasonable to talk about a spin current. Theoretical physicists have quite a complicated deﬁnition: they say the spin current is a tensor. We don’t need to go into any of the complications. We shall just use the simpliﬁed deﬁnition,

(a)

J = Jup – Jdown . F1

N

F2

F1

N

F2

(b)

Fig. 11.25 Voltage applied to an F–N–F junction. The spin orientations of the two ferromagnetic materials are (a) in the same direction, and (b) in the opposite direction.

∗ The idea came from Mott (Nobel Prize,

1977) in the 1930s. The two types of spin are responsible for two different kinds of current. The spins which scatter less encounter less resistance, and those which scatter more are presented with a higher resistance.

Gate

Source

Oxide

Drain

Silicon substrate

Fig. 11.26 A spin ﬁeld-effect transistor is analogous to its non-magnetic counterpart. The source and drain are constructed of ferromagnetic materials.

(11.51)

The variation of the magnetization in the two materials is shown in Fig. 11.24(b). There is a tendency towards spin equilibrium in N, hence the spin current must decline. How fast will it decline? We may introduce a ‘diffusion length’ or ‘coherence length’ to describe the distance, after which the number of electrons with spin up declines by a factor of e. Practical values for a non-magnetic metal are between 100 nm and 1 µm. Note that the coherence length is much longer in semiconductors than in metals. It extends from a few µm to about 100 µm. Have we seen similar phenomena before? The situation is analogous to an n–i junction, i.e. a junction between an n-type and an intrinsic semiconductor. When a forward voltage is applied the electrons are injected into the intrinsic material. There will be an excess of electrons over holes there but eventually that excess disappears. Far away from the junction in the intrinsic material, equilibrium is re-established. Based on the above analogy we can talk about majority and minority electrons. In F, the majority electrons can be spin up or spin down depending on the magnetization. In N there is equilibrium. One cannot talk about majority or minority electrons. It needs to be made clear that whether the spin is up or down in a ferromagnetic material they may still belong to the majority or to the minority. In general, minority electrons in a given ferromagnetic material suffer more scattering, and hence they contribute less to the total current, as if they had to ﬂow through a higher electrical resistance.∗ Continuing with the semiconductor analogy we can make the twosome into a threesome and construct an F1 –N–F2 junction (Fig. 11.25). If the N region is sufﬁciently thin (thinner than the spin diffusion length) then the spin-up current can penetrate the second ferromagnetic material. How will it be received? If F2 is polarized in the same direction as F1 (Fig. 11.25a) then the spin-up electrons can happily continue their journey in F2 . If F2 is polarized in the opposite direction (Fig. 11.25b), then the ex-majority electrons suddenly ﬁnd themselves to be the minority electrons and the current will be much less. Clearly this effect is important for applications. The current is large or small depending on the polarization of F2 . And the effect can be further enhanced by having a large number of alternate layers of ferromagnets and normal metals (the dimensions are in the nanometre range, so practical realizations had to wait for the advent of nanotechnology). What we have described so far is an operation analogous to that of a bipolar transistor. Can we make an analogy of the ﬁeld-effect transistor as well? Yes, all the necessary elements are there. The source and the drain should be made of ferromagnetic materials polarized in the same direction, and the channel could be a semiconductor (see Fig. 11.26). In the presence of an applied drain-source voltage the electrons with the majority spin would be injected into the semiconductor and would carry on into the drain, provided that the path

Spintronics

289

(a) C

B

D (b)

A

E

Ferromagnetic electrodes Non-magnetic material

F

J Jc

Fig. 11.27 Jc = 0

Js

through the semiconductor is short enough. For zero gate voltage the majority electrons would be accepted by the drain leading to a high current. A voltage applied to the gate could then destroy the spin uniformity and a smaller current will appear. Another variant of this three-terminal device would need to satisfy more stringent requirements. In the absence of the gate voltage the electrons arrive with the right spin, and when the gate voltage is switched on they arrive with the opposite, unfavourable, spin.∗ Note that the Spin Field-Effect Transistor has considerable advantages over its non-spin counterpart. The energy to change the spin orientation is less and the time needed to do so is shorter than the corresponding energy and switch time for a traditional transistor. Next let us look at the conﬁguration shown in Fig. 11.27(a), where there are three ferromagnetic electrodes on the top of a non-magnetic metal. This is essentially the same as that shown in Fig. 11.25, where there was a nonmagnetic metal between two ferromagnetic materials. The difference is that we now have a third electrode as well. When a voltage is applied between points B and A, a charge current will ﬂow from B to A along points E and F. At E we shall have a large concentration of spin-up electrons. They diffuse, i.e. the number of spin-up electrons declines, when they reach point F. However diffusion is not only to the right of point E. There is spin diffusion also in the direction to the left. At point E the density of spin-up electrons is high. They are bound to diffuse towards the left as well. Diffusion means that their numbers decline as they turn into spin-down electrons. But that means that the difference between the spin-up and spin-down electrons is continually changing. And that means that there is a spin current ﬂowing from F to D. Electrode C would then sense the change of spin current under it. The variation of charge and spin currents with distance between points D and F is shown in Fig. 11.27(b).

Charge currents and spin currents between ferromagnetic and non-magnetic materials.

∗ This

is known as the Datta–Das SpinField-Effect Transistor.

11.11.2 Spin tunnelling Having looked at the passage of spin polarized electrons from one ferromagnetic material to another via a non-magnetic metal (Fig. 11.25), the idea of a tunnel junction is bound to arise. The tunnelling conﬁguration is only slightly different (see Fig. 11.28). The non-magnetic conductor is now replaced by an insulator that is thin enough for tunnelling to take place. We have seen

F1

I

F2

Fig. 11.28 A ferromagnet–insulator–ferromagnet tunnel junction. The spin polarization remains unchanged after tunnelling.

290

Magnetic materials H M

Fig. 11.29 A propagating spin wave.

before that polarization persists when moving from a ferromagnetic into a nonmagnetic material. The same situation occurs in tunnelling; the polarization persists. A spin-up electron will still be a spin-up electron after it has tunnelled through the insulator. But whether it is cordially welcome in F2 or grudgingly accepted depends on the polarization of F2 whether its electrons are polarized in the same or the opposite direction. If in the same direction, the resistance is low, if in the opposite direction the resistance is high, the same phenomenon that occurred in the conducting device. The difference is that the change in resistance is higher at tunnelling than at conduction by about a factor of 2.

11.11.3 Jc

Spin up

Jc

Spin down

Fig. 11.30 In the presence of a charge current consisting of spin-up and spin-down electrons, it is observed that the different polarizations are deﬂected in opposite directions.

∗ The

coupling between an element’s spin and its orbital magnetism.

† This

follows from the Onsager relations which establish reciprocal relationships between various physical quantities.

Spin waves and magnons

Although spin waves were discovered long before anybody thought of spintronics, I think this is still the best place to brieﬂy describe it. The wave may be characterized by the magnetization vector precessing about an applied magnetic ﬁeld, B, as shown in Fig. 11.29. The wave can also be regarded as a particle (the analogue of the electromagnetic wave–photon duality), in which case it is called a magnon.

11.11.4

Spin Hall effect and its inverse

The conﬁguration in which the spin Hall effect is observed is even simpler than that for the ordinary Hall effect. There is no need for an applied magnetic ﬁeld nor is there a need for a magnetic material. It can be observed in a non-magnetic metal or semiconductor; the only condition is to have spin–orbit interaction∗ and of course a charge current needs to ﬂow. The result is that spin-up and spin-down electrons are deﬂected in opposite directions as shown in Fig. 11.30. Hence at the top of the material, perpendicular to the charge current, there is an excess of spin-up electrons and at the bottom of the material there is an excess of spin-down electrons. Note that there is no charge current in the perpendicular direction but there is a spin current, another example of a pure spin current. This is again something hard to get used to. There is no movement of charge but a spin current is nonetheless present. The inverse effect can also be observed. If a spin current ﬂows, that will induce a charge current perpendicular to it.† The effect is useful for detecting spin current.

11.11.5

Spin and light

We know that both electric and magnetic vectors rotate in circularly polarized light. Hence comes the reasonable hypothesis that spin polarized carriers can

Some applications be excited by circularly polarized light. Such interaction has indeed been reported in GaMnAs. This turns out to be a very fast effect, in the femtosecond range, suggesting direct transformation from the angular momentum of light to magnetic moment.

11.11.6

Spin transfer torque

Spin polarized current is known to exert a torque that can rotate the local magnetic moment when it is injected into a ferromagnetic material. The local magnetic moments feel the torque and start to precess (i.e. spin waves are excited) around the local effective magnetic ﬁeld. This will go on until the local magnetization becomes parallel with the injected spin polarization. Interestingly, the effect is still there in the absence of charge current. Rotation of magnetic moment may also be caused by pure spin current, as has been proved using the conﬁguration of Fig. 11.27(a). In terms of the F1 –N–F2 and F1 –I–F2 sandwiches this means that the polarization of the second ferromagnetic layer could be changed by a spin current injected into it. This provides the basis of a very promising memory element, discussed in A6.3.5. Another effect of spin-transfer torque is to move domain walls by interacting with the magnetic moments present there. The inverse effect may also occur. Spin waves may generate spin currents. The phenomenon is known as spin pumping.

11.12

Some applications

Until the 1950s the only signiﬁcant application was for electrical machines and transformers. Modern technology brought some new applications: most notable among these being the use of magnetism for storing information. In fact, in 1985 for the ﬁrst time, the sales of magnetic products for Information Technology in the USA exceeded those for all other technologies. We shall discuss information storage in more detail in Appendix VI. In the present section we shall brieﬂy mention only four applications, a unique one, as isolators, a general one, as sensors, an old one, magnetic read-heads, and an even older one, electric motors.

11.12.1 Isolators My next example is a device which lets an electromagnetic wave pass in one direction but heavily attenuates it in the reverse direction. It is called an isolator. The version I am going to discuss works at microwave frequencies and uses a ferrite rod, which is placed into a waveguide and biased by the magnetic ﬁeld of a permanent magnet (Fig. 11.31). The input circularly polarized wave may propagate unattenuated, but the reﬂected circularly polarized wave (which is now rotating in the opposite direction) is absorbed. Thus, the operation of the device is based on the different attenuations of circularly polarized waves that rotate in opposite directions. The usual explanation is given in classical terms. We have seen that a magnetic dipole will precess in a constant magnetic ﬁeld. Now if in addition to the constant magnetic ﬁeld in the z-direction there appears a magnetic vector in the x-direction (Fig. 11.32), then there is a further torque acting upon the

291

292

Magnetic materials Permanent magnet or solenoid

Incident circularly polarized wave

Reﬂected circularly polarized wave

Fig. 11.31 Schematic representation of an isolator.

Ferrite rod

y μ Bx

B z

x

Fig. 11.32 The magnetic dipole moment precesses around the constant magnetic ﬁeld, B. An additional magnetic ﬁeld, Bx , gives an extra torque, trying to increase the angle of precession.

Circular waveguide

magnetic dipole. The effect of this torque is insigniﬁcant, except when the extra magnetic ﬁeld rotates with the speed of precession—and, of course, in the right direction. But this is exactly what happens for one of the circularly polarized waves when its frequency is equal to the frequency of precession. The interaction is then strong, and energy is taken out of the electromagnetic wave in order to increase the angle of precession. Hence, for one given frequency (the resonance frequency) and one sense of rotation (that of the reﬂected wave) the electromagnetic wave is absorbed. The quantum explanation is based on the resonance phenomena discussed in the last section. The electromagnetic wave is absorbed because its energy is used to sponsor transitions between the respective energy levels. Unfortunately, quantum mechanics provides no intuitive description of the effect of circularly polarized waves. You either believe that the result comes out of the mathematical description of the problem or, alternatively, you stick to the classical picture. This is what many quantum physicists do, but to ease their conscience, they put the offending noun between inverted commas. They do not claim that anything is really precessing, nonetheless, they talk of ‘precession’.

11.12.2

Sensors

Magnets can be used to sense position, force, torque, speed, rotation, acceleration, and of course current and magnetic ﬁeld. Since the advent of light and powerful neo-magnets, their use has been rapidly expanding, as for example in anti-lock brakes and in activating airbags.

11.12.3

Magnetic read-heads

Practical devices for recording sound appeared in the middle of the 1930s and their video counterparts, which needed a much wider bandwidth, came about 20 years later. The information had to be read by so-called read-heads, which were also suitable for writing the information upon the tape. The revolution in read-heads came with the discovery of the giant magnetoresistance. It was so much better than those existing at the time that they reached commercial application in less than a decade after the discovery, earning billions of dollars for IBM. Interestingly enough their reign was short-lived. Within a few years

Exercises

293

they were supplanted by another magnetoresistive effect based on tunnelling, as discussed in Section 11.11.2.

11.12.4 Electric motors This is one of the oldest applications of magnetism, the conversion of electrical into mechanical power. Have there been any major advances? Well, our illustration of what happened to the magnetic circuit of moving-coil meters (Fig. 11.13) applies just as well to electric motors. They have come down in size, so much so that in a modern motor car there is room for as many as two dozen permanent magnet motors, which drive practically everything that moves (apart from the car, of course). Some forty years ago, all the electric motors that we moved about the laboratory or our homes were ‘fractional horse power’. In fact, a 12 h.p. motor was rather large and heavy. Anything greater than 1 h.p. was classed as ‘industrial’ and had a built-in fan or water cooling. Now our domestic motors are smaller, cooler, and quieter; and where power is needed, such as in portable drills, lawnmowers, and shredders, ratings of up to 1.6 kW (i.e. more than 2 h.p.) are quite common and reasonably portable. What has happened besides the discovery of better magnetic alloys? This is something we should have mentioned in the last chapter in the section about insulators. The makers of motors woke up to the fact that new polymeric insulations were available that were more effective than the brown paper soaked in transformer oil which they had been using for the previous century. I am telling you this story because it illustrates that some improvements in technology, which the public is hardly aware of, can have a signiﬁcant impact upon how we live.

Exercises 11.1. Check whether eqn (11.12) is dimensionally correct. Take reasonable values for Na , Z and r and calculate the order of magnitude of the diamagnetic susceptibility in solids.

(iii) Conﬁrm that in the stable equilibrium position the magnetic ﬁeld of the loop augments the applied ﬁeld. I

11.2. The magnetic moment of an electron in the ground state of the hydrogen atom is 1 Bohr magneton. Calculate the induced magnetic moment in a ﬁeld of 1 T. Compare the two. 11.3. A magnetic ﬂux density, B, is applied at an angle θ to the normal of the plane of a rectangular current loop (Fig. 11.33). (i) Determine the energy of the loop by ﬁnding the work done by the magnetic ﬁeld when lining up (bringing to a stable equilibrium) the loop. (ii) By deﬁning the energy of a magnetic dipole as E = μm · B,

and by identifying the loop with a magnetic dipole, determine the magnetic moment vector of the loop.

θ I B

Fig. 11.33 11.4. How have domains in ferromagnetic materials been observed? 11.5. Check the calculation leading to the values of the Weiss constant, magnetic moment, and saturation magnetization for iron given in eqn (11.28).

Magnetic materials

11.6. Show that the data for the magnetic susceptibility of nickel given below is consistent with the Curie law [eqn (11.26)] and evaluate the Curie constant and temperature. Hence ﬁnd the effective number of Bohr magnetons per atom. Atomic weight 58.7, density 8850 kg m–3 . 500 600 700 800 900 T(◦ C) 10.6 9.73 χm 105 38.4 19.5 15 11.7. An alloy of copper and cobalt consists of spherical precipitates, averaging 10 nm diameter, of pure cobalt in a matrix of pure copper. The precipitates form 2 per cent by volume of the alloy. Cobalt is ferromagnetic, with saturation magnetization of 1.4 MA m–1 . Each cobalt precipitate is a single domain, and acts as a strong dipole, which responds to any external ﬁeld as a paramagnetic dipole. The effect is called ‘superparamagnetism’. Calculate the susceptibility of the alloy at 300 K. [Hint: The total magnetic moment of each precipitate is equal to the product of magnetic moment density (saturation magnetization) with the volume of the precipitate.]

11.10. The energy levels of a free electron gas in the presence of an applied magnetic ﬁeld are shown in Fig. 11.34 for absolute zero temperature. The relative numbers of electrons with spins ‘up’ and ‘down’ will adjust so that the energies are equal at the Fermi level. Show that the paramagnetic susceptibility is given by the approximate expression, χm = μ2m μ0 Z(EF ), where μm is the magnetic moment of a free electron. μ0 the free space permeability, and Z(EF ) the density of states at the Fermi level. Assume that μm μ0 H ≪ EF . Energy

294

EF , Fermi level Spin ‘up’

11.8. A system of electron spins is placed in a magnetic ﬁeld B = 2 T at a temperature T. The number of spins parallel to the magnetic ﬁeld is twice as large as the number of antiparallel spins. Determine T. 11.9. In a magnetic ﬂux density of 0.1 T, at about what frequencies would you expect to observe (i) electron spin resonance, (ii) proton spin resonance?

Spin ‘down’

Density of states 2μm μ0H

Fig. 11.34

Lasers

12

What goes up must come down. It’s all done with mirrors. 19th century aphorisms

12.1 Equilibrium We have several times arrived at useful results by using the concept of equilibrium. It is a pretty basic tenet of science and as with a similar idea, conservation of energy, it is always coming in handy. When we say that the electrons in a solid have a Fermi–Dirac distribution of energies, we are really saying two things: ﬁrst, that the system is in equilibrium; second, that it has a particular temperature. Temperature is a statistical concept and is bound up with the idea of equilibrium. On the one hand, we cannot meaningfully speak of the temperature of a single particle; on the other, if we have a system of particles that is perturbed from equilibrium, say by accelerating some of them, then for a transient period the temperature cannot be speciﬁed, since there is no value of T that will make the Fermi function describe the actual distribution. Of course, for electrons in a solid, or atoms in the gaseous state, the effect of collisions rapidly ﬂattens out the perturbation, the whole system returns to its equilibrium state, and the idea of temperature becomes valid again, although its actual value may have changed. We have on one or two occasions considered perturbed equilibrium. We saw, for example, in Chapter 1 that large currents may ﬂow in a conductor with a very slight change in the energy distribution. Thus, we could describe low ﬁeld conduction in metals and semiconductors without departing from the equilibrium picture. Lasers are different. They have massively perturbed population distributions that are nevertheless in some kind of equilibrium. But when we come to consider what temperature corresponds to that equilibrium, it turns out to be negative. Now you know that 0 K is a temperature that can never quite be obtained by the most elaborate refrigerator; so how can we get a negative temperature? It is not inconsistent really because, as we shall show, a negative temperature is hotter than the greatest positive temperature. But before going further into Erewhon∗ let us return to earth and start from the beginning.

12.2 Two-state systems Let us consider a material in which atoms have only two narrow allowed energy levels, as illustrated in Fig. 12.1. Provided that the whole system containing the material is in thermal equilibrium, the two allowed levels will be populated corresponding to a dynamic energy equilibrium between the atoms. The

∗ Erewhon

(approximately ‘nowhere’ backwards) was a country in the book of the same name by Samuel Butler, where all habits and beliefs were the opposite of ours and were justiﬁed with impeccable logic and reasonableness.

296

Lasers E

E3

Fig. 12.1 Number of atoms in a natural two-state system as a function of energy. The dotted line shows the Boltzmann function, decaying exponentially with increasing energy.

E1 N3

N1

logeN(E)

population of the energy levels is, therefore, accurately described by the temperature, T, of the system and its appropriate statistics, which we shall take as Boltzmann statistics. The two levels we are considering are labelled E1 and E3 in Fig. 12.1. Later on we shall see what happens in a three-level system, with the third level called E2 ; but for the moment do not be put off by this notation; we are still talking of only two levels. The numbers of electrons N1 , N3 in the levels E1 , E3 are related by the Boltzmann function, so that they will be of the general form

N0 is a constant.

We shall follow here the custom adopted in laser theory of using the frequency, ν, instead of the angular frequency, ω.

ρ(ν) is the radiation density emanating from a body at temperature, T, in a band of the frequency spectrum of width, dν, and at a frequency, ν.

N = N0 exp(–E/kB T).

(12.1)

E3 – E1 . N3 = N1 exp – kB T

(12.2)

Therefore,

As I said above, the atoms are in dynamic equilibrium, which means that the number of atoms descending from E3 to E1 is the same as the number leaping from E1 to E3 . An atom at E3 can lose the energy E3 – E1 either by radiative or by non-radiative processes. I shall consider only the former case here. When a radiative transition between E3 and E1 occurs during the thermal equilibrium process, it is called spontaneous emission for the ‘down’ process and photon absorption for the ‘up’ process. In each case, the photon energy is given by hν31 = E3 – E1 .

(12.3)

What do we mean by talking about photons being present? It is a very basic law of physics that every body having a ﬁnite temperature will radiate thermal or ‘black body’ radiation. This radiation comes from the sort of internal transitions that I have just mentioned. As we saw in Chapter 2, the whole business of quantum theory historically started at this point. In order to derive a radiation law that agreed with experiments, Planck found it necessary to say that atomic radiation was quantized. This famous radiation equation is ρ(ν)dν =

8π n3 hν 3 dν . exp(hν/kB T) – 1 c3

The derivation can be found in many textbooks.

(12.4)

Two-state systems So far we have talked about photons generated within the material. Now if photons of energy hν31 are shone on to the system from outside, a process called stimulated emission occurs. Either the photon gets together with an atom in a lower (E1 ) state and pushes it up to E3 ; or, less obviously, it stimulates the emission by an E3 -state atom of a photon (hν31 ). In the latter case one photon enters the system, and two photons leave it. It was one of Einstein’s many remarkable contributions to physics to recognize, as early as 1917, that both these events must be occurring in a thermodynamical equilibrium; he then went on to prove that the probabilities of a photon stimulating an ‘up’ or a ‘down’ transition were exactly equal. The proof is simple and elegant. Consider our system, remembering that we have two states in equilibrium. The rate of stimulated transitions (R1→3 ) from the lower to the upper state will be proportional to both the number of atoms in the lower state and the number of photons that can cause the transition. So we can write R1→3 = N1 B13 ρ(ν31 )dν.

(12.5)

For the reverse transition, from E3 to E1 we have a similar expression for stimulated emission, except that we will write the Einstein B-coefﬁcient as B31 . There is also spontaneous emission. The rate for this to occur will be proportional only to the number of atoms in the upper state, since the spontaneous effect is not dependent on external stimuli. The constant of proportionality or the probability of each atom in the upper state spontaneously emitting is called the Einstein A-coefﬁcient, denoted by A31 . Hence, R3→1 = N3 {A31 + B31 ρ(ν31 )}dν.

(12.6)

In equilibrium the rates are equal, R1→3 = R3→1 ,

(12.7)

N1 B13 ρ(ν31 )dν = N3 {A31 + B31 ρ(ν31 )}dν.

(12.8)

that is,

After a little algebra, using eqn (12.2) to relate N3 to N1 , we get ρ(ν31 )dν =

A31 dv . B13 exp(hν31 /kB T) – B31

(12.9)

Comparing this with eqn (12.4), which is a universal truth as far as we can tell, we ﬁnd that our (or rather Einstein’s) B-coefﬁcients must be equal, B13 = B31 ,

(12.10)

that is, stimulated emission and absorption are equally likely. Also, A31 = B31

3 8π n3 hν31 , c3

(12.11)

that is, the coefﬁcient of spontaneous emission is related to the coefﬁcient of stimulated emission.

297

The constant of proportionality B13 is the probability of absorbing a photon, often referred to as the Einstein B-coefﬁcient.

298

Lasers What is the physical signiﬁcance of A31 ? It is a measure of the spontaneous depopulation of state 3. Assuming, as usual, an exponential decay, the rate of change of population is dN3 = A31 N3 , (12.12) dt which leads to a decay time constant, called spontaneous lifetime, by deﬁning –

tspont =

E

Excited population Slope deﬁning temperature

E3 E2

Population removed

E1 N3

N2

N1 logeN(E)

Fig. 12.2 The three-level system. The strong ‘pump’ signal has equalized levels E1 and E3 , so that E3 now has a greater population than E2 . The dotted line shows how population is changing with energy, as in Fig. 12.1, but now it has a positive slope.

1 . A31

(12.13)

We should, by now, have quite a good picture of what happens when light of frequency v31 shines on the two-state system. In the presence of an input light spontaneous decay is usually negligible, and although the probabilities of upward and downward transitions are exactly equal, there will be more transitions from E1 to E3 because there are many more atoms in the lower state. In other words, the result is a net absorption of photons. This we often see in nature. For example, many crystalline copper salts have two energy bands, separated by photon energy corresponding to yellow light. Thus, when viewed in white light, the yellow part is absorbed, and the crystal transmits and reﬂects the complementary colour, blue. Ruby (chromium ions in crystalline alumina) has an absorption band in the green by this mechanism, and hence looks red in white light. When light is absorbed, the population of the upper level is increased. Normally this perturbation from the equilibrium condition is small. But if we have an increasingly intense ‘pump’ light source, the number in level 3 will go on increasing, by the same amount as those in level 1 decrease. Fairly obviously, there is a limit, when the levels are equally populated, and the pump is inﬁnitely strong. This is illustrated in Fig. 12.2. For the case of intense pumping, the non-equilibrium level populations (denoted by an asterisk) become almost equal, N1 + N3 . (12.14) 2 Now let us consider a three-level system, with the third level E2 between E1 and E3 , also shown in Fig. 12.2. The pumping will have no effect on its population, which is the equilibrium value N2 . So with the three-level system strongly pumped, the number of electrons in the three states are N1∗ , N2 , and N3∗ . Suppose that some photons come along with energy N1∗ ≃ N3∗ ≃

hν32 = E3 – E2 .

(12.15)

They will clearly interact with the system, causing stimulated emission by transitions from E3 to E2 and absorption by transitions from E2 to E3 . But now we have an unnatural occurrence: there are more electrons in the upper state (E3 ) than in the lower (E2 ). So instead of there being a net absorption of photons of energy, hv32 , there will be a net emission. The three-level system will amplify a photon of frequency, v32 , which is called the signal frequency. The whole thing is called a laser, which stands for light ampliﬁcation by stimulated emission of radiation. When there are more atoms in an upper than a lower level, as in the case of E3 and E2 in Fig. 12.2, it is justiﬁable jargon to speak of an ‘inverted

Lineshape function

299

population’. The other point we should clear up, before describing some real system with inverted populations, is the one concerned with temperature. From eqn (12.1) the locus of the line representing the populations of the various energy levels, kB T dE =– (12.16) dN N (shown as a dotted curve in Fig. 12.1), has a negative slope proportional to T/N. Now look at Fig. 12.2. First consider the populations N3∗ and N1∗ . They are in a steady state in the sense that as long as the pump continues steadily, they do not change with time. But for these two levels with a ﬁnite energy difference there is virtually no difference in population. Therefore, if we regard eqn (12.16) as a way of deﬁning temperature, for a well-pumped two-level system the temperature is inﬁnite. If we now consider the energy-level populations at E3 and E2 in Fig. 12.2, we see that N3∗ > N2 ,

(12.17)

and the dE/dN locus has a positive slope, which by eqn (12.16) corresponds to a negative temperature. Again, this is a fairly reasonable shorthand description of there being more atoms in an upper state than in a lower one. Now if you imagine a naturalstate system pumped increasingly until it attains an inﬁnite temperature and then eventually an inverted population, you will see there is some sense in the statement that a negative temperature is hotter than a positive one.

12.3 Lineshape function So far we have assumed that energy levels are inﬁnitely narrow. In practice they are not, and they cannot be as we have already discussed in Section 3.10. All states have a ﬁnite lifetime, and one can use the uncertainty relationship in the form Et = ℏ.

(12.18)

Since E = hν, we shall ﬁnd for the uncertainty in frequency (which we identify with the frequency range between half-power points, also called the linewidth), ν =

1 . 2π tspont

(12.19)

Unfortunately, the uncertainty relationship will not yield the shape of the line function. To ﬁnd that we need to use other kinds of physical arguments. But before trying to do that, let us deﬁne the lineshape, g(ν). We deﬁne it so that g(ν)dν is the probability that spontaneous emission from an upper to a lower level will yield a photon between ν and ν + dν. The total probability must then be unity, which imposes the normalization condition ∞ g(ν)dν = 1. (12.20) –∞

Let us stick for the moment to spontaneous decay (or natural decay) and derive the linewidth by a circuit analogy.

We may now identify t with tspont .

300

Lasers A lossless resonant circuit has a well-deﬁned resonant frequency. However, in the presence of losses the resonance broadens. In what form will the voltage decay in a lossy resonant circuit? If the losses are relatively small, then circuit theory provides the equation U(t) = U0 exp(–t/τ ) cos 2π ν0 t.

(12.21)

What is the corresponding frequency spectrum? If the oscillations decay, then they can no longer be built up from a single frequency. The range of necessary frequencies, that is the spectrum, is given by the Fourier transform ∞ U(t) exp(i2π νt)dt. (12.22) f (ν) = 0

Restricting ourselves to the region in the vicinity of ν0 and after proper normalization, we obtain

g(ν) is known as a Lorentzian lineshape.

g(ν) =

(1/2)π τ , 2π [(ν – ν0 )2 + (1/2(π τ ))2 ]

(12.23)

If we work out now the frequency range between the half-power points, we obtain 1 , (12.24) ν = 2π τ which is the same as eqn (12.19), provided we identify the decay constant of the circuit with the spontaneous lifetime of the quantum-mechanical state. So again, a simple argument based on the uncertainty relationship agrees with that based on a quite different set of assumptions. In a practical case spontaneous emission is not the only reason why a state has ﬁnite lifetime. Interaction with acoustic waves could be another reason (electron–phonon collision in quantum-mechanical parlance) or collisions with other atoms. The latter becomes important when lots of atoms are present in a gas, leading to so-called pressure broadening. All those mentioned so far belong to the category of homogeneous broadening, where homogeneous means that conditions are the same everywhere in the material. When conditions differ (say strain varies in a solid) then we talk of inhomogeneous broadening. The best example of inhomogeneous broadening is the so-called Doppler broadening, owing to the fact that an atom moving with velocity, v, will emit at a frequency, v . (12.25) ν = ν0 1 + c In thermal equilibrium the atomic gas has a Maxwellian velocity distribution, hence the corresponding broadening may be calculated. The result (see Exercise 12.8) for the normalized lineshape is g(ν) = C1 exp[–C2 (ν – ν0 )2 ], M is the atomic mass.

(12.26)

where c C1 = v0

M 2π kB T

1/2

and

M C2 = 2 kB T

c v0

2

.

(12.27)

Resonators and conditions of oscillation

12.4 Absorption and ampliﬁcation Let us look now at energy levels 2 and 3 and consider the induced transition rate between them. It is W32 = B32 ρ(ν) =

c3 ρ(ν) , 8π n3 hν 3 tspont

(12.28)

where eqns (12.11) and (12.13) have been used. The transition rate will of course depend on the lineshape function, so we need to multiply eqn (12.28) by g(ν). We shall also introduce the power density (measured in W m–2 ) instead of the radiation density (measured in J m–3 ) with the relation, Pd =

c ρ, n

(12.29)

leading to the form, W32 =

c2 Pd g(ν) . 8π n2 hν 3 tspont

(12.30)

Now the number of induced transition per second is N3 W32 per unit volume, and the corresponding energy density per second is N3 W32 hν. For upward transitions, we obtain similarly N2 W32 hν, and hence the power lost in a dz thickness of the material is (N3 – N2 )W32 hν dz. Denoting the change in power density across the dz element by dρd , we obtain the differential equation, dρd = γ (ν)ρd , dz

γ (ν) = (N3 – N2 )

c2 g(ν) , 8π n2 ν 2 tspont

(12.31)

which has the solution, Pd (Z) = Pd (0) exp γ (ν)z.

(12.32)

Under thermal equilibrium conditions N3 < N2 , and consequently, the input light suffers absorption. However, when N3 > N2 , that is there is a population inversion, the input light is ampliﬁed.

12.5 Resonators and conditions of oscillation As we have said before, the energy levels are not inﬁnitely narrow, hence emission occurs in a ﬁnite frequency band. For single-frequency emission (by single frequency, we mean here a single narrow frequency range) all the excited states should decay in unison. But how would an atom in one corner of the material know when its mate in the other corner decides to take the plunge? They need some kind of coordinating agent or—in the parlance of the electronic engineer—a feedback mechanism. What could give the required feedback? The photons themselves. They stimulate the emission of further photons as discussed in the previous section and also ensure that the emissions occur at the right time. If we want to form a somewhat better physical picture of

301

302

∗ In

fact, lasers are nearly always used as oscillators rather than ampliﬁers. So the phenomenon should be referred to as light oscillation by stimulated emission of radiation but, somehow, the corresponding acronym never caught on.

Lasers this feedback mechanism, it is advisable to return to the language of classical physics and talk of waves and relative phases. Thus, instead of a photon being emitted, we may say that an electromagnetic wave propagates in a way in which any two points bear strict phase relationships relative to each other. This phase information will be retained if we put perfect reﬂectors in the path of the waves on both sides, constructing thereby a resonator. The electromagnetic wave will then bounce to and fro between the two reﬂectors establishing standing waves, which also implies that the region between the two reﬂectors must be an integer multiple of half wavelengths. Thus, in a practical case, we have a relatively wide frequency band in which population inversion is achieved, and the actual frequencies of oscillation within this band are determined by the possible resonant frequencies of the resonator. A resonator consisting of two parallel plate mirrors is known as a Fabry– Perot resonator after two professors of the Ecole Polytechnique, who followed each other (mind you, in the wrong order, Perot preceded Fabry). What will determine the condition of oscillation∗ in a resonator? Obviously, the loop gain must be unity. If we denote the attenuation coefﬁcient by α (discussed previously in Sections 1.5 and 10.15—talking about lossy waves) the intensity in a resonator of length, l, changes by a factor, exp[(γ – α)2l]. Denoting further the two mirror’s amplitude reﬂectivity by R1 and R2 , respectively, we ﬁnd that the condition for unity loop gain is R1 R2 exp[(γ – α)2l] = 1.

† This

is one of the reasons why it is more difﬁcult to obtain laser action in the ultraviolet and soft X-ray region. According to eqn (12.11) the coefﬁcient of spontaneous emission increases by the third power of frequency.

(12.33)

We know what determines γ . How can we ﬁnd α? It represents all the losses in the system except mirror losses, which may be summarized as ohmic losses in the material, diffraction losses in the cavity, and losses due to spontaneous emission.† Just one more word on diffraction losses. If the resonator consists of two parallel mirrors, then it is quite obvious that some of the electromagnetic power will leak out. In any open resonator there is bound to be some diffraction loss. Then why don’t we use a closed resonator, something akin to a microwave cavity? The answer is that we would indeed eliminate diffraction losses, but on the whole we would lose out because ohmic losses would signiﬁcantly increase.

12.6

Some practical laser systems

How can we build a practical laser? We need a material with suitable energy levels, a pump, and a resonator. Is it easy to ﬁnd a combination of these three factors which will result in laser oscillation? It is like many other things; it seems prohibitively difﬁcult before you’ve done it and exceedingly easy afterwards. By now thousands of ‘lasing’ materials have been reported, and there must be millions in which laser oscillations are possible. There are all kinds of lasers in existence; they can be organic or inorganic, crystalline or non-crystalline, insulator or semiconductor, gas or liquid, they can be of ﬁxed frequency or tunable, high power or low power, CW or pulsed. They may be pumped by another laser, by ﬂuorescent lamps, by electric arcs, by electron irradiation, by injected electrons, or by entirely non-electrical means, as in a chemical laser. You can see that a mere enumeration of the various

Some practical laser systems

303

realizations could easily take up all our time. I shall be able to do no more than describe a few of the better-known lasers.

12.6.1

Solid state lasers

The ﬁrst laser constructed in 1960 was a ruby laser. The energy-level diagram for the transitions in ruby (Cr ions in an Al2 O3 lattice) is given in Fig. 12.3. I remarked above that ruby owed its characteristic red colour, to absorption bands of the complementary colour, green. This absorption is used in the pumping process. A typical arrangement is sketched in Fig. 12.4, which shows how the light from a xenon discharge ﬂash tube ‘pumps’ the ruby to an excited state. Now the emission process is somewhat different here from that which I sketched previously for three-level systems. The atoms go from level 3 into level 2 by giving up their energy to the lattice in the form of heat. They spend a long enough time∗ in level 2 to permit the population there to become greater than that of level 1. So laser action may now take place between levels 2 and 1, giving out red light. The ruby itself is an artiﬁcially grown single crystal that is usually a cylinder, with its ends polished optically ﬂat. The ends have dielectric (or metal) mirrors evaporated on to them. Thus, as envisaged in the previous section, the resonator comprises two reﬂectors. Some power is certainly lost by diffraction, but these losses are small provided the dimensions of the mirror are much larger than the wavelength. It needs to be noted that one of the mirrors must be imperfect in order to get the power out. Another notable representative of solid-state crystalline lasers is Nd3+ : YAG, that is neodymium ions in an yttrium–aluminium–garnet. It is a fourlevel laser radiating at a wavelength of 1.06 µm, pumped by a tungsten or mercury lamp. Laser operation at the same frequency may be achieved by putting the neodymium ions into a glass host material. Glasses have several advantages in comparison with crystals: they are isotropic, they can be doped at high concentrations with excellent uniformity, they can be fabricated by a variety of processes (drilling, drawing, fusion, cladding), they can have indices of refraction in a fairly wide range, and last but not least, they are considerably cheaper than crystalline materials. Their disadvantage is low thermal conductivity, which makes glass lasers unsuitable for high average-power applications.

Mirrored ends

∗ Energy

levels in which atoms can pause for a fairly long time (a few milliseconds in the present case) are called ‘metastable’.

Non-radiative transitions

Pump levels 3 2

Laser transition Ground state

1

Fig. 12.3 Energy levels of the Cr3+ ion in ruby. The pump levels are broad bands in the green and blue, which efﬁciently absorb the ﬂash tube light. Level 2 is really a doublet (two lines very close to each other) so that the laser light consists of the two red lines of wavelengths 694.3 and 692.9 nm.

Ruby rod Parallel laser beam

Fig. 12.4 Flash tube Elliptic cylinder reﬂecting container

General arrangement of a ruby laser. The ruby and the ﬂash tube are mounted along the foci of the elliptic cylinder reﬂector for maximum transference of pump light.

304

Lasers

12.6.2

The gaseous discharge laser

When a current is passed through a gas, as happens in a ﬂuorescent lamp or a neon sign, most of the charged particles making up the current come from gas atoms that have been ionized by collision. But as well as completely dispossessing atoms of their electrons, the collisional process causes some bound electrons to gain extra energy and go into a higher state, that is, a state described by higher quantum numbers. You will remember that we had a formula for the simplest gas, hydrogen, in Chapter 4: En = –

13.6 . n2

(12.34)

This shows that there is an inﬁnite number of excited states above the ground state at –13.6 eV, getting closer together as the ionization level (0 eV) is approached. In the helium–neon laser the active ‘lasing’ gas is neon, but there is about 7– 10 times as much helium as neon present. Consequently, there are quite a lot of helium atoms excited to states about 20 eV above the ground state (Fig. 12.5). Now helium atoms in these particular states can get rid of their energy in one favourable way—by collision with other atoms that also have levels at the same energies. Since neon happens to have suitably placed energy levels, it can take over the extra energy making the population of the upper levels (3a′ , 3b′ ) more numerous than that of the lower level (2′ ), and thus laser action may occur. It is, of course, necessary to adjust gas pressures, discharge tube dimensions, and current quite critically to get the inverted population; in particular it is obtained only in a fairly narrow range of gas pressures around 1 Torr. The reﬂectors are external to the tube, as shown in Fig. 12.6. Note that the windows are optical ﬂats, oriented at the Brewster angle, θB , in order to

21 3a

3a′ Collisions

20

3b′

3b

The energy levels of interest for a helium–neon laser. Helium atoms get excited to levels 3a and 3b due to the impact of accelerated electrons. Neon atoms, which happen to have the same energy levels (3a′ , 3b′ ) collide with helium atoms and take over the extra energy. Laser action may now occur at two distinct wavelengths, corresponding to radiative transitions from levels 3a′ and 3b′ to a lower level 2′ .

Energy (eV)

Fig. 12.5 1.15 μm

19

18

0

632.8 nm

2′

Electron impact

1 Helium

1′ Neon

Some practical laser systems

305

Discharge power supply Eoptical

B

Output beam Glass gas envelope Brewster windows

Fig. 12.6 External mirrors

minimize reﬂections for the desired polarization. The advantage of spherical mirrors is that their adjustment is not critical, and they also improve efﬁciency. Dielectric mirrors are also used, not only because they give better reﬂections than metal mirrors but because they can also select the required wavelength from the two possible transitions shown in Fig. 12.5. A close, though more powerful, relative of the He–Ne laser is the argon ion laser, operating in a pure Ar discharge. The pumping into the upper level is achieved by multiple collisions between electrons and argon ions. It can deliver CW power up to about 40 W at 488 and 514 nm wavelengths. It is in the company of the He–Ne laser, the one most often seen on laboratory benches. The CO2 laser is capable of delivering even higher power (tens of kW) at the wavelength of 10.6 µm. It is still a discharge laser, but the energy levels of interest are different from those discussed up to now. They are due to the internal vibrations of the CO2 molecule. All such molecular lasers oscillate in the infrared; some of them (e.g. the HCN laser working at 537 µm) approach the microwave range.

12.6.3

Dye lasers

This is an interesting class of lasers, employing ﬂuorescent organic dyes as the active material. Their distinguishing feature is the broad emission spectrum, which permits the tuning of the laser oscillations. The energy levels of interest are shown in Fig. 12.7(a). The heavy lines represent vibrational states, and the lighter lines represent the rotational ﬁne structure, which provides a near continuum of states. The pump (ﬂashlamp or another laser) will excite states in the S1 band (A → b transition) which will decay non-radiatively to B and will then make a radiative transition (B → a) to an energy level in the S0 band. Depending on the endpoint, a, a wide range of frequencies may be emitted. Finally, the cycle is closed by the nonradiative a → A transition. Unfortunately, at any given frequency of operation, there are some other competing non-radiative processes indicated by the dotted lines. A photon may be absorbed by exciting some state in the higher S2 band, or there might be a non-radiative decay to the ground state via some other energy levels. There is net gain (meaning the gain of the wave during a single transit between the reﬂectors) if the absorptive processes are weaker than the ﬂuorescent processes.

Schematic representation of a gas laser.

306

Lasers (a)

Absorption

(b) b S1

Fluorescence Absorption

Relative intensity

Emission

Energy

Absorption

Excitation

B

Tuning range 560

a

S0

580 600 620 Wavelength (nm)

A

Fig. 12.7 (a) The relevant energy levels of a dye molecule. The wavy arrows from b to B and from a to A represent non-radiative transitions. The broken lines leading to the right also represent non-radiative transitions in which some other states are involved. (b) The tuning range of rhodamine 6G as a function of wavelength. (c) Schematic representation of a tuneable dye laser.

Note that this range is not the end of the dye laser’s tuneability. By choosing the appropriate dyes any frequency within the visible range may be obtained.

(c)

Dielectric mirror

Diffraction grating

Flashlamp

Laser output

Dye cuvette Dye out

Dye in

Rotation for tuning

The tuning range of a speciﬁc dye laser (rhodamine 6G) is shown in Fig. 12.7(b) by the shaded area, where the ﬂuorescent and absorption curves are also plotted as a function of wavelength. Laser action becomes possible when the absorption curve intersects the ﬂuorescence curve. At the long wavelength extreme, the gain of the laser (meaning the gain of the wave during a single transit between the reﬂectors) becomes too small for oscillation, as a result of the decrease in ﬂuorescence efﬁciency. How can we tune the laser? An ingenious solution is shown in Fig. 12.7(c), where one of the mirrors is a rotatable diffraction grating. The oscillation frequency of the laser will be determined by the angular position of the grating, which will reﬂect a different frequency at each position. The tuneable range is a respectable 7%.

12.6.4

Gas-dynamic lasers

The essential difference between these lasers and all the others discussed so far is that no electric input is needed. One starts with a hot gas (e.g. CO2 ) in

Semiconductor lasers

307

the so-called stagnation region. Then most of the energy is associated with the random translation and rotation of the gas molecules and only about one-tenth of the energy is associated with vibration. Next, the gas is expanded through a supersonic nozzle, causing the translational and rotational energies to change into the directed kinetic energy of the ﬂow. The vibrational energy would disappear entirely if it remained in equilibrium with the decreasing gas temperature. But the vibrational relaxation times are long in comparison with the expansion time, hence the population of the vibrational levels remains practically unchanged. At the same time, the lower level population diminishes rapidly with the expansion, leading to signiﬁcant population inversion after a few centimetres downstream. For CO2 gas the emission wavelength is again 10.6 µm, using other gases the typical range is from 8 to 14 µm, although oscillations may be achieved at much shorter wavelengths, as well. The advantage of gas-dynamic lasers is the potential for high average powers because waste energy can be removed quickly by high-speed ﬂow.

12.6.5

Excimer lasers

Excimers are molecules which happen to be bound in an excited state and not in the ground state, so their operation differs somewhat from the general scheme. Their main representatives are the rare gas halides like KrF or XeCl. They need powerful pumps in the form of discharges, optical excitation, or high-current, high-voltage electron beams. Their advantages are high efﬁciency and high pulse energy in a part of the spectrum (in the ultraviolet down to wavelengths of about 100 nm) which was inaccessible before. Most of them are inherently broadband and offer the further advantage of tuneability.

12.6.6

Chemical lasers

As the name suggests, the population inversion comes about as a result of chemical reactions. The classiﬁcation is not quite clear. Some of the excimer lasers relying on chemical reactive collisional processes could also be included within this category. The clearest examples are those when two commercially available bottled gases are let together, and monochromatic light emission is brought about by the chemical reaction.∗

12.7 Semiconductor lasers 12.7.1

Fundamentals

We shall dwell on semiconductor lasers a little longer because they are in a quite special category. For us they are important for the reason that we have already invested much effort in understanding semiconductors, so that any return on that investment is welcome. There are, though, some more compelling reasons as well. 1. They are of interest because the technology and properties of semiconductors are better known than those of practically any other family of materials. 2. Laser action is due to injection of charged carriers, so semiconductor lasers are eminently suitable for electronic control.

∗ The

advent of chemical lasers raises an intriguing problem I have often asked myself about. What path would technology have followed if electricity had never been discovered? The question may be posed because electricity and technology developed separately, the former being a purely scientiﬁc pastime until the fourth decade of the nineteenth century. Had scientists been less interested in electricity or had they been just a bit lazier, it is quite conceivable that the social need for fast communications (following the invention of the locomotive) would have been satisﬁed by systems based on modulated light. In the search for better light sources, the chemical laser could then have been invented by the joint efforts of chemists and communication engineers a century ago.

308

Lasers 3. 4. 5. 6. 7. 8.

They have high efﬁciency. They operate at low voltage. They are small. They are robust. They have long life. The technique for their production is suitable for mass manufacture, so they are potentially inexpensive. 9. They can be produced in arrays. 10. They may be made to work in the wavelength range in which optical ﬁbres have favourable loss (near to minimum) and dispersion properties. I am sure if I tried hard, I could come up with a few more advantages but, I think, ten are enough to show that semiconductor lasers merit special attention. How does a semiconductor laser work? The basic idea is very simple. It is radiative recombination in a direct-gap semiconductor which leads eventually to laser action. Why a direct gap? Because we want the probability of a transition from the bottom of the conduction band to the top of the valence band to be high. What else do we need? We need a piece of material in which there are lots of electrons in the conduction band eager to descend, and in which there are lots of empty states at the top of the valence band eager to receive the electrons. A homogeneous piece of semiconductor is obviously not suitable because we cannot achieve both conditions simultaneously, only one at a time. But that gives an idea. We can have lots of electrons in a degenerate (discussed in Section 9.10 when talking of tunnel diodes) n-type semiconductor and, similarly, we can have lots of holes in a degenerate p-type semiconductor. So let us put them together, that is, produce a p–n junction, and then in the middle of it both conditions may be expected to be satisﬁed, provided the forward bias, U1 , is close to the energy gap. The energy band structure and the distribution of electrons and holes for this case are shown in Fig. 12.8(a) and (b) for thermal equilibrium and for forward bias, respectively. The overlap region in the middle of the junction, where both electrons and holes are present with high density, is called the active region, and that is where radiative recombination takes place. In order to keep up the process, whenever an electron–hole pair disappears by emitting a photon, it must be replaced by injecting new carriers. If we examine the simple model shown in Fig. 12.9, the total number of electrons in the active region is Ne lwd, where Ne , as usual, denotes the density (a)

(b)

Photon emission EF

Fig. 12.8 A degenerate p–n junction at (a) thermal equilibrium, (b) forward bias.

p

n

eU1≈Eg

Semiconductor lasers

309

of electrons. The rate of change of the number of electrons, due to spontaneous recombination, is Ne lwd/trec , and this loss should be replenished by injection of electrons, that is the number required is (Ii /e)η, where Ii is the injected current and η, the quantum efﬁciency, is the fraction of injected electrons which recombine radiatively, leading to the formula Ne lwd Ii η = . trec e

I

Active region

d

(12.35) w

Recognizing now that the recombination time in the above equation corresponds to tspont discussed before, we may now use eqn (12.31) to ﬁnd the ampliﬁcation of the optical wave. For simplicity, we may take the population of the lower level as zero, and obtain γ (ν) =

c2 g(ν)η Ii . 8π n2 ν 2 elwd

(12.36)

For laser oscillations we need the loop gain to be unity. When both mirrors have the same reﬂectivity, the condition of oscillation is R exp(γ – α)l = 1,

(12.37)

whence the threshold current density is Ii 8π n2 ν 2 ed = 2 lw c ηg(ν)

1 α – 1n R . l

(12.38)

As we have said before α represents the losses in the material. But are there any losses at all? The optical wave propagating in the active region will surely grow and not decay. True, but there is no reason why the optical wave should be conﬁned to the active region. A well calculated plunge (one we shall not take here) into the mysteries of electromagnetic theory would show that a not inconsiderable portion of the electric ﬁeld propagates outside the active region, where there is no population inversion. The losses there are mainly caused by the so-called free-carrier absorption, which comes about by electrons and holes excited to higher energies within their own bands. What is the value of R? In the simplest laser diode the mirror consists of the cleaved end of the semiconductor crystal, that is one relies on the difference in refractive index between semiconductor and air. A typical refractive index is 3.35, which yields for the reﬂection coefﬁcient, R = 0.54. For a practical case (see Exercise 12.10) the threshold current comes to a value of about 820 A cm–2 . This is quite a large value. Can we reduce it by some clever trick? Yes, we can, and the trick is to use a heterojunction instead of a homojunction. A schematic drawing of the device is shown in Fig. 12.10. What is the role of the various layers? The insulating SiO2 layers are there in order to steer the current towards the middle of the device and thus increase the current density. The heavily doped GaAs layers next to the metal electrodes are there to provide ohmic contacts. The p-type and n-type AlGaAs layers serve to provide the p–n junction, and then we come to the star of the show, the thin

l

Fig. 12.9 Schematic representation of a laser diode.

310

Lasers Forward-bias voltage

Metal Silicon dioxide Heavily p-doped gallium arsenide p-Doped gallium aluminium arsenide Gallium arsenide n-Doped gallium aluminium arsenide Heavily n-doped gallium arsenide

Fig. 12.10 Schematic drawing of a double heterojunction diode laser.

Note, however, that our aim is now to conﬁne the carriers to the narrow GaAs region and not to the extremely narrow triangular wells. These blips in the energy diagram are now embarrassments rather than assets. In fact, by gradually increasing the proportion of A1 in the junction, the blips can be removed (we no longer show them in Fig. 12.11(b)).

Laser beam

Metal

Heat sink

layer (≈100 nm) of GaAs in between. Very remarkably, we can kill two birds with that one layer. It will serve both to conﬁne the wave and to conﬁne the carriers. It is very easy to see why the wave is conﬁned. GaAs has a higher index of refraction than AlGaAs, hence the mechanism of conﬁnement is simply that of total internal reﬂection, as mentioned in Section 10.15 when talking about optical ﬁbres. Why are the carriers conﬁned? Well, we have been through this before, haven’t we? We discussed this type of heterojunction in Section 9.15 and came clearly to the conclusion that the electrons are conﬁned to a very narrow potential well. So why do I ask this question again? The reason is that the conﬁnement of carriers is due now to a different mechanism. The crucial thing is still the lower energy gap of GaAs relative to AlGaAs, but we no longer rely on the triangular potential well for conﬁnement. To see in detail what happens in the p-type AlGaAs–undoped GaAs–n-type AlGaAs heterojunction, I shall ﬁrst show the energy diagram at thermal equilibrium [Fig. 12.11(a)]. This is drawn by exactly the same technique which led to Fig. 9.41(c). The triangular well we have seen in Section 9.15 is there at the right-hand junction. A new kind of triangular well, in which the holes are conﬁned, may be seen at the left-hand junction. What happens when we apply a forward bias? The barriers decline [Fig. 12.11(b)], but in contrast to those in the homojunction, the remaining barriers (for electrons towards the left and for holes towards the right) are still high enough to prevent carriers spilling over into the oppositely doped region and disappearing by the wrong kind of non-radiative recombination. The electrons injected from the left have little other choice but to take the plunge into the empty states in the valence band and emit a photon, meanwhile. The threshold current density of our heterojunction will be much smaller because the fraction of electrons which recombine radiatively will be much

Semiconductor lasers (a)

EF

311

(b)

EC

EC

eU1

Fig. 12.11 eU1 EV

EV

An AlGaAs–GaAs heterojunction (a) at thermal equilibrium, (b) at a forward bias of eU1 .

p+– Ga As p – Ga Al As p – Ga As n – Ga Al As n – Ga As

higher. The threshold current will also be small on account of the small thickness, d, of the active region [see eqn (12.38)] which is 100 nm in our example. Can we further decrease the threshold current? Yes, both common sense and eqn (12.38) tell us that we need higher reﬂectivity mirrors. One way of doing this is to use an external Bragg reﬂector, as shown in Fig. 12.12. Each slight corrugation will cause a small reﬂection which all add up in phase at the right wavelength.∗ By these means threshold currents as small as 0.5 mA have been achieved. It is very nice, indeed, to reduce the threshold current because that will reduce the power consumption of devices (e.g. compact disk players) using semiconductor lasers. But those lasers have to deliver a certain amount of power. There is no way of getting out a fair amount of power without putting in a fair amount of power, so it is also of crucial importance how the output power increases as the current exceeds its threshold value. Let us now come back to the role of d, the thickness of the active region. As we reduce it, the threshold current decreases simply because fewer electrons need to be supplied to make up for spontaneous emission. Fewer electrons being available will also reduce the achievable power output. For this reason d cannot be usefully reduced to a value smaller than about 100 nm. Actually, if our aim is to reduce the thickness further without losing output power, we could simply increase the number of wells, say by a factor of 10, and make each of them a thickness of d/10.

Fig. 12.12 Schematic representation of a double heterojunction GaAlAs laser with external Bragg reﬂector mirrors.

∗ The

corrugations (or slight bumps) can actually be inside the laser, in which case we talk about a Distributed Bragg Reﬂector laser or DBR.

312

Lasers

12.7.2

Wells, wires, and dots

On the whole, is it an advantage to have multiple quantum wells? One might be permitted to see only disadvantages. Surely, the more quantum wells, the more complicated must be the production process. In order to see the advantages, we need to investigate what happens as we further reduce the thickness of the active region. The main effect is that the discrete nature of the energy levels will be more manifest. Let us remember (eqn 6.1) the energy levels in a potential well: E=

h2 n2 . 8mL2

(12.39)

If the lateral dimension of the well is 10 nm, then the lowest energy level comes to 0.056 eV (where we have taken the effective mass of the electron at m∗ m–1 = 0.067). In terms of the energies we talk about this is not negligible. It comprises about 4% of the energy gap of GaAs. If this is the lowest energy available above the bottom of the conduction band, and similarly, there is a highest discrete level for holes in the valence band, then the wavelength of emitted radiation is determined by the energy difference between these levels. Thus, one advantage should now be clear. Our laser can be tuned by choosing the thickness of the active layer in a Multiple Quantum Well (MQW) device. The tuning range might be as much as 20%. Are there any other advantages? To answer this question, we need to make a digression and look again at the density of states function which we worked out in Chapter 6. Let us start with the energy levels of a three-dimensional well, as given by eqn (6.2) but permitting well dimensions to be different: h2 E= 8m

2 n2x ny n2z + + L2x L2y L2z

.

(12.40)

In MQW lasers the dimensions Ly and Lz are much larger than Lx = d, the thickness of the active region. We may just as well take Ly = Lz = l, with which eqn (12.40) modiﬁes to E = E0

n2x

! 2 d 2 2 ny + nz , + l

(12.41)

where E0 =

h2 . 8m d 2

(12.42)

It is clear from eqn (12.41) that nx has a much higher inﬂuence on the allowed energies then ny and nz . There will be big steps at nx = 1, 2, 3, etc. Our primary interest is in the density of states because that will tell us how many electrons within an energy range dE can make the plunge downwards. Next, let us determine the density of states in the region between nx = 1 and nx = 2. This is then determined by ny and nz . Within a radius of n(≫ 1) the

Semiconductor lasers

313

number of possible states are π n2 , since there is a state for each integer value of ny and nz . Solving for n2 = n2y + n2z from eqn (12.41) we obtain 2 l E n π =π –1 . d E0 2

(12.43)

Thus, eqn (12.43) gives the number of states∗ having energies less than E. Similarly, the number of states having energies less than E + dE is π

2 E + dE l –1 . d E0

∗ This

is exactly analogous to the calculation of the three-dimensional density of states we performed in Section 6.2.

(12.44)

Consequently, the states having energies between E and E + dE (and that deﬁnes the density of states function Z(E)) may be found as 2 dE l . Z(E)dE = π d E0

(12.45)

Remember that only positive integers count, so we need to divide by 4. On the other hand, there is spin as well, which is taken into account by multiplying by 2. Thus, the density of states in eqn (12.45) needs to be divided by 2. That is actually a minor detail. The important thing is that the density of states is independent of energy in the range nx = 1 to nx = 2. Taking l = 300 µm and d = 10 nm, we get (l/d)2 = 9×108 . Thus, when n2 = n2y +n2z = 27×108 , then E reaches the value of 4E0 . We may alternatively, however, obtain an energy 4E0 with ny and nz being very small and nx = 2. It is clear that above 4E0 , the same energy level may be reached in two different ways: with ny and nz relatively small and nx = 2, or with ny and nz large and nx = 1. Thus, the number of available states suddenly doubles at E = 4E0 . Between E = 4E0 and E = 9E0 , the density of states remains constant again, and there is a new contribution at E = 9E0 , which leads to trebling of the initial density of states. The fruit of our calculations, Z(E) as a function of energy for a twodimensional potential well, is shown in Fig. 12.13. The density of states increases stepwise at the discrete points En = n2x E0 , where it reaches the value 2 l nx . Z(En ) = 2E0 d

(12.46)

Eliminating nx , we may obtain the envelope function (dotted lines) as Z(En ) =

1 1/2 En (E0 )–3/2 2

2 l , d

(12.47)

which gives the same functional relationship as that found earlier (eqn 6.10) for the three-dimensional density of states function. The truth is that it is the two-dimensional density of states function which is responsible for the superior performance of quantum wells, but to provide a quantitative proof is beyond the scope of the present book. We shall, instead, provide a qualitative argument.

Two-dimensional density of states

E0

4E0

9E0 E

Fig. 12.13 The two-dimensional density of states as a stepwise function of energy.

314

Lasers In lasers without two-dimensional conﬁnement, the low energy states near to the bottom of the band play no role. When the probability of occupation is taken into account, maximum inversion (which deﬁnes the centre frequency of the laser) occurs at an energy higher than the gap energy. These low lying states are wasted, hence their elimination in MQW lasers is beneﬁcial. Consequently, when the injected current is increased above its threshold, better use is made of the available electrons. There is, therefore, a much higher increase of output power with current. This also implies a faster reaction to the increase or decrease of current, hence MQW lasers may be electronically modulated up to higher frequencies. O.K., you might argue, MQW lasers are superior in performance, but surely they are much more expensive. Oddly enough they are not. When they are produced by one of the new techniques (MBE or MOCVD) they hardly cost more than ordinary semiconductor lasers. With GaAs comprising the active region, it is possible to produce lasers in the wavelength region 650–850 nm by varying the thickness of the quantum wells, although they are commercially available only at a few of these wavelengths. If it is possible to conﬁne carriers in one dimension then, surely, it is possible to conﬁne them in two dimensions. The resulting structures are called quantum wires. We can determine the density of states for that conﬁguration by following the arguments used for quantum wells. Assuming a wire of square cross-section with side d which is of the order of 100 nm, we can take in Eqn (12.40), Lx = Ly = d

and

Lz = ℓ,

where d ≪ ℓ.

(12.48)

Now the variations in nx and ny lead to sudden discrete changes in energy whereas the variation in nz can be regarded as smooth continuous change, so we can still talk about the density of states. The calculation is left to the reader. The result for the nx = ny = 1 case is Z(E) =

∗ That

raises the question of how many dimensions quantum dots have. If quantum wells are two-dimensional and quantum wires one-dimensional, then quantum dots, which conﬁne the electrons in one fewer dimension, cannot be anything but zero-dimensional. It is an odd terminology but one can get used to it.

#–1/2 1 ℓ" E0 (E – 2E0 ) . 2d

(12.49)

There is a singularity at E = 2E0 which means a discrete state. And there are of course singularities for all integral values of nx and ny . Is there any interest in producing devices using quantum wires? There are a few laboratories interested but, on the whole, it has not been a success. It is a kind of halfway house. If we want to do more carrier conﬁnement, why not go the whole hog and conﬁne them in all three dimensions? This leads us to the quantum dot in which all dimensions∗ are small. All the energy states, both for electrons and holes, are now discrete. What are the advantages of quantum dot lasers? Higher spectral purity, lower threshold current, and ability to work at high temperatures, all because the energy levels are discrete and there is a much more efﬁcient use of the available electrons. It is also easy to design a quantum dot laser to work at a given wavelength. The energy levels depend only on the size of the dot. The problems are mainly technological; how to make them of the same size, how to control their spatial distribution, and how to incorporate them in the active layer.

Semiconductor lasers First, how to make them. We know how to produce quantum wells. The obvious way of making quantum dots is then to etch away the other two dimensions. This was indeed tried, and the dots produced worked in a fashion but not very well. The reason was the high density of surface states created during etching. The technique used nowadays is strained-layer epitaxy. It is called self-organized because the quantum dots organize themselves. How? Let us talk about growing InAs on GaAs. The mismatch between their lattices is about 7%, causing strain. After the growth of a few monolayers the strain becomes unbearable,∗ and the layers break up and create 3D islands. Once the growth of the islands starts, it quickly reaches saturation. Typical quantum dot densities may vary between 108 and 1011 cm–2 . The shapes are quasi-pyramidal with a base of 10–20 nm and a height of 3–10 nm. In order to incorporate these dots into a device they need to be ‘capped’, i.e. ﬁlled up with a material, which would be GaAs in the present case. During the capping process, as may be expected, the heights of the InAs islands collapse down to maybe 2 nm after a GaAs cap of 2 nm. An obvious way of increasing the number of quantum dots is to have more layers. With the materials mentioned above, another layer of InGaAs needs to be deposited, and then one can repeat the same procedure. An atomic force microscopy image of a bilayer structure† (in this case the second layer of quantum dots is just above the ﬁrst layer) is shown in Fig. 12.14. When will quantum dot lasers appear commercially? Reliable mass production techniques are still far away, but that is not all. There are actually still unresolved problems concerning their operation. The emission process is not as simple as it ﬁrst appears, because the relevant energy levels are nearly degenerate, i.e. very close to each other. When an electron descends from the conduction band and recombines with a hole it does emit a photon, but that photon may be immediately reabsorbed by promoting another electron into the conduction band. This is known as Auger recombination. A possible remedy is to coat the quantum dot with another material which can localize electrons and holes on opposing sides of the interface.

315

∗ In

more sophisticated language, one should say that after a critical thickness, the increasing strain between the layers makes it energetically favourable for the strain to be relieved by formation of 3D islands.

† The

number of quantum dots in Fig. 12.14 can be counted to be 31. Since this is for an area of 0.25 µm2 , the density comes to 1.24 × 1010 cm–2 .

Fig. 12.14 0.5 m × 0.5 m

A highly uniform dot ensemble produced by self-organization.

316

Lasers

Lattice spacing (Å)

6.5

InSb

AlSb

GaSb InAs 6.0 InP

AlAs

GaAs 5.5

Fig. 12.15 Relationship between energy gap and lattice spacing for some mixed III–V semiconductors.

0.0

12.7.3

∗ Strain

introduced by having somewhat different lattice constants can actually be beneﬁcial, as pointed out in Section 9.15 on heterostructures.

Table 12.1 Compounds for laser diodes Wavelength range (nm)

Laser diodes based on

342–375 375–700 600–900 630–750 870–1040 1040–1600 1100–1670

GaN InGaN A1GaAs GaInP InGaAs InGaAsP GaInNAs

GaP 0.5

1.0 1.5 Energy gap (eV)

2.0

2.5

Bandgap engineering

Commercial applications of quantum dot lasers may not be far away but tailoring the properties of semiconductor lasers does not need to wait for that. Semiconductor lasers from infrared to ultraviolet can now be readily produced. The technique is based on each compound having a certain lattice spacing and a certain energy gap. This is shown for a number of compounds of varying compositions in Fig. 12.15. It may for example be seen that the line connecting GaAs with AlAs is nearly horizontal, that is, by adding judicious amount of Al to GaAs, we can realize compounds which have a fairly large range of energy gaps with roughly the same lattice constant. The general problem may be stated as follows. Once the wavelength is chosen (say 1.55 µm, desirable for ﬁbre communications) three compounds with approximately the same lattice spacing∗ must be found: compound 1 to serve as the highly doped substrate, compound 2 to provide the active region, and compound 3 to provide the material with the higher energy gap and lower refractive index. Bandgap engineering has become a sophisticated science. A guide to materials and laser wavelength ranges is given in Table 12.1 and a ‘road map’ of how to construct ternary compounds for particular bandgaps and lattice spacing is given in Fig. 12.15, where we give most of the III–V compounds having a cubic lattice (zinc blende types). The hexagonal lattice of the nitrides does not ﬁt this pattern, neither do they ﬁt comfortably on any substrate. However, considerable alloying is possible within the InN, GaN, and AlN materials to get practically any energy gap between 1.9 and 6.2 eV, even below 1.9 eV because of band bowing. For the cubic structures, alloys even stretch to quaternary compounds, which gives the possibility of a range of energy gaps for a ﬁxed lattice, or vice versa.

Semiconductor lasers The nitrides have added another facet to bandgap engineering. Generally among the III–Vs we ﬁnd that large lattice spacing corresponds to small energy gap—see the extremes of InSb and GaP in Fig. 12.15; nitrogen is the smallest atom we consider in the semiconductor components of Table 8.2, even smaller than carbon and boron which have lower atomic numbers and weights. So adding N as an isoelectronic replacement for As or P will decrease the mean lattice spacing, but the highly electronegative and piezoelectric nature of N means that the bandgap is reduced by the large bowing factor.∗ There is an interesting group called the ‘Gina’ alloys (Ga In N As). Gallium arsenide has the most advanced technology of all the III–Vs so it is much in demand as a substrate, good quality slices are available to grow on other compounds by MBE or MOCVD. However they have to be lattice matched. From Fig. 12.15 it can be seen that GaAlAs will lattice match all the way to AlAs, that is the bandgap can go to 2.2 eV well into the visible. Now by adding N and In to GaAs it is possible to keep the mean lattice spacing constant (N goes down, In up), provided the added concentrations of In and N are in the ratio of 3:1. Both these materials reduce the energy gap. So a Gina alloy to lattice match GaAs is Ga1–3x In3x Nx As1–x . An example is 3x = 0.53 which gives a bandgap of 0.74 eV. These infrared alloys have been used to make lasers to match the desirable optical ﬁbre wavelength of 1.3 µm, and for solar cells. At the other end of the spectrum, the shortest wavelength of 342 nm (corresponding to a gap of 3.6 eV) was achieved with a GaN compound which contained no indium. What should we do if we wish to have a high power semiconductor laser? Instead of one laser, we can produce an array of lasers (Fig. 12.16) grown on the same substrate and lightly coupled to each other. There may be as many as 40 diodes in an array capable of producing several watts of output power. The difﬁculty is to persuade all the lasers to radiate in phase. Next, I wish to mention a relatively new development in which the diode lasers emit light in the same direction as the current ﬂows. They are called Vertical Cavity Surface Emitting Lasers. Their structure is shown in Fig. 12.17.

317

∗ When

Ga and In are mixed in the proportion of 1 – x and x, one would expect the resulting energy gap to be Eg (Ga1–x Inx N) = (1 – x)Eg (GaN) + xEg (InN), but the actual energy gap turns out to be smaller. An empirical formula gives the reduction in the form bx(1 – x) where b is called the bowing factor. In any case it is difﬁcult to predict the exact energy gap owing to the fact that nitrides do not form large single crystals or uniform alloys. There are compositional variations and strains as well as piezoelectric effects throughout the MOCVD layers.

Fig. 12.16 An array of lasers.

Top contact

Bragg reﬂectors Active layer Bragg reﬂectors

Substrate

Fig. 12.17 Light output

Schematic representation of a Vertical Cavity Surface Emitting Laser.

318

Lasers

λ0,2

λ0,1 λ0,0

λ1,0

λ2,0

Fig. 12.18 An array of VCSEL lasers.

The active layer still consists of multiple quantum wells. The main difference is that the Bragg reﬂectors are at the top and bottom. They can be produced by the same techniques as the wells, and they can be made highly reﬂective. In the realization of Fig. 12.17, the reﬂector at the top has a reﬂection coefﬁcient very near to unity, whereas the reﬂection coefﬁcient of the bottom reﬂector is somewhat smaller, allowing the radiation to come through the transparent substrate. The area of the laser can now be made very small leading to even smaller threshold currents (≪ 0.1 mA). A further advantage is the ease with which arrays can be made. A two-dimensional array is shown in Fig. 12.18, where each microlaser may work at the same wavelength (to produce a high output) or may be tuned to different wavelengths.

12.7.4

Quantum cascade lasers

Before concluding the story of semiconductor lasers, it may be worth mentioning a relative, the quantum cascade laser, that does not quite belong to the family. The family trait, as repeated many times, is the descent of the electron from the conduction band to the valence band and the subsequent emission of a photon, of one single photon. The quantum cascade laser, conceived in the early 1970s, is an exception. All the things that matter happen in the conduction band. The basic principle of operation of the quantum cascade laser is shown in Fig. 12.19. There are two semiconductor materials, A and B, which are alternately deposited upon each other (say, one hundred of them) by molecular beam epitaxy (Fig. 12.19). A is the active material which has a conduction band edge much below that of semiconductor B. Lasing action takes place between energy levels 1 and 2. The wavelength of the emitted light depends on E, the difference between the two energy levels. There is also a voltage applied across the whole sandwich. For simplicity let us assume that there is a voltage drop, VB across each piece of semiconductor B but none across semiconductor A, and choose this voltage to be eVB . Let’s start with an electron, on the left-hand end of Fig. 12.19, just entering from semiconductor B into semiconductor A at the energy level 2. It sees energy level 1 to be empty. Hence it descends from level 2 to level 1 by emitting a photon of frequency f = E/h. But semiconductor B is designed to be thin enough so that electrons can tunnel through it if they ﬁnd a convenient

B A B Level 2

A

B A

ΔE Level 1

Fig. 12.19 Energy diagram for a quantum cascade laser.

B

Laser modes and control techniques energy level on the other side to tunnel into. The drop across semiconductor B being equal to VB ensures that the electron can tunnel from level 1 of semiconductor A on the left-hand side of B to level 2 of the next semiconductor A on the right-hand side of B, and then the whole thing starts again. The electron descends, emits a photon, tunnels across, descends, emits a photon, and so on until it ﬁnds the last semiconductor A. If there are 50 layers of semiconductor A, then a single electron will produce 50 photons. From the point of view of the electron, this is like a cascaded ornamental waterfall. By the end the electron will have lost all its energy. From the point of view of the photon, this is an exercise in gathering strength. The energy difference between levels 1 and 2 depends on the thickness of semiconductor A. Hence, the laser wavelength can be changed by choosing the appropriate material thickness. The wavelength range quantum cascade lasers can cover is large, from about 3 to 17 µm. The principles upon which quantum cascade lasers work were enunciated in the 1970s but they have only recently entered the market place. Why? You can appreciate the reasons: it is the extreme accuracy required. Each layer must have a certain number of atoms, not an atom more not an atom less. As you can see, semiconductor lasers of all kinds have made and are making great leaps forward. They are poised to acquire the same dominance in lasers as other semiconductor devices enjoy in generating and amplifying lower frequency signals and in the ﬁeld of switching.

12.8 Laser modes and control techniques Having discussed the principles of operation of a large number of lasers, let us see now in a little more detail how the electric ﬁeld varies inside a laser resonator and describe a few methods of controlling the mode purity and the duration of laser oscillations.

12.8.1

Transverse modes

What will be the amplitude distribution of the electromagnetic wave in the laser resonator? Will it be more or less uniform, or will it vary violently over the cross-section? These questions were answered in a classical paper by Kogelnik and Li in 1966, showing both theoretically and experimentally the possible modes in a laser resonator. The experiments were performed in a He–Ne laser, producing the mode patterns of Fig. 12.20. For most applications we would like a nice clean beam, as shown in the upper left-hand corner. How can we eliminate the others? By introducing losses for the higher-order modes. This may be done, for example, by reducing the size of the reﬂector. Since the higherorder modes have higher diffraction losses (they radiate out more), this will distinguish them in favour of the fundamental mode. However, this will inﬂuence laser operation in the fundamental mode as well; thus a more effective method is to place an iris diaphragm into the resonator, which lets through the fundamental mode but ‘intercepts’ the higher-order modes.

319

320

Lasers

Fig. 12.20 Experimentally measured transverse mode patterns in a He–Ne laser having a resonator of rectangular symmetry (H. Kogelnik and T. Li, Proc. IEEE 54, pp. 1312–1329, Oct. 1966).

12.8.2

Resonator loss Laser gain f cm /2L Laser output

f

Fig. 12.21 The inversion curve of a laser and the possible axial modes as a function of frequency.

Axial modes

As mentioned in Section 12.5 and shown in Fig. 12.21, laser oscillations are possible at a number of axial modes, each having an integral number of halfwavelengths in the resonator. The frequency difference between the nearest modes is cm /2L (see Exercise 12.7), where L is the length of the resonator, and cm is the velocity of light in the medium. How can we have a single frequency output? One way is to reduce the length of the resonator so that only one mode exists within the inversion range of the laser. Another technique is to use the good ofﬁces of another resonator. This is shown in Fig. 12.22, where a so-called Fabry–Perot etalon, a piece of dielectric slab with two partially reﬂecting mirrors, is inserted into the laser resonator. It turns out that the resonances of this composite structure follow those of the etalon, that is, the frequency spacing is cm /2d, where d is the etalon thickness. Since d ≪ L, single frequency operation becomes possible. Are we not losing too much power by eliminating that many axial modes? No, we lose very little power because the modes are not independent of each other. The best explanation is a kind of optical Darwinism or the survival of the ﬁttest. Imagine a pack of young animals (modes) competing for a certain amount of food (inverted population). If the growth of some of the animals is prevented, the others grow fatter. This is called mode competition.

Laser modes and control techniques

321

L

Tilted etalon

Laser gain medium

Fig. 12.22

M1

12.8.3

M2

Q switching

This is a method for concentrating a large amount of power into a short time period. It is based on the fact that for the build-up of oscillations a feedback mechanism is needed, usually provided by mirrors. If pumping goes on, but we spoil the reﬂectivity of one of the mirrors (i.e. spoil the Q of the resonator) by some means, then there will be a lot of population inversion without any output. If the reﬂectivity is restored (i.e. the Q is switched) for a short period to its normal value, the laser oscillations can suddenly build up, resulting in a giant pulse output. The pulse duration might be as short as a few nanoseconds, the power as much as 1010 W, and the repetition frequency may be up to 100 kHz. The easiest, though not the most practical, way of spoiling the Q is by rotating the mirror. The Q is then high only for the short period the mirrors are nearly parallel.

12.8.4

Cavity dumping

This is another, very similar method for obtaining short pulses also based on manipulating the Q of the resonator (called also ‘cavity’; that’s where the name comes from). We let the pump work and make the reﬂectivity 100% for a certain period, so the oscillations can build up but cannot get out. If we now lower the reﬂectivity to zero, all the accumulated energy will be dumped in a time equal to twice the transit time across the resonator. The method may be used up to about a repetition rate of 30 MHz.

12.8.5

Mode locking

We have implied earlier that it is undesirable to have a number of axial modes in a laser. This is not always so. The large number of modes may come useful if we wish to produce very short pulses of the order of picoseconds. The trick is to bring the various axial modes into deﬁnite relationships with each other. How will that help in producing short pulses? It is possible to get a rough idea by doing a little mathematics. Let us assume that there are N + 1 modes oscillating at frequencies ω0 + lω, where l = (–N/2, . . . , 0, . . . , N/2), that they all have the same phase and amplitude, and they all travel in the positive z-direction

Schematic representation of a laser oscillator in which single mode operation is achieved with the aid of an etalon.

322

Lasers (the set travelling in the opposite direction will make a similar contribution). The electric ﬁeld may then be written in the form,

E (z, t) = E0

N/2

exp[–i(ω0 + lω)(t – z/cm )]

l = –N/2

= E0 exp[–iω0 (t – z/cm )]F(t – z/cm ),

(12.50)

where E0 is a constant, and F(x) =

These are usually two-section devices, one section to provide optical gain, and the other one to act as a saturable absorber.

sin( 21 Nωx) sin( 21 ωx)

.

(12.51)

Equation (12.50) represents a travelling wave, whose frequency is ω0 , and its shape (envelope) is given by the function, F. If N ≫ 1, F is of the form of a sharp pulse of width 4π/Nω, and it is repeated with a frequency of ω. Taking N = 100, a resonator length of 10 cm, and a refractive index of 2, we get a pulsewidth of 27 ps and a repetition frequency of 750 MHz. The situation is, of course, a lot more complicated in a practical laser, but the above ﬁgures give good guidance. The shortest pulses to date have been obtained in dye lasers with pulsewidths well below 1 ps. How can we lock the modes? The most popular method is to put a saturable absorber in the resonator which attenuates at low ﬁelds but not at high ﬁelds. Why would a saturable absorber lock the modes? A rough answer may be produced by the following argument: when the modes are randomly phased relative to each other, the sum of the amplitudes at any given moment is small, hence they will be adversely affected by the saturable absorber. However, if they all add up in phase, their amplitude becomes large, and they will not be affected by the saturable absorber. Thus, the only mode of operation that has a chance of building up is the one where the modes are locked; consequently, that will be the only one to survive in the long run (where long means a few nanoseconds). This is another example of optical Darwinism.

12.9

Parametric oscillators

In principle, this is the same thing as already explained in connection with varactor diodes in Section 9.13. The main differences are that in the present case (i) the nonlinear capacitance is replaced by a nonlinear optical medium, (ii) the dimensions are now large in comparison with the wavelength; hence wave propagation effects need to be taken into account, and (iii) instead of ampliﬁers, we are concerned here with oscillators (although optical parametric ampliﬁers also exist). What is the advantage of parametric oscillators? Why should we worry about three separate frequencies, when we can easily build oscillators at single frequencies? The reason is that we can have tuneable outputs. A schematic diagram of the optical parametric oscillator is shown in Fig. 12.23. The parametric pump (not to be confused with the pump needed to make the laser work) is a laser oscillating at ω3 . There is also a resonator

Optical ﬁbre ampliﬁers Laser oscillator

ω3

Focusing lens

Optic axis of crystal

323 ω1, ω2, ω3 ω1

q

ω3

ω3

ω2 ω3

Laser medium R1 ≅ 100% R2 ≅ 100% R3 = 0%

Nonlinear crystal

R1 (high but 1.85 eV tunnel junction second junction GaAs absorbs light 1.85eV > E > 1.4eV tunnel junction third junction GaInAs absorbs light 1.4eV > E > 1eV tunnel junction fourth junction Ge absorbs light 1eV > E > 0.67eV GaAs or Ge substrate

Fig. 13.3 Schematic drawing of proposed four-junction solar cell, parts of which have been made and tested.

In a phototransistor the base is not connected. Instead, it is exposed to the input light, which creates the carriers providing the base current. The base current is then ampliﬁed in the usual manner. Perhaps I should add that ampliﬁcation is a good thing but not the only thing to consider. Under certain conditions noise performance may be a more important criterion when choosing a particular detector. All the photodetectors mentioned so far needed an applied voltage. It should be noted, however, that it is not necessary in this case. Light may be detected in a p–n junction simply by short-circuiting it via a microammeter of very low resistance, which serves as the load. The electrons and holes generated by light in the junction will move under the effect of the built-in voltage and drive a current through the ammeter. The measured current turns out to be proportional to the input light intensity. This arrangement is usually referred to as the photovoltaic operation of the junction. A photovoltaic cell energized by the sun becomes a solar battery. When we used to worry about the ‘energy crisis’ it was hoped that acres of solar cells would replace nasty, dirty power stations. This has not quite come off, mainly for economic reasons. A simple calculation shows that, even with a generous estimate for the lifetime of a solar cell, the total energy it will generate is less than that required to purify and fabricate the single crystal slice from which it is made. So single crystals are deﬁnitely out, except for applications when money is no object—as in space vehicles. Amorphous materials, however, which we brieﬂy discussed in Section 8.9, can be used, as the economics are more favourable. The amorphous semiconductor with the most advanced technology is silicon. It is possible to process it in a wide variety of ways, so that its texture absorbs light well, and the actual absorption edge can be shifted to give a better match to the sun’s output than is obtained by the much more clearly deﬁned single crystal. Amorphous silicon is usually deposited in a vacuum or reduced gas pressure as a thin ﬁlm. This makes it possible to optimize the ﬁlm thickness—thick enough to absorb light, but not so massive that the much shorter carrier lifetimes and diffusion lengths lead to loss of carriers before they participate in useful current. A typical solar cell would consist of successive n- and p-layers sputtered on a metallized substrate and superposed by a transparent metal top electrode. There are many varieties and, in fact, the variables are so numerous that solar cells have made many PhD theses but have not yet solved the energy problem. However, one commercial realization, now commonplace, is the solar battery driven calculator. Other materials that have seemed promising include CdTe and CuInSe2 as components in multistage solar converters which absorb some of the light photovoltaically and reﬂect or transmit other wavelengths to different energy gap devices. One advantage of working as a photovoltaic engineer is that you have two levels of costing and seeking efﬁciency. On the one hand, there is the space vehicle market where photovoltaics are looked upon as essential but relatively cheap accessories to a vehicle whose cost is astronomical, so a bit more efﬁciency is worth paying for. On the other hand there is the power station replacement market where you need acres of photo cells and your competitor is coal which comes out of the ground with low cost. Figure 13.3 is a schematic drawing of a four-level solar cell. It uses a thin top layer of GaInP with an energy gap of 1.85 eV, then successive layers of

Light emitting diodes (LEDs) materials to utilize the longer wavelengths in sunlight, including a GINA alloy mentioned in Section 12.7.3. The expected conversion efﬁciency is 41% compared with about 30% for a single junction device. The four-stage device is made by MOCVD so is more expensive than coal, but it can be used with mirrors or lenses to concentrate light up to 500 suns, where its expected efﬁciency is over 50%. Possibly some hope for the terrestrial market as the technology advances. So far we have talked about light detectors but since the principles are more or less the same, this is also the place to treat infrared∗ detectors. The primary form of detection in that region too is the change in the conductivity of the material induced by incident radiation. The materials are again semiconductors. The devices rely on band-to-band transition up to 10 µm, requiring small energy gap semiconductors. Semiconductors of even smaller energy gap can be found, so in principle, band-to-band transition could be used for even longer wavelengths, but in practice this range from 10–100 µm is covered by impurity semiconductors in which the increased conductivity is obtained by exciting an electron from a donor level into the conduction band (or from the valence band into an acceptor level). Infrared radiation between† 100 µm and 1 mm is usually detected with the aid of the so-called ‘free carrier absorption’. This is concerned with the excitation of electrons from lower to higher energy levels in the conduction band. The number of electrons available for conduction does not change, but the mobility does, owing to the perturbed energy distribution of the electrons. The change (not necessarily increase) in conductivity may then be related to the strength of the incident infrared radiation. Since electrons may be excited to higher energy levels by lattice vibrations as well (thus masking the effect of the input infrared radiation) the crystal is usually cooled. Relative newcomers to the family are the QWIPs (Quantum Well Infrared Photodetectors) and the QDIPs (Quantum Dot Infrared Photodetectors) which work by exciting electrons from discrete energy levels into the high energy continuum.

13.3 Light emitting diodes (LEDs) Semiconductor lasers have been discussed in some detail in Section 12.7. We came to the conclusion that it is a good thing to have a good semiconductor laser: it has many applications. Are bad lasers good for anything? Yes, certainly, as long as they can emit light. How do we make a bad laser? By depriving a good laser of its cavity. The injected carriers may still recombine and emit light but in the absence of the cavity there is no agent to take care of the phase relationships and consequently the emitted light will not be coherent and will not emerge as a narrow beam. But that is exactly what we want if the aim is to use the semiconductor diode for lighting: we want a diffuse light coming out in all directions. This light source does indeed exist. It is called a light emitting diode, abbreviated as an LED. In fact, LEDs were invented in 1960, a few years before semiconductor lasers. The ﬁrst specimen emitted red light. They were made initially of GaAsP alloys (GaAs has an infrared energy gap, which is increased by adding the lighter element P). Too much P induces an indirect gap, so the other alloy

341

∗ Purists

might object saying that the command ‘let there be light’ was restricted to the visible region, but we think that is a too narrow interpretation.

† Some

care needs to be exercised with terminology. This region used to be called the submillimetre region. The latest fashion is to talk about frequency rather than wavelength. 300 GHz would correspond to 1 mm wavelength, 1 THz to 0.3 mm and 100 THz to 3 µm.

342

Optoelectronics

∗ Electronegative

atoms

When a covalent bond is formed between two different elements such as the III–Vs or II–VIs, the electron distribution is not symmetrical between the elements because it is energetically favourable for the electron pair to be found closer to one atom. The atom which draws the bonding electrons more closely to it is called more electronegative. This is a polar bond, in other words the covalent bond is partly ionic, as we have shown for some cases in Table 8.3. The following table was compiled by Linus Pauling (Table 13.1).

Table 13.1 Electronegativities of elements Be 1.5

B 2.0

C 2.5

N 3.0

O 3.5

Mg 1.2

Al 1.5

Si 1.8

P 2.1

S 2.5

Ca 1.0

Ga 1.6

Ge 1.8

As 2.0

Se 2.4

Sr 1.0

In 1.7

Sn 1.8

Sb 1.9

Te 2.1

The above table appears to have been produced by intuition and genius, a powerful combination. Somewhat similar results can be obtained by equating the electronegativity to the average of the ionization energy and electron afﬁnity of the element, namely, E = 12 (I + Eaff ). This is common sense, since high Eaff means the atom wants to collect spare electrons, and high I means it will hold on to them. From the table, it can be seen that the nitrides of Ga, In, and Al have a marked imbalance of electrons, giving a large ionic or polar component to the covalent bond. † A crucial factor in the success of the In-

GaN story was that the Nichia Chemical Industries outﬁt in Japan had alone and presciently worked on making and processing GaN during most of the 1980s. Their principal scientist Shuji Nakamura and his colleagues published the crucial paper in 1992, and many further results since.

GaAlAs has been used to get well into the visible. These energy gaps are shown in Fig. 12.15 which also shows that the lattice parameters of GaAs and AlAs are very similar, so AlAs layers can be grown on GaAs substrate. LEDs in the blue and green were intially made from ZnS and ZnSe, using MBE, or even ion implantation, to get both n- and p-types. But the whole scenario of applications and usefulness of LEDs has changed in the past decade by the advent of InGaN devices. The nitrides were regarded by most people making LEDs in 1990 as ‘scientiﬁcally interesting’, which to commercially minded scientists, meant ‘black hole for time and money’. However, the basic idea was attractive; if alloys of InN, GaN, and AlN were available, LEDs could be made from direct gap semiconductors from the red (1.89 eV) into the UV (6.2 eV). The main problem had been that there was no way of getting a suitable substrate that could be used for epitaxial growth. The nitrides, typically GaN, have the wurtzite structure, with strong ionicity due to the small, electronegative N atoms.∗ So, the ionic as well as covalent nature of the bond gives a very high melting point. Attempts to grow single crystals by the method outlined in Section 8.11, and even more modern and sophisticated versions of this apparatus failed to produce anything better than fractured crystals a few millimetres across. The ﬁrst breakthrough came when it proved possible to grow a good mirror ﬁnish GaN layer on a sapphire substrate. This used a MOCVD process. First a ‘nucleating’ layer was put down at a relatively low substrate temperature 700–800 K, then a second faster deposition at 1100– 1300 K, this coalesced the ﬁrst layer and surprisingly good LEDs were made. Surprising, because the large lattice mismatch (about 16%) caused threading defects to reach through to the active layer even though different buffer layers and thicker active layers were tried. The dislocation density could not be reduced below 108 –1010 cm–2 . But the LEDs shone brilliantly, particularly in the blue and green where the II–VI opposition devices immediately became obsolete. LED law, based on GaAsP and GaP(ZnO), the earlier red diodes which some of us still have in our pocket calculators, was that dislocation density greater than 104 cm–2 killed light emission. InGaN was outside this law. The In is important because pure GaN does not luminesce very well. Around 1 part in 100 of In makes all the difference, and of course you need more In than that to get through the visible spectrum. A second problem that had to be solved before these diodes could be made was that initially it was difﬁcult to make ptype material. This is a snag that cropped up many years ago when CdS seemed a good optical device material. It was never completely solved although some p-type CdS was made by MBE. The crucial thing was to avoid thermodynamic equilibrium that caused p-type centres to be swamped. The same sort of problem with GaN was occasioned largely by the fact that heat treatment (faster growth) of a p-type impurity led to compensating reactions (electrons cluster round holes). It was solved by using Mg impurity in the MOCVD process and annealing in N2 which stopped the compensation. Thus, by 1992† good quality InGaN ﬁlms were available to make the ﬁrst successful blue DH LEDs. A further reﬁnement was to add a single quantum well (SQW) to the structure and soon after, a multiple quantum well (MQW). A typical LED is sketched in Fig. 13.4. Quite complicated compared to the simple pn junction of earlier days. In particular, there is a special thin InGaN emitting layer, where the recombination of electrons and holes from the pn layers occurs. This controls the

Light emitting diodes (LEDs)

343

p-electrode p-GaN p-Al0.3Ga0.7N In0.2Ga0.8N n-In0.02Ga0.98N

n-electrode

n-Al0.3Ga0.7N n-GaN GaN buffer layer

Sapphire substrate

Fig. 13.4 Typical layer structure of a QW based nitride LED. ∗ Not

only does composition deﬁne the wavelength. The nitrides are very non-centro-symmetric and have a large piezo-electric constant (Section 10.11), so the strains and dislocations cause a big internal ﬁeld; this gives wavelength shift by the Stark effect, particularly in the quantum well structure (Section 13.10.3 and 13.4). 100 Relative intensity (arb. units)

operating wavelength.∗ Forming and consolidating the buffer layer is almost an art form. A black art many say. However, an elaborate process called epitaxial lateral overgrowth (ELOG) involving chemical vapour deposition (CVD) of a layer of SiO2 , subsequently penetrated by windows a few micrometres wide by conventional masking and etching. This structure is overlaid by further InGaN MOCVD grading and growth layers. The distortion causes lots of extra strain, but in some regions of the resulting overlayer the dislocation density is below 106 cm–2 . Unfortunately, there is very little change in device performance across such a layer, except that for pure GaN, which is not very luminescent, there is a marked improvement at low defect density. So the practical answer is to keep some In and no ELOG. This is borne out by Fig. 13.5, which shows how the quantum efﬁciency varies with In content, from work done a few years ago. Recently the quantum efﬁciency of InGaN LEDs reached 30% at violetblue wavelengths at 20 mA current, a power of 21 mW emitted in the blue, and 7 mW in the green, corresponding to about 60–30 lumens W–1 . High brightness red LEDs are up to 50% efﬁcient. This has led the way to commercial usage of LEDs. There are large colour displays,† signal and trafﬁc lights, automotive uses including stop and rear lights, also for cycles. The estimated life of InGaN LEDs at present, from accelerated and projected life testing is about 10 years’ continuous use. For an average room light duty cycle this gives 60 years! The long life, low maintenance, is also the main selling point for trafﬁc lights. It makes some local authorities, even in the UK, look further forward than the next ﬁnancial year, normally their absolute limit to thinking ahead. So how can we assess the state of InGaN LED technology? The nitrides are still difﬁcult to grow as reasonable epitaxial layers, and the very successful LEDs have been made on small crystals, typically a 5 nm-thick active layer. There is no good theory of why they work. So we are in a situation of technological success leading to a rapidly expanding semiconductor lighting industry without proper scientiﬁc backing. This has happened before, maybe steam engines were somewhat like this before thermodynamics caught up. But following the precise science/technology advance of solid state circuit electronics, it is a bit of a shock. We must hope that all will become clearer when better material is available. Meanwhile, we can conjecture that the necessary

80 60 40 20 0 367 369 371 373 375 377 379 381 Emission peak wavelength (nm)

Fig. 13.5 Relative output power of uv InGaN SQW LEDs as a function of emission peak wavelength. The dots show increasing In mole fractions from practically 0% on the left to 4% on the right. † A display that can be described as large

without any exaggeration was used to illuminate the stage at the opening ceremony of the Beijing Olympics in 2008. It employed 44 000 LEDs in a display having dimensions of 36 m × 147 m.

344

∗ In

the book edited by B. Gil listed in further reading Appendix VIII.

Optoelectronics small quantity of In in GaN leads to localized deep levels that produce relatively stable excitons; and as their constituents move in the strong ﬁelds the recombination is rapid. It has been estimated that the diffusion length of minority carriers (before recombination) is 50–60 nm. Thus radiative recombination would occur before a non radiative encounter at a threading dislocation, even with dislocation densities of 1010 cm–2 . As we have said several times, the variable quality, internal strains and piezo electric ﬁelds mask the correlation between bandgap and emitted light. An interesting summary based on experimental results of numerous InGaN LEDs has been made by P. K. O’Donnell∗ who gives the following equation in terms of x, the molecular fraction of In in InGaN (i.e. Inx Ga1–x N) for the peak of the emitted light Ep (in eV). Ep = 3.41 – 4.3x

† For

example, recent work [H. Hirayama et al., Appl. Phys. Express 1, 051101 (2008)] with deep ultraviolet diodes has shown that if threading dislocations in the buffer layer are reduced, efﬁciency is improved. The deep UV region around 230–380 nm (over 5 eV) is potentially important as a sterilizing antibiotic agent for surgical instruments, food-processing machinery, and water supplies, which usually cannot be ﬂooded with sterilizing liquids. It is getting close to soft X-rays and could be useful for imaging the large molecules that are important for life. The diodes used were made of an Alx Ga1-x N alloy as the energy gap is beyond GaN (see Table 8.3), with an x value of about 0.87. They were grown on sapphire substrates by low-pressure MOCVD, with a buffer layer. This is a very difﬁcult device region; initially, Hirayama et al. obtained a diode output of 5 µW with a quantum efﬁciency of 0.001%, but by reducing the quantum well thickness to only 1.3 nm and introducing an AlN buffer layer to reduce dislocations from about 3.2 × 109 cm–2 to 1.8 × 109 cm–2 , they obtained an output of 150 µW with a quantum efﬁciency of 0.2%. So the device is still of low efﬁciency but better, a striking advance.

There is a spread of about 10% in these coefﬁcients, and it applies only for x between 0–0.5. In summary, we can say that considerable progress continues in many features† of LEDs, including substrates of slightly larger GaN “mirror ﬁnish” slices (still grown on sapphire). Skilled provision of buffer layers reduces spreading dislocations. Selection of inclined planes for growth has improved performance and yield in some devices. But the main goal of room lighting is still some way off. Blue LEDs coated with composite phosphors have produced white light, fairly well matched to sunlight, at 15 lumens W–1 , giving about 20 lumens per diode. The snag is that they are still expensive and around 100 are needed to match a 100 W tungsten ﬁlament bulb. However, we routinely use LED torches and lanterns, battery powered. So if we were prepared to bulk buy white diodes and rewire our lighting system to 5 V d.c., we could have energy-efﬁcient room lights now. But if this were seriously proposed we think the voters would rebel at the capital cost, even although they can no longer get their 100 W bulbs from Woolworths. So room lighting is still a challenge. Maybe InGaN LEDs will have to compete with OLEDs (Organic LEDs) for efﬁcient replacement of our old fashioned lighting, see Appendix I. Finally, a word about the environment. Electricity is mainly produced by fossil fuel which causes the undesirable CO2 emission. Over one ﬁfth of the electricity consumption in developed countries is due to lighting and the proportion is even higher in developing countries. If the use of LED lamps will halve that consumption that, would save, it has been calculated, 300 Megatons of CO2 emission in the US alone. Will that happen? As I said, I feel quite certain that white LEDs will come in due course. High power white LEDs for practical lighting systems have already been developed by several companies (for example, Cree, Nicia, and Seoul Semiconductor). Global trials took place in 2012 in 12 major cities (including Kolkata, London, Rio de Janeiro, Sydney, Toronto, and New York) and showed up to 85% energy saving. On a lesser but a more local scale, trials took place in 2010 at Imperial College, London, which suggested a lifetime of 7 years (3–4 times that of conventional lighting) with a payback period of 4 years for the ﬁttings. LED lighting is coming.

Electro-optic, photorefractive, and nonlinear materials

345

13.4 Electro-optic, photorefractive, and nonlinear materials Before talking more about applications, I shall ﬁrst review some properties of materials which make them suitable components for devices. In electro-optic materials, the application of an electric ﬁeld will affect the index of refraction that an optical wave ‘sees’. Note that waves with different electric polarizations are differently affected. The exact relationships are given by tensors, a subject I am reluctant to enter, but if you are interested you can attempt Exercise 13.6. Let me just say that the dielectric tensor (which relates the three components of the electric ﬁeld to the three components of the dielectric displacement) has nine terms, and each of these terms may depend on the three components of the electric ﬁeld. Thus, altogether, the electro-optic tensor has 27 components (only 18 if the symmetry of the dielectric tensor is taken into account). There is no need to worry. In practice, usually, only one of the numerous components is needed, and the effect may be presented in the form, 1 = rE . (13.1) ǫr

r is the electro-optic coefﬁcient.

Since ǫr = n2 , the change in refractive index may be written as n = – 21 n3 rE .

(13.2)

Taking LiNbO3 as an example, n = 2.29, and for a certain orientation of the crystal we have r = 3.08 × 10–11 m V–1 . With reasonable voltages, one may obtain an electric ﬁeld of about 106 V m–1 , causing a change in the refractive index of n = 1.86 × 10–4 . It does not seem a lot, but it is more than enough for a number of applications. The indices of refraction and the electro-optic coefﬁcients for some often used materials are given in Table 13.2. The essential thing to remember is that in electro-optic crystals the refractive index, and consequently the propagation of the wave, may be changed by applying an electric ﬁeld. The properties of electro-optic materials are dependent, of course, on direction, but since the aim is no more than to give a general idea of the ranges involved, only the largest components are listed for each material. The wavelengths at which these values were measured are also indicated. Table 13.2 Properties of electro-optic materials Substance

Wavelength (µm)

Electro-optic coefﬁcient (10–12 m V–1 )

Index of refraction

Static dielectric constant

Bi12 SiO20 BaTiO3 CdTe GaAs KNbO3 LiNbO3 ZnO

0.514 0.514 1.0 1.15 0.633 0.633 0.633

2.3 820 4.5 1.43 380 32.6 2.6

2.22 2.49 2.84 3.43 2.33 2.29 2.01

56 4300 9.4 12.3 50 78 8.15

Note that r may be positive or negative depending on crystal orientation.

346

Optoelectronics

χ (1) is the linear susceptibility (what we called before simply susceptibility and denoted by χ ), and χ (2) and χ (3) are known as the quadratic and cubic susceptibilities. I is the intensity, n0 is the index of refraction under linear conditions, and n2 is the measure of nonlinearity.

Photorefractive materials represent a rather special class of crystals which are both electro-optic and photoconductive. Some representatives of these materials are LiNbO3 , Bi12 SiO20 and BaTiO3 . I shall return to them in the next section. Nonlinear materials are usually characterized by relating the dielectric polarization, P, to the electric ﬁeld. The linear relationship given by eqn (10.5) may be generalized and written in the form, $ % (13.3) P = ǫ0 χ (1) E + χ (2) E 2 + χ (3) E 3 . In some materials the nonlinearity may be more conveniently expressed with the aid of the index of refraction as n = n0 + n2 I.

(13.4)

Intensity dependent absorption is also possible. In fact one of the very interesting devices to be presented in Section 13.11 operates on that basis.

13.5

Volume holography and phase conjugation

I have already mentioned (Section 12.13) some of the interesting optical phenomena holography can produce. I shall now brieﬂy talk about one particular branch of holography, known as volume holography, and discuss what happens in the simplest possible case, when both the reference beam and the object beam are plane waves (Fig. 13.6). The distinguishing feature of volume holography is that the recording process takes place in the volume of the photosensitive material. Let us now do a little mathematics. The amplitudes of the two waves may be written in the form,

Photosensitive medium object wave

θ

θ

Aref = A10 exp[ik(x cos θ + y sin θ )] Aobj = A20 exp[ik(x cos θ – y sin θ )],

reference wave Interference pattern

(13.5) (13.6)

leading to the interference pattern (note that the intensity, I, is proportional to the square of the amplitude),

y

x

Fig. 13.6 Two plane waves incident upon a photosensitive medium.

I = |Aref + Aobj |2 = A210 + A220 + 2A10 A20 cos(2ky sin θ ).

It may now be seen from the above equation that the intensity varies periodically in the y-direction with a period, =

ǫr1 is the amplitude of the modulation (ǫr1 ≪ ǫr0 ). We may call ǫr a dielectric grating or, considering that the dielectric constant affects the phase, a volume phase hologram.

(13.7)

2π λ = , 2k sin θ 2n sin θ

(13.8)

which is nothing else but the Bragg relation once more. The symbol, , is usually referred to as the grating spacing. After recording comes the processing (a black art for all known photosensitive materials) with a result that the interference pattern is turned into a modulation of the dielectric constant, that is, the end product is a dielectric constant varying as ǫr = ǫr0 + ǫr1 cos(2ky sin θ ).

(13.9)

Volume holography and phase conjugation What happens when we illuminate the hologram with the reference wave? According to the rules of holography, the object wave springs into existence. Interestingly, we could reach the same conclusion, considering Bragg diffraction. If a wave is incident upon a material with a periodic structure at an angle and wavelength that satisﬁes eqn (13.8), then a diffracted beam of appreciable amplitude will emerge. In fact, under certain circumstances it is possible to transfer all the power of the incident reference wave into the diffracted object wave. What happens when the object wave is not a plane wave but carries some pictorial information in the form of some complicated amplitude and phase distribution? Since any wave can be represented by a set of plane waves, and since the modulation of the dielectric constant is small, one can apply the principle of superposition, leading to the result that each constituent plane wave, and thus the whole picture, will be properly reconstituted. The photosensitive media most often used are silver halide emulsion (basically the same as that used for photography but with smaller grain size) and dichromated gelatin. In the former case, the refractive index modulation is due to the density variation of silver halide in the gelatin matrix. In the latter case, the mechanism has still not been reliably identiﬁed. It is quite likely that the refractive index modulation is caused again by density variations mediated by chromium, but explanations claiming the presence of voids cannot be discounted. Unfortunately, it is rather difﬁcult to know what goes on inside a material when chemical processing takes place. We can, however, trust physics. It involves much less witchcraft. So I shall make an attempt to give an explanation of the origin of dielectric constant modulation in photorefractive materials. As I mentioned previously, a photorefractive material is both photoconductive and electro-optic. Let us assume again that two plane waves are incident upon such a material, but now a voltage is applied as well, as shown in Fig. 13.7. The light intensity distribution [given by eqn (13.7)] is plotted in Fig. 13.8(a). How will the material react? The energy gap is usually large, so there will be no band-to-band transitions but, nevertheless, charge carriers (say electrons) will be excited from donor atoms, the number of excited carriers being proportional to the incident light intensity. Thus, initially, the distribution of electrons (Ne ) and ionized donor atoms (ND+ ) is as shown in Fig. 13.8(b) and (c). Note, however, that the electrons are mobile, so under the forces of diffusion (due to a gradient in carrier density) and electric ﬁeld (due to the applied voltage) they will move in the crystal. Some of them will recombine with the donor atoms while some fresh electrons will be elevated into the conduction band by the light still incident. At the end an equilibrium will be established when, at every point in space, the rate of generation will be equal to the rate of recombination. A sketch of the resulting electron and donor densities shown in Fig. 13.8(d). Since the spatial distributions of electrons and ionized donors no longer coincide, there is now a net space charge, as shown in Fig. 13.8(e). Now remember Poisson’s equation. A net space charge will necessarily lead to the appearance of an electric ﬁeld [Fig. 13.8(f)]. So we have got an electric ﬁeld which is constant in time and periodic in space. Next, we invoke the electrooptic property of the crystal which causes the dielectric constant to vary in proportion with the electric ﬁeld. We take r, the electro-optic coefﬁcient, as positive, so the dielectric constant is in anti-phase with the electric ﬁeld. We

347

photorefractive crystal

V y

Fig. 13.7 Two plane waves incident upon a photorefractive crystal across which a voltage is applied.

348

Optoelectronics (a)

I

y

0 (b)

Ne

y

0 (c)

+ ND

y

0 (d)

I + ND

Ne

y

0 net charge density

(e)

y

0 (f)

E

y

0

Fig. 13.8 The variation of a number of physical quantities in a photorefractive crystal in the y-direction: (a) intensity, (b) electron density, (c) ionized donor density, (d) electron and ionized donor density in the stationary case, (e) the net charge density, (f) the resulting electric ﬁeld, (g) the resulting dielectric constant.

(g)

εr ε rO

y

0 Λ

Λ

Λ

have come to the end of the process. The input interference pattern has now been turned into the dielectric constant variation shown in Fig. 13.8(g). We may now argue again that the process works for more complicated waves as well, so we have got the means to record holograms in photorefractive materials. Noting that the process by which the dielectric grating is produced

Volume holography and phase conjugation

349

may occur quickly (it is in a range extending from nanoseconds to seconds) we have here a real-time holographic material. In fact, the major application of photorefractive materials is not for real-time holography but for wave interaction. The phenomenon by which the incident light brings forth a dielectric constant modulation and the way this modulation reacts back (by diffracting the waves) upon the light beams, leads to all sorts of interesting effects. I shall mention only the most notable one among them, phase conjugation. The physical conﬁguration is shown in Fig. 13.9. There are three beams incident upon the material, and a fourth beam is generated. For this reason the phenomenon is often referred to as four-wave mixing. Beams 1 and 2 are known as the pump beams and beam 4 as the probe beam (usually much weaker than the pump beams). As a result of the interaction, beam 3, the so-called phase conjugate beam, is generated. The physical mechanism is fairly easy to explain. Beams 1 and 4 create a dielectric grating, as shown in Fig. 13.9(b). Beam 2, incident upon the grating, is then diffracted to produce beam 3, as shown in Fig. 13.9(c). What is so interesting about beam 3? Well, it is in a direction opposite to beam 4, but there is a lot more to it. If beam 4 consists of a range of plane

be

am

be

am

3

be

am

2

4

am

1

(a)

be

be

am

am

4

1

(b)

be

be

am

3

am

Fig. 13.9

2

be

(c)

Schematic representation of phase conjugation. (a) Incident beams 1, 2, and 4 produce the phase conjugate beam 3. (b) Beams 1 and 4 produce a grating. (c) Beam 2 is diffracted into beam 3 by the grating recorded.

350

Optoelectronics 1

Conventional mirror

4 2

3

2

3

dielectric

(a)

1

4

dielectric

Fig. 13.10 Plane waves passing through a dielectric and reﬂected by (a) a conventional mirror, (b) a phase conjugate mirror.

Phase conjugate mirror

(b)

waves, each separate plane wave is reversed to create, in the ofﬁcial jargon, a phase conjugate beam. The whole device is called a phase conjugate mirror. In what respect is a phase conjugate mirror different from an ordinary mirror? We shall give two examples. In Fig. 13.10(a) a piece of dielectric is in the way of an incident plane wave. The wavefront of the plane wave moving to the right is illustrated by continuous lines: 1 is that of the incident wave, and 2 is the wavefront after passing partially through the dielectric. After reﬂection by an ordinary mirror, the retarded part of the wavefront is still retarded, as given by 3 (dotted lines). After passing through the dielectric once more, there is a further retardation of the wavefront, as indicated by 4. In Fig. 13.10(b) wavefronts 1 and 2 are the same as previously. The phase conjugate mirror, however, ‘reverses’ the input wave. The wavefront that was retarded will now be promoted to the front as shown by 3. After passing through the dielectric for the second time, the wavefront 4 will again be smooth. The conclusion is that the phase conjugate mirror corrected the wavefront distortion introduced by the dielectric. And this would actually be true for other kinds of disturbances as well. The phase conjugate mirror reﬂects the incident wave with an opposite phase and direction. My second example is a beam diverging towards the mirror. After reﬂection the conventional mirror will make the beam diverge further [Fig. 13.11(a)] whereas the phase conjugate mirror will produce a convergent wave [Fig. 13.11(b)]. A fascinating phenomenon you must agree but, I am afraid, still at the laboratory stage.

Acousto-optic interaction

351

Conventional mirror

Phase conjugate mirror

Fig. 13.11 (a)

A divergent beam reﬂected by (a) a conventional mirror, (b) a phase conjugate mirror.

(b)

13.6 Acousto-optic interaction We have seen that periodic variation of the dielectric constant within a volume of material may help to produce a diffracted beam by the mechanism of Bragg interaction. The periodic variation may be achieved by using photosensitive and photorefractive materials, but there is one more obvious possibility which we shall now discuss. An acoustic wave propagating in a material will cause a strain, and the strain may cause a change in the dielectric constant (refractive index). The relationship between the change in the dielectric constant and the strain is given by the so-called strain–optic tensor. In the simplest case, when only one coefﬁcient needs to be considered, this may be written in the form, 1 = pS, (13.10) ǫr where p is the photoelastic coefﬁcient, and S is the strain. Thus, we can produce a volume hologram simply by launching an acoustic wave. But is a volume hologram much good if it moves? Well, it is all relative. For us anything moving with the speed of sound appears to be fast, but for an electromagnetic wave which propagates by nearly ﬁve orders of magnitude faster than a sound wave, the hologram appears to be practically stationary. There is, however, an effect characteristic to moving gratings that I must mention, and that is the Doppler shift. The frequency of the electromagnetic wave is shifted by the frequency of the acoustic wave; an effect that becomes occasionally useful in signal processing. Let us now work out the frequency of an acoustic wave needed to deﬂect an optical wave of 633 nm wavelength (the most popular line of a He–Ne laser) by, say, 2◦ . The Bragg angle is then 1◦ . Taking further LiNbO3 as the material in which the waves interact, we ﬁnd for the grating spacing, λ 633 × 10–9 = 7.92 µm, = = 2n sin θ 2 × 2.29 × sin 1◦

(13.11a)

Noting that the velocity of a longitudinal wave in LiNbO3 is 6.57 × 103 m s–1 [see Table 13.3], we ﬁnd for the frequency of the acoustic wave f = 8.30 × 108 Hz. A device which can deﬂect an optical beam can, of course, be used for modulation as well. When the acoustic wave is on, the power in the transmitted beam decreases, and a diffracted beam appears. Thus, by varying the amplitude of the acoustic wave, both output beams are modulated. It may be

is the required wavelength of the acoustic wave. This is regarded as quite high frequency, which cannot be excited without exercising due care, but nevertheless such an acoustic wave can be produced in bulk LiNbO3 and can be duly used for deﬂecting an optical beam. The device is known as a Bragg cell.

352

Optoelectronics Table 13.3 Properties of some materials used for acousto-optic interaction Substance

Wavelength (µm)

Density (103 kg m–3 )

Index of refraction

Sound velocity (103 m s–1 )

Water Fused quartz GaAs LiNbO3 LiTaO3 PbMoO4 ZnS

0.633 0.633 1.15 0.633 0.633 0.633 0.633

1 2.2 5.34 4.7 7.45 6.95 4.10

1.33 1.46 3.43 2.29 2.18 2.4 2.35

1.5 5.95 5.15 6.57 6.19 3.75 5.51

an advantage to use the diffracted beam as the modulated beam because the power in it is completely cut off when the acoustic wave is absent, whereas it is less straightforward to extinguish the transmitted beam. Could we use an acoustic wave for scanning the optical beam within a certain angular region? It can be done in more than one way. I shall just show the arrangement which makes the best sense in principle. (a)

transmitted beam

Optical input beam

θ

θ

diffracted beam

acoustic beam (b)

transmitted beam Optical input beam

θ + Δθ

θ

Fig. 13.12 Bragg reﬂection of a light beam by an acoustic wave. (a) Deﬂection angle of 2θ at an acoustic wavelength of λc , (b) deﬂection angle of 2θ + θ at an acoustic wavelength of λc + λc .

diffracted beam

Δθ /2

acoustic beam

Integrated optics

353

transmitted beam Optical input beam

diffracted beam

Fig. 13.13

photodetector array

acoustic beam

A spectrometer relying on acousto-optic interaction.

Let us say we have an optical beam incident at an angle θ to the horizontal direction. If we want to deﬂect it by 2θ , then we need an acoustic wave propagating in the vertical direction [see Fig. 13.12(a)] and having a wavelength of λac = λop /2n sin θ . How could we deﬂect the beam by a further θ ? In order to have the Bragg interaction, we need to change the acoustic wavelength to λac + λac =

λop 2n sin(θ + θ )

(13.11b)

and, in addition, tilt the acoustic wave (it can be done by using an appropriate launching array) by θ/2, as shown in Fig. 13.12(b). Our ﬁnal example is a spectrum analyser. It is essentially the same device as the beam scanner but used the other way round. The unknown input frequency to be determined is fed into the device in the form of an acoustic wave via an acoustic transducer. It will deﬂect the input optical beam by an amount which depends on the frequency of the acoustic wave. The deﬂected optical beam is then detected by an array of photodetectors (Fig. 13.13). The position of the photodetector upon which the beam is incident will then determine the unknown frequency.

13.7 Integrated optics This is not unlike integrated circuits, a subject we have discussed in detail when talking about semiconductor devices. The basic idea was to ‘integrate’, that is to put everything on a single chip and by doing so achieve compactness, ruggedness, economy of scale, etc. The same idea of integration (advanced towards the end of the 1960s) can also be applied to optical circuits with all the corresponding advantages. In principle one could have lasers, waveguides, optical processing circuits, all on the same chip. In practice, the results have been rather limited due to technological difﬁculties and, probably, inadequacy of the scale of effort. The economic imperative which was the driving force behind the integrated circuit revolution has simply not been there for their optical

354

Optoelectronics counterparts. It looks as though optical communications can come about on a wide scale, without the beneﬁt of integrated optics, so unless there is some new and urgent impetus provided by the need to develop optical computers or some other forms of optical processing, further progress is likely to remain slow. Nevertheless, it is a very promising technique, so I must give at least an introduction to its basic precepts.

13.7.1

Waveguides

The principle is very simple. If a material exhibiting a certain index of refraction is surrounded by a material of lower index of refraction, then a wave may be guided in the former material by successive total internal reﬂections. Optical ﬁbres (mentioned before) represent one such possibility for guiding waves, but that is not suitable for integrated optics. We can however rely on the fact that the refractive index of GaAs is higher than that of AlGaAs and, consequently, a GaAs layer grown on the top of AlGaAs will serve as a waveguide. As may be seen in Table 13.2, GaAs is an electro-optic crystal, it is also suitable for producing junction lasers, microwave oscillators, and transistors. Thus, altogether, GaAs seems to be the ideal material for integrated optics. Well, it is indeed the ideal material, but the problems of integration have not as yet been solved. It is still very much at the laboratory stage. Nearer to commercial application are the LiNbO3 devices, which I shall describe in more detail. In these devices the waveguides are produced by indiffusing Ti into a LiNbO3 substrate through appropriately patterned masks (the same kind of photolithography we met in Section 9.22 when discussing integrated circuits). Where Ti is indiffused the refractive index increases sufﬁciently to form a waveguide.

13.7.2

Phase shifter

Considering that LiNbO3 is electro-optic, we may construct a simple device, using two electrodes on the surface of the crystal on either side of the waveguide, and apply a voltage to it, as shown in Fig. 13.14. With a voltage V0 , we may create an electric ﬁeld roughly equal to V0 /d, where d is the distance between the electrodes. Hence, the total phase difference that can be created is V0

d

electrodes L

LiNbO3 substrate

Fig. 13.14 A phase shifter relying on the change of dielectric constant caused by the applied voltage.

Ti indiffused waveguide

Integrated optics φ =

2π Ln . λ

(13.12)

355 L is the length of the electrodes.

A voltage of 5 V with a distance of 5 µm between the electrodes gives an electric ﬁeld of 106 V m–1 for which we found previously (Section 13.4) n = 1.86 × 10–4 . A little algebra will then tell us that in order to produce a phase difference of π at a wavelength of about 1.5 µ m (good for optical communications) we need electrode lengths of about 4 mm. So we have now a phase shifter, or if we keep on varying the voltage between 0 and 5 V, we have a phase modulator.

13.7.3

Directional coupler

One of the elementary requirements of signal processing is the facility to direct the signals into different locations. In its simplest form it means [see Fig. 13.15(a)] that a signal coming in at port 1 should be divided between output ports 1′ and 2′ in any desired proportion, including the possibility that all the input power should appear at one single output port. And, similarly, power coming in at input 2 should be divided between the same output ports. The realization in integrated optics form is shown in Fig. 13.15(b). For a length of L, the two waveguides are so close to each other that there is leakage of power from one to the other. In addition, it is possible to change the relative velocity of wave propagation in the two waveguides by applying a voltage between the two electrodes. As shown in Fig. 13.15(c), the vertical component of the electric ﬁeld is in the opposite direction for the two waveguides. Hence, according to eqn (13.1) the indices of refraction will vary in the opposite direction. Let us now formulate this problem mathematically. A wave propagating in the positive z-direction with a wavenumber k1 is of the form (recall Chapter 1), (a) 1

1 Coupler

2

2

Waveguides

(b)

1

(c)

Buffer layer

Electrodes

2 Electrodes

Electric field line

Fig. 13.15

L Substrate

1

2

(a) Schematic representation of a directional coupler. (b) Integrated optics realization of the directional coupler. (c) Cross-section of the device showing also an electric ﬁeld line.

356 A10 is the amplitude of the wave at z = 0.

Optoelectronics A1 = A10 exp ik1 z.

(13.13)

This may be described by the differential equation, dA1 = ik1 A1 . dz

(13.14)

Another wave propagating in the same direction with a wavenumber, k2 , would then analogously be described by the differential equation, dA2 = ik2 A2 . dz

(13.15)

Let us identify now waves 1 and 2 with those propagating in waveguides 1 and 2. Next, we shall have to take into account coupling between the waveguides. In order to do so, we may advance the following argument. If there is coupling between the two waveguides, then the rate of change of the amplitude of the wave in waveguide 1 will also depend on the amplitude of the wave in waveguide 2, and the higher the coupling, the larger is the effect of wave 2. In mathematical form, dA1 = ik1 A1 + iκA2 . dz

(13.16)

And, similarly, the rate of change of the amplitude of wave 2 is dA2 = iκA1 + ik2 A2 . dz

The coupling coefﬁcient has been taken as iκ.

(13.17)

Note that we have met this type of coupled differential equation before when discussing quantum-mechanical problems in Chapters 5 and 7. The solution is not particularly difﬁcult; I shall leave it as an exercise (13.7) for the reader. I shall give here only the solution for the case when k1 = k2 = k, and when all the input power appears at port 1 with an amplitude A. We obtain then for the two outputs, A1 = A10 exp(ikz) cos κz

(13.18)

A2 = iA10 exp(ikz) sin κz.

(13.19)

and

It may be clearly seen that the amount of power transfer depends on the length of the coupler section. When z = L = π/2κ, all the power from waveguide 1 can be transferred to waveguide 2. With L = π/κ, the power launched in waveguide 1 will ﬁrst cross over into waveguide 2, but it will then duly return. At the output, all the power is in waveguide 1. This exchange of power may take place when k1 = k2 , that is, when the velocities are identical. If we apply a voltage, the velocity of propagation increases in one waveguide and decreases in the other one. In the absence of synchronism the amount of power transferable may be shown to decrease. When the velocities in the two waveguides are radically different, then they simply ignore each other; there is no power transfer from one to the other irrespective of the amount of coupling.

Spatial light modulators

357

Electrode Corrugation Waveguide

L

λg 2

Fig. 13.16 A Bragg type ﬁlter employing grooves as the reﬂecting elements.

W0 Input prism coupler

Incident light beam Acoustic transducers

Y-cut LiNbO3 waveguide

Bragg diffracted light beam Output prism coupler Undiffracted light beam

What can we use such a coupler for? Well, it is obviously a switch. In the absence of a voltage, all the power can be transferred from waveguide 1 to waveguide 2. Destroying the synchronism by then applying a voltage, we can switch the power to waveguide 1 or vice versa.

13.7.4

Filters

One type of ﬁlter, which reﬂects the signal in a certain wavelength band and transmits the rest, may be realized by relying once more on Bragg reﬂection. Cumulative reﬂection may be obtained by placing reﬂecting elements at the right period into the waveguide. This is shown in Fig. 13.16, where the reﬂecting elements are grooves at a distance of λg /2 from each other, with λg being the wavelength in the waveguide. Obviously, a large number of other devices exist which I cannot possibly include in this course, but let me just brieﬂy mention one more, namely the integrated optics realization of the acousto-optic beam deﬂector. In this case, the steerable acoustic column is provided by interdigital surface acoustic wave transducers (see Section 10.13) and the optical beam is conﬁned to the vicinity of the surface by a so-called planar waveguide. The optical beam will then sense the periodic perturbation caused by the surface acoustic wave and will be duly diffracted, as shown in Fig. 13.17.

13.8 Spatial light modulators We have several times mentioned light modulators which modulate the intensity of the incident light beam. Note that in those devices there is only one light

Fig. 13.17 A beam deﬂector in Integrated Optics form.

358

Optoelectronics beam, and it is affected everywhere in the same way by the modulation. Spatial light modulators do the same thing, but different parts of the beam are differently affected. A simple deﬁnition would be that a spatial light modulator is a device which gives a desired light distribution over a certain area. Thus, in principle, all programmable display devices may be regarded as spatial light modulators, including possibly a display at a railway station which announces the departure of trains. Other examples are a cathode-ray tube in a television set or a liquid crystal display in a calculator. I shall discuss here the operation of only one of the modern spatial light modulators, which may also be called an incoherent-to-coherent light converter. Such a device is needed because coherent light is usually more suitable for further processing than incoherent light. A schematic diagram of such a converter is shown in Fig. 13.18. In the absence of input incoherent light from the left (the writing beam) the photoconductor does not conduct, and consequently there is a high voltage drop across the photoconductor and a low voltage across the liquid crystal (in practice the liquid crystal layer is much thinner than the photoconductor). The role of the liquid crystal is to transmit or to absorb the coherent light (reading light) coming from the right, depending on whether there is a voltage across it or not. Thus, the intensity modulation of the writing beam is converted into the intensity modulation of the reading beam. The optical isolator is usually in the form of a wide-band dielectric mirror, which separates the writing and reading beams from each other.

Optical isolator Photoconductor

Liquid crystal

Reading beam

Writing beam

Glass

Fig. 13.18 An incoherent-to-coherent light converter.

~ Transparent electrodes

Glass

Nonlinear Fabry–Perot cavities

359

We have already mentioned the quest for a liquid crystal display in Section 10.15. The ideal device that still needs to be produced is a spatial light modulator which is voltage addressable with a resolution of the order of a wavelength and a speed (say nanoseconds) comparable with that of fast digital computers.

13.9 Nonlinear Fabry–Perot cavities A number of interesting effects occur when either the absorption coefﬁcient or the dielectric constant depend on the intensity of light. In this section we shall discuss one particular manifestation of this nonlinear effect when a dielectric, whose index of refraction obeys eqn (13.4), forms a Fabry–Perot cavity. It is fairly easy to show that the relationship between It , and Ii , the output and input intensity of the cavity, is –1 4R It 2 sin kl , = 1+ Ii (1 – R)2

(13.20)

where l is the length of the cavity, k is the wavenumber, and R is the power reﬂection coefﬁcient. Equation (13.20) makes good sense. When kl = mπ or l = mλ/2, the transmission is maximum (all power is transmitted), whereas minimum transmission occurs when kl = 2(m + 1)(π/2), or l = (2m + 1)(λ/4). For R = 0.36 and 0.7, eqn (13.20) is plotted in Fig. 13.19 for one period as a function of kl. Obviously, the greater is R the sharper is the resonance. Large values of R at a given frequency can be easily achieved by multiple element dielectric mirrors. But, even in the simplest case when we rely upon reﬂection at a dielectric–air interface, we can get quite high values. For InSb, for example, which has been used in bistability experiments, ǫr = 15.9, and R = 0.36. If the dielectric is linear, then an increase in input intensity would lead to a proportional increase in output intensity. Consider now the case when the index of refraction obeys the equation n = n0 + n2 I (assuming that the intensity 1

B A

It Ii

R = 0.36

0.5 R = 0.7

Fig. 13.19

0 mπ

(2m+1) π 2

kl

(m+1)π

A plot of eqn (13.20) for R = 0.36 and 0.7.

360

Optoelectronics inside the cavity is the same as that leaving) and take a point on the It /Ii curve, where the function is increasing (A in Fig. 13.19). What happens now if Ii is increased? Then ﬁrst, we may argue, It will increase as in the linear regime. But an increase in It will lead to an increase in n and k, and consequently, we need to move up to a point higher on the curve, say B. But this means that, for a given value of Ii , we have an even higher value of It , which increases n even further, and in turn makes us move higher up on the curve, etc. Because of this positive feedback, a small increase in Ii may lead to a large increase in It . So the It versus Ii curve may turn out to be highly nonlinear. What could we use this high nonlinearity for? An input–output characteristic shown in Fig. 13.20(a) can be used as an OR gate. The bias input light is OA. The corresponding light output, equivalent to digital zero, is AB. If a pulse is incident upon either output of the OR gate [the (0, 1) or the (1, 0) variety as shown in Fig. 13.20(b)], then the output is another pulse which may be regarded as a logical 1. For an input of (1, 1), that is, when pulses are incident on both inputs of the gate, there is little difference in the intensity of the output beam, as shown in Fig. 13.20(c). This can still be regarded as a logical 1. The same input–output characteristic may also be used as a logical AND gate by biasing it at C [Fig. 13.21(a)]. The output level for logical zero is now determined as being less than AB, which is satisﬁed for inputs (0, 0), (0, 1), and (1, 0). For an input of (1, 1) the output is a logical 1 [Fig. 13.21(b)]. Other types of nonlinear characteristics are, of course, also possible. Under certain conditions we may for example obtain bistability, that is two possible outputs for a given input power. To see when such multiple solutions are possible, let us plot again in Fig. 13.22, It /Ii for R = 0.7, but this time against (a)

(b)

It

B

B

0

0

A

Ii

It

B

Nonlinear, It versus Ii characteristics used as an OR gate.

Ii

1

(c)

Fig. 13.20

1

It

Nonlinear Fabry–Perot cavities (a)

It

It

361

(b)

B C

C

Ii

Ii

1

J

K

L

M

Fig. 13.21 A non linear It versus Ii characteristic used as an AND gate.

N

It Ii

0.5

Fig. 13.22

0

A graphical construction ﬁnding the intersection of the curve given by eqn (13.20) with the straight lines given by eqn (13.21).

(k - k0)1

(k – k0 )l, where k = 2π n/λ. The zero value of k – k0 has been conveniently chosen for our purpose. We are interested in the intersections of this curve with the set of straight lines shown, which were obtained by the following considerations. From eqn (13.4), It =

n – n0 λ = (k – k0 ), n2 2π n2

(13.21)

whence It λ = (k – k0 )l. Ii 2π n2 lIi

(13.22)

According to the above equation, It /Ii is a linear function of (k – k0 )l. There are lots of constants on the right-hand side of eqn (13.22) which are irrelevant, but note the presence of Ii . Each straight line in Fig. 13.22 corresponds to a different value of Ii . For each value of Ii the permissible values of It are given by the intersections of the straight line with the curve. For OJ, a low value of Ii (i.e. high value of the slope), there is only one solution. As Ii increases there are two solutions for OK, three solutions for OL, two solutions for OM, and again, only one solution for ON. Using this graphical method, the It versus Ii curve can be constructed. In the present case it looks roughly like that shown in Fig. 13.23(a). Physically what happens is that as Ii reaches the value of Iil , the value of It will jump from It1 to It2 (see Fig. 13.23(b)) and then will follow

362

Optoelectronics (a) 50

It

0

Ii

0

90

(b) 50 It3 It2 It

Fig. 13.23 (a) The It versus Ii relationship as determined by the construction in Fig. 13.22. (b) The It versus Ii characteristic as it would be measured.

It4 It1 0

0

Iil

Ii

Iih

90

the upper curve. In the reverse direction, when Ii decreases, It will suddenly jump from It3 to the lower curve at It4 and will then follow the lower curve. What is bistability good for? Quite obviously, just as in the case of the similarly looking ferrite hysteresis loop, we can make memory elements out of them. By adding for example a switching beam to a holding beam the device can switch from a low output state to a high output state. Summarizing, our nonlinear cavity has yielded components both for logical arithmetic and storage. The hope is that one day they will be parts of all-optical computers. Their main advantage in the applications discussed in the present section is speed. The physical mechanism causing the nonlinearity is fast. Switching speeds of the order of 1 ps have been measured.

13.10

Optical switching

MEMS were mentioned in Section 9.26. They represent a new way of doing things. Parts of the structures produced that way can actually move, so it is possible, for example, to produce movable mirrors which can redirect a beam of light. But that is exactly the thing we need for optical switching. We need it badly. The present practice is rather cumbersome. It may be likened to the plight of the traveller who wants to travel from Oxford to Cambridge in the comfort of a railway carriage. He can certainly take a train from Oxford to Paddington Station, London, but there he is forced to disembark. He must then travel by tube to Liverpool Street Station from where he is allowed the luxury of boarding another train. The journey by tube is a nuisance. Signals travelling in optical ﬁbres face the same problems. They can rarely reach their destination

Optical switching

363

without change of a rather brutal nature. Within picoseconds of their arrival they are unceremoniously converted into electronic form, interrogated as to their ﬁnal destination, reconverted into optical form, and ﬁnally bundled into the appropriate optical output ﬁbre. Obviously, this conversion–reconversion business is a nuisance. Actually, it is more than a nuisance. Electrons generate heat and as the density of elements increases, the point might have already been reached where there is no easy way to keep the temperature rise to an acceptable limit. It is as if the carriages in the tube that take you from Paddington to Liverpool Street Station are not only uncomfortable but unbearably hot as well. So let us see how such an interchange will be done in the future. The movable mirror, whose construction was brieﬂy discussed in Section 9.26, can of course be constructed in two-dimensional arrays. A ﬁne example of a 6 × 6 array, in which the angular position of each element can be controlled, is shown in Fig. 13.24(a). Two such arrays may then be used in an optical cross-connect switch, as shown in Figure 13.24(b). The inputs and outputs are two square bundles of optical ﬁbres equipped with collimators to produce small diameter free-space beams. Each input beam is arranged to strike one of the MEMS mirrors in the ﬁrst array. This mirror may turn to point at any mirror in the second array, which may then turn to route the beam to its corresponding output ﬁbre. Switches of this type may be extremely large, with up to 1000 inputs and 1000 outputs. What about speed? Is mechanical movement not bound to be slow? Yes, it is, but it does not matter. It is a massively parallel operation. We can switch simultaneously hundreds of beams. It is optics. The beams can cross each other

(a) Mirror element

Local electronics

Sensing and control lines Fibre j

(b)

Mirror j Mirror array 2

Input ﬁbre array

Lens array Output ﬁbre array Mirror array 1 Mirror i

Fibre i

Lens array

Fig. 13.24 (a) A 6 × 6 mirror array of dual-axis MEMS torsion mirror. (b) Optical cross-connect constructed from two mirror arrays. After R.R.A. Syms, J. Lightwave Technol. 20, 1084, 2002.

364

Optoelectronics without any cross-talk. And, besides, a single mirror can switch an enormous amount of information from ﬁbre A to ﬁbre B, and may be a 100 Gigabits or may be even more in the future. Who would worry then about a switching time that might be a few milliseconds?

Absorption

13.11

0

100 hf - Eg(meV)

200

Fig. 13.25 Absorption as a function of excess photon energy for bulk material (continuous lines) and 30 nm-thick quantum well material (dotted lines).

Electro-absorption in quantum well structures

This is a fairly new phenomenon with potential for device applications. We shall include it not only because it might become a winner (it is rather hazardous to predict which device will prove to be commercially competitive), but also because it is such a good illustration of a number of physical principles discussed in this course. We shall touch upon such topics as the conﬁnement of electrons and holes to a certain region by the erection of potential barriers, the modiﬁcation of semiconductor absorption characteristics when excitons (bound electron–hole pairs) are taken into account, what happens to excitons in a potential well, how an electric ﬁeld inﬂuences the energy levels, and in particular, how it affects conﬁned excitons (known as the Quantum Conﬁned Stark Effect), and ﬁnally, how these varied phenomena can be exploited in devices. I have already talked a lot about quantum wells. One of the examples we looked at was made of GaAs and AlGaAs. For our present purpose, it is important that the wells are wide enough for tunnelling to be negligible, but narrow enough so that the electrons and holes know that they are not in an inﬁnitely thick material. The energy levels in such two-dimensional wells were discussed in Section 12.7. We know that the available energies may be represented by a set of sub-bands. The momentum is quantized in the direction perpendicular to the walls, but not in the other two. Let us consider now optical absorption in such a quantum well material. It is still true that when a photon excites an electron–hole pair, both energy and momentum must be conserved. Therefore, the transitions will occur between a sub-band in the valence band and a sub-band in the conduction band, having the same value of n. As the photon frequency increases, it is still possible, for a while, to ﬁnd transitions between the same two sub-bands, and as long as the sub-bands are the same, the absorption remains constant. The theoretical plot of the absorption coefﬁcient as a function of hf – Eg (photon energy – gap energy) is a series of steps, as shown in Fig. 13.25 for a 30 nm-wide quantum well.

13.11.1

Excitons

We have mentioned excitons before in Section 9.4, rather facetiously, when contrasting them with electron–hole pairs, which disappear by recombination. Let me say again what excitons are. They are electron–hole pairs bound together by Coulomb forces. Their existence can usually be ignored, but they must be taken into account when looking at optical absorption on a ﬁne scale. Up to now we have argued that, in order to absorb a photon and to create an electron–hole pair, the minimum amount of energy is the gap energy. However, if we take excitons into account, then we may realize that photons incident

Electro-absorption in quantum well structures

365

with an energy somewhat less than the gap energy may also be absorbed because creating a bound electron–hole pair (i.e. an exciton) needs less energy than creating a free electron–hole pair. The difference between the two is the binding energy. How can we determine this binding energy? We may simply argue that the binding energy between an electron and a hole is the same type as that between an electron and a proton, and we may then use the hydrogen atom formulae into which we need to substitute the actual values of dielectric constant and effective mass. In bulk GaAs the binding energy may be calculated to be 4.2 meV, and the orbit of the exciton in its lowest state (called the 1s state in analogy with the hydrogen atom) is about 30 nm. Does this mean that we see a sharply deﬁned energy level below the gap? No, because we have to take into account that the lifetime of an exciton is not more than a few hundred femtoseconds and, therefore, the line will be considerably broadened. The outcome of all this is that, in bulk materials at room temperature, the excitonic resonance can hardly be noticed.

This is the same calculation as we did in Section 8.3 for silicon for ﬁnding the ionization energy needed to promote an electron from a donor level into the conduction band. The physics for the energy levels of excitons is fairly similar.

13.11.2 Excitons in quantum wells Let us now consider the effect of excitons upon the absorption spectrum in a quantum well material. If the width of the well is larger than the exciton orbit then, obviously, the excitons will hardly be affected. But if the width of the well is less than the diameter of the lowest orbit, then the exciton has no other option but to get squashed in the direction perpendicular to the layers. What will happen in the other directions? A good indication can be obtained by solving the problem of the two-dimensional hydrogen atom. It turns out that the diameter will reduce by a factor of 4. So we may come to the conclusion that the size of the exciton will be reduced in all three dimensions, and consequently its binding energy will be increased. Calculations yield a binding energy of 10 meV, indicating that the exciton absorption effect is much stronger. We may expect to see exciton peaks associated with each absorption step. Experiments show that our expectations are correct. For a GaAs quantum well of 10 nm width, the measured absorption spectrum is shown in Fig. 13.26. Both the peaks and the steps may be clearly distinguished. Do not worry about the double peak. It is simply due to the fact that there are both heavy and light holes present, which has not so far been mentioned, because they do not affect the basic argument.

13.11.3 Electro-absorption This means optical absorption in the presence of an electric ﬁeld. Will the excitons know that an electric ﬁeld is present? They certainly will. An electric ﬁeld will try to move the two particles in opposite directions. Since there is a tendency anyway for the two particles to part company, they can more easily do so in the presence of an electric ﬁeld. Consequently, the exciton is more likely to be ionized (this is called ﬁeld ionization), its lifetime will be shorter, and the absorption line will be broader. All this is true for the bulk material. But will the argument change in any way for a quantum well material? If the electric ﬁeld is applied in the direction of the layers, then the same argument will still roughly hold: the chances of being able to ionize the exciton with

366

Optoelectronics

Absorption (105/m-1)

20

15

10

Fig. 13.26 Measured absorption spectrum of a GaAs quantum well of 10 nm thickness.

0

1.46

1.54 1.62 Photon energy (eV)

1.7

the aid of the electric ﬁeld must be high. However, when the electric ﬁeld is applied perpendicular to the layers, then the good intentions of the electric ﬁeld in trying to separate the particles are frustrated by the presence of the walls. Provided the well is narrow enough, the exciton is not ﬁeld ionized. Thus, the exciton resonance is still there albeit with reduced amplitude due to the increased separation of the electron–hole pair. There is also a shift in the position of the resonance due to the electrostatic energy (this is nothing else but the energy of a dipole in an electric ﬁeld, something we have discussed before). The expectations based on the above qualitative argument are borne out by the experimental observations, as shown in Fig. 13.27, where the absorption spectrum measured for a GaAs–AlGaAs quantum well structure is plotted against photon energy. This phenomenon is known as the Quantum Conﬁned Stark Effect. The excitons are obviously quantum conﬁned, and the Stark

4

(i)

Fig. 13.27 Measured absorption spectrum of a quantum well for electric ﬁeld applied perpendicularly to the layers, (i) 1.6 × 104 V m–1 , (ii) 105 V m–1 , (iii) 1.4 × 105 V m–1 , (iv) 1.8 × 105 V m–1 , (v) 2.2 × 105 V m–1 .

log transmission

(ii) (iii)

2

(iv) (v)

0 1.42

1.46 Photon energy (eV)

A

1.5

Electro-absorption in quantum well structures effect is the description used for the shift and splitting of energy levels in an electric ﬁeld. Talking of electro-absorption, I should also mention the Franz–Keldysh effect, which is usually observed at electric ﬁelds considerably higher than that needed to see the effect upon exciton resonance. It bears some similarity to the Schottky effect (see Section 6.6), in which electrons excited thermally to high enough energy levels could tunnel across a barrier made thin by the presence of a high electric ﬁeld. For the Franz–Keldysh effect, the energy is provided by an input photon with an energy less than the bandgap energy, and then tunnelling can do the rest to provide an electron–hole pair.

367

It earned the 1919 Nobel Prize for Stark. He was the only Nobel prizewinner who became a strong supporter of Nazism. His job (he did it very well) was to ‘purify’ German universities of ‘contaminated blood’. The ‘impure’ refugees from German and Austrian universities played a large part in defeating Nazism.

13.11.4 Applications If I had to classify the quantum conﬁned Stark effect in literary terms, I would not quite know where to place it. Perhaps melodrama would be the right category, considering the touching affection between electrons and holes. If we consider, however, how they stave off brutal intervention by the electric ﬁeld, with their backs against the potential wall, and how quickly all these things happen, then melodrama might give way to a thriller. And that is certainly the category to which our ultimate question belongs: ‘can these effects be used for something?’ Well, if the attenuation of the device depends on the electric ﬁeld, then the amount of light across it may be modulated by changing the applied voltage. We need relatively high ﬁelds, which we know may be achieved by placing the multiple quantum well structure inside a junction as shown in Fig. 13.28. It is a reverse bias p–i–n junction, in which the p+ and n+ materials are made of AlGaAs, and the quantum well provides the intrinsic part of the junction.

GaAs Substrate Quantum well structure

Al Ga As Contact metal

Light out

Contact metal

Al Ga As

Light in

Fig. 13.28 A quantum well structure inside a reverse bias p–i–n junction used as a light modulator.

368

Optoelectronics Pin R

– V0

P i n

Quantum well

+

Fig. 13.29 The device of Fig. 13.24 in a circuit in which it can exhibit bistability.

Pout

It is grown on a GaAs substrate, which needs to be etched away, since it is not transparent at the wavelength where the mechanism is suitable for modulation. What else can we do with this device? It can be used for light detection in the same manner as an ordinary p–i–n junction. The added advantage of the multiple quantum well structure is that the resulting photocurrent is strongly dependent on the applied voltage and on the wavelength. It can therefore be used, admittedly in a very narrow range, for measuring wavelength. The most interesting application is, however, for a bistable device, shown schematically in Fig. 13.29. The wavelength of the incident light is chosen, so that decreasing reverse bias voltage gives increasing optical absorption (line A in Fig. 13.27). In the absence of optical input, no current ﬂows, and hence all the applied voltage appears across the quantum wells. As light is incident, a photocurrent ﬂows, hence the voltage across the quantum wells decreases, which leads to higher absorption, which in turn leads to lower voltage, etc. There is obviously positive feedback, which under certain circumstances may be shown to lead to switching to a high absorption state with low voltage across the junction. The problem can of course be solved rigorously by considering the relationship between the four variables, namely the input optical power, Pin , the output optical power, Pout , the voltage across the quantum wells, V , and the current ﬂowing in the circuit, I. First, we need Pout = Pout (Pin , V , λ),

(13.23)

which can be derived from experimental results like those shown in Fig. 13.27. Second, we need the current–voltage characteristics of the circuit of Fig. 13.25, which may be written simply as V = V0 – IR.

(13.24)

And third, we need to determine the current which ﬂows in response to the light power incident upon the junction, I = I(V , Pin , λ).

(13.25)

From eqns (13.23–13.25) we may then derive the Pout versus Pin curve which, in many cases, will exhibit bistability similar to that shown in Fig. 13.23.

Exercises

369

Let us now summarize the advantages of multiple quantum well structures for the applications discussed. The main advantage is compatibility, that is the voltages are compatible with the electronics, and the wavelengths are compatible with laser diodes. In addition, the materials are compatible with those used both in electronics and for laser diodes, so the devices are potential candidates for components in integrated opto-electronic systems. I have only mentioned GaAs–AlGaAs structures, but there are, of course, others as well. The rules are clearly the same, that apply to the production of heterojunction lasers. The lattice constants must be close, and the bandgaps must be in the right range. Interestingly, some of the combinations offer quite new physics; for example in an InAs–GaSb quantum well, the electrons are conﬁned in one layer and the holes in the other. As you may have gathered, I ﬁnd this topic quite fascinating, so perhaps I have spent a little more time on it than its present status would warrant. I hope you will forgive me.

Exercises 13.1. Light of frequency ν and intensity I0 is incident upon a photoconductor (Fig. 13.30) which has an attenuation coefﬁcient α. Assuming that only electrons are generated, show that the excess current due to the input light is 1 – e–αd b ηI0 τe μe V , c hν α where τe is the electron lifetime and η is the quantum efﬁciency (average number of electrons generated per incident photon). I = e

Find an expression for this for the photoconductor discussed in Exercise 13.1. 13.3. In a p–i–n diode the so-called intrinsic region is usually a lightly doped n-type region. Determine the electric ﬁeld and potential distribution for a reverse bias of Ur when the impurity densities of the three regions are NA , ND1 , and ND2 (see Fig. 13.31). p+

n

n+

NA

N D1

N D2

d1

d2

d3

Light

N D2

N D1

d

b c

Fig. 13.31 V

Fig. 13.30 13.2. The photoconductive gain is deﬁned as G=

Number of photocarriers crossing the electrodes per unit time . Number of photocarriers generated per unit time

When this device is used as a photodetector with light incident from the left, the p+ region must be made extremely thin. Why? [Hint: Assume that the depletion region is all in the lightly doped n-region. Neglect the built-in voltage.] 13.4. A volume hologram is recorded in a photosensitive material with a refractive index of 1.52, at a wavelength of

370

Optoelectronics

514.5 nm, by two beams incident from air at angles ±5◦ in the geometry of Fig. 13.3. (i) What is the grating spacing in the material? (ii) What should be the incident angle if the hologram is to be replayed at 633 nm? (iii) If the hologram is to be replayed at the second Bragg angle, what will that angle be at the two above mentioned wavelengths? 13.5. A volume hologram is recorded by two beams incident perpendicularly upon a photosensitive medium from opposite sides (the so-called reﬂection geometry). (i) What will be the grating spacing at wavelengths 514.5 nm and 633 nm? Take n = 1.52. (ii) Which conﬁguration do you think will be more sensitive to replay wavelength, the transmission type or the reﬂection type? 13.6. Some crystals have the property that they are isotropic in the absence of an electric ﬁeld but become aniostropic when an electric ﬁeld is applied. The dielectric constant tensor in such a material in the XYZ coordinate system (Fig. 13.32) is as follows: ⎤ ⎡ ǫXX 0 0 ǫ = ǫ0 ⎣ 0 ǫYY 0 , 0 0 ǫZZ

where

ǫr = ǫXX = ǫYY = ǫZZ . y Y

X x

Z,z Electric ﬁeld polarized vertically

–ǫXY = ǫr2 rXYZ EZ . (i) Find the dielectric tensor in the presence of an electric ﬁeld applied in the Z-direction. (ii) Transform this dielectric tensor into the xyz coordinate system. Note that x, y is 45◦ clockwise from XY . (iii) Will the input wave, shown in Fig. 13.28, be affected by the applied electric ﬁeld? (Note: This is the actual tensor of a Bi12 SiO20 crystal cut in a certain way, apart from optical activity which we have disregarded here.) 13.7. The differential equations for the amplitudes of waves in two coupled waveguides are given in eqns (13.16) and (13.17). (i) Find the solution with boundary conditions A1 = A10 and A2 = 0 at z = 0. (ii) Show that the solution reduces to those of eqns (13.18) and (13.19) when k1 = k2 = k. (iii) If the length of the interaction region is 1 cm, what should be the value of the coupling constant in order to achieve complete power transfer from waveguide 1 into waveguide 2? (iv) By how much should v2 the phase velocity in waveguide 2 be different from that in waveguide 1 in order to reduce the power coupled into waveguide 2 by a factor 2? Take L = 1 cm, K = π/2 cm–1 , λ = 633 nm, and, initially, v1 = v2 = v = 108 m s–1 . 13.8. An electromagnetic wave with an electric ﬁeld Ei is incident perpendicularly on the Fabry–Perot resonator shown in Fig. 13.33. The amplitude reﬂectivities and transmittivities of the mirrors are r1 , t1 and r2 , t2 respectively, the wave number is k, and the gain coefﬁcient of the medium ﬁlling the resonator is γ . Derive an expression (by summing an inﬁnite geometrical series) for the transmitted electric ﬁeld, Et . Fabry–Perot resonator

incident beam

Fig. 13.32 The electro-optic coefﬁcient may now be assumed to have a component which relates, in the same coordinate system, the change in the ǫXY component of the dielectric tensor to the Z, component of the electric ﬁeld as

i

Fig. 13.33

t

Superconductivity

14

I go on for ever. Tennyson The Brook

14.1 Introduction Superconductivity was a scientiﬁc curiosity for a long time, but by now there are some actual applications like producing high magnetic ﬁelds for magnetic resonance imaging; and there are lots of potential applications. The big prize would of course be superconductive lines for power transmission which would eliminate losses. But quite apart from applications, I feel that some acquaintance with superconductivity should be part of modern engineering education. Superconductivity is, after all, such an extraordinary phenomenon, so much in contrast with everything we are used to. It is literally out of this world. Our world is classical, but superconductivity is a quantum phenomenon—a quantum phenomenon on a macroscopic scale. The wavefunctions, for example, that lead an artiﬁcial existence in quantum mechanics proper appear in superconductivity as measurable quantities. The discovery of superconductivity was not very dramatic. When Kamerlingh Onnes (Nobel Prize, 1913) succeeded in liquefying helium in 1908, he looked around for something worth measuring at that temperature range. His choice fell upon the resistivity of metals. He tried platinum ﬁrst and found that its resistivity continued to decline at lower temperatures, tending to some small but ﬁnite value as the temperature approached absolute zero. He could have tried a large number of other metals with similar prosaic results. But he was in luck. His second metal, mercury, showed quite unorthodox behaviour. Its resistivity (as shown in Fig. 14.1) suddenly decreased to such a small value that he was unable to measure it—and no one has succeeded in measuring it ever since. The usual technique is to induce a current in a ring made of superconducting material and measure the magnetic ﬁeld due to this current. In a normal metal the current would decay in about 10–12 s. In a superconductor the current can go round for a considerably longer time—measured not in picoseconds but in years. One of the longest experiments was made somewhere in the United States; the current was going round and round for three whole years without any detectable decay. Unfortunately, the experiment came to an abrupt end when a res